advertisement

Semiconductor Physics and Devices Basic Principles Fourth Edition Donald A. Neamen University of New Mexico TM nea29583_fm_i-xxiv.indd i 12/11/10 1:01 PM TM SEMICONDUCTOR PHYSICS & DEVICES: BASIC PRINCIPLES, FOURTH EDITION Published by McGraw-Hill, a business unit of The McGraw-Hill Companies, Inc., 1221 Avenue of the Americas, New York, NY 10020. Copyright © 2012 by The McGraw-Hill Companies, Inc. All rights reserved. Previous editions © 2003, 1997 and 1992. No part of this publication may be reproduced or distributed in any form or by any means, or stored in a database or retrieval system, without the prior written consent of The McGraw-Hill Companies, Inc., including, but not limited to, in any network or other electronic storage or transmission, or broadcast for distance learning. Some ancillaries, including electronic and print components, may not be available to customers outside the United States. This book is printed on acid-free paper. 1 2 3 4 5 6 7 8 9 0 DOC/DOC 1 0 9 8 7 6 5 4 3 2 1 ISBN MHID 978-0-07-352958-5 0-07-352958-3 Vice President & Editor-in-Chief: Marty Lange Vice President EDP/Central Publishing Services: Kimberly Meriwether David Publisher: Raghu Srinivasan Sponsoring Editor: Peter E. Massar Marketing Manager: Curt Reynolds Development Editor: Lora Neyens Project Manager: Melissa M. Leick Design Coordinator: Brenda A. Rolwes Cover Designer: Studio Montage, St. Louis, Missouri Cover Image: © Getty Images RF Buyer: Sherry L. Kane Media Project Manager: Balaji Sundararaman Compositor: MPS Limited, a Macmillan Company Typeface: 10/12 Times Roman Printer: RR Donnelley, Crawfordsville All credits appearing on page or at the end of the book are considered to be an extension of the copyright page. Library of Congress Cataloging-in-Publication Data Neamen, Donald A. Semiconductor physics and devices : basic principles / Donald A. Neamen. — 4th ed. p. cm. Includes index. ISBN 978-0-07-352958-5 (alk. paper) 1. Semiconductors. I. Title. QC611.N39 2011 537.6'22—dc22 2010045765 www.mhhe.com nea29583_fm_i-xxiv.indd ii 12/11/10 1:01 PM ABOUT THE AUTHOR Donald A. Neamen is a professor emeritus in the Department of Electrical and Computer Engineering at the University of New Mexico where he taught for more than 25 years. He received his Ph.D. from the University of New Mexico and then became an electronics engineer at the Solid State Sciences Laboratory at Hanscom Air Force Base. In 1976, he joined the faculty in the ECE department at the University of New Mexico, where he specialized in teaching semiconductor physics and devices courses and electronic circuits courses. He is still a part-time instructor in the department. He also recently taught for a semester at the University of Michigan-Shanghai Jiao Tong University (UM-SJTU) Joint Institute in Shanghai, China. In 1980, Professor Neamen received the Outstanding Teacher Award for the University of New Mexico. In 1983 and 1985, he was recognized as Outstanding Teacher in the College of Engineering by Tau Beta Pi. In 1990, and each year from 1994 through 2001, he received the Faculty Recognition Award, presented by graduating ECE students. He was also honored with the Teaching Excellence Award in the College of Engineering in 1994. In addition to his teaching, Professor Neamen served as Associate Chair of the ECE department for several years and has also worked in industry with Martin Marietta, Sandia National Laboratories, and Raytheon Company. He has published many papers and is the author of Microelectronics Circuit Analysis and Design, 4th edition, and An Introduction to Semiconductor Devices. nea29583_fm_i-xxiv.indd iii 12/11/10 1:01 PM CONTENTS Preface x 2.2 Prologue—Semiconductors and the Integrated Circuit xvii PART I—Semiconductor Material Properties CHAPTER 2.2.1 2.2.2 2.2.3 2.3 1 Preview 1 Semiconductor Materials Types of Solids 2 Space Lattices 3 1.3.1 1.3.2 1.3.3 1.3.4 1.4 1.5 *1.6 2.4 Primitive and Unit Cell 3 Basic Crystal Structures 4 Crystal Planes and Miller Indices 6 Directions in Crystals 9 The Diamond Structure 10 Atomic Bonding 12 Imperfections and Impurities in Solids 1.6.1 1.6.2 *1.7 1 14 Imperfections in Solids 14 Impurities in Solids 16 Growth of Semiconductor Materials 17 1.7.1 Growth from a Melt 17 1.7.2 Epitaxial Growth 19 1.8 3.0 3.1 Preview 58 Allowed and Forbidden Energy Bands 59 Electrical Conduction in Solids 72 3.2.1 The Energy Band and the Bond Model 72 3.2.2 Drift Current 74 3.2.3 Electron Effective Mass 75 3.2.4 Concept of the Hole 78 3.2.5 Metals, Insulators, and Semiconductors 80 Introduction to Quantum Mechanics 25 2.1.1 Energy Quanta 26 2.1.2 Wave–Particle Duality 27 2.1.3 The Uncertainty Principle 30 3 3.1.1 Formation of Energy Bands 59 *3.1.2 The Kronig–Penney Model 63 3.1.3 The k-Space Diagram 67 2 Preview 25 Principles of Quantum Mechanics Summary 51 Problems 52 Introduction to the Quantum Theory of Solids 58 3.2 2.0 2.1 The One-Electron Atom 46 The Periodic Table 50 CHAPTER Summary 20 Problems 21 CHAPTER Electron in Free Space 35 The Infinite Potential Well 36 The Step Potential Function 39 The Potential Barrier and Tunneling 44 Extensions of the Wave Theory to Atoms 46 2.4.1 2.4.2 2.5 31 The Wave Equation 31 Physical Meaning of the Wave Function 32 Boundary Conditions 33 Applications of Schrodinger’s Wave Equation 34 2.3.1 2.3.2 2.3.3 2.3.4 The Crystal Structure of Solids 1 1.0 1.1 1.2 1.3 Schrodinger’s Wave Equation 26 3.3 Extension to Three Dimensions 3.3.1 3.3.2 83 The k-Space Diagrams of Si and GaAs 83 Additional Effective Mass Concepts 85 iv nea29583_fm_i-xxiv.indd iv 12/11/10 1:01 PM Contents 3.4 Density of States Function 4.7 85 3.4.1 Mathematical Derivation 85 3.4.2 Extension to Semiconductors 88 3.5 Statistical Mechanics 91 3.6 4 Preview 106 Charge Carriers in Semiconductors 4.1.1 4.1.2 4.1.3 4.1.4 4.2 107 Equilibrium Distribution of Electrons and Holes 107 The n0 and p0 Equations 109 The Intrinsic Carrier Concentration 113 The Intrinsic Fermi-Level Position 116 Dopant Atoms and Energy Levels The Extrinsic Semiconductor 123 4.3.1 Equilibrium Distribution of Electrons and Holes 123 4.3.2 The n0 p0 Product 127 *4.3.3 The Fermi–Dirac Integral 128 4.3.4 Degenerate and Nondegenerate Semiconductors 130 4.4 5.2 5.3 Statistics of Donors and Acceptors 131 Charge Neutrality 135 *5.4 5.5 4.6 Position of Fermi Energy Level nea29583_fm_i-xxiv.indd v Graded Impurity Distribution 176 Induced Electric Field 176 The Einstein Relation 178 The Hall Effect 180 Summary 183 Problems 184 6 Nonequilibrium Excess Carriers in Semiconductors 192 6.0 6.1 Preview 192 Carrier Generation and Recombination 6.1.1 6.1.2 6.2 198 6.2.1 Continuity Equations 198 6.2.2 Time-Dependent Diffusion Equations Ambipolar Transport 6.3.1 6.3.2 6.3.3 6.3.4 *6.3.5 193 The Semiconductor in Equilibrium 193 Excess Carrier Generation and Recombination 194 Characteristics of Excess Carriers 141 4.6.1 Mathematical Derivation 142 4.6.2 Variation of EF with Doping Concentration and Temperature 144 4.6.3 Relevance of the Fermi Energy 145 172 Diffusion Current Density 172 Total Current Density 175 CHAPTER 6.3 4.5.1 Compensated Semiconductors 135 4.5.2 Equilibrium Electron and Hole Concentrations 136 Carrier Diffusion 5.3.1 5.3.2 4.4.1 Probability Function 131 4.4.2 Complete Ionization and Freeze-Out 132 4.5 Preview 156 Carrier Drift 157 5.2.1 5.2.2 118 4.2.1 Qualitative Description 118 4.2.2 Ionization Energy 120 4.2.3 Group III–V Semiconductors 122 4.3 5.0 5.1 5.1.1 Drift Current Density 157 5.1.2 Mobility Effects 159 5.1.3 Conductivity 164 5.1.4 Velocity Saturation 169 The Semiconductor in Equilibrium 106 4.0 4.1 5 Carrier Transport Phenomena 156 Summary 98 Problems 100 CHAPTER Summary 147 Problems 149 CHAPTER 3.5.1 Statistical Laws 91 3.5.2 The Fermi–Dirac Probability Function 91 3.5.3 The Distribution Function and the Fermi Energy 93 v 199 201 Derivation of the Ambipolar Transport Equation 201 Limits of Extrinsic Doping and Low Injection 203 Applications of the Ambipolar Transport Equation 206 Dielectric Relaxation Time Constant 214 Haynes–Shockley Experiment 216 12/11/10 1:01 PM vi 6.4 *6.5 Contents 6.5.1 6.5.2 *6.6 8.1.4 Minority Carrier Distribution 283 8.1.5 Ideal pn Junction Current 286 8.1.6 Summary of Physics 290 8.1.7 Temperature Effects 292 8.1.8 The “Short” Diode 293 Quasi-Fermi Energy Levels 219 Excess Carrier Lifetime 221 Shockley–Read–Hall Theory of Recombination 221 Limits of Extrinsic Doping and Low Injection 225 Surface Effects 8.2 227 6.6.1 Surface States 227 6.6.2 Surface Recombination Velocity 229 6.7 Summary 231 Problems 233 PART 8.2.1 Generation–Recombination Currents 296 8.2.2 High-Level Injection 302 8.3 *8.4 7 Preview 241 Basic Structure of the pn Junction Zero Applied Bias 243 242 7.2.1 Built-in Potential Barrier 243 7.2.2 Electric Field 246 7.2.3 Space Charge Width 249 7.3 Reverse Applied Bias 251 7.3.1 Space Charge Width and Electric Field 251 7.3.2 Junction Capacitance 254 7.3.3 One-Sided Junctions 256 7.4 *7.5 Junction Breakdown 258 Nonuniformly Doped Junctions *8.5 8.6 CHAPTER 9.0 9.1 9.2 8.1.1 9.3 277 Qualitative Description of Charge Flow in a pn Junction 277 8.1.2 Ideal Current–Voltage Relationship 278 8.1.3 Boundary Conditions 279 nea29583_fm_i-xxiv.indd vi 318 9 Preview 331 The Schottky Barrier Diode 332 Metal–Semiconductor Ohmic Contacts 349 9.2.1 Ideal Nonrectifying Barrier 349 9.2.2 Tunneling Barrier 351 9.2.3 Specific Contact Resistance 352 8 Preview 276 pn Junction Current The Tunnel Diode Summary 321 Problems 323 9.1.1 Qualitative Characteristics 332 9.1.2 Ideal Junction Properties 334 9.1.3 Nonideal Effects on the Barrier Height 338 9.1.4 Current–Voltage Relationship 342 9.1.5 Comparison of the Schottky Barrier Diode and the pn Junction Diode 345 The pn Junction Diode 276 8.0 8.1 314 Metal–Semiconductor and Semiconductor Heterojunctions 331 262 Summary 267 Problems 269 304 The Turn-off Transient 315 The Turn-on Transient 317 CHAPTER 7.5.1 Linearly Graded Junctions 263 7.5.2 Hyperabrupt Junctions 265 7.6 Charge Storage and Diode Transients 8.4.1 8.4.2 The pn Junction 241 7.0 7.1 7.2 Small-Signal Model of the pn Junction 8.3.1 Diffusion Resistance 305 8.3.2 Small-Signal Admittance 306 8.3.3 Equivalent Circuit 313 II—Fundamental Semiconductor Devices CHAPTER Generation–Recombination Currents and High-Injection Levels 295 Heterojunctions 9.3.1 9.3.2 9.3.3 *9.3.4 *9.3.5 354 Heterojunction Materials 354 Energy-Band Diagrams 354 Two-Dimensional Electron Gas 356 Equilibrium Electrostatics 358 Current–Voltage Characteristics 363 12/11/10 1:01 PM Contents 9.4 11.1.2 Channel Length Modulation 446 11.1.3 Mobility Variation 450 11.1.4 Velocity Saturation 452 11.1.5 Ballistic Transport 453 Summary 363 Problems 365 CHAPTER 10 Fundamentals of the Metal–Oxide– Semiconductor Field-Effect Transistor 371 10.0 10.1 Preview 371 The Two-Terminal MOS Structure Capacitance–Voltage Characteristics The Basic MOSFET Operation Frequency Limitations 10.4.1 10.4.2 *10.5 10.6 11.4 CHAPTER 394 422 Additional Electrical Characteristics Radiation and Hot-Electron Effects 11.5.1 11.5.2 11.5.3 11.6 464 475 Radiation-Induced Oxide Charge 475 Radiation-Induced Interface States 478 Hot-Electron Charging Effects 480 Summary 481 Problems 483 CHAPTER 12 The Bipolar Transistor 491 12.0 12.1 Preview 491 The Bipolar Transistor Action 12.1.1 12.1.2 427 12.1.3 12.1.4 12.2 492 The Basic Principle of Operation 493 Simplified Transistor Current Relation— Qualitative Discussion 495 The Modes of Operation 498 Amplification with Bipolar Transistors 500 Minority Carrier Distribution 501 12.2.1 Forward-Active Mode 502 12.2.2 Other Modes of Operation 508 11 Preview 443 Nonideal Effects 444 11.1.1 Subthreshold Conduction 444 nea29583_fm_i-xxiv.indd vii *11.5 403 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts 443 11.0 11.1 457 11.4.1 Breakdown Voltage 464 *11.4.2 The Lightly Doped Drain Transistor 470 11.4.3 Threshold Adjustment by Ion Implantation 472 Small-Signal Equivalent Circuit 422 Frequency Limitation Factors and Cutoff Frequency 425 The CMOS Technology Summary 430 Problems 433 Threshold Voltage Modifications 11.3.1 Short-Channel Effects 457 11.3.2 Narrow-Channel Effects 461 10.3.1 MOSFET Structures 403 10.3.2 Current–Voltage Relationship—Concepts 404 *10.3.3 Current–Voltage Relationship— Mathematical Derivation 410 10.3.4 Transconductance 418 10.3.5 Substrate Bias Effects 419 10.4 MOSFET Scaling 455 11.2.1 Constant-Field Scaling 455 11.2.2 Threshold Voltage—First Approximation 456 11.2.3 Generalized Scaling 457 11.3 10.2.1 Ideal C–V Characteristics 394 10.2.2 Frequency Effects 399 10.2.3 Fixed Oxide and Interface Charge Effects 400 10.3 11.2 372 10.1.1 Energy-Band Diagrams 372 10.1.2 Depletion Layer Thickness 376 10.1.3 Surface Charge Density 380 10.1.4 Work Function Differences 382 10.1.5 Flat-Band Voltage 385 10.1.6 Threshold Voltage 388 10.2 vii 12.3 Transistor Currents and Low-Frequency Common-Base Current Gain 509 12.3.1 12.3.2 Current Gain—Contributing Factors 509 Derivation of Transistor Current Components and Current Gain Factors 512 12/11/10 1:01 PM viii Contents 12.3.3 12.3.4 12.4 Nonideal Effects 12.4.1 12.4.2 12.4.3 12.4.4 *12.4.5 12.4.6 12.5 Summary 517 Example Calculations of the Gain Factors 517 *13.3 13.3.1 13.3.2 13.3.3 522 Base Width Modulation 522 High Injection 524 Emitter Bandgap Narrowing 526 Current Crowding 528 Nonuniform Base Doping 530 Breakdown Voltage 531 Equivalent Circuit Models *13.4 *13.5 536 Frequency Limitations 12.7 Large-Signal Switching 13.6 549 Other Bipolar Transistor Structures 551 552 14.0 14.1 14.2.3 14.2.4 14.2.5 13.1.1 13.1.2 13.2 14.3 572 The Device Characteristics 578 13.2.1 Internal Pinchoff Voltage, Pinchoff Voltage, and Drain-to-Source Saturation Voltage 578 13.2.2 Ideal DC Current–Voltage Relationship— Depletion Mode JFET 582 13.2.3 Transconductance 587 13.2.4 The MESFET 588 nea29583_fm_i-xxiv.indd viii 14.4 619 624 The pn Junction Solar Cell 624 Conversion Efficiency and Solar Concentration 627 Nonuniform Absorption Effects 628 The Heterojunction Solar Cell 629 Amorphous Silicon Solar Cells 630 Photodetectors 14.3.1 14.3.2 14.3.3 14.3.4 14.3.5 Basic pn JFET Operation 572 Basic MESFET Operation 576 618 Photon Absorption Coefficient 619 Electron–Hole Pair Generation Rate 622 Solar Cells 14.2.1 14.2.2 13 Preview 571 JFET Concepts 14 Preview 618 Optical Absorption 14.1.1 14.1.2 The Junction Field-Effect Transistor 571 13.0 13.1 III—Specialized Semiconductor Devices Optical Devices 14.2 Summary 558 Problems 560 CHAPTER 602 Summary 609 Problems 611 CHAPTER 12.8.1 Polysilicon Emitter BJT 552 12.8.2 Silicon–Germanium Base Transistor 554 12.8.3 Heterojunction Bipolar Transistors 556 12.9 High Electron Mobility Transistor PART 546 12.7.1 Switching Characteristics 549 12.7.2 The Schottky-Clamped Transistor *12.8 Small-Signal Equivalent Circuit 598 Frequency Limitation Factors and Cutoff Frequency 600 13.5.1 Quantum Well Structures 603 13.5.2 Transistor Performance 604 545 12.6.1 Time-Delay Factors 545 12.6.2 Transistor Cutoff Frequency 593 Channel Length Modulation 594 Velocity Saturation Effects 596 Subthreshold and Gate Current Effects 596 Equivalent Circuit and Frequency Limitations 598 13.4.1 13.4.2 *12.5.1 Ebers–Moll Model 537 12.5.2 Gummel–Poon Model 540 12.5.3 Hybrid-Pi Model 541 12.6 Nonideal Effects 633 Photoconductor 633 Photodiode 635 PIN Photodiode 640 Avalanche Photodiode 641 Phototransistor 642 Photoluminescence and Electroluminescence 643 14.4.1 Basic Transitions 644 14.4.2 Luminescent Efficiency 645 14.4.3 Materials 646 12/13/10 6:09 PM Contents 14.5 Light Emitting Diodes 14.6 Laser Diodes 654 15.7 Summary 701 Problems 703 APPENDIX 14.6.1 Stimulated Emission and Population Inversion 655 14.6.2 Optical Cavity 657 14.6.3 Threshold Current 658 14.6.4 Device Structures and Characteristics 660 14.7 15.6.3 SCR Turn-Off 697 15.6.4 Device Structures 697 648 14.5.1 Generation of Light 648 14.5.2 Internal Quantum Efficiency 649 14.5.3 External Quantum Efficiency 650 14.5.4 LED Devices 652 Summary 661 Problems 664 ix A Selected List of Symbols 707 APPENDIX B System of Units, Conversion Factors, and General Constants 715 APPENDIX C The Periodic Table 719 CHAPTER 15 Semiconductor Microwave and Power Devices 670 15.0 15.1 15.2 15.3 15.4 Preview 670 Tunnel Diode 671 Gunn Diode 672 Impatt Diode 675 Power Bipolar Transistors Power MOSFETs The Thyristor 15.6.1 15.6.2 nea29583_fm_i-xxiv.indd ix E “Derivation” of Schrodinger’s Wave Equation 722 677 684 15.5.1 Power Transistor Structures 684 15.5.2 Power MOSFET Characteristics 685 15.5.3 Parasitic BJT 689 15.6 D Unit of Energy—The Electron Volt 720 APPENDIX 15.4.1 Vertical Power Transistor Structure 677 15.4.2 Power Transistor Characteristics 678 15.4.3 Darlington Pair Configuration 682 15.5 APPENDIX 691 The Basic Characteristics 691 Triggering the SCR 694 APPENDIX F Effective Mass Concepts 724 APPENDIX G The Error Function 729 APPENDIX H Answers to Selected Problems 730 Index 738 12/11/10 1:01 PM PREFACE PHILOSOPHY AND GOALS The purpose of the fourth edition of this book is to provide a basis for understanding the characteristics, operation, and limitations of semiconductor devices. In order to gain this understanding, it is essential to have a thorough knowledge of the physics of the semiconductor material. The goal of this book is to bring together quantum mechanics, the quantum theory of solids, semiconductor material physics, and semiconductor device physics. All of these components are vital to the understanding of both the operation of present-day devices and any future development in the field. The amount of physics presented in this text is greater than what is covered in many introductory semiconductor device books. Although this coverage is more extensive, the author has found that once the basic introductory and material physics have been thoroughly covered, the physics of the semiconductor device follows quite naturally and can be covered fairly quickly and efficiently. The emphasis on the underlying physics will also be a benefit in understanding and perhaps in developing new semiconductor devices. Since the objective of this text is to provide an introduction to the theory of semiconductor devices, there is a great deal of advanced theory that is not considered. In addition, fabrication processes are not described in detail. There are a few references and general discussions about processing techniques such as diffusion and ion implantation, but only where the results of this processing have direct impact on device characteristics. PREREQUISITES This text is intended for junior and senior undergraduates majoring in electrical engineering. The prerequisites for understanding the material are college mathematics, up to and including differential equations, basic college physics, and an introduction to electromagnetics. An introduction to modern physics would be helpful, but is not required. Also, a prior completion of an introductory course in electronic circuits is helpful, but not essential. ORGANIZATION The text is divided into three parts—Part I covers the introductory quantum physics and then moves on to the semiconductor material physics; Part II presents the physics of the fundamental semiconductor devices; and Part III deals with specialized semiconductor devices including optical, microwave, and power devices. Part I consists of Chapters 1 through 6. Chapter 1 presents an introduction to the crystal structure of solids leading to the ideal single-crystal semiconductor material. x nea29583_fm_i-xxiv.indd x 12/11/10 1:01 PM Preface xi Chapters 2 and 3 introduce quantum mechanics and the quantum theory of solids, which together provide the necessary basic physics. Chapters 4 through 6 cover the semiconductor material physics. Chapter 4 considers the physics of the semiconductor in thermal equilibrium, Chapter 5 treats the transport phenomena of the charge carriers in a semiconductor, and the nonequilibrium excess carrier characteristics are developed in Chapter 6. Understanding the behavior of excess carriers in a semiconductor is vital to the goal of understanding the device physics. Part II consists of Chapters 7 through 13. Chapter 7 treats the electrostatics of the basic pn junction and Chapter 8 covers the current–voltage, including the dc and small-signal, characteristics of the pn junction diode. Metal–semiconductor junctions, both rectifying and ohmic, and semiconductor heterojunctions are considered in Chapter 9. The basic physics of the metal–oxide–semiconductor fieldeffect transistor (MOSFET) is developed in Chapters 10 with additional concepts presented in Chapter 11. Chapter 12 develops the theory of the bipolar transistor and Chapter 13 covers the junction field-effect transistor (JFET). Once the physics of the pn junction is developed, the chapters dealing with the three basic transistors may be covered in any order—these chapters are written so as not to depend on one another. Part III consists of Chapters 14 and 15. Chapter 14 considers optical devices, such as the solar cell and light emitting diode. Finally, semiconductor microwave devices and semiconductor power devices are presented in Chapter 15. Eight appendices are included at the end of the book. Appendix A contains a selected list of symbols. Notation may sometimes become confusing, so this appendix may aid in keeping track of all the symbols. Appendix B contains the system of units, conversion factors, and general constants used throughout the text. Appendix H lists answers to selected problems. Most students will find this appendix helpful. USE OF THE BOOK The text is intended for a one-semester course at the junior or senior level. As with most textbooks, there is more material than can be conveniently covered in one semester; this allows each instructor some flexibility in designing the course to his or her own specific needs. Two possible orders of presentation are discussed later in a separate section in this preface. However, the text is not an encyclopedia. Sections in each chapter that can be skipped without loss of continuity are identified by an asterisk in both the table of contents and in the chapter itself. These sections, although important to the development of semiconductor device physics, can be postponed to a later time. The material in the text has been used extensively in a course that is required for junior-level electrical engineering students at the University of New Mexico. Slightly less than half of the semester is devoted to the first six chapters; the remainder of the semester is devoted to the pn junction, the metal–oxide–semiconductor field-effect transistor, and the bipolar transistor. A few other special topics may be briefly considered near the end of the semester. nea29583_fm_i-xxiv.indd xi 12/11/10 1:01 PM xii Preface As mentioned, although the MOS transistor is discussed prior to the bipolar transistor or junction field-effect transistor, each chapter dealing with the basic types of transistors is written to stand alone. Any one of the transistor types may be covered first. NOTES TO THE READER This book introduces the physics of semiconductor materials and devices. Although many electrical engineering students are more comfortable building electronic circuits or writing computer programs than studying the underlying principles of semiconductor devices, the material presented here is vital to an understanding of the limitations of electronic devices, such as the microprocessor. Mathematics is used extensively throughout the book. This may at times seem tedious, but the end result is an understanding that will not otherwise occur. Although some of the mathematical models used to describe physical processes may seem abstract, they have withstood the test of time in their ability to describe and predict these physical processes. The reader is encouraged to continually refer to the preview sections at the beginning of each chapter so that the objective of the chapter and the purpose of each topic can be kept in mind. This constant review is especially important in the first six chapters, dealing with the basic physics. The reader must keep in mind that, although some sections may be skipped without loss of continuity, many instructors will choose to cover these topics. The fact that sections are marked with an asterisk does not minimize the importance of these subjects. It is also important that the reader keep in mind that there may be questions still unanswered at the end of a course. Although the author dislikes the phrase, “it can be shown that . . . ,” there are some concepts used here that rely on derivations beyond the scope of the text. This book is intended as an introduction to the subject. Those questions remaining unanswered at the end of the course, the reader is encouraged to keep “in a desk drawer.” Then, during the next course in this area of concentration, the reader can take out these questions and search for the answers. ORDER OF PRESENTATION Each instructor has a personal preference for the order in which the course material is presented. Listed below are two possible scenarios. The first case, called the MOSFET approach, covers the MOS transistor before the bipolar transistor. It may be noted that the MOSFET in Chapters 10 and 11 may be covered before the pn junction diode. The second method of presentation listed, called the bipolar approach, is the classical approach. Covering the bipolar transistor immediately after discussing the pn junction diode is the traditional order of presentation. However, because the MOSFET is left until the end of the semester, time constraints may shortchange the amount of class time devoted to this important topic. Unfortunately, because of time constraints, every topic in each chapter cannot be covered in a one-semester course. The remaining topics must be left for a secondsemester course or for further study by the reader. nea29583_fm_i-xxiv.indd xii 12/11/10 1:01 PM Preface xiii MOSFET approach Chapter 1 Chapters 2, 3 Chapter 4 Chapter 5 Chapter 6 Chapter 7 Chapters 10, 11 Chapter 8 Chapter 9 Chapter 12 Crystal structure Selected topics from quantum mechanics and theory of solids Semiconductor physics Transport phenomena Selected topics from nonequilibrium characteristics The pn junction The MOS transistor The pn junction diode A brief discussion of the Schottky diode The bipolar transistor Other selected topics Bipolar approach Chapter 1 Chapters 2, 3 Chapter 4 Chapter 5 Chapter 6 Chapters 7, 8 Chapter 9 Chapter 12 Chapters 10, 11 Crystal structure Selected topics from quantum mechanics and theory of solids Semiconductor physics Transport phenomena Selected topics from nonequilibrium characteristics The pn junction and pn junction diode A brief discussion of the Schottky diode The bipolar transistor The MOS transistor Other selected topics NEW TO THE FOURTH EDITION Order of Presentation: The two chapters dealing with MOSFETs were moved ahead of the chapter on bipolar transistors. This change emphasizes the importance of the MOS transistor. Semiconductor Microwave Devices: A short section was added in Chapter 15 covering three specialized semiconductor microwave devices. New Appendix: A new Appendix F has been added dealing with effective mass concepts. Two effective masses are used in various calculations in the text. This appendix develops the theory behind each effective mass and discusses when to use each effective mass in a particular calculation. Preview Sections: Each chapter begins with a brief introduction, which then leads to a preview section given in bullet form. Each preview item presents a particular objective for the chapter. Exercise Problems: Over 100 new Exercise Problems have been added. An Exercise Problem now follows each example. The exercise is very similar to the worked example so that readers can immediately test their understanding of the material just covered. Answers are given to each exercise problem. nea29583_fm_i-xxiv.indd xiii 12/11/10 1:01 PM xiv Preface Test Your Understanding: Approximately 40 percent new Test Your Understanding problems are included at the end of many of the major sections of the chapter. These exercise problems are, in general, more comprehensive than those presented at the end of each example. These problems will also reinforce readers’ grasp of the material before they move on to the next section. End-of-Chapter Problems: There are 330 new end-of-chapter problems, which means that approximately 48 percent of the problems are new to this edition. RETAINED FEATURES OF THE TEXT ■ ■ ■ ■ ■ ■ ■ ■ ■ ■ nea29583_fm_i-xxiv.indd xiv Mathematical Rigor: The mathematical rigor necessary to more clearly understand the basic semiconductor material and device physics has been maintained. Examples: An extensive number of worked examples are used throughout the text to reinforce the theoretical concepts being developed. These examples contain all the details of the analysis or design, so the reader does not have to fill in missing steps. Summary section: A summary section, in bullet form, follows the text of each chapter. This section summarizes the overall results derived in the chapter and reviews the basic concepts developed. Glossary of important terms: A glossary of important terms follows the Summary section of each chapter. This section defines and summarizes the most important terms discussed in the chapter. Checkpoint: A checkpoint section follows the Glossary section. This section states the goals that should have been met and the abilities the reader should have gained. The Checkpoints will help assess progress before moving on to the next chapter. Review questions: A list of review questions is included at the end of each chapter. These questions serve as a self-test to help the reader determine how well the concepts developed in the chapter have been mastered. End-of-chapter problems: A large number of problems are given at the end of each chapter, organized according to the subject of each section in the chapter. Summary and Review Problems: A few problems, in a Summary and Review section, are open-ended design problems and are given at the end of most chapters. Reading list: A reading list finishes up each chapter. The references, which are at an advanced level compared with that of this text, are indicated by an asterisk. Answers to selected problems: Answers to selected problems are given in the last appendix. Knowing the answer to a problem is an aid and a reinforcement in problem solving. 12/11/10 1:01 PM Preface xv ONLINE RESOURCES A website to accompany this text is available at www.mhhe.com/neamen. The site includes the solutions manual as well as an image library for instructors. Instructors can also obtain access to C.O.S.M.O.S. for the fourth edition. C.O.S.M.O.S. is a Complete Online Solutions Manual Organization System instructors can use to create exams and assignments, create custom content, and edit supplied problems and solutions. ACKNOWLEDGMENTS I am indebted to the many students I have had over the years who have helped in the evolution of this fourth edition as well as to the previous editions of this text. I am grateful for their enthusiasm and constructive criticism. I want to thank the many people at McGraw-Hill for their tremendous support. To Peter Massar, sponsoring editor, and Lora Neyens, development editor, I am grateful for their encouragement, support, and attention to the many details of this project. I also appreciate the efforts of project managers who guided this work through its final phase toward publication. This effort included gently, but firmly, pushing me through proofreading. Let me express my continued appreciation to those reviewers who read the manuscripts of the first three editions in its various forms and gave constructive criticism. I also appreciate the efforts of accuracy checkers who worked through the new problem solutions in order to minimize any errors I may have introduced. Finally, my thanks go out to those individuals who have reviewed the book prior to this new edition being published. Their contributions and suggestions for continued improvement are very valuable. REVIEWERS FOR THE FOURTH EDITION The following reviewers deserve thanks for their constructive criticism and suggestions for the fourth edition of this book. Sandra Selmic, Louisiana Tech University Terence Brown, Michigan State University Timothy Wilson, Oklahoma State University Lili He, San Jose State University Jiun Liou, University of Central Florida Michael Stroscio, University of Illinois-Chicago Andrei Sazonov, University of Waterloo nea29583_fm_i-xxiv.indd xv 12/11/10 1:01 PM xvi Preface McGRAW-HILL CREATE™ Craft your teaching resources to match the way you teach! With McGraw-Hill Create™, www.mcgrawhillcreate.com, you can easily rearrange chapters, combine material from other content sources, and quickly upload content you have written like your course syllabus or teaching notes. Find the content you need in Create by searching through thousands of leading McGraw-Hill textbooks. Arrange your book to fit your teaching style. Create even allows you to personalize your book’s appearance by selecting the cover and adding your name, school, and course information. Order a Create book and you’ll receive a complimentary print review copy in 3–5 business days or a complimentary electronic review copy (eComp) via email in minutes. Go to www.mcgrawhillcreate.com today and register to experience how McGraw-Hill Create™ empowers you to teach your students your way. MCGRAW-HILL HIGHER EDUCATION AND BLACKBOARD HAVE TEAMED UP. Blackboard, the Web-based course-management system, has partnered with McGraw-Hill to better allow students and faculty to use online materials and activities to complement face-to-face teaching. Blackboard features exciting social learning and teaching tools that foster more logical, visually impactful and active learning opportunities for students. You’ll transform your closed-door classrooms into communities where students remain connected to their educational experience 24 hours a day. This partnership allows you and your students access to McGraw-Hill’s Create™ right from within your Blackboard course—all with one single sign-on. McGraw-Hill and Blackboard can now offer you easy access to industry leading technology and content, whether your campus hosts it, or we do. Be sure to ask your local McGraw-Hill representative for details. ELECTRONIC TEXTBOOK OPTIONS E-textbooks are an innovative way for students to save money and create a greener environment at the same time. An e-book can save students about half the cost of a traditional textbook and offers unique features like a powerful search engine, highlighting, and the ability to share notes with classmates using e-books. McGraw-Hill offers this text as an e-book. To talk about the e-book options, contact your McGraw-Hill sales rep or visit the site www.coursesmart.com to learn more. nea29583_fm_i-xxiv.indd xvi 12/11/10 1:01 PM P R O L O G U E Semiconductors and the Integrated Circuit PREVIEW W e often hear that we are living in the information age. Large amounts of information can be obtained via the Internet, for example, and can be obtained very quickly over long distances via satellite communications systems. The information technologies are based upon digital and analog electronic systems, with the transistor and integrated circuit (IC) being the foundation of these remarkable capabilities. Wireless communication systems, including printers, faxes, laptop computers, ipods, and of course the cell phones are big users of today’s IC products. The cell phone is not just a telephone any longer, but includes e-mail services and video cameras, for example. Today, a relatively small laptop computer has more computing capability than the equipment used to send a man to the moon a few decades ago. The semiconductor electronics field continues to be a fast-changing one, with thousands of technical papers published and many new electronic devices developed each year. ■ HISTORY The semiconductor device has a fairly long history, although the greatest explosion of IC technology has occured during the last two or three decades.1 The metal– semiconductor contact dates back to the early work of Braun in 1874, who discovered the asymmetric nature of electrical conduction between metal contacts and semiconductors, such as copper, iron, and lead sulfide. These devices were used as detectors in early experiments on radio. In 1906, Pickard took out a patent for a point contact 1 This brief introduction is intended to give a flavor of the history of the semiconductor device and integrated circuit. Thousands of engineers and scientists have made significant contributions to the development of semiconductor electronics—the few events and names mentioned here are not meant to imply that these are the only significant events or people involved in the semiconductor history. xvii nea29583_pro_xvii-xxiv.indd xvii 12/11/10 1:18 PM xviii Prolouge Compliments of Texas Instruments Incorporated nea29583_pro_xvii-xxiv.indd xviii 12/11/10 1:18 PM Prolouge xix detector using silicon and, in 1907, Pierce published rectification characteristics of diodes made by sputtering metals onto a variety of semiconductors. By 1935, selenium rectifiers and silicon point contact diodes were available for use as radio detectors. A significant advance in our understanding of the metal– semiconductor contact was aided by developments in semiconductor physics. In 1942, Bethe developed the thermionic-emission theory, according to which the current is determined by the process of emission of electrons into the metal rather than by drift or diffusion. With the development of radar, the need for better and more reliable detector diodes and mixers increased. Methods of achieving high-purity silicon and germanium were developed during this time and germanium diodes became a key component in radar systems during the Second World War. Another big breakthrough came in December 1947 when the first transistor was constructed and tested at Bell Telephone Laboratories by William Shockley, John Bardeen, and Walter Brattain. This first transistor was a point contact device and used polycrystalline germanium. The transistor effect was soon demonstrated in silicon as well. A significant improvement occurred at the end of 1949 when single-crystal material was used rather than the polycrystalline material. The single crystal yields uniform and improved properties throughout the whole semiconductor material. The next significant step in the development of the transistor was the use of the diffusion process to form the necessary junctions. This process allowed better control of the transistor characteristics and yielded higher-frequency devices. The diffused mesa transistor was commercially available in germanium in 1957 and in silicon in 1958. The diffusion process also allowed many transistors to be fabricated on a single silicon slice, so the cost of these devices decreased. THE INTEGRATED CIRCUIT (IC) The transistor led to a revolution in electronics since it is smaller and more reliable than vacuum tubes used previously. The circuits at that time were discrete in that each element had to be individually connected by wires to form the circuit. The integrated circuit has led to a new revolution in electronics that was not possible with discrete devices. Integration means that complex circuits, consisting of millions of devices, can be fabricated on a single chip of semiconductor material. The first IC was fabricated in February of 1959 by Jack Kilby of Texas Instruments. In July 1959, a planar version of the IC was independently developed by Robert Noyce of Fairchild. The first integrated circuits incorporated bipolar transistors. Practical MOS transistors were then developed in the mid-1960s and 1970s. The MOS technologies, especially CMOS, have become a major focus for IC design and development. Silicon is the main semiconductor material, while gallium arsenide and other compound semiconductor materials are used for optical devices and for special applications requiring very high frequency devices. Since the first IC, very sophisticated and complex circuits have been designed and fabricated. A single silicon chip may be on the order of 1 square centimeter and some ICs may have more than a hundred terminals. An IC can contain the arithmetic, logic, and memory functions on a single chip—the primary example of this type of IC nea29583_pro_xvii-xxiv.indd xix 12/11/10 1:18 PM xx Prolouge is the microprocessor. Integration means that circuits can be miniaturized for use in satellites and laptop computers where size, weight, and power are critical parameters. An important advantage of ICs is the result of devices being fabricated very close to each other. The time delay of signals between devices is short so that highfrequency and high-speed circuits are now possible with ICs that were not practical with discrete circuits. In high-speed computers, for example, the logic and memory circuits can be placed very close to each other to minimize time delays. In addition, parasitic capacitance and inductance between devices are reduced which also provides improvement in the speed of the system. Intense research on silicon processing and increased automation in design and manufacturing have led to lower costs, higher fabrication yields, and greater reliability of integrated circuits. FABRICATION The integrated circuit is a direct result of the development of various processing techniques needed to fabricate the transistor and interconnect lines on the single chip. The total collection of these processes for making an IC is called a technology. The following few paragraphs provide an introduction to a few of these processes. This introduction is intended to provide the reader with some of the basic terminology used in processing. Thermal Oxidation A major reason for the success of silicon ICs is the fact that an excellent native oxide, SiO2, can be formed on the surface of silicon. This oxide is used as a gate insulator in the MOSFET and is also used as an insulator, known as the field oxide, between devices. Metal interconnect lines that connect various devices can be placed on top of the field oxide. Most other semiconductors do not form native oxides that are of sufficient quality to be used in device fabrication. Silicon will oxidize at room temperature in air forming a thin native oxide of approximately 25 Å thick. However, most oxidations are done at elevated temperatures since the basic process requires that oxygen diffuse through the existing oxide to the silicon surface where a reaction can occur. A schematic of the oxidation process is shown in Figure 0.1. Oxygen diffuses across a stagnant gas layer directly adjacent SiO2 Gas Silicon Diffusion of O2 Stagnant gas layer Diffusion of O2 through existing oxide to silicon surface Figure 0.1 | Schematic of the oxidation process. nea29583_pro_xvii-xxiv.indd xx 12/11/10 1:18 PM Prolouge xxi UV source Photomask Glass UV-absorbing material Photoresist Silicon Figure 0.2 | Schematic showing the use of a photomask. to the oxide surface and then diffuses through the existing oxide layer to the silicon surface where the reaction between O2 and Si forms SiO2. Because of this reaction, silicon is actually consumed from the surface of the silicon. The amount of silicon consumed is approximately 44 percent of the thickness of the final oxide. Photomasks and Photolithography The actual circuitry on each chip is created through the use of photomasks and photolithography. The photomask is a physical representation of a device or a portion of a device. Opaque regions on the mask are made of an ultraviolet-light-absorbing material. A photosensitive layer, called photoresist, is first spread over the surface of the semiconductor. The photoresist is an organic polymer that undergoes chemical change when exposed to ultraviolet light. The photoresist is exposed to ultraviolet light through the photomask as indicated in Figure 0.2. The photoresist is then developed in a chemical solution. The developer is used to remove the unwanted portions of the photoresist and generate the appropriate patterns on the silicon. The photomasks and photolithography process is critical in that it determines how small the devices can be made. Instead of using ultraviolet light, electrons and x-rays can also be used to expose the photoresist. Etching After the photoresist pattern is formed, the remaining photoresist can be used as a mask, so that the material not covered by the photoresist can be etched. Plasma etching is now the standard process used in IC fabrication. Typically, an etch gas such as chlorofluorocarbons is injected into a low-pressure chamber. A plasma is created by applying a radio-frequency voltage between cathode and anode terminals. The silicon wafer is placed on the cathode. Positively charged ions in the plasma are accelerated toward the cathode and bombard the wafer normal to the surface. The actual chemical and physical reaction at the surface is complex, but the net result is that silicon can be etched anisotropically in very selected regions of the wafer. If photoresist is applied on the surface of silicon dioxide, then the silicon dioxide can also be etched in a similar way. Diffusion A thermal process that is used extensively in IC fabrication is diffusion. Diffusion is the process by which specific types of “impurity” atoms can be introduced into the silicon material. This doping process changes the conductivity type of the silicon so that pn junctions can be formed. (The pn junction is a basic building block of semiconductor devices.) Silicon wafers are oxidized to form a layer of nea29583_pro_xvii-xxiv.indd xxi 12/11/10 1:18 PM xxii Prolouge silicon dioxide, and windows are opened in the oxide in selected areas using photolithography and etching as just described. The wafers are then placed in a high-temperature furnace (about 1100⬚C) and dopant atoms such as boron or phosphorus are introduced. The dopant atoms gradually diffuse or move into the silicon due to a density gradient. Since the diffusion process requires a gradient in the concentration of atoms, the final concentration of diffused atoms is nonlinear, as shown in Figure 0.3. When the wafer is removed from the furnace and the wafer temperature returns to room temperature, the diffusion coefficient of the dopant atoms is essentially zero so that the dopant atoms are then fixed in the silicon material. Doping concentration Ion Implantation A fabrication process that is an alternative to high-temperature diffusion is ion implantation. A beam of dopant ions is accelerated to a high energy and is directed at the surface of a semiconductor. As the ions enter the silicon, they collide with silicon atoms and lose energy and finally come to rest at some depth within the crystal. Since the collision process is statistical in nature, there is a distribution in the depth of penetration of the dopant ions. Figure 0.4 shows such an example of the implantation of boron into silicon at a particular energy. Two advantages of the ion implantation process compared to diffusion are (1) the ion implantation process is a low-temperature process and (2) very well Diffused impurities Background doping Surface Distance Doping concentration Figure 0.3 | Final concentration of diffused impurities into the surface of a semiconductor. Surface Rp Distance (Projected range) Figure 0.4 | Final concentration of ion-implanted boron into silicon. nea29583_pro_xvii-xxiv.indd xxii 12/11/10 1:18 PM Prolouge xxiii defined doping layers can be achieved. Photoresist layers or layers of oxide can be used to block the penetration of dopant atoms so that ion implantation can occur in very selected regions of the silicon. One disadvantage of ion implantation is that the silicon crystal is damaged by the penetrating dopant atoms because of collisions between the incident dopant atoms and the host silicon atoms. However, most of the damage can be removed by thermal annealing the silicon at an elevated temperature. The thermal annealing temperature, however, is normally much less that the diffusion process temperature. Metallization, Bonding, and Packaging After the semiconductor devices have been fabricated by the processing steps discussed, they need to be connected to each other to form the circuit. Metal films are generally deposited by a vapor deposition technique, and the actual interconnect lines are formed using photolithography and etching. In general, a protective layer of silicon nitride is finally deposited over the entire chip. The individual integrated circuit chips are separated by scribing and breaking the wafer. The integrated circuit chip is then mounted in a package. Lead bonders are finally used to attach gold or aluminum wires between the chip and package terminals. Summary: Simplified Fabrication of a pn Junction Figure 0.5 shows the basic steps in forming a pn junction. These steps involve some of the processing described in the previous paragraphs. PR SiO2 SiO2 n type n 1. Start with n-type substrate UV light 2. Oxidize surface n 3. Apply photoresist over SiO2 Photomask Exposed PR removed SiO2 etched n n n 3. Expose photoresist through photomask 4. Remove exposed photoresist 5. Etch exposed SiO2 Ion implant or diffuse p regions Apply Al p n p 6. Ion implant or diffuse boron into silicon Al contacts n 7. Remove PR and sputter Al on surface p n p 8. Apply PR, photomask, and etch to form Al contacts over p regions Figure 0.5 | The basic steps in forming a pn junction. nea29583_pro_xvii-xxiv.indd xxiii 12/11/10 1:18 PM xxiv Prolouge READING LIST 1. 2. 3. 4. 5. 6. nea29583_pro_xvii-xxiv.indd xxiv Campbell, S. A. The Science and Engineering of Microelectronic Fabrication. 2nd ed. New York: Oxford University Press, 2001. Ghandhi, S. K. VLSI Fabrication Principles: Silicon and Gallium Arsenide. New York: John Wiley and Sons, 1983. Rhoderick, E. H. Metal-Semiconductor Contacts. Oxford: Clarendon Press, 1978. Runyan, W. R., and K. E. Bean. Semiconductor Integrated Circuit Processing Technology. Reading, MA: Addison-Wesley, 1990. Torrey, H. C., and C. A. Whitmer. Crystal Rectifiers. New York: McGraw-Hill, 1948. Wolf, S., and R. N. Tauber. Silicon Processing for the VLSI Era, 2nd ed. Sunset Beach, CA: Lattice Press, 2000. 12/11/10 1:18 PM C 1 H A P T E R The Crystal Structure of Solids T his text deals with the electrical properties and characteristics of semiconductor materials and devices. The electrical properties of solids are therefore of primary interest. The semiconductor is in general a single-crystal material. The electrical properties of a single-crystal material are determined not only by the chemical composition but also by the arrangement of atoms in the solid; this being true, a brief study of the crystal structure of solids is warranted. The formation, or growth, of the single-crystal material is an important part of semiconductor technology. A short discussion of several growth techniques is included in this chapter to provide the reader with some of the terminology that describes semiconductor device structures. ■ 1.0 | PREVIEW In this chapter, we will: ■ Describe three classifications of solids—amorphous, polycrystalline, and single crystal. ■ Discuss the concept of a unit cell. ■ Describe three simple crystal structures and determine the volume and surface density of atoms in each structure. ■ Describe the diamond crystal structure. ■ Briefly discuss several methods of forming single-crystal semiconductor materials. 1.1 | SEMICONDUCTOR MATERIALS Semiconductors are a group of materials having conductivities between those of metals and insulators. Two general classifications of semiconductors are the elemental semiconductor materials, found in group IV of the periodic table, and the compound semiconductor materials, most of which are formed from special combinations of group III and group V elements. Table 1.1 shows a portion of the periodic table in 1 nea29583_ch01_001-024.indd 1 12/11/10 9:46 AM 2 CHAPTER 1 The Crystal Structure of Solids Table 1.1 | A portion of the periodic table III IV V Table 1.2 | A list of some semiconductor materials Elemental semiconductors 5 6 B Boron C Carbon 13 14 15 Al Aluminum Si Silicon P Phosphorus 31 32 33 Ga Gallium Ge Germanium As Arsenic Si Ge 49 51 In Indium Sb Antimony Silicon Germanium Compound semiconductors AlP AlAs GaP GaAs InP Aluminum phosphide Aluminum arsenide Gallium phosphide Gallium arsenide Indium phosphide which the more common semiconductors are found and Table 1.2 lists a few of the semiconductor materials. (Semiconductors can also be formed from combinations of group II and group VI elements, but in general these will not be considered in this text.) The elemental materials, those that are composed of single species of atoms, are silicon and germanium. Silicon is by far the most common semiconductor used in integrated circuits and will be emphasized to a great extent. The two-element, or binary, compounds such as gallium arsenide or gallium phosphide are formed by combining one group III and one group V element. Gallium arsenide is one of the more common of the compound semiconductors. Its good optical properties make it useful in optical devices. GaAs is also used in specialized applications in which, for example, high speed is required. We can also form a three-element, or ternary, compound semiconductor. An example is AlxGa1xAs, in which the subscript x indicates the fraction of the lower atomic number element component. More complex semiconductors can also be formed that provide flexibility when choosing material properties. 1.2 | TYPES OF SOLIDS Amorphous, polycrystalline, and single crystals are the three general types of solids. Each type is characterized by the size of an ordered region within the material. An ordered region is a spatial volume in which atoms or molecules have a regular geometric arrangement or periodicity. Amorphous materials have order only within a few atomic or molecular dimensions, while polycrystalline materials have a high degree of order over many atomic or molecular dimensions. These ordered regions, or single-crystal regions, vary in size and orientation with respect to one another. The single-crystal regions are called grains and are separated from one another by grain boundaries. Single-crystal materials, ideally, have a high degree of order, or regular geometric periodicity, throughout the entire volume of the material. The advantage of a single-crystal material is that, in general, its electrical properties are superior nea29583_ch01_001-024.indd 2 12/11/10 9:46 AM 1.3 (a) (b) Space Lattices 3 (c) Figure 1.1 | Schematics of three general types of crystals: (a) amorphous, (b) polycrystalline, (c) single. to those of a nonsingle-crystal material, since grain boundaries tend to degrade the electrical characteristics. Two-dimensional representations of amorphous, polycrystalline, and single-crystal materials are shown in Figure 1.1. 1.3 | SPACE LATTICES Our primary emphasis in this text will be on the single-crystal material with its regular geometric periodicity in the atomic arrangement. A representative unit, or a group of atoms, is repeated at regular intervals in each of the three dimensions to form the single crystal. The periodic arrangement of atoms in the crystal is called the lattice. 1.3.1 Primitive and Unit Cell We can represent a particular atomic array by a dot that is called a lattice point. Figure 1.2 shows an infinite two-dimensional array of lattice points. The simplest means of repeating an atomic array is by translation. Each lattice point in Figure 1.2 can be translated a distance a1 in one direction and a distance b1 in a second noncolinear direction to generate the two-dimensional lattice. A third noncolinear translation will produce the three-dimensional lattice. The translation directions need not be perpendicular. Since the three-dimensional lattice is a periodic repetition of a group of atoms, we do not need to consider the entire lattice, but only a fundamental unit that is being repeated. A unit cell is a small volume of the crystal that can be used to reproduce the entire crystal. A unit cell is not a unique entity. Figure 1.3 shows several possible unit cells in a two-dimensional lattice. The unit cell A can be translated in directions a2 and b2, the unit cell B can be translated in directions a3 and b3, and the entire two-dimensional lattice can be constructed by the translations of either of these unit cells. The unit cells C and D in Figure 1.3 can also be used to construct the entire lattice by using the appropriate translations. This discussion of two-dimensional unit cells can easily be extended to three dimensions to describe a real single-crystal material. nea29583_ch01_001-024.indd 3 12/11/10 9:46 AM 4 CHAPTER 1 The Crystal Structure of Solids b2 A a2 b3 B b1 b4 b1 a1 D a3 a4 C a1 Figure 1.2 | Two-dimensional representation of a single-crystal lattice. Figure 1.3 | Two-dimensional representation of a single-crystal lattice showing various possible unit cells. A primitive cell is the smallest unit cell that can be repeated to form the lattice. In many cases, it is more convenient to use a unit cell that is not a primitive cell. Unit cells may be chosen that have orthogonal sides, for example, whereas the sides of a primitive cell may be nonorthogonal. A generalized three-dimensional unit cell is shown in Figure 1.4. The _relation_ _ ship between this cell and the lattice is characterized by three vectors a, b, and c, which need not be perpendicular and which may or may not be equal in length. Every equivalent lattice point in the three-dimensional crystal can be found using the vector _ _ _ _ r pa qb sc (1.1) where p, q, and s are integers. Since the location of the origin is arbitrary, we will let _ _ p, q, and s be positive integers for simplicity. The magnitudes of the vectors a, b, and _ c are the lattice constants of the unit cell. 1.3.2 Basic Crystal Structures Before we discuss the semiconductor crystal, let us consider three crystal structures and determine some of the basic characteristics of these crystals. Figure 1.5 shows the simple cubic, body-centered cubic, and face-centered cubic structures. For these _ _ _ simple structures, we may choose unit cells such that the general vectors a, b, and c c b a Figure 1.4 | A generalized primitive unit cell. nea29583_ch01_001-024.indd 4 12/11/10 9:46 AM 1.3 a a a a (a) 5 a a a Space Lattices a a (b) (c) Figure 1.5 | Three lattice types: (a) simple cubic, (b) body-centered cubic, (c) face-centered cubic. are perpendicular to each other and the lengths are equal. The lattice constant of each unit cell in Figure 1.5 is designated as “a.” The simple cubic (sc) structure has an atom located at each corner; the body-centered cubic (bcc) structure has an additional atom at the center of the cube; and the face-centered cubic (fcc) structure has additional atoms on each face plane. By knowing the crystal structure of a material and its lattice dimensions, we can determine several characteristics of the crystal. For example, we can determine the volume density of atoms. Objective: Find the volume density of atoms in a crystal. EXAMPLE 1.1 Consider a single-crystal material that is a body-centered cubic, as shown in Figure 1.5b, with a lattice constant a 5 Å 5 108 cm. A corner atom is shared by eight unit cells that meet at each corner so that each corner atom effectively contributes one-eighth of its volume to each unit cell. The eight corner atoms then contribute an equivalent of one atom to the unit cell. If we add the body-centered atom to the corner atoms, each unit cell contains an equivalent of two atoms. ■ Solution 1812 The number of atoms per unit cell is __ 8 The volume density of atoms is then found as # atoms per unit cell Volume Density _________________ volume of unit cell So 2 __________ 2 Volume Density __ 1.6 1022 atoms/cm3 a3 (5 108)3 ■ EXERCISE PROBLEM Ex 1.1 The lattice constant of a face-centered cubic lattice is 4.25 Å. Determine the (a) effective number of atoms per unit cell and (b) volume density of atoms. [Ans. (a) 4; (b) 5.21 1022 cm3] nea29583_ch01_001-024.indd 5 12/11/10 9:46 AM 6 CHAPTER 1 1.3.3 The Crystal Structure of Solids Crystal Planes and Miller Indices Since real crystals are not infinitely large, they eventually terminate at a surface. Semiconductor devices are fabricated at or near a surface, so the surface properties may influence the device characteristics. We would like to be able to describe these surfaces in terms of the lattice. Surfaces, or planes through the crystal, can be _ _ _ described by first considering the intercepts of the plane along the a, b, and c axes used to describe the lattice. EXAMPLE 1.2 Objective: Describe the plane shown in Figure 1.6. (The lattice points in Figure 1.6 are _ _ _ shown along the a, b, and c axes only.) 1c 2b 3a Figure 1.6 | A representative crystallattice plane. ■ Solution From Equation (1.1), the intercepts of the plane correspond to p 3, q 2, and s 1. Now write the reciprocals of the intercepts, which gives ( __31, __12, __11 ) Multiply by the lowest common denominator, which in this case is 6, to obtain (2, 3, 6). The plane in Figure 1.6 is then referred to as the (236) plane. The integers are referred to as the Miller indices. We will refer to a general plane as the (hkl) plane. ■ Comment We can show that the same three Miller indices are obtained for any plane that is parallel to the one shown in Figure 1.6. Any parallel plane is entirely equivalent to any other. ■ EXERCISE PROBLEM nea29583_ch01_001-024.indd 6 Describe the lattice plane shown in Figure 1.7. [Ans. (211) plane] Ex 1.2 12/11/10 9:46 AM 1.3 Space Lattices 7 2c 2b a Figure 1.7 | Figure for Exercise Problem Ex 1.2. Three planes that are commonly considered in_a cubic crystal are shown in Fig_ ure 1.8. The plane in Figure 1.8a is parallel to the b and c axes so the intercepts are given as p 1, q , and s . Taking the reciprocal, we obtain the Miller indices as (1, 0, 0), so the plane shown in Figure 1.8a is referred to as the (100) plane. Again, any plane parallel to the one shown in Figure 1.8a and separated by an integral number of lattice constants is equivalent and is referred to as the (100) plane. One advantage to taking the reciprocal of the intercepts to obtain the Miller indices is that the use of infinity is avoided when describing a plane that is parallel to an axis. If we were to describe a plane passing through the origin of our system, we would obtain infinity as one or more of the Miller indices after taking the reciprocal of the intercepts. However, the location of the origin of our system is entirely arbitrary and so, by translating the origin to another equivalent lattice point, we can avoid the use of infinity in the set of Miller indices. For the simple cubic structure, the body-centered cubic, and the face-centered cubic, there is a high degree of symmetry. The axes can be rotated by 90° in each c– c– c– – b – b a– a– (a) – b a– (b) (c) Figure 1.8 | Three lattice planes: (a) (100) plane, (b) (110) plane, (c) (111) plane. nea29583_ch01_001-024.indd 7 12/11/10 9:46 AM 8 CHAPTER 1 The Crystal Structure of Solids of the three dimensions and each lattice point can again be described by Equation (1.1) as _ _ _ _ r pa qb sc (1.1) Each face plane of the cubic structure shown in Figure 1.8a is entirely equivalent. These planes are grouped together and are referred to as the {100} set of planes. We may also consider the planes shown in Figures 1.8b and 1.8c. The intercepts of the plane shown in Figure 1.8b are p 1, q 1, and s . The Miller indices are found by taking the reciprocal of these intercepts and, as a result, this plane is referred to as the (110) plane. In a similar way, the plane shown in Figure 1.8c is referred to as the (111) plane. One characteristic of a crystal that can be determined is the distance between nearest equivalent parallel planes. Another characteristic is the surface concentration of atoms, number per square centimeter (#/cm2), that are cut by a particular plane. Again, a single-crystal semiconductor is not infinitely large and must terminate at some surface. The surface density of atoms may be important, for example, in determining how another material, such as an insulator, will “fit” on the surface of a semiconductor material. EXAMPLE 1.3 Objective: Calculate the surface density of atoms on a particular plane in a crystal. Consider the body-centered cubic structure and the (110) plane shown in Figure 1.9a. Assume the atoms can be represented as hard spheres with the closest atoms touching each other. Assume the lattice constant is a1 5 Å. Figure 1.9b shows how the atoms are cut by the (110) plane. The atom at each corner is shared by four similar equivalent lattice planes, so each corner atom effectively contributes one-fourth of its area to this lattice plane as indicated in the figure. The four corner atoms then effectively contribute one atom to this lattice plane. The atom in the center is completely enclosed in the lattice plane. There is no other equivalent plane that –c a1 2 a1 a1 – b a1 a1 a– (a) (b) Figure 1.9 | (a) The (110) plane in a body-centered cubic and (b) the atoms cut by the (110) plane in a body-centered cubic. nea29583_ch01_001-024.indd 8 12/11/10 9:46 AM 1.3 Space Lattices 9 cuts the center atom and the corner atoms, so the entire center atom is included in the number of atoms in the crystal plane. The lattice plane in Figure 1.9b, then, contains two atoms. ■ Solution 1412 The number of atoms per lattice plane is __ 4 The surface density of atoms is then found as # of atoms per lattice plane Surface Density _______________________ area of lattice plane So 2 2 __ ____________ __ Surface Density _________ (a1)(a1冑2 ) (5 10− 8)2冑 2 5.66 1014 atoms/cm2 ■ Comment The surface density of atoms is a function of the particular crystal plane in the lattice and generally varies from one crystal plane to another. ■ EXERCISE PROBLEM Ex 1.3 The lattice constant of a face-centered-cubic structure is 4.25 Å. Calculate the surface density of atoms for a (a) (100) plane and (b) (110) plane. [Ans. (a) 1.11 1015 cm2; (b) 7.83 1014 cm2] 1.3.4 Directions in Crystals In addition to describing crystal planes in a lattice, we may want to describe a particular direction in the crystal. The direction can be expressed as a set of three integers that are the components of a vector in that direction. For example, the body diagonal in a simple cubic lattice is composed of vector components 1, 1, 1. The body diagonal is then described as the [111] direction. The brackets are used to designate direction as distinct from the parentheses used for the crystal planes. The three basic directions and the associated crystal planes for the simple cubic structure are shown in Figure 1.10. Note that in the simple cubic lattices, the [hkl] direction is perpendicular to the (hkl) plane. This perpendicularity may not be true in noncubic lattices. TEST YOUR UNDERSTANDING TYU 1.1 The volume density of atoms for a simple cubic lattice is 4 10 22 cm3. Assume that the atoms are hard spheres with each atom touching its nearest neighbor. Determine the lattice constant and the radius of the atom. TYU 1.2 Consider a simple cubic structure with a lattice constant of a 4.65 Å. Determine the surface density of atoms in the (a) (100) plane, (b) (110) plane, and (c) (111) plane. TYU 1.3 (a) Determine the distance between nearest (100) planes in a simple cubic lattice with a lattice constant of a 4.83 Å. (b) Repeat part (a) for the (110) plane. (Ans. a 2.92 Å, r 1.46 Å) [Ans. (a) 4.62 10 14 cm2; (b) 3.27 10 14 cm2; (c) 2.67 1014 cm2] [Ans. (a) 4.83 Å; (b) 3.42 Å] nea29583_ch01_001-024.indd 9 12/11/10 9:46 AM 10 CHAPTER 1 The Crystal Structure of Solids –c –c –c [111] – b – b – b [110] [100] a– a– (a) a– (b) (c) Figure 1.10 | Three lattice directions and planes: (a) (100) plane and [100] direction, (b) (110) plane and [110] direction, (c) (111) plane and [111] direction. 1.4 | THE DIAMOND STRUCTURE As already stated, silicon is the most common semiconductor material. Silicon is referred to as a group IV element and has a diamond crystal structure. Germanium is also a group IV element and has the same diamond structure. A unit cell of the diamond structure, shown in Figure 1.11, is more complicated than the simple cubic structures that we have considered up to this point. We may begin to understand the diamond lattice by considering the tetrahedral structure shown in Figure 1.12. This structure is basically a body-centered cubic with four of the corner atoms missing. Every atom in the tetrahedral structure has four nearest neighbors and it is this structure that is the basic building block of the diamond lattice. a Figure 1.11 | The diamond structure. nea29583_ch01_001-024.indd 10 a/2 Figure 1.12 | The tetrahedral structure of closest neighbors in the diamond lattice. 12/11/10 9:46 AM 1.4 The Diamond Structure 11 a a (a) (b) Figure 1.13 | Portions of the diamond lattice: (a) bottom half and (b) top half. There are several ways to visualize the diamond structure. One way to gain a further understanding of the diamond lattice is by considering Figure 1.13. Figure 1.13a shows two body-centered cubic, or tetrahedral, structures diagonally adjacent to each other. The open circles represent atoms in the lattice that are generated when the structure is translated to the right or left, one lattice constant, a. Figure 1.13b represents the top half of the diamond structure. The top half again consists of two tetrahedral structures joined diagonally, but which are at 90° with respect to the bottom-half diagonal. An important characteristic of the diamond lattice is that any atom within the diamond structure will have four nearest neighboring atoms. We will note this characteristic again in our discussion of atomic bonding in the next section. The diamond structure refers to the particular lattice in which all atoms are of the same species, such as silicon or germanium. The zincblende (sphalerite) structure differs from the diamond structure only in that there are two different types of atoms in the lattice. Compound semiconductors, such as gallium arsenide, have the zincblende structure shown in Figure 1.14. The important feature of both the diamond and the zincblende structures is that the atoms are joined together to form a tetrahedron. Figure 1.15 shows the basic tetrahedral structure of GaAs in which each Ga atom has four nearest As neighbors and each As atom has four nearest Ga neighbors. This figure also begins to show the interpenetration of two sublattices that can be used to generate the diamond or zincblende lattice. TEST YOUR UNDERSTANDING TYU 1.4 Consider the diamond unit cell shown in Figure 1.11. Determine the (a) number of corner atoms, (b) number of face-centered atoms, and (c) number of atoms totally enclosed in the unit cell. TYU 1.5 The lattice constant of silicon is 5.43 Å. Calculate the volume density of silicon atoms. [Ans. (a) 8; (b) 6; (c) 4] (Ans. 5 10 22 cm3) nea29583_ch01_001-024.indd 11 12/11/10 9:46 AM 12 CHAPTER 1 The Crystal Structure of Solids Ga a As Figure 1.14 | The zincblende (sphalerite) lattice of GaAs. Figure 1.15 | The tetrahedral structure of closest neighbors in the zincblende lattice. 1.5 | ATOMIC BONDING We have been considering various single-crystal structures. The question arises as to why one particular crystal structure is favored over another for a particular assembly of atoms. A fundamental law of nature is that the total energy of a system in thermal equilibrium tends to reach a minimum value. The interaction that occurs between atoms to form a solid and to reach the minimum total energy depends on the type of atom or atoms involved. The type of bond, or interaction, between atoms, then, depends on the particular atom or atoms in the crystal. If there is not a strong bond between atoms, they will not “stick together” to create a solid. The interaction between atoms can be described by quantum mechanics. Although an introduction to quantum mechanics is presented in the next chapter, the quantum-mechanical description of the atomic bonding interaction is still beyond the scope of this text. We can nevertheless obtain a qualitative understanding of how various atoms interact by considering the valence, or outermost, electrons of an atom. The atoms at the two extremes of the periodic table (excepting the inert elements) tend to lose or gain valence electrons, thus forming ions. These ions then essentially have complete outer energy shells. The elements in group I of the periodic table tend to lose their one electron and become positively charged, while the elements in group VII tend to gain an electron and become negatively charged. These oppositely charged ions then experience a coulomb attraction and form a bond referred to as an ionic bond. If the ions were to get too close, a repulsive force would become dominant, so an equilibrium distance results between these two ions. In a crystal, negatively charged ions tend to be surrounded by positively charged ions and positively charged ions tend to be surrounded by negatively charged ions, so a periodic array of the atoms is formed to create the lattice. A classic example of ionic bonding is sodium chloride. nea29583_ch01_001-024.indd 12 12/11/10 9:46 AM 1.5 Atomic Bonding 13 Si Si Si Si Si Si Si Si Si H H H H (b) Si Figure 1.16 | Representation of (a) hydrogen valence electrons and (b) covalent bonding in a hydrogen molecule. (a) (a) (b) Figure 1.17 | Representation of (a) silicon valence electrons and (b) covalent bonding in the silicon crystal. The interaction of atoms tends to form closed valence shells such as we see in ionic bonding. Another atomic bond that tends to achieve closed-valence energy shells is covalent bonding, an example of which is found in the hydrogen molecule. A hydrogen atom has one electron and needs one more electron to complete the lowest energy shell. A schematic of two noninteracting hydrogen atoms, and the hydrogen molecule with the covalent bonding, is shown in Figure 1.16. Covalent bonding results in electrons being shared between atoms, so that in effect the valence energy shell of each atom is full. Atoms in group IV of the periodic table, such as silicon and germanium, also tend to form covalent bonds. Each of these elements has four valence electrons and needs four more electrons to complete the valence energy shell. If a silicon atom, for example, has four nearest neighbors, with each neighbor atom contributing one valence electron to be shared, then the center atom will in effect have eight electrons in its outer shell. Figure 1.17a schematically shows five noninteracting silicon atoms with the four valence electrons around each atom. A two-dimensional representation of the covalent bonding in silicon is shown in Figure 1.17b. The center atom has eight shared valence electrons. A significant difference between the covalent bonding of hydrogen and of silicon is that, when the hydrogen molecule is formed, it has no additional electrons to form additional covalent bonds, while the outer silicon atoms always have valence electrons available for additional covalent bonding. The silicon array may then be formed into an infinite crystal, with each silicon atom having four nearest neighbors and eight shared electrons. The four nearest neighbors in silicon forming the covalent bond correspond to the tetrahedral structure and the diamond lattice, which were shown in Figures 1.12 and 1.11 respectively. Atomic bonding and crystal structure are obviously directly related. The third major atomic bonding scheme is referred to as metallic bonding. Group I elements have one valence electron. If two sodium atoms (Z 11), for example, are brought into close proximity, the valence electrons interact in a way similar to that in covalent bonding. When a third sodium atom is brought into close proximity with the nea29583_ch01_001-024.indd 13 12/11/10 9:46 AM 14 CHAPTER 1 The Crystal Structure of Solids first two, the valence electrons can also interact and continue to form a bond. Solid sodium has a body-centered cubic structure, so each atom has eight nearest neighbors with each atom sharing many valence electrons. We may think of the positive metallic ions as being surrounded by a sea of negative electrons, the solid being held together by the electrostatic forces. This description gives a qualitative picture of the metallic bond. A fourth type of atomic bond, called the Van der Waals bond, is the weakest of the chemical bonds. A hydrogen fluoride (HF) molecule, for example, is formed by an ionic bond. The effective center of the positive charge of the molecule is not the same as the effective center of the negative charge. This nonsymmetry in the charge distribution results in a small electric dipole that can interact with the dipoles of other HF molecules. With these weak interactions, solids formed by the Van der Waals bonds have a relatively low melting temperature—in fact, most of these materials are in gaseous form at room temperature. *1.6 | IMPERFECTIONS AND IMPURITIES IN SOLIDS Up to this point, we have been considering an ideal single-crystal structure. In a real crystal, the lattice is not perfect, but contains imperfections or defects; that is, the perfect geometric periodicity is disrupted in some manner. Imperfections tend to alter the electrical properties of a material and, in some cases, electrical parameters can be dominated by these defects or impurities. 1.6.1 Imperfections in Solids One type of imperfection that all crystals have in common is atomic thermal vibration. A perfect single crystal contains atoms at particular lattice sites, the atoms separated from each other by a distance we have assumed to be constant. The atoms in a crystal, however, have a certain thermal energy, which is a function of temperature. The thermal energy causes the atoms to vibrate in a random manner about an equilibrium lattice point. This random thermal motion causes the distance between atoms to randomly fluctuate, slightly disrupting the perfect geometric arrangement of atoms. This imperfection, called lattice vibrations, affects some electrical parameters, as we will see later in our discussion of semiconductor material characteristics. Another type of defect is called a point defect. There are several of this type that we need to consider. Again, in an ideal single-crystal lattice, the atoms are arranged in a perfect periodic arrangement. However, in a real crystal, an atom may be missing from a particular lattice site. This defect is referred to as a vacancy; it is schematically shown in Figure 1.18a. In another situation, an atom may be located between lattice sites. This defect is referred to as an interstitial and is schematically shown in Figure 1.18b. In the case of vacancy and interstitial defects, not only is the perfect *Indicates sections that will aid in the total summation of understanding of semiconductor devices, but may be skipped the first time through the text without loss of continuity. nea29583_ch01_001-024.indd 14 12/11/10 9:46 AM 1.6 Imperfections and Impurities in Solids 15 Vacancy Interstitial (a) (b) Figure 1.18 | Two-dimensional representation of a single-crystal lattice showing (a) a vacancy defect and (b) an interstitial defect. geometric arrangement of atoms broken but also the ideal chemical bonding between atoms is disrupted, which tends to change the electrical properties of the material. A vacancy and interstitial may be in close enough proximity to exhibit an interaction between the two point defects. This vacancy–interstitial defect, also known as a Frenkel defect, produces different effects than the simple vacancy or interstitial. The point defects involve single atoms or single-atom locations. In forming single-crystal materials, more complex defects may occur. A line defect, for example, occurs when an entire row of atoms is missing from its normal lattice site. This defect is referred to as a line dislocation and is shown in Figure 1.19. As with a point defect, a line dislocation disrupts both the normal geometric periodicity of the lattice and the ideal atomic bonds in the crystal. This dislocation can also alter the electrical properties of the material, usually in a more unpredictable manner than the simple point defects. Other complex dislocations can also occur in a crystal lattice. However, this introductory discussion is intended only to present a few of the basic types of defect, and to show that a real crystal is not necessarily a perfect lattice structure. The effect of these imperfections on the electrical properties of a semiconductor will be considered in later chapters. Figure 1.19 | A twodimensional representation of a line dislocation. nea29583_ch01_001-024.indd 15 12/11/10 9:46 AM 16 CHAPTER 1 The Crystal Structure of Solids Substitutional impurity Interstitial impurity (a) (b) Figure 1.20 | Two-dimensional representation of a single-crystal lattice showing (a) a substitutional impurity and (b) an intersitital impurity. 1.6.2 Impurities in Solids Foreign atoms, or impurity atoms, may be present in a crystal lattice. Impurity atoms may be located at normal lattice sites, in which case they are called substitutional impurities. Impurity atoms may also be located between normal sites, in which case they are called interstitial impurities. Both these impurities are lattice defects and are schematically shown in Figure 1.20. Some impurities, such as oxygen in silicon, tend to be essentially inert; however, other impurities, such as gold or phosphorus in silicon, can drastically alter the electrical properties of the material. In Chapter 4 we will see that, by adding controlled amounts of particular impurity atoms, the electrical characteristics of a semiconductor material can be favorably altered. The technique of adding impurity atoms to a semiconductor material in order to change its conductivity is called doping. There are two general methods of doping: impurity diffusion and ion implantation. The actual diffusion process depends to some extent on the material but, in general, impurity diffusion occurs when a semiconductor crystal is placed in a hightemperature (艐1000ºC) gaseous atmosphere containing the desired impurity atom. At this high temperature, many of the crystal atoms can randomly move in and out of their single-crystal lattice sites. Vacancies may be created by this random motion so that impurity atoms can move through the lattice by hopping from one vacancy to another. Impurity diffusion is the process by which impurity particles move from a region of high concentration near the surface to a region of lower concentration within the crystal. When the temperature decreases, the impurity atoms become permanently frozen into the substitutional lattice sites. Diffusion of various impurities into selected regions of a semiconductor allows us to fabricate complex electronic circuits in a single semiconductor crystal. Ion implantation generally takes place at a lower temperature than diffusion. A beam of impurity ions is accelerated to kinetic energies in the range of 50 keV or greater and then directed to the surface of the semiconductor. The high-energy impurity ions enter the crystal and come to rest at some average depth from the surface. One advantage of ion implantation is that controlled numbers of impurity atoms can be introduced into specific regions of the crystal. A disadvantage of this technique is that the incident impurity atoms collide with the crystal atoms, causing nea29583_ch01_001-024.indd 16 12/11/10 9:46 AM 1.7 Growth of Semiconductor Materials 17 lattice-displacement damage. However, most of the lattice damage can be removed by thermal annealing, in which the temperature of the crystal is raised for a short time. Thermal annealing is a required step after implantation. *1.7 | GROWTH OF SEMICONDUCTOR MATERIALS The success in fabricating very large scale integrated (VLSI) circuits is a result, to a large extent, of the development of and improvement in the formation or growth of pure single-crystal semiconductor materials. Semiconductors are some of the purest materials. Silicon, for example, has concentrations of most impurities of less than 1 part in 1010 atoms. The high purity requirement means that extreme care is necessary in the growth and the treatment of the material at each step of the fabrication process. The mechanics and kinetics of crystal growth are extremely complex and will be described in only very general terms in this text. However, a general knowledge of the growth techniques and terminology is valuable. 1.7.1 Growth from a Melt A common technique for growing single-crystal materials is called the Czochralski method. In this technique, a small piece of single-crystal material, known as a seed, is brought into contact with the surface of the same material in liquid phase, and then slowly pulled from the melt. As the seed is slowly pulled, solidification occurs along the plane between the solid–liquid interface. Usually the crystal is also rotated slowly as it is being pulled, to provide a slight stirring action to the melt, resulting in a more uniform temperature. Controlled amounts of specific impurity atoms, such as boron or phosphorus, may be added to the melt so that the grown semiconductor crystal is intentionally doped with the impurity atom. Figure 1.21a shows a schematic of the Czochralski growth process and a silicon ingot or boule grown by this process. Some impurities may be present in the ingot that are undesirable. Zone refining is a common technique for purifying material. A high-temperature coil, or r-f induction coil, is slowly passed along the length of the boule. The temperature induced by the coil is high enough so that a thin layer of liquid is formed. At the solid–liquid interface, there is a distribution of impurities between the two phases. The parameter that describes this distribution is called the segregation coefficient: the ratio of the concentration of impurities in the solid to the concentration in the liquid. If the segregation coefficient is 0.1, for example, the concentration of impurities in the liquid is a factor of 10 greater than that in the solid. As the liquid zone moves through the material, the impurities are driven along with the liquid. After several passes of the r-f coil, most impurities are at the end of the bar, which can then be cut off. The moving molten zone, or the zone-refining technique, can result in considerable purification. After the semiconductor is grown, the boule is mechanically trimmed to the proper diameter and a flat is ground over the entire length of the boule to denote *Indicates sections that will aid in the total summation of understanding of semiconductor devices, but may be skipped the first time through the text without loss of continuity. nea29583_ch01_001-024.indd 17 12/11/10 9:46 AM 18 CHAPTER 1 The Crystal Structure of Solids Container Chuck Seed Crystal Tube Heaters Melt Crucible (a) (b) Figure 1.21 | (a) Model of a crystal puller and (b) photograph of a silicon wafer with an array of integrated circuits. The circuits are tested on the wafer then sawed apart into chips that are mounted into packages. (Photo courtesy of Intel Corporation.) nea29583_ch01_001-024.indd 18 12/11/10 9:46 AM 1.7 Growth of Semiconductor Materials 19 the crystal orientation. The flat is perpendicular to the [110] direction or indicates the (110) plane. (See Figure 1.21b.) This then allows the individual chips to be fabricated along given crystal planes so that the chips can be sawed apart more easily. The boule is then sliced into wafers. The wafer must be thick enough to mechanically support itself. A mechanical two-sided lapping operation produces a flat wafer of uniform thickness. Since the lapping procedure can leave a surface damaged and contaminated by the mechanical operation, the surface must be removed by chemical etching. The final step is polishing. This provides a smooth surface on which devices may be fabricated or further growth processes may be carried out. This final semiconductor wafer is called the substrate material. 1.7.2 Epitaxial Growth A common and versatile growth technique that is used extensively in device and integrated circuit fabrication is epitaxial growth. Epitaxial growth is a process whereby a thin, single-crystal layer of material is grown on the surface of a single-crystal substrate. In the epitaxial process, the single-crystal substrate acts as the seed, although the process takes place far below the melting temperature. When an epitaxial layer is grown on a substrate of the same material, the process is termed homoepitaxy. Growing silicon on a silicon substrate is one example of a homoepitaxy process. At present, a great deal of work is being done with heteroepitaxy. In a heteroepitaxy process, although the substrate and epitaxial materials are not the same, the two crystal structures should be very similar if single-crystal growth is to be obtained and if a large number of defects are to be avoided at the epitaxial–substrate interface. Growing epitaxial layers of the ternary alloy AlGaAs on a GaAs substrate is one example of a heteroepitaxy process. One epitaxial growth technique that has been used extensively is called chemical vapor-phase deposition (CVD). Silicon epitaxial layers, for example, are grown on silicon substrates by the controlled deposition of silicon atoms onto the surface from a chemical vapor containing silicon. In one method, silicon tetrachloride reacts with hydrogen at the surface of a heated substrate. The silicon atoms are released in the reaction and can be deposited onto the substrate, while the other chemical reactant, HCl, is in gaseous form and is swept out of the reactor. A sharp demarcation between the impurity doping in the substrate and in the epitaxial layer can be achieved using the CVD process. This technique allows great flexibility in the fabrication of semiconductor devices. Liquid-phase epitaxy is another epitaxial growth technique. A compound of the semiconductor with another element may have a melting temperature lower than that of the semiconductor itself. The semiconductor substrate is held in the liquid compound and, since the temperature of the melt is lower than the melting temperature of the substrate, the substrate does not melt. As the solution is slowly cooled, a singlecrystal semiconductor layer grows on the seed crystal. This technique, which occurs at a lower temperature than the Czochralski method, is useful in growing group III–V compound semiconductors. A versatile technique for growing epitaxial layers is the molecular beam epitaxy (MBE) process. A substrate is held in vacuum at a temperature normally in the range nea29583_ch01_001-024.indd 19 12/11/10 9:46 AM 20 CHAPTER 1 The Crystal Structure of Solids of 400 to 800C, a relatively low temperature compared with many semiconductorprocessing steps. Semiconductor and dopant atoms are then evaporated onto the surface of the substrate. In this technique, the doping can be precisely controlled resulting in very complex doping profiles. Complex ternary compounds, such as AlGaAs, can be grown on substrates, such as GaAs, where abrupt changes in the crystal composition are desired. Many layers of various types of epitaxial compositions can be grown on a substrate in this manner. These structures are extremely beneficial in optical devices such as laser diodes. 1.8 | SUMMARY ■ ■ ■ ■ ■ ■ A few of the most common semiconductor materials were listed. Silicon is the most common semiconductor material and appears in column IV of the periodic table. The properties of semiconductors and other materials are determined to a large extent by the single-crystal lattice structure. The unit cell is a small volume of the crystal that is used to reproduce the entire crystal. Three basic unit cells are the simple cubic, bodycentered cubic, and face-centered cubic. Silicon has the diamond crystal structure. Atoms are formed in a tetrahedral configuration with four nearest neighbor atoms. The binary semiconductors have a zincblende lattice that is basically the same as the diamond lattice. Miller indices are used to describe planes in a crystal lattice. These planes may be used to describe the surface of a semiconductor material. The Miller indices are also used to describe directions in a crystal. Imperfections do exist in semiconductor materials. A few of these imperfections are vacancies, substitutional impurities, and interstitial impurities. Small amounts of controlled substitutional impurities can favorably alter semiconductor properties as we will see in later chapters. A brief description of semiconductor growth methods was given. Bulk growth, such as the Czochralski method, produces the starting semiconductor material or substrate. Epitaxial growth can be used to control the surface properties of a semiconductor. Most semiconductor devices are fabricated in the epitaxial layer. GLOSSARY OF IMPORTANT TERMS binary semiconductor A two-element compound semiconductor, such as gallium arsenide (GaAs). covalent bonding The bonding between atoms in which valence electrons are shared. diamond lattice The atomic crystal structure of silicon, for example, in which each atom has four nearest neighbors in a tetrahedral configuration. doping The process of adding specific types of atoms to a semiconductor to favorably alter the electrical characteristics. elemental semiconductor A semiconductor composed of a single species of atom, such as silicon or germanium. epitaxial layer A thin, single-crystal layer of material formed on the surface of a substrate. ion implantation One particular process of doping a semiconductor. lattice The periodic arrangement of atoms in a crystal. nea29583_ch01_001-024.indd 20 12/11/10 9:46 AM Problems 21 Miller indices The set of integers used to describe a crystal plane. primitive cell The smallest unit cell that can be repeated to form a lattice. substrate A semiconductor wafer or other material used as the starting material for further semiconductor processing, such as epitaxial growth or diffusion. ternary semiconductor A three-element compound semiconductor, such as aluminum gallium arsenide (AlGaAs). unit cell A small volume of a crystal that can be used to reproduce the entire crystal. zincblende lattice A lattice structure identical to the diamond lattice except that there are two types of atoms instead of one. CHECKPOINT After studying this chapter, the reader should have the ability to: ■ ■ ■ ■ ■ ■ ■ ■ List the most common elemental semiconductor material. Describe the concept of a unit cell. Determine the volume density of atoms for various lattice structures. Determine the Miller indices of a crystal-lattice plane. Sketch a lattice plane given the Miller indices. Determine the surface density of atoms on a given crystal-lattice plane. Describe the tetrahedral configuration of silicon atoms. Understand and describe various defects in a single-crystal lattice. REVIEW QUESTIONS 1. 2. 3. 4. 5. 6. 7. 8. List two elemental semiconductor materials and two compound semiconductor materials. Sketch three lattice structures: (a) simple cubic, (b) body-centered cubic, and (c) face-centered cubic. Describe the procedure for finding the volume density of atoms in a crystal. Describe the procedure for obtaining the Miller indices that describe a plane in a crystal. Describe the procedure for finding the surface density of atoms on a particular lattice plane. Describe why a unit cell, that is not a primitive unit cell, might be preferable to a primitive unit cell. Describe covalent bonding in silicon. What is meant by a substitutional impurity in a crystal? What is meant by an interstitial impurity? PROBLEMS Section 1.3 1.1 1.2 Space Lattices Determine the number of atoms per unit cell in a (a) face-centered cubic, (b) bodycentered cubic, and (c) diamond lattice. Assume that each atom is a hard sphere with the surface of each atom in contact with the surface of its nearest neighbor. Determine the percentage of total unit cell volume nea29583_ch01_001-024.indd 21 12/11/10 9:46 AM 22 CHAPTER 1 The Crystal Structure of Solids that is occupied in (a) a simple cubic lattice, (b) a face-centered cubic lattice, (c) a body-centered cubic lattice, and (d) a diamond lattice. 1.3 If the lattice constant of silicon is 5.43 Å, calculate (a) the distance from the center of one silicon atom to the center of its nearest neighbor, (b) the number density of silicon atoms (#/cm3), and (c) the mass density (g/cm3) of silicon. 1.4 (a) The lattice constant of GaAs is 5.65 Å. Determine the number of Ga atoms and As atoms per cm3. (b) Determine the volume density of germanium atoms in a germanium semiconductor. The lattice constant of germanium is 5.65 Å. 1.5 The lattice constant of GaAs is a 5.65 Å. Calculate (a) the distance between the centers of the nearest Ga and As atoms, and (b) the distance between the centers of the nearest As atoms. 1.6 Calculate the angle between any pair of bonds in the tetrahedral structure. 1.7 Assume the radius of an atom, which can be represented as a hard sphere, is r 1.95 Å. The atom is placed in a (a) simple cubic, (b) fcc, (c) bcc, and (d) diamond lattice. Assuming that nearest atoms are touching each other, what is the lattice constant of each lattice? 1.8 A crystal is composed of two elements, A and B. The basic crystal structure is a facecentered cubic with element A at each of the corners and element B in the center of each face. The effective radius of element A is rA 1.035 Å. Assume that the elements are hard spheres with the surface of each A-type atom in contact with the surface of its nearest A-type neighbor. Calculate (a) the maximum radius of the B-type element that will fit into this structure, (b) the lattice constant, and (c) the volume density (#/cm3) of both the A-type atoms and the B-type atoms. 1.9 (a) A crystal with a simple cubic lattice structure is composed of atoms with an effective radius of r 2.25 Å and has an atomic weight of 12.5. Determine the mass density assuming the atoms are hard spheres and nearest neighbors are touching each other. (b) Repeat part (a) for a body-centered cubic structure. 1.10 A material, with a volume of 1 cm3, is composed of an fcc lattice with a lattice constant of 2.5 mm. The “atoms” in this material are actually coffee beans. Assume the coffee beans are hard spheres with each bean touching its nearest neighbor. Determine the volume of coffee after the coffee beans have been ground. (Assume 100% packing density of the ground coffee.) 1.11 The crystal structure of sodium chloride (NaCl) is a simple cubic with the Na and Cl atoms alternating positions. Each Na atom is then surrounded by six Cl atoms and likewise each Cl atom is surrounded by six Na atoms. (a) Sketch the atoms in a (100) plane. (b) Assume the atoms are hard spheres with nearest neighbors touching. The effective radius of Na is 1.0 Å and the effective radius of Cl is 1.8 Å. Determine the lattice constant. (c) Calculate the volume density of Na and Cl atoms. (d ) Calculate the mass density of NaCl. 1.12 (a) A material is composed of two types of atoms. Atom A has an effective radius of 2.2 Å and atom B has an effective radius of 1.8 Å. The lattice is a bcc with atoms A at the corners and atom B in the center. Determine the lattice constant and the volume densities of A atoms and B atoms. (b) Repeat part (a) with atoms B at the corners and atom A in the center. (c) What comparison can be made of the materials in parts (a) and (b)? 1.13 (a) Consider the materials described in Problem 1.12(a) and 1.12(b). For each case, calculate the surface density of A atoms and B atoms in the (100) plane. What comparison can be made of the two materials? (b) Repeat part (a) for the (110) plane. nea29583_ch01_001-024.indd 22 12/11/10 9:46 AM Problems 1.14 1.15 1.16 1.17 1.18 1.19 1.20 1.21 23 (a) The crystal structure of a particular material consists of a single atom in the center of a cube. The lattice constant is a0 and the diameter of the atom is a0. Determine the volume density of atoms and the surface density of atoms in the (110) plane. (b) Compare the results of part (a) to the results for the case of the simple cubic structure shown in Figure 1.5a with the same lattice constant. The lattice constant of a simple cubic lattice is a0. (a) Sketch the following planes: (i) (110), (ii) (111), (iii) (220), and (iv) (321). (b) Sketch the following directions: (i) [110], (ii) [111], (iii) [220], and (iv) [321]. For a simple cubic lattice, determine the Miller indices for the planes shown in Figure P1.16. A body-centered cubic lattice has a lattice constant of 4.83 Å. A plane cutting the lattice has intercepts of 9.66 Å, 19.32 Å, and 14.49 Å along the three cartesian coordinates. What are the Miller indices of the plane? The lattice constant of a simple cubic primitive cell is 5.28 Å. Determine the distance between the nearest parallel (a) (100), (b) (110), and (c) (111) planes. The lattice constant of a single crystal is 4.73 Å. Calculate the surface density (#/cm2) of atoms on the (i) (100), (ii) (110), and (iii) (111) plane for a (a) simple cubic, (b) body-centered cubic, and (c) face-centered cubic lattice. Determine the surface density of atoms for silicon on the (a) (100) plane, (b) (110) plane, and (c) (111) plane. Consider a face-centered cubic lattice. Assume the atoms are hard spheres with the surfaces of the nearest neighbors touching. Assume the effective radius of the atom is 2.37 Å. (a) Determine the volume density of atoms in the crystal. (b) Calculate the surface density of atoms in the (110) plane. (c) Determine the distance between nearest (110) planes. (d ) Repeat parts (b) and (c) for the (111) plane. z z 4a a y y 3a 2a a x x (a) 4a (b) Figure P1.16 | Figure for Problem 1.16. nea29583_ch01_001-024.indd 23 12/11/10 9:46 AM 24 CHAPTER 1 The Crystal Structure of Solids Section 1.5 Atomic Bonding 1.22 1.23 Calculate the density of valence electrons in silicon. The structure of GaAs is the zincblende lattice. The lattice constant is 5.65 Å. Calculate the density of valence electrons in GaAs. Section 1.6 Imperfections and Impurities in Solids (a) If 5 1017 phosphorus atoms per cm3 are add to silicon as a substitutional impurity, determine the percentage of silicon atoms per unit volume that are displaced in the single crystal lattice. (b) Repeat part (a) for 2 1015 boron atoms per cm3 added to silicon. 1.25 (a) Assume that 2 1016 cm3 of boron atoms are distributed homogeneously throughout single crystal silicon. What is the fraction by weight of boron in the crystal? (b) If phosphorus atoms, at a concentration of 1018 cm3, are added to the material in part (a), determine the fraction by weight of phosphorus. 1.26 If 2 1016 cm3 boron atoms are added to silicon as a substitutional impurity and are distributed uniformly throughout the semiconductor, determine the distance between boron atoms in terms of the silicon lattice constant. (Assume the boron atoms are distributed in a rectangular or cubic array.) 1.27 Repeat Problem 1.26 for 4 1015 cm3 phosphorus atoms being added to silicon. 1.24 READING LIST 1. 2. 3. 4. *5. 6. 7. 8. 9. 10. 11. *12. Azaroff, L.V., and J. J. Brophy. Electronic Processes in Materials. New York: McGraw-Hill, 1963. Campbell, S. A. The Science and Engineering of Microelectronic Fabrication. New York: Oxford University Press, 1996. Dimitrijev, S. Principles of Semiconductor Devices. New York: Oxford University Press, 2006. Kittel, C. Introduction to Solid State Physics, 7th ed. Berlin: Springer-Verlag, 1993. Li, S. S. Semiconductor Physical Electronics. New York: Plenum Press, 1993. McKelvey, J. P. Solid State Physics for Engineering and Materials Science. Malabar, FL: Krieger, 1993. Pierret, R. F. Semiconductor Device Fundamentals. Reading, MA: Addison-Wesley, 1996. Runyan, W. R., and K. E. Bean. Semiconductor Integrated Circuit Processing and Technology. Reading, MA: Addison-Wesley, 1990. Singh, J. Semiconductor Devices: Basic Principles. New York: John Wiley and Sons, 2001. Streetman, B. G., and S. K. Banerjee. Solid State Electronic Devices, 6th ed. Upper Saddle River, NJ: Pearson Prentice Hall, 2006. Sze, S. M. VLSI Technology. New York: McGraw-Hill, 1983. Wolfe, C. M., N. Holonyak, Jr., and G. E. Stillman. Physical Properties of Semiconductors. Englewood Cliffs, NJ: Prentice Hall, 1989. *Indicates references that are at an advanced level compared to this text. nea29583_ch01_001-024.indd 24 12/11/10 9:46 AM C 2 H A P T E R Introduction to Quantum Mechanics T he goal of this text is to help readers understand the operation and characteristics of semiconductor devices. Ideally, we would like to begin discussing these devices immediately. However, in order to understand the current– voltage characteristics, we need some knowledge of electron behavior in a semiconductor when the electron is subjected to various potential functions. The motion of large objects, such as planets and satellites, can be predicted to a high degree of accuracy using classical theoretical physics based on Newton’s laws of motion. But certain experimental results, involving electrons and light waves, appear to be inconsistent with classical physics. However, these experimental results can be predicted using the principles of quantum mechanics. The behavior and characteristics of electrons in a semiconductor can be described by the formulation of quantum mechanics called wave mechanics. The essential elements of this wave mechanics, using Schrodinger’s wave equation, are presented in this chapter. The goal of this chapter is to provide a brief introduction to quantum mechanics so that readers gain an understanding of and become comfortable with the analysis techniques. This introductory material forms the basis of semiconductor physics. ■ 2.0 | PREVIEW In this chapter, we will: ■ Discuss a few basic principles of quantum mechanics that apply to semiconductor device physics. ■ State Schrodinger’s wave equation and discuss the physical meaning of the wave function. ■ Consider the application of Schrodinger’s wave equation to various potential functions to determine some of the fundamental properties of electron behavior in a crystal. 25 nea29583_ch02_025-057.indd 25 12/11/10 9:59 AM 26 CHAPTER 2 ■ Introduction to Quantum Mechanics Apply Schrodinger’s wave equation to the one-electron atom. The result of this analysis yields the four basic quantum numbers, the concept of discrete energy bands, and the initial buildup of the periodic table. 2.1 | PRINCIPLES OF QUANTUM MECHANICS Before we delve into the mathematics of quantum mechanics, there are three principles we need to consider: the principle of energy quanta, the wave–particle duality principle, and the uncertainty principle. 2.1.1 Energy Quanta Incident monochromatic light Photoelectron kinetic energy T Material (a) Maximum kinetic energy, Tmax One experiment that demonstrates an inconsistency between experimental results and the classical theory of light is called the photoelectric effect. If monochromatic light is incident on a clean surface of a material, then under certain conditions, electrons (photoelectrons) are emitted from the surface. According to classical physics, if the intensity of the light is large enough, the work function of the material will be overcome and an electron will be emitted from the surface independent of the incident frequency. This result is not observed. The observed effect is that at a constant incident intensity, the maximum kinetic energy of the photoelectron varies linearly with frequency with a limiting frequency 0, below which no photoelectron is produced. This result is shown in Figure 2.1. If the incident intensity varies at a constant frequency, the rate of photoelectron emission changes, but the maximum kinetic energy remains the same. Planck postulated in 1900 that thermal radiation is emitted from a heated surface in discrete packets of energy called quanta. The energy of these quanta is given by E h, where is the frequency of the radiation and h is a constant now known as Planck’s constant (h 6.625 1034 J-s). Then in 1905, Einstein interpreted the photoelectric results by suggesting that the energy in a light wave is also contained 0 0 Frequency, (b) Figure 2.1 | (a) The photoelectric effect and (b) the maximum kinetic energy of the photoelectron as a function of incident frequency. nea29583_ch02_025-057.indd 26 12/11/10 9:59 AM 2.1 Principles of Quantum Mechanics 27 in discrete packets or bundles. The particle-like packet of energy is called a photon, whose energy is also given by E h. A photon with sufficient energy, then, can knock an electron from the surface of the material. The minimum energy required to remove an electron is called the work function of the material and any excess photon energy goes into the kinetic energy of the photoelectron. This result was confirmed experimentally as demonstrated in Figure 2.1. The photoelectric effect shows the discrete nature of the photon and demonstrates the particle-like behavior of the photon. The maximum kinetic energy of the photoelectron can be written as 1 mv2 hv hv hv (v v0) (2.1) T __ 0 2 hv0 where hv is the incident photon energy and h0 is the minimum energy, or work function, required to remove an electron from the surface. Objective: Calculate the photon energy corresponding to a particular wavelength. EXAMPLE 2.1 Consider an x-ray with a wavelength of 0.708 108 cm. ■ Solution The energy is (6.625 1034)(3 1010) hc _____________________ E hv _ 2.81 1015 J 0.708 108 This value of energy may be given in the more common unit of electron-volt (see Appendix D). We have 2.81 1015 1.75 104 eV E ___________ 1.6 1019 ■ Comment The reciprocal relation between photon energy and wavelength is demonstrated: A large energy corresponds to a short wavelength. ■ EXERCISE PROBLEM Ex 2.1 Determine the energy (in eV) of a photon having a wavelength of (a) 100 Å and (b) 4500 Å. 2.1.2 Wave–Particle Duality [Ans. (a) 124 eV; (b) 2.76 eV] We have seen in the last section that light waves, in the photoelectric effect, behave as if they are particles. The particle-like behavior of electromagnetic waves was also instrumental in the explanation of the Compton effect. In this experiment, an x-ray beam was incident on a solid. A portion of the x-ray beam was deflected and the frequency of the deflected wave had shifted compared with the incident wave. The observed change in frequency and the deflected angle corresponded exactly to the expected results of a “billiard ball” collision between an x-ray quanta, or photon, and an electron in which both energy and momentum are conserved. nea29583_ch02_025-057.indd 27 12/11/10 9:59 AM 28 CHAPTER 2 Introduction to Quantum Mechanics In 1924, de Broglie postulated the existence of matter waves. He suggested that since waves exhibit particle-like behavior, particles should be expected to show wave-like properties. The hypothesis of de Broglie was the existence of a wave– particle duality principle. The momentum of a photon is given by h p_ (2.2) where is the wavelength of the light wave. Then, de Broglie hypothesized that the wavelength of a particle can be expressed as h (2.3) __ p where p is the momentum of the particle and is known as the de Broglie wavelength of the matter wave. The wave nature of electrons has been tested in several ways. In one experiment by Davisson and Germer in 1927, electrons from a heated filament were accelerated at normal incidence onto a single crystal of nickel. A detector measured the scattered electrons as a function of angle. Figure 2.2 shows the experimental setup and Figure 2.3 shows the results. The existence of a peak in the density of scattered electrons can be explained as a constructive interference of waves scattered by the periodic atoms in the planes of the nickel crystal. The angular distribution is very similar to an interference pattern produced by light diffracted from a grating. In order to gain some appreciation of the frequencies and wavelengths involved in the wave-particle duality principle, Figure 2.4 shows the electromagnetic frequency spectrum. We see that a wavelength of 72.7 Å obtained in the next example is in the ultraviolet range. Typically, we will be considering wavelengths in the Sample Electron beam Azimuthal angle Sample Incident electron beam 0 Scattered electrons 45 90 Galvanometer Figure 2.2 | Experimental arrangement of the Davisson– Germer experiment. nea29583_ch02_025-057.indd 28 Figure 2.3 | Scattered electron flux as a function of scattering angle for the Davisson–Germer experiment. 12/11/10 9:59 AM viole t 1000 29 Extreme 40 6.0 Far Medium 1.5 0.770 Orange Red Near 0.622 0.597 0.577 Green Yellow 0.492 0.455 Principles of Quantum Mechanics Visible Ultra Blue 0.390 Violet 0.30 Near 0.20 Far Extreme (m) 0.01 2.1 Infrared X-rays Gamma rays 1 fm 1015 1023 Ultraviolet Infrared Radio spectrum 1 Å 1 nm 1 m 1 mm 1m 1 km 1 Mm 1012 1010 109 106 103 1 103 106 1 pm 1021 1018 1015 Wavelength (m) 108 1 THz 1 GHz 1 MHz 1 kHz 1 Hz 1012 109 106 103 1 Frequency (Hz) Figure 2.4 | The electromagnetic frequency spectrum. ultraviolet and visible range. These wavelengths are very short compared to the usual radio spectrum range.1 Objective: Calculate the de Broglie wavelength of a particle. EXAMPLE 2.2 Consider an electron traveling at a velocity of 107 cm/s 105 m/s. ■ Solution The momentum is given by p mv (9.11 1031)(105) 9.11 1026 kg-m/s Then, the de Broglie wavelength is 6.625 1034 7.27 109 m h ____________ __ p 9.11 1026 or 72.7 Å ■ Comment This calculation shows the order of magnitude of the de Broglie wavelength for a “typical” electron. ■ EXERCISE PROBLEM (a) An electron has a kinetic energy of 12 meV. Determine the de Broglie wavelength (in Å), (b) A particle with mass 2.2 10−31 kg has a de Broglie wavelength of 112 Å. Determine the momentum and kinetic energy of the particle. E 4.97 10–2 eV] Ex 2.2 [Ans. (a) 112 Å; (b) p 5.915 10–26 kg-m/s, 1 An electron microscope is a microscope that produces a magnified image of a specimen. The electron microscope has a magnification approximately 1000 times that of an optical microscope, because the electrons have wavelengths on the order of 100,000 times shorter than the light waves. nea29583_ch02_025-057.indd 29 12/11/10 9:59 AM 30 CHAPTER 2 Introduction to Quantum Mechanics In some cases, electromagnetic waves behave as if they are particles (photons) and sometimes particles behave as if they are waves. This wave–particle duality principle of quantum mechanics applies primarily to small particles such as electrons, but it has also been shown to apply to protons and neutrons. For very large particles, we can show that the relevant equations reduce to those of classical mechanics. The wave–particle duality principle is the basis on which we will use wave theory to describe the motion and behavior of electrons in a crystal. 2.1.3 The Uncertainty Principle The Heisenberg uncertainty principle, given in 1927, also applies primarily to very small particles and states that we cannot describe with absolute accuracy the behavior of these subatomic particles. The uncertainty principle describes a fundamental relationship between conjugate variables, including position and momentum and also energy and time. The first statement of the uncertainty principle is that it is impossible to simultaneously describe with absolute accuracy the position and momentum of a particle. If the uncertainty in the momentum is p and the uncertainty in the postion is x, then the uncertainty principle is stated as2 p x (2.4) where is defined as h/2 1.054 1034 J-s and is called a modified Planck’s constant. This statement may be generalized to include angular position and angular momentum. The second statement of the uncertainty principle is that it is impossible to simultaneously describe with absolute accuracy the energy of a particle and the instant of time the particle has this energy. Again, if the uncertainty in the energy is given by E and the uncertainty in the time is given by t, then the uncertainty principle is stated as E t (2.5) One way to visualize the uncertainty principle is to consider the simultaneous measurement of position and momentum, and the simultaneous measurement of energy and time. The uncertainty principle implies that these simultaneous measurements are in error to a certain extent. However, the modified Planck’s constant is very small; the uncertainty principle is only significant for subatomic particles. We must keep in mind nevertheless that the uncertainty principle is a fundamental statement and does not deal only with measurements. One consequence of the uncertainty principle is that we cannot, for example, determine the exact position of an electron. We will, instead, determine the probability of finding an electron at a particular position. In later chapters, we will develop a In some texts, the uncertainty principle is stated as p x 2. We are interested here in the order of magnitude and will not be concerned with small differences. 2 nea29583_ch02_025-057.indd 30 12/11/10 9:59 AM 2.2 Schrodinger’s Wave Equation 31 probability density function that will allow us to determine the probability that an electron has a particular energy. So in describing electron behavior, we will be dealing with probability functions. TEST YOUR UNDERSTANDING TYU 2.1 The uncertainty in position of an electron is x 8 Å. (a) Determine the minimum uncertainly in momentum. (b) If the nominal value of momentum is p 1.2 10–23 kg-m/s, determine the corresponding uncertainty in kinetic energy. (The uncertainty in kinetic energy can be found from E (dE/dp) p (p p/m) TYU 2.2 (a) A proton’s energy is measured with an uncertainty of 0.8 eV. Determine the minimum uncertainty in time over which this energy is measured. (b) Repeat part (a) for an electron. [Ans. (a) p 1.318 10–25 kg-m/s; (b) E 10.85 eV] [Ans. (a) t 8.23l0–16 s; (b) same as part (a)] 2.2 | SCHRODINGER’S WAVE EQUATION The various experimental results involving electromagnetic waves and particles, which could not be explained by classical laws of physics, showed that a revised formulation of mechanics was required. Schrodinger, in 1926, provided a formulation called wave mechanics, which incorporated the principles of quanta introduced by Planck, and the wave–particle duality principle introduced by de Broglie. On the basis of wave–particle duality principle, we will describe the motion of electrons in a crystal by wave theory. This wave theory is described by Schrodinger’s wave equation. 2.2.1 The Wave Equation The one-dimensional, nonrelativistic Schrodinger’s wave equation is given by (x, t) 2 ⴢ ________ ____ 2 2m x2 (x, t) V(x) (x, t) j __ t (2.6) where (x, t) is the wave function, V(x) is the potential function assumed to be inde___ pendent of time, m is the mass of the particle, and j is the imaginary constant 1 . There are theoretical arguments that justify the form of Schrodinger’s wave equation, but the equation is a basic postulate of quantum mechanics. The wave function (x, t) will be used to describe the behavior of the system and, mathematically, (x, t) can be a complex quantity. We may determine the time-dependent portion of the wave function and the position-dependent, or time-independent, portion of the wave function by using the technique of separation of variables. Assume that the wave function can be written in the form (x, t) (x)(t) nea29583_ch02_025-057.indd 31 (2.7) 12/11/10 9:59 AM 32 CHAPTER 2 Introduction to Quantum Mechanics where (x) is a function of the position x only and (t) is a function of time t only. Substituting this form of the solution into Schrodinger’s wave equation, we obtain (x) 2 (t) ______ ____ (t) V(x) (x)(t) j (x) _____ t 2 2m x2 (2.8) If we divide by the total wave function, Equation (2.8) becomes (x) 2 ____ 1 ______ ____ 2 2m (x) x2 (t) 1 ⴢ _____ V(x) j ⴢ ____ t (t) (2.9) Since the left side of Equation (2.9) is a function of position x only and the right side of the equation is a function of time t only, each side of this equation must be equal to a constant. We will denote this separation of variables constant by . The time-dependent portion of Equation (2.9) is then written as (t) 1 ⴢ _____ j ⴢ ____ t (t) (2.10) where again the parameter is called a separation constant. The solution of Equation (2.10) can be written in the form (t) ej( )t (2.11a) The form of this solution is the classical exponential form of a sinusoidal wave. We have that E h or E h2. Then E so that the separation constant is equal to the total energy E of the particle. We can then write (t) ej(E )t ejt (2.11b) We see that E and is the radian or angular frequency of the sinusoidal wave. The time-independent portion of Schrodinger’s wave equation can now be written from Equation (2.9) as (x) 2 ⴢ ____ 1 ⴢ ______ ____ 2 2m (x) x2 V(x) E (2.12) where the separation constant is the total energy E of the particle. Equation (2.12) may be written as (x) __ 2 x2 2m (E V(x))(x) 0 _ 2 (2.13) where again m is the mass of the particle, V(x) is the potential experienced by the particle, and E is the total energy of the particle. This time-independent Schrodinger’s wave equation can also be justified on the basis of the classical wave equation as shown in Appendix E. The pseudo-derivation in the appendix is a simple approach but shows the plausibility of the time-independent Schrodinger’s equation. 2.2.2 Physical Meaning of the Wave Function We are ultimately trying to use the wave function (x, t) to describe the behavior of an electron in a crystal. The function (x, t) is a wave function, so it is reasonable to nea29583_ch02_025-057.indd 32 12/11/10 9:59 AM 2.2 Schrodinger’s Wave Equation 33 ask what the relation is between the function and the electron. The total wave function is the product of the position-dependent, or time-independent, function and the time-dependent function. From Equation (2.7) we have (x, t) (x) (t) (x) ej(E )t (x) ejt (2.14) Since the total wave function (x, t) is a complex function, it cannot by itself represent a real physical quantity. Max Born postulated in 1926 that the function (x, t)2 dx is the probability of finding the particle between x and x dx at a given time, or that (x, t)2 is a probability density function. We have that (x, t)2 where (x, t) ⴢ * (x, t) (2.15) * (x, t) is the complex conjugate function. Therefore (x, t) *(x) ⴢ e * j(E )t Then the product of the total wave function and its complex conjugate is given by (x, t) (x, t) (x)ej(E )t *(x)e * j(E )t (x)*(x) (2.16) Therefore, we have that (x, t)2 (x)*(x) ()2 (2.17) is the probability density function and is independent of time. One major difference between classical and quantum mechanics is that in classical mechanics, the position of a particle or body can be determined precisely, whereas in quantum mechanics, the position of a particle is found in terms of a probability. We will determine the probability density function for several examples, and since this property is independent of time, we will, in general, only be concerned with the time-independent wave function. 2.2.3 Boundary Conditions Since the function (x)2 represents the probability density function, then for a single particle, we must have |(x)|2 dx 1 (2.18) The probability of finding the particle somewhere is certain. Equation (2.18) allows us to normalize the wave function and is one boundary condition that is used to determine some wave function coefficients. The remaining boundary conditions imposed on the wave function and its derivative are postulates. However, we may state the boundary conditions and present arguments that justify why they must be imposed. The wave function and its first derivative must have the following properties if the total energy E and the potential V(x) are finite everywhere. Condition 1. Condition 2. nea29583_ch02_025-057.indd 33 (x) must be finite, single-valued, and continuous. (x) x must be finite, single-valued, and continuous. 12/11/10 9:59 AM 34 CHAPTER 2 Introduction to Quantum Mechanics V(x) V(x) V(x) V(x) V0 V0 V0 V(x) V0 (x) (x) x0 xa (a) x0 xa (b) Figure 2.5 | Potential functions and corresponding wave function solutions for the case (a) when the potential function is finite everywhere and (b) when the potential function is infinite in some regions. Since (x)2 is a probability density, then (x) must be finite and single-valued. If the probability density were to become infinite at some point in space, then the probability of finding the particle at this position would be certain and the uncertainty principle would be violated. If the total energy E and the potential V(x) are finite everywhere, then from Equation (2.13), the second derivative must be finite, which implies that the first derivative must be continuous. The first derivative is related to the particle momentum, which must be finite and single-valued. Finally, a finite first derivative implies that the function itself must be continuous. In some of the specific examples that we will consider, the potential function will become infinite in particular regions of space. For these cases, the first derivative will not necessarily be continuous, but the remaining boundary conditions will still hold. Figure 2.5 shows two possible examples of potential functions and the corresponding wave solutions. In Figure 2.5a, the potential function is finite everywhere. The wave function as well as its first derivative is continuous. In Figure 2.5b, the potential function is infinite for x 0 and for x a. The wave function is continuous at the boundaries, but the first derivative is discontinuous. We will actually determine the wave functions in the following sections and in end-of-chapter problems. 2.3 | APPLICATIONS OF SCHRODINGER’S WAVE EQUATION We will now apply Schrodinger’s wave equation in several examples using various potential functions. These examples will demonstrate the techniques used in the solution of Schrodinger’s differential equation and the results of these examples will provide an indication of the electron behavior under these various potentials. nea29583_ch02_025-057.indd 34 12/11/10 9:59 AM 2.3 Applications of Schrodinger’s Wave Equation 35 We will utilize the resulting concepts later in the discussion of semiconductor properties. 2.3.1 Electron in Free Space As a first example of applying the Schrodinger’s wave equation, consider the motion of an electron in free space. If there is no force acting on the particle, then the potential function V(x) will be constant and we must have E V(x). Assume, for simplicity, that the potential function V(x) 0 for all x. Then, the time-independent wave equation can be written from Equation (2.13) as (x) ______ 2 x2 2mE (x) 0 ____ (2.19) 2 The solution to this differential equation can be written in the form ____ jx 2mE (x) A exp __ ____ jx 2mE B exp __ (2.20a) or (x) A exp( jkx) B exp(jkx) (2.20b) where _____ k _ 2mE (2.21) 2 and is called a wave number. Recall that the time-dependent portion of the solution is (t) ej(E )t ejt (2.22) Then the total solution for the wave function is given by (x, t) A exp[ j(kx t)] B exp[j(kx t)] (2.23) This wave function solution is a traveling wave, which means that a particle moving in free space is represented by a traveling wave. The first term, with the coefficient A, is a wave traveling in the x direction, while the second term, with the coefficient B, is a wave traveling in the x direction. The value of these coefficients will be determined from boundary conditions. We will again see the traveling-wave solution for an electron in a crystal or semiconductor material. Assume, for a moment, that we have a particle traveling in the x direction, which will be described by the x traveling wave. The coefficient B 0. We can write the traveling-wave solution in the form (x, t) A exp[ j(kx t)] (2.24) where k is the wave number given by _____ k nea29583_ch02_025-057.indd 35 2mE _ 2 ___ 2 p p _ _ 2 (2.25a) 12/11/10 9:59 AM 36 CHAPTER 2 Introduction to Quantum Mechanics or p k Also recall that the de Broglie wavelength was given by 2 h _ _ p p (2.25b) (2.26) Combining Equations (2.25a) and (2.26), the wavelength can also be written in terms of the wave number as 2 _ k (2.27a) 2 k_ (2.27b) or A free particle with a well-defined energy will also have a well-defined wavelength and momentum. The probability density function is (x, t) *(x, t) AA*, which is a constant independent of position. A free particle with a well-defined momentum can be found anywhere with equal probability. This result is in agreement with the Heisenberg uncertainty principle in which a precise momentum implies an undefined position. A localized free particle is defined by a wave packet, formed by a superposition of wave functions with different momentum or k values. We will not consider the wave packet here. 2.3.2 The Infinite Potential Well The problem of a particle in the infinite potential well is a classic example of a bound particle. The potential V(x) as a function of position for this problem is shown in Figure 2.6. The particle is assumed to exist in region II, so the particle is contained within a finite region of space. The time-independent Schrodinger’s wave equation is again given by Equation (2.13) as (x) __ 2 2m (E V(x))(x) 0 _ 2 x2 (2.13) where E is the total energy of the particle. If E is finite, the wave function must be zero, or (x) 0, in both regions I and III. A particle cannot penetrate these infinite potential barriers, so the probability of finding the particle in regions I and III is zero. The time-independent Schrodinger’s wave equation in region II, where V 0, becomes (x) __ 2 x2 nea29583_ch02_025-057.indd 36 2mE (x) 0 _ 2 (2.28) 12/11/10 9:59 AM 2.3 Applications of Schrodinger’s Wave Equation 37 V(x) Region I Region II Region III x0 xa Figure 2.6 | Potential function of the infinite potential well. A particular form of solution to this equation is given by (x) A1 cos kx A2 sin kx (2.29) where _____ k _ 2mE 2 (2.30) One boundary condition is that the wave function (x) must be continuous so that (x 0) (x a) 0 (2.31) Applying the boundary condition at x 0, we must have that A1 0. At x a, we have (x a) 0 A2 sin ka (2.32) This equation is valid if ka n, where the parameter n is a positive integer, or n 1, 2, 3, . . . . The parameter n is referred to as a quantum number. We can write n k_ a (2.33) Negative values of n simply introduce a negative sign in the wave function and yield redundant solutions for the probability density function. We cannot physically distinguish any difference between n and n solutions. Because of this redundancy, negative values of n are not considered. The coefficient A2 can be found from the normalization boundary condition that was given by Equation (2.18) as (x)* (x)dx 1. If we assume that the wave nea29583_ch02_025-057.indd 37 12/13/10 1:44 PM 38 CHAPTER 2 Introduction to Quantum Mechanics function solution (x) is a real function, then (x) *(x). Substituting the wave function into Equation (2.18), we have a 0 A22 sin2 kx dx 1 (2.34) Evaluating this integral gives3 __ A2 _2a (2.35) Finally, the time-independent wave solution is given by __ (x) nx a _2a sin _ where n 1, 2, 3, . . . (2.36) This solution represents the electron in the infinite potential well and is a standing wave solution. The free electron was represented by a traveling wave, and now the bound particle is represented by a standing wave. The parameter k in the wave solution was defined by Equations (2.30) and (2.33). Equating these two expressions for k, we obtain k2 2 2 2mEn _ k2n _ n 2 2 a (2.37) The total energy can then be written as 2 2 2 n E En __ 2ma2 where n 1, 2, 3, . . . (2.38) For the particle in the infinite potential well, the wave function is now given by __ (x) _2a sin k x n (2.39) where the constant kn, from Equation (2.37), must have discrete values, implying that the total energy of the particle can only have discrete values. This result means that the energy of the particle is quantized. That is, the energy of the particle can only have particular discrete values. The quantization of the particle energy is contrary to results from classical physics, which would allow the particle to have continuous energy values. The discrete energies lead to quantum states that will be considered in more detail in this and later chapters. The quantization of the energy of a bound particle is an important result. This quantization of electron energy will be observed again at the end of the chapter for an electron bound to an ion forming an atom. ____ A more analysis____ shows that A22 2a, so solutions for the coefficient ____ thorough ____ ____A2 include 2a . 2a , j2a , −j2a , or any complex number whose magnitude is 2a . Since the wave function itself has no physical meaning, the choice of which coefficient to use is immaterial: They all produce the same probability density function. 3 nea29583_ch02_025-057.indd 38 12/11/10 9:59 AM Applications of Schrodinger’s Wave Equation 39 Objective: Calculate the first three energy levels of an electron in an infinite potential well. EXAMPLE 2.3 2.3 Consider an electron in an infinite potential well of width 5 Å. ■ Solution From Equation (2.38) we have4 2 2 2 n2(1.054 1034)22 n _____ En __ n2(2.41 1019) J 2 2ma 2(9.11 1031)(5 1010)2 or n2(2.41 1019) En ___ n2(1.51) eV 1.6 1019 Then, E1 1.51 eV, E2 6.04 eV, E3 13.59 eV ■ Comment This calculation shows the order of magnitude of the energy levels of a bound electron. ■ EXERCISE PROBLEM Ex 2.3 (a) The width of an infinite potential well is 12 Å. Determine the first three allowed energy levels (in eV) for an electron. (b) Repeat part (a) for a proton. [Ans. (a) 0.261eV, 1.045 eV, 2.351 eV; (b) 1.425 10−4 eV, 5.70 l0−4 eV, 1.28 10−3 eV] Figure 2.7a shows the first four allowed energies for the particle in the infinite potential well, and Figure 2.7b,c shows the corresponding wave functions and probability functions. We may note that as the energy increases, the probability of finding the particle at any given value of x becomes more uniform. 2.3.3 The Step Potential Function Consider now a step potential function as shown in Figure 2.8. In the previous section, we considered a particle being confined between two potential barriers. In this example, we will assume that a flux of particles is incident on the potential barrier. We will assume that the particles are traveling in the x direction and that they originated at x . A particularly interesting result is obtained for the case when the total energy of the particle is less than the barrier height, or E V0. We again need to consider the time-independent wave equation in each of the two regions. This general equation was given in Equation (2.13) as 2(x) x2 2m 2(E V(x))(x) 0. The wave equation in region I, in which V 0, is 1(x) __ 2 x2 2mE (x) 0 _ 1 2 (2.40) 4 See Appendix D for a discussion of the electron-volt (eV) as a unit of energy. nea29583_ch02_025-057.indd 39 12/13/10 1:44 PM 40 CHAPTER 2 Introduction to Quantum Mechanics n4 10 n n2 n3 冉 2 2 E units of 2 2ma 冊 15 5 n2 n1 x0 xa (a) x0 xa (c) (b) Figure 2.7 | Particle in an infinite potential well: (a) four lowest discrete energy levels, (b) corresponding wave functions, and (c) corresponding probability functions. (From Pierret [10].) The general solution to this equation can be written in the form 1(x) A1ejk x B1ejk x 1 1 (x 0) (2.41) where the constant k1 is _____ k1 _ 2mE 2 (2.42) The first term in Equation (2.41) is a traveling wave in the x direction that represents the incident wave, and the second term is a traveling wave in the x direction V(x) Incident particles V0 Region I Region II x0 Figure 2.8 | The step potential function. nea29583_ch02_025-057.indd 40 12/11/10 9:59 AM 2.3 Applications of Schrodinger’s Wave Equation 41 that represents a reflected wave. As in the case of a free particle, the incident and reflected particles are represented by traveling waves. For the incident wave, A1 ⴢ A1* is the probability density function of the incident particles. If we multiply this probability density function by the incident velocity, then vi ⴢ A1 ⴢ A1* is the flux of incident particles in units of #/cm2-s. Likewise, the quantity vr ⴢ B1 ⴢ B1* is the flux of the reflected particles, where vr is the velocity of the reflected wave. (The parameters vi and vr in these terms are actually the magnitudes of the velocity only.) In region II, the potential is V V0. If we assume that E V0, then the differential equation describing the wave function in region II can be written as 2(x) _ __ 2m2 (V0 E)2(x) 0 2 2 x (2.43) The general solution may then be written in the form 2(x) A2ek x B2e 2 k2x (x 0) (2.44) where __________ k2 2m(V0 E) __ 2 (2.45) One boundary condition is that the wave function 2(x) must remain finite, which means that the coefficient B2 0. The wave function is now given by 2(x) A2ek x (x 0) 2 (2.46) The wave function at x 0 must be continuous so that 1(0) 2(0) (2.47) Then from Equations (2.41), (2.46), and (2.47), we obtain B1 A2 A1 (2.48) Since the potential function is everywhere finite, the first derivative of the wave function must also be continuous so that 1 _ x x0 _2 x x0 (2.49) Using Equations (2.41), (2.46), and (2.49), we obtain jk1A1 jk1B1 k2A2 (2.50) We can solve Equations (2.48) and (2.50) to determine the coefficients B1 and A2 in terms of the incident wave coefficient A1. The results are (k22 2jk1k2 k21) B1 ____ ⴢ A1 k22 k21 (2.51a) 2k1(k1 jk2) A2 ___ ⴢ A1 k22 k21 (2.51b) and nea29583_ch02_025-057.indd 41 12/11/10 9:59 AM 42 CHAPTER 2 Introduction to Quantum Mechanics The reflected probability density function is given by (k22 k21 2jk1k2)(k22 k21 2jk1k2) B1 ⴢ B*1 ______ ⴢ A1 ⴢ A*1 (k22 k21)2 (2.52) We can define a reflection coefficient, R, as the ratio of the reflected flux to the incident flux, which is written as vr ⴢ B1 ⴢ B*1 R __ v1 ⴢ A1 ⴢ A*1 (2.53) where i and r are the incident and reflected velocities, respectively, of the particles. In region I, V 0 so that E T, where T is the kinetic energy of the particle. The kinetic energy is given by 1 mv2 T_ (2.54) 2 so that the constant k1, from Equation (2.42) may be written as __________ k1 2 2m _ 1 mv2 _ 2 _____ m _ _ 2 v2 mv 2 (2.55) The incident velocity can then be written as vi _ m ⴢ k1 (2.56) Since the reflected particle also exists in region I, the reflected velocity (magnitude) is given by vr _ m ⴢ k1 (2.57) The incident and reflected velocities (magnitudes) are equal. The reflection coefficient is then vr ⴢ B1 ⴢ B* B1 ⴢ B*1 R __*1 __ vi ⴢ A1 ⴢ A1 A1 ⴢ A*1 (2.58) Substituting the expression from Equation (2.52) into Equation (2.58), we obtain B1 ⴢ B* k22 k21 4k21k22 1.0 R __1* ___ A1 ⴢ A1 k22 k21 (2.59) The result of R 1 implies that all of the particles incident on the potential barrier for E V0 are eventually reflected. Particles are not absorbed or transmitted through the potential barrier. This result is entirely consistent with classical physics and one might ask why we should consider this problem in terms of quantum mechanics. The interesting result is in terms of what happens in region II. The wave solution in region II was given by Equation (2.46) as 2(x) A2ek x. The coefficient A2 from Equation (2.48) is A2 A1 B1, which we derived from the boundary conditions. For the case of E V0, the coefficient A2 is not zero. If A2 is not zero, then the probability density function 2(x) ⴢ 2*(x) of the particle being found in region II is not equal to zero. This result implies that there is a finite 2 nea29583_ch02_025-057.indd 42 12/11/10 9:59 AM 2.3 Applications of Schrodinger’s Wave Equation 43 probability that the incident particle will penetrate the potential barrier and exist in region II. The probability of a particle penetrating the potential barrier is another difference between classical and quantum mechanics: The quantum mechanical penetration is classically not allowed. Although there is a finite probability that the particle may penetrate the barrier, since the reflection coefficient in region I is unity, the particle in region II must eventually turn around and move back into region I. Objective: Calculate the penetration depth of a particle impinging on a potential barrier. EXAMPLE 2.4 Consider an incident electron that is traveling at a velocity of 1 105 m/s in region I. ■ Solution With V(x) 0, the total energy is also equal to the kinetic energy so that 1 mv2 4.56 1021 J 2.85 102 eV ET_ 2 Now, assume that the potential barrier at x 0 is twice as large as the total energy of the incident particle, or that V0 2E. The _____________ wave function solution in region II is 2(x) A2e−k2, where the constant k2 is given by k2 2m(V0 E) 2 . In this example, we want to determine the distance x d at which the wave function magnitude has decayed to e−1 of its value at x 0. Then, for this case, we have k2d 1 or ___________ 1d 2m(2E E) ___ d 2 _____ _ 2mE 2 The distance is then given by _____ d or 1.054 10 _________________________ ______ 11.6 10 2mE 2(9.11 10 ) (4.56 10 ) _ 2 34 31 21 10 m d 11.6 Å ■ Comment This penetration distance corresponds to approximately two lattice constants of silicon. The numbers used in this example are rather arbitrary. We used a distance at which the wave function decayed to e1 of its initial value. We could have arbitrarily used e2, for example, but the results give an indication of the magnitude of penetration depth. ■ EXERCISE PROBLEM Ex 2.4 The probability of finding a particle at a distance d in region II compared with that at x 0 is given by exp (2k2d). Consider an electron traveling in region I at a velocity of 105 m/s incident on a potential barrier whose height is three times the kinetic energy of the electron. Find the probability of finding the electron at a distance d compared with x 0 where d is (a) 10 Å and (b) 100 Å into the potential barrier. [Ans. (a) P 8.680%; (b) P 2.43 109%] The case when the total energy of a particle, which is incident on the potential barrier, is greater than the barrier height, or E V0, is left as an exercise at the end of the chapter. nea29583_ch02_025-057.indd 43 12/11/10 9:59 AM 44 CHAPTER 2 Introduction to Quantum Mechanics V(x) V0 Incident particles (E V0) Region I Region II x0 Region III xa Figure 2.9 | The potential barrier function. 2.3.4 The Potential Barrier and Tunneling We now want to consider the potential barrier function, which is shown in Figure 2.9. The more interesting problem, again, is in the case when the total energy of an incident particle is E V0. Again assume that we have a flux of incident particles originating on the negative x-axis traveling in the x direction. As before, we need to solve Schrodinger’s time-independent wave equation in each of the three regions. The solutions of the wave equation in regions I, II, and III are given, respectively, as 1(x) A1ejk x B1ejk x 1 1 2(x) A2e k2x k2x B2e 3(x) A3e jk1x jk1x B3e (2.60a) (2.60b) (2.60c) where _____ k1 _ 2mE 2 (2.61a) and ___________ k2 _ (V E) 2m 2 0 (2.61b) The coefficient B3 in Equation (2.60c) represents a negative traveling wave in region III. However, once a particle gets into region III, there are no potential changes to cause a reflection; therefore, the coefficient B3 must be zero. We must keep both exponential terms in Equation (2.60b) since the potential barrier width is finite; that is, neither term will become unbounded. We have four boundary relations for the boundaries at x 0 and x a corresponding to the wave function and its first derivative being continuous. We can solve for the four coefficients B1, A2, B2, and A3 in terms of A1. The wave solutions in the three regions are shown in Figure 2.10. nea29583_ch02_025-057.indd 44 12/11/10 9:59 AM 2.3 Applications of Schrodinger’s Wave Equation 45 (x) 0 x0 xa Figure 2.10 | The wave functions through the potential barrier. One particular parameter of interest is the transmission coefficient, in this case defined as the ratio of the transmitted flux in region III to the incident flux in region I. Then the transmission coefficient T is vt ⴢ A3 ⴢ A* A3 ⴢ A*3 T __3* __ A1 ⴢ A*1 vi ⴢ A1 ⴢ Ai (2.62) where vt and vi are the velocities of the transmitted and incident particles, respectively. Since the potential V 0 in both regions I and III, the incident and transmitted velocities are equal. The transmission coefficient may be determined by solving the boundary condition equations. For the special case when E V0, we find that T E 1_ E exp (2k a) 16 _ 2 V0 V0 (2.63) Equation (2.63) implies that there is a finite probability that a particle impinging a potential barrier will penetrate the barrier and will appear in region III. This phenomenon is called tunneling and it, too, contradicts classical mechanics. We will see later how this quantum mechanical tunneling phenomenon can be applied to semiconductor device characteristics, such as in the tunnel diode. Objective: Calculate the probability of an electron tunneling through a potential barrier. EXAMPLE 2.5 Consider an electron with an energy of 2 eV impinging on a potential barrier with V0 20 eV and a width of 3 Å. ■ Solution Equation (2.63) is the tunneling probability. The factor k2 is __________ k2 2m(V0 E) __ 2 _______________________________ 2(9.11 10 )(20 2)(1.6 10 ) _______ 31 19 (1.054 10 34 2 ) or k2 2.17 1010 m1 Then T 16(0.1)(1 0.1) exp [2(2.17 1010)(3 1010)] nea29583_ch02_025-057.indd 45 12/11/10 9:59 AM 46 CHAPTER 2 Introduction to Quantum Mechanics and finally T 3.17 106 ■ Comment The tunneling probability may appear to be a small value, but the value is not zero. If a large number of particles impinge on a potential barrier, a significant number can penetrate the barrier. ■ EXERCISE PROBLEM Ex 2.5 (a)Estimate the probability of an electron with energy E 0.l2 eV tunneling through a rectangular potential barrier with a height of V0 1.2 eV and a width of a 5 Å. (b) Repeat part (a) for a barrier width of a 25 Å. [Ans. (a) T 7.02 103; (b) T 3.97 1012] Additional applications of Schrodinger’s wave equation with various onedimensional potential functions are found in problems at the end of the chapter. Several of these potential functions represent quantum well structures that are found in modern semiconductor devices. TEST YOUR UNDERSTANDING TYU 2.3 (a) Estimate the probability of an electron with energy E 0.10 eV tunneling through a rectangular potential barrier with a barrier height of V0 0.8 eV and width a 12 Å. (b) Repeat part (a) for a barrier height of V0 1.5 eV. TYU 2.4 A certain semiconductor device requires a tunneling probability of T 5 106 for an electron tunneling through a rectangular barrier with a barrier height of V0 0.8 eV. The electron energy is E 0.08 eV. Determine the maximum barrier width. [Ans. (a) T 5.97 10−5; (b) T 4.79 107] (Ans. a 14.46 Å) 2.4 | EXTENSIONS OF THE WAVE THEORY TO ATOMS5 So far in this chapter, we have considered several one-dimensional potential energy functions and solved Schrodinger’s time-independent wave equation to obtain the probability function of finding a particle at various positions. Consider now the one-electron, or hydrogen, atom potential function. We will only briefly consider the mathematical details and wave function solutions, but the results are interesting and important. 2.4.1 The One-Electron Atom The nucleus is a heavy, positively charged proton and the electron is a light, negatively charged particle that, in the classical Bohr theory, is revolving around the 5 The detailed mathematical analysis is beyond the scope of this text, but the results, which are emphasized in this section, are important in the following discussions of semiconductor physics. nea29583_ch02_025-057.indd 46 12/11/10 9:59 AM 2.4 Extensions of the Wave Theory to Atoms 47 nucleus. The potential function is due to the coulomb attraction between the proton and electron and is given by e2 V(r) _ 4 0r (2.64) where e is the magnitude of the electronic charge and 0 is the permittivity of free space. This potential function, although spherically symmetric, leads to a threedimensional problem in spherical coordinates. We may generalize the time-independent Schrodinger’s wave equation to three dimensions by writing 2m0 2(r, , ) _ (E V(r))(r, , ) 0 (2.65) 2 where 2 is the Laplacian operator and must be written in spherical coordinates for this case. The parameter m0 is the rest mass of the electron.6 In spherical coordinates, Schrodinger’s wave equation may be written as r 1 ⴢ _ r2 _ _ 2 r 1 ⴢ_ __ 2 2 2 2 r 2m0 _ 2 r sin 1 ⴢ _ sin ⴢ_ __ 2 r sin (2.66) (E V(r)) 0 The solution to Equation (2.66) can be determined by the separation-of-variables technique. We will assume that the solution to the time-independent wave equation can be written in the form (r, , ) R(r) ⴢ ( ) ⴢ () (2.67) where R, , and , are functions only of r, , and , respectively. Substituting this form of solution into Equation (2.66), we will obtain 2 r 1 ⴢ_ _ 2 2 sin ⴢ _ r2 _ _ R R r r2 sin2 ⴢ 2m _0 2 sin ⴢ _ sin _ ⴢ_ (2.68) (E V) 0 We may note that the second term in Equation (2.68) is a function of only, whereas all the other terms are functions of either r or . We may then write that 1 ⴢ_ _ m2 2 2 (2.69) where m is a separation of variables constant.7 The solution to Equation (2.69) is of the form e jm (2.70) 6 The mass should be the rest mass of the two-particle system, but since the proton mass is much greater than the electron mass, the equivalent mass reduces to that of the electron. 7 Where m means the separation-of-variables constant developed historically. That meaning will be retained here even though there may be some confusion with the electron mass. In general, the mass parameter will be used in conjunction with a subscript. nea29583_ch02_025-057.indd 47 12/11/10 9:59 AM 48 CHAPTER 2 Introduction to Quantum Mechanics Since the wave function must be single-valued, we impose the condition that m is an integer, or m 0, 1, 2, 3, . . . (2.71) Incorporating the separation-of-variables constant, we can further separate the variables and r and generate two additional separation-of-variables constants l and n. The separation-of-variables constants n, l, and m are known as quantum numbers. The parameter n is referred to as the principal quantum number, l is the azimuthal or angular quantum number, and m is the magnetic quantum number. The quantum numbers are related by n 1, 2, 3, . . . l n 1, n 2, n |m| l, l 1, . . . , 0 3, . . . 0 (2.72) Each set of quantum numbers corresponds to a quantum state that the electron may occupy. The electron energy may be written in the form m0e4 En ___ (4 0)22 2n2 (2.73) where again n is the principal quantum number. The negative energy indicates that the electron is bound to the nucleus and we again see that the energy of the bound electron is quantized. If the energy were to become positive, then the electron would no longer be a bound particle and the total energy would no longer be quantized. Since the parameter n in Equation (2.73) is an integer, the total energy of the electron can take on only discrete values. The quantized energy is again a result of the particle being bound in a finite region of space. EXAMPLE 2.6 Objective: Calculate the first three energy levels of an electron for the one-electron atom. ■ Solution We have (9.11 1031)(1.6 1019)4 m0e4 En ___ _______ (4 0)2 2 2n2 [4(8.85 1012)]2 2(1.054 1034)2 n2 21.726 10 J ___ n2 19 13.58 eV or __ n2 For n 1; E1 13.58 eV n 2; E2 3.39 eV n 3; E3 1.51 eV ■ Comment As the energy levels increase, the energy becomes less negative, which means that the electron is becoming less tightly bound to the atom. ■ EXERCISE PROBLEM Ex 2.6 In Example 2.6, assume the permittivity of free space, 0, is replaced by the permittivity of a material where r 0. Repeat the calculations in Example 2.6 if r 11.7 (silicon). (Ans. E1 −99.2 meV, E2 −24.8 meV, E3 −11.0 meV) nea29583_ch02_025-057.indd 48 12/11/10 9:59 AM 2.4 Extensions of the Wave Theory to Atoms 49 The solution of the wave equation may be designated by nlm, where n, l, and m are again the various quantum numbers. For the lowest energy state, n 1, l 0, and m 0, and the wave function is given by 1__ ⴢ _ 1 100 _ a0 32 era (2.74) 0 This function is spherically symmetric, and the parameter a0 is given by 4 0 2 a0 __ 0.529 Å m0e2 (2.75) and is equal to the Bohr radius. The radial probability density function, or the probability of finding the electron at a particular distance from the nucleus, is proportional to the product 100 ⴢ *100 and also to the differential volume of the shell around the nucleus. The probability density function for the lowest energy state is plotted in Figure 2.11a. The most probable distance from the nucleus is at r a0, which is the same as the Bohr theory. Considering this spherically symmetric probability function, we may now begin to conceive the concept of an electron cloud, or energy shell, surrounding the nucleus rather than a discrete particle orbiting around the nucleus. The radial probability density function for the next higher, spherically symmetric wave function, corresponding to n 2, l 0, and m 0, is shown in Figure 2.11b. This figure shows the idea of the next-higher energy shell of the electron. The second energy shell is at a greater radius from the nucleus than the first energy shell. As indicated in the figure, though, there is still a small probability that the electron will exist at the smaller radius. For the case of n 2 and l 1, there are three possible states corresponding to the three allowed values of the quantum number m. These wave functions are no longer spherically symmetric. Although we have not gone into a great deal of mathematical detail for the one-electron atom, three results are important for the further analysis of semiconductor materials. 0.5 0.3 n1 l0 0.2 0.2 a0 Pnl (r) a0 Pnl (r) 0.4 0.1 0 5 r a0 (a) 10 n 2, l 0 0.1 0 5 10 15 r a0 (b) Figure 2.11 | The radial probability density function for the one-electron atom in the (a) lowest energy state and (b) next-higher energy state. (From Eisberg and Resnick [5].) nea29583_ch02_025-057.indd 49 12/11/10 9:59 AM 50 CHAPTER 2 Introduction to Quantum Mechanics The first is the solution of Schrodinger’s wave equation, which again yields electron probability functions, as it did for the simpler potential functions. In developing the physics of semiconductor materials in later chapters, we will also be considering electron probability functions. The second result is the quantization of allowed energy levels for the bound electron. The third is the concept of quantum numbers and quantum states, which evolved from the separation-of-variables technique. We will consider this concept again in the next section and in later chapters when we deal with the semiconductor material physics. 2.4.2 The Periodic Table The initial portion of the periodic table of elements may be determined by using the results of the one-electron atom plus two additional concepts. The first concept needed is that of electron spin. The electron has an intrinsic angular momentum, or spin, which is quantized and may take on one of two possible values. The spin is designated by a quantum number s, which has a value of s __12 or s __12 . We now have four basic quantum numbers: n, l, m, and s. The second concept needed is the Pauli exclusion principle. The Pauli exclusion principle states that, in any given system (an atom, molecule, or crystal), no two electrons may occupy the same quantum state. In an atom, the exclusion principle means that no two electrons may have the same set of quantum numbers. We will see that the exclusion principle is also an important factor in determining the distribution of electrons among available energy states in a crystal. Table 2.1 shows the first few elements of the periodic table. For the first element, hydrogen, we have one electron in the lowest energy state corresponding to n 1. From Equation (2.72) both quantum numbers l and m must be zero. However, the electron can take on either spin factor __21 or __21. For helium, two electrons may exist in the lowest energy state. For this case, l m 0, so now both electron spin states are occupied and the lowest energy shell is full. The chemical activity of an element is determined primarily by the valence, or outermost, electrons. Since the valence energy shell of helium is full, helium does not react with other elements and is an inert element. Table 2.1 | Initial portion of the periodic table Element Hydrogen Helium Lithium Beryllium Boron Carbon Nitrogen Oxygen Fluorine Neon nea29583_ch02_025-057.indd 50 Notation 1 1s 1s2 1s22s1 1s22s2 1s22s22p1 1s22s22p2 1s22s22p3 1s22s22p4 1s22s22p5 1s22s22p6 n 1 1 2 2 2 2 2 2 2 2 l 0 0 0 0 1 1 1 1 1 1 m 0 0 0 0 s 1 1 __ __ 2 or 2 1 1 __ __ 2 and 2 1 1 __ or __ 2 2 1 1 __ __ 2 and 2 m 0, 1, 1 s __12 , __12 12/11/10 9:59 AM Glossary of Important Terms 51 The third element, lithium, has three electrons. The third electron must go into the second energy shell corresponding to n 2. When n 2, the quantum number l may be 0 or 1, and when l 1, the quantum number m may be 1, 0, or 1. In each case, the electron spin factor may be __12 or __12 . For n 2, then, there are eight possible quantum states. Neon has 10 electrons. Two electrons are in the n 1 energy shell and eight electrons are in the n 2 energy shell. The second energy shell is now full, which means that neon is also an inert element. From the solution of Schrodinger’s wave equation for the one-electron atom, plus the concepts of electron spin and the Pauli exclusion principle, we can begin to build up the periodic table of elements. As the atomic numbers of the elements increase, electrons will begin to interact with each other, so that the buildup of the periodic table will deviate somewhat from the simple method. 2.5 | SUMMARY ■ ■ ■ ■ ■ ■ ■ ■ A few basic concepts of quantum mechanics, which can be used to describe the behavior of electrons under various potential functions, were considered. The understanding of electron behavior is crucial in understanding semiconductor physics. The wave–particle duality principle is an important element in quantum mechanics. Particles can have wave-like behavior and waves can have particle-like behavior. Schrodinger’s wave equation forms the basis for describing and predicting the behavior of electrons. Max Born postulated that |(x)|2 is a probability density function. A result of applying Schrodinger’s wave equation to a bound particle is that the energy of the bound particle is quantized. A result of applying Schrodinger’s wave equation to an electron incident on a potential barrier is that there is a finite probability of tunneling. The concept of quantum numbers was developed from the results of applying Schrodinger’s wave equation to the one-electron atom. The basic structure of the periodic table is predicted by applying Schrodinger’s wave equation to the one-electron atom and using the Pauli exclusion principle. GLOSSARY OF IMPORTANT TERMS de Broglie wavelength The wavelength of a particle given as the ratio of Planck’s constant to momentum. Heisenberg uncertainty principle The principle that states that we cannot describe with absolute accuracy the relationship between sets of conjugate variables that describe the behavior of particles, such as momentum and position. Pauli exclusion principle The principle that states that no two electrons can occupy the same quantum state. photon The particle-like packet of electromagnetic energy. quanta The particle-like packet of thermal radiation. quantized energies The allowed discrete energy levels that bound particles may occupy. quantum numbers A set of numbers that describes the quantum state of a particle, such as an electron in an atom. nea29583_ch02_025-057.indd 51 12/11/10 9:59 AM 52 CHAPTER 2 Introduction to Quantum Mechanics quantum state A particular state of an electron that may be described, for example, by a set of quantum numbers. tunneling The quantum mechanical phenomenon by which a particle may penetrate through a thin potential barrier. wave–particle duality The characteristic by which electromagnetic waves sometimes exhibit particle-like behavior and particles sometimes exhibit wave-like behavior. CHECKPOINT After studying this chapter, the reader should have the ability to: ■ ■ ■ ■ ■ ■ Discuss the principle of energy quanta, the wave–particle duality principle, and the uncertainty principle. Apply Schrodinger’s wave equation and boundary conditions to problems with various potential functions. Determine quantized energy levels of bound particles. Determine the approximate tunneling probability of aaaaaaaaaaaa particle incident on a potential barrier. State Pauli exclusion principle. Discuss the results of the one-electron atom analysis, including quantum numbers and their interrelationship as well as the initial formation of the periodic table. REVIEW QUESTIONS 1. 2. 3. 4. 5. 6. 7. 8. State the wave–particle duality principle and state the relationship between momentum and wavelength. What is the physical meaning of Schrodinger’s wave function? What is meant by a probability density function? List the boundary conditions for solutions to Schrodinger’s wave equation. What is meant by quantized energy levels? Can an electron contained in a potential well have an arbitrary energy? Describe the concept of tunneling. List the quantum numbers of the one-electron atom and discuss how they were developed. State the interrelationship between the quantum numbers of the one-electron atom and how this result leads to, for example, the development of inert elements. PROBLEMS 2.1 2.2 2.3 2.4 nea29583_ch02_025-057.indd 52 The classical wave equation for a two-wire transmission line is given by 2V(x, t) x2 LC ⴢ 2V(x, t) t2. One possible ___solution is given by V(x, t) (sin Kx) ⴢ (sin t) where K na and K LC . Sketch, on the same graph, the function V(x, t) as a function of x for 0 x a and n 1 when (i) t 0, (ii) t 2, (iii) t , (i) t 32, and () t 2. The function V(x, t) cos (2 x t) is also a solution to the classical wave equation. Sketch on the same graph the function V(x, t) as a function of x for 0 x 3 when: (i) t 0, (ii) t 0.25, (iii) t 0.5, (i) t 0.75, and () t . Repeat Problem 2.2 for the function V(x, t) cos (2x t). Determine the phase velocities of the traveling waves described in Problems 2.2 and 2.3. 12/11/10 9:59 AM Problems Section 2.1 2.5 2.6 2.7 2.8 2.9 2.10 2.11 2.12 2.13 2.14 2.15 Principles of Quantum Mechanics The work function of a material refers to the minimum energy required to remove an electron from the material. Assume that the work function of gold is 4.90 eV and that of cesium is 1.90 eV. Calculate the maximum wavelength of light for the photoelectric emission of electrons for gold and cesium. (a) The wavelength of green light is 550 nm. If an electron has the same wavelength, determine the electron velocity and momentum. (b) Repeat part (a) for red light with a wavelength of 440 nm. (c) For parts (a) and (b), is the momentum of the photon equal to the momentum of the electron? Determine the de Broglie wavelength for (a) an electron with kinetic energy of (i) 1.2 eV, (ii) 12 eV, (iii) 120 eV; and for (b) a hydrogen atom with a kinetic energy of 1.2 eV. According to classical physics, the average energy of an electron in an electron gas at thermal equilibrium is 3kT2. Determine, for T 300 K, the average electron energy (in eV), average electron momentum, and the de Broglie wavelength. An electron and a photon have the same energy. At what value of energy (in eV) will the wavelength of the photon be 10 times that of the electron? (a) The de Broglie wavelength of an electron is 85 Å. Determine the electron energy (eV), momentum, and velocity. (b) An electron is moving with a velocity of 8 105 cm/s. Determine the electron energy (eV), momentum, and de Broglie wavelength (in Å). It is desired to produce x-ray radiation with a wavelength of 1 Å. (a) Through what potential voltage difference must the electron be accelerated in vacuum so that it can, upon colliding with a target, generate such a photon? (Assume that all of the electron’s energy is transferred to the photon.) (b) What is the de Broglie wavelength of the electron in part (a) just before it hits the target? When the uncertainty principle is considered, it is not possible to locate a photon in space more precisely than about one wavelength. Consider a photon with wavelength 1 m. What is the uncertainty in the photon’s momentum? (a) The uncertainty in position is 12 Å for a particle of mass 9 1031 kg. The nominal energy of the particle is 16 eV. Determine the minimum uncertainty in (i) momentum and (ii) kinetic energy of the particle. (b) Repeat part (a) for a particle of mass 5 1028 kg. An automobile has a mass of 1500 kg. What is the uncertainty in the velocity (in miles per hour) when its center of mass is located with an uncertainty no greater than 1 cm? (a) The electron’s energy is measured with an uncertainty no greater than 0.8 eV. Determine the minimum uncertainty in the time over which the measurement is made. (b) The uncertainty in the position of an electron is no greater than 1.5 Å. Determine the minimum uncertainty in its momentum. Section 2.2 2.16 53 Schrodinger’s Wave Equation Assume that 1(x, t) and 2(x, t) are solutions of the one-dimensional time-dependent Schrodinger’s wave equation. (a) Show that 1 2 is a solution. (b) Is 1 ⴢ 2 a solution of the Schrodinger’s equation in general? Why or why not? nea29583_ch02_025-057.indd 53 12/11/10 9:59 AM 54 CHAPTER 2 2.17 Introduction to Quantum Mechanics Consider the wave function 3 x ejt for 1 x (x, t) A cos _ 2 3. Determine A so that (x, t)2dx 1. 1 2.18 Consider the wave function (x, t) A(cos nx)ejt for 12 x 12 where n is an integer. Determine A so that 12, (x, t)2dx 1. 12 2.19 The solution to Schrodinger’s wave equation for a particular situation is given by ____ (x) 2a0 ⴢ ex/a . Determine the probability of finding the particle between the following limits: (a) 0 x a04, (b) a04 x a02, and (c) 0 x a0. 0 __ x 2 _ An electron is described by a wave function given by (x) _ a cos a a x _ a . The wave function is zero elsewhere. Calculate the probability of for _ 2 2 a , (b) _ ax_ a , and (c) _ a x _ a. finding the electron between (a) 0 x _ 4 4 2 2 __ 2 2x 2 _ 2.21 Repeat Problem 2.20 if the wave function is given by (x) _ a sin a . 2.20 Section 2.3 Applications of Schrodinger’s Wave Equation 2.22 2.23 2.24 2.25 2.26 2.27 2.28 2.29 *2.30 (a) An electron in free space is described by a plane wave given by (x, t) Aej(kxt). If k 8 108 m1 and 8 1012 rad/s, determine the (i) phase velocity and wavelength of the plane wave, and the (ii) momentum and kinetic energy (in eV) of the electron. (b) Repeat part (a) for k 1.5 109 m1 and 1.5 1013 rad/s. An electron is traveling in the negative x direction with a kinetic energy of 0.025 eV. (a) Write the equation of a plane wave that describes this particle. (b) What is the wave number, wavelength, and angular frequency of the wave that describes this electron. Determine the wave number, wavelength, angular frequency, and period of a wave function that describes an electron traveling in free space at a velocity of (a) v 5 106 cm/s and (b) v 108 cm/s. An elecron is bound in a one-dimesional infinite potential well with a width of 75 Å. Determine the electron energy levels (in eV) for n 1, 2, 3. An electron is bound in a one-dimensional infinite potential well with a width of 10 Å. (a) Calculate the first three energy levels that the electron may occupy. (b) If the electron drops from the third to the second energy level, what is the wavelength of a photon that might be emitted? A particle with a mass of 15 mg is bound in a one-dimensional infinite potential well that is 1.2 cm wide. (a) If the energy of the particle is 15 mJ, determine the value of n for that state. (b) What is the energy of the (n 1) state? (c) Would quantum effects be observable for this particle? Calculate the lowest energy level for a neutron in a nucleus, by treating it as if it were in an infinite potential well of width equal to 10−14 m. Compsare this with the lowest energy level for an electron in the same infinite potential well. Consider the particle in the infinite potential well as shown in Figure P2.29. Derive and sketch the wave functions corresponding to the four lowest energy levels. (Do not normalize the wave functions.) Consider a three-dimensional infinite potential well. The potential function is given by V(x) 0 for 0 x a, 0 y a, 0 z a, and V(x) elsewhere. Start with *Asterisks next to problems indicate problems that are more difficult. nea29583_ch02_025-057.indd 54 12/13/10 1:44 PM Problems V(x) 55 V(x) Incident particles V0 x a 2 x0 x a 2 x0 Figure P2.29 | Potential function for Problem 2.29. x Figure P2.33 | Potential function for Problem 2.33. Schrodinger’s wave equation, use the separation of variables technique, and show that the energy is quantized and is given by 2 2 n2 n2 n2 En n n _ x y z 2ma2 where nx 1, 2, 3, . . ., ny 1, 2, 3, . . . , nz 1, 2, 3, . . . . Consider a free electron bound within a two-dimensional infinite potential well defined by V 0 for 0 x 40 Å, 0 y 20 Å, and V elsewhere. (a) Determine the expression for the allowed electron energies. (b) Describe any similarities and any differences with the results of the one-dimensional infinite potential well. Consider a proton in a one-dimensional infinite potential well shown in Figure 2.6. (a) Derive the expression for the allowed energy states of the proton. (b) Calculate the energy difference (in units of eV) between the lowest possible energy and the next higher energy state for (i) a 4 Å, and (ii) a 0.5 cm. For the step potential function shown in Figure P2.33, assume that E V0 and that particles are incident from the x direction traveling in the x direction. (a) Write the wave solutions for each region. (b) Derive expressions for the transmission and reflection coefficients. Consider an electron with a kinetic energy of 2.8 eV incident on a step potential function of height 3.5 eV. Determine the relative probability of finding the electron at a distance (a) 5 Å beyond the barrier, (b) 15 Å beyond the barrier, and (c) 40 Å beyond the barrier compared with the probability of finding the incident particle at the barrier edge. (a) Calculate the transmission coefficient of an electron with a kinetic energy of 0.1 eV impinging on a potential barrier of height 1.0 eV and a width of 4 Å (b) Repeat part (a) for a barrier width of 12 Å. (c) Using the results of part (a), determine the density of electrons per second that impinge the barrier if the tunneling current density is 1.2 mA/cm2. (a) Estimate the tunneling probability of a particle with an effective mass of 0.067m0 (an electron in gallium arsenide), where m0 is the mass of an electron, tunneling through a rectangular potential barrier of height V0 0.8 eV and width 15 Å. The particle kinetic energy is 0.20 eV. (b) Repeat part (a) if the effective mass of the particle is 1.08m0 (an electron in silicon). x y z 2.31 2.32 2.33 2.34 2.35 2.36 nea29583_ch02_025-057.indd 55 12/13/10 1:44 PM 56 CHAPTER 2 Introduction to Quantum Mechanics V(x) Incident particles E V2 V2 V0 V1 I II I III x0 II x0 xa III xa Figure P2.40 | Potential function for Problem 2.40. Figure P2.39 | Potential function for Problem 2.39. 2.37 (a) A proton with a kinetic energy of 1 MeV is incident on a potential barrier of height 12 MeV and width 1014 m. What is the tunneling probability. (b) The width of the potential barrier in part (a) is to be decreased so that the tunneling probability is increased by a factor of 10. What is the width of the potential barrier? *2.38 An electron with energy E is incident on a rectangular potential barrier as shown in Figure 2.9. The potential barrier is of width a and height V0 E. (a) Write the form of the wave function in each of the three regions. (b) For this geometry, determine what coefficient in the wave function solutions is zero. (c) Derive the expression for the transmission coefficient for the electron (tunneling probability). (d) Sketch the wave function for the electron in each region. *2.39 A potential function is shown in Figure P2.39 with incident particles coming from with a total energy E V2. The constants k are defined as _____ k1 2mE _ 2 ___________ k2 2m (E V ) _ 1 2 ___________ k3 _ (E V ) 2m 2 2 Assume a special case for which k2a 2n, n 1, 2, 3, . . . . Derive the expression, in terms of the constants, k1, k2, and k3, for the transmission coefficient. The transmission coefficient is defined as the ratio of the flux of particles in region III to the incident flux in region I. *2.40 Consider the one-dimensional potential function shown in Figure P2.40. Assume the total energy of an electron is E V0. (a) Write the wave solutions that apply in each region. (b) Write the set of equations that result from applying the boundary conditions. (c) Show explicitly why, or why not, the energy levels of the electron are quantized. Section 2.4 2.41 2.42 nea29583_ch02_025-057.indd 56 Extensions of the Wave Theory to Atoms Calculate the energy of the electron in the hydrogen atom (in units of eV) for the first four allowed energy levels. Show that the most probable value of the radius r for the 1s electron in a hydrogen atom is equal to the Bohr radius a0. 12/13/10 1:44 PM Reading List 57 Show that the wave function for 100 given by Equation (2.74) is a solution to the differential equation given by Equation (2.65). 2.44 What property do H, Li, Na, and K have in common? 2.43 READING LIST *1. *2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. Datta, S. Quantum Phenomena. Vol. 8 of Modular Series on Solid State Devices. Reading, MA: Addison–Wesley, 1989. deCogan, D. Solid State Devices: A Quantum Physics Approach. New York: SpringerVerlag, 1987. Dimitrijev, S. Principles of Semiconductor Devices. New York: Oxford University, 2006. Eisberg, R. M. Fundamentals of Modern Physics. New York: Wiley, 1961. Eisberg, R., and R. Resnick. Quantum Physics of Atoms, Molecules, Solids, Nuclei, and Particles. New York: Wiley, 1974. Kano, K. Semiconductor Devices. Upper Saddle River, NJ: Prentice Hall, 1998. Kittel, C. Introduction to Solid State Physics, 7th ed. Berlin: Springer-Verlag, 1993. McKelvey, J. P. Solid State Physics for Engineering and Materials Science. Malabar, FL: Krieger Publishing, 1993. Pauling, L., and E. B. Wilson. Introduction to Quantum Mechanics. New York: McGraw-Hill, 1935. Pierret, R. F. Semiconductor Device Fundamentals. Reading, MA: Addison-Wesley Publishing Co., 1996. Pohl, H. A. Quantum Mechanics for Science and Engineering. Englewood Cliffs, NJ: Prentice Hall, 1967. Schiff, L. I. Quantum Mechanics. New York: McGraw-Hill, 1955. Shur, M. Introduction to Electronic Devices. New York: John Wiley and Sons, 1996. *Indicates references that are at an advanced level compared to this text. nea29583_ch02_025-057.indd 57 12/11/10 9:59 AM C 3 H A P T E R Introduction to the Quantum Theory of Solids I n the last chapter, we applied quantum mechanics and Schrodinger’s wave equation to determine the behavior of electrons in the presence of various potential functions. We found one important characteristic of an electron bound to an atom or bound within a finite space to be that the electron can take on only discrete values of energy; that is, the energies are quantized. We also discussed the Pauli exclusion principle, which stated that only one electron is allowed to occupy any given quantum state. In this chapter, we will generalize these concepts to the electron in a crystal lattice. One of our goals is to determine the electrical properties of a semiconductor material, which we will then use to develop the current–voltage characteristics of semiconductor devices. Toward this end, we have two tasks in this chapter: to determine the properties of electrons in a crystal lattice and to determine the statistical characteristics of the very large number of electrons in a crystal. ■ 3.0 | PREVIEW In this chapter, we will: ■ Develop the concept of allowed and forbidden electron energy bands in a single-crystal material, and describe conduction and valence energy bands in a semiconductor material. ■ Discuss the concept of negatively charged electrons and positively charged holes as two distinct charge carriers in a semiconductor material. ■ Develop electron energy versus momentum curves in a single-crystal material, which yields the concept of direct and indirect bandgap semiconductor materials. ■ Discuss the concept of effective mass of an electron and a hole. ■ Derive the density of quantum states in the allowed energy bands. 58 nea29583_ch03_058-105.indd 58 12/11/10 10:09 AM 3.1 ■ Allowed and Forbidden Energy Bands 59 Develop the Fermi-Dirac probability function, which describes the statistical distribution of electrons among the allowed energy levels, and define the Fermi energy level. 3.1 | ALLOWED AND FORBIDDEN ENERGY BANDS In the last chapter, we considered the one-electron, or hydrogen, atom. That analysis showed that the energy of the bound electron is quantized: Only discrete values of electron energy are allowed. The radial probability density for the electron was also determined. This function gives the probability of finding the electron at a particular distance from the nucleus and shows that the electron is not localized at a given radius. We can extrapolate these single-atom results to a crystal and qualitatively derive the concepts of allowed and forbidden energy bands. We will then apply quantum mechanics and Schrodinger’s wave equation to the problem of an electron in a single crystal. We find that the electronic energy states occur in bands of allowed states that are separated by forbidden energy bands. 3.1.1 Formation of Energy Bands p(r) p(r) a0 r (a) p(r) a0 Electron energy Figure 3.1a shows the radial probability density function for the lowest electron energy state of the single, noninteracting hydrogen atom, and Figure 3.1b shows the same probability curves for two atoms that are in close proximity to each other. The wave functions of the electrons of the two atoms overlap, which means that the two electrons will interact. This interaction or perturbation results in the discrete quantized energy level splitting into two discrete energy levels, schematically shown in Figure 3.1c. The splitting of the discrete state into two states is consistent with the Pauli exclusion principle. A simple analogy of the splitting of energy levels by interacting particles is the following. Two identical race cars and drivers are far apart on a race track. There is no interaction between the cars, so they both must provide the same power to achieve a given speed. However, if one car pulls up close behind the other car, there is an interaction called draft. The second car will be pulled to an extent by the lead car. The lead car will therefore require more power to achieve the same speed since it is pulling the second car, and the second car will require less power since it is being n⫽1 n⫽1 a0 (b) (c) Figure 3.1 | (a) Probability density function of an isolated hydrogen atom. (b) Overlapping probability density functions of two adjacent hydrogen atoms. (c) The splitting of the n 1 state. nea29583_ch03_058-105.indd 59 12/11/10 10:09 AM CHAPTER 3 Introduction to the Quantum Theory of Solids Electron energy 60 r0 Interatomic distance Figure 3.2 | The splitting of an energy state into a band of allowed energies. pulled by the lead car. So there is a “splitting” of power (energy) of the two interacting race cars. (Keep in mind not to take analogies too literally.) Now, if we somehow start with a regular periodic arrangement of hydrogen-type atoms that are initially very far apart, and begin pushing the atoms together, the initial quantized energy level will split into a band of discrete energy levels. This effect is shown schematically in Figure 3.2, where the parameter r0 represents the equilibrium interatomic distance in the crystal. At the equilibrium interatomic distance, there is a band of allowed energies, but within the allowed band, the energies are at discrete levels. The Pauli exclusion principle states that the joining of atoms to form a system (crystal) does not alter the total number of quantum states regardless of size. However, since no two electrons can have the same quantum number, the discrete energy must split into a band of energies in order that each electron can occupy a distinct quantum state. We have seen previously that, at any energy level, the number of allowed quantum states is relatively small. In order to accommodate all of the electrons in a crystal, we must have many energy levels within the allowed band. As an example, suppose that we have a system with 1019 one-electron atoms and also suppose that, at the equilibrium interatomic distance, the width of the allowed energy band is 1 eV. For simplicity, we assume that each electron in the system occupies a different energy level and, if the discrete energy states are equidistant, then the energy levels are separated by 1019 eV. This energy difference is extremely small, so that for all practical purposes, we have a quasi-continuous energy distribution through the allowed energy band. The fact that 1019 eV is a very small difference between two energy states can be seen from the following example. EXAMPLE 3.1 Objective: Calculate the change in kinetic energy of an electron when the velocity changes by a small amount. Consider an electron traveling at a velocity of 107 cm/s. Assume that the velocity increases by a value of 1 cm/s. The increase in kinetic energy is given by 1 mv2 _ 1 mv2 _ 1 m v 2 v 2 E _ 2 1 2 2 2 1 2 Let v2 v1 v. Then v 22 (v1 v)2 v21 2v1v (v)2 nea29583_ch03_058-105.indd 60 12/11/10 10:09 AM 3.1 But v Allowed and Forbidden Energy Bands 61 v1, so we have that 1 m(2v v) mv v E _ 1 1 2 ■ Solution Substituting the number into this equation, we obtain E (9.11 1031)(105)(0.01) 9.11 1028 J which may be converted to units of electron volts as 9.11 10 5.7 109 eV E ___ 1.6 1019 28 ■ Comment A change in velocity of 1 cm/s compared with 107 cm/s results in a change in energy of 5.7 109 eV, which is orders of magnitude larger than the change in energy of 1019 eV between energy states in the allowed energy band. This example serves to demonstrate that a difference in adjacent energy states of 1019 eV is indeed very small, so that the discrete energies within an allowed band may be treated as a quasi-continuous distribution. ■ EXERCISE PROBLEM Ex 3.1 The initial velocity of an electron is 107 cm/s. If the kinetic energy of the electron increases by E 1012 eV, determine the increase in velocity. (Ans. v 1.76 104 cm/s) Consider again a regular periodic arrangement of atoms, in which each atom now contains more than one electron. Suppose the atom in this imaginary crystal contains electrons up through the n 3 energy level. If the atoms are initially very far apart, the electrons in adjacent atoms will not interact and will occupy the discrete energy levels. If these atoms are brought closer together, the outermost electrons in the n 3 energy shell will begin to interact initially, so that this discrete energy level will split into a band of allowed energies. If the atoms continue to move closer together, the electrons in the n 2 shell may begin to interact and will also split into a band of allowed energies. Finally, if the atoms become sufficiently close together, the innermost electrons in the n 1 level may interact, so that this energy level may also split into a band of allowed energies. The splitting of these discrete energy levels is qualitatively shown in Figure 3.3. If the equilibrium interatomic distance is r0, then we have bands of allowed energies that the electrons may occupy separated by bands of forbidden energies. This energy-band splitting and the formation of allowed and forbidden bands is the energy-band theory of single-crystal materials. The actual band splitting in a crystal is much more complicated than indicated in Figure 3.3. A schematic representation of an isolated silicon atom is shown in Figure 3.4a. Ten of the 14 silicon atom electrons occupy deep-lying energy levels close to the nucleus. The four remaining valence electrons are relatively weakly bound and are the electrons involved in chemical reactions. Figure 3.4b shows the band splitting of silicon. We need only consider the n 3 level for the valence nea29583_ch03_058-105.indd 61 12/11/10 10:09 AM 62 CHAPTER 3 Introduction to the Quantum Theory of Solids Electron energy n⫽3 n⫽2 n⫽1 r0 Interatomic distance Figure 3.3 | Schematic showing the splitting of three energy states into allowed bands of energies. 4N states 0 electrons 6N states 2N electrons Six allowed levels at same energy ⫹14 Two allowed levels at same energy sp n⫽3 n⫽1 2 electrons (a) Electron energy 3p n⫽2 8 electrons Eg 3s 4N states 4N electrons 2N states 2N electrons a0 r (b) Figure 3.4 | (a) Schematic of an isolated silicon atom. (b) The splitting of the 3s and 3p states of silicon into the allowed and forbidden energy bands. (From Shockley [6].) electrons, since the first two energy shells are completely full and are tightly bound to the nucleus. The 3s state co rresponds to n 3 and l 0 and contains two quantum states per atom. This state will contain two electrons at T 0 K. The 3p state corresponds to n 3 and l 1 and contains six quantum states per atom. This state will contain the remaining two electrons in the individual silicon atom. As the interatomic distance decreases, the 3s and 3p states interact and overlap. At the equilibrium interatomic distance, the bands have again split, but now four quantum states per atom are in the lower band and four quantum states per atom are in the upper band. At absolute zero degrees, electrons are in the lowest energy state, so that all states in the lower band (the valence band) will be full and all states in the nea29583_ch03_058-105.indd 62 12/11/10 10:09 AM 3.1 Allowed and Forbidden Energy Bands 63 upper band (the conduction band) will be empty. The bandgap energy Eg between the top of the valence band and the bottom of the conduction band is the width of the forbidden energy band. We have discussed qualitatively how and why bands of allowed and forbidden energies are formed in a crystal. The formation of these energy bands is directly related to the electrical characteristics of the crystal, as we will see later in our discussion. *3.1.2 The Kronig–Penney Model1 In the previous section, we discussed qualitatively the splitting of allowed electron energies as atoms are brought together to form a crystal. The concept of allowed and forbidden energy bands can be developed more rigorously by considering quantum mechanics and Schrodinger’s wave equation. It may be easy for the reader to “get lost” in the following derivation, but the result forms the basis for the energy-band theory of semiconductors. The potential function of a single, noninteracting, one-electron atom is shown in Figure 3.5a. Also indicated on the figure are the discrete energy levels allowed for the electron. Figure 3.5b shows the same type of potential function for the case when several atoms in close proximity are arranged in a one-dimensional array. The potential functions of adjacent atoms overlap, and the net potential function for this case is shown in Figure 3.5c. It is this potential function we would need to use in Schrodinger’s wave equation to model a one-dimensional single-crystal material. The solution to Schrodinger’s wave equation, for this one-dimensional singlecrystal lattice, is made more tractable by considering a simpler potential function. Figure 3.6 is the one-dimensional Kronig–Penney model of the periodic potential function, which is used to represent a one-dimensional single-crystal lattice. We need to solve Schrodinger’s wave equation in each region. As with previous quantum mechanical problems, the more interesting solution occurs for the case when E V0, which corresponds to a particle being bound within the crystal. The electrons are contained in the potential wells, but we have the possibility of tunneling between wells. The Kronig–Penney model is an idealized periodic potential representing a one-dimensional single crystal, but the results will illustrate many of the important features of the quantum behavior of electrons in a periodic lattice. To obtain the solution to Schrodinger’s wave equation, we make use of a mathematical theorem by Bloch. The theorem states that all one-electron wave functions, for problems involving periodically varying potential energy functions, must be of the form (x) u(x)ejkx (3.1) *Indicates sections that will aid in the total summation of understanding of semiconductor devices, but may be skipped the first time through the text without loss of continuity. 1 Other techniques, such as the nearly free electron model, can be used to predict the energy-band theory of semiconductor materials. See, for example, Kittel [3] or Wolfe et al. [14]. nea29583_ch03_058-105.indd 63 12/11/10 10:09 AM 64 CHAPTER 3 Introduction to the Quantum Theory of Solids V⫽0 v(r)⬀ 1 r E3 E2 E1 E4 Atom (a) V⫽0 Atom Atom Atom Atom (b) V⫽0 E4 E2 E3 E1 Atom Atom Atom Atom (c) Figure 3.5 | (a) Potential function of a single isolated atom. (b) Overlapping potential functions of adjacent atoms. (c) Net potential function of a one-dimensional single crystal. V(x) V0 II I ⫺(a ⫹ b) ⫺b II I 0 II a (a ⫹ b) I II x Figure 3.6 | The one-dimensional periodic potential function of the Kronig–Penney model. nea29583_ch03_058-105.indd 64 12/11/10 10:09 AM 3.1 Allowed and Forbidden Energy Bands 65 The parameter k is called a constant of motion and will be considered in more detail as we develop the theory. The function u(x) is a periodic function with period (a b). We stated in Chapter 2 that the total solution to the wave equation is the product of the time-independent solution and the time-dependent solution, or (x, t) (x)(t) u(x)ejkx ej(E )t (3.2) which may be written as (x, t) u(x)ej(kx(E )t) (3.3) This traveling-wave solution represents the motion of an electron in a single-crystal material. The amplitude of the traveling wave is a periodic function and the parameter k is also referred to as a wave number. We can now begin to determine a relation between the parameter k, the total energy E, and the potential V0. If we consider region I in Figure 3.6 (0 x a) in which V(x) 0, take the second derivative of Equation (3.1), and substitute this result into the time-independent Schrodinger’s wave equation given by Equation (2.13), we obtain the relation 2 d u1(x) du1(x) __ 2jk _ (k2 2)u1(x) 0 2 dx dx (3.4) The function u1(x) is the amplitude of the wave function in region I and the parameter is defined as 2m E 2 _ 2 (3.5) Consider now a specific region II, −b x 0, in which V(x) V0, and apply Schrodinger’s wave equation. We obtain the relation 2 d u2(x) du2(x) 2mV0 __ 2jk _ k2 2 _ u2(x) 0 2 2 dx dx (3.6) where u2(x) is the amplitude of the wave function in region II. We may define 2mV0 2m (E V ) 2 _ _ 2 0 2 2 (3.7) so that Equation (3.6) may be written as 2 du2(x) d u2(x) __ 2jk _ (k2 2)u2(x) 0 2 dx dx (3.8) Note that from Equation (3.7), if E V0, the parameter is real, whereas if E V0, then is imaginary. The solution to Equation (3.4), for region I, is of the form u1(x) Ae j(k)x Bej(k)x for (0 x a) (3.9) and the solution to Equation (3.8), for region II, is of the form u2(x) Ce j(k)x Dej(k)x for (b x 0) nea29583_ch03_058-105.indd 65 (3.10) 12/11/10 10:09 AM 66 CHAPTER 3 Introduction to the Quantum Theory of Solids Since the potential function V(x) is everywhere finite, both the wave function (x) and its first derivative ⭸(x)⭸x must be continuous. This continuity condition implies that the wave amplitude function u(x) and its first derivative ⭸u(x)⭸x must also be continuous. If we consider the boundary at x ⫽ 0 and apply the continuity condition to the wave amplitude, we have u1(0) ⫽ u2(0) (3.11) Substituting Equations (3.9) and (3.10) into Equation (3.11), we obtain A⫹B⫺C⫺D⫽0 (3.12) Now applying the condition that du1 _ dx x⫽0 du ⫽ _2 dx x⫽0 (3.13) we obtain ( ⫺ k)A ⫺ ( ⫹ k)B ⫺ ( ⫺ k)C ⫹ ( ⫹ k)D ⫽ 0 (3.14) We have considered region I as 0 ⬍ x ⬍ a and region II as −b ⬍ x ⬍ 0. The periodicity and the continuity condition mean that the function u1, as x → a, is equal to the function u2, as x → ⫺b. This condition may be written as u1(a) ⫽ u2(⫺b) (3.15) Applying the solutions for u1(x) and u2(x) to the boundary condition in Equation (3.15) yields Aej(⫺k)a ⫹ Be⫺j(⫹k)a ⫺ Ce⫺j(⫺k)b ⫺ De j(⫹k)b ⫽ 0 (3.16) The last boundary condition is du1 _ dx x⫽a du ⫽ _2 dx x⫽⫺b (3.17) which gives ( ⫺ k)Aej(⫺k)a ⫺ ( ⫹ k)Be⫺j(⫹k)a ⫺ ( ⫺ k)Ce⫺j(⫺k)b ⫹ ( ⫹ k)De j(⫹k)b ⫽ 0 (3.18) We now have four homogeneous equations, Equations (3.12), (3.14), (3.16), and (3.18), with four unknowns as a result of applying the four boundary conditions. In a set of simultaneous, linear, homogeneous equations, there is a nontrivial solution if, and only if, the determinant of the coefficients is zero. In our case, the coefficients in question are the coefficients of the parameters A, B, C, and D. The evaluation of this determinant is extremely laborious and will not be considered in detail. The result is ⫺( ⫹ ) __ (sin a)(sin b) ⫹ (cos a)(cos b) ⫽ cos k(a ⫹ b) 2 2 nea29583_ch03_058-105.indd 66 2 (3.19) 12/13/10 1:44 PM 3.1 Allowed and Forbidden Energy Bands 67 Equation (3.19) relates the parameter k to the total energy E (through the parameter ) and the potential function V0 (through the parameter ). As we mentioned, the more interesting solutions occur for E ⬍ V0, which applies to the electron bound within the crystal. From Equation (3.7), the parameter is then an imaginary quantity. We may define ⫽ j (3.20) where is a real quantity. Equation (3.19) can be written in terms of as ⫺ __ (sin a)(sinh b) ⫹ (cos a)(cosh b) ⫽ cos k(a ⫹ b) 2 2 2 (3.21) Equation (3.21) does not lend itself to an analytical solution, but must be solved using numerical or graphical techniques to obtain the relation between k, E, and V0. The solution of Schrodinger’s wave equation for a single bound particle resulted in discrete allowed energies. The solution of Equation (3.21) will result in a band of allowed energies. To obtain an equation that is more susceptible to a graphical solution and thus will illustrate the nature of the results, let the potential barrier width b → 0 and the barrier height V0 → ⬁, but such that the product bV0 remains finite. Equation (3.21) then reduces to mV ba __ sin a ⫹ cos a ⫽ cos ka __ ប a 0 2 (3.22) We may define a parameter P⬘ as mV0ba P⬘ ⫽ __ ប2 (3.23) sin a ⫹ cos a ⫽ cos ka P⬘ __ a (3.24) Then, finally, we have the relation Equation (3.24) again gives the relation between the parameter k, total energy E (through the parameter ), and the potential barrier bV0. We may note that Equation (3.24) is not a solution of Schrodinger’s wave equation but gives the conditions for which Schrodinger’s wave equation will have a solution. If we assume that the crystal is infinitely large, then k in Equation (3.24) can assume a continuum of values and must be real. 3.1.3 The k-Space Diagram To begin to understand the nature of the solution, initially consider the special case for which V0 ⫽ 0. In this case P⬘ ⫽ 0, which corresponds to a free particle since there are no potential barriers. From Equation (3.24), we have that cos a ⫽ cos ka (3.25) ⫽k (3.26) or nea29583_ch03_058-105.indd 67 12/13/10 1:44 PM 68 CHAPTER 3 Introduction to the Quantum Theory of Solids E p⫽0 p or k Figure 3.7 | The parabolic E versus k curve for the free electron. Since the potential is equal to zero, the total energy E is equal to the kinetic energy, so that, from Equation (3.5), Equation (3.26) may be written as _____ 2m E _ 2 _________ 2m _12 mv2 p __ _k 2 (3.27) where p is the particle momentum. The constant of the motion parameter k is related to the particle momentum for the free electron. The parameter k is also referred to as a wave number. We can also relate the energy and momentum as p2 k2 2 (3.28) E__ 2m 2m Figure 3.7 shows the parabolic relation of Equation (3.28) between the energy E and momentum p for the free particle. Since the momentum and wave number are linearly related, Figure 3.7 is also the E versus k curve for the free particle. We now want to consider the relation between E and k from Equation (3.24) for the particle in the single-crystal lattice. As the parameter P increases, the particle becomes more tightly bound to the potential well or atom. We may define the left side of Equation (3.24) to be a function f (a), so that sin a cos a f (a) P __ a (3.29) Figure 3.8a is a plot of the first term of Equation (3.29) versus a. Figure 3.8b shows a plot of the cos a term and Figure 3.8c is the sum of the two terms, or f (a). Now from Equation (3.24), we also have that f (a) cos ka (3.30) For Equation (3.30) to be valid, the allowed values of the f (a) function must be bounded between 1 and 1. Figure 3.8c shows the allowed values of f (a) and the allowed values of a in the shaded areas. Also shown on the figure are the values of ka from the right side of Equation (3.30), which correspond to the allowed values of f (a). nea29583_ch03_058-105.indd 68 12/11/10 10:09 AM 3.1 Allowed and Forbidden Energy Bands 69 sin ␣a P⬘ ␣a ⫺4 ⫺3 ⫺2 ⫺ 2 3 4 ␣a 3 4 ␣a 4 ␣a (a) cos ␣a ⫺4 ⫺3 ⫺2 ⫺ 2 (b) f (␣a) ⫹1 ⫺4 ⫺3 ⫺2 ⫺ ka ⫽ 0 ka ⫽ 2 2 ⫺1 ka ⫽ ka ⫽ 3 ka ⫽ 3 (c) Figure 3.8 | A plot of (a) the first term in Equation (3.29), (b) the second term in Equation (3.29), and (c) the entire f (a) function. The shaded areas show the allowed values of (a) corresponding to real values of k. The parameter is related to the total energy E of the particle through Equation (3.5), which is 2 2m E 2. A plot of the energy E of the particle as a function of the wave number k can be generated from Figure 3.8c. Figure 3.9 shows this plot and thus shows the concept of allowed energy bands for the particle propagating in the crystal lattice. Since the energy E has discontinuities, we also have the concept of forbidden energies for the particles in the crystal. Objective: Determine the width (in eV) of a forbidden energy band. EXAMPLE 3.2 Determine the width of the forbidden bandgap that exists at ka (see Figure 3.9). Assume that the coefficient P 8 and the potential width is a 4.5 Å. ■ Solution Combining Equations (3.29) and (3.30), we have sin a cos a cos ka P __ a nea29583_ch03_058-105.indd 69 12/11/10 10:09 AM 70 CHAPTER 3 Introduction to the Quantum Theory of Solids E Allowed energy band Forbidden energy band ⫺ 3 a ⫺ 2 a a 0 ⫺a 2 a 3 a k Figure 3.9 | The E versus k diagram generated from Figure 3.8. The allowed energy bands and forbidden energy bandgaps are indicated. At ka and using P 8, we have sin a cos a 1 8 __ a We need to find the smallest values of a that satisfy this equation and then relate to the energy E to find the bandgap energy. From Figure 3.8, we see that, at one value of ka , we have a 1a. Then _____ 1a 2mE1 _ 2 a or 2(1.054 1034)2 2 2 _____ E1 _ 2.972 1019 J 2ma2 2(9.11 1031) (4.5 1010)2 From Figure 3.8, we see that, at the other value of ka , a is in the range a 2. By trial and error, we find a 5.141 2a. Then _____ 2a 2mE2 _ 2 a 5.141 or (5.141)2 2 (5.141)2(1.054 1034)2 E2 __ _____ 7.958 1019 J 2 2ma 2(9.11 1031) (4.5 1010)2 The bandgap energy is then Eg E2 E1 7.958 1019 2.972 1019 4.986 1019 J nea29583_ch03_058-105.indd 70 12/11/10 10:09 AM 3.1 Allowed and Forbidden Energy Bands 71 or 4.986 10 3.12 eV Eg ___ 1.6 1019 19 ■ Comment The results of this example give an order of magnitude of forbidden energy band widths. ■ EXERCISE PROBLEM Using the parameters given in Example 3.2, determine the width of the allowed energy band in the range ka 2. (Ans. E 2.46 eV) Ex 3.2 Consider again the right side of Equation (3.24), which is the function cos ka. The cosine function is periodic so that cos ka cos(ka 2n) cos(ka 2n) (3.31) where n is a positive integer. We may consider Figure 3.9 and displace portions of the curve by 2. Mathematically, Equation (3.24) is still satisfied. Figure 3.10 shows how various segments of the curve can be displaced by the 2 factor. Figure 3.11 shows the case in which the entire E versus k plot is contained within a k a. This plot is referred to as a reduced k-space diagram, or a reduced-zone representation. We noted in Equation (3.27) that for a free electron, the particle momentum and the wave number k are related by p k. Given the similarity between the free E E A A⬘ E⬘ Eo B ⫺ 3 a ⫺ 2 a B⬘ ⫺a 0 a 2 a 3 a k Figure 3.10 | The E versus k diagram showing 2 displacements of several sections of allowed energy bands. nea29583_ch03_058-105.indd 71 ⫺a 0 a k Reduced k space Figure 3.11 | The E versus k diagram in the reduced-zone representation. 12/11/10 10:09 AM 72 CHAPTER 3 Introduction to the Quantum Theory of Solids electron solution and the results of the single crystal shown in Figure 3.9, the parameter k in a single crystal is referred to as the crystal momentum. This parameter is not the actual momentum of the electron in the crystal but is a constant of the motion that includes the crystal interaction. We have been considering the Kronig–Penney model, which is a one-dimensional periodic potential function used to model a single-crystal lattice. The principal result of this analysis, so far, is that electrons in the crystal occupy certain allowed energy bands and are excluded from the forbidden energy bands. For real threedimensional single-crystal materials, a similar energy-band theory exists. We will obtain additional electron properties from the Kronig–Penney model in the next sections. TEST YOUR UNDERSTANDING TYU 3.1 Using the parameters given in Example 3.2, determine the width (in eV) of the second forbidden energy band existing at ka 2 (see Figure 3.8(c)). TYU 3.2 Using the parameters given in Example 3.2, determine the width (in eV) of the allowed energy band in the range 0 ka (see Figure 3.8(c)). (Ans. Eg 4.23 eV) (Ans. E 0.654 eV) 3.2 | ELECTRICAL CONDUCTION IN SOLIDS Again, we are eventually interested in determining the current–voltage characteristics of semiconductor devices. We will need to consider electrical conduction in solids as it relates to the band theory we have just developed. Let us begin by considering the motion of electrons in the various allowed energy bands. 3.2.1 The Energy Band and the Bond Model In Chapter 1, we discussed the covalent bonding of silicon. Figure 3.12 shows a twodimensional representation of the covalent bonding in a single-crystal silicon lattice. This figure represents silicon at T 0 K in which each silicon atom is surrounded by eight valence electrons that are in their lowest energy state and are directly involved in the covalent bonding. Figure 3.4b represented the splitting of the discrete silicon energy states into bands of allowed energies as the silicon crystal is formed. At T 0 K, the 4N states in the lower band, the valence band, are filled with the valence electrons. All of the valence electrons schematically shown in Figure 3.12 are in the valence band. The upper energy band, the conduction band, is completely empty at T 0 K. As the temperature increases above 0 K, a few valence band electrons may gain enough thermal energy to break the covalent bond and jump into the conduction band. Figure 3.13a shows a two-dimensional representation of this bond-breaking nea29583_ch03_058-105.indd 72 12/11/10 10:09 AM 3.2 Electrical Conduction in Solids 73 Figure 3.12 | Two-dimensional representation of the covalent bonding in a semiconductor at T 0 K. e⫺ Conduction band e⫺ Eg Valence band (a) ⫹ (b) Figure 3.13 | (a) Two-dimensional representation of the breaking of a covalent bond. (b) Corresponding line representation of the energy band and the generation of a negative and positive charge with the breaking of a covalent bond. effect and Figure 3.13b, a simple line representation of the energy-band model, shows the same effect. The semiconductor is neutrally charged. This means that, as the negatively charged electron breaks away from its covalent bonding position, a positively charged “empty state” is created in the original covalent bonding position in the valence band. As the temperature further increases, more covalent bonds are broken, more electrons jump to the conduction band, and more positive “empty states” are created in the valence band. We can also relate this bond breaking to the E versus k energy bands. Figure 3.14a shows the E versus k diagram of the conduction and valence bands at T 0 K. The energy states in the valence band are completely full and the states in the conduction band are empty. Figure 3.14b shows these same bands for T 0 K, in which some electrons have gained enough energy to jump to the conduction band and have left empty states in the valence band. We are assuming at this point that no external forces are applied so the electron and “empty state” distributions are symmetrical with k. nea29583_ch03_058-105.indd 73 12/11/10 10:09 AM 74 CHAPTER 3 Introduction to the Quantum Theory of Solids E E k k (a) (b) Figure 3.14 | The E versus k diagram of the conduction and valence bands of a semiconductor at (a) T 0 K and (b) T 0 K. 3.2.2 Drift Current Current is due to the net flow of charge. If we had a collection of positively charged ions with a volume density N (cm3) and an average drift velocity vd (cm/s), then the drift current density would be J qNvd A/cm2 (3.32) If, instead of considering the average drift velocity, we considered the individual ion velocities, then we could write the drift current density as N Jq vi (3.33) i=1 where vi is the velocity of the ith ion. The summation in Equation (3.33) is taken over a unit volume so that the current density J is still in units of A/cm2. Since electrons are charged particles, a net drift of electrons in the conduction band will give rise to a current. The electron distribution in the conduction band, as shown in Figure 3.14b, is an even function of k when no external force is applied. Recall that k for a free electron is related to momentum so that, since there are as many electrons with a k value as there are with a k value, the net drift current density due to these electrons is zero. This result is certainly expected since there is no externally applied force. If a force is applied to a particle and the particle moves, it must gain energy. This effect is expressed as dE F dx F v dt (3.34) where F is the applied force, dx is the differential distance the particle moves, v is the velocity, and dE is the increase in energy. If an external force is applied to the electrons in the conduction band, there are empty energy states into which the electrons can move; therefore, because of the external force, electrons can gain energy and a nea29583_ch03_058-105.indd 74 12/11/10 10:09 AM 3.2 Electrical Conduction in Solids 75 E k Figure 3.15 | The asymmetric distribution of electrons in the E versus k diagram when an external force is applied. net momentum. The electron distribution in the conduction band may look like that shown in Figure 3.15, which implies that the electrons have gained a net momentum. We may write the drift current density due to the motion of electrons as n J e vi (3.35) i=1 where e is the magnitude of the electronic charge and n is the number of electrons per unit volume in the conduction band. Again, the summation is taken over a unit volume so that the current density is still in units of A/cm2. We may note from Equation (3.35) that the current is directly related to the electron velocity; that is, the current is related to how well the electron can move in the crystal. 3.2.3 Electron Effective Mass The movement of an electron in a lattice will, in general, be different from that of an electron in free space. In addition to an externally applied force, there are internal forces in the crystal due to positively charged ions or protons and negatively charged electrons, which will influence the motion of electrons in the lattice. We can write Ftotal Fext Fint ma (3.36) where Ftotal, Fext, and Fint are the total force, the externally applied force, and the internal forces, respectively, acting on a particle in a crystal. The parameter a is the acceleration and m is the rest mass of the particle. Since it is difficult to take into account all of the internal forces, we will write the equation Fext m*a (3.37) where the acceleration a is now directly related to the external force. The parameter m*, called the effective mass, takes into account the particle mass and also takes into account the effect of the internal forces. To use an analogy for the effective mass concept, consider the difference in motion between a glass marble in a container filled with water and in a container filled with oil. In general, the marble will drop through the water at a faster rate than through the oil. The external force in this example is the gravitational force and the internal nea29583_ch03_058-105.indd 75 12/11/10 10:09 AM 76 CHAPTER 3 Introduction to the Quantum Theory of Solids forces are related to the viscosity of the liquids. Because of the difference in motion of the marble in these two cases, the mass of the marble would appear to be different in water than in oil. (As with any analogy, we must be careful not to be too literal.) We can also relate the effective mass of an electron in a crystal to the E versus k curves, such as is shown in Figure 3.11. In a semiconductor material, we will be dealing with allowed energy bands that are almost empty of electrons and other energy bands that are almost full of electrons. To begin, consider the case of a free electron whose E versus k curve is shown in Figure 3.7. Recalling Equation (3.28), the energy and momentum are related by E p22m 2k22m, where m is the mass of the electron. The momentum and wave number k are related by p k. If we take the derivative of Equation (3.28) with respect to k, we obtain 2 p dE _ k_ _ (3.38) m m dk Relating momentum to velocity, Equation (3.38) can be written as p dE _ 1_ _ (3.39) mv dk where v is the velocity of the particle. The first derivative of E with respect to k is related to the velocity of the particle. If we now take the second derivative of E with respect to k, we have 2 d E = _2 _ (3.40) 2 E_ 1 1 d_ _ (3.41) dk2 m We may rewrite Equation (3.40) as 2 dk2 m The second derivative of E with respect to k is inversely proportional to the mass of the particle. For the case of a free electron, the mass is a constant (nonrelativistic effect), so the second derivative function is a constant. We may also note from Figure 3.7 that d 2Edk2 is a positive quantity, which implies that the mass of the electron is also a positive quantity. If we apply an electric field to the free electron and use Newton’s classical equation of motion, we can write F ma eE (3.42) where a is the acceleration, E is the applied electric field, and e is the magnitude of the electronic charge. Solving for the acceleration, we have eE a_ m (3.43) The motion of the free electron is in the opposite direction to the applied electric field because of the negative charge. We may now apply the results to the electron in the bottom of an allowed energy band. Consider the allowed energy band in Figure 3.16a. The energy near the bottom nea29583_ch03_058-105.indd 76 12/11/10 10:09 AM 3.2 Electrical Conduction in Solids 77 E E Parabolic approximation EV EC Parabolic approximation k⫽0 k⫽0 k k (b) (a) Figure 3.16 | (a) The conduction band in reduced k space, and the parabolic approximation. (b) The valence band in reduced k space, and the parabolic approximation. of this energy band may be approximated by a parabola, just as that of a free particle. We may write E Ec C1(k)2 (3.44) The energy Ec is the energy at the bottom of the band. Since E Ec, the parameter C1 is a positive quantity. Taking the second derivative of E with respect to k from Equation (3.44), we obtain 2 d E 2C _ (3.45) 1 dk2 We may put Equation (3.45) in the form 2C1 d E_ 1 _ _ 2 (3.46) 2 dk2 Comparing Equation (3.46) with Equation (3.41), we may equate 22C1 to the mass of the particle. However, the curvature of the curve in Figure 3.16a will not, in general, be the same as the curvature of the free-particle curve. We may write 2 2C1 _ d E_ 1 _ _ 1 2 2 dk2 2 m* (3.47) where m* is called the effective mass. Since C1 0, we have that m* 0 also. The effective mass is a parameter that relates the quantum mechanical results to the classical force equations. In most instances, the electron in the bottom of the conduction band can be thought of as a classical particle whose motion can be modeled by Newtonian mechanics, provided that the internal forces and quantum mechanical properties are taken into account through the effective mass. If we apply an electric field to the electron in the bottom of the allowed energy band, we may write the acceleration as eE a_ m*n (3.48) where mn* is the effective mass of the electron. The effective mass mn* of the electron near the bottom of the conduction band is a constant. nea29583_ch03_058-105.indd 77 12/11/10 10:09 AM 78 CHAPTER 3 3.2.4 Introduction to the Quantum Theory of Solids Concept of the Hole In considering the two-dimensional representation of the covalent bonding shown in Figure 3.13a, a positively charged “empty state” was created when a valence electron was elevated into the conduction band. For T 0 K, all valence electrons may gain thermal energy; if a valence electron gains a small amount of thermal energy, it may hop into the empty state. The movement of a valence electron into the empty state is equivalent to the movement of the positively charged empty state itself. Figure 3.17 shows the movement of valence electrons in the crystal, alternately filling one empty state and creating a new empty state—a motion equivalent to a positive charge moving in the valence band. The crystal now has a second equally important charge carrier that can give rise to a current. This charge carrier is called a hole and, as we will see, can also be thought of as a classical particle whose motion can be modeled using Newtonian mechanics. The drift current density due to electrons in the valence band, such as shown in Figure 3.14b, can be written as J e vi (3.49) i (filled) where the summation extends over all filled states. This summation is inconvenient since it extends over a nearly full valence band and takes into account a very large number of states. We may rewrite Equation (3.49) in the form J e vi e i (total) vi (3.50) i (empty) If we consider a band that is totally full, all available states are occupied by electrons. The individual electrons can be thought of as moving with a velocity as given by Equation (3.39): dE 1 _ v(E) _ dk (3.39) The band is symmetric in k and each state is occupied so that, for every electron with a velocity v , there is a corresponding electron with a velocity v . Since the band is full, the distribution of electrons with respect to k cannot be changed with an (a) (b) (c) Figure 3.17 | Visualization of the movement of a hole in a semiconductor. nea29583_ch03_058-105.indd 78 12/11/10 10:09 AM 3.2 Electrical Conduction in Solids 79 E E ++ k ++ ++ + k (b) (a) Figure 3.18 | (a) Valence band with conventional electron-filled states and empty states. (b) Concept of positive charges occupying the original empty states. externally applied force. The net drift current density generated from a completely full band, then, is zero, or e vi 0 (3.51) i (total) We can now write the drift current density from Equation (3.50) for an almost full band as J e vi (3.52) i (empty) where the vi in the summation is the dE 1 _ v(E) _ dk associated with the empty state. Equation (3.52) is entirely equivalent to placing a positively charged particle in the empty states and assuming all other states in the band are empty, or neutrally charged. This concept is shown in Figure 3.18. Figure 3.18a shows the valence band with the conventional electron-filled states and empty states, whereas Figure 3.18b shows the new concept of positive charges occupying the original empty states. This concept is consistent with the discussion of the positively charged “empty state” in the valence band, as shown in Figure 3.17. The vi in the summation of Equation (3.52) is related to how well this positively charged particle moves in the semiconductor. Now consider an electron near the top of the allowed energy band shown in Figure 3.16b. The energy near the top of the allowed energy band may again be approximated by a parabola so that we may write (E Ev) C2(k)2 (3.53) The energy Ev is the energy at the top of the energy band. Since E Ev for electrons in this band, the parameter C2 must be a positive quantity. Taking the second derivative of E with respect to k from Equation (3.53), we obtain d 2E 2C _ (3.54) 2 dk 2 We may rearrange this equation so that 2C2 d E_ 1 _ _ 2 2 nea29583_ch03_058-105.indd 79 dk2 2 (3.55) 12/11/10 10:09 AM 80 CHAPTER 3 Introduction to the Quantum Theory of Solids Comparing Equation (3.55) with Equation (3.41), we may write 2C2 _ d E_ 1 _ _ 1 2 2 dk2 2 m* (3.56) where m* is again an effective mass. We have argued that C2 is a positive quantity, which now implies that m* is a negative quantity. An electron moving near the top of an allowed energy band behaves as if it has a negative mass. We must keep in mind that the effective mass parameter is used to relate quantum mechanics and classical mechanics. The attempt to relate these two theories leads to this strange result of a negative effective mass. However, we must recall that solutions to Schrodinger’s wave equation also led to results that contradicted classical mechanics. The negative effective mass is another such example. In discussing the concept of effective mass in the previous section, we used an analogy of marbles moving through two liquids. Now consider placing an ice cube in the center of a container filled with water: the ice cube will move upward toward the surface in a direction opposite to the gravitational force. The ice cube appears to have a negative effective mass since its acceleration is opposite to the external force. The effective mass parameter takes into account all internal forces acting on the particle. If we again consider an electron near the top of an allowed energy band and use Newton’s force equation for an applied electric field, we will have F m*a eE (3.57) However, m* is now a negative quantity, so we may write eE _ eE a __ m* m* (3.58) An electron moving near the top of an allowed energy band moves in the same direction as the applied electric field. The net motion of electrons in a nearly full band can be described by considering just the empty states, provided that a positive electronic charge is associated with each state and that the negative of m* from Equation (3.56) is associated with each state. We now can model this band as having particles with a positive electronic charge and a positive effective mass. The density of these particles in the valence band is the same as the density of empty electronic energy states. This new particle is the hole. The hole, then, has a positive effective mass denoted by mp* and a positive electronic charge, so it will move in the same direction as an applied field. 3.2.5 Metals, Insulators, and Semiconductors Each crystal has its own energy-band structure. We noted that the splitting of the energy states in silicon, for example, to form the valence and conduction bands, was complex. Complex band splitting occurs in other crystals, leading to large variations in band structures between various solids and to a wide range of electrical characteristics observed in these various materials. We can qualitatively begin to understand some basic differences in electrical characteristics caused by variations in band structure by considering some simplified energy bands. nea29583_ch03_058-105.indd 80 12/11/10 10:09 AM 3.2 Electrical Conduction in Solids 81 Allowed energy band (almost empty) Allowed energy band (empty) (a) (a) Allowed energy band (almost full) Allowed energy band (full) (b) (b) Conduction band (almost empty) Conduction band (empty) Electrons Eg Empty electronic states Valence band (almost full) Eg Valence band (full) (c) (c) Figure 3.19 | Allowed energy bands showing (a) an empty band, (b) a completely full band, and (c) the bandgap energy between the two allowed bands. Figure 3.20 | Allowed energy bands showing (a) an almost empty band, (b) an almost full band, and (c) the bandgap energy between the two allowed bands. There are several possible energy-band conditions to consider. Figure 3.19a shows an allowed energy band that is completely empty of electrons. If an electric field is applied, there are no particles to move, so there will be no current. Figure 3.19b shows another allowed energy band whose energy states are completely full of electrons. We argued in the previous section that a completely full energy band will also not give rise to a current. A material that has energy bands either completely empty or completely full is an insulator. The resistivity of an insulator is very large or, conversely, the conductivity of an insulator is very small. There are essentially no charged particles that can contribute to a drift current. Figure 3.19c shows a simplified energy-band diagram of an insulator. The bandgap energy Eg of an insulator is usually on the order of 3.5 to 6 eV or larger, so that at room temperature, there are essentially no electrons in the conduction band and the valence band remains completely full. There are very few thermally generated electrons and holes in an insulator. Figure 3.20a shows an energy band with relatively few electrons near the bottom of the band. Now, if an electric field is applied, the electrons can gain energy, move to higher energy states, and move through the crystal. The net flow of charge is a current. Figure 3.20b shows an allowed energy band that is almost full of electrons, which means that we can consider the holes in this band. If an electric field is applied, the holes can move and give rise to a current. Figure 3.20c shows the simplified energy-band diagram for this case. The bandgap energy may be on the order of 1 eV. nea29583_ch03_058-105.indd 81 12/11/10 10:09 AM 82 CHAPTER 3 Introduction to the Quantum Theory of Solids Partially filled band Upper band Lower band Full band Electrons (b) (a) Figure 3.21 | Two possible energy bands of a metal showing (a) a partially filled band and (b) overlapping allowed energy bands. This energy-band diagram represents a semiconductor for T 0 K. The resistivity of a semiconductor, as we will see in the next chapter, can be controlled and varied over many orders of magnitude. The characteristics of a metal include a very low resistivity. The energy-band diagram for a metal may be in one of two forms. Figure 3.21a shows the case of a partially full band in which there are many electrons available for conduction, so that the material can exhibit a large electrical conductivity. Figure 3.21b shows another possible energy-band diagram of a metal. The band splitting into allowed and forbidden energy bands is a complex phenomenon, and Figure 3.21b shows a case in which the conduction and valence bands overlap at the equilibrium interatomic distance. As in the case shown in Figure 3.21a, there are large numbers of electrons as well as large numbers of empty energy states into which the electrons can move, so this material can also exhibit a very high electrical conductivity. TEST YOUR UNDERSTANDING TYU 3.3 A simplified E versus k curve for an electron in the conduction band is given. The value of a is 10 Å. Determine the relative effective mass m*m0. TYU 3.4 A simplified E versus k curve for a hole in the valence band is given. Assume a value of a 12 Å. Determine the relative effective mass m*m0 . (Ans. m*m0 1.175) (Ans. m*m0 0.2985) E E E = Ec + 0.32 eV Ec ⫺a 0 a k Figure 3.22 | Figure for Exercise TYU 3.3. nea29583_ch03_058-105.indd 82 Ev ⫺a 0 a k E ⫽ Ev ⫺ 0.875 eV Figure 3.23 | Figure for Exercise TYU 3.4. 12/11/10 10:09 AM 3.3 Extension to Three Dimensions 83 3.3 | EXTENSION TO THREE DIMENSIONS The basic concepts of allowed and forbidden energy bands and effective mass have been developed in the previous sections. In this section, we will extend these concepts to three dimensions and to real crystals. We will qualitatively consider particular characteristics of the three-dimensional crystal in terms of the E versus k plots, bandgap energy, and effective mass. We must emphasize that we will only briefly touch on the basic three-dimensional concepts; therefore, many details will not be considered. One problem encountered in extending the potential function to a threedimensional crystal is that the distance between atoms varies as the direction through the crystal changes. Figure 3.24 shows a face-centered cubic structure with the [100] and [110] directions indicated. Electrons traveling in different directions encounter different potential patterns and therefore different k-space boundaries. The E versus k diagrams are, in general, a function of the k-space direction in a crystal. 3.3.1 The k-Space Diagrams of Si and GaAs Figure 3.25 shows an E versus k diagram of gallium arsenide (GaAs) and of silicon (Si). These simplified diagrams show the basic properties considered in this text but do not show many of the details more appropriate for advanced-level courses. Note that in place of the usual positive and negative k axes, we now show two different crystal directions. The E versus k diagram for the one-dimensional model was symmetric in k so that no new information is obtained by displaying the negative axis. It is normal practice to plot the [100] direction along the normal k axis and to plot the [111] portion of the diagram so the k points to the left. In the case of diamond or zincblende lattices, the maxima in the valence band energy and minima in the conduction band energy occur at k 0 or along one of these two directions. Figure 3.25a shows the E versus k diagram for GaAs. The valence band maximum and the conduction band minimum both occur at k 0. The electrons in the – b [110] direction [100] direction –a Figure 3.24 | The (100) plane of a face-centered cubic crystal showing the [100] and [110] directions. nea29583_ch03_058-105.indd 83 12/11/10 10:09 AM 84 CHAPTER 3 Introduction to the Quantum Theory of Solids 4 4 GaAs Conduction band Si 3 3 2 ⌬E ⫽ 0.31 1 Energy (eV) Energy (eV) 2 Eg 1 Eg 0 0 ⫺1 ⫺1 ⫺2 Conduction band Valence band [111] 0 [100] ⫺2 Valence band [111] 0 [100] k k (a) (b) Figure 3.25 | Energy-band structures of (a) GaAs and (b) Si. (From Sze [12].) conduction band tend to settle at the minimum conduction band energy that is at k 0. Similarly, holes in the valence band tend to congregate at the uppermost valence band energy. In GaAs, the minimum conduction band energy and maximum valence band energy occur at the same k value. A semiconductor with this property is said to be a direct bandgap semiconductor; transitions between the two allowed bands can take place with no change in crystal momentum. This direct nature has significant effect on the optical properties of the material. GaAs and other direct bandgap materials are ideally suited for use in semiconductor lasers and other optical devices. The E versus k diagram for silicon is shown in Figure 3.25b. The maximum in the valence band energy occurs at k 0 as before. The minimum in the conduction band energy occurs not at k 0, but along the [100] direction. The difference between the minimum conduction band energy and the maximum valence band energy is still defined as the bandgap energy Eg. A semiconductor whose maximum valence band energy and minimum conduction band energy do not occur at the same k value is called an indirect bandgap semiconductor. When electrons make a transition between the conduction and valence bands, we must invoke the law of conservation of momentum. A transition in an indirect bandgap material must necessarily include an interaction with the crystal so that crystal momentum is conserved. Germanium is also an indirect bandgap material, whose valence band maximum occurs at k 0 and whose conduction band minimum occurs along the [111] direction. GaAs is a direct bandgap semiconductor, but other compound semiconductors, such as GaP and AlAs, have indirect bandgaps. nea29583_ch03_058-105.indd 84 12/11/10 10:09 AM 3.4 3.3.2 Density of States Function 85 Additional Effective Mass Concepts The curvature of the E versus k diagrams near the minimum of the conduction band energy is related to the effective mass of the electron. We may note from Figure 3.25 that the curvature of the conduction band at its minimum value for GaAs is larger than that of silicon, so the effective mass of an electron in the conduction band of GaAs will be smaller than that in silicon. For the one-dimensional E versus k diagram, the effective mass was defined by Equation (3.41) as 1m* 1 2 d2Edk2. A complication occurs in the effective mass concept in a real crystal. A three-dimensional crystal can be described by three k vectors. The curvature of the E versus k diagram at the conduction band minimum may not be the same in the three k directions. In later sections and chapters, the effective mass parameters used in calculations will be a kind of statistical average that is adequate for most device calculations.2 3.4 | DENSITY OF STATES FUNCTION As we have stated, we eventually wish to describe the current–voltage characteristics of semiconductor devices. Since current is due to the flow of charge, an important step in the process is to determine the number of electrons and holes in the semiconductor that will be available for conduction. The number of carriers that can contribute to the conduction process is a function of the number of available energy or quantum states since, by the Pauli exclusion principle, only one electron can occupy a given quantum state. When we discussed the splitting of energy levels into bands of allowed and forbidden energies, we indicated that the band of allowed energies was actually made up of discrete energy levels. We must determine the density of these allowed energy states as a function of energy in order to calculate the electron and hole concentrations. 3.4.1 Mathematical Derivation To determine the density of allowed quantum states as a function of energy, we need to consider an appropriate mathematical model. Electrons are allowed to move relatively freely in the conduction band of a semiconductor but are confined to the crystal. As a first step, we will consider a free electron confined to a three-dimensional infinite potential well, where the potential well represents the crystal. The potential of the infinite potential well is defined as V(x, y, z) 0 for 0 x a (3.59) 0ya 0za V(x, y, z) elsewhere where the crystal is assumed to be a cube with length a. Schrodinger’s wave equation in three dimensions can be solved by using the separation of variables technique. 2 See Appendix F for further discussion of effective mass concepts. nea29583_ch03_058-105.indd 85 12/11/10 10:09 AM 86 CHAPTER 3 Introduction to the Quantum Theory of Solids ky ky dk k k kx kx kx ⫹ 1 kz kx (b) (a) Figure 3.26 | (a) A two-dimensional array of allowed quantum states in k space. (b) The positive one-eighth of the spherical k space. Extrapolating the results from the one-dimensional infinite potential well, we can show (see Problem 3.23) that a 2 2m k2 k2 k2 k2 n2 n2 n2 _ _ x x y z y z 2 2 (3.60) where nx, ny, and nz are positive integers. (Negative values of nx, ny, and nz yield the same wave function, except for the sign, as the positive integer values, resulting in the same probability function and energy; therefore the negative integers do not represent a different quantum state.) We can schematically plot the allowed quantum states in k space. Figure 3.26a shows a two-dimensional plot as a function of kx and ky. Each point represents an allowed quantum state corresponding to various integral values of nx and ny. Positive and negative values of kx, ky, or kz have the same energy and represent the same energy state. Since negative values of kx, ky, or kz do not represent additional quantum states, the density of quantum states will be determined by considering only the positive one-eighth of the spherical k space as shown in Figure 3.26b. The distance between two quantum states in the kx direction, for example, is given by n _ _ kx1 kx (nx 1) _ (3.61) x a a a Generalizing this result to three dimensions, the volume Vk of a single quantum state is 3 Vk _ (3.62) a We can now determine the density of quantum states in k space. A differential volume in k space is shown in Figure 3.26b and is given by 4k2 dk, so the differential density of quantum states in k space can be written as 4k2 dk 1 __ gT (k) dk 2 _ 3 8 _ a nea29583_ch03_058-105.indd 86 (3.63) 12/11/10 10:09 AM 3.4 Density of States Function 87 The first factor, 2, takes into account the two spin states allowed for each quantum state; the next factor, _18 , takes into account that we are considering only the quantum states for positive values of kx, ky, and kz. The factor 4k2 dk is again the differential volume and the factor (/a)3 is the volume of one quantum state. Equation (3.63) may be simplified to k2 dk a3 gT (k) dk __ (3.64) 3 Equation (3.64) gives the density of quantum states as a function of momentum, through the parameter k. We can now determine the density of quantum states as a function of energy E. For a free electron, the parameters E and k are related by 2mE k2 _ (3.65a) 2 or ____ 1 2mE k_ (3.65b) The differential dk is 1 dk _ ___ m _ 2E dE (3.66) Then, substituting the expressions for k2 and dk into Equation (3.64), the number of energy states between E and E dE is given by a3 _ 2mE gT (E ) dE _ 2 3 Since ___ m dE _ 2E 1 _ (3.67) h2, Equation (3.67) becomes 3 __ 4a (2m)32 E dE gT (E ) dE _ h3 (3.68) Equation (3.68) gives the total number of quantum states between the energy E and E dE in the crystal space volume of a3. If we divide by the volume a3, then we will obtain the density of quantum states per unit volume of the crystal. Equation (3.68) then becomes 4(2m)32 __ g (E ) __ E h3 (3.69) The density of quantum states is a function of energy E. As the energy of this free electron becomes small, the number of available quantum states decreases. This density function is really a double density, in that the units are given in terms of states per unit energy per unit volume. Objective: Calculate the density of states per unit volume over a particular energy range. EXAMPLE 3.3 Consider the density of states for a free electron given by Equation (3.69). Calculate the density of states per unit volume with energies between 0 and 1 eV. nea29583_ch03_058-105.indd 87 12/11/10 10:09 AM 88 CHAPTER 3 Introduction to the Quantum Theory of Solids ■ Solution The volume density of quantum states, from Equation (3.69), is 1 eV 1 eV __ 4(2m)32 g(E) dE __ N E dE 3 or h 0 0 4(2m)32 _ 2 E 32 N __ 3 h3 The density of states is now 4[2(9.11 1031)]32 _ 2 (1.6 1019)32 4.5 1027 m3 N ____ 3 (6.625 1034)3 or N 4.5 1021 states/cm3 ■ Comment The density of quantum states is typically a large number. An effective density of states in a semiconductor, as we will see in the following sections and in the next chapter, is also a large number but is usually less than the density of atoms in the semiconductor crystal. ■ EXERCISE PROBLEM Ex 3.3 For a free electron, calculate the density of quantum states (#/cm3) over the energy range of (a) 0 E 2.0 eV and (b) 1 E 2 eV. [Ans. (a) N 1.28 10 22 cm−3; (b) N 8.29 10 21 cm−3] 3.4.2 Extension to Semiconductors In the previous section, we derived a general expression for the density of allowed electron quantum states using the model of a free electron with mass m bounded in a three-dimensional infinite potential well. We can extend this same general model to a semiconductor to determine the density of quantum states in the conduction band and the density of quantum states in the valence band. Electrons and holes are confined within the semiconductor crystal, so we will again use the basic model of the infinite potential well. The parabolic relationship between energy and momentum of a free electron is given in Equation (3.28) as E p22m 2k22m. Figure 3.16a shows the conduction energy band in the reduced k space. The E versus k curve near k 0 at the bottom of the conduction band can be approximated as a parabola, so we may write 2 2 k E Ec _ (3.70) 2mn* where Ec is the bottom edge of the conduction band and mn* is the electron density of states effective mass.3 Equation (3.70) may be rewritten to give 2 2 k E Ec _ (3.71) 2mn* 3 nea29583_ch03_058-105.indd 88 Again, see Appendix F for further discussion of effective mass concepts. 12/11/10 10:09 AM 3.4 Density of States Function 89 The general form of the E versus k relation for an electron in the bottom of a conduction band is the same as the free electron, except the mass is replaced by the effective mass. We can then think of the electron in the bottom of the conduction band as being a “free” electron with its own particular mass. The right side of Equation (3.71) is of the same form as the right side of Equation (3.28), which was used in the derivation of the density of states function. Because of this similarity, which yields the “free” conduction electron model, we may generalize the free electron results of Equation (3.69) and write the density of allowed electronic energy states in the conduction band as 4(2m*n)32 ______ gc(E) __ E Ec h3 (3.72) Equation (3.72) is valid for E Ec. As the energy of the electron in the conduction band decreases, the number of available quantum states also decreases. The density of quantum states in the valence band can be obtained by using the same infinite potential well model, since the hole is also confined in the semiconductor crystal and can be treated as a “free” particle. The density of states effective mass of the hole is m*p. Figure 3.16b shows the valence energy band in the reduced k space. We may also approximate the E versus k curve near k 0 by a parabola for a “free” hole, so that 2 2 k E Ev _ 2mp* (3.73) Equation (3.73) may be rewritten to give 2 2 k Ev E _ 2mp* (3.74) Again, the right side of Equation (3.74) is of the same form used in the general derivation of the density of states function. We may then generalize the density of states function from Equation (3.69) to apply to the valence band, so that 4(2m*p)32 ______ gv(E) __ Ev E h3 (3.75) Equation (3.75) is valid for E Ev. We have argued that quantum states do not exist within the forbidden energy band, so g(E) 0 for Ev E Ec. Figure 3.27 shows the plot of the density of quantum states as a function of energy. If the electron and hole effective masses were equal, then the functions gc(E) and gv(E) would be symmetrical about the energy midway between Ec and Ev, or the midgap energy, Emidgap. nea29583_ch03_058-105.indd 89 12/11/10 10:09 AM 90 CHAPTER 3 Introduction to the Quantum Theory of Solids gC (E) E EC EV gV (E) g(E) Figure 3.27 | The density of energy states in the conduction band and the density of energy states in the valence band as a function of energy. EXAMPLE 3.4 Objective: Determine the number (#/cm3) of quantum states in silicon between Ec and Ec kT at T 300 K. ■ Solution Using Equation (3.72), we can write E kT ______ 4 2m*n 32 E Ec dE __ N 3 h C EC 4 2m*n 32 _ 2 (E E )32 E kT __ c 3 E 3 h 31 32 4[2(1.08)(9.11 10 )] 2 (0.0259)(1.6 1019) _ _____ 3 (6.625 1034)3 c C 32 2.12 1025 m3 or N 2.12 1019 cm−3 ■ Comment The result of this example shows the order of magnitude of the density of quantum states in a semiconductor. ■ EXERCISE PROBLEM Ex3.4 Determine the number (#/cm3) of quantum states in silicon between (Ev kT) and Ev at T 300 K. (Ans. N 7.92 × 1018 cm−3) nea29583_ch03_058-105.indd 90 12/11/10 10:09 AM 3.5 Statistical Mechanics 91 3.5 | STATISTICAL MECHANICS In dealing with large numbers of particles, we are interested only in the statistical behavior of the group as a whole rather than in the behavior of each individual particle. For example, gas within a container will exert an average pressure on the walls of the vessel. The pressure is actually due to the collisions of the individual gas molecules with the walls, but we do not follow each individual molecule as it collides with the wall. Likewise in a crystal, the electrical characteristics will be determined by the statistical behavior of a large number of electrons. 3.5.1 Statistical Laws In determining the statistical behavior of particles, we must consider the laws that the particles obey. There are three distribution laws determining the distribution of particles among available energy states. One distribution law is the Maxwell–Boltzmann probability function. In this case, the particles are considered to be distinguishable by being numbered, for example, from 1 to N, with no limit to the number of particles allowed in each energy state. The behavior of gas molecules in a container at fairly low pressure is an example of this distribution. A second distribution law is the Bose–Einstein function. The particles in this case are indistinguishable and, again, there is no limit to the number of particles permitted in each quantum state. The behavior of photons, or black body radiation, is an example of this law. The third distribution law is the Fermi–Dirac probability function. In this case, the particles are again indistinguishable, but now only one particle is permitted in each quantum state. Electrons in a crystal obey this law. In each case, the particles are assumed to be noninteracting. 3.5.2 The Fermi–Dirac Probability Function Figure 3.28 shows the ith energy level with gi quantum states. A maximum of one particle is allowed in each quantum state by the Pauli exclusion principle. There are gi ways of choosing where to place the first particle, (gi 1) ways of choosing where to place the second particle, (gi 2) ways of choosing where to place the third particle, and so on. Then the total number of ways of arranging Ni particles in the ith energy level (where Ni gi) is gi! (3.76) (gi)(gi 1) (gi (Ni 1)) __ (gi Ni)! This expression includes all permutations of the Ni particles among themselves. ith energy level 1 2 3 . . . . . . gi Quantum states Figure 3.28 | The ith energy level with gi quantum states. nea29583_ch03_058-105.indd 91 12/11/10 10:09 AM 92 CHAPTER 3 Introduction to the Quantum Theory of Solids However, since the particles are indistinguishable, the Ni! number of permutations that the particles have among themselves in any given arrangement do not count as separate arrangements. The interchange of any two electrons, for example, does not produce a new arrangement. Therefore, the actual number of independent ways of realizing a distribution of Ni particles in the ith level is gi ! (3.77) Wi ___ Ni!(gi Ni)! EXAMPLE 3.5 Objective: Determine the possible number of ways of realizing a particular distribution for (a) gi Ni 10 and (b) gi 10, Ni 9. ■ Solution (a) gi Ni 10: We may note that (gi Ni)! 0! 1. Then, from Equation (3.77), we find gi! 10! 1 ___ _ Ni! (gi Ni)! 10! (b) gi 10, Ni 9: We may note that (gi − Ni)! 1! 1. Then, we find gi! (10) (9!) 10! __ ___ __ 10 Ni! (gi Ni)! (9!) (1) (9!) ■ Comment In part (a), we have 10 particles to be arranged in 10 quantum states. There is only one possible arrangement. Each quantum state contains one particle. In part (b), we have 9 particles to be arranged in 10 quantum states. There is one empty quantum state, and there are 10 possible positions in which that empty state may occur. Thus, there are 10 possible arrangements for this case. ■ EXERCISE PROBLEM Ex3.5 Determine the possible number of ways of realizing a particular distribution if gi 10 and Ni 8. (Ans. 45) Equation (3.77) gives the number of independent ways of realizing a distribution of Ni particles in the ith level. The total number of ways of arranging (N1, N2, N3, . . . , Nn) indistinguishable particles among n energy levels is the product of all distributions, or n W i1 gi! __ (3.78) Ni!(gi Ni)! The parameter W is the total number of ways in which N electrons can be arranged n in this system, where N i1 Ni is the total number of electrons in the system. We want to find the most probable distribution, which means that we want to find the maximum W. The maximum W is found by varying Ni among the Ei levels, which varies the distribution, but at the same time, we will keep the total number of particles and total energy constant. We may write the most probable distribution function as N(E) 1 _ fF (E) ___ g(E) EE 1 exp __F nea29583_ch03_058-105.indd 92 kT (3.79) 12/11/10 10:09 AM 3.5 Statistical Mechanics 93 The number density N(E) is the number of particles per unit volume per unit energy and the function g(E) is the number of quantum states per unit volume per unit energy. The function fF(E) is called the Fermi–Dirac distribution or probability function and gives the probability that a quantum state at the energy E will be occupied by an electron. The energy EF is called the Fermi energy. Another interpretation of the distribution function is that fF (E) is the ratio of filled to total quantum states at any energy E. 3.5.3 The Distribution Function and the Fermi Energy To begin to understand the meaning of the distribution function and the Fermi energy, we can plot the distribution function versus energy. Initially, let T ⫽ 0 K and consider the case when E ⬍ EF. The exponential term in Equation (3.79) becomes exp [(E ⫺ EF)kT] → exp (⫺⬁) ⫽ 0. The resulting distribution function is fF (E ⬍ EF) ⫽ 1. Again let T ⫽ 0 K and consider the case when E ⬎ EF. The exponential term in the distribution function becomes exp [(E − EF)kT ] → exp (⫹⬁) → ⫹⬁. The resulting Fermi–Dirac distribution function now becomes fF(E ⬎ EF) ⫽ 0. The Fermi–Dirac distribution function for T ⫽ 0 K is plotted in Figure 3.29. This result shows that, for T ⫽ 0 K, the electrons are in their lowest possible energy states. The probability of a quantum state being occupied is unity for E ⬍ EF and the probability of a state being occupied is zero for E ⬎ EF. All electrons have energies below the Fermi energy at T ⫽ 0 K. Figure 3.30 shows discrete energy levels of a particular system as well as the number of available quantum states at each energy. If we assume, for this case, that the system contains 13 electrons, then Figure 3.30 shows how these electrons are distributed among the various quantum states at T ⫽ 0 K. The electrons will be in the lowest possible energy state, so the probability of a quantum state being occupied in energy levels E1 through E4 is unity, and the probability of a quantum state being occupied in energy level E5 is zero. The Fermi energy, for this case, must be above E4 but less than E5. The Fermi energy determines the statistical distribution of electrons and does not have to correspond to an allowed energy level. Now consider a case in which the density of quantum states g(E) is a continuous function of energy, as shown in Figure 3.31. If we have N0 electrons in this system, E5 fF (E) E4 E3 1.0 E2 0 E1 E EF Figure 3.29 | The Fermi probability function versus energy for T ⫽ 0 K. nea29583_ch03_058-105.indd 93 Figure 3.30 | Discrete energy states and quantum states for a particular system at T ⫽ 0 K. 12/13/10 1:44 PM 94 CHAPTER 3 Introduction to the Quantum Theory of Solids g(E) E5 E4 g(E) or n(E) n(E) No ⫽ E3 0 g(E) dE EF E2 E1 E EF Figure 3.32 | Discrete energy states and quantum states for the same system shown in Figure 3.30 for T 0 K. Figure 3.31 | Density of quantum states and electrons in a continuous energy system at T 0 K. then the distribution of these electrons among the quantum states at T 0 K is shown by the dashed line. The electrons are in the lowest possible energy state so that all states below EF are filled and all states above EF are empty. If g(E) and N0 are known for this particular system, then the Fermi energy EF can be determined. Consider the situation when the temperature increases above T 0 K. Electrons gain a certain amount of thermal energy so that some electrons can jump to higher energy levels, which means that the distribution of electrons among the available energy states will change. Figure 3.32 shows the same discrete energy levels and quantum states as in Figure 3.30. The distribution of electrons among the quantum states has changed from the T 0 K case. Two electrons from the E4 level have gained enough energy to jump to E5, and one electron from E3 has jumped to E4. As the temperature changes, the distribution of electrons versus energy changes. The change in the electron distribution among energy levels for T 0 K can be seen by plotting the Fermi–Dirac distribution function. If we let E EF and T 0 K, then Equation (3.79) becomes 1 1 _ 1 fF(E EF) __ _ 1 exp (0) 1 1 2 The probability of a state being occupied at E EF is _12 . Figure 3.33 shows the Fermi–Dirac distribution function plotted for several temperatures, assuming that the Fermi energy is independent of temperature. T ⫽ T2 ⬎ T 1 T ⫽ T1 fF (E) 1.0 T⫽0 1 2 0 E EF Figure 3.33 | The Fermi probability function versus energy for different temperatures. nea29583_ch03_058-105.indd 94 12/11/10 10:09 AM 3.5 Statistical Mechanics 95 We can see that for temperatures above absolute zero, there is a nonzero probability that some energy states above EF will be occupied by electrons and some energy states below EF will be empty. This result again means that some electrons have jumped to higher energy levels with increasing thermal energy. Objective: Calculate the probability that an energy state above EF is occupied by an electron. EXAMPLE 3.6 Let T 300 K. Determine the probability that an energy level 3kT above the Fermi energy is occupied by an electron. ■ Solution From Equation (3.79), we can write 1 1 fF(E ) ___ ___ E EF 3kT __ 1 exp _ 1 exp kT kT which becomes 1 0.0474 4.74% fF (E ) __ 1 20.09 ■ Comment At energies above EF, the probability of a state being occupied by an electron can become significantly less than unity, or the ratio of electrons to available quantum states can be quite small. ■ EXERCISE PROBLEM Ex3.6 Assume the Fermi energy level is 0.30 eV below the conduction band energy Ec. Assume T 300 K. (a) Determine the probability of a state being occupied by an electron at E Ec kT4. (b) Repeat part (a) for an energy state at E Ec kT. [Ans. (a) 7.26 10 6; (b) 3.43 10 6] We can see from Figure 3.33 that the probability of an energy above EF being occupied increases as the temperature increases and the probability of a state below EF being empty increases as the temperature increases. Objective: Determine the temperature at which there is 1 percent probability that an energy EXAMPLE 3.7 state is empty. Assume that the Fermi energy level for a particular material is 6.25 eV and that the electrons in this material follow the Fermi–Dirac distribution function. Calculate the temperature at which there is a 1 percent probability that a state 0.30 eV below the Fermi energy level will not contain an electron. ■ Solution The probability that a state is empty is 1 1 fF (E ) 1 ____ 1 exp nea29583_ch03_058-105.indd 95 E kTE F __ 12/11/10 10:09 AM 96 CHAPTER 3 Introduction to the Quantum Theory of Solids Then 1 0.01 1 _____ 5.95 6.25 ___ 1 exp kT Solving for kT, we find kT 0.06529 eV, so that the temperature is T 756 K. ■ Comment The Fermi probability function is a strong function of temperature. ■ EXERCISE PROBLEM Ex 3.7 Assume that EF is 0.3 eV below Ec. Determine the temperature at which the probability of an electron occupying an energy state at E (Ec 0.025) eV is 8 106. (Ans. T 321 K) We may note that the probability of a state a distance dE above EF being occupied is the same as the probability of a state a distance dE below EF being empty. The function fF (E) is symmetrical with the function 1 − fF (E) about the Fermi energy, EF. This symmetry effect is shown in Figure 3.34 and will be used in the next chapter. Consider the case when E − EF kT, where the exponential term in the denominator of Equation (3.79) is much greater than unity. We may neglect the 1 in the denominator, so the Fermi–Dirac distribution function becomes (E EF) fF (E ) exp __ kT (3.80) Equation (3.80) is known as the Maxwell–Boltzmann approximation, or simply the Boltzmann approximation, to the Fermi–Dirac distribution function. Figure 3.35 shows the Fermi–Dirac probability function and the Boltzmann approximation. This figure gives an indication of the range of energies over which the approximation is valid. fF (E) 1 ⫺ fF (E) 1.0 1 2 E EF Figure 3.34 | The probability of a state being occupied, fF (E ), and the probability of a state being empty, 1 fF (E ). nea29583_ch03_058-105.indd 96 12/11/10 10:09 AM 3.5 Statistical Mechanics 97 Fermi–Dirac function 1.0 Boltzmann approximation 1 2 E EF Figure 3.35 | The Fermi–Dirac probability function and the Maxwell–Boltzmann approximation. Objective: Determine the energy at which the Boltzmann approximation may be considered EXAMPLE 3.8 valid. Calculate the energy, in terms of kT and EF, at which the difference between the Boltzmann approximation and the Fermi–Dirac function is 5 percent of the Fermi function. ■ Solution We can write (E EF) 1 ____ exp __ kT E EF 1 exp __ kT _______ 0.05 1 ____ E EF 1 exp __ kT If we multiply both numerator and denominator by the 1 exp ( ) function, we have (E EF) EE exp __ ⴢ 1 exp __F kT kT 1 0.05 which becomes (E EF) exp __ 0.05 kT or 1 3kT (E EF) kT ln _ 0.05 ■ Comment As seen in this example and in Figure 3.35, the E EF kT notation is somewhat misleading. The Maxwell–Boltzmann and Fermi–Dirac functions are within 5 percent of each other when E EF 3kT. ■ EXERCISE PROBLEM Ex 3.8 Repeat Example 3.8 for the case when the difference between the Boltzmann approximation and the Fermi–Dirac function is 2 percent of the Fermi function. (Ans. E EF 3.9kT) nea29583_ch03_058-105.indd 97 12/11/10 10:09 AM 98 CHAPTER 3 Introduction to the Quantum Theory of Solids The actual Boltzmann approximation is valid when exp [(E E,)kT] 1. However, it is still common practice to use the E EF kT notation when applying the Boltzmann approximation. We will use this Boltzmann approximation in our discussion of semiconductors in the next chapter. TEST YOUR UNDERSTANDING TYU 3.5 Assume that the Fermi energy level is 0.35 eV above the valence band energy. Let T 300 K. (a) Determine the probability of a state being empty of an electron at E Ev kT2. (b) Repeat part (a) for an energy state at E Ev 3kT2. [Ans. (a) 8.20 107; (b) 3.02 107] TYU 3.6 Repeat Exercise Problem Ex 3.6 for T 400 K. [Ans. (a) 1.31 104; (b) 6.21 105] TYU 3.7 Repeat Exercise Problem TYU 3.5 for T 400 K. [Ans. (a) 2.41 105; (b) 8.85 106] 3.6 | SUMMARY ■ ■ ■ ■ ■ ■ ■ Discrete allowed electron energies split into a band of allowed energies as atoms are brought together to form a crystal. The concept of allowed and forbidden energy bands was developed more rigorously by considering quantum mechanics and Schrodinger’s wave equation using the Kronig– Penney model representing the potential function of a single-crystal material. This result forms the basis of the energy-band theory of semiconductors. The concept of effective mass was developed. Effective mass relates the motion of a particle in a crystal to an externally applied force and takes into account the effect of the crystal lattice on the motion of the particle. Two charged particles exist in a semiconductor. An electron is a negatively charged particle with a positive effective mass existing at the bottom of an allowed energy band. A hole is a positively charged particle with a positive effective mass existing at the top of an allowed energy band. The E versus k diagrams of silicon and gallium arsenide were given and the concept of direct and indirect bandgap semiconductors was discussed. Energies within an allowed energy band are actually at discrete levels and each contains a finite number of quantum states. The density per unit energy of quantum states was determined by using the three-dimensional infinite potential well as a model. In dealing with large numbers of electrons and holes, we must consider the statistical behavior of these particles. The Fermi–Dirac probability function was developed, which gives the probability of a quantum state at an energy E of being occupied by an electron. The Fermi energy was defined. GLOSSARY OF IMPORTANT TERMS allowed energy band A band or range of energy levels that an electron in a crystal is allowed to occupy based on quantum mechanics. density of states function The density of available quantum states as a function of energy, given in units of number per unit energy per unit volume. nea29583_ch03_058-105.indd 98 12/11/10 10:09 AM Review Questions 99 electron effective mass The parameter that relates the acceleration of an electron in the conduction band of a crystal to an external force; a parameter that takes into account the effect of internal forces in the crystal. Fermi–Dirac probability function The function describing the statistical distribution of electrons among available energy states and the probability that an allowed energy state is occupied by an electron. fermi energy In the simplest definition, the energy below which all states are filled with electrons and above which all states are empty at T 0 K. forbidden energy band A band or range of energy levels that an electron in a crystal is not allowed to occupy based on quantum mechanics. hole The positively charged “particle” associated with an empty state in the top of the valence band. hole effective mass The parameter that relates the acceleration of a hole in the valence band of a crystal to an applied external force (a positive quantity); a parameter that takes into account the effect of internal forces in a crystal. k-space diagram The plot of electron energy in a crystal versus k, where k is the momentum-related constant of the motion that incorporates the crystal interaction. Kronig–Penney model The mathematical model of a periodic potential function representing a one-dimensional single-crystal lattice by a series of periodic step functions. Maxwell–Boltzmann approximation The condition in which the energy is several kT above the Fermi energy or several kT below the Fermi energy so that the Fermi–Dirac probability function can be approximated by a simple exponential function. CHECKPOINT After studying this chapter, the reader should have the ability to ■ ■ ■ ■ ■ ■ ■ ■ Discuss the concept of allowed and forbidden energy bands in a single crystal both qualitatively and more rigorously from the results of using the Kronig–Penney model. Discuss the splitting of energy bands in silicon. State the definition of effective mass from the E versus k diagram and discuss its meaning in terms of the movement of a particle in a crystal. Discuss the concept of a hole. Discuss the characteristics of a direct and an indirect bandgap semiconductor. Qualitatively, in terms of energy bands, discuss the difference between a metal, an insulator, and semiconductor. What is meant by the density of states function? Understand the meaning of the Fermi–Dirac distribution function and the Fermi energy. REVIEW QUESTIONS 1. 2. 3. 4. 5. What is the Kronig–Penney model? What does it represent? State two results of using the Kronig–Penney model with Schrodinger’s wave equation. What is effective mass? How is effective mass defined in terms of the E versus k diagram? What is a direct bandgap semiconductor? What is an indirect bandgap semiconductor? What is the meaning of the density of states function? nea29583_ch03_058-105.indd 99 12/11/10 10:09 AM 100 CHAPTER 3 6. 7. 8. 9. Introduction to the Quantum Theory of Solids What was the mathematical model used in deriving the density of states function? In general, what is the relation between density of states and energy? What is the meaning of the Fermi–Dirac probability function? What is the Fermi energy? PROBLEMS Section 3.1 Allowed and Forbidden Energy Bands 3.1 Consider Figure 3.4b, which shows the energy-band splitting of silicon. If the equilibrium lattice spacing were to change by a small amount, discuss how you would expect the electrical properties of silicon to change. Determine at what point the material would behave like an insulator or like a metal. 3.2 Show that Equations (3.4) and (3.6) are derived from Schrodinger’s wave equation, using the form of solution given by Equation (3.3). 3.3 Show that Equations (3.9) and (3.10) are solutions of the differential equations given by Equations (3.4) and (3.8), respectively. 3.4 Show that Equations (3.12), (3.14), (3.16), and (3.18) result from the boundary conditions in the Kronig–Penney model. 3.5 (a) Plot the function f (a) 12(sin a)a cos a for 0 a 4. Also, given the function f (a) cos ka, indicate the allowed values of a that will satisfy this equation. (b) Determine the values of a at (i) ka and (ii) ka 2. 3.6 Repeat Problem 3.5 for the function f(a) 5(sin a)a cos a cos ka. 3.7 Using Equation (3.24), show that dEdk 0 at k na, where n 0, 1, 2, . . . . 3.8 Using the parameters of Problem 3.5 for a free electron and letting a 4.2 Å, determine the width (in eV) of the forbidden energy bands that exist at (a) ka and (b) ka 2. (Refer to Figure 3.8c). 3.9 Using the parameters in Problem 3.5 for a free electron and letting a 4.2 Å, determine the width (in eV) of the allowed energy bands that exist for (a) 0 ka and (b) ka 2. 3.10 Repeat Problem 3.8 using the parameters in Problem 3.6. 3.11 Repeat Problem 3.9 using the parameters in Problem 3.6. 3.12 The bandgap energy in a semiconductor is usually a slight function of temperature. In some cases, the bandgap energy versus temperature can be modeled by T Eg Eg(0) __ ( T) 2 where Eg(0) is the value of the bandgap energy at T 0 K. For silicon, the parameter values are Eg(0) 1.170 eV, 4.73 104 eV/K, and 636 K. Plot Eg versus T over the range 0 T 600 K. In particular, note the value at T 300 K. Section 3.2 3.13 nea29583_ch03_058-105.indd 100 Electrical Conduction in Solids Two possible conduction bands are shown in the E versus k diagram given in Figure P3.13. State which band will result in the heavier electron effective mass; state why. 12/11/10 10:09 AM Problems E 101 E k B A k B A Figure P3.13 | Conduction bands for Problem 3.13. Figure P3.14 | Valence bands for Problem 3.14. E (eV) E 0.5 A D B 0.05 B A C 0 0 ⫺a k Figure P3.15 | Figure for Problem 3.15. 3.14 3.15 3.16 3.17 3.18 3.19 a ⫺0.08 0 0.08 k (Å⫺1) Figure P3.16 | Figure for Problem 3.16. Two possible valence bands are shown in the E versus k diagram given in Figure P3.14. State which band will result in the heavier hole effective mass; state why. The E versus k diagram for a particular allowed energy band is shown in Figure P3.15. Determine (a) the sign of the effective mass and (b) the direction of velocity for a particle at each of the four positions shown. Figure P3.16 shows the parabolic E versus k relationship in the conduction band for an electron in two particular semiconductor materials. Determine the effective mass (in units of the free electron mass) of the two electrons. Figure P3.17 shows the parabolic E versus k relationship in the valence band for a hole in two particular semiconductor materials. Determine the effective mass (in units of the free electron mass) of the two holes. (a) The forbidden bandgap energy in GaAs is 1.42 eV. (i) Determine the minimum frequency of an incident photon that can interact with a valence electron and elevate the electron to the conduction band. (ii) What is the corresponding wavelength? (b) Repeat part (a) for silicon with a bandgap energy of 1.12 eV. The E versus k diagrams for a free electron (curve A) and for an electron in a semiconductor (curve B) are shown in Figure P3.19. Sketch (a) dEdk versus k and (b) d2Edk2 versus k for each curve. (c) What conclusion can you make concerning a comparison in effective masses for the two cases? nea29583_ch03_058-105.indd 101 12/11/10 10:09 AM 102 CHAPTER 3 Introduction to the Quantum Theory of Solids E (eV) ⫺0.08 EV E 0 k (Å⫺1) 0.08 B A EV ⫺ 0.025 A B EV ⫺ 0.3 ⫺a 0 a k Figure P3.17 | Figure for Problem 3.17. Section 3.3 3.20 Figure P3.19 | Figure for Problem 3.19. Extension to Three Dimensions The energy-band diagram for silicon is shown in Figure 3.25b. The minimum energy in the conduction band is in the [100] direction. The energy in this one-dimensional direction near the minimum value can be approximated by E E0 E1 cos (k k0) where k0 is the value of k at the minimum energy. Determine the effective mass of the particle at k k0 in terms of the equation parameters. 3.21 The constant kinetic energy curves for electrons in the conduction band of germanium consists of four ellipsoids similar to those in silicon (see Appendix F). The longitudinal and transverse effective masses are ml 1.64m0 and mt 0.082m0, respectively. Determine the (a) density of states effective mass and (b) conductivity effective mass. 3.22 Heavy and light holes exist in GaAs with effective masses mhh 0.45m0 and mlh 0.082m0, respectively. Determine the (a) density of states effective mass and (b) conductivity effective mass. Section 3.4 3.23 3.24 3.25 3.26 3.27 3.28 nea29583_ch03_058-105.indd 102 Density of States Function Starting with the three-dimensional infinite potential well function given by Equation (3.59) and using the separation of variables technique, derive Equation (3.60). Show that Equation (3.69) can be derived from Equation (3.64). Derive the density of states function for a one-dimensional electron gas in GaAs (mn* 0.067m0). Note that the kinetic energy may be written as E ( p)22mn*, which means that there are two momentum states for each energy level. (a) Determine the total number (#/cm3) of energy states in silicon between Ec and Ec 2kT at (i) T 300 K and (ii) T 400 K. (b) Repeat part (a) for GaAs. (a) Determine the total number (#/cm3) of energy states in silicon between Ev and Ev 3 kT at (i) T 300 K and (ii) T 400 K. (b) Repeat part (a) for GaAs. (a) Plot the density of states in the conduction band of silicon over the range Ec E Ec 0.4 eV. (b) Repeat part (a) for the density of states in the valence band over the range Ev 0.4 eV E Ev. 12/11/10 10:09 AM Problems 3.29 (a) For silicon, find the ratio of the density of states in the conduction band at E Ec kT to the density of states in the valence band at E Ev kT. (b) Repeat part (a) for GaAs. Section 3.5 3.30 3.31 3.32 3.33 3.34 3.35 3.36 3.37 3.38 3.39 3.40 3.41 3.42 103 Statistical Mechanics Plot the Fermi–Dirac probability function, given by Equation (3.79), over the range 0.2 (E EF) 0.2 eV for (a) T 200 K, (b) T 300 K, and (c) T 400 K. (a) Repeat Example 3.5 for the case when gi 10 and Ni 7. (b) Repeat part (a) for (i) gi 12, Ni 10 and (ii) gi 12, Ni 8. Determine the probability that an energy level is occupied by an electron if the state is above the Fermi level by (a) kT, (b) 5kT, and (c) 10kT. Determine the probability that an energy level is empty of an electron if the state is below the Fermi level by (a) kT, (b) 5kT, and (c) 10kT. (a) The Fermi energy in silicon is 0.30 eV below the conduction band energy Ec at T 300 K. Plot the probability of a state being occupied by an electron in the conduction band over the range Ec E Ec 2kT. (b) The Fermi energy in silicon is 0.25 eV above the valence band energy Ev. Plot the probability of a state being empty by an electron in the valence band over the range Ev 2kT eV E Ev. The probability that a state at Ec kT is occupied by an electron is equal to the probability that a state at Ev kT is empty. Determine the position of the Fermi energy level as a function of Ec and Ev. Six free electrons exist in a one-dimensional infinite potential well of width a 12 Å. Determine the Fermi energy level at T 0 K. (a) Five free electrons exist in a three-dimensional infinite potential well with all three widths equal to a 12 Å. Determine the Fermi energy level at T 0 K. (b) Repeat part (a) for 13 electrons. Show that the probability of an energy state being occupied E above the Fermi energy is the same as the probability of a state being empty E below the Fermi level. (a) Determine for what energy above EF (in terms of kT ) the Fermi–Dirac probability function is within 1 percent of the Boltzmann approximation. (b) Give the value of the probability function at this energy. The Fermi energy level for a particular material at T 300 K is 5.50 eV. The electrons in this material follow the Fermi–Dirac distribution function. (a) Find the probability of an electron occupying an energy at 5.80 eV. (b) Repeat part (a) if the temperature is increased to T 700 K. (Assume that EF is a constant.) (c) Determine the temperature at which there is a 2 percent probability that a state 0.25 eV below the Fermi level will be empty of an electron. The Fermi energy for copper at T 300 K is 7.0 eV. The electrons in copper follow the Fermi–Dirac distribution function. (a) Find the probability of an energy level at 7.15 eV being occupied by an electron. (b) Repeat part (a) for T 1000 K. (Assume that EF is a constant.) (c) Repeat part (a) for E 6.85 eV and T 300 K. (d) Determine the probability of the energy state at E EF being occupied at T 300 K and at T 1000 K. Consider the energy levels shown in Figure P3.42. Let T 300 K. (a) If E1 EF 0.30 eV, determine the probability that an energy state at E E1 is occupied by nea29583_ch03_058-105.indd 103 12/11/10 10:09 AM 104 CHAPTER 3 Introduction to the Quantum Theory of Solids E1 Energy EF 1.12 eV E2 Figure P3.42 | Energy levels for Problem 3.42. 3.43 3.44 3.45 3.46 3.47 an electron and the probability that an energy state at E E2 is empty. (b) Repeat part (a) if EF E2 0.40 eV. Repeat problem 3.42 for the case when E1 E2 1.42 eV. Determine the derivative with respect to energy of the Fermi–Dirac distribution function. Plot the derivative with respect to energy for (a) T 0 K, (b) T 300 K, and (c) T 500 K. Assume that the Fermi energy level is exactly in the center of the bandgap energy of a semiconductor at T 300 K. (a) Calculate the probability that an energy state in the bottom of the conduction band is occupied by an electron for Si, Ge, and GaAs. (b) Calculate the probability that an energy state in the top of the valence band is empty for Si, Ge, and GaAs. (a) Calculate the temperature at which there is a 108 probability that an energy state 0.60 eV above the Fermi energy level is occupied by an electron. (b) Repeat part (a) for a probability of 106. Calculate the energy range (in eV) between fF 0.95 and fF 0.05 for EF 5.0 eV at (a) T 200 K and (b) T 400 K. READING LIST 1. 2. 3. 4. 5. *6. 7. *8. 9. 10. nea29583_ch03_058-105.indd 104 Dimitrijev, S. Principles of Semiconductor Devices. New York: Oxford University, 2006. Kano, K. Semiconductor Devices. Upper Saddle River, NJ: Prentice Hall, 1998. Kittel, C. Introduction to Solid State Physics, 7th ed. Berlin: Springer-Verlag, 1993. McKelvey, J. P. Solid State Physics for Engineering and Materials Science. Malabar, FL: Krieger, 1993. Pierret, R. F. Semiconductor Device Fundamentals. Reading, MA: Addison-Wesley, 1996. Shockley, W. Electrons and Holes in Semiconductors. New York: D. Van Nostrand, 1950. Shur, M. Introduction to Electronic Devices. New York: John Wiley and Sons, 1996. Shur, M. Physics of Semiconductor Devices. Englewood Cliffs, NJ: Prentice Hall, 1990. Singh, J. Semiconductor Devices: An Introduction. New York: McGraw-Hill, 1994. Singh, J. Semiconductor Devices: Basic Principles. New York: John Wiley and Sons, 2001. 12/11/10 10:09 AM Reading List 105 Streetman, B. G., and S. K. Banerjee. Solid State Electronic Devices, 6th ed. Upper Saddle River, NJ: Pearson Prentice Hall, 2006. 12. Sze, S. M. Semiconductor Devices: Physics and Technology, 2nd ed. New York: John Wiley and Sons, 2001. *13. Wang, S. Fundamentals of Semiconductor Theory and Device Physics. Englewood Cliffs, NJ: Prentice Hall, 1988. 14. Wolfe, C. M., N. Holonyak, Jr., and G. E. Stillman. Physical Properties of Semiconductors. Englewood Cliffs, NJ: Prentice Hall, 1989. 11. *Indicates references that are at an advanced level compared to this text. nea29583_ch03_058-105.indd 105 12/11/10 10:09 AM C 4 H A P T E R The Semiconductor in Equilibrium S o far, we have been considering a general crystal and applying to it the concepts of quantum mechanics in order to determine a few of the characteristics of electrons in a single-crystal lattice. In this chapter, we apply these concepts specifically to a semiconductor material. In particular, we use the density of quantum states in the conduction band and the density of quantum states in the valence band along with the Fermi–Dirac probability function to determine the concentration of electrons and holes in the conduction and valence bands, respectively. We also apply the concept of the Fermi energy to the semiconductor material. This chapter deals with the semiconductor in equilibrium. Equilibrium, or thermal equilibrium, implies that no external forces such as voltages, electric fields, magnetic fields, or temperature gradients are acting on the semiconductor. All properties of the semiconductor will be independent of time in this case. ■ 4.0 | PREVIEW In this chapter, we will: ■ Derive the thermal-equilibrium concentrations of electrons and holes in a semiconductor as a function of the Fermi energy level. ■ Discuss the process by which the properties of a semiconductor material can be favorably altered by adding specific impurity atoms to the semiconductor. ■ Determine the thermal-equilibrium concentrations of electrons and holes in a semiconductor as a function of the concentration of dopant atoms added to the semiconductor. ■ Determine the position of the Fermi energy level as a function of the concentrations of dopant atoms added to the semiconductor. 106 nea29583_ch04_106-155.indd 106 12/11/10 10:10 AM 4.1 Charge Carriers in Semiconductors 107 4.1 | CHARGE CARRIERS IN SEMICONDUCTORS Current is the rate at which charge flows. In a semiconductor, two types of charge carrier, the electron and the hole, can contribute to a current. Since the current in a semiconductor is determined largely by the number of electrons in the conduction band and the number of holes in the valence band, an important characteristic of the semiconductor is the density of these charge carriers. The density of electrons and holes is related to the density of states function and the Fermi distribution function, both of which we have considered. A qualitative discussion of these relationships will be followed by a more rigorous mathematical derivation of the thermal-equilibrium concentration of electrons and holes. 4.1.1 Equilibrium Distribution of Electrons and Holes The distribution (with respect to energy) of electrons in the conduction band is given by the density of allowed quantum states times the probability that a state is occupied by an electron. This statement is written in equation form as n(E) gc(E)fF (E) (4.1) where fF (E) is the Fermi–Dirac probability function and gc(E) is the density of quantum states in the conduction band. The total electron concentration per unit volume in the conduction band is then found by integrating Equation (4.1) over the entire conduction-band energy. Similarly, the distribution (with respect to energy) of holes in the valence band is the density of allowed quantum states in the valence band multiplied by the probability that a state is not occupied by an electron. We may express this as p(E) gv(E)[1 fF (E)] (4.2) The total hole concentration per unit volume is found by integrating this function over the entire valence-band energy. To find the thermal-equilibrium electron and hole concentrations, we need to determine the position of the Fermi energy EF with respect to the bottom of the conduction-band energy Ec and the top of the valence-band energy Ev. To address this question, we will initially consider an intrinsic semiconductor. An ideal intrinsic semiconductor is a pure semiconductor with no impurity atoms and no lattice defects in the crystal (e.g., pure silicon). We have argued in the previous chapter that, for an intrinsic semiconductor at T 0 K, all energy states in the valence band are filled with electrons and all energy states in the conduction band are empty of electrons. The Fermi energy must, therefore, be somewhere between Ec and Ev. (The Fermi energy does not need to correspond to an allowed energy.) As the temperature begins to increase above 0 K, the valence electrons will gain thermal energy. A few electrons in the valence band may gain sufficient energy to jump to the conduction band. As an electron jumps from the valence band to the conduction band, an empty state, or hole, is created in the valence band. In an intrinsic nea29583_ch04_106-155.indd 107 12/11/10 10:10 AM 108 CHAPTER 4 The Semiconductor in Equilibrium E gc(E)fF (E) n(E) gc(E) E fF (E) gc(E) Area n0 electron concentration Ec Ec fF (E) 0 (b) EF gv(E)(1 fF (E)) p(E) Ev [1 fF (E)] Ev gv(E) gv(E) E Area p0 hole concentration fF (E) 0 fF (E) 1 (a) (c) Figure 4.1 | (a) Density of states functions, Fermi–Dirac probability function, and areas representing electron and hole concentrations for the case when EF is near the midgap energy; (b) expanded view near the conduction-band energy; and (c) expanded view near the valence-band energy. semiconductor, then, electrons and holes are created in pairs by the thermal energy so that the number of electrons in the conduction band is equal to the number of holes in the valence band. Figure 4.1a shows a plot of the density of states function in the conduction-band gc(E), the density of states function in the valence-band gv(E), and the Fermi–Dirac probability function for T 0 K when EF is approximately halfway between Ec and Ev. If we assume, for the moment, that the electron and hole effective masses are equal, then gc(E) and gv(E) are symmetrical functions about the midgap energy (the energy midway between Ec and Ev). We noted previously that the function fF (E ) for E EF is symmetrical to the function 1 fF (E) for E EF about the energy E EF. This also means that the function fF(E) for E EF dE is equal to the function 1 fF (E ) for E EF dE. nea29583_ch04_106-155.indd 108 12/11/10 10:10 AM 4.1 Charge Carriers in Semiconductors 109 Figure 4.1b is an expanded view of the plot in Figure 4.1a showing fF (E) and gc(E) above the conduction-band energy Ec. The product of gc(E) and fF (E) is the distribution of electrons n(E ) in the conduction band given by Equation (4.1). This product is plotted in Figure 4.1a. Figure 4.1c, which is an expanded view of the plot in Figure 4.1a shows [1 fF (E)] and gv(E ) below the valence-band energy Ev. The product of gv(E) and [1 fF (E)] is the distribution of holes p(E) in the valence band given by Equation (4.2). This product is also plotted in Figure 4.1a. The areas under these curves are then the total density of electrons in the conduction band and the total density of holes in the valence band. From this we see that if gc(E ) and gv(E) are symmetrical, the Fermi energy must be at the midgap energy in order to obtain equal electron and hole concentrations. If the effective masses of the electron and hole are not exactly equal, then the effective density of states functions gc(E) and gv(E) will not be exactly symmetrical about the midgap energy. The Fermi level for the intrinsic semiconductor will then shift slightly from the midgap energy in order to obtain equal electron and hole concentrations. 4.1.2 The n0 and p0 Equations We have argued that the Fermi energy for an intrinsic semiconductor is near midgap. In deriving the equations for the thermal-equilibrium concentration of electrons n0 and the thermal-equilibrium concentration of holes p0, we will not be quite so restrictive. We will see later that, in particular situations, the Fermi energy can deviate from this midgap energy. We will assume initially, however, that the Fermi level remains within the bandgap energy. Thermal-Equilibrium Electron Concentration The equation for the thermalequilibrium concentration of electrons may be found by integrating Equation (4.1) over the conduction band energy, or n0 gc(E)fF (E) dE (4.3) The lower limit of integration is Ec and the upper limit of integration should be the top of the allowed conduction band energy. However, since the Fermi probability function rapidly approaches zero with increasing energy as indicated in Figure 4.1a, we can take the upper limit of integration to be infinity. We are assuming that the Fermi energy is within the forbidden-energy bandgap. For electrons in the conduction band, we have E Ec. If (Ec EF) kT, then (E EF) kT, so that the Fermi probability function reduces to the Boltzmann approximation,1 which is (E EF) 1 fF(E) ____ exp __ (4.4) (E EF) kT __ 1 exp kT 1 The Maxwell–Boltzmann and Fermi–Dirac distribution functions are within 5 percent of each other when E EF 3kT (see Figure 3.35). The notation is then somewhat misleading to indicate when the Boltzmann approximation is valid, although it is commonly used. nea29583_ch04_106-155.indd 109 12/11/10 10:10 AM 110 CHAPTER 4 The Semiconductor in Equilibrium Applying the Boltzmann approximation to Equation (4.3), the thermal-equilibrium density of electrons in the conduction band is found from 4 (2m*)32 ______ (E EF) n __ n0 dE (4.5) E Ec exp __ 3 kT h E c The integral of Equation (4.5) may be solved more easily by making a change of variable. If we let EE __c (4.6) kT then Equation (4.5) becomes 4 (2m*n kT)32 (Ec EF) 12 __ exp exp () d (4.7) n0 ___ kT h3 0 The integral is the gamma function, with a value of 1 __ 12 exp () d _ 2 (4.8) 0 Then Equation (4.7) becomes 2m*n kT n0 2 __ h2 We may define a parameter Nc as 32 (Ec EF) exp __ kT (4.9) 2m*n kT 32 Nc 2 __ (4.10) h2 The parameter mn* is the density of states effective mass of the electron. The thermalequilibrium electron concentration in the conduction band can be written as (Ec EF) n0 Nc exp __ kT (4.11) The parameter Nc is called the effective density of states function in the conduction band. If we were to assume that m*n m0, then the value of the effective density of states function at T 300 K is Nc 2.5 1019 cm3, which is the order of magnitude of Nc for most semiconductors. If the effective mass of the electron is larger or smaller than m0, then the value of the effective density of states function changes accordingly, but is still of the same order of magnitude. EXAMPLE 4.1 Objective: Calculate the probability that a quantum state in the conduction band at E Ec kT2 is occupied by an electron, and calculate the thermal-equilibrium electron concentration in silicon at T 300 K. Assume the Fermi energy is 0.25 eV below the conduction band. The value of Nc for silicon at T 300 K is Nc 2.8 1019 cm3 (see Appendix B). ■ Solution The probability that a quantum state at E Ec kT2 is occupied by an electron is given by 1 fF(E) ____ E EF 1 exp __ kT nea29583_ch04_106-155.indd 110 (Ec (kT2) EF) (E EF) exp ____ exp __ kT kT 12/11/10 10:10 AM 4.1 or Charge Carriers in Semiconductors 111 (0.25 (0.02592)) fF(E) exp ____ 3.90 105 0.0259 The electron concentration is given by (Ec EF) 0.25 n0 Nc exp __ (2.8 1019) exp __ kT 0.0259 or n0 1.80 1015 cm3 ■ Comment The probability of a state being occupied can be quite small, but the fact that there are a large number of states means that the electron concentration is a reasonable value. ■ EXERCISE PROBLEM Ex 4.1 Determine the probability that a quantum state at energy E Ec kT is occupied by an electron, and calculate the electron concentration in GaAs at T 300 K if the Fermi energy level is 0.25 eV below Ec. [Ans. fF(E) 2.36 105, n0 3.02 1013 cm3] Thermal-Equilibrium Hole Concentration The thermal-equilibrium concentration of holes in the valence band is found by integrating Equation (4.2) over the valence-band energy, or p0 gv(E)[1 fF (E)] dE (4.12) We may note that 1 1 fF(E) ___ EF E 1 exp __ kT (4.13a) For energy states in the valence band, E Ev. If (EF Ev) kT (the Fermi function is still assumed to be within the bandgap), then we have a slightly different form of the Boltzmann approximation. Equation (4.13a) may be written as 1 1 fF(E) ___ EF E 1 exp __ kT (EF E) exp __ kT (4.13b) Applying the Boltzmann approximation of Equation (4.13b) to Equation (4.12), we find the thermal-equilibrium concentration of holes in the valence band is E 4 (2m*)32 ______ (EF E) p __ p0 dE (4.14) Ev E exp __ kT h3 v where the lower limit of integration is taken as minus infinity instead of the bottom of the valence band. The exponential term decays fast enough so that this approximation is valid. nea29583_ch04_106-155.indd 111 12/11/10 10:10 AM 112 CHAPTER 4 The Semiconductor in Equilibrium Equation (4.14) may be solved more easily by again making a change of variable. If we let Ev E __ kT (4.15) then Equation (4.14) becomes 4(2m*p kT)32 (EF Ev) __ exp p0 ___ kT h3 0 ( )12 exp ( ) d (4.16) where the negative sign comes from the differential dE kTd . Note that the lower limit of becomes when E . If we change the order of integration, we introduce another minus sign. From Equation (4.8), Equation (4.16) becomes 2mp* kT 32 (EF Ev) p0 2 __ exp __ (4.17) kT h2 We may define a parameter Nv as 2m*p kT 32 Nv 2 __ (4.18) h2 which is called the effective density of states function in the valence band. The parameter m*p is the density of states effective mass of the hole. The thermalequilibrium concentration of holes in the valence band may now be written as (EF Ev) p0 Nv exp __ kT (4.19) The magnitude of Nv is also on the order of 1019 cm3 at T 300 K for most semiconductors. EXAMPLE 4.2 Objective: Calculate the thermal-equilibrium hole concentration in silicon at T 400 K. Assume that the Fermi energy is 0.27 eV above the valence-band energy. The value of Nv for silicon at T 300 K is Nv 1.04 1019 cm3. (See Appendix B) ■ Solution The parameter values at T 400 K are found as: 400 Nv (1.04 1019) _ 300 32 1.60 1019 cm3 and 400 0.03453 eV kT (0.0259) _ 300 The hole concentration is then (EF Ev) 0.27 p0 Nv exp __ (1.60 1019) exp __ kT 0.03453 or p0 6.43 1015 cm3 nea29583_ch04_106-155.indd 112 12/11/10 10:10 AM 4.1 Charge Carriers in Semiconductors 113 ■ Comment The parameter values at any temperature can easily be found by using the 300 K values and the temperature dependence. ■ EXERCISE PROBLEM Ex 4.2 (a) Repeat Example 4.2 at T 250 K. (b) What is the ratio of p0 at T 250 K to that at T 400 K? [Ans. (a) p0 2.92 1013 cm3; (b) 4.54 103] The effective density of states functions, Nc and Nv, are constant for a given semiconductor material at a fixed temperature. Table 4.1 gives the values of the density of states function and of the density of states effective masses for silicon, gallium arsenide, and germanium. Note that the value of Nc for gallium arsenide is smaller than the typical 1019 cm3 value. This difference is due to the small electron effective mass in gallium arsenide. The thermal-equilibrium concentrations of electrons in the conduction band and of holes in the valence band are directly related to the effective density of states constants and to the Fermi energy level. TEST YOUR UNDERSTANDING TYU 4.1 Calculate the thermal equilibrium electron and hole concentration in silicon at T 300 K for the case when the Fermi energy level is 0.22 eV below the conduction-band energy Ec. The value of Eg is given in Appendix B.4. TYU 4.2 Determine the thermal equilibrium electron and hole concentration in GaAs at T 300 K for the case when the Fermi energy level is 0.30 eV above the valence-band energy Ev. The value of Eg is given in Appendix B.4. (Ans. n0 5.73 1015 cm3, p0 8.43 103 cm3) (Ans. n0 0.0779 cm3, p0 6.53 1013 cm3) 4.1.3 The Intrinsic Carrier Concentration For an intrinsic semiconductor, the concentration of electrons in the conduction band is equal to the concentration of holes in the valence band. We may denote ni and pi as the electron and hole concentrations, respectively, in the intrinsic semiconductor. These parameters are usually referred to as the intrinsic electron concentration and intrinsic hole concentration. However, ni pi, so normally we simply use the parameter ni as the intrinsic carrier concentration, which refers to either the intrinsic electron or hole concentration. Table 4.1 | Effective density of states function and density of states effective mass values Silicon Gallium arsenide Germanium nea29583_ch04_106-155.indd 113 Nc (cm−3) Nv (cm−3) mn*兾m0 mp*兾m0 2.8 10 4.7 1017 1.04 1019 1.04 10 7.0 1018 6.0 1018 1.08 0.067 0.55 0.56 0.48 0.37 19 19 12/11/10 10:10 AM 114 CHAPTER 4 The Semiconductor in Equilibrium The Fermi energy level for the intrinsic semiconductor is called the intrinsic Fermi energy, or EF EFi. If we apply Equations (4.11) and (4.19) to the intrinsic semiconductor, then we can write (Ec EFi) n0 ni Nc exp __ (4.20) kT and (EFi Ev) p0 pi ni Nv exp __ (4.21) kT If we take the product of Equations (4.20) and (4.21), we obtain (Ec EFi) (EFi Ev) n2i Nc Nv exp __ exp __ kT kT (4.22) (4.23) or Eg (Ec Ev) Nc Nv exp _ n2i Nc Nv exp __ kT kT where Eg is the bandgap energy. For a given semiconductor material at a constant temperature, the value of ni is a constant, and independent of the Fermi energy. The intrinsic carrier concentration for silicon at T 300 K may be calculated by using the effective density of states function values from Table 4.1. The value of ni calculated from Equation (4.23) for Eg 1.12 eV is ni 6.95 109 cm3. The commonly accepted value2 of ni for silicon at T 300 K is approximately 1.5 1010 cm3. This discrepancy may arise from several sources. First, the values of the effective masses are determined at a low temperature where the cyclotron resonance experiments are performed. Since the effective mass is an experimentally determined parameter, and since the effective mass is a measure of how well a particle moves in a crystal, this parameter may be a slight function of temperature. Next, the density of states function for a semiconductor was obtained by generalizing the model of an electron in a three-dimensional infinite potential well. This theoretical function may also not agree exactly with experiment. However, the difference between the theoretical value and the experimental value of ni is approximately a factor of 2, which, in many cases, is not significant. Table 4.2 lists the commonly accepted values of ni for silicon, gallium arsenide, and germanium at T 300 K. The intrinsic carrier concentration is a very strong function of temperature. Table 4.2 | Commonly accepted values of ni at T 300 K Silicon Gallium arsenide Germanium ni 1.5 1010 cm3 ni 1.8 106 cm3 ni 2.4 1013 cm3 2 Various references may list slightly different values of the intrinsic silicon concentration at room temperature. In general, they are all between 1 1010 and 1.5 1010 cm3. This difference is, in most cases, not significant. nea29583_ch04_106-155.indd 114 12/11/10 10:10 AM 4.1 Charge Carriers in Semiconductors 115 Calculate the intrinsic carrier concentration in silicon at T 250 K and at T 400 K. The values of Nc and Nv for silicon at T 300 K are 2.8 1019 cm3 and 1.04 1019 3 cm , respectively. Both Nc and Nv vary as T 32. Assume the bandgap energy of silicon is 1.12 eV and does not vary over this temperature range. EXAMPLE 4.3 Objective: ■ Solution Using Equation (4.23), we find, at T 250 K 250 3 exp ___ 1.12 n2i (2.8 1019)(1.04 1019) _ 300 (0.0259)(250300) 4.90 1015 or ni 7.0 107 cm3 At T 400 K, we find 400 3 exp ____ 1.12 n2i (2.8 1019)(1.04 1019) _ 300 (0.0259)(400300) 5.67 1024 or ni 2.38 1012 cm3 ■ Comment We may note from this example that the intrinsic carrier concentration increased by over 4 orders of magnitude as the temperature increased by 150°C. ■ EXERCISE PROBLEM Ex 4.3 (a) Calculate the intrinsic carrier concentration in GaAs at T 400 K and at T 250 K. Assume that Eg 1.42 eV is constant over this temperature range. (b) What is the ratio of ni at T 400 K to that at T 250 K? [Ans. (a) ni(400) 3.29 109 cm3, ni(250) 7.13 103 cm3; (b) 4.61 105] Figure 4.2 is a plot of ni from Equation (4.23) for silicon, gallium arsenide, and germanium as a function of temperature. As seen in the figure, the value of ni for these semiconductors may easily vary over several orders of magnitude as the temperature changes over a reasonable range. TEST YOUR UNDERSTANDING TYU 4.3 Calculate the intrinsic concentration in silicon at (a) T 200 K and (b) T 450 K. (c) Determine the ratio of ni at T 450 K to that at T 200 K. TYU 4.4 Repeat TYU 4.3 for GaAs. TYU 4.5 Repeat TYU 4.3 for Ge. [Ans. (a) ni 7.63 104 cm3; (b) ni 1.72 1013 cm3; (c) 2.26 108] [Ans. (a) ni 1.37 cm3; (b) ni 3.85 1010 cm3; (c) 2.81 1010] [Ans. (a) ni 2.15 1010 cm3; (b) ni 2.97 1015 cm3; (c) 1.38 105] nea29583_ch04_106-155.indd 115 12/11/10 10:10 AM 116 CHAPTER 4 The Semiconductor in Equilibrium T(•C) 200 100 1500 1000 500 19 10 27 0—20 1018 1017 Ge Intrinsic carrier density ni (cm3) 1016 1015 Si 1014 1013 1012 1011 1010 GaAs 109 108 107 106 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0 1000T(K 1) Figure 4.2 | The intrinsic carrier concentration of Ge, Si, and GaAs as a function of temperature. (From Sze [14].) 4.1.4 The Intrinsic Fermi-Level Position We have qualitatively argued that the Fermi energy level is located near the center of the forbidden bandgap for the intrinsic semiconductor. We can specifically calculate the intrinsic Fermi-level position. Since the electron and hole concentrations are equal, setting Equations (4.20) and (4.21) equal to each other, we have (Ec EFi) (EFi Ev) Nc exp __ Nv exp __ kT kT nea29583_ch04_106-155.indd 116 (4.24) 12/11/10 10:10 AM 4.1 Charge Carriers in Semiconductors 117 If we take the natural log of both sides of this equation and solve for EFi, we obtain Nv 1 (E E ) _ 1 kT ln _ EFi _ (4.25) v Nc 2 c 2 From the definitions for Nc and Nv given by Equations (4.10) and (4.18), respectively, Equation (4.25) may be written as m*p 3 kT ln _ 1 (E E ) _ EFi _ (4.26a) c v mn* 2 4 1 _ The first term, 2 (Ec Ev), is the energy exactly midway between Ec and Ev, or the midgap energy. We can define 1 (E E ) E _ v midgap 2 c so that m*p 3 kT ln _ EFi Emidgap _ m*n 4 (4.26b) If the electron and hole effective masses are equal so that m*p m*n , then the intrinsic Fermi level is exactly in the center of the bandgap. If m*p m*n , the intrinsic Fermi level is slightly above the center, and if m*p m*n , it is slightly below the center of the bandgap. The density of states function is directly related to the carrier effective mass; thus, a larger effective mass means a larger density of states function. The intrinsic Fermi level must shift away from the band with the larger density of states in order to maintain equal numbers of electrons and holes. Objective: Calculate the position of the intrinsic Fermi level with respect to the center of EXAMPLE 4.4 the bandgap in silicon at T 300 K. The density of states effective carrier masses in silicon are m*n 1.08m0 and mp* 0.56m0. ■ Solution The intrinsic Fermi level with respect to the center of the bandgap is m*p 3 kT ln _ 3 (0.0259) ln _ 0.56 EFi Emidgap _ _ m*n 4 4 1.08 or EFi Emidgap 0.0128 eV 12.8 meV ■ Comment The intrinsic Fermi level in silicon is 12.8 meV below the midgap energy. If we compare 12.8 meV to 560 meV, which is one-half of the bandgap energy of silicon, we can, in many applications, simply approximate the intrinsic Fermi level to be in the center of the bandgap. ■ EXERCISE PROBLEM Ex 4.4 Determine the position of the intrinsic Fermi level at T 300 K with respect to the center of the bandgap for (a) GaAs and (b) Ge. [Ans. (a) 38.25 meV; (b) 7.70 meV] nea29583_ch04_106-155.indd 117 12/11/10 10:10 AM 118 CHAPTER 4 The Semiconductor in Equilibrium TEST YOUR UNDERSTANDING TYU 4.6 Determine the position of the intrinsic Fermi level with respect to the center of the bandgap in silicon at (a) T 200 K and (b) T 400 K. Assume the effective masses are constant over this temperature range. [Ans. (a) 8.505 meV; (b) 17.01meV] 4.2 | DOPANT ATOMS AND ENERGY LEVELS The intrinsic semiconductor may be an interesting material, but the real power of semiconductors is realized by adding small, controlled amounts of specific dopant, or impurity, atoms. This doping process, described briefly in Chapter 1, can greatly alter the electrical characteristics of the semiconductor. The doped semiconductor, called an extrinsic material, is the primary reason we can fabricate the various semiconductor devices that we will consider in later chapters. 4.2.1 Qualitative Description In Chapter 3, we discussed the covalent bonding of silicon and considered the simple two-dimensional representation of the single-crystal silicon lattice as shown in Figure 4.3. Now consider adding a group V element, such as phosphorus, as a substitutional impurity. The group V element has five valence electrons. Four of these will contribute to the covalent bonding with the silicon atoms, leaving the fifth more loosely bound to the phosphorus atom. This effect is schematically shown in Figure 4.4. We refer to the fifth valence electron as a donor electron. The phosphorus atom without the donor electron is positively charged. At very low temperatures, the donor electron is bound to the phosphorus atom. However, by intuition, it should seem clear that the energy required to elevate the donor electron into the conduction band is considerably less than that for the electrons involved in the covalent bonding. Figure 4.5 shows the energy-band diagram that we would expect. The energy level, Ed, is the energy state of the donor electron. Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si P Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si e Si Si Si Si Si Figure 4.3 | Two-dimensional representation of the intrinsic silicon lattice. nea29583_ch04_106-155.indd 118 Figure 4.4 | Two-dimensional representation of the silicon lattice doped with a phosphorus atom. 12/11/10 10:10 AM 4.2 ⴚ Ec Ed Ev Valence band ⴚ ⴙ Electron energy Conduction band Electron energy Dopant Atoms and Energy Levels ⴚ ⴙ 119 Ec Ed ⴙ Ev (a) (b) Figure 4.5 | The energy-band diagram showing (a) the discrete donor energy state and (b) the effect of a donor state being ionized. If a small amount of energy, such as thermal energy, is added to the donor electron, it can be elevated into the conduction band, leaving behind a positively charged phosphorus ion. The electron in the conduction band can now move through the crystal generating a current, while the positively charged ion is fixed in the crystal. This type of impurity atom donates an electron to the conduction band and so is called a donor impurity atom. The donor impurity atoms add electrons to the conduction band without creating holes in the valence band. The resulting material is referred to as an n-type semiconductor (n for the negatively charged electron). Now consider adding a group III element, such as boron, as a substitutional impurity to silicon. The group III element has three valence electrons, which are all taken up in the covalent bonding. As shown in Figure 4.6a, one covalent bonding position appears to be empty. If an electron were to occupy this “empty” position, its energy would have to be greater than that of the valence electrons, since the net charge state of the boron atom would now be negative. However, the electron occupying this “empty” position does not have sufficient energy to be in the conduction band, so its energy is far smaller than the conduction-band energy. Figure 4.6b shows how valence electrons may gain a small amount of thermal energy and move about in Si Si Si Si Si Si Si Si Si Si Si Si Si Si B Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si Si (a) Si Si B Si Si Si Si Si Si Si Si (b) Figure 4.6 | Two-dimensional representation of a silicon lattice (a) doped with a boron atom and (b) showing the ionization of the boron atom resulting in a hole. nea29583_ch04_106-155.indd 119 12/11/10 10:10 AM 120 CHAPTER 4 The Semiconductor in Equilibrium Conduction band Ec Valence band (a) Ea Ev Electron energy Electron energy Ec ⴚ ⴙ ⴚ ⴚ ⴙ ⴙ Ea Ev (b) Figure 4.7 | The energy-band diagram showing (a) the discrete acceptor energy state and (b) the effect of an acceptor state being ionized. the crystal. The “empty” position associated with the boron atom becomes occupied, and other valence electron positions become vacated. These other vacated electron positions can be thought of as holes in the semiconductor material. Figure 4.7 shows the expected energy state of the “empty” position and also the formation of a hole in the valence band. The hole can move through the crystal generating a current, while the negatively charged boron atom is fixed in the crystal. The group III atom accepts an electron from the valence band and so is referred to as an acceptor impurity atom. The acceptor atom can generate holes in the valence band without generating electrons in the conduction band. This type of semiconductor material is referred to as a p type material (p for the positively charged hole). The pure single-crystal semiconductor material is called an intrinsic material. Adding controlled amounts of dopant atoms, either donors or acceptors, creates a material called an extrinsic semiconductor. An extrinsic semiconductor will have either a preponderance of electrons (n type) or a preponderance of holes (p type). 4.2.2 Ionization Energy We can calculate the approximate distance of the donor electron from the donor impurity ion, and also the approximate energy required to elevate the donor electron into the conduction band. This energy is referred to as the ionization energy. We will use the Bohr model of the atom for these calculations. The justification for using this model is that the most probable distance of an electron from the nucleus in a hydrogen atom, determined from quantum mechanics, is the same as the Bohr radius. The energy levels in the hydrogen atom determined from quantum mechanics are also the same as obtained from the Bohr theory. In the case of the donor impurity atom, we may visualize the donor electron orbiting the donor ion, which is embedded in the semiconductor material. We will need to use the permittivity of the semiconductor material in the calculations rather than the permittivity of free space as is used in the case of the hydrogen atom. We will also use the effective mass of the electron in the calculations. nea29583_ch04_106-155.indd 120 12/11/10 10:10 AM 4.2 Dopant Atoms and Energy Levels 121 The analysis begins by setting the coulomb force of attraction between the electron and ion equal to the centripetal force of the orbiting electron. This condition will give a steady orbit. We have 2 2 m*v e __ _ 4 r rn 2 n (4.27) where v is the magnitude of the velocity and rn is the radius of the orbit. If we assume the angular momentum is also quantized, then we can write m* rnv n (4.28) where n is a positive integer. Solving for v from Equation (4.28), substituting into Equation (4.27), and solving for the radius, we obtain n 4 rn __ (4.29) m*e2 The assumption of the angular momentum being quantized leads to the radius also being quantized. The Bohr radius is defined as 40 2 a0 __ 0.53 Å (4.30) m0e2 We can normalize the radius of the donor orbital to that of the Bohr radius, which gives 2 2 m* m0 rn _ _ 2 a n r 0 (4.31) where r is the relative dielectric constant of the semiconductor material, m0 is the rest mass of an electron, and m* is the conductivity effective mass of the electron in the semiconductor.3 If we consider the lowest energy state in which n 1, and if we consider silicon in which r 11.7 and the conductivity effective mass is m*m0 0.26, then we have that r1 _ (4.32) a0 45 or r1 23.9 Å. This radius corresponds to approximately four lattice constants of silicon. Recall that one unit cell in silicon effectively contains eight atoms, so the radius of the orbiting donor electron encompasses many silicon atoms. The donor electron is not tightly bound to the donor atom. The total energy of the orbiting electron is given by ETV (4.33) where T is the kinetic energy and V is the potential energy of the electron. The kinetic energy is 1 m*v2 (4.34) T_ 2 3 The conductivity effective mass is used when electrons and holes are in motion. See Appendix F for a discussion of effective mass concepts. nea29583_ch04_106-155.indd 121 12/11/10 10:10 AM 122 CHAPTER 4 The Semiconductor in Equilibrium Using the velocity v from Equation (4.28) and the radius rn from Equation (4.29), the kinetic energy becomes m*e4 T ___ (4.35) 2(n )2(4)2 The potential energy is m*e4 e2 __ (4.36) V_ 4rn (n )2(4)2 The total energy is the sum of the kinetic and potential energies, so that m*e4 E T V ___ (4.37) 2(n )2(4)2 For the hydrogen atom, m* m0 and 0. The ionization energy of the hydrogen atom in the lowest energy state is then E 13.6 eV. If we consider silicon, the ionization energy is E 25.8 meV, much less than the bandgap energy of silicon. This energy is the approximate ionization energy of the donor atom, or the energy required to elevate the donor electron into the conduction band. For ordinary donor impurities such as phosphorus or arsenic in silicon or germanium, this hydrogenic model works quite well and gives some indication of the magnitudes of the ionization energies involved. Table 4.3 lists the actual experimentally measured ionization energies for a few impurities in silicon and germanium. Germanium and silicon have different relative dielectric constants and effective masses; thus, we expect the ionization energies to differ. 4.2.3 Group III–V Semiconductors In the previous sections, we have discussed the donor and acceptor impurities in a group IV semiconductor, such as silicon. The situation in the group III–V compound semiconductors, such as gallium arsenide, is more complicated. Group II elements, such as beryllium, zinc, and cadmium, can enter the lattice as substitutional impurities, replacing the group III gallium element to become acceptor impurities. Similarly, group VI elements, such as selenium and tellurium, can enter the lattice substitutionally, replacing the group V arsenic element to become donor impurities. The corresponding ionization energies for these impurities are smaller than those for the impurities in silicon. The ionization energies for the donors in gallium arsenide Table 4.3 | Impurity ionization energies in silicon and germanium Impurity Donors Phosphorus Arsenic Acceptors Boron Aluminum nea29583_ch04_106-155.indd 122 Ionization energy (eV) Si Ge 0.045 0.05 0.012 0.0127 0.045 0.06 0.0104 0.0102 12/11/10 10:10 AM 4.3 The Extrinsic Semiconductor 123 Table 4.4 | Impurity ionization energies in gallium arsenide Impurity Donors Selenium Tellurium Silicon Germanium Acceptors Beryllium Zinc Cadmium Silicon Germanium Ionization energy (eV) 0.0059 0.0058 0.0058 0.0061 0.028 0.0307 0.0347 0.0345 0.0404 are also smaller than those for the acceptors, because of the smaller effective mass of the electron compared to that of the hole. Group IV elements, such as silicon and germanium, can also be impurity atoms in gallium arsenide. If a silicon atom replaces a gallium atom, the silicon impurity will act as a donor, but if the silicon atom replaces an arsenic atom, then the silicon impurity will act as an acceptor. The same is true for germanium as an impurity atom. Such impurities are called amphoteric. Experimentally in gallium arsenide, it is found that germanium is predominantly an acceptor and silicon is predominantly a donor. Table 4.4 lists the ionization energies for the various impurity atoms in gallium arsenide. TEST YOUR UNDERSTANDING TYU 4.7 (a) Calculate the ionization energy and the radius (normalized to the Bohr radius) of a donor electron in its lowest energy state in GaAs. (b) Repeat part (a) for Ge. [Ans. (a) 5.30 meV, r1a0 195.5; (b) 6.37 meV, r1a0 133.3] 4.3 | THE EXTRINSIC SEMICONDUCTOR We defined an intrinsic semiconductor as a material with no impurity atoms present in the crystal. An extrinsic semiconductor is defined as a semiconductor in which controlled amounts of specific dopant or impurity atoms have been added so that the thermal-equilibrium electron and hole concentrations are different from the intrinsic carrier concentration. One type of carrier will predominate in an extrinsic semiconductor. 4.3.1 Equilibrium Distribution of Electrons and Holes Adding donor or acceptor impurity atoms to a semiconductor will change the distribution of electrons and holes in the material. Since the Fermi energy is related to the distribution function, the Fermi energy will change as dopant atoms are added. nea29583_ch04_106-155.indd 123 12/11/10 10:10 AM 124 CHAPTER 4 The Semiconductor in Equilibrium E gc(E) Ec EF Area n0 electron concentration fF (E) EFi Ev gv(E) fF (E) 0 Area p0 hole concentration fF (E) 1 Figure 4.8 | Density of states functions, Fermi–Dirac probability function, and areas representing electron and hole concentrations for the case when EF is above the intrinsic Fermi energy. If the Fermi energy changes from near the midgap value, the density of electrons in the conduction band and the density of holes in the valence band will change. These effects are shown in Figures 4.8 and 4.9. Figure 4.8 shows the case for EF EFi and Figure 4.9 shows the case for EF EFi. When EF EFi, the electron concentration is larger than the hole concentration, and when EF EFi, the hole concentration is larger than the electron concentration. When the density of electrons is greater than the density of holes, the semiconductor is n type; donor impurity atoms have been added. When the density of holes is greater than the density of electrons, the semiconductor is p type; acceptor impurity atoms have been added. The Fermi energy level in a semiconductor changes as the electron and hole concentrations change and, again, the Fermi energy changes as donor or acceptor impurities are added. The change in the Fermi level as a function of impurity concentrations is considered in Section 4.6. nea29583_ch04_106-155.indd 124 12/11/10 10:10 AM 4.3 The Extrinsic Semiconductor 125 E gc(E) Ec Area n0 electron concentration fF (E) EFi EF Ev gv(E) Area p0 hole concentration fF (E) 0 fF (E) 1 Figure 4.9 | Density of states functions, Fermi–Dirac probability function, and areas representing electron and hole concentrations for the case when EF is below the intrinsic Fermi energy. The expressions previously derived for the thermal-equilibrium concentration of electrons and holes, given by Equations (4.11) and (4.19), are general equations for n0 and p0 in terms of the Fermi energy. These equations are again given as (Ec EF) n0 Nc exp __ kT and (EF Ev) p0 Nv exp __ kT As we just discussed, the Fermi energy may vary through the bandgap energy, which will then change the values of n0 and p0. nea29583_ch04_106-155.indd 125 12/11/10 10:10 AM 126 CHAPTER 4 The Semiconductor in Equilibrium EXAMPLE 4.5 Objective: Calculate the thermal equilibrium concentrations of electrons and holes for a given Fermi energy. Consider silicon at T 300 K so that Nc 2.8 1019 cm3 and Nv 1.04 1019 cm3. Assume that the Fermi energy is 0.25 eV below the conduction band. If we assume that the bandgap energy of silicon is 1.12 eV, then the Fermi energy will be 0.87 eV above the valence band. ■ Solution Using Equation (4.11), we have 0.25 1.8 1015 cm3 n0 (2.8 1019) exp __ 0.0259 From Equation (4.19), we can write 0.87 2.7 104 cm3 p0 (1.04 1019) exp __ 0.0259 ■ Comment The change in the Fermi level is actually a function of the donor or acceptor impurity concentrations that are added to the semiconductor. However, this example shows that electron and hole concentrations change by orders of magnitude from the intrinsic carrier concentration as the Fermi energy changes by a few tenths of an electron-volt. ■ EXERCISE PROBLEM Ex 4.5 Determine the thermal-equilibrium concentrations of electrons and holes in silicon at T 300 K if the Fermi energy level is 0.215 eV above the valence-band energy Ev. (Ans. p0 2.58 l0 l5 cm3, n0 1.87 10 4 cm3) In the previous example, since n0 p0, the semiconductor is n type. In an n-type semiconductor, electrons are referred to as the majority carrier and holes as the minority carrier. By comparing the relative values of n0 and p0 in the example, it is easy to see how this designation came about. Similarly, in a p-type semiconductor where p0 n0, holes are the majority carrier and electrons are the minority carrier. We may derive another form of the equations for the thermal-equilibrium concentrations of electrons and holes. If we add and subtract an intrinsic Fermi energy in the exponent of Equation (4.11), we can write (Ec EFi) (EF EFi) n0 Nc exp _____ kT (4.38a) or (Ec EFi) (EF EFi) n0 Nc exp __ exp __ kT kT (4.38b) The intrinsic carrier concentration is given by Equation (4.20) as (Ec EFi) ni Nc exp __ kT nea29583_ch04_106-155.indd 126 12/11/10 10:10 AM 4.3 The Extrinsic Semiconductor 127 so that the thermal-equilibrium electron concentration can be written as EF EFi n0 ni exp __ kT (4.39) Similarly, if we add and subtract an intrinsic Fermi energy in the exponent of Equation (4.19), we will obtain (EF EFi) p0 ni exp ___ kT (4.40) As we will see, the Fermi level changes when donors and acceptors are added, but Equations (4.39) and (4.40) show that, as the Fermi level changes from the intrinsic Fermi level, n0 and p0 change from the ni value. If EF EFi, then we will have n0 ni and p0 ni. One characteristic of an n-type semiconductor is that EF EFi so that n0 p0. Similarly, in a p-type semiconductor, EF EFi so that p0 ni and n0 ni; thus, p0 n0. We can see the functional dependence of n0 and p0 with EF in Figures 4.8 and 4.9. As EF moves above or below EFi, the overlapping probability function with the density of states functions in the conduction band and valence band changes. As EF moves above EFi, the probability function in the conduction band increases, while the probability, 1 fF (E ), of an empty state (hole) in the valence band decreases. As EF moves below EFi, the opposite occurs. 4.3.2 The n0 p0 Product We may take the product of the general expressions for n0 and p0 as given in Equations (4.11) and (4.19), respectively. The result is (Ec EF) (EF Ev) n0 p0 Nc Nv exp __ exp __ (4.41) kT kT which may be written as Eg n0 p0 Nc Nv exp _ kT (4.42) As Equation (4.42) was derived for a general value of Fermi energy, the values of n0 and p0 are not necessarily equal. However, Equation (4.42) is exactly the same as Equation (4.23), which we derived for the case of an intrinsic semiconductor. We then have that, for the semiconductor in thermal equilibrium, n0 p0 n2i (4.43) Equation (4.43) states that the product of n0 and p0 is always a constant for a given semiconductor material at a given temperature. Although this equation seems nea29583_ch04_106-155.indd 127 12/11/10 10:10 AM 128 CHAPTER 4 The Semiconductor in Equilibrium very simple, it is one of the fundamental principles of semiconductors in thermal equilibrium. The significance of this relation will become more apparent in the chapters that follow. It is important to keep in mind that Equation (4.43) was derived using the Boltzmann approximation. If the Boltzmann approximation is not valid, then likewise, Equation (4.43) is not valid. An extrinsic semiconductor in thermal equilibrium does not, strictly speaking, contain an intrinsic carrier concentration, although some thermally generated carriers are present. The intrinsic electron and hole carrier concentrations are modified by the donor or acceptor impurities. However, we may think of the intrinsic concentration ni in Equation (4.43) simply as a parameter of the semiconductor material. *4.3.3 The Fermi–Dirac Integral In the derivation of the Equations (4.11) and (4.19) for the thermal equilibrium electron and hole concentrations, we assumed that the Boltzmann approximation was valid. If the Boltzmann approximation does not hold, the thermal equilibrium electron concentration is written from Equation (4.3) as (E Ec)12 dE 4 (2m*)32 ___ n0 _ (4.44) n 3 E EF h E 1 exp __ kT If we again make a change of variable and let c EE __c kT (4.45a) and also define EF Ec F __ kT then we can rewrite Equation (4.44) as 12 d 2m*n kT 32 ___ n0 4 __ 2 1 exp ( F) h The integral is defined as F12 (F) 0 (4.45b) (4.46) 0 d ___ 12 1 exp ( F) (4.47) This function, called the Fermi–Dirac integral, is a tabulated function of the variable F. Figure 4.10 is a plot of the Fermi–Dirac integral. Note that if F 0, then EF Ec; thus, the Fermi energy is actually in the conduction band. EXAMPLE 4.6 Objective: Calculate the electron concentration using the Fermi–Dirac integral. Let F 2 so that the Fermi energy is above the conduction band by approximately 52 meV at T 300 K. ■ Solution Equation (4.46) can be written as 2__ N F ( ) n0 _ c 12 F nea29583_ch04_106-155.indd 128 12/11/10 10:10 AM 4.3 The Extrinsic Semiconductor 129 For silicon at T 300 K, Nc 2.8 1019 cm3 and, from Figure 4.10, the Fermi–Dirac integral has a value or F12 (2) 2.7. Then 2__ 2.8 1019 2.7 8.53 1019 cm3 n0 _ ■ Comment Note that if we had used Equation (4.11), the thermal equilibrium value of n0 would be n0 2.08 1020 cm3, which is incorrect since the Boltzmann approximation is not valid for this case. ■ EXERCISE PROBLEM If n0 1.5 1020 cm3 in silicon at T 300 K, determine the position of the Fermi level relative to the conduction-band energy Ec. (Ans. EF Ec Ex 4.6 0.08288 eV) We may use the same general method to calculate the thermal equilibrium concentration of holes. We obtain 2m*p kT 32 ____ ( )12 d p0 4 __ (4.48) 2 1 exp ( F) h 0 10 冢 2 冣 exp(F) Fermi–Dirac integral (F12) 1 101 102 x 12 d F12(F) 0 103 6 4 1 exp( F ) 2 0 (EF Ec)kT 2 F 4 6 Figure 4.10 | The Fermi–Dirac integral F12 as a function of the Fermi energy. (From Sze [14].) nea29583_ch04_106-155.indd 129 12/11/10 10:10 AM 130 CHAPTER 4 The Semiconductor in Equilibrium where Ev E __ kT (4.49a) Ev E F __F kT (4.49b) and The integral in Equation (4.48) is the same Fermi–Dirac integral defined by Equation (4.47), although the variables have slightly different definitions. We may note that if F 0, then the Fermi level is in the valence band. TEST YOUR UNDERSTANDING TYU 4.8 (a) Calculate the thermal-equilibrium electron concentration in silicon at T 300 K for the case when EF Ec. (b) Calculate the thermal-equilibrium hole concentration in silicon at T 300 K for the case when EF Ev. [Ans. (a) n0 2.05 10 19 cm3; (b) p0 7.63 10 18 cm3] 4.3.4 Degenerate and Nondegenerate Semiconductors In our discussion of adding dopant atoms to a semiconductor, we have implicitly assumed that the concentration of dopant atoms added is small when compared to the density of host or semiconductor atoms. The small number of impurity atoms are spread far enough apart so that there is no interaction between donor electrons, for example, in an n-type material. We have assumed that the impurities introduce discrete, noninteracting donor energy states in the n-type semiconductor and discrete, noninteracting acceptor states in the p-type semiconductor. These types of semiconductors are referred to as nondegenerate semiconductors. If the impurity concentration increases, the distance between the impurity atoms decreases and a point will be reached when donor electrons, for example, will begin to interact with each other. When this occurs, the single discrete donor energy will split into a band of energies. As the donor concentration further increases, the band of donor states widens and may overlap the bottom of the conduction band. This overlap occurs when the donor concentration becomes comparable with the effective density of states. When the concentration of electrons in the conduction band exceeds the density of states Nc, the Fermi energy lies within the conduction band. This type of semiconductor is called a degenerate n-type semiconductor. In a similar way, as the acceptor doping concentration increases in a p-type semiconductor, the discrete acceptor energy states will split into a band of energies and may overlap the top of the valence band. The Fermi energy will lie in the valence band when the concentration of holes exceeds the density of states Nv. This type of semiconductor is called a degenerate p-type semiconductor. Schematic models of the energy-band diagrams for a degenerate n-type and degenerate p-type semiconductor are shown in Figure 4.11. The energy states below EF nea29583_ch04_106-155.indd 130 12/11/10 10:10 AM 4.4 Statistics of Donors and Acceptors Conduction band Conduction band EF Ec Ec Filled states (electrons) Ev Valence band Empty states (holes) Electron energy Electron energy 131 Ev Valence band EF (b) (a) Figure 4.11 | Simplified energy-band diagrams for degenerately doped (a) n-type and (b) p-type semiconductors. are mostly filled with electrons and the energy states above EF are mostly empty. In the degenerate n-type semiconductor, the states between EF and Ec are mostly filled with electrons; thus, the electron concentration in the conduction band is very large. Similarly, in the degenerate p-type semiconductor, the energy states between Ev and EF are mostly empty; thus, the hole concentration in the valence band is very large. 4.4 | STATISTICS OF DONORS AND ACCEPTORS In the previous chapter, we discussed the Fermi–Dirac distribution function, which gives the probability that a particular energy state will be occupied by an electron. We need to reconsider this function and apply the probability statistics to the donor and acceptor energy states. 4.4.1 Probability Function One postulate used in the derivation of the Fermi–Dirac probability function was the Pauli exclusion principle, which states that only one particle is permitted in each quantum state. The Pauli exclusion principle also applies to the donor and acceptor states. Suppose we have Ni electrons and gi quantum states, where the subscript i indicates the ith energy level. There are gi ways of choosing where to put the first particle. Each donor level has two possible spin orientations for the donor electron; thus, each donor level has two quantum states. The insertion of an electron into one quantum state, however, precludes putting an electron into the second quantum state. By adding one electron, the vacancy requirement of the atom is satisfied, and the addition of a second electron in the donor level is not possible. The distribution function of donor electrons in the donor energy states is then slightly different than the Fermi–Dirac function. The probability function of electrons occupying the donor state is Nd nd ____ Ed EF 1 exp __ 1_ 2 kT nea29583_ch04_106-155.indd 131 (4.50) 12/11/10 10:10 AM 132 CHAPTER 4 The Semiconductor in Equilibrium where nd is the density of electrons occupying the donor level and Ed is the energy of the donor level. The factor _12 in this equation is a direct result of the spin factor just mentioned. The _12 factor is sometimes written as 1g, where g is called a degeneracy factor. Equation (4.50) can also be written in the form nd Nd N d (4.51) d where N is the concentration of ionized donors. In many applications, we will be interested more in the concentration of ionized donors than in the concentration of electrons remaining in the donor states. If we do the same type of analysis for acceptor atoms, we obtain the expression Na pa ____ EF Ea Na N a 1 _ __ 1 g exp kT (4.52) where Na is the concentration of acceptor atoms, Ea is the acceptor energy level, pa is the concentration of holes in the acceptor states, and N a is the concentration of ionized acceptors. A hole in an acceptor state corresponds to an acceptor atom that is neutrally charged and still has an “empty” bonding position as we have discussed in Section 4.2.1. The parameter g is, again, a degeneracy factor. The ground state degeneracy factor g is normally taken as 4 for the acceptor level in silicon and gallium arsenide because of the detailed band structure. 4.4.2 Complete Ionization and Freeze-Out The probability function for electrons in the donor energy state was just given by Equation (4.50). If we assume that (Ed EF) kT, then nd Nd (Ed EF) ___ 2Nd exp __ kT E E d 1 exp __F _ 2 kT (4.53) If (Ed EF) kT, then the Boltzmann approximation is also valid for the electrons in the conduction band so that, from Equation (4.11), (Ec EF) n0 Nc exp __ kT We can determine the relative number of electrons in the donor state compared with the total number of electrons; therefore, we can consider the ratio of electrons in the donor state to the total number of electrons in the conduction band plus donor state. Using the expressions of Equations (4.53) and (4.11), we write (Ed EF) 2Nd exp __ n kT d __ ________ nd n0 E ) (E (Ec EF) d F 2Nd exp __ Nc exp __ kT kT nea29583_ch04_106-155.indd 132 (4.54) 12/11/10 10:10 AM 4.4 Statistics of Donors and Acceptors 133 The Fermi energy cancels out of this expression. Dividing by the numerator term, we obtain nd 1 __ _____ nd n0 (Ec Ed) Nc _ 1 exp __ 2Nd kT (4.55) The factor (Ec Ed) is just the ionization energy of the donor electrons. Objective: Determine the fraction of total electrons still in the donor states at T 300 K. EXAMPLE 4.7 Consider phosphorus doping in silicon, for T 300 K, at a concentration of Nd 1016 cm3. ■ Solution Using Equation (4.55), we find nd 1 __ 0.0041 0.41% _____ n0 nd 2.8 1019 exp __ 0.045 1 __ 0.0259 2(1016) ■ Comment This example shows that there are very few electrons in the donor state compared with the conduction band. Essentially all of the electrons from the donor states are in the conduction band and, since only about 0.4 percent of the donor states contain electrons, the donor states are said to be completely ionized. ■ EXERCISE PROBLEM Ex 4.7 Repeat Example 4.7 for (a) T 250 K and (b) T 200 K. (c) What can be said about the fraction as the temperature decreases? [Ans. (a) 7.50 103; (b) 1.75 102; (c) Fraction increases as temperature decreases.] At room temperature, then, the donor states are essentially completely ionized and, for a typical doping of 1016 cm3, almost all donor impurity atoms have donated an electron to the conduction band. At room temperature, there is also essentially complete ionization of the acceptor atoms. This means that each acceptor atom has accepted an electron from the valence band so that pa is zero. At typical acceptor doping concentrations, a hole is created in the valence band for each acceptor atom. This ionization effect and the creation of electrons and holes in the conduction band and valence band, respectively, are shown in Figure 4.12. The opposite of complete ionization occurs at T 0 K. At absolute zero degrees, all electrons are in their lowest possible energy state; that is, for an n-type semiconductor, each donor state must contain an electron, therefore nd Nd or Nd 0. We must have, then, from Equation (4.50) that exp [(Ed EF)kT] 0. Since T 0 K, this will occur for exp () 0, which means that EF Ed. The Fermi energy level must be above the donor energy level at absolute zero. In the case of a p-type semiconductor at absolute zero temperature, the impurity atoms will not contain any electrons, so that the Fermi energy level must be below the acceptor energy state. The distribution of electrons among the various energy states, and hence the Fermi energy, is a function of temperature. nea29583_ch04_106-155.indd 133 12/11/10 10:10 AM ⴚ ⴚ ⴙ ⴙ The Semiconductor in Equilibrium Conduction band ⴚ ⴚ ⴚ ⴚ ⴙ ⴙ ⴙ ⴙ Conduction band ⴚ ⴙ Ec Ed EFi Ev Valence band Ec Electron energy CHAPTER 4 Electron energy 134 EFi ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ E a ⴙ ⴙ ⴙ ⴙ ⴙ Valence band ⴙ ⴙ (a) Ev (b) Figure 4.12 | Energy-band diagrams showing complete ionization of (a) donor states and (b) acceptor states. Conduction band Conduction band Ec Ed EFi Valence band Ev Ec Electron energy Electron energy EF EFi EF Valence band (a) Ea Ev (b) Figure 4.13 | Energy-band diagram at T 0 K for (a) n-type and (b) p-type semiconductors. A detailed analysis, not given in this text, shows that at T 0 K, the Fermi energy is halfway between Ec and Ed for the n-type material and halfway between Ea and Ev for the p-type material. Figure 4.13 shows these effects. No electrons from the donor state are thermally elevated into the conduction band; this effect is called freeze-out. Similarly, when no electrons from the valance band are elevated into the acceptor states, the effect is also called freeze-out. Between T 0 K, freeze-out, and T 300 K, complete ionization, we have partial ionization of donor or acceptor atoms. EXAMPLE 4.8 Objective: Determine the temperature at which 90 percent of acceptor atoms are ionized. Consider p-type silicon doped with boron at a concentration of Na 1016 cm3. ■ Solution Find the ratio of holes in the acceptor state to the total number of holes in the valence band plus acceptor state. Taking into account the Boltzmann approximation and assuming the degeneracy factor is g 4, we write pa 1 __ _____ p0 pa (Ea Ev) Nv _ exp __ 1 4Na kT nea29583_ch04_106-155.indd 134 12/11/10 10:10 AM 4.5 Charge Neutrality 135 For 90 percent ionization, pa 1 __ 0.10 ________ p0 pa T 32 (1.04 1019) _ 300 0.045 1 ____ ⴢ exp ___ T 4(1016) 0.0259 _ 300 Using trial and error, we find that T 193 K. ■ Comment This example shows that at approximately 100 C below room temperature, we still have 90 percent of the acceptor atoms ionized; in other words, 90 percent of the acceptor atoms have “donated” a hole to the valence band. ■ EXERCISE PROBLEM Ex 4.8 Determine the fraction of total holes still in the acceptor states in silicon for Na 1016 cm3 at (a) T 250 K and (b) T 200 K. [Ans. (a) 3.91 102; (b) 8.736 102] TEST YOUR UNDERSTANDING TYU 4.9 Determine the fraction of total holes still in the acceptor states in silicon at T 300 K for a boron impurity concentration of Na 1017 cm3. TYU 4.10 Consider silicon with a phosphorus impurity concentration of Nd 1015 cm3. Determine the percent of ionized phosphorus atoms at (a) T 100 K, (b) T 200 K, (c) T 300 K, and (d) T 400 K. (Ans. 0.179) [Ans. (a) 93.62%; (b) 99.82%; (c) 99.96%; (d) 99.98%] 4.5 | CHARGE NEUTRALITY In thermal equilibrium, the semiconductor crystal is electrically neutral. The electrons are distributed among the various energy states, creating negative and positive charges, but the net charge density is zero. This charge-neutrality condition is used to determine the thermal-equilibrium electron and hole concentrations as a function of the impurity doping concentration. We will define a compensated semiconductor and then determine the electron and hole concentrations as a function of the donor and acceptor concentrations. 4.5.1 Compensated Semiconductors A compensated semiconductor is one that contains both donor and acceptor impurity atoms in the same region. A compensated semiconductor can be formed, for example, by diffusing acceptor impurities into an n-type material or by diffusing donor impurities into a p-type material. An n-type compensated semiconductor occurs when Nd Na, and a p-type compensated semiconductor occurs when Na Nd. If Na Nd, we have a completely compensated semiconductor that has, as we will show, the characteristics of an intrinsic material. Compensated semiconductors are created quite naturally during device fabrication as we will see later. nea29583_ch04_106-155.indd 135 12/11/10 10:10 AM 136 CHAPTER 4 The Semiconductor in Equilibrium Total electron concentration Thermal electrons Donor electrons n0 ⴚⴚⴚ ⴚ ⴚ ⴚ ⴚ Ec ⴙ ⴙ ⴙ ⴙ ⴙ Un-ionized donors Nd (Nd nd) Ionized donors Un-ionized acceptors Na (Na pa) Ionized acceptors ⴚ ⴚ ⴙⴙⴙ Thermal holes p0 Total hole concentration ⴙ Ed EFi ⴚ ⴚ ⴚ ⴚ ⴙ ⴙ ⴙ ⴙ Ea Ev Acceptor holes Figure 4.14 | Energy-band diagram of a compensated semiconductor showing ionized and un-ionized donors and acceptors. 4.5.2 Equilibrium Electron and Hole Concentrations Figure 4.14 shows the energy-band diagram of a semiconductor when both donor and acceptor impurity atoms are added to the same region to form a compensated semiconductor. The figure shows how the electrons and holes can be distributed among the various states. The charge neutrality condition is expressed by equating the density of negative charges to the density of positive charges. We then have n0 N a p0 Nd (4.56) n0 (Na pa) p0 (Nd nd) (4.57) or where n0 and p0 are the thermal-equilibrium concentrations of electrons and holes in the conduction band and valence band, respectively. The parameter nd is the concentration of electrons in the donor energy states, so Nd Nd nd is the concentration of positively charged donor states. Similarly, pa is the concentration of holes in the acceptor states, so N a Na pa is the concentration of negatively charged acceptor states. We have expressions for n0, p0, nd, and pa in terms of the Fermi energy and temperature. nea29583_ch04_106-155.indd 136 12/11/10 10:10 AM 4.5 Charge Neutrality 137 Thermal-Equilibrium Electron Concentration If we assume complete ionization, nd and pa are both zero, and Equation (4.57) becomes n0 Na p0 nd (4.58) If we express p0 as n n0, then Equation (4.58) can be written as n2i n0 Na _ n0 Nd 2 i (4.59a) which in turn can be written as n20 (Nd Na)n0 n2i 0 (4.59b) The electron concentration n0 can be determined using the quadratic formula, or (Nd Na) n0 __ 2 ______________ N N n 2 __ d a 2 2 i (4.60) The positive sign in the quadratic formula must be used, since, in the limit of an intrinsic semiconductor when Na Nd 0, the electron concentration must be a positive quantity, or n0 ni. Equation (4.60) is used to calculate the electron concentration in an n-type semiconductor, or when Nd Na. Although Equation (4.60) was derived for a compensated semiconductor, the equation is also valid for Na 0. Objective: Determine the thermal-equilibrium electron and hole concentrations EXAMPLE 4.9 in silicon at T 300 K for given doping concentrations. (a) Let Nd 1016 cm3 and Na 0. (b) Let Nd 5 1015 cm3 and Na 2 1015 cm3. Recall that ni 1.5 1010 cm3 in silicon at T 300 K. ■ Solution (a) From Equation (4.60), the majority carrier electron concentration is ____________________ 16 10 n0 _ 2 10 1.5 10 2 _ 16 2 10 2 1016 cm3 The minority carrier hole concentration is found to be n2i (1.5 1010) 2 __ p0 _ 2.25 104 cm3 n0 1016 (b) Again, from Equation (4.60), the majority carrier electron concentration is 5 10 2 10 n0 ____ 2 15 15 ________________________________ 5 10 2 10 (1.5 10 ) 2 ____ 15 15 2 10 2 3 1015 cm3 The minority carrier hole concentration is n2 (1.5 1010) 2 3 10 i ___ 7.5 104 cm3 p0 _ 15 n 0 nea29583_ch04_106-155.indd 137 12/11/10 10:10 AM 138 CHAPTER 4 The Semiconductor in Equilibrium ■ Comment In both parts of this example, (Nd Na) ni, so the thermal-equilibrium majority carrier electron concentration is essentially equal to the difference between the donor and acceptor concentrations. Also, in both cases, the majority carrier electron concentration is orders of magnitude larger than the minority carrier hole concentration. ■ EXERCISE PROBLEM Ex 4.9 Find the thermal-equilibrium electron and hole concentrations in silicon with doping concentrations of Na 7 1015 cm3 and Na 3 1015 cm3 for (a) T 250 K and (b) T 400 K. 1.416 109 cm3] [Ans. (a) n0 4 1015 cm3, p0 1.225 cm3; (b) n0 4 1015 cm3, p0 We have argued in our discussion and we may note from the results of Example 4.9 that the concentration of electrons in the conduction band increases above the intrinsic carrier concentration as we add donor impurity atoms. At the same time, the minority carrier hole concentration decreases below the intrinsic carrier concentration as we add donor atoms. We must keep in mind that as we add donor impurity atoms and the corresponding donor electrons, there is a redistribution of electrons among available energy states. Figure 4.15 shows a schematic of this physical redistribution. A few of the donor electrons will fall into the empty states in the valence band and, in doing so, will annihilate some of the intrinsic holes. The minority carrier hole concentration will therefore decrease as we have seen in Example 4.9. At the Intrinsic electrons ⴚⴚⴚⴚⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ Ec ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ Ionized donors Ed Un-ionized donors EFi A few donor electrons annihilate some intrinsic holes ⴙ ⴙ ⴙ ⴙ Intrinsic holes Ev ni2 Net p0 n 0 Figure 4.15 | Energy-band diagram showing the redistribution of electrons when donors are added. nea29583_ch04_106-155.indd 138 12/11/10 10:10 AM 4.5 Charge Neutrality 139 same time, because of this redistribution, the net electron concentration in the conduction band is not simply equal to the donor concentration plus the intrinsic electron concentration. Objective: Calculate the thermal-equilibrium electron and hole concentrations in germanium for a given doping concentration. Consider a germanium sample at T 300 K in which Nd 2 1014 cm3 and Na 0. Assume that ni 2.4 1013 cm3. EXAMPLE 4.10 ■ Solution Again, from Equation (4.60), the majority carrier electron concentration is 2 10 n0 __ 2 14 ________________________ 2.4 10 2 __ 2 1014 2 13 2 2.028 1014 cm3 The minority carrier hole concentration is n2i 2.4 1013 2 ___ 12 3 p0 _ n0 2.028 1014 2.84 10 cm ■ Comment If the donor impurity concentration is not too different in magnitude from the intrinsic carrier concentration, then the thermal-equilibrium majority carrier electron concentration is influenced by the intrinsic concentration. ■ EXERCISE PROBLEM Ex 4.10 Repeat Example 4.10 for (a) T 250 K and (b) T 350 K. (c) What can be said about a very low-doped material as the temperature increases? [Ans. (a) n0 2 1014 cm3, p0 9.47 109 cm3; (b) n0 3.059 1014 cm3, p0 1.059 1014 cm3; (c) Material approaches an intrinsic semiconductor] We have seen that the intrinsic carrier concentration ni is a very strong function of temperature. As the temperature increases, additional electron–hole pairs are thermally generated so that the n2i term in Equation (4.60) may begin to dominate. The semiconductor will eventually lose its extrinsic characteristics. Figure 4.16 shows the electron concentration versus temperature in silicon doped with 5 1014 donors per cm3 . As the temperature increases, we can see where the intrinsic concentration begins to dominate. Also shown is the partial ionization, or the onset of freeze-out, at the low temperature. Thermal-Equilibrium Hole Concentration If we reconsider Equation (4.58) and express n0 as n2i p0, then we have n2i _ (4.61a) p0 Na p0 Nd which we can write as p20 (Na Nd)p0 n2i 0 nea29583_ch04_106-155.indd 139 (4.61b) 12/11/10 10:10 AM 140 CHAPTER 4 The Semiconductor in Equilibrium 1016 Intrinsic 1015 Extrinsic n0 (cm3) 5 1014 Partial ionization 1013 ni 1012 100 200 300 400 T (K) 500 600 700 Figure 4.16 | Electron concentration versus temperature showing the three regions: partial ionization, extrinsic, and intrinsic. Using the quadratic formula, the hole concentration is given by Na Nd p0 __ 2 ______________ N N n 2 __ a d 2 2 i (4.62) where the positive sign, again, must be used. Equation (4.62) is used to calculate the thermal-equilibrium majority carrier hole concentration in a p-type semiconductor, or when Na Nd. This equation also applies for Nd 0. EXAMPLE 4.11 Objective: Calculate the thermal-equilibrium electron and hole concentrations in a compensated p-type semiconductor. Consider a silicon semiconductor at T 300 K in which Na 1016 cm3 and Nd 3 15 10 cm3. Assume ni 1.5 1010 cm3. ■ Solution Since Na Nd, the compensated semiconductor is p-type and the thermal-equilibrium majority carrier hole concentration is given by Equation (4.62) as 1016 3 1015 p0 ___ 2 so that _____________________________ 10 3 10 (1.5 10 ) 2 ___ 16 15 2 10 2 p0 7 1015 cm3 The minority carrier electron concentration is n2i (1.5 1010)2 ___ 4 3 n0 _ p0 7 1015 3.21 10 cm ■ Comment If we assume complete ionization and if (Na Nd) ni, then the majority carrier hole concentration is, to a very good approximation, just the difference between the acceptor and donor concentrations. nea29583_ch04_106-155.indd 140 12/11/10 10:10 AM 4.6 Position of Fermi Energy Level 141 ■ EXERCISE PROBLEM Ex 4.11 Consider silicon at T 300 K. Calculate the thermal-equilibrium electron and hole concentrations for impurity concentrations of (a) Na 4 1016 cm3, Nd 8 1015 cm3 and (b) Na Nd 3 1015 cm3. [Ans. (a) p0 3.2 1016 cm3, n0 7.03 103 cm3; (b) p0 n0 1.5 1010 cm3] We may note that, for a compensated p-type semiconductor, the minority carrier electron concentration is determined from n2i n2i __ n0 _ p0 (Na Nd) Equations (4.60) and (4.62) are used to calculate the majority carrier electron concentration in an n-type semiconductor and majority carrier hole concentration in a p-type semiconductor, respectively. The minority carrier hole concentration in an n-type semiconductor could, theoretically, be calculated from Equation (4.62). However, we would be subtracting two numbers on the order of 1016 cm3, for example, to obtain a number on the order of 104 cm3, which from a practical point of view is not possible. The minority carrier concentrations are calculated from n0p0 n2i once the majority carrier concentration has been determined. TEST YOUR UNDERSTANDING TYU 4.11 Consider a compensated GaAs semiconductor at T 300 K doped at Nd 5 1015 cm3 and Na 2 1016 cm3. Calculate the thermal equilibrium electron and hole concentrations. TYU 4.12 Silicon is doped at Nd 1015 cm3 and Na 0. (a) Plot the concentration of electrons versus temperature over the range 300 T 600 K. (b) Calculate the temperature at which the electron concentration is equal to 1.1 1015 cm3. (Ans. p0 1.5 1016 cm3, n0 2.16 104 cm3) (Ans. T 552 K) TYU 4.13 A silicon device with n-type material is to be operated at T 550 K. At this temperature, the intrinsic carrier concentration must contribute no more than 5 percent of the total electron concentration. Determine the minimum donor concentration required to meet this specification. (Ans. Nd 1.40 10 15 cm3) 4.6 | POSITION OF FERMI ENERGY LEVEL We have discussed qualitatively in Section 4.3.1 how the electron and hole concentrations change as the Fermi energy level moves through the bandgap energy. Then, in Section 4.5, we calculated the electron and hole concentrations as a function of donor and acceptor impurity concentrations. We can now determine the position of the Fermi energy level as a function of the doping concentrations and as a function of temperature. The relevance of the Fermi energy level will be further discussed after the mathematical derivations. nea29583_ch04_106-155.indd 141 12/11/10 10:10 AM 142 CHAPTER 4 4.6.1 The Semiconductor in Equilibrium Mathematical Derivation The position of the Fermi energy level within the bandgap can be determined by using the equations already developed for the thermal-equilibrium electron and hole concentrations. If we assume the Boltzmann approximation to be valid, then from Equation (4.11) we have n0 Nc exp [(Ec EF)kT]. We can solve for Ec EF from this equation and obtain Nc Ec EF kT ln _ n0 (4.63) where n0 is given by Equation (4.60). If we consider an n-type semiconductor in which Nd ni, then n0 Nd, so that N Ec EF kT ln _c (4.64) Nd The distance between the bottom of the conduction band and the Fermi energy is a logarithmic function of the donor concentration. As the donor concentration increases, the Fermi level moves closer to the conduction band. Conversely, if the Fermi level moves closer to the conduction band, then the electron concentration in the conduction band is increasing. We may note that if we have a compensated semiconductor, then the Nd term in Equation (4.64) is simply replaced by Nd Na, or- the net effective donor concentration. DESIGN EXAMPLE 4.12 Objective: Determine the required donor impurity concentration to obtain a specified Fermi energy. Silicon at T 300 K contains an acceptor impurity concentration of Na 1016 cm3. Determine the concentration of donor impurity atoms that must be added so that the silicon is n type and the Fermi energy is 0.20 eV below the conduction-band edge. ■ Solution From Equation (4.64), we have Nc Ec EF kT ln __ Nd Na which can be rewritten as (Ec EF) Nd Na Nc exp __ kT Then 0.20 1.24 1016 cm3 Nd Na 2.8 1019 exp __ 0.0259 or Nd 1.24 1016 Na 2.24 1016 cm3 ■ Comment A compensated semiconductor can be fabricated to provide a specific Fermi energy level. nea29583_ch04_106-155.indd 142 12/11/10 10:10 AM 4.6 Position of Fermi Energy Level 143 ■ EXERCISE PROBLEM Ex 4.12 Consider silicon at T 300 K with doping concentrations of Nd 8 1015 cm3 and Na 5 1015 cm3. Determine the position of the Fermi energy level with respect to Ec. (Ans. Ec EF 0.2368 eV) We may develop a slightly different expression for the position of the Fermi level. We had from Equation (4.39) that n0 ni exp [(EF EFi)kT]. We can solve for EF EFi as n0 EF EFi kT ln _ ni (4.65) Equation (4.65) can be used specifically for an n-type semiconductor, where n0 is given by Equation (4.60), to find the difference between the Fermi level and the intrinsic Fermi level as a function of the donor concentration. We may note that, if the net effective donor concentration is zero, that is, Nd Na 0, then n0 ni and EF EFi. A completely compensated semiconductor has the characteristics of an intrinsic material in terms of carrier concentration and Fermi-level position. We can derive the same types of equations for a p-type semiconductor. From Equation (4.19), we have p0 Nv exp [(EF Ev)kT], so that Nv EF Ev kT ln _ p0 (4.66) If we assume that Na ni, then Equation (4.66) can be written as N EF Ev kT ln _v Na (4.67) The distance between the Fermi level and the top of the valence-band energy for a p-type semiconductor is a logarithmic function of the acceptor concentration: as the acceptor concentration increases, the Fermi level moves closer to the valence band. Equation (4.67) still assumes that the Boltzmann approximation is valid. Again, if we have a compensated p-type semiconductor, then the Na term in Equation (4.67) is replaced by Na Nd, or the net effective acceptor concentration. We can also derive an expression for the relationship between the Fermi level and the intrinsic Fermi level in terms of the hole concentration. We have from Equation (4.40) that p0 ni exp [(EF EFi)kT], which yields p0 EFi EF kT ln _ ni (4.68) Equation (4.68) can be used to find the difference between the intrinsic Fermi level and the Fermi energy in terms of the acceptor concentration. The hole concentration p0 in Equation (4.68) is given by Equation (4.62). nea29583_ch04_106-155.indd 143 12/11/10 10:10 AM 144 CHAPTER 4 The Semiconductor in Equilibrium Ec Ec Electron energy Electron energy EF EFi Ev EFi EF Ev ( b) (a) Figure 4.17 | Position of Fermi level for an (a) n-type (Nd Na) and (b) p-type (Nd Na) semiconductor. We may again note from Equation (4.65) that, for an n-type semiconductor, n0 ni and EF EFi. The Fermi level for an n-type semiconductor is above EFi. For a p-type semiconductor, p0 ni, and from Equation (4.68) we see that EFi EF. The Fermi level for a p-type semiconductor is below EFi. These results are shown in Figure 4.17. 4.6.2 Variation of EF with Doping Concentration and Temperature We may plot the position of the Fermi energy level as a function of the doping concentration. Figure 4.18 shows the Fermi energy level as a function of donor concentration (n type) and as a function of acceptor concentration (p type) for silicon at T 300 K. As the doping levels increase, the Fermi energy level moves closer to the conduction band for the n-type material and closer to the valence band for the p-type material. Keep in mind that the equations for the Fermi energy level that we have derived assume that the Boltzmann approximation is valid. Nd (cm3) Ec 1012 1013 1014 1015 1016 1017 1018 1017 1018 n type EFi p type Ev 1012 1013 1014 1015 1016 Na (cm3) Figure 4.18 | Position of Fermi level as a function of donor concentration (n type) and acceptor concentration (p type). nea29583_ch04_106-155.indd 144 12/11/10 10:10 AM 4.6 Position of Fermi Energy Level 145 Determine the Fermi energy level and the maximum doping concentration at which the Boltzmann approximation is still valid. Consider p-type silicon, at T 300 K, doped with boron. We may assume that the limit of the Boltzmann approximation occurs when EF Ea 3kT. (See Section 4.1.2.) EXAMPLE 4.13 Objective: ■ Solution From Table 4.3, we find the ionization energy is Ea Ev 0.045 eV for boron in silicon. If we assume that EFi Emidgap, then from Equation (4.68), the position of the Fermi level at the maximum doping is given by Eg Na EFi EF _ (Ea Ev) (EF Ea) kT ln _ ni 2 or Na 0.56 0.045 3(0.0259) 0.437 (0.0259) ln _ ni We can then solve for the doping as 0.437 3.2 1017 cm3 Na ni exp __ 0.0259 ■ Comment If the acceptor (or donor) concentration in silicon is greater than approximately 3 1017 cm3, then the Boltzmann approximation of the distribution function becomes less valid and the equations for the Fermi-level position are no longer quite as accurate. ■ EXERCISE PROBLEM Ex 4.13 Consider n-type silicon at T 300 K doped with arsenic. Determine the maximum doping at which the Boltzmann approximation is still valid. Assume the limit is such that Ed EF 3kT. (Ans. n0 2.02 1017 cm3) The intrinsic carrier concentration ni, in Equations (4.65) and (4.68), is a strong function of temperature, so that EF is a function of temperature also. Figure 4.19 shows the variation of the Fermi energy level in silicon with temperature for several donor and acceptor concentrations. As the temperature increases, ni increases, and EF moves closer to the intrinsic Fermi level. At high temperature, the semiconductor material begins to lose its extrinsic characteristics and begins to behave more like an intrinsic semiconductor. At the very low temperature, freeze-out occurs; the Boltzmann approximation is no longer valid and the equations we derived for the Fermi-level position no longer apply. At the low temperature where freeze-out occurs, the Fermi level goes above Ed for the n-type material and below Ea for the p-type material. At absolute zero degrees, all energy states below EF are full and all energy states above EF are empty. 4.6.3 Relevance of the Fermi Energy We have been calculating the position of the Fermi energy level as a function of doping concentrations and temperature. This analysis may seem somewhat arbitrary and fictitious. However, these relations do become significant later in our discussion of pn junctions and the other semiconductor devices we consider. An important nea29583_ch04_106-155.indd 145 12/11/10 10:10 AM 146 CHAPTER 4 The Semiconductor in Equilibrium 1.0 Si 0.8 Conduction band 0.6 N 1018cm3 EF EFi (eV) 0.4 n type 0.2 1012 Intrinsic level 0 1012 0.2 1014 1016 1016 1014 p type 0.4 1018 0.6 0.8 1.0 Valence band 0 100 200 300 T (K ) 400 500 600 Figure 4.19 | Position of Fermi level as a function of temperature for various doping concentrations. (From Sze [14].) point is that, in thermal equilibrium, the Fermi energy level is a constant throughout a system. We will not prove this statement, but we can intuitively see its validity by considering the following example. Suppose we have a particular material, A, whose electrons are distributed in the energy states of an allowed band as shown in Figure 4.20a. Most of the energy states below EFA contain electrons and most of the energy states above EFA are empty of electrons. Consider another material, B, whose electrons are distributed in the energy states of an allowed band as shown in Figure 4.20b. The energy states below EFB are mostly full and the energy states above EFB are mostly empty. If these two materials are brought into intimate contact, the electrons in the entire system will tend to seek the lowest possible energy. Electrons from material A will flow into the lower energy states of material B, as indicated in Figure 4.20c, until thermal equilibrium is reached. Thermal equilibrium occurs when the distribution of electrons, as a function of energy, is the same in the two materials. This equilibrium state occurs when the Fermi energy is the same in the two materials as shown in Figure 4.20d. The Fermi energy, important in the physics of the semiconductor, also provides a good pictorial representation of the characteristics of the semiconductor materials and devices. TEST YOUR UNDERSTANDING TYU 4.14 Determine the position of the Fermi level with respect to the valence-band energy in p-type GaAs at T 300 K. The doping concentrations are Na 5 1016 cm3 and Nd 4 1015 cm3. TYU 4.15 Calculate the position of the Fermi energy level in n-type silicon at T 300 K with respect to the intrinsic Fermi energy level. The doping concentrations are Nd 2 1017 cm3 and Na 3 1016 cm3. (Ans. EF Ev 0.130 eV) (Ans. EF EFi 0.421 eV) nea29583_ch04_106-155.indd 146 12/11/10 10:10 AM 4.7 Summary 147 E 0 E Allowed energy states EFA 1 2 1 Allowed energy states EFB 0 fF 1 1 2 (a) fF (b) EFA EFB EF EF (c) (d) Figure 4.20 | The Fermi energy of (a) material A in thermal equilibrium, (b) material B in thermal equilibrium, (c) materials A and B at the instant they are placed in contact, and (d) materials A and B in contact at thermal equilibrium. 4.7 | SUMMARY ■ ■ ■ The concentration of electrons in the conduction band is the integral over the conduction-band energy of the product of the density of states function in the conduction band and the Fermi–Dirac probability function. The concentration of holes in the valence band is the integral over the valence-band energy of the product of the density of states function in the valence band and the probability of a state being empty, which is [1 fF (E)]. Using the Maxwell–Boltzmann approximation, the thermal-equilibrium concentration of electrons in the conduction band is given by (Ec EF) n0 Nc exp __ kT ■ where Nc is the effective density of states in the conduction band. Using the Maxwell–Boltzmann approximation, the thermal-equilibrium concentration of holes in the valence band is given by (EF Ev) p0 Nv exp __ kT ■ where Nv is the effective density of states in the valence band. The intrinsic carrier concentration is found from Eg n2i NcNv exp _ kT nea29583_ch04_106-155.indd 147 12/11/10 10:10 AM 148 CHAPTER 4 ■ ■ ■ ■ ■ The Semiconductor in Equilibrium The concept of doping the semiconductor with donor (group V elements) impurities and acceptor (group III elements) impurities to form n-type and p-type extrinsic semiconductors was discussed. The fundamental relationship of n0p0 n2i was derived. Using the concepts of complete ionization and charge neutrality, equations for the electron and hole concentrations as a function of impurity doping concentrations were derived. The position of the Fermi energy level as a function of impurity doping concentrations was derived. The relevance of the Fermi energy was discussed. The Fermi energy is a constant throughout a semiconductor that is in thermal equilibrium. GLOSSARY OF IMPORTANT TERMS acceptor atoms Impurity atoms added to a semiconductor to create a p-type material. charge carrier The electron and/or hole that moves inside the semiconductor and gives rise to electrical currents. compensated semiconductor A semiconductor that contains both donors and acceptors in the same semiconductor region. complete ionization The condition when all donor atoms are positively charged by giving up their donor electrons and all acceptor atoms are negatively charged by accepting electrons. degenerate semiconductor A semiconductor whose electron concentration or hole concentration is greater than the effective density of states, so that the Fermi level is in the conduction band (n type) or in the valence band (p type). donor atoms Impurity atoms added to a semiconductor to create an n-type material. effective density of states The parameter Nc, which results from integrating the density of quantum states gc (E ) times the Fermi function fF (E ) over the conduction-band energy, and the parameter Nv, which results from integrating the density of quantum states gv (E ) times [1 fF (E)] over the valence-band energy. extrinsic semiconductor A semiconductor in which controlled amounts of donors and/or acceptors have been added so that the electron and hole concentrations change from the intrinsic carrier concentration and a preponderance of either electrons (n type) or holes (p type) is created. freeze-out The condition that occurs in a semiconductor when the temperature is lowered and the donors and acceptors become neutrally charged. The electron and hole concentrations become very small. CHECKPOINT After studying this chapter, the reader should have the ability to: ■ ■ ■ ■ nea29583_ch04_106-155.indd 148 Derive the equations for the thermal equilibrium concentrations of electrons and holes in terms of the Fermi energy. Derive the equation for the intrinsic carrier concentration. Disscuss what is meant by the effective density of states for electrons and holes. Describe the effect of adding donor and acceptor impurity atoms to a semiconductor. 12/11/10 10:10 AM Problems ■ ■ ■ ■ ■ ■ ■ 149 Understand the concept of complete ionization. Derive the fundamental relationship n0 p0 n2i . Describe the meaning of degenerate and nondegenerate semiconductor materials. Discuss the concept of charge neutrality. Derive the equations for n0 and p0 in terms of impurity doping concentrations. Derive the equations for the Fermi energy in terms of the impurity doping concentrations. Discuss the variation of the Fermi energy with doping concentration and temperature. REVIEW QUESTIONS 1. How does the electron concentration in the conduction band change with energy E for E Ec? 2. In deriving the equation for n0 in terms of the Fermi function, the upper limit of the integral should be the energy at the top of the conduction band. Justify using infinity instead. 3. Assuming the Boltzmann approximation applies, write the equations for n0 and p0 in terms of the Fermi energy. 4. What is the source of electrons and holes in an intrinsic semiconductor? 5. Under what condition would the intrinsic Fermi level be at the midgap energy? 6. What is a donor impurity? What is an acceptor impurity? 7. What is meant by complete ionization? What is meant by freeze-out? 8. What is the product of n0 and p0 equal to? 9. Write the equation for charge neutrality for the condition of complete ionization. 10. Sketch a graph of n0 versus temperature for an n-type material. 11. Sketch graphs of the Fermi energy versus donor impurity concentration and versus temperature. 12. What is the relevance of the Fermi energy? PROBLEMS Section 4.1 4.1 4.2 4.3 4.4 Charge Carriers in Semiconductors Calculate the intrinsic carrier concentration, ni, at T 200, 400, and 600 K for (a) silicon, (b) germanium, and (c) gallium arsenide. Plot the intrinsic carrier concentration, ni, for a temperature range of 200 T 600 K for (a) silicon, (b) germanium, and (c) gallium arsenide. (Use a log scale for ni. ) (a) The maximum intrinsic carrier concentration in a silicon device must be limited to 5 1011 cm3. Assume Eg 1.12 eV. Determine the maximum temperature allowed for the device. (b) Repeat part (a) if the maximum intrinsic carrier concentration is limited to 5 1012 cm3. In a particular semiconductor material, the effective density of states functions are given by Nc Nc0· (T兾300)3兾2 and Nv Nv0· (T兾300)3兾2 where Nc0 and Nv0 are constants independent of temperature. Experimentally determined intrinsic carrier concentrations are found to be ni 1.40 102 cm3 at T 200 K and ni 7.70 1010 cm2 at T 400 K. Determine the product Nc0 ⴢ Nv0 and the bandgap energy Eg. (Assume Eg is constant over this temperature range.) nea29583_ch04_106-155.indd 149 12/13/10 1:49 PM 150 CHAPTER 4 4.5 4.6 4.7 4.8 4.9 4.10 4.11 4.12 4.13 4.14 Two semiconductor materials have exactly the same properties except material A has a bandgap energy of 0.90 eV and material B has a bandgap energy of 1.10 eV. Determine the ratio of ni of material B to that of material A for (a) T 200 K, (b) T 300 K, and (c) T 400 K. (a) The magnitude of the product gC(E )fF (E ) in the conduction band is a function of energy as shown in Figure 4.1. Assume the Boltzmann approximation is valid. Determine the energy with respect to Ec at which the maximum occurs. (b) Repeat part (a) for the magnitude of the product gv (E ) [1 fF (E)] in the valence band. Assume the Boltzmann approximation in a semiconductor is valid. Determine the ratio of n(E) gC (E) fF (E ) at E Ec 4 kT to that at E Ec kT2. Assume that Ec EF 0.20 eV in silicon. Plot n(E ) gC (E ) fF (E ) over the range Ec E Ec 0.10 eV for (a) T 200 K and (b) T 400 K. (a) Consider silicon at T 300 K. Plot the thermal equilibrium electron concentration n0 (on a log scale) over the energy range 0.2 Ec EF 0.4 eV. (b) Repeat part (a) for the hole concentration over the range 0.2 EF Ev 0.4 eV. Given the effective masses of electrons and holes in silicon, germanium, and gallium arsenide, calculate the position of the intrinsic Fermi energy level with respect to the center of the bandgap for each semiconductor at T 300 K. Calculate EFi with respect to the center of the bandgap in silicon for T 200, 400, and 600 K. (a) The carrier effective masses in a semiconductor are m*n 1.21 m0 and m*p 0.70 m0. Determine the position of the intrinsic Fermi level with respect to the center of the bandgap at T 300 K. (b) Repeat part (a) if m*n 0.080 m0 and m*p 0.75 m0. If the density of states function in the conduction band of a particular semiconductor is a constant equal to K, derive the expression for the thermal-equilibrium concentration of electrons in the conduction band, assuming Fermi–Dirac statistics and assuming the Boltzmann approximation is valid. Repeat Problem 4.13 if the density of states function is given by gc(E) C1(E Ec) for E Ec where C1 is a constant. Section 4.2 4.15 4.16 The Semiconductor in Equilibrium Dopant Atoms and Energy Levels Calculate the ionization energy and radius of the donor electron in germanium using the Bohr theory. Repeat Problem 4.15 for gallium arsenide. Section 4.3 The Extrinsic Semiconductor Silicon at T 300 K is doped with arsenic atoms such that the concentration of electrons is n0 7 1015 cm3. (a) Find Ec EF. (b) Determine EF Ev. (c) Calculate p0. (d) Which carrier is the minority carrier? (e) Find EF EFi. 4.18 The value of p0 in silicon at T 300 K is 2 1016 cm3. (a) Determine EF Ev. (b) Calculate the value of Ec EF. (c) What is the value of n0? (d) Determine EFi EF. 4.19 The electron concentration in silicon at T 300 K is n0 2 105 cm3. (a) Determine the position of the Fermi level with respect to the valence band energy level. (b) Determine p0. (c) Is this n- or p-type material? 4.17 nea29583_ch04_106-155.indd 150 12/11/10 10:10 AM Problems 4.20 4.21 4.22 4.23 4.24 4.25 4.26 4.27 4.28 4.29 4.30 151 (a) If Ec EF 0.28 eV in gallium arsenide at T 375 K, calculate the values of n0 and p0. (b) Assuming the value of n0 in part (a) remains constant, determine Ec EF and p0 at T 300 K. Repeat Problem 4.20 for silicon. The Fermi energy level in silicon at T 300 K is as close to the top of the valence band as to the midgap energy. (a) Is the material n type or p type? (b) Calculate the values of n0 and p0 . (a) The Fermi energy level in silicon at T 300 K is 0.22 eV above the intrinsic Fermi level. Determine n0 and p0 . (b) Repeat part (a) for GaAs. Silicon at T 300 K is doped with boron atoms such that the concentration of holes is p0 5 1015 cm3. (a) Find EF Ev. (b) Determine Ec EF. (c) Determine n0. (d) Which carrier is the majority carrier? (e) Determine EFi EF. Repeat Problem 4.24 for T 400 K, assuming the hole concentration remains constant. (a) Determine the values of n0 and p0 in GaAs at T 300 K if EF Ev 0.25 eV. (b) Assuming the value of p0 in part (a) remains constant, determine the values of EF Ev and n0 at T 400 K. Repeat Problem 4.26 for silicon. (a) Assume that EF Ec kT2 at T 300 K in silicon. Determine n0. (b) Repeat part (a) for GaAs. Consider silicon at T 300 K in which the hole concentration is p0 5 1019 cm3. Determine Ev EF. (a) In silicon at T 300 K, we find that EF EC 4 kT. Determine the electron concentration. (b) Repeat part (a) for GaAs. Section 4.4 Statistics of Donors and Acceptors *4.31 The electron and hole concentrations as a function of energy in the conduction band and valence band peak at a particular energy as shown in Figure 4.8. Consider silicon and assume Ec EF 0.20 eV. Determine the energy, relative to the band edges, at which the concentrations peak. *4.32 For the Boltzmann approximation to be valid for a semiconductor, the Fermi level must be at least 3 kT below the donor level in an n-type material and at least 3 kT above the acceptor level in a p-type material. If T 300 K, determine the maximum electron concentration in an n-type semiconductor and the maximum hole concentration in a p-type semiconductor for the Boltzmann approximation to be valid in (a) silicon and (b) gallium arsenide. 4.33 Plot the ratio of un-ionized donor atoms to the total electron concentration versus temperature for silicon over the range 50 T 200 K. Section 4.5 4.34 Charge Neutrality Determine the equilibrium electron and hole concentrations in silicon for the following conditions: (a) T 300 K, Nd 1015 cm3, Na 4 1015 cm3 (b) T 300 K, Nd 3 1016 cm3, Na 0 *Asterisks next to problems indicate problems that are more difficult. nea29583_ch04_106-155.indd 151 12/11/10 10:10 AM 152 CHAPTER 4 4.35 4.36 *4.37 4.38 4.39 4.40 4.41 4.42 4.43 4.44 4.45 4.46 4.47 nea29583_ch04_106-155.indd 152 The Semiconductor in Equilibrium (c) T 300 K, Nd Na 2 1015 cm3 (d) T 375 K, Nd 0, Na 4 1015 cm3 (e) T 450 K, Nd 1014 cm3, Na 0 Repeat Problem 4.34 for GaAs. (a) Consider a germanium semiconductor at T 300 K. Calculate the thermal equilibrium electron and hole concentrations for (i) Nd 2 1015 cm3, Na 0, and (ii) Na 1016 cm3, Nd 7 1015 cm3. (b) Repeat part (a) for GaAs. (c) For the case of GaAs in part (b), the minority carrier concentrations are on the order of 103 cm3. What does this result mean physically? The Fermi level in n-type silicon at T 300 K is 245 meV below the conduction band and 200 meV below the donor level. Determine the probability of finding an electron (a) in the donor level and (b) in a state in the conduction-band kT above the conduction-band edge. Assume that silicon, germanium, and gallium arsenide each have dopant concentrastions of Nd 1 1013 cm3 and Na 2.5 1013 cm3 at T 300 K. For each of the three materials: (a) Is this material n type or p type? (b) Calculate n0 and p0. A silicon semiconductor material at T 300 K is doped with arsenic atoms to a concentration of 2 1015 cm3 and with boron atoms to a concentration of 1.2 1015 cm3. (a) Is the material n type or p type? (b) Determine n0 and p0. (c) Additional boron atoms are to be added such that the hole concentration is 4 1015 cm3. What concentration of boron atoms must be added and what is the new value of n0? The thermal equilibrium hole concentration in silicon at T 300 K is p0 2 105 cm3. Determine the thermal-equilibrium electron concentration. Is the material n type or p type? In a germanium sample at T 250 K, it is found that p0 4n0 and that Nd 0. Determine p0, n0, and Na. Consider a sample of silicon doped at Nd 0 and Na 1014 cm3. Plot the majority carrier concentration versus temperature over the range 200 T 500 K. The temperature of a sample of silicon is T 300 K and the acceptor doping concentration is Na 0. Plot the minority carrier concentration (on a log–log plot) versus Nd over the range 1015 Nd 1018 cm3. Repeat problem 4.43 for GaAs. A particular semiconductor material is doped at Nd 2 1014 cm3 and Na 1.2 1014 cm3. The thermal equilibrium electron concentration is found to be n0 1.1 1014 cm3. Assuming complete ionization, determine the intrinsic carrier concentration and the thermal equilibrium hole concentration. (a) Silicon at T 300 K is uniformly doped with boron atoms to a concentration of 3 1016 cm3 and with arsenic atoms to a concentration of 1.5 1016 cm3. Is the material n type or p type? Calculate the thermal equilibrium concentrations of majority and minority carriers. (b) Additional impurity atoms are added such that holes are the majority carrier and the thermal equilibrium concentration is p0 5 1016 cm3. What type and concentration of impurity atoms must be added? What is the new value of n0? In silicon at T 300 K, it is found that Na 7 1015 cm3 and p0 2 10 4 cm3. (a) Is the material n type or p type? (b) What are the majority and minority carrier concentrations? (c) What must be the concentration of donor impurities? 12/11/10 10:10 AM Problems Section 4.6 4.48 4.49 4.50 4.51 4.52 4.53 4.54 4.55 4.56 4.57 153 Position of Fermi Energy Level Consider germanium with an acceptor concentration of Na 1015 cm3 and a donor concentration of Nd 0. Consider temperatures of T 200, 400, and 600 K. Calculate the position of the Fermi energy with respect to the intrinsic Fermi level at these temperatures. Consider silicon at T 300 K with donor concentrations of Nd 1014, 1015, 1016, and 1017, cm3. Assume Na 0. (a) Calculate the position of the Fermi energy level with respect to the conduction band for these donor concentrations. (b) Determine the position of the Fermi energy level with respect to the intrinsic Fermi energy level for the donor concentrations given in part (a). A silicon device is doped with donor impurity atoms at a concentration of 1015 cm3. For the device to operate properly, the intrinsic carriers must contribute no more than 5 percent to the total electron concentration. (a) What is the maximum temperature that the device may operate? (b) What is the change in Ec EF from the T 300 K value to the maximum temperature value determined in part (a). (c) Is the Fermi level closer or further from the intrinsic value at the higher temperature? Silicon is doped with acceptor impurity atoms at a concentration of Na 3 1015 cm3. Assume Nd 0. Plot the position of the Fermi energy level with respect to the intrinsic Fermi energy level over the temperature range of 200 T 600 K. Consider GaAs at T 300 K with Nd 0. (a) Plot the position of the Fermi energy level with respect to the intrinsic Fermi energy level as a function of the acceptor impurity concentration over the range of 1014 Na 1017 cm3. (b) Plot the position of the Fermi energy level with respect to the valence-band energy over the same acceptor impurity concentration as given in part (a). For a particular semiconductor, Eg 1.50 eV, m*p 10 m*n , T 300 K, and ni 1 105 cm3. (a) Determine the position of the intrinsic Fermi energy level with respect to the center of the bandgap. (b) Impurity atoms are added so that the Fermi energy level is 0.45 eV below the center of the bandgap. (i) Are acceptor or donor atoms added? (ii) What is the concentration of impurity atoms added? Silicon at T 300 K contains acceptor atoms at a concentration of Na 5 1015 cm3. Donor atoms are added forming an n-type compensated semiconductor such that the Fermi level is 0.215 eV below the conduction-band edge. What concentration of donor atoms are added? (a) Silicon at T 300 K is doped with donor impurity atoms at a concentration of Nd 6 1015 cm3. (i) Determine Ec EF. (ii) Calculate the concentration of additional donor impurity atoms that must be added to move the Fermi energy level a distance kT closer to the conduction band edge. (b) Repeat part (a) for GaAs if the original donor impurity concentration is Nd 1 1015 cm3. (a) Determine the position of the Fermi energy level with respect to the intrinsic Fermi level in silicon at T 300 K that is doped with boron atoms at a concentration of Na 2 1016 cm3. (b) Repeat part (a) if the silicon is doped with phosphorus atoms at a concentration of Nd 2 1016 cm3. (c) Calculate n0 and p0 in parts (a) and (b). GaAs at T 300 K is doped with donor impurity atoms at a concentration of 7 1015 cm3. Additional impurity atoms are to be added such that the Fermi level is 0.55 eV above the intrinsic Fermi level. Determine the type (donor or acceptor) and concentration of impurity atoms to be added. nea29583_ch04_106-155.indd 153 12/11/10 10:10 AM 154 CHAPTER 4 4.58 4.59 4.60 The Semiconductor in Equilibrium Determine the Fermi energy level with respect to the intrinsic Fermi level for each condition given in Problem 4.34. Find the Fermi energy level with respect to the valence-band energy for the conditions given in Problem 4.35. Calculate the position of the Fermi energy level with respect to the intrinsic Fermi for the conditions given in Problem 4.47. Summary and Review 4.61 A new semiconductor material is to be “designed.” The semiconductor is to be p type and doped with 5 1015 cm3 acceptor atoms. Assume complete ionization and assume Nd 0. The effective density of states functions are Nc 1.2 1019 cm3 and Nv 1.8 1019 cm3 at T 300 K and vary as T 2. A special semiconductor device fabricated with this material requires that the hole concentration be no greater than 5.08 1015 cm3 at T 350 K. What is the minimum bandgap energy required in this new material? 4.62 Silicon atoms, at a concentration of 7 1015 cm3, are added to gallium arsenide. Assume that the silicon atoms act as fully ionized dopant atoms and that 5 percent of the concentration added replace gallium atoms and 95 percent replace arsenic atoms. Let T 300 K. (a) Determine the donor and acceptor concentrations. (b) Is the material n type or p type? (c) Calculate the electron and hole concentrations. (d) Determine the position of the Fermi level with respect to EFi. 4.63 Defects in a semiconductor material introduce allowed energy states within the forbidden bandgap. Assume that a particular defect in silicon introduces two discrete levels: a donor level 0.25 eV above the top of the valence band and an acceptor level 0.65 eV above the top of the valence band. The charge state of each defect is a function of the position of the Fermi level. (a) Sketch the charge density of each defect as the Fermi level moves from Ev to Ec. Which defect level dominates in (i) heavily doped n type material and (ii) in heavily doped p-type material? (b) Determine the electron and hole concentrations and the location of the Fermi level in (i) an n type sample doped at Nd 1017 cm3 and (ii) in a p-type sample doped at Na 1017 cm3 . (c) Determine the Fermi-level position if no dopant atoms are added. Is the material n type, p type, or intrinsic? READING LIST *1. Hess, K. Advanced Theory of Semiconductor Devices. Englewood Cliffs, NJ: Prentice Hall, 1988. 2. Hu, C. C. Modern Semiconductor Devices for Integrated Circuits. Upper Saddle River, NJ: Pearson Prentice Hall, 2010. 3. Kano, K. Semiconductor Devices. Upper Saddle River, NJ: Prentice Hall, 1998. *4. Li, S. S. Semiconductor Physical Electronics. New York: Plenum Press, 1993. 5. McKelvey, J. P. Solid State Physics for Engineering and Materials Science. Malabar, FL.: Krieger Publishing, 1993. 6. Navon, D. H. Semiconductor Microdevices and Materials. New York: Holt, Rinehart & Winston, 1986. nea29583_ch04_106-155.indd 154 12/11/10 10:10 AM Reading List 155 7. Pierret, R. F. Semiconductor Device Fundamentals. Reading, MA: Addison-Wesley, 1996. 8. Shur, M. Introduction to Electronic Devices. New York: John Wiley and Sons, 1996. *9. Shur, M. Physics of Semiconductor Devices. Englewood Cliffs, NJ: Prentice Hall, 1990. 10. Singh, J. Semiconductor Devices: An Introduction. New York: McGraw-Hill, 1994. 11. Singh, J. Semiconductor Devices: Basic Principles. New York: John Wiley and Sons, 2001. *12. Smith, R. A. Semiconductors. 2nd ed. New York; Cambridge University Press, 1978. 13. Streetman, B. G., and S. Banerjee. Solid State Electronic Devices, 6th ed. Upper Saddle River, NJ: Pearson Prentice Hall, 2006. 14. Sze, S. M., and K. K. Ng. Physics of Semiconductor Devices. 3rd ed. Hoboken, NJ: John Wiley and Sons, 2007. *15. Wang, S. Fundamentals of Semiconductor Theory and Device Physics. Englewood Cliffs, NJ: Prentice Hall, 1989. *16. Wolfe, C. M., N. Holonyak, Jr., and G. E. Stillman. Physical Properties of Semiconductors. Englewood Cliffs, NJ: Prentice Hall, 1989. 17. Yang, E. S. Microelectronic Devices. New York: McGraw-Hill, 1988. *Indicates references that are at an advanced level compared to this text. nea29583_ch04_106-155.indd 155 12/11/10 10:10 AM C 5 H A P T E R Carrier Transport Phenomena I n the previous chapter, we considered the semiconductor in equilibrium and determined electron and hole concentrations in the conduction and valence bands, respectively. A knowledge of the densities of these charged particles is important toward an understanding of the electrical properties of a semiconductor material. The net flow of the electrons and holes in a semiconductor will generate currents. The process by which these charged particles move is called transport. In this chapter we consider two basic transport mechanisms in a semiconductor crystal: drift— the movement of charge due to electric fields, and diffusion—the flow of charge due to density gradients. The carrier transport phenomena are the foundation for finally determining the current–voltage characteristics of semiconductor devices. We will implicitly assume in this chapter that, although there will be a net flow of electrons and holes due to the transport processes, thermal equilibrium will not be substantially disturbed. Nonequilibrium processes are considered in the next chapter. ■ 5.0 | PREVIEW In this chapter, we will: ■ Describe the mechanism of carrier drift and induced drift current due to an applied electric field. ■ Define and describe the characteristics of carrier mobility. ■ Describe the mechanism of carrier diffusion and induced diffusion current due to a gradient in the carrier concentration. ■ Define the carrier diffusion coefficient. ■ Describe the effects of a nonuniform impurity doping concentration in a semiconductor material. ■ Discuss and analyze the Hall effect in a semiconductor material. 156 nea29583_ch05_156-191.indd 156 12/11/10 10:15 AM 5.1 Carrier Drift 157 5.1 | CARRIER DRIFT An electric field applied to a semiconductor will produce a force on electrons and holes so that they will experience a net acceleration and net movement, provided there are available energy states in the conduction and valence bands. This net movement of charge due to an electric field is called drift. The net drift of charge gives rise to a drift current. 5.1.1 Drift Current Density If we have a positive volume charge density moving at an average drift velocity vd, the drift current density is given by Jdrf vd (5.1a) Coul _ Coul A __ _ Jdrf _ cm s cm2 s cm2 cm3 (5.1b) In terms of units, we have If the volume charge density is due to positively charged holes, then Jpdrf (ep)vdp (5.2) where Jpdrf is the drift current density due to holes and vdp is the average drift velocity of the holes. The equation of motion of a positively charged hole in the presence of an electric field is F m*cp a eE (5.3) where e is the magnitude of the electronic charge, a is the acceleration, E is the electric field, and m*cp is the conductivity effective mass of the hole.1 If the electric field is constant, then we expect the velocity to increase linearly with time. However, charged particles in a semiconductor are involved in collisions with ionized impurity atoms and with thermally vibrating lattice atoms. These collisions, or scattering events, alter the velocity characteristics of the particle. As the hole accelerates in a crystal due to the electric field, the velocity increases. When the charged particle collides with an atom in the crystal, for example, the particle loses most, or all, of its energy. The particle will again begin to accelerate and gain energy until it is again involved in a scattering process. This continues over and over again. Throughout this process, the particle will gain an average drift velocity which, for low electric fields, is directly proportional to the electric field. We may then write vdp p E (5.4) where p is the proportionality factor and is called the hole mobility. The mobility is an important parameter of the semiconductor since it describes how well a particle 1 The conductivity effective mass is used when carriers are in motion. See Appendix F for further discussion of effective mass concepts. nea29583_ch05_156-191.indd 157 12/11/10 10:15 AM 158 CHAPTER 5 Carrier Transport Phenomena Table 5.1 | Typical mobility values at T 300 K and low doping concentrations Silicon Gallium arsenide Germanium n (cm2/V-s) p (cm2/V-s) 1350 8500 3900 480 400 1900 will move due to an electric field. The unit of mobility is usually expressed in terms of cm2V-s. By combining Equations (5.2) and (5.4), we may write the drift current density due to holes as Jpdrf (ep)vdp eppE (5.5) The drift current due to holes is in the same direction as the applied electric field. The same discussion of drift applies to electrons. We may write Jndrf vdn (en)vdn (5.6) where Jndrf is the drift current density due to electrons and vdn is the average drift velocity of electrons. The net charge density of electrons is negative. The average drift velocity of an electron is also proportional to the electric field for small fields. However, since the electron is negatively charged, the net motion of the electron is opposite to the electric field direction. We can then write vdn n E (5.7) where n is the electron mobility and is a positive quantity. Equation (5.6) may now be written as Jndrf (en)(n E) en nE (5.8) The conventional drift current due to electrons is also in the same direction as the applied electric field even though the electron movement is in the opposite direction. Electron and hole mobilities are functions of temperature and doping concentrations, as we will see in the next section. Table 5.1 shows some typical mobility values at T 300 K for low doping concentrations. Since both electrons and holes contribute to the drift current, the total drift current density is the sum of the individual electron and hole drift current densities, so we may write Jdrf e(n n p p)E EXAMPLE 5.1 (5.9) Objective: Calculate the drift current density in a semiconductor for a given electric field. Consider a gallium arsenide sample at T 300 K with doping concentrations of Na 0 and Nd 1016 cm3. Assume complete ionization and assume electron and hole mobilities given in Table 5.1. Calculate the drift current density if the applied electric field is E 10 V/cm. nea29583_ch05_156-191.indd 158 12/11/10 10:15 AM 5.1 Carrier Drift 159 ■ Solution Since Nd Na, the semiconductor is n type and the majority carrier electron concentration, from Chapter 4 is given by Nd Na n __ 2 ______________ Nd Na __ 2 n 2 2 i 1016 cm3 The minority carrier hole concentration is n2i (1.8 106)2 __ 3.24 104 cm3 p_ n 1016 For this extrinsic n-type semiconductor, the drift current density is Jdrf e(n n p p)E en Nd E Then Jdrf (1.6 1019)(8500)(1016)(10) 136 A /cm2 ■ Comment Significant drift current densities can be obtained in a semiconductor applying relatively small electric fields. We may note from this example that the drift current will usually be due primarily to the majority carrier in an extrinsic semiconductor. ■ EXERCISE PROBLEM Ex 5.1 A drift current density of Jdrf 75 A/cm2 is required in a device using p-type silicon when an electric field of E 120 V/cm is applied. Determine the required impurity doping concentration to achieve this specification. Assume that electron and hole mobilities given in Table 5.1 apply. 5.1.2 Mobility Effects (Ans. Na 8.14 1015 cm3) In the previous section, we defined mobility, which relates the average drift velocity of a carrier to the electric field. Electron and hole mobilities are important semiconductor parameters in the characterization of carrier drift, as seen in Equation (5.9). Equation (5.3) related the acceleration of a hole to a force such as an electric field. We may write this equation as dv eE (5.10) F m*cp _ dt where v is the velocity of the particle due to the electric field and does not include the random thermal velocity. If we assume that the conductivity effective mass and electric field are constants, then we may integrate Equation (5.10) and obtain eEt v_ (5.11) * mcp where we have assumed the initial drift velocity to be zero. Figure 5.1a shows a schematic model of the random thermal velocity and motion of a hole in a semiconductor with zero electric field. There is a mean time nea29583_ch05_156-191.indd 159 12/11/10 10:15 AM 160 CHAPTER 5 Carrier Transport Phenomena 4 1 4 1 2 2 3 3 E field (b) (a) Figure 5.1 | Typical random behavior of a hole in a semiconductor (a) without an electric field and (b) with an electric field. between collisions which may be denoted by cp. If a small electric field (E-field) is applied as indicated in Figure 5.1b, there will be a net drift of the hole in the direction of the E-field, and the net drift velocity will be a small perturbation on the random thermal velocity, so the time between collisions will not be altered appreciably. If we use the mean time between collisions cp in place of the time t in Equation (5.11), then the mean peak velocity just prior to a collision or scattering event is ecp vdpeak _ E * mcp (5.12a) The average drift velocity is one half the peak value so that we can write ecp 1 _ vd _ E * 2 mcp (5.12b) However, the collision process is not as simple as this model, but is statistical in nature. In a more accurate model including the effect of a statistical distribution, the factor _12 in Equation (5.12b) does not appear. The hole mobility is then given by vdp ecp p _ _ (5.13) m*cp E The same analysis applies to electrons; thus, we can write the electron mobility as ecn n _ m*cn (5.14) where cn is the mean time between collisions for an electron. There are two collision or scattering mechanisms that dominate in a semiconductor and affect the carrier mobility: phonon or lattice scattering, and ionized impurity scattering. The atoms in a semiconductor crystal have a certain amount of thermal energy at temperatures above absolute zero that causes the atoms to randomly vibrate about their lattice position within the crystal. The lattice vibrations cause a disruption in the perfect periodic potential function. A perfect periodic potential in a solid allows nea29583_ch05_156-191.indd 160 12/11/10 10:15 AM 5.1 Carrier Drift 161 electrons to move unimpeded, or with no scattering, through the crystal. But the thermal vibrations cause a disruption of the potential function, resulting in an interaction between the electrons or holes and the vibrating lattice atoms. This lattice scattering is also referred to as phonon scattering. Since lattice scattering is related to the thermal motion of atoms, the rate at which the scattering occurs is a function of temperature. If we denote L as the mobility that would be observed if only lattice scattering existed, then the scattering theory states that to first order L T 32 (5.15) Mobility that is due to lattice scattering increases as the temperature decreases. Intuitively, we expect the lattice vibrations to decrease as the temperature decreases, which implies that the probability of a scattering event also decreases, thus increasing mobility. Figure 5.2 shows the temperature dependence of electron and hole mobilities in silicon. In lightly doped semiconductors, lattice scattering dominates and the carrier mobility decreases with temperature as we have discussed. The temperature dependence of mobility is proportional to T n. The inserts in the figure show that the parameter n is not equal to _32 as the first-order scattering theory predicted. However, mobility does increase as the temperature decreases. The second interaction mechanism affecting carrier mobility is called ionized impurity scattering. We have seen that impurity atoms are added to the semiconductor to control or alter its characteristics. These impurities are ionized at room temperature so that a coulomb interaction exists between the electrons or holes and the ionized impurities. This coulomb interaction produces scattering or collisions and also alters the velocity characteristics of the charge carrier. If we denote I as the mobility that would be observed if only ionized impurity scattering existed, then to first order we have T 32 I _ (5.16) NI where NI Nd Na is the total ionized impurity concentration in the semiconductor. If temperature increases, the random thermal velocity of a carrier increases, reducing the time the carrier spends in the vicinity of the ionized impurity center. The less time spent in the vicinity of a coulomb force, the smaller the scattering effect and the larger the expected value of I. If the number of ionized impurity centers increases, then the probability of a carrier encountering an ionized impurity center increases, implying a smaller value of I. Figure 5.3 is a plot of electron and hole mobilities in germanium, silicon, and gallium arsenide at T 300 K as a function of impurity concentration. More accurately, these curves are of mobility versus ionized impurity concentration NI. As the impurity concentration increases, the number of impurity scattering centers increases, thus reducing mobility. If L is the mean time between collisions due to lattice scattering, then dtL is the probability of a lattice scattering event occurring in a differential time dt. Likewise, if I is the mean time between collisions due to ionized impurity scattering, then dtI is the probability of an ionized impurity scattering event occurring in the differential time dt. nea29583_ch05_156-191.indd 161 12/11/10 10:15 AM 162 nea29583_ch05_156-191.indd 162 12/11/10 10:15 AM n (cm2/ V-s) ND 10 0 16 50 10 50 100 0 NA 1019 NA 1018 NA 1017 50 200 T 22 150 500 T (K) NA 1014 cm3 100 100 100 200 p 500 1000 (b) 200 1000 NA 1016 (a) 150 200 500 T (K) NA 1014 T ( C) 100 100 500 N 1014 cm3 D T 22 1000 T ( C) ND 1019 ND 1018 ND 1017 ND 1014 2000 n 1000 4000 Figure 5.2 | (a) Electron and (b) hole mobilities in silicon versus temperature for various doping concentrations. Inserts show temperature dependence for “almost” intrinsic silicon. (From Pierret [8].) 50 50 100 500 1000 2000 5000 p (cm2/ V-s) 200 1000 5.1 104 163 T 300 K n Ge p 103 Carrier Drift 102 Mobility (cm2/V-s) 104 n 103 Si p 102 104 n GaAs 103 102 1014 p 1015 1016 1017 1018 1019 Impurity concentration (cm3) Figure 5.3 | Electron and hole mobilities versus impurity concentrations for germanium, silicon, and gallium arsenide at T 300 K. (From Sze [14].) If these two scattering processes are independent, then the total probability of a scattering event occurring in the differential time dt is the sum of the individual events, or dt _ dt _ dt _ I L (5.17) where is the mean time between any scattering event. Comparing Equation (5.17) with the definitions of mobility given by Equation (5.13) or (5.14), we can write 1 1 1 _ _ _ I L (5.18) where I is the mobility due to the ionized impurity scattering process and L is the mobility due to the lattice scattering process. The parameter is the net mobility. With two or more independent scattering mechanisms, the inverse mobilities add, which means that the net mobility decreases. nea29583_ch05_156-191.indd 163 12/11/10 10:15 AM 164 CHAPTER 5 Carrier Transport Phenomena EXAMPLE 5.2 Objective: Determine the electron mobility in silicon at various doping concentrations and various temperatures. Using Figure 5.2, find the electron mobility in silicon for: (a) T 25°C for (i) Nd 1016 cm3 and (ii) Nd 1017 cm3. (b) Nd 1016 cm3 for (i) T 0°C and (ii) T 100°C. ■ Solution: From Figure 5.2, we find the following: (a) T 25°C; (i) Nd 1016 cm3 ⇒ n 1200 cm2/V-s. (ii) Nd 1017 cm3 ⇒ n 800 cm2/V-s. 16 (b) Nd 10 cm3; (i) T 0°C ⇒ n 1400 cm2/V-s. (ii) T 100°C ⇒ n 780 cm2/V-s. ■ Comment The results of this example show that the mobility values are strong functions of the doping concentration and temperature. These variations must be taken into account in the design of semiconductor devices. ■ EXERCISE PROBLEM Ex 5.2 Using Figure 5.2, find the hole mobility in silicon for: (a) T 25°C for (i) Na 1016 cm3 and (ii) Na 1018 cm3, and (b) Na 1014 cm3 for (i) T 0°C and (ii) T 100°C. 5.1.3 Conductivity [(Ans. (a) (i) p 410 cm2/V-s, (ii) p 130 cm2/V-s; (b) (i) p 550 cm2/V-s, (ii) p 300 cm2/V-s)] The drift current density, given by Equation (5.9), may be written as Jdrf e(n n p p)E E (5.19) where is the conductivity of the semiconductor material. The conductivity is given in units of ( -cm)1 and is a function of the electron and hole concentrations and mobilities. We have just seen that the mobilities are functions of impurity concentrations; conductivity, then is a somewhat complicated function of impurity concentration. The reciprocal of conductivity is resistivity, which is denoted by and is given in units of ohm-cm. We can write the formula for resistivity as2 1 ___ 1 _ e(n n p p) (5.20) Figure 5.4 is a plot of resistivity as a function of impurity concentration in silicon, germanium, gallium arsenide, and gallium phosphide at T 300 K. Obviously, the curves are not linear functions of Nd or Na because of mobility effects. 2 The symbol is also used for volume charge density. The context in which is used should make it clear whether it stands for charge density or resistivity. nea29583_ch05_156-191.indd 164 12/11/10 10:15 AM 104 Silicon 300 K 103 Resistivity ( –cm) 102 101 n type (phosphorus) p type (boron) 100 101 102 103 104 1012 1013 1014 1015 1016 1017 1018 1019 1020 1021 Impurity concentration (cm3) 102 T 300 K n type p type 101 p GaP n GaP Resistivity ( –cm) 1 101 p-Ge n-Ge 103 104 1014 p-GaAs n-GaAs 102 1015 1016 1017 1018 Impurity concentration 1019 1020 1021 (cm3) Figure 5.4 | Resistivity versus impurity concentration at T 300 K in (a) silicon and (b) germanium, gallium arsenide, and gallium phosphide. (From Sze [14].) 165 nea29583_ch05_156-191.indd 165 12/11/10 10:15 AM 166 CHAPTER 5 Carrier Transport Phenomena I L V Area A Figure 5.5 | Bar of semiconductor material as a resistor. If we have a bar of semiconductor material as shown in Figure 5.5 with a voltage applied that produces a current I, then we can write I J_ A (5.21a) V E_ L (5.21b) and We can now rewrite Equation (5.19) as L (5.22a) (5.22b) V I _ _ A or L L I _ V _ I IR A A Equation (5.22b) is Ohm’s law for a semiconductor. The resistance is a function of resistivity, or conductivity, as well as the geometry of the semiconductor. If we consider, for example, a p-type semiconductor with an acceptor doping Na(Nd 0) in which Na ni, and if we assume that the electron and hole mobilities are of the same order of magnitude, then the conductivity becomes e(n n p p) ep p (5.23) If we also assume complete ionization, then Equation (5.23) becomes e Na 1 _ (5.24) The conductivity and resistivity of an extrinsic semiconductor are a function primarily of the majority carrier parameters. nea29583_ch05_156-191.indd 166 12/11/10 10:15 AM 5.1 167 T (K) 200 100 75 1016 10 1015 1.0 n 1014 0.1 Conductivity ( – cm)1 Electron concentration (cm3) 1017 500 1000 300 Carrier Drift ni 1013 0 4 8 1000 T 12 16 20 (K1) Figure 5.6 | Electron concentration and conductivity versus inverse temperature for silicon. (After Sze [14].) We may plot the carrier concentration and conductivity of a semiconductor as a function of temperature for a particular doping concentration. Figure 5.6 shows the electron concentration and conductivity of silicon as a function of inverse temperature for the case when Nd 1015 cm3. In the midtemperature range, or extrinsic range, as shown, we have complete ionization—the electron concentration remains essentially constant. However, the mobility is a function of temperature so the conductivity varies with temperature in this range. At higher temperatures, the intrinsic carrier concentration increases and begins to dominate the electron concentration as well as the conductivity. In the lower temperature range, freeze-out begins to occur; the electron concentration and conductivity decrease with decreasing temperature. Objective: Determine the doping concentration and majority carrier mobility given the type EXAMPLE 5.3 and conductivity of a compensated semiconductor. Consider compensated n-type silicon at T 300 K, with a conductivity of 16 ( -cm)1 and an acceptor doping concentration of 1017 cm3. Determine the donor concentration and the electron mobility. ■ Solution For n-type silicon at T 300 K, we can assume complete ionization; therefore the conductivity, assuming Nd Na ni, is given by en n en (Nd Na) We have that 16 (1.6 1019)n(Nd 1017) nea29583_ch05_156-191.indd 167 12/11/10 10:15 AM 168 CHAPTER 5 Carrier Transport Phenomena Since mobility is a function of the ionized impurity concentration, we can use Figure 5.3 along with trial and error to determine n and Nd. For example, if we choose Nd 2 1017, then NI Nd Na 3 1017 so that n 510 cm2/V-s which gives 8.16 ( -cm)1. If 17 we choose Nd 5 10 , then NI 6 1017 so that n 325 cm2/V-s, which gives 20.8 ( -cm)1. The doping is bounded between these two values. Further trial and error yields Nd 3.5 1017 cm3 and n 400 cm2/V-s which gives 16 ( -cm)1 ■ Comment We can see from this example that, in a high-conductivity semiconductor material, mobility is a strong function of carrier concentration. ■ EXERCISE PROBLEM A compensated p-type silicon material at T 300 K has impurity doping concentrations of Na 2.8 1017 cm3 and Nd 8 1016 cm3. Determine the (a) hole mobility, (b) conductivity, and (c) resistivity. 6.4 ( -cm)1, (c) 0.156 ( -cm)] DESIGN EXAMPLE 5.4 [Ans. (a) p 200 cm2/V-s; (b) Ex 5.3 Objective: Design a semiconductor resistor with a specified resistance to handle a given current density. A silicon semiconductor at T 300 K is initially doped with donors at a concentration of Nd 5 1015 cm3. Acceptors are to be added to form a compensated p-type material. The resistor is to have a resistance of 10 k and handle a current density of 50 A/cm2 when 5 V is applied. ■ Solution For 5 V applied to a 10-k resistor, the total current is V_ 5 0.5 mA I_ R 10 If the current density is limited to 50 A/cm2, then the cross-sectional area is 0.5 10 105 cm2 A _I __ J 50 3 If we, somewhat arbitrarily at this point, limit the electric field to E 100 V/cm, then the length of the resistor is V_ 5 5 102 cm L_ E 100 From Equation (5.22b), the conductivity of the semiconductor is 5 10 0.50 ( -cm)1 L __ _ RA (104)(105) 2 nea29583_ch05_156-191.indd 168 12/11/10 10:15 AM 5.1 Carrier Drift 169 The conductivity of a compensated p-type semiconductor is ep p ep (Na Nd) where the mobility is a function of the total ionized impurity concentration Na Nd. Using trial and error, if Na 1.25 1016 cm3, then Na Nd 1.75 1016 cm3, and the hole mobility, from Figure 5.3, is approximately p 410 cm2/V-s. The conductivity is then ep(Na Nd) (1.6 1019)(410)(1.25 1016 5 1015) 0.492 which is very close to the value we need. ■ Comment Since the mobility is related to the total ionized impurity concentration, the determination of the impurity concentration to achieve a particular conductivity is not straightforward. ■ EXERCISE PROBLEM Ex 5.4 A bar of p-type silicon, such as shown in Figure 5.5, has a cross-sectional area A 106 cm2 and a length L 1.2 103 cm. For an applied voltage of 5 V, a current of 2 mA is required. What is the required (a) resistance, (b) resistivity, and (c) impurity doping concentration? (d ) What is the resulting hole mobility? [Ans. (a) 2.5 k ; (b) 2.083 ( -cm); (c) Na 7.3 1015 cm3; (d ) p 410 cm2/V-s] For an intrinsic material, the conductivity can be written as i e(n p) ni (5.25) The concentrations of electrons and holes are equal in an intrinsic semiconductor, so the intrinsic conductivity includes both the electron and hole mobility. Since, in general, the electron and hole mobilities are not equal, the intrinsic conductivity is not the minimum value possible at a given temperature. 5.1.4 Velocity Saturation So far in our discussion of drift velocity, we have assumed that mobility is not a function of electric field, meaning that the drift velocity will increase linearly with applied electric field. The total velocity of a particle is the sum of the random thermal velocity and drift velocity. At T 300 K, the average random thermal energy is given by 3 kT _ 3 (0.0259) 0.03885 eV 1 mv2 _ _ (5.26) 2 th 2 2 7 This energy translates into a mean thermal velocity of approximately 10 cm /s for an electron in silicon. If we assume an electron mobility of n 1350 cm2/ V-s in low-doped silicon, a drift velocity of 105 cm/s, or 1 percent of the thermal velocity, is achieved if the applied electric field is approximately 75 V/cm. This applied electric field does not appreciably alter the energy of the electron. Figure 5.7 is a plot of average drift velocity as a function of applied electric field for electrons and holes in silicon, gallium arsenide, and germanium. At low electric fields, where there is a linear variation of velocity with electric field, the slope of nea29583_ch05_156-191.indd 169 12/11/10 10:15 AM 170 CHAPTER 5 Carrier Transport Phenomena Carrier drift velocity (cm /s) 108 GaAs (electrons) 107 Ge 106 105 102 T 300 K Electrons Holes Si 103 104 Electric field (V/cm) 105 106 Figure 5.7 | Carrier drift velocity versus electric field for high-purity silicon, germanium, and gallium arsenide. (From Sze [14].) the drift velocity versus electric field curve is the mobility. The behavior of the drift velocity of carriers at high electric fields deviates substantially from the linear relationship observed at low fields. The drift velocity of electrons in silicon, for example, saturates at approximately 107 cm /s at an electric field of approximately 30 kV/cm. If the drift velocity of a charge carrier saturates, then the drift current density also saturates and becomes independent of the applied electric field. The experimental carrier drift velocity versus electric field in silicon can be approximated for electrons by [2] vs vn ___ (5.27a) Eon 2 12 1 _ E and for holes by vs vp __ Eop 1 _ E (5.27b) The variables are vs 107 cm/s at T 300 K, Eon 7 103 V/cm, and Eop 2 104 V/cm. We may note that for small electric fields, the drift velocities reduce to E v vn _ s Eon (5.28a) (5.28b) and E vp _ Eop vs nea29583_ch05_156-191.indd 170 12/11/10 10:15 AM 5.1 Carrier Drift 171 At low electric fields, the drift velocities are linear functions of the electric field as we have discussed. However, for large electric fields, the drift velocities approach the saturation value. The drift velocity versus electric field characteristic of gallium arsenide is more complicated than for silicon or germanium. At low fields, the slope of the drift velocity versus E-field is constant and is the low-field electron mobility, which is approximately 8500 cm2/V-s for gallium arsenide. The low-field electron mobility in gallium arsenide is much larger than in silicon. As the field increases, the electron drift velocity in gallium arsenide reaches a peak and then decreases. A differential mobility is the slope of the vd versus E curve at a particular point on the curve and the negative slope of the drift velocity versus electric field represents a negative differential mobility. The negative differential mobility produces a negative differential resistance; this characteristic is used in the design of oscillators. The negative differential mobility can be understood by considering the E versus k diagram for gallium arsenide, which is shown again in Figure 5.8. The density of states effective mass of the electron in the lower valley is m*n 0.067 m0. The small effective mass leads to a large mobility. As the E-field increases, the energy of the electron increases and the electron can be scattered into the upper valley, where the density of states effective mass is 0.55 m0. The larger effective mass in the upper valley yields a smaller mobility. This intervalley transfer mechanism results in a decreasing average drift velocity of electrons with electric field, or the negative differential mobility characteristic. Conduction band GaAs Upper valley E 0.31 Lower valley Eg Valence band [111] 0 [100] Figure 5.8 | Energy-band structure for gallium arsenide showing the upper valley and lower valley in the conduction band. (From Sze [15].) nea29583_ch05_156-191.indd 171 12/11/10 10:15 AM 172 CHAPTER 5 Carrier Transport Phenomena TEST YOUR UNDERSTANDING TYU 5.1 Consider a sample of silicon at T 300 K doped at an impurity concentration of Nd 1015 cm3 and Na 1014 cm3. Assume electron and hole mobilities given in Table 5.1. Calculate the drift current density if the applied electric field is E 35 V/cm. Silicon at T 300 K is doped with impurity concentrations of Nd 5 1016 cm3 and Na 2 1016 cm3. (a) What are the electron and hole mobilities? (b) Determine the conductivity and resistivity of the material. (Ans. 6.80 A/cm2) -cm] TYU 5.3 [Ans. (a) n 1000 cm2/V-s, p 350 cm2/V-s; (b) 4.8 ( -cm)1, 0.208 TYU 5.2 For a particular silicon semiconductor device at T 300 K, the required material is n type with a resistivity of 0.10 -cm. (a) Determine the required impurity doping concentration and (b) the resulting electron mobility. [Ans. (a) From Figure 5.4, Nd 9 10 16 cm3; (b) n 695 cm2/V-s] 5.2 | CARRIER DIFFUSION There is a second mechanism, in addition to drift, that can induce a current in a semiconductor. We may consider a classic physics example in which a container, as shown in Figure 5.9, is divided into two parts by a membrane. The left side contains gas molecules at a particular temperature and the right side is initially empty. The gas molecules are in continual random thermal motion so that, when the membrane is broken, the gas molecules flow into the right side of the container. Diffusion is the process whereby particles flow from a region of high concentration toward a region of low concentration. If the gas molecules were electrically charged, the net flow of charge would result in a diffusion current. 5.2.1 Diffusion Current Density To begin to understand the diffusion process in a semiconductor, we will consider a simplified analysis. Assume that an electron concentration varies in one dimension as shown in Figure 5.10. The temperature is assumed to be uniform so that the average thermal velocity of electrons is independent of x. To calculate the current, we will determine the net flow of electrons per unit time per unit area crossing the plane at x 0. If the distance l shown in Figure 5.10 is less than the mean-free path of an electron, that is, the average x0 Figure 5.9 | Container divided by a membrane with gas molecules on one side. nea29583_ch05_156-191.indd 172 12/11/10 10:15 AM Carrier Diffusion 173 n(x) 5.2 n(l) n(0) n(l) x l x0 x l x Figure 5.10 | Electron concentration versus distance. distance an electron travels between collisions (l vth cn), then on the average, electrons moving to the right at x l and electrons moving to the left at x l will cross the x 0 plane. One half of the electrons at x l will be traveling to the right at any instant of time and one half of the electrons at x l will be traveling to the left at any given time. The net rate of electron flow, Fn, in the x direction at x 0 is given by 1 n(l)v _ 1 n(l )v _ 1 v [n(l ) n(l )] Fn _ th th 2 2 2 th (5.29) If we expand the electron concentration in a Taylor series about x 0 keeping only the first two terms, then we can write Equation (5.29) as 1v Fn _ 2 th dn n(0) l _ dn n(0) l _ dx dx (5.30) which becomes dn Fn vth l _ dx (5.31) Each electron has a charge (e), so the current is dn J eFn evth l _ dx (5.32) The current described by Equation (5.32) is the electron diffusion current and is proportional to the spatial derivative, or density gradient, of the electron concentration. The diffusion of electrons from a region of high concentration to a region of low concentration produces a flux of electrons flowing in the negative x direction for this example. Since electrons have a negative charge, the conventional current direction is in the positive x direction. Figure 5.11a shows these one-dimensional flux and nea29583_ch05_156-191.indd 173 12/11/10 10:15 AM CHAPTER 5 Carrier Transport Phenomena Electron concentration, n 174 Electron flux Electron diffusion current density x Hole concentration, p (a) Hole flux Hole diffusion current density x (b) Figure 5.11 | (a) Diffusion of electrons due to a density gradient. (b) Diffusion of holes due to a density gradient. current directions. We may write the electron diffusion current density for this onedimensional case, in the form dn Jnxdif eDn _ dx (5.33) where Dn is called the electron diffusion coefficient, has units of cm2/s, and is a positive quantity. If the electron density gradient becomes negative, the electron diffusion current density will be in the negative x direction. Figure 5.11b shows an example of a hole concentration as a function of distance in a semiconductor. The diffusion of holes, from a region of high concentration to a region of low concentration, produces a flux of holes in the negative x direction. Since holes are positively charged particles, the conventional diffusion current density is also in the negative x direction. The hole diffusion current density is proportional to the hole density gradient and to the electronic charge, so we may write dp Jpxdif eDp _ dx (5.34) for the one-dimensional case. The parameter Dp is called the hole diffusion coefficient, has units of cm2/s, and is a positive quantity. If the hole density gradient becomes negative, the hole diffusion current density will be in the positive x direction. nea29583_ch05_156-191.indd 174 12/11/10 10:15 AM 5.2 Carrier Diffusion Objective: Calculate the diffusion current density given a density gradient. 175 EXAMPLE 5.5 Assume that, in an n-type gallium arsenide semiconductor at T 300 K, the electron concentration varies linearly from 1 1018 to 7 1017 cm3 over a distance of 0.10 cm. Calculate the diffusion current density if the electron diffusion coefficient is Dn 225 cm2/s. ■ Solution The diffusion current density is given by dn eD _ n Jndif eDn _ n dx x 1 1018 7 1017 108 A /cm2 (1.6 1019)(225) ____ 0. 10 ■ Comment A significant diffusion current density can be generated in a semiconductor material with only a modest density gradient. ■ EXERCISE PROBLEM Ex 5.5 The hole density in silicon is given by p(x) 1016 e(xLp) (x 0) where Lp 2 104 cm. Assume the hole diffusion coefficient is Dp 8 cm2/s. Determine the hole diffusion current density at (a) x 0, (b) x 2 104 cm, and (c) x 103 cm. [Ans. (a) Jp 64 A/cm 2; (b) Jp 23.54 A/cm 2; (c) Jp 0.431 A/cm2] 5.2.2 Total Current Density We now have four possible independent current mechanisms in a semiconductor. These components are electron drift and diffusion currents and hole drift and diffusion currents. The total current density is the sum of these four components, or, for the one-dimensional case, dp dn eD _ J enn Ex epp Ex eDn _ p dx dx (5.35) This equation may be generalized to three dimensions as J enn E epp E eDnn eDpp (5.36) The electron mobility gives an indication of how well an electron moves in a semiconductor as a result of the force of an electric field. The electron diffusion coefficient gives an indication of how well an electron moves in a semiconductor as a result of a density gradient. The electron mobility and diffusion coefficient are not independent parameters. Similarly, the hole mobility and diffusion coefficient are not independent parameters. The relationship between mobility and the diffusion coefficient is developed in the next section. The expression for the total current in a semiconductor contains four terms. Fortunately in most situations, we will only need to consider one term at any one time at a particular point in a semiconductor. nea29583_ch05_156-191.indd 175 12/11/10 10:15 AM 176 CHAPTER 5 Carrier Transport Phenomena TEST YOUR UNDERSTANDING TYU 5.4 The electron concentration in silicon is given by n(x) 1015 e(xLn) cm3 (x 0) where Ln 104 cm. The electron diffusion coefficient is Dn 25 cm2/s. Determine the electron diffusion current density at (a) x 0, (b) x 104 cm, and (c) x → . The hole concentration in silicon varies linearly from x 0 to x 0.01 cm. The hole diffusion coefficient is Dp 10 cm2/s, the hole diffusion current density is 20 A/cm2, and the hole concentration at x 0 is p 4 1017 cm3. What is the value of the hole concentration at x 0.01 cm? [Ans. (a) 40 A/cm 2; (b) 14.7 A/cm 2; (c) 0] TYU 5.5 (Ans. 2.75 10 17 cm3) 5.3 | GRADED IMPURITY DISTRIBUTION In most cases so far, we have assumed that the semiconductor is uniformly doped. In many semiconductor devices, however, there may be regions that are nonuniformly doped. We will investigate how a nonuniformly doped semiconductor reaches thermal equilibrium and, from this analysis, we will derive the Einstein relation, which relates mobility and the diffusion coefficient. 5.3.1 Induced Electric Field Consider a semiconductor that is nonuniformly doped with donor impurity atoms. If the semiconductor is in thermal equilibrium, the Fermi energy level is constant through the crystal so the energy-band diagram may qualitatively look like that shown in Figure 5.12. The doping concentration decreases as x increases in this case. There will be a diffusion of majority carrier electrons from the region of high concentration to the region of low concentration, which is in the x direction. The flow of negative electrons leaves behind positively charged donor ions. The separation of Ec EF EFi Ev x Figure 5.12 | Energy-band diagram for a semiconductor in thermal equilibrium with a nonuniform donor impurity concentration. nea29583_ch05_156-191.indd 176 12/11/10 10:15 AM 5.3 Graded Impurity Distribution 177 positive and negative charge induces an electric field that is in a direction to oppose the diffusion process. When equilibrium is reached, the mobile carrier concentration is not exactly equal to the fixed impurity concentration and the induced electric field prevents any further separation of charge. In most cases of interest, the space charge induced by this diffusion process is a small fraction of the impurity concentration, thus the mobile carrier concentration is not too different from the impurity dopant density. The electric potential is related to electron potential energy by the charge (e), so we can write 1 (E E ) _ Fi e F (5.37) The electric field for the one-dimensional situation is defined as d 1 _ dEFi Ex _ _ e dx dx (5.38) If the intrinsic Fermi-level changes as a function of distance through a semiconductor in thermal equilibrium, an electric field exists in the semiconductor. If we assume a quasi-neutrality condition in which the electron concentration is almost equal to the donor impurity concentration, then we can still write EF EFi n0 ni exp __ Nd (x) kT Solving for EF EFi, we obtain (5.39) Nd (x) EF EFi kT ln _ (5.40) ni The Fermi level is constant for thermal equilibrium so when we take the derivative with respect to x we obtain dNd (x) dEFi _ _ kT __ Nd (x) dx dx (5.41) The electric field can then be written, combining Equations (5.41) and (5.38), as dNd (x) kT _ 1 __ Ex _ e Nd (x) dx (5.42) Since we have an electric field, there will be a potential difference through the semiconductor due to the nonuniform doping. Objective: Determine the induced electric field in a semiconductor in thermal equilibrium, EXAMPLE 5.6 given a linear variation in doping concentration. Assume that the donor concentration in an n-type semiconductor at T 300 K is given by Nd (x) 1016 1019 x (cm3) where x is given in cm and ranges between 0 x 1 m nea29583_ch05_156-191.indd 177 12/11/10 10:15 AM 178 CHAPTER 5 Carrier Transport Phenomena ■ Solution Taking the derivative of the donor concentration, we have dNd (x) __ (cm4) 1019 dx The electric field is given by Equation (5.42), so we have (0.0259)(1019) Ex ___ (1016 1019x) At x 0, for example, we find Ex 25.9 V/cm ■ Comment We may recall from our previous discussion of drift current that fairly small electric fields can produce significant drift current densities, so that an induced electric field from nonuniform doping can significantly influence semiconductor device characteristics. ■ EXERCISE PROBLEM Ex 5.6 Assume the donor concentration in an n-type semiconductor at T 300 K is given by Nd (x) 1016 exL where L 2 102 cm. Determine the induced electric field in the semiconductor at (a) x 0 and (b) x 104 cm. 5.3.2 The Einstein Relation [Ans. E 1.295 V/cm for (a) and (b)] If we consider the nonuniformly doped semiconductor represented by the energyband diagram shown in Figure 5.12 and assume there are no electrical connections so that the semiconductor is in thermal equilibrium, then the individual electron and hole currents must be zero. We can write dn (5.43) Jn 0 enn Ex eDn _ dx If we assume quasi-neutrality so that n Nd (x), then we can rewrite Equation (5.43) as dNd (x) Jn 0 en Nd (x)Ex eDn __ (5.44) dx Substituting the expression for the electric field from Equation (5.42) into Equation (5.44), we obtain dNd (x) dNd (x) kT _ 1 __ __ 0 en Nd (x) _ (5.45) e Nd (x) dx eDn dx Equation (5.45) is valid for the condition Dn kT _ _ (5.46a) n e The hole current must also be zero in the semiconductor. From this condition, we can show that Dp kT _ _ (5.46b) p e nea29583_ch05_156-191.indd 178 12/11/10 10:15 AM 5.3 Graded Impurity Distribution 179 Combining Equations (5.46a) and (5.46b) gives Dp Dn kT _ _ _ e n (5.47) p The diffusion coefficient and mobility are not independent parameters. This relation between the mobility and diffusion coefficient, given by Equation (5.47), is known as the Einstein relation. Objective: Determine the diffusion coefficient given the carrier mobility. EXAMPLE 5.7 Assume that the mobility of a particular carrier is 1000 cm2/V-s at T 300 K. ■ Solution Using the Einstein relation, we have that kT (0.0259)(1000) 25.9 cm2/s D _ e ■ Comment Although this example is fairly simple and straightforward, it is important to keep in mind the relative orders of magnitude of the mobility and diffusion coefficient. The diffusion coefficient is approximately 40 times smaller than the mobility at room temperature. ■ EXERCISE PROBLEM Ex 5.7 Assume the electron diffusion coefficient of a semiconductor at T 300 K is Dn 215 cm2/s. Determine the electron mobility. (Ans. n 8301 cm 2 /V-s) Table 5.2 shows the diffusion coefficient values at T 300 K corresponding to the mobilities listed in Table 5.1 for silicon, gallium arsenide, and germanium. The relation between the mobility and diffusion coefficient given by Equation (5.47) contains temperature. It is important to keep in mind that the major temperature effects are a result of lattice scattering and ionized impurity scattering processes, as discussed in Section 5.1.2. As the mobilities are strong functions of temperature because of the scattering processes, the diffusion coefficients are also strong functions of temperature. The specific temperature dependence given in Equation (5.47) is a small fraction of the real temperature characteristic. Table 5.2 | Typical mobility and diffusion coefficient values at T 300 K ( = cm2/V-s and D = cm2/s) Silicon Gallium arsenide Germanium nea29583_ch05_156-191.indd 179 m Dn p Dp 1350 8500 3900 35 220 101 480 400 1900 12.4 10.4 49.2 12/11/10 10:15 AM 180 CHAPTER 5 Carrier Transport Phenomena *5.4 | THE HALL EFFECT The Hall effect is a consequence of the forces that are exerted on moving charges by electric and magnetic fields. The Hall effect is used to distinguish whether a semiconductor is n type or p type3 and to measure the majority carrier concentration and majority carrier mobility. The Hall effect device, as discussed in this section, is used to experimentally measure semiconductor parameters. However, it is also used extensively in engineering applications as a magnetic probe and in other circuit applications. The force on a particle having a charge q and moving in a magnetic field is given by F qv B (5.48) where the cross product is taken between velocity and magnetic field so that the force vector is perpendicular to both the velocity and magnetic field. Figure 5.13 illustrates the Hall effect. A semiconductor with a current Ix is placed in a magnetic field perpendicular to the current. In this case, the magnetic field is in the z direction. Electrons and holes flowing in the semiconductor will experience a force as indicated in the figure. The force on both electrons and holes is in the (y) direction. In a p-type semiconductor ( p0 n0), there will be a buildup of positive charge on the y 0 surface of the semiconductor and, in an n-type semiconductor (n0 p0), there will be a buildup of negative charge on the y 0 surface. This net charge induces an electric field in the y direction as shown in the figure. In steady Bz VH e h EH z d EH W y x L Ix Vx Figure 5.13 | Geometry for measuring the Hall effect. *Indicates sections that will aid in the total summation of understanding of semiconductor devices, but may be skipped the first time through the text without loss of continuity. 3 We will assume an extrinsic semiconductor material in which the majority carrier concentration is much larger than the minority carrier concentration. nea29583_ch05_156-191.indd 180 12/11/10 10:15 AM 5.4 The Hall Effect 181 state, the magnetic field force will be exactly balanced by the induced electric field force. This balance may be written as F q[E v B] 0 (5.49a) qEy qvx Bz (5.49b) which becomes The induced electric field in the y direction is called the Hall field. The Hall field produces a voltage across the semiconductor which is called the Hall voltage. We can write VH EH W (5.50) where EH is assumed positive in the y direction and VH is positive with the polarity shown. In a p-type semiconductor, in which holes are the majority carrier, the Hall voltage will be positive as defined in Figure 5.13. In an n-type semiconductor, in which electrons are the majority carrier, the Hall voltage will have the opposite polarity. The polarity of the Hall voltage is used to determine whether an extrinsic semiconductor is n type or p type. Substituting Equation (5.50) into Equation (5.49) gives VH vx WBz (5.51) For a p-type semiconductor, the drift velocity of holes can be written as Jx Ix __ vdx _ ep (ep)(Wd ) (5.52) where e is the magnitude of the electronic charge. Combining Equations (5.52) and (5.50), we have Ix Bz VH _ epd (5.53) or, solving for the hole concentration, we obtain Ix Bz p_ edVH (5.54) The majority carrier hole concentration is determined from the current, magnetic field, and Hall voltage. For an n-type semiconductor, the Hall voltage is given by Ix Bz VH _ ned (5.55) Ix Bz n _ edVH (5.56) so that the electron concentration is Note that the Hall voltage is negative for the n-type semiconductor; therefore, the electron concentration determined from Equation (5.56) is actually a positive quantity. nea29583_ch05_156-191.indd 181 12/11/10 10:15 AM 182 CHAPTER 5 Carrier Transport Phenomena Once the majority carrier concentration has been determined, we can calculate the low-field majority carrier mobility. For a p-type semiconductor, we can write Jx epp Ex (5.57) The current density and electric field can be converted to current and voltage so that Equation (5.57) becomes eppVx Ix _ __ (5.58) L Wd The hole mobility is then given by Ix L p __ epVx Wd (5.59) Similarly for an n-type semiconductor, the low-field electron mobility is determined from Ix L n __ enVx Wd EXAMPLE 5.8 (5.60) Objective: Determine the majority carrier concentration and mobility, given Hall effect parameters. Consider the geometry shown in Figure 5.13. Let L 101 cm, W 102 cm, and d 103 cm. Also assume that Ix 1.0 mA, Vx 12.5 V, Bz 500 gauss 5 102 tesla, and VH 6.25 mV. ■ Solution A negative Hall voltage for this geometry implies that we have an n-type semiconductor. Using Equation (5.56), we can calculate the electron concentration as (103)(5 102) n ______ 5 1021 m3 5 1015 cm3 (1.6 1019)(105)(6.25 103) The electron mobility is then determined from Equation (5.60) as (103)(103) n _______ 0.10 m2/V-s 19 (1.6 10 )(5 1021)(12.5)(104)(105) or n 1000 cm2/V-s ■ Comment It is important to note that the MKS units must be used consistently in the Hall effect equations to yield correct results. ■ EXERCISE PROBLEM Ex 5.8 A p-type silicon sample with the geometry shown in Figure 5.13 has parameters L 0.2 cm, W 102 cm, and d 8 104 cm. The semiconductor parameters are p 1016 cm3 and p 320 cm2/V-s. For Vx 10 V and Bz 500 gauss 5 102 tesla, determine Ix and VH . (Ans. Ix 0.2048 mA, VH 0.80 mV) nea29583_ch05_156-191.indd 182 12/11/10 10:15 AM Glossary of Important Terms 183 5.5 | SUMMARY ■ ■ ■ ■ ■ ■ ■ ■ The two basic transport mechanisms are drift, due to an applied electric field, and diffusion, due to a density gradient. Carriers reach an average drift velocity in the presence of an applied electric field, due to scattering events. Two scattering processes within a semiconductor are lattice scattering and impurity scattering. The average drift velocity is a linear function of the applied electric field for small values of electric field, but the drift velocity reaches a saturation limit that is on the order of 10 7 cm/s at high electric fields. Carrier mobility is the ratio of the average drift velocity and applied electric field. The electron and hole mobilities are functions of temperature and of the ionized impurity concentration. The drift current density is the product of conductivity and electric field (a form of Ohm’s law). Conductivity is a function of the carrier concentrations and mobilities. Resistivity is the inverse of conductivity. The diffusion current density is proportional to the carrier diffusion coefficient and the carrier density gradient. The diffusion coefficient and mobility are related through the Einstein relation. The Hall effect is a consequence of a charged carrier moving in the presence of perpendicular electric and magnetic fields. The charged carrier is deflected, inducing a Hall voltage. The polarity of the Hall voltage is a function of the semiconductor conductivity type. The majority carrier concentration and mobility can be determined from the Hall voltage. GLOSSARY OF IMPORTANT TERMS conductivity A material parameter related to carrier drift; quantitatively, the ratio of drift current density to electric field. diffusion The process whereby particles flow from a region of high concentration to a region of low concentration. diffusion coefficient The parameter relating particle flux to the particle density gradient. diffusion current The current that results from the diffusion of charged particles. drift The process whereby charged particles move while under the influence of an electric field. drift current The current that results from the drift of charged particles. drift velocity The average velocity of charged particles in the presence of an electric field. Einstein relation The relation between the mobility and the diffusion coefficient. Hall voltage The voltage induced across a semiconductor in a Hall effect measurement. ionized impurity scattering The interaction between a charged carrier and an ionized impurity center. lattice scattering The interaction between a charged carrier and a thermally vibrating lattice atom. mobility The parameter relating carrier drift velocity and electric field. resistivity The reciprocal of conductivity; a material parameter that is a measure of the resistance to current. velocity saturation The saturation of carrier drift velocity with increasing electric field. nea29583_ch05_156-191.indd 183 12/11/10 10:15 AM 184 CHAPTER 5 Carrier Transport Phenomena CHECKPOINT After studying this chapter, the reader should have the ability to: ■ ■ ■ ■ ■ ■ ■ ■ ■ Discuss carrier drift current density. Explain why carriers reach an average drift velocity in the presence of an applied electric field. Discuss the mechanisms of lattice scattering and impurity scattering. Define mobility and discuss the temperature and ionized impurity concentration dependence on mobility. Define conductivity and resistivity. Discuss velocity saturation. Discuss carrier diffusion current density. State the Einstein relation. Describe the Hall effect. REVIEW QUESTIONS 1. Write the equation for the total drift current density. Is the linear relationship between drift current density and electric field always valid? Why or why not. 2. Define electron and hole mobility. What is the unit of mobility? 3. Explain the temperature dependence of mobility. Why is the carrier mobility a function of the ionized impurity concentrations? 4. Define conductivity. Define resistivity. What are the units of conductivity and resistivity? 5. Sketch the drift velocity of electrons in silicon versus electric field. Repeat for GaAs. 6. Write the equations for the diffusion current densities of electrons and holes. 7. What is the Einstein relation? 8. What is the direction of the induce electric field in a semiconductor with a graded donor impurity concentration? Repeat for a graded acceptor impurity concentration. 9. Describe the Hall effect. 10. Explain why the polarity of the Hall voltage changes depending on the conductivity type (n type or p type) of the semiconductor. PROBLEMS (Note: Use the semiconductor parameters given in Appendix B if the parameters are not specifically given in a problem.) Section 5. 1 5.1 5.2 nea29583_ch05_156-191.indd 184 Carrier Drift The concentration of donor impurity atoms in silicon is Nd 1015 cm3. Assume an electron mobility of n 1300 cm2/V-s and a hole mobility of p 450 cm2/V-s. (a) Calculate the resistivity of the material. (b) What is the conductivity of the material? A p-type silicon material is to have a conductivity of 1.80 ( -cm)1. If the mobility values are n 1250 cm2/V-s and p 380 cm2/V-s, what must be the acceptor impurity concentration in the material? 12/11/10 10:15 AM Problems 185 (a) The required conductivity of an n-type silicon sample at T 300 K is to be 10 ( -cm)1. What donor impurity concentration is required? What is the electron mobility corresponding to this impurity concentration? (b) A p-type silicon material is required to have a resistivity of 0.20 ( -cm). What acceptor impurity concentration is required and what is the corresponding hole mobility? 5.4 (a) The resistivity of a p-type GaAs material at T 300 K is required to be 0.35 ( -cm). Determine the acceptor impurity concentration that is required. What is the hole mobility corresponding to this impurity concentration? (b) An n-type GaAs material is required to have a conductivity of 120 ( -cm)1. What donor impurity concentration is required and what is the corresponding electron mobility? 5.5 A silicon sample is 2.5 cm long and has a cross-sectional area of 0.1 cm2. The silicon is n type with a donor impurity concentration of Nd 2 1015 cm3. The resistance of the sample is measured and found to be 70 . What is the electron mobility? 5.6 Consider a homogeneous gallium arsenide semiconductor at T 300 K with Nd 1016 cm3 and Na 0. (a) Calculate the thermal-equilibrium values of electron and hole concentrations. (b) For an applied E-field of 10 V/cm, calculate the drift current density. (c) Repeat parts (a) and (b) if Nd 0 and Na 1016 cm3. 5.7 A silicon crystal having a cross-sectional area of 0.001 cm2 and a length of 103 cm is connected at its ends to a 10-V battery. At T 300 K, we want a current of 100 mA in the silicon. Calculate (a) the required resistance R, (b) the required conductivity, (c) the density of donor atoms to be added to achieve this conductivity, and (d) the concentration of acceptor atoms to be added to form a compensated p-type material with the conductivity given from part (b) if the initial concentration of donor atoms is Nd 1015 cm3. 5.8 (a) A silicon semiconductor resistor is in the shape of a rectangular bar with a crosssectional area of 8.5 104 cm2, a length of 0.075 cm, and is doped with a concentration of 2 1016 cm3 boron atoms. Let T 300 K. A bias of 2 volts is applied across the length of the silicon device. Calculate the current in the resistor. (b) Repeat part (a) if the length is increased by a factor of three. (c) Determine the average drift velocity of holes in parts (a) and (b). 5.9 (a) A GaAs semiconductor resistor is doped with donor impurities at a concentration of Nd 2 1015 cm3 and has a cross-sectional area of 5 105 cm2. A current of I 25 mA is induced in the resistor with an applied bias of 5 V. Determine the length of the resistor. (b) Using the results of part (a), calculate the drift velocity of the electrons. (c) If the bias applied to the resistor in part (a) increases to 20 V, determine the resulting current if the electrons are traveling at their saturation velocity of 5 106 cm/s. 5.10 (a) Three volts is applied across a 1-cm-long semiconductor bar. The average electron drift velocity is 104 cm/s. Find the electron mobility. (b) If the electron mobility in part (a) were 800 cm2/V-s, what is the average electron drift velocity? 5.11 Use the velocity–field relations for silicon and gallium arsenide shown in Figure 5.7 to determine the transit time of electrons through a 1-m distance in these materials for an electric field of (a) 1 kV/cm and (b) 50 kV/cm. 5.12 A perfectly compensated semiconductor is one in which the donor and acceptor impurity concentrations are exactly equal. Assuming complete ionization, determine the resistivity of silicon at T 300 K in which the impurity concentrations are (a) Na Nd 1014 cm3, (b) Na Nd 1016 cm3, and (c) Na Nd 1018 cm3. 5.3 nea29583_ch05_156-191.indd 185 12/11/10 10:15 AM 186 CHAPTER 5 5.13 5.14 5.15 5.16 5.17 5.18 5.19 Carrier Transport Phenomena (a) In a p-type gallium arsenide semiconductor, the conductivity is 5 ( -cm)1 at T 300 K. Calculate the thermal-equilibrium values of the electron and hole concentrations. (b) Repeat part (a) for n-type silicon if the resistivity is 8 -cm. In a particular semiconductor material, n 1000 cm2/V-s, p 600 cm2/V-s, and NC NV 1019 cm3. These parameters are independent of temperature. The measured conductivity of the intrinsic material is 106 ( -cm)1 at T 300 K. Find the conductivity at T 500 K. (a) Calculate the resistivity at T 300 K of intrinsic (i) silicon, (ii) germanium, and (iii) gallium arsenide. (b) If rectangular semiconductor bars are fabricated using the materials in part (a), determine the resistance of each bar if its cross-sectional area is 85 m2 and length is 200 m. An n-type silicon material at 300 K has a conductivity of 0.25 ( -cm)1. (a) What is the donor impurity concentration and the corresponding electron mobility? (b) Determine the expected conductivity of the material at (i) T 250 K and (ii) T 400 K. The conductivity of a semiconductor layer varies with depth as (x) o exp(xd) where o 20 ( -cm)1 and d 0.3 m. If the thickness of the semiconductor layer is t 1.5 m, determine the average conductivity of this layer. An n-type silicon resistor has a length L 150 m, width W 7.5 m, and thickness T 1 m. A voltage of 2 V is applied across the length of the resistor. The donor impurity concentration varies linearly through the thickness of the resistor with Nd 2 1016 cm3 at the top surface and Nd 2 1015 cm3 at the bottom surface. Assume an average carrier mobility of n 750 cm2/V-s. (a) What is the electric field in the resistor? (b) Determine the average conductivity of the silicon. (c) Calculate the current in the resistor. (d) Determine the current density near the top surface and the current density near the bottom surface. Consider silicon doped at impurity concentrations of Nd 2 1016 cm3 and Na 0. An empirical expression relating electron drift velocity to electric field is given by n0E ___________ vd ___ n0E 2 1 _ vsat 7 2 where n0 1350 cm /V-s, vsat 1.8 10 cm/s, and E is given in V/cm. Plot electron drift current density (magnitude) versus electric field (log–log scale) over the range 0 E 106 V/cm. Consider silicon at T 300 K. Assume the electron mobility is n 1350 cm2/V-s. The kinetic energy of an electron in the conduction band is (12)m*n v2d, where m*n is the effective mass and vd is the drift velocity. Determine the kinetic energy of an electron in the conduction band if the applied electric field is (a) 10 V/cm and (b) 1 kV/cm. Consider a semiconductor that is uniformly doped with Nd 1014 cm3 and Na 0, with an applied electric field of E 100 V/cm. Assume that n 1000 cm2/V-s and p 0. Also assume the following parameters: 5.20 5.21 Nc 2 1019 (T300)32 cm3 Nv 1 1019 (T300)32 cm3 Eg 1.10 eV (a) Calculate the electric-current density at T 300 K. (b) At what temperature will this current increase by 5 percent? (Assume the mobilities are independent of temperature.) nea29583_ch05_156-191.indd 186 12/11/10 10:15 AM Problems 5.22 187 A semiconductor material has electron and hole mobilities n and p, respectively. When the conductivity is considered as a function of the hole concentration p0, (a) show that the minimum value of conductivity, min, can be written as 2i (n p)12 min ___ (n p) 5.23 5.24 5.25 5.26 5.27 where i is the intrinsic conductivity, and (b) show that the corresponding hole concentration is p0 ni(np)12. Consider three samples of silicon at T 300 K. The n-type sample is doped with arsenic atoms to a concentration of Nd 5 1016 cm3. The p-type sample is doped with boron atoms to a concentration of Na 2 1016 cm3. The compensated sample is doped with both the donors and acceptors described in the n-type and p-type samples. (a) Find the equilibrium electron and hole concentrations in each sample, (b) determine the majority carrier mobility in each sample, (c) calculate the conductivity of each sample, (d) and determine the electric field required in each sample to induce a drift current density of J 120 A/cm2. Three scattering mechanisms are present in a particular semiconductor material. If only the first scattering mechanism were present, the mobility would be 1 2000 cm2/V-s, if only the second mechanism were present, the mobility would be 2 1500 cm2/V-s, and if only the third mechanism were present, the mobility would be 3 500 cm2/V-s. What is the net mobility? Assume that the mobility of electrons in silicon at T 300 K is n 1300 cm2/V-s. Also assume that the mobility is limited by lattice scattering and varies as T32. Determine the electron mobility at (a) T 200 K and (b) T 400 K. Two scattering mechanisms exist in a semiconductor. If only the first mechanism were present, the mobility would be 250 cm2/V-s. If only the second mechanism were present, the mobility would be 500 cm2/V-s. Determine the mobility when both scattering mechanisms exist at the same time. The effective density of states functions in silicon can be written in the form T Nc 2.8 1019 _ 300 32 T Nv 1.04 1019 _ 300 32 Assume the mobilities are given by T n 1350 _ 300 32 T p 480 _ 300 32 Assume the bandgap energy is Eg 1.12 eV and independent of temperature. Plot the intrinsic conductivity as a function of T over the range 200 T 600 K. 5.28 (a) Assume that the electron mobility in an n-type semiconductor is given by 1350 n ___ cm2/V-s 12 Nd 1 __ 5 1016 where Nd is the donor concentration in cm3. Assuming complete ionization, plot the conductivity as a function of Nd over the range 1015 Nd 1018 cm3. (b) Compare the results of part (a) to that if the mobility were assumed to be a constant equal to 1350 cm2/V-s. (c) If an electric field of E 10 V/cm is applied to the semiconductor, plot the electron drift current density of parts (a) and (b). nea29583_ch05_156-191.indd 187 12/11/10 10:15 AM 188 CHAPTER 5 Carrier Transport Phenomena Section 5.2 Carrier Diffusion 5.29 5.30 5.31 5.32 5.33 5.34 5.35 Consider a sample of silicon at T 300 K. Assume that the electron concentration varies linearly with distance, as shown in Figure P5.29. The diffusion current density is found to be Jn 0.19 A/cm2. If the electron diffusion coefficient is Dn 25 cm2/s, determine the electron concentration at x 0. The steady-state electron distribution in silicon can be approximated by a linear function of x. The maximum electron concentration occurs at x 0 and is n(0) 2 1016 cm3. At x 0.012 cm, the electron concentration is 5 1015 cm3. If the electron diffusion coefficient is Dn 27 cm2/s, determine the electron diffusion current density. The electron diffusion current density in a semiconductor is a constant and is given by Jn 2 A/cm2. The electron concentration at x 0 is n(0) 1015 cm3. (a) Calculate the electron concentration at x 20 m if the material is silicon with Dn 30 cm2/s. (b) Repeat part (a) if the material is GaAs with Dn 230 cm2/s. The hole concentration in p-type GaAs is given by p(x) 1016 (1 xL)2 cm3 for L x 0 where L 12 m. The hole diffusion coefficient is Dp 10 cm2/s. Calculate the hole diffusion current density at (a) x 0, (b) x 6 m, and (c) x 12 m. In silicon, the electron concentration is given by n(x) 1015exLn cm3 for x 0 and the hole concentration is given by p(x) 5 1015exLp cm3 for x 0 . The parameter values are Ln 2 103 cm and LP 5 104 cm. The electron and hole diffusion coefficients are Dn 25 cm2/s and DP 10 cm2/s, respectively. The total current density is defined as the sum of the electron and hole diffusion current densities at x 0. Calculate the total current density. The concentration of holes in a semiconductor is given by p(x) 5 1015exLp cm3 for x 0. Determine the hole diffusion current density at (a) x 0 and (b) x Lp if the material is (i) silicon with Dp 10 cm2/s and Lp 50 m, and (ii) germanium with Dp 48 cm2/s and Lp 22.5 m. The electron concentration in silicon at T 300 K is given by x cm3 n(x) 1016 exp _ 18 where x is measured in m and is limited to 0 x 25 m. The electron diffusion coefficient is Dn 25 cm2/s and the electron mobility is n 960 cm2/V-s. The total electron current density through the semiconductor is constant and equal to n (cm3) 5 1014 n(0) 0 x (cm) 0.010 Figure P5.29 | Figure for Problem 5.29. nea29583_ch05_156-191.indd 188 12/11/10 10:15 AM Problems 189 Jn 40 A/cm2. The electron current has both diffusion and drift current components. Determine the electric field as a function of x which must exist in the semiconductor. 5.36 The total current in a semiconductor is constant and equal to J 10 A/cm2. The total current is composed of a hole drift current and electron diffusion current. Assume that the hole concentration is a constant and equal to 1016 cm3 and assume that the electron concentration is given by n(x) 2 1015exL cm3 where L 15 m. The electron diffusion coefficient is Dn 27 cm2/s and the hole mobility is p 420 cm2/V-s. Calculate (a) the electron diffusion current density for x 0, (b) the hole drift current density for x 0, and (c) the required electric field for x 0. *5.37 A constant electric field, E 12 V/cm, exists in the x direction of an n-type gallium arsenide semiconductor for 0 x 50 m. The total current density is a constant and is J 100 A/cm2. At x 0, the drift and diffusion currents are equal. Let T 300 K and n 8000 cm2/V-s. (a) Determine the expression for the electron concentration n(x). (b) Calculate the electron concentration at x 0 and at x 50 m. (c) Calculate the drift and diffusion current densities at x 50 m. *5.38 In n-type silicon, the Fermi energy level varies linearly with distance over a short range. At x 0, EF EFi 0.4 eV and, at x 103 cm, EFEFi 0.15 eV. (a) Write the expression for the electron concentration over the distance. (b) If the electron diffusion coefficient is Dn 25 cm2/s, calculate the electron diffusion current density at (i) x 0 and (ii) x 5 104 cm. *5.39 (a) The electron concentration in a semiconductor is given by n 1016(1 xL) cm3 for 0 x L, where L 10 m. The electron mobility and diffusion coefficient are n 1000 cm2/V-s and Dn 25.9 cm2/s. An electric field is applied such that the total electron current density is a constant over the given range of x and is Jn 80 A/cm2. Determine the required electric field versus distance function. (b) Repeat part (a) if Jn 20 A/cm2. Section 5.3 5.40 5.41 5.42 *5.43 5.44 Graded Impurity Distribution Consider an n-type semiconductor at T 300 K in thermal equilibrium (no current). Assume that the donor concentration varies as Nd(x) Nd0exL over the range 0 x L where Nd0 1016 cm3 and L 10 m. (a) Determine the electric field as a function of x for 0 x L. (b) Calculate the potential difference between x 0 and x L (with the potential at x 0 being positive with respect to that at x L). Using the data in Example 5.6, calculate the potential difference between x 0 and x 1 m. Determine the doping profile in a semiconductor at T 300 K that will induce a constant electric field of 500 V/cm over a length of 0.1 cm. In GaAs, the donor impurity concentration varies as Nd0 exp (xL) for 0 x L, where L 0. 1 m and Nd0 5 1016 cm3. Assume n 6000 cm2/V-s and T 300 K. (a) Derive the expression for the electron diffusion current density versus distance over the given range of x. (b) Determine the induced electric field that generates a drift current density that compensates the diffusion current density. (a) Consider the electron mobility in silicon for Nd 1017cm3 from Figure 5.2a. Calculate and plot the electron diffusion coefficient versus temperature over the range 50 T 200°C. (b) Repeat part (a) if the electron diffusion coefficient is given by Dn (0.0259)n for all temperatures. What conclusion can be made about the temperature dependence of the diffusion coefficient? *Asterisks next to problems indicate problems that are more difficult. nea29583_ch05_156-191.indd 189 12/11/10 10:15 AM 190 CHAPTER 5 5.45 Carrier Transport Phenomena Consider a semiconductor at T 300 K. (a) (i) Determine the electron diffusion coefficient if the electron mobility is n 1150 cm2/V-s. (ii) Repeat (i) of part (a) if the electron mobility is n 6200 cm2/V-s. (b) (i) Determine the hole mobility if the hole diffusion coefficient is Dp 8 cm2/s. (ii) Repeat (i) of part (b) if the hole diffusion coefficient is Dp 35 cm2/s. Section 5.4 The Hall Effect (Note: Refer to Figure 5.13 for the geometry of the Hall effect.) 5.46 Silicon, at T 300 K, is uniformly doped with phosphorus atoms at a concentration of 2 1016 cm3. A Hall device has the same geometrical dimensions as given in Example 5.8. The current is Ix 1.2 mA and the magnetic field is BZ 500 gauss 5 102 tesla. Determine (a) the Hall voltage and (b) the Hall field. 5.47 Germanium is doped with 5 1015 donor atoms per cm3 at T 300 K. The dimensions of the Hall device are d 5 103 cm, W 2 102 cm, and L 101 cm. The current is Ix 250 A, the applied voltage is Vx 100 mV, and the magnetic flux density is Bz 500 gauss 5 102 tesla. Calculate: (a) the Hall voltage, (b) the Hall field, and (c) the carrier mobility. 5.48 A semiconductor Hall device at T 300 K has the following geometry: d 103 cm, W 102 cm, and L 101 cm. The following parameters are measured: IX 0.50 mA, VX 15 V, VH 5.2 mV, and BZ 0.10 tesla. Determine the (a) conductivity type, (b) majority carrier concentration, and (c) majority carrier mobility. 5.49 Consider silicon at T 300 K. A Hall effect device is fabricated with the following geometry: d 5 103 cm, W 5 102 cm, and L 0.50 cm. The electrical parameters measured are: Ix 0.50 mA, Vx 1.25 V, and Bz 650 gauss 6.5 102 tesla. The Hall field is EH 16.5 mV/cm. Determine (a) the Hall voltage, (b) the conductivity type, (c) the majority carrier concentration, and (d) the majority carrier mobility. 5.50 Consider a gallium arsenide sample at T 300 K. A Hall effect device has been fabricated with the following geometry: d 0.0 1 cm, W 0.05 cm, and L 0.5 cm. The electrical parameters are: Ix 2.5 mA, Vx 2.2 V, and Bz 2.5 102 tesla. The Hall voltage is VH 4.5 mV. Find: (a) the conductivity type, (b) the majority carrier concentration, (c) the mobility, and (d) the resistivity. Summary and Review 5.51 An n-type silicon semiconductor resistor is to be designed so that it carries a current of 5 mA with an applied voltage of 5 V. (a) If Nd 3 1014 cm3 and Na 0, design a resistor to meet the required specifications. (b) If Nd 3 1016 cm3 and Na 2.5 1016 cm3, redesign the resistor. (c) Discuss the relative lengths of the two designs compared to the doping concentration. Is there a linear relationship? 5.52 In fabricating a Hall effect device, the two points at which the Hall voltage is measured may not be lined up exactly perpendicular to the current Ix (see Figure 5.13). Discuss the effect this misalignment will have on the Hall voltage. Show that a valid Hall voltage can be obtained from two measurements: first with the magnetic field in the z direction, and then in the z direction. 5.53 Another technique for determining the conductivity type of a semiconductor is called the hot probe method. It consists of two probes and an ammeter that indicates the nea29583_ch05_156-191.indd 190 12/11/10 10:15 AM Reading List 191 direction of current. One probe is heated and the other is at room temperature. No voltage is applied, but a current will exist when the probes touch the semiconductor. Explain the operation of this hot probe technique and sketch a diagram indicating the direction of current for p- and n-type semiconductor samples. READING LIST *1. Bube, R. H. Electrons in Solids: An Introductory Survey, 3rd ed. San Diego, CA: Academic Press, 1992. 2. Caughey, D. M., and R. E. Thomas. “Carrier Mobilities in Silicon Empirically, Related to Doping and Field.” Proc. IEEE 55 (1967), p. 2192. 3. Dimitrijev, S. Principles of Semiconductor Devices. New York: Oxford University, 2006. 4. Kano, K. Semiconductor Devices. Upper Saddle River, NJ: Prentice Hall, 1998. *5. Lundstrom, M. Fundamentals of Carrier Transport. Vol. X of Modular Series on Solid State Devices. Reading, MA: Addison-Wesley, 1990. 6. Muller, R. S., and T. I. Kamins. Device Electronics for Integrated Circuits, 2nd ed. New York: Wiley, 1986. 7. Navon, D. H. Semiconductor Microdevices and Materials. New York: Holt, Rinehart & Winston, 1986. 8. Pierret, R. F. Semiconductor Device Fundamentals. Reading, MA: Addison-Wesley, 1996. 9. Shur, M. Introduction to Electronic Devices. New York: John Wiley and Sons, 1996. *10. Shur, M. Physics of Semiconductor Devices. Englewood Cliffs, NJ: Prentice Hall, 1990. 11. Singh, J. Semiconductor Devices: An Introduction. New York: McGraw-Hill, 1994. 12. Singh, J. Semiconductor Devices: Basic Principles. New York: John Wiley and Sons, 2001. 13. Streetman, B. G., and S. K. Banerjee. Solid State Electronic Devices, 6th ed. Upper Saddle River, NJ: Pearson Prentice Hall, 2006. 14. Sze, S. M. and K. K. Ng. Physics of Semiconductor Devices, 3rd ed. Hoboken, NJ: John Wiley and Sons, 2007. 15. Sze, S. M. Semiconductor Devices: Physics and Technology, 2nd ed. New York: John Wiley and Sons, 2001. *16. van der Ziel, A. Solid State Physical Electronics, 2nd ed. Englewood Cliffs, NJ: Prentice Hall, 1968. 17. Wang, S. Fundamentals of Semiconductor Theory and Device Physics. Englewood Cliffs, NJ: Prentice Hall, 1989. 18. Yang, E. S. Microelectronic Devices. New York: McGraw-Hill, 1988. *Indicates references that are at an advanced level compared to this text. nea29583_ch05_156-191.indd 191 12/11/10 10:15 AM C 6 H A P T E R Nonequilibrium Excess Carriers in Semiconductors O ur discussion of the physics of semiconductors in Chapter 4 was based on thermal equilibrium. When a voltage is applied or a current exists in a semiconductor device, the semiconductor is operating under nonequilibrium conditions. In our discussion of current transport in Chapter 5, we did not address nonequilibrium conditions but implicitly assumed that equilibrium was not significantly disturbed. Excess electrons in the conduction band and excess holes in the valence band may exist in addition to the thermal-equilibrium concentrations if an external excitation is applied to the semiconductor. In this chapter, we discuss the behavior of nonequilibrium electron and hole concentrations as functions of time and space coordinates. Excess electrons and excess holes do not move independently of each other. These excess carriers diffuse, drift, and recombine with the same effective diffusion coefficient, drift mobility, and lifetime. This phenomenon is called ambipolar transport. We develop the ambipolar transport equation that describes the behavior of excess electrons and holes. Excess carriers dominate the electrical properties of a semiconductor material, and the behavior of excess carriers is fundamental to the operation of semiconductor devices. ■ 6.0 | PREVIEW In this chapter, we will: ■ Describe the process of generation and recombination of excess carriers in a semiconductor. ■ Define the recombination rate and generation rate of excess carriers, and define the excess carrier lifetime. ■ Discuss why excess electrons and excess holes do not move independently of each other. The movement of excess carriers is called ambipolar transport, and the ambipolar transport equation is derived. 192 nea29583_ch06_192-240.indd 192 12/11/10 11:17 AM 6.1 ■ ■ ■ ■ Carrier Generation and Recombination 193 Apply the ambipolar transport equation to various situations to determine the time behavior and spatial behavior of excess carriers. Define the quasi-Fermi energy level. Analyze the effect of defects in a semiconductor on the excess carrier lifetime. Analyze the effect of defects at a semiconductor surface on the excess carrier concentration. 6.1 | CARRIER GENERATION AND RECOMBINATION In this chapter, we discuss carrier generation and recombination, which we can define as follows: generation is the process whereby electrons and holes are created, and recombination is the process whereby electrons and holes are annihilated. Any deviation from thermal equilibrium will tend to change the electron and hole concentrations in a semiconductor. A sudden increase in temperature, for example, will increase the rate at which electrons and holes are thermally generated so that their concentrations will change with time until new equilibrium values are reached. An external excitation, such as light (a flux of photons), can also generate electrons and holes, creating a nonequilibrium condition. To understand the generation and recombination processes, we first consider direct band-to-band generation and recombination, and then, later, the effect of allowed electronic energy states within the bandgap, referred to as traps or recombination centers. 6.1.1 The Semiconductor in Equilibrium We have determined the thermal-equilibrium concentration of electrons and holes in the conduction and valence bands, respectively. In thermal equilibrium, these concentrations are independent of time. However, electrons are continually being thermally excited from the valence band into the conduction band by the random nature of the thermal process. At the same time, electrons moving randomly through the crystal in the conduction band may come in close proximity to holes and “fall” into the empty states in the valence band. This recombination process annihilates both the electron and hole. Since the net carrier concentrations are independent of time in thermal equilibrium, the rate at which electrons and holes are generated and the rate at which they recombine must be equal. The generation and recombination processes are schematically shown in Figure 6.1. Ec Electron–hole generation Electron–hole recombination Ev Figure 6.1 Electron–hole generation and recombination. nea29583_ch06_192-240.indd 193 12/11/10 11:17 AM 194 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors Let G n0 and G p0 be the thermal-generation rates of electrons and holes, respectively, given in units of #/cm3-s. For the direct band-to-band generation, the electrons and holes are created in pairs, so we must have that Gn0 Gp0 (6.1) Let Rn0 and Rp0 be the recombination rates of electrons and holes, respectively, for a semiconductor in thermal equilibrium, again given in units of #/cm3-s. In direct band-to-band recombination, electrons and holes recombine in pairs, so that Rn0 Rp0 (6.2) In thermal equilibrium, the concentrations of electrons and holes are independent of time; therefore, the generation and recombination rates are equal, so we have Gn0 Gp0 Rn0 Rp0 6.1.2 (6.3) Excess Carrier Generation and Recombination Additional notation is introduced in this chapter. Table 6.1 lists some of the more pertinent symbols used throughout the chapter. Other symbols will be defined as we advance through the chapter. Electrons in the valence band may be excited into the conduction band when, for example, high-energy photons are incident on a semiconductor. When this happens, not only is an electron created in the conduction band, but a hole is created in the valence band; thus, an electron–hole pair is generated. The additional electrons and holes created are called excess electrons and excess holes. The excess electrons and holes are generated by an external force at a particular rate. Let gn be the generation rate of excess electrons and gp be that of excess holes. These generation rates also have units of #/cm3-s. For the direct band-toband generation, the excess electrons and holes are also created in pairs, so we must have gn gp (6.4) Table 6.1 Relevant notation used in Chapter 6 Symbol n0, p0 n, p n n n0 p p p0 gn , gp Rn , Rp n0, p0 nea29583_ch06_192-240.indd 194 Definition Thermal-equilibrium electron and hole concentrations (independent of time and also usually position) Total electron and hole concentrations (may be functions of time and/or position) Excess electron and hole concentrations (may be functions of time and/or position) Excess electron and hole generation rates Excess electron and hole recombination rates Excess minority carrier electron and hole lifetimes 12/11/10 11:17 AM 6.1 Carrier Generation and Recombination 195 When excess electrons and holes are created, the concentration of electrons in the conduction band and of holes in the valence band increase above their thermalequilibrium value. We may write n n0 n (6.5a) p p0 p (6.5b) and where n0 and p0 are the thermal-equilibrium concentrations, and n and p are the excess electron and hole concentrations. Figure 6.2 shows the excess electron–hole generation process and the resulting carrier concentrations. The external force has perturbed the equilibrium condition so that the semiconductor is no longer in thermal equilibrium. We may note from Equations (6.5a) and (6.5b) that, in a nonequilibrium condition, np ⬆ n0p0 n2i . A steady-state generation of excess electrons and holes will not cause a continual buildup of the carrier concentrations. As in the case of thermal equilibrium, an electron in the conduction band may “fall down” into the valence band, leading to the process of excess electron–hole recombination. Figure 6.3 shows this process. The n0 ␦n E c h Ev P0 ␦p Figure 6.2 Creation of excess electron and hole densities by photons. n0 Ec Ev p0 Figure 6.3 Recombination of excess carriers reestablishing thermal equilibrium. nea29583_ch06_192-240.indd 195 12/11/10 11:17 AM 196 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors recombination rate for excess electrons is denoted by Rn and for excess holes by Rp. Both parameters have units of #/cm3-s. The excess electrons and holes recombine in pairs, so the recombination rates must be equal. We can then write Rn Rp (6.6) In the direct band-to-band recombination that we are considering, the recombination occurs spontaneously; thus, the probability of an electron and hole recombining is constant with time. The rate at which electrons recombine must be proportional to the electron concentration and must also be proportional to the hole concentration. If there are no electrons or holes, there can be no recombination. The net rate of change in the electron concentration can be written as dn(t) _ r n2i n(t)p(t) (6.7) n(t) n0 n(t) (6.8a) p(t) p0 p(t) (6.8b) dt where and The first term, n , in Equation (6.7) is the thermal-equilibrium generation rate. Since excess electrons and holes are created and recombine in pairs, we have that n(t) p(t). (Excess electron and hole concentrations are equal so we can simply use the phrase excess carriers to mean either.) The thermal-equilibrium parameters, n0 and p0, are independent of time; therefore, Equation (6.7) becomes 2 r i d(n(t)) __ r n2i (n0 n(t))(p0 p(t)) dt r n(t)[(n0 p0) n(t)] (6.9) Equation (6.9) can easily be solved if we impose the condition of low-level injection. Low-level injection puts limits on the magnitude of the excess carrier concentration compared with the thermal-equilibrium carrier concentrations. In an extrinsic n-type material, we generally have n0 p0 and, in an extrinsic p-type material, we generally have p0 n0. Low-level injection means that the excess carrier concentration is much less than the thermal-equilibrium majority carrier concentration. Conversely, high-level injection occurs when the excess carrier concentration becomes comparable to or greater than the thermal-equilibrium majority carrier concentrations. If we consider a p-type material (p0 n0) under low-level injection (n(t) p0), then Equation (6.9) becomes d(n(t)) __ r p0n(t) dt (6.10) The solution to the equation is an exponential decay from the initial excess concentration, or n(t) n(0)er p0t n(0)et/n0 nea29583_ch06_192-240.indd 196 (6.11) 12/11/10 11:17 AM 6.1 Carrier Generation and Recombination 197 where n0 (r p0)1 and is a constant for the low-level injection. Equation (6.11) describes the decay of excess minority carrier electrons so that n0 is often referred to as the excess minority carrier lifetime.1 The recombination rate—which is defined as a positive quantity—of excess minority carrier electrons can be written, using Equation (6.10), as d(n(t)) n(t) Rn __ r p0n(t) _ n0 dt (6.12) For the direct band-to-band recombination, the excess majority carrier holes recombine at the same rate, so that for the p-type material n(t) Rn Rp _ n0 (6.13) In the case of an n-type material (n0 p0) under low-level injection (n(t) n0), the decay of minority carrier holes occurs with a time constant p0 (r n0)1, where p0 is also referred to as the excess minority carrier lifetime. The recombination rate of the majority carrier electrons will be the same as that of the minority carrier holes, so we have n(t) Rn Rp _ p0 (6.14) The generation rates of excess carriers are not functions of electron or hole concentrations. In general, the generation and recombination rates may be functions of the space coordinates and time. Objective: Determine the behavior of excess carriers as a function of time. EXAMPLE 6.1 Assume that excess carriers have been generated uniformly in a semiconductor to a concentration of n(0) 1015 cm3. The forcing function generating the excess carriers turns off at time t 0. Assuming the excess carrier lifetime is n0 106 s, determine n(t) for t 0. ■ Solution From Equation (6.11), we have 6 n(t) n(0)et/n0 1015 et/10 cm3 For example, at: t 0, n 1015 cm3 t 1s, n 1015 e1/1 3.68 1014 cm3 t 4s, n 1015 e4/1 1.83 1013 cm3 t 10s, n 1015 e10/1 4.54 1010 cm3 ■ Comment These results simply demonstrate the exponential decay of excess carriers with time after an excitation source is removed. In Chapter 5 we defined as a mean time between collisions. We define here as the mean time before a recombination event occurs. The two parameters are not related. 1 nea29583_ch06_192-240.indd 197 12/11/10 11:17 AM 198 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors ■ EXERCISE PROBLEM Ex 6.1 Using the parameters in Example 6.1, calculate the recombination rate of the excess carriers for (a) t 0, (b) t 1s, (c) t 4s, and (d) t 10s. [Ans. (a) 10 21 cm3s1; (b) 3.68 10 20 cm3s1; (c) 1.83 10 19 cm3s1; (d ) 4.54 10 16 cm3s1] 6.2 | CHARACTERISTICS OF EXCESS CARRIERS The generation and recombination rates of excess carriers are important parameters, but how the excess carriers behave with time and in space in the presence of electric fields and density gradients is of equal importance. As mentioned at the beginning of this chapter, the excess electrons and holes do not move independently of each other, but they diffuse and drift with the same effective diffusion coefficient and with the same effective mobility. This phenomenon is called ambipolar transport. The question that must be answered is what is the effective diffusion coefficient and what is the effective mobility that characterizes the behavior of these excess carriers? To answer these questions, we must develop the continuity equations for the carriers and then develop the ambipolar transport equations. The final results show that, for an extrinsic semiconductor under low injection (this concept will be defined in the analysis), the effective diffusion coefficient and mobility parameters are those of the minority carrier. This result is thoroughly developed in the following derivations. As will be seen in the following chapters, the behavior of the excess carriers has a profound impact on the characteristics of semiconductor devices. 6.2.1 Continuity Equations The continuity equations for electrons and holes are developed in this section. Figure 6.4 shows a differential volume element in which a one-dimensional holeparticle flux is entering the differential element at x and is leaving the element at x dx. The parameter Fpx is the hole-particle flux, or flow, and has units of number of holes/cm2-s. For the x component of the particle current density shown, we may write F px F px (x dx) F px (x) _ dx x dz F px(x) (6.15) F px(x dx) dy x x dx Figure 6.4 Differential volume showing x component of the hole-particle flux. nea29583_ch06_192-240.indd 198 12/11/10 11:17 AM 6.2 Characteristics of Excess Carriers 199 This equation is a Taylor expansion of F px (x dx), where the differential length dx is small, so that only the first two terms in the expansion are significant. The net increase in the number of holes per unit time within the differential volume element due to the x-component of hole flux is given by F px p _ dx dy dz [F px (6.16) (x) F px (x dx)] dy dz _ dx dy dz t x If F px (x) F px (x dx), for example, there will be a net increase in the number of holes in the differential volume element with time. If we generalize to a three-dimensional hole flux, then the right side of Equation (6.16) may be written as F p dx dy dz, where F p is the divergence of the flux vector. We will limit ourselves to a one-dimensional analysis. The generation rate and recombination rate of holes will also affect the hole concentration in the differential volume. The net increase in the number of holes per unit time in the differential volume element is then given by F p p p _ dx dy dz _ dx dy dz gp dx dy dz _ (6.17) pt dx dy dz t x where p is the density of holes. The first term on the right side of Equation (6.17) is the increase in the number of holes per unit time due to the hole flux, the second term is the increase in the number of holes per unit time due to the generation of holes, and the last term is the decrease in the number of holes per unit time due to the recombination of holes. The recombination rate for holes is given by p/ pt where pt includes the thermal-equilibrium carrier lifetime and the excess carrier lifetime. If we divide both sides of Equation (6.17) by the differential volume dx dy dz, the net increase in the hole concentration per unit time is F p p p _ _ gp _ (6.18) pt t x Equation (6.18) is known as the continuity equation for holes. Similarly, the one-dimensional continuity equation for electrons is given by Fn n __ n _ gn _ nt x t (6.19) where Fn is the electron-particle flow, or flux, also given in units of number of electrons/cm2-s. 6.2.2 Time-Dependent Diffusion Equations In Chapter 5, we derived the hole and electron current densities, which are given, in one dimension, by p Jp ep pE eDp _ (6.20) x and n (6.21) Jn en nE eDn _ x nea29583_ch06_192-240.indd 199 12/11/10 11:17 AM 200 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors If we divide the hole current density by (e) and the electron current density by (e), we obtain each particle flux. These equations become Jp p _ F p p pE Dp _ (6.22) Jn n _ F n n nE Dn _ (6.23) x (e) and x (e) Taking the divergence of Equations (6.22) and (6.23), and substituting back into the continuity equations of (6.18) and (6.19), we obtain 2 p ( pE) p p _ p _ Dp _2 gp _ (6.24) (nE) n _ ng _ n _ Dn _ n n 2 (6.25) t x x pt and 2 t x x nt Keeping in mind that we are limiting ourselves to a one-dimensional analysis, we can expand the derivative of the product as (pE) p E _ E_ p_ x x x (6.26) In a more generalized three-dimensional analysis, Equation (6.26) would have to be replaced by a vector identity. Equations (6.24) and (6.25) can be written in the form (6.27) (6.28) 2 p p p p E g _ Dp _2 p E _ p _ _ p pt x x t x and 2 n E_ n n_ E g _ n n _ Dn _ n n nt t x x x2 Equations (6.27) and (6.28) are the time-dependent diffusion equations for holes and electrons, respectively. Since both the hole concentration p and the electron concentration n contain the excess concentrations, Equations (6.27) and (6.28) describe the space and time behavior of the excess carriers. The hole and electron concentrations are functions of both the thermal equilibrium and the excess values, which are given in Equations (6.5a) and (6.5b). The thermalequilibrium concentrations, n0 and p0, are not functions of time. For the special case of a homogeneous semiconductor, n0 and p0 are also independent of the space coordinates. Equations (6.27) and (6.28) may then be written in the form (6.29) (6.30) 2 (p) (p) p (p) E g _ _ Dp __ p E _ p _ p pt t x x x2 and 2 (n) (n) (n) E g _ n _ Dn __ n E _ n _ n nt t x x x2 nea29583_ch06_192-240.indd 200 12/11/10 11:17 AM 6.3 Ambipolar Transport 201 Note that Equations (6.29) and (6.30) contain terms involving the total concentrations, p and n, and terms involving only the excess concentrations, p and n. 6.3 | AMBIPOLAR TRANSPORT Originally, we assumed that the electric field in the current Equations (6.20) and (6.21) was an applied electric field. This electric field term appears in the timedependent diffusion equations given by Equations (6.29) and (6.30). If a pulse of excess electrons and a pulse of excess holes are created at a particular point in a semiconductor with an applied electric field, the excess holes and electrons will tend to drift in opposite directions. However, because the electrons and holes are charged particles, any separation will induce an internal electric field between the two sets of particles. This internal electric field will create a force attracting the electrons and holes back toward each other. This effect is shown in Figure 6.5. The electric field term in Equations (6.29) and (6.30) is then composed of the externally applied field plus the induced internal field. This E-field may be written as E Eapp Eint (6.31) where Eapp is the applied electric field and Eint is the induced internal electric field. Since the internal E-field creates a force attracting the electrons and holes, this E-field will hold the pulses of excess electrons and excess holes together. The negatively charged electrons and positively charged holes then will drift or diffuse together with a single effective mobility or diffusion coefficient. This phenomenon is called ambipolar diffusion or ambipolar transport. 6.3.1 Derivation of the Ambipolar Transport Equation The time-dependent diffusion Equations (6.29) and (6.30) describe the behavior of the excess carriers. However, a third equation is required to relate the excess electron and hole concentrations to the internal electric field. This relation is Poisson’s equation, which may be written as e(p n) _ E Eint __ int s x (6.32) where s is the permittivity of the semiconductor material. Eapp ␦n Eint ␦p x Figure 6.5 The creation of an internal electric field as excess electrons and holes tend to separate. nea29583_ch06_192-240.indd 201 12/11/10 11:17 AM 202 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors To make the solution of Equations (6.29), (6.30), and (6.32) more tractable, we need to make some approximations. We can show that only a relatively small internal electric field is sufficient to keep the excess electrons and holes drifting and diffusing together. Hence, we can assume that EintEapp (6.33) However, the Eint term may not be negligible. We will impose the condition of charge neutrality: We will assume that the excess electron concentration is just balanced by an equal excess hole concentration at any point in space and time. If this assumption were exactly true, there would be no induced internal electric field to keep the two sets of particles together. However, only a very small difference in the excess electron concentration and excess hole concentration will set up an internal E-field sufficient to keep the particles diffusing and drifting together. We can show that a 1 percent difference in p and n, for example, will result in non-negligible values of the E Eint term in Equations (6.29) and (6.30). We can combine Equations (6.29) and (6.30) to eliminate the E term. Considering Equations (6.1) and (6.4), we can define gn gp g (6.34) and considering Equations (6.2) and (6.6), we can define p n _ Rn _ nt Rp pt R (6.35) The lifetimes in Equation (6.35) include the thermal-equilibrium carrier lifetimes and the excess carrier lifetimes. If we impose the charge neutrality condition, then n p. We will denote both the excess electron and excess hole concentrations in Equations (6.29) and (6.30) by n. We may then rewrite Equations (6.29) and (6.30) as (6.36) (6.37) 2 (n) (n) (n) E gR_ Dp __ p E _ p _ x x t x2 and 2 (n) (n) (n) E gR_ n E _ n _ Dn __ x x t x2 If we multiply Equation (6.36) by n n, multiply Equation (6.37) by p p, and add the two equations, the E E/ x term will be eliminated. The result of this addition gives 2 (n) (n) (n n Dp p pDn) __ (n p)( p n) E _ x x2 (n) (n n p p)(g R) (n n p p)_ (6.38) t If we divide Equation (6.38) by the term (nn p p), this equation becomes 2 (n) (n) (n) E _ g R _ D __ x t x2 nea29583_ch06_192-240.indd 202 (6.39) 12/11/10 11:17 AM 6.3 where Ambipolar Transport n nDp p pDn D ___ nn p p (6.40) n p (p n) ___ nn p p (6.41) 203 and Equation (6.39) is called the ambipolar transport equation and describes the behavior of the excess electrons and holes in time and space. The parameter D is called the ambipolar diffusion coefficient and is called the ambipolar mobility. The Einstein relation relates the mobility and diffusion coefficient by p n e _ _ _ Dn Dp kT (6.42) Using these relations, the ambipolar diffusion coefficient may be written in the form Dn Dp (n p) D ___ Dnn Dpp (6.43) The ambipolar diffusion coefficient, D, and the ambipolar mobility, , are functions of the electron and hole concentrations, n and p, respectively. Since both n and p contain the excess carrier concentration n, the coefficient in the ambipolar transport equation are not constants. The ambipolar transport equation, given by Equation (6.39), then, is a nonlinear differential equation. 6.3.2 Limits of Extrinsic Doping and Low Injection The ambipolar transport equation may be simplified and linearized by considering an extrinsic semiconductor and by considering low-level injection. The ambipolar diffusion coefficient, from Equation (6.43), may be written as DnDp[(n0 n) (p0 n)] D _____ Dn (n0 n) Dp (p0 n) (6.44) where n0 and p0 are the thermal-equilibrium electron and hole concentrations, respectively, and n is the excess carrier concentration. If we consider a p-type semiconductor, we can assume that p0 n0. The condition of low-level injection, or just low injection, means that the excess carrier concentration is much smaller than the thermal-equilibrium majority carrier concentration. For the p-type semiconductor, then, low injection implies that n p0. Assuming that n0 p0 and n p0, and assuming that Dn and Dp are on the same order of magnitude, the ambipolar diffusion coefficient from Equation (6.44) reduces to D Dn nea29583_ch06_192-240.indd 203 (6.45) 12/11/10 11:17 AM 204 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors If we apply the conditions of an extrinsic p-type semiconductor and low injection to the ambipolar mobility, Equation (6.41) reduces to n (6.46) It is important to note that for an extrinsic p-type semiconductor under low injection, the ambipolar diffusion coefficient and the ambipolar mobility coefficient reduce to the minority carrier electron parameter values, which are constants. The ambipolar transport equation reduces to a linear differential equation with constant coefficients. If we now consider an extrinsic n-type semiconductor under low injection, we may assume that p0 n0 and n n0. The ambipolar diffusion coefficient from Equation (6.43) reduces to D Dp (6.47) and the ambipolar mobility from Equation (6.41) reduces to p (6.48) The ambipolar parameters again reduce to the minority-carrier values, which are constants. Note that, for the n-type semiconductor, the ambipolar mobility is a negative value. The ambipolar mobility term is associated with carrier drift; therefore, the sign of the drift term depends on the charge of the particle. The equivalent ambipolar particle is negatively charged, as one can see by comparing Equations (6.30) and (6.39). If the ambipolar mobility reduces to that of a positively charged hole, a negative sign is introduced as shown in Equation (6.48). The remaining terms we need to consider in the ambipolar transport equation are the generation rate and the recombination rate. Recall that the electron and hole recombination rates are equal and are given by Equation (6.35) as Rn Rp nnt ppt R, where nt and pt are the mean electron and hole lifetimes, respectively. If we consider the inverse lifetime functions, then 1/nt is the probability per unit time that an electron will encounter a hole and recombine. Likewise, 1/pt is the probability per unit time that a hole will encounter an electron and recombine. If we again consider an extrinsic p-type semiconductor under low injection, the concentration of majority carrier holes will be essentially constant, even when excess carriers are present. Then, the probability per unit time of a minority carrier electron encountering a majority carrier hole will be essentially constant. Hence, the minority carrier electron lifetime, nt n, will remain a constant for the extrinsic p-type semiconductor under low injection. Similarly, if we consider an extrinsic n-type semiconductor under low injection, the minority carrier hole lifetime, pt p, will remain constant. Even under the condition of low injection, the minority carrier hole concentration may increase by several orders of magnitude. The probability per unit time of a majority carrier electron encountering a hole may change drastically. The majority carrier lifetime, then, may change substantially when excess carriers are present. Consider, again, the generation and recombination terms in the ambipolar transport equation. For electrons we may write g R gn Rn (Gn0 gn) (Rn0 Rn) nea29583_ch06_192-240.indd 204 (6.49) 12/11/10 11:17 AM 6.3 Ambipolar Transport 205 where Gn0 and gn are the thermal-equilibrium electron and excess electron generation rates, respectively. The terms Rn0 and Rn are the thermal-equilibrium electron and excess electron recombination rates, respectively. For thermal equilibrium, we have that (6.50) Gn0 Rn0 so Equation (6.49) reduces to n g R gn Rn gn _ n (6.51) where n is the excess minority carrier electron lifetime. For the case of holes, we may write g R gp Rp (Gp0 gp) (Rp0 Rp) (6.52) where Gp0 and gp are the thermal-equilibrium hole and excess hole generation rates, respectively. The terms Rp0 and Rp are the thermal-equilibrium hole and excess hole recombination rates, respectively. Again, for thermal equilibrium, we have that Gp0 Rp0 (6.53) p g R gp Rp gp _ p (6.54) so that Equation (6.52) reduces to where p is the excess minority carrier hole lifetime. The generation rate for excess electrons must equal the generation rate for excess holes. We may then define a generation rate for excess carriers as g, so that gn gp g. We also determined that the minority carrier lifetime is essentially a constant for low injection. Then, the term g R in the ambipolar transport equation may be written in terms of the minority carrier parameters. The ambipolar transport equation, given by Equation (6.39), for a p-type semiconductor under low injection then becomes 2 (n) (n) (n) n _ Dn __ nE _ g _ 2 n0 x t x (6.55) The parameter n is the excess minority carrier electron concentration, the parameter n0 is the minority carrier lifetime under low injection, and the other parameters are the usual minority carrier electron parameters. Similarly, for an extrinsic n-type semiconductor under low injection, the ambipolar transport equation becomes 2 (p) (p) p _ (p) Dp __ p E _ g _ p0 t x x2 (6.56) The parameter p is the excess minority carrier hole concentration, the parameter p0 is the minority carrier hole lifetime under low injection, and the other parameters are the usual minority carrier hole parameters. nea29583_ch06_192-240.indd 205 12/11/10 11:17 AM 206 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors It is extremely important to note that the transport and recombination parameters in Equations (6.55) and (6.56) are those of the minority carrier. Equations (6.55) and (6.56) describe the drift, diffusion, and recombination of excess minority carriers as a function of spatial coordinates and as a function of time. Recall that we had imposed the condition of charge neutrality; the excess minority carrier concentration is equal to the excess majority carrier concentration. The excess majority carriers, then, diffuse and drift with the excess minority carriers; thus, the behavior of the excess majority carrier is determined by the minority carrier parameters. This ambipolar phenomenon is extremely important in semiconductor physics, and is the basis for describing the characteristics and behavior of semiconductor devices. 6.3.3 Applications of the Ambipolar Transport Equation We solve the ambipolar transport equation for several problems. These examples help illustrate the behavior of excess carriers in a semiconductor material, and the results are used later in the discussion of the pn junction and the other semiconductor devices. The following examples use several common simplifications in the solution of the ambipolar transport equation. Table 6.2 summarizes these simplifications and their effects. EXAMPLE 6.2 Objective: Determine the time behavior of excess carriers as a semiconductor returns to thermal equilibrium. Consider an infinitely large, homogeneous n-type semiconductor with zero applied electric field. Assume that at time t ⫽ 0, a uniform concentration of excess carriers exists in the crystal, but assume that g⬘ ⫽ 0 for t ⬎ 0. If we assume that the concentration of excess carriers is much smaller than the thermal-equilibrium electron concentration, then the lowinjection condition applies. Calculate the excess carrier concentration as a function of time for t ⱖ 0. Table 6.2 | Common ambipolar transport equation simplifications Specification Steady state Uniform distribution of excess carriers (uniform generation rate) Zero electric field No excess carrier generation No excess carrier recombination (infinite lifetime) nea29583_ch06_192-240.indd 206 Effect ⭸(␦n) _ ⫽ 0, ⭸t ⭸2 (␦n) Dn __ ⫽ 0, ⭸x2 ⭸(␦n) E_ ⫽ 0, ⭸x ⭸(␦p) _ ⫽0 ⭸t ⭸2 (␦n) Dp__ ⫽0 ⭸x2 ⭸(␦p) E_ ⫽ 0 ⭸x g⬘ ⫽ 0 ␦p ␦n _ ⫽ 0, _ ⫽ 0 n0 p0 12/13/10 10:48 PM 6.3 Ambipolar Transport 207 ■ Solution For the n-type semiconductor, we need to consider the ambipolar transport equation for the minority carrier holes, which is given by Equation (6.56). The equation is 2 (p) (p) (p) p _ Dp __ p E _ g _ p0 t x x2 We are assuming a uniform concentration of excess holes so that 2 (p) x2 (p) x 0. For t 0, we are also assuming that g 0. Equation (6.56) reduces to d(p) p _ _ dt (6.57) p0 Since there is no spatial variation, the total time derivative may be used. At low injection, the minority carrier hole lifetime, p0, is a constant. The left-side of Equation (6.57) is the time rate of change of p and the right-side of the equation is the recombination rate. The solution to Equation (6.57) is p(t) p(0)et (6.58) p0 where p(0) is the uniform concentration of excess carriers that exists at time t 0. The concentration of excess holes decays exponentially with time, with a time constant equal to the minority carrier hole lifetime. From the charge-neutrality condition, we have that n p, so the excess electron concentration is given by n(t) p(t) p(0)et p0 (6.59) ■ Comment The excess electrons and holes recombine at the rate determined by the excess minority carrier hole lifetime in the n-type semiconductor. ■ EXERCISE PROBLEM Ex 6.2 Consider n-type GaAs doped at Nd 1016 cm3. Assume that 1014 electron–hole pairs have been uniformly created per cm3 at t 0, and assume the minority carrier hole lifetime is p0 50 ns. Determine the time at which the minority carrier hole concentration reaches (a) 1/e of its initial value and (b) 10% of its initial value. [Ans. (a) t 50 ns; (b) t 115 ns] Objective: Determine the time dependence of excess carriers in reaching a steady-state condition. Again consider an infinitely large, homogeneous n-type semiconductor with a zero applied electric field. Assume that, for t 0, the semiconductor is in thermal equilibrium and that, for t 0, a uniform generation rate exists in the crystal. Calculate the excess carrier concentration as a function of time assuming the condition of low injection. nea29583_ch06_192-240.indd 207 EXAMPLE 6.3 12/11/10 11:17 AM 208 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors ■ Solution The condition of a uniform generation rate and a homogeneous semiconductor again implies that 2 (p) x2 (p) x 0 in Equation (6.56). The equation, for this case, reduces to p _ d(p) g _ p0 dt (6.60) The solution to this differential equation is p(t) gp0(1 et/p0) (6.61) ■ Comment We may note that, as t → , a steady-state excess hole and electron concentration of gp 0 is reached. Equation (6.60) contains both a generation rate term and a recombination rate term for the excess carriers. ■ EXERCISE PROBLEM Ex 6.3 In Example 6.3, consider n-type silicon at T 300 K doped to Nd 5 1016 cm3. Assume that g 5 1021 cm3 s1 and let p0 107 s. (a) Determine p(t) at (i) t 0, (ii) t 107 s, (iii) t 5 107 s, and (iv) t → . (b) Considering the results of part (a), is the low-injection condition maintained? [Ans. (a) (i) 0; (ii) 3.16 1014 cm3; (iii) 4.966 1014 cm3; (iv) 5 1014 cm3; (b) p(max) 0.01Nd, yes] The excess minority carrier hole concentration increases with time with the same time constant p0, which is the excess minority carrier lifetime. The excess carrier concentration reaches a steady-state value as time goes to infinity, even though a steady-state generation of excess electrons and holes exists. This steady-state effect can be seen from Equation (6.60) by setting d(p)/dt 0. The remaining terms simply state that, in steady state, the generation rate is equal to the recombination rate. TEST YOUR UNDERSTANDING TYU 6.1 Silicon at T300 K has been doped with boron atoms to a concentration of Na 5 1016 cm3. Excess carriers have been generated in the uniformly doped material to a concentration of 1015 cm3. The minority carrier lifetime is 5 s. (a) What carrier type is the minority carrier? (b) Assuming g E 0 for t 0, determine the minority carrier concentration for t 0. TYU 6.2 Consider silicon with the same parameters as given in TYU 6.1. The material is in thermal equilibrium for t 0. At t 0, a source generating excess carriers is turned on, producing a generation rate of g 1020 cm3-s1. (a) What carrier type is the minority carrier? (b) Determine the minority carrier concentration for t 0. (c) What is the minority carrier concentration as t → ? [Ans. (a) electrons; (b) 1015 et510 6 cm3] [Ans. (a) electrons; (b) 5 1014 [1 et510 ] cm3 (c) 5 1014 cm3] 6 nea29583_ch06_192-240.indd 208 12/11/10 11:17 AM 6.3 Ambipolar Transport 209 Objective: Determine the steady-state spatial dependence of the excess carrier concentration. EXAMPLE 6.4 Consider a p-type semiconductor that is homogeneous and infinite in extent. Assume a zero applied electric field. For a one-dimensional crystal, assume that excess carriers are being generated at x 0 only, as indicated in Figure 6.6. The excess carriers being generated at x 0 will begin diffusing in both the x and x directions. Calculate the steady-state excess carrier concentration as a function of x. ■ Solution The ambipolar transport equation for excess minority carrier electrons is given by Equation (6.55), and is written as 2 (n) (n) (n) n _ Dn __ n E _ g _ n0 t x x2 From our assumptions, we have E 0, g 0 for x ⬆ 0, and (n) t 0 for steady state. Assuming a one-dimensional crystal, Equation (6.55) reduces to d2(n) _ Dn __ n 0 n0 dx2 (6.62) Dividing by the diffusion coefficient, Equation (6.62) may be written as d (n) __ d (n) n __ n __ _ 0 2 2 dx2 Dn n0 dx2 L2n (6.63) where we have defined L2n Dnn0. The parameter Ln has the unit of length and is called the minority carrier electron diffusion length. The general solution to Equation (6.63) is n(x) AexLn BexLn (6.64) As the minority carrier electrons diffuse away from x 0, they will recombine with the majority carrier holes. The minority carrier electron concentration will then decay toward zero at both x and x . These boundary conditions mean that B 0 for x 0 and A 0 for x 0. The solution to Equation (6.63) may then be written as n(x) n(0)exLn x 0 (6.65a) g x0 x Figure 6.6 | Steady-state generation rate at x 0. nea29583_ch06_192-240.indd 209 12/11/10 11:17 AM 210 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors and n(x) n(0)exLn x 0 (6.65b) where n(0) is the value of the excess electron concentration at x 0. The steady-state excess electron concentration decays exponentially with distance away from the source at x 0. ■ Comment We may note that the steady-state excess concentration decays to 1/e of its value at x Ln. ■ EXERCISE PROBLEM Ex 6.4 In Example 6.4, consider p-type silicon at T 300 K doped to Na 5 1016 cm3. Assume that n0 5 107 s, Dn 25 cm2 /s, and n(0) 1015 cm3. (a) Calculate the value of diffusion length Ln. (b) Determine n at (i) x 0, (ii) x 30 m, (iii) x 50 m, (iv) x 85 m, and (v) x 120 m. [Ans. (a) Ln 35.36 m; (b) (i) 1015 cm3; (ii) 4.28 1014 cm3, (iii) 2.43 1014 cm3, (iv) 9.04 1013 cm3, (v) 3.36 1013 cm3] As before, we will assume charge neutrality; thus, the steady-state excess majority carrier hole concentration also decays exponentially with distance with the same characteristic minority carrier electron diffusion length Ln. Figure 6.7 is a plot of the total electron and hole concentrations as a function of distance. We are assuming low injection, that is, n(0) p0 in the p-type semiconductor. The total concentration of Carrier concentration (log scale) p0 ␦n(0) p0 n0 ␦n(0) n0 x0 x Figure 6.7 | Steady-state electron and hole concentrations for the case when excess electrons and holes are generated at x 0. nea29583_ch06_192-240.indd 210 12/11/10 11:17 AM 6.3 Ambipolar Transport 211 majority carrier holes barely changes. However, we may have n(0) n0 and still satisfy the low-injection condition. The minority carrier concentration may change by many orders of magnitude. TEST YOUR UNDERSTANDING TYU 6.3 Excess electrons and holes are generated at the end of a silicon bar (x 0). The silicon is doped with phosphorus atoms to a concentration of Nd 1017 cm3. The minority carrier lifetime is 1 s, the electron diffusion coefficient is Dn 25 cm2/s, and the hole diffusion coefficient is Dp 10 cm2/s. If n(0) p(0) 1015 cm3, determine the steady-state electron and hole concentrations in the silicon for x 0. TYU 6.4 Using the parameters given in TYU 6.3, calculate the electron and hole diffusion current densities at x 10 m. [Ans. n(x) p(x) 1015ex3.1610 cm3, where x is in cm] 3 [Ans. Jp 0.369 A/cm2, Jn 0.369 A/cm2] The three previous examples, which applied the ambipolar transport equation to specific situations, assumed either a homogeneous or a steady-state condition; only the time variation or the spatial variation was considered. Now consider an example in which both the time and spatial dependence are considered in the same problem. Objective: Determine both the time dependence and spatial dependence of the excess carrier concentration. Assume that a finite number of electron–hole pairs is generated instantaneously at time t 0 and at x 0, but assume g 0 for t 0. Assume we have an n-type semiconductor with a constant applied electric field equal to E0, which is applied in the x direction. Calculate the excess carrier concentration as a function of x and t. EXAMPLE 6.5 ■ Solution The one-dimensional ambipolar transport equation for the minority carrier holes can be written from Equation (6.56) as 2 (p) (p) (p) p _ Dp __ p E0 _ _ p0 t x x2 (6.66) The solution to this partial differential equation is of the form p(x, t) p(x, t)e tp0 (6.67) By substituting Equation (6.67) into Equation (6.66), we are left with the partial differential equation 2 p(x, t) p(x, t) p(x, t) Dp __ p E0 __ __ x t x2 nea29583_ch06_192-240.indd 211 (6.68) 12/11/10 11:17 AM 212 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors Equation (6.68) is normally solved using Laplace transform techniques. The solution, without going through the mathematical details, is (x p E0 t)2 1 p(x, t) __ exp ___ 12 4Dp t (4Dp t) (6.69) The total solution, from Equations (6.67) and (6.69), for the excess minority carrier hole concentration is (x p E0t)2 etp0 exp ___ p(x, t) __ 12 4Dpt (4Dpt) (6.70) ■ Comment We could show that Equation (6.70) is a solution to the partial differential equation, Equation (6.66), by direct substitution. We may also note that Equation (6.70) is not normalized. ■ EXERCISE PROBLEM Ex 6.5 Consider the result of Example 6.5. Let Dp 10 cm2 /s, p0 107 s, p 400 cm2/V-s, and E0 100 V/cm. (a) Determine p for t 107 s at (i) x 20 m, (ii) x 40 m, and (iii) x 60 m. (b) Determine p for x 40 m at (i) t 5 108 s, (ii) t 107 s, and (iii) t 2 107 s. Compare the results to the curves shown in Figure 6.9. [Ans. (a) (i) 38.18, (ii) 103.8, (iii) 38.18; (b) (i) 32.75, (ii) 103.8, (iii) 3.65] Equation (6.70) can be plotted as a function of distance x, for various times. Figure 6.8 shows such a plot for the case when the applied electric field is zero. For t 0, the excess minority carrier holes diffuse in both the x and x directions. During this time, the excess majority carrier electrons, which were generated, diffuse at exactly the same rate as the holes. As time proceeds, the excess holes recombine with the excess electrons so that at t the excess hole concentration is zero. In this particular example, both diffusion and recombination processes are occurring at the same time. Figure 6.9 shows a plot of Equation (6.70) as a function of distance x at various times for the case when the applied electric field is not zero. In this case, the pulse of excess minority carrier holes is drifting in the x direction, which is the direction of the electric field. We still have the same diffusion and recombination processes as we had before. An important point to consider is that, with charge neutrality, n p at any instant of time and at any point in space. The excess electron concentration is equal to the excess hole concentration. In this case, then, the excess electron pulse is moving in the same direction as the applied electric field even though the electrons have a negative charge. In the ambipolar transport process, the excess carriers are characterized by the minority carrier parameters. In this example, the excess carriers behave according to the minority carrier hole parameters, which include Dp, p, and p0. The excess majority carrier electrons are being pulled along by the excess minority carrier holes. nea29583_ch06_192-240.indd 212 12/11/10 11:17 AM 6.3 Ambipolar Transport 213 ␦p(x, t) t t1 0 E0 t t2 t1 t t3 x0 t2 Distance, x Figure 6.8 | Excess hole concentration versus distance at various times for zero applied electric field. ␦p(x, t) t t1 0 t t2 t1 E0 t t3 x0 t2 Distance, x Figure 6.9 | Excess hole concentration versus distance at various times for a constant applied electric field. nea29583_ch06_192-240.indd 213 12/11/10 11:17 AM 214 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors TEST YOUR UNDERSTANDING TYU 6.5 As a good approximation, the peak value of a normalized excess carrier concentration, given by Equation (6.70), occurs at x pE 0t. Assume the following parameters: p0 5 s, Dp 10 cm2/s, p 386 cm2/V-s, and E 0 10 V/cm. Calculate the peak value at times of (a) t 1 s, (b) t 5 s, (c) t 15 s, and (d) t 25 s. What are the corresponding values of x for parts (a) to (d)? TYU 6.6 The excess carrier concentration, given by Equation (6.70), is to be calculated at distances of one diffusion length away from the peak value. Using the parameters given in TYU 6.5, calculate the values of p for (a) t 1 s at (i) 1.093 102 cm and (ii) x 3.21 103 cm; (b) t 5 s at (i) x 2.64 102 cm and (ii) x 1.22 102 cm; (c) t 15 s at (i) x 6.50 102 cm and (ii) x 5.08 102 cm. [Ans. (a) 73.0, x 38.6 m; (b) 14.7, x 193 m; (c) 1.15, x 579 m; (d ) 0.120, x 965 m] [Ans. (a) (i) 20.9, (ii) 20.9; (b) (i) 11.4, (ii) 11.4; (c) (i) 1.05, (ii) 1.05] 6.3.4 Dielectric Relaxation Time Constant We have assumed in the previous analysis that a quasi-neutrality condition exists— that is, the concentration of excess holes is balanced by an equal concentration of excess electrons. Suppose that we have a situation as shown in Figure 6.10, in which a uniform concentration of holes p is suddenly injected into a portion of the surface of a semiconductor. We will instantly have a concentration of excess holes and a net positive charge density that is not balanced by a concentration of excess electrons. How is charge neutrality achieved and how fast? There are three defining equations to be considered. Poisson’s equation is E_ (6.71) The current equation, Ohm’s law, is J E (6.72) The continuity equation, neglecting the effects of generation and recombination, is J_ (6.73) t ␦p holes n type Figure 6.10 | The injection of a concentration of holes into a small region at the surface of an n-type semiconductor. nea29583_ch06_192-240.indd 214 12/11/10 11:17 AM 6.3 Ambipolar Transport 215 The parameter is the net charge density and the initial value is given by e(p). We will assume that p is uniform over a short distance at the surface. The parameter is the permittivity of the semiconductor. Taking the divergence of Ohm’s law and using Poisson’s equation, we find E_ J (6.74) Substituting Equation (6.74) into the continuity equation, we have d _ _ _ t dt (6.75) Since Equation (6.75) is a function of time only, we can write the equation as a total derivative. Equation (6.75) can be rearranged as d _ _ 0 dt (6.76) Equation (6.76) is a first-order differential equation whose solution is (t) (0)e(t ) (6.77) d _ (6.78) d where and is called the dielectric relaxation time constant. Objective: Calculate the dielectric relaxation time constant for a particular semiconductor. EXAMPLE 6.6 Consider n-type silicon with a donor impurity concentration of Nd 1016 cm3. ■ Solution The conductivity is found as enNd (1.6 1019)(1200)(1016) 1.92 (-cm)1 where the value of mobility is the approximate value found from Figure 5.3. The permittivity of silicon is r 0 (11.7)(8.85 1014) F/cm The dielectric relaxation time constant is then (11.7)(8.85 1014) ____ d _ 5.39 1013 s 1.92 or d 0.539 ps nea29583_ch06_192-240.indd 215 12/11/10 11:17 AM 216 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors ■ Comment Equation (6.77) then predicts that in approximately four time constants, or in approximately 2 ps, the net charge density is essentially zero; that is, quasi-neutrality has been achieved. Since the continuity equation, Equation (6.73), does not contain any generation or recombination terms, the initial positive charge is then neutralized by pulling in electrons from the bulk n-type material to create excess electrons. This process occurs very quickly compared to the normal excess carrier lifetimes of approximately 0.1 s. The condition of quasi-chargeneutrality is then justified. ■ EXERCISE PROBLEM Ex 6.6 (a) Consider n-type GaAs doped to Nd 5 1015 cm3. Determine the dielectric relaxation time. (b) Repeat part (a) for p-type silicon doped to Na 2 1016 cm3. [Ans. (a) d 0.193 ps; (b) d 0.809 ps] *6.3.5 Haynes–Shockley Experiment We have derived the mathematics describing the behavior of excess carriers in a semiconductor. The Haynes–Shockley experiment was one of the first experiments to actually measure excess carrier behavior. Figure 6.11 shows the basic experimental arrangement. The voltage source V1 establishes an applied electric field E0 in the x direction in the n-type semiconductor sample. Excess carriers are effectively injected into the semiconductor at contact A. Contact B is a rectifying contact that is under reverse bias by the voltage source V2. The contact B will collect a fraction of the excess carriers as they drift through the semiconductor. The collected carriers will generate an output voltage, V0. This experiment corresponds to the problem we discussed in Example 6.5. Figure 6.12 shows the excess carrier concentrations at contacts A and B for two conditions. Figure 6.12a shows the idealized excess carrier pulse at contact A at time t 0. For a given electric field E01, the excess carriers will drift along the Vin V2 R V0 d A B R2 n type E0 R1 V1 Figure 6.11 | The basic Haynes–Shockley experimental arrangement. nea29583_ch06_192-240.indd 216 12/11/10 11:17 AM Ambipolar Transport 217 Input pulse 6.3 Time (a) Electric field, E01 V0 t0 Time (b) Electric field, E02 E01 V0 t0 Time (c) Figure 6.12 | (a) The idealized excess carrier pulse at terminal A at t 0. (b) The excess carrier pulse versus time at terminal B for a given applied electric field. (c) The excess carrier pulse versus time at terminal B for a smaller applied electric field. semiconductor producing an output voltage as a function of time given in Figure 6.12b. The peak of the pulse will arrive at contact B at time t0. If the applied electric field is reduced to a value E02, E02 E01, the output voltage response at contact B will look approximately as shown in Figure 6.12c. For the smaller electric field, the drift velocity of the pulse of excess carriers is smaller, and so it will take a longer time for the pulse to reach the contact B. During this longer time period, there is more diffusion and more recombination. The excess carrier pulse shapes shown in Figure 6.12b, c are different for the two electric field conditions. nea29583_ch06_192-240.indd 217 12/11/10 11:17 AM 218 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors The minority carrier mobility, lifetime, and diffusion coefficient can be determined from this single experiment. As a good first approximation, the peak of the minority carrier pulse will arrive at contact B when the exponent involving distance and time in Equation (6.70) is zero, or x p E0 t 0 (6.79a) In this case x d, where d is the distance between contacts A and B, and t t0, where t0 is the time at which the peak of the pulse reaches contact B. The mobility may be calculated as d p _ E0 t0 (6.79b) Figure 6.13 again shows the output response as a function of time. At times t1 and t2, the magnitude of the excess concentration is e1 of its peak value. If the time difference between t1 and t2 is not too large, et/ and (4 Dp t)1 2 do not change appreciably during this time; then the equation p0 (d p E0 t)2 4Dp t (6.80) is satisfied at both t t1 and t t2. If we set t t1 and t t2 in Equation (6.80) and add the two resulting equations, we may show that the diffusion coefficient is given by (p E0)2(t)2 Dp __ (6.81) 16t0 where t t2 t1 (6.82) The area S under the curve shown in Figure 6.13 is proportional to the number of excess holes that have not recombined with majority carrier electrons. We may write t0 d __ S K exp _ p0 K exp p E0p0 (6.83) where K is a constant. By varying the electric field, the area under the curve will change. A plot of ln (S) as a function of (dp E0) will yield a straight line whose slope is (1/p 0), so the minority carrier lifetime can also be determined from this experiment. V0 t1 t0 t2 Time Figure 6.13 | The output excess carrier pulse versus time to determine the diffusion coefficient. nea29583_ch06_192-240.indd 218 12/11/10 11:17 AM 6.4 Quasi-Fermi Energy Levels 219 The Haynes–Shockley experiment is elegant in the sense that the three basic processes of drift, diffusion, and recombination are all observed in a single experiment. The determination of mobility is straightforward and can yield accurate values. The determination of the diffusion coefficient and lifetime is more complicated and may lead to some inaccuracies. 6.4 | QUASI-FERMI ENERGY LEVELS The thermal-equilibrium electron and hole concentrations are functions of the Fermi energy level. We can write (6.84a) (6.84b) EF EFi n0 ni exp __ kT and EFi EF p0 ni exp __ kT where EF and EFi are the Fermi energy and intrinsic Fermi energy, respectively, and ni is the intrinsic carrier concentration. Figure 6.14a shows the energy-band diagram for an n-type semiconductor in which EF EFi. For this case, we may note from Equations (6.84a) and (6.84b) that n0 ni and p0 ni, as we would expect. Similarly, Figure 6.14b shows the energy-band diagram for a p-type semiconductor in which EF EFi. Again we may note from Equations (6.84a) and (6.84b) that n0 ni and p0 ni, as we would expect for the p-type material. These results are for thermal equilibrium. If excess carriers are created in a semiconductor, we are no longer in thermal equilibrium and the Fermi energy is strictly no longer defined. However, we may define a quasi-Fermi level for electrons and a quasi-Fermi level for holes that apply for nonequilibrium. If n and p are the excess electron and hole concentrations, respectively, we may write EFn EFi n0 n ni exp __ kT (6.85a) Ec Ev (a) Electron energy Electron energy EF EFi Ec EFi EF Ev (b) Figure 6.14 | Thermal-equilibrium energy-band diagrams for (a) n-type semiconductor and (b) p-type semiconductor. nea29583_ch06_192-240.indd 219 12/11/10 11:17 AM 220 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors and EFi EFp p0 p ni exp __ kT (6.85b) where EFn and EFp are the quasi-Fermi energy levels for electrons and holes, respectively. The total electron concentration and the total hole concentration are functions of the quasi-Fermi levels. EXAMPLE 6.7 Objective: Calculate the quasi-Fermi energy levels. Consider an n-type semiconductor at T 300 K with carrier concentrations of n0 1015 cm3, ni 1010 cm3, and p0 105 cm3. In nonequilibrium, assume that the excess carrier concentrations are n p 1013 cm3. ■ Solution The Fermi level for thermal equilibrium can be determined from Equation (6.84a). We have n0 EF EFi kT ln _ ni 0.2982 eV We can use Equation (6.85a) to determine the quasi-Fermi level for electrons in nonequilibrium. We can write n0 n EFn EFi kT ln __ 0.2984 eV ni Equation (6.85b) can be used to calculate the quasi-Fermi level for holes in nonequilibrium. We can write p0 p EFi EFp kT ln __ 0.179 eV ni ■ Comment We may note that the quasi-Fermi level for electrons is above EFi while the quasi-Fermi level for holes is below EFi. ■ EXERCISE PROBLEM Ex 6.7 Impurity concentrations of Nd 3 1015 cm3 and Na 1016 cm3 are added to silicon at T 300 K. Excess carriers are generated in the semiconductor such that the steady-state excess carrier concentrations are n p 4 1014 cm3. (a) Determine the thermal-equilibrium Fermi level with respect to the intrinsic Fermi level. (b) Find EFn and EFp with respect to EFi. [Ans. (a) EFi EF 0.33808 eV; (b) EFi EFp 0.33952 eV, EFn EFi 0.26395 eV] Figure 6.15a shows the energy-band diagram with the Fermi energy level corresponding to thermal equilibrium. Figure 6.15b now shows the energy-band diagram under the nonequilibrium condition. Since the majority carrier electron concentration does not change significantly for this low-injection condition, the quasi-Fermi level for electrons is not much different from the thermal-equilibrium Fermi level. nea29583_ch06_192-240.indd 220 12/11/10 11:17 AM 6.5 221 0.2982 eV 0.2984 eV 0.2982 eV EFi Ev EFn Electron energy Ec EF Electron energy Excess Carrier Lifetime (a) Ec EF EFi EFp 0.179 eV Ev (b) Figure 6.15 | (a) Thermal-equilibrium energy-band diagram for Nd 1015 cm3 and ni 1010 cm3. (b) Quasi-Fermi levels for electrons and holes if 1013 cm3 excess carriers are present. The quasi-Fermi energy level for the minority carrier holes is significantly different from the Fermi level and illustrates the fact that we have deviated from thermal equilibrium significantly. Since the electron concentration has increased, the quasiFermi level for electrons has moved slightly closer to the conduction band. The hole concentration has increased significantly so that the quasi-Fermi level for holes has moved much closer to the valence band. We will consider the quasi-Fermi energy levels again when we discuss forward-biased pn junctions. *6.5 | EXCESS CARRIER LIFETIME The rate at which excess electrons and holes recombine is an important characteristic of the semiconductor and influences many of the device characteristics, as we will see in later chapters. We considered recombination briefly at the beginning of this chapter and argued that the recombination rate is inversely proportional to the mean carrier lifetime. We have assumed up to this point that the mean carrier lifetime is simply a parameter of the semiconductor material. We have been considering an ideal semiconductor in which electronic energy states do not exist within the forbidden-energy bandgap. This ideal effect is present in a perfect single-crystal material with an ideal periodic-potential function. In a real semiconductor material, defects occur within the crystal and disrupt the perfect periodic-potential function. If the density of these defects is not too great, the defects will create discrete electronic energy states within the forbidden-energy band. These allowed energy states may be the dominant effect in determining the mean carrier lifetime. The mean carrier lifetime may be determined from the Shockley–Read– Hall theory of recombination. 6.5.1 Shockley–Read–Hall Theory of Recombination An allowed energy state, also called a trap, within the forbidden bandgap may act as a recombination center, capturing both electrons and holes with almost equal probability. This equal probability of capture means that the capture cross sections for nea29583_ch06_192-240.indd 221 12/11/10 11:17 AM 222 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors Process 1 Process 2 Ec Ec Ev Ev Electron capture Electron emission Process 3 Process 4 Ec Ec Hole capture Ev Ev Hole emission Figure 6.16 | The four basic trapping and emission processes for the case of an acceptortype trap. electrons and holes are approximately equal. The Shockley–Read–Hall theory of recombination assumes that a single recombination center, or trap, exists at an energy Et within the bandgap. There are four basic processes, shown in Figure 6.16, that may occur at this single trap. We will assume that the trap is an acceptor-type trap; that is, it is negatively charged when it contains an electron and is neutral when it does not contain an electron. The four basic processes are as follows: Process 1: The capture of an electron from the conduction band by an initially neutral empty trap. Process 2: The inverse of process 1—the emission of an electron that is initially occupying a trap level back into the conduction band. Process 3: The capture of a hole from the valence band by a trap containing an electron. (Or we may consider the process to be the emission of an electron from the trap into the valence band.) Process 4: The inverse of process 3—the emission of a hole from a neutral trap into the valence band. (Or we may consider this process to be the capture of an electron from the valence band.) In process 1, the rate at which electrons from the conduction band are captured by the traps is proportional to the density of electrons in the conduction band and nea29583_ch06_192-240.indd 222 12/11/10 11:17 AM 6.5 Excess Carrier Lifetime 223 proportional to the density of empty trap states. We can then write the electron capture rate as Rcn CnNt[1 fF(Et)]n (6.86) where Rcn capture rate (#/cm3-s) Cn constant proportional to electron-capture cross section Nt total concentration of trapping centers n electron concentration in the conduction band fF(Et) Fermi function at the trap energy The Fermi function at the trap energy is given by 1 fF (Et) ____ Et EF 1 exp __ kT (6.87) which is the probability that a trap will contain an electron. The function [1 fF(Et)] is then the probability that the trap is empty. In Equation (6.87), we have assumed that the degeneracy factor is 1, which is the usual approximation made in this analysis. However, if a degeneracy factor is included, it will eventually be absorbed in other constants later in the analysis. For process 2, the rate at which electrons are emitted from filled traps back into the conduction band is proportional to the number of filled traps, so that Ren En Nt fF (Et) (6.88) where Ren emission rate (#/cm3-s) En constant fF(Et) probability that the trap is occupied In thermal equilibrium, the rate of electron capture from the conduction band and the rate of electron emission back into the conduction band must be equal. Then RenRcn (6.89) En Nt fF0 (Et) Cn Nt [1 fF0(Et)]n0 (6.90) so that where fF0 denotes the thermal-equilibrium Fermi function. Note that, in thermal equilibrium, the value of the electron concentration in the capture rate term is the equilibrium value n0. Using the Boltzmann approximation for the Fermi function, we can find En in terms of Cn as En nCn nea29583_ch06_192-240.indd 223 (6.91) 12/11/10 11:17 AM 224 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors where n is defined as (Ec Et) n Nc exp __ kT (6.92) The parameter n is equivalent to an electron concentration that would exist in the conduction band if the trap energy Et coincided with the Fermi energy EF. In nonequilibrium, excess electrons exist, so that the net rate at which electrons are captured from the conduction band is given by Rn Rcn Ren (6.93) which is just the difference between the capture rate and the emission rate. Combining Equations (6.86) and (6.88) with (6.93) gives Rn [Cn Nt (1 fF (Et))n] [En Nt fF (Et)] (6.94) We may note that, in this equation, the electron concentration n is the total concentration, which includes the excess electron concentration. The remaining constants and terms in Equation (6.94) are the same as defined previously and the Fermi energy in the Fermi probability function needs to be replaced by the quasi-Fermi energy for electrons. The constants En and Cn are related by Equation (6.91), so the net recombination rate can be written as Rn Cn Nt [n(1 fF (Et)) nfF (Et)] (6.95) If we consider processes 3 and 4 in the recombination theory, the net rate at which holes are captured from the valence band is given by Rp Cp Nt [pfF(Et) p(1 fF (Et))] (6.96) where Cp is a constant proportional to the hole capture rate, and p is given by (Et Ev) p Nv exp __ kT (6.97) In a semiconductor in which the trap density is not too large, the excess electron and hole concentrations are equal and the recombination rates of electrons and holes are equal. If we set Equation (6.95) equal to Equation (6.96) and solve for the Fermi function, we obtain Cn n Cp p fF (Et) _____ Cn(n n) Cp(p p) (6.98) We may note that n p n2i . Then, substituting Equation (6.98) back into either Equation (6.95) or (6.96) gives CnCp Nt np n2i Rn Rp _____ R Cn(n n) Cp(p p) (6.99) Equation (6.99) is the recombination rate of electrons and holes due to the recombination center at E Et. If we consider thermal equilibrium, then np n0 p0 n2, so i nea29583_ch06_192-240.indd 224 12/11/10 11:17 AM 6.5 Excess Carrier Lifetime 225 that Rn Rp 0. Equation (6.99), then, is the recombination rate of excess electrons and holes. Since R in Equation (6.99) is the recombination rate of the excess carriers, we may write n R_ (6.100) where n is the excess carrier concentration and is the lifetime of the excess carriers. 6.5.2 Limits of Extrinsic Doping and Low Injection We simplified the ambipolar transport equation, Equation (6.39), from a nonlinear differential equation to a linear differential equation by applying limits of extrinsic doping and low injection. We may apply these same limits to the recombination rate equation. Consider an n-type semiconductor under low injection. Then n0 p0, n0 p, n0 n, n0 p where p is the excess minority carrier hole concentration. The assumptions of n0 n and n0 p imply that the trap level energy is near midgap so that n and p are not too different from the intrinsic carrier concentration. With these assumptions, Equation (6.99) reduces to R Cp Nt p (6.101) The recombination rate of excess carriers in the n-type semiconductor is a function of the parameter Cp, which is related to the minority carrier hole capture cross section. The recombination rate, then, is a function of the minority carrier parameter in the same way that the ambipolar transport parameters reduced to their minority carrier values. The recombination rate is related to the mean carrier lifetime. Comparing Equations (6.100) and (6.101), we may write p n C N p _ R_ p t p0 (6.102) 1 p0 _ Cp Nt (6.103) where and where p0 is defined as the excess minority carrier hole lifetime. If the trap concentration increases, the probability of excess carrier recombination increases; thus, the excess minority carrier lifetime decreases. Similarly, if we have a strongly extrinsic p-type material under low injection, we can assume that p0 n0, nea29583_ch06_192-240.indd 225 p0 n, p0 n, p0 p 12/11/10 11:17 AM 226 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors The lifetime then becomes that of the excess minority carrier electron lifetime, or 1 n0 _ Cn Nt (6.104) Again note that for the n-type material, the lifetime is a function of Cp, which is related to the capture rate of the minority carrier hole. And for the p-type material, the lifetime is a function of Cn, which is related to the capture rate of the minority carrier electron. The excess carrier lifetime for an extrinsic material under low injection reduces to that of the minority carrier. EXAMPLE 6.8 Objective: Determine the excess carrier lifetime in an intrinsic semiconductor. If we substitute the definitions of excess carrier lifetimes from Equations (6.103) and (6.104) into Equation (6.99), the recombination rate can be written as np n2 R _____ p0(n n) n0(p p) i (6.105) Consider an intrinsic semiconductor containing excess carriers. Then n ni n and p ni n. Also assume that n p ni. ■ Solution Equation (6.105) now becomes 2ni n (n)2 R ____ (2ni n)(p0 n0) If we also assume very low injection, so that n 2ni, then we can write n n _ R __ p0 n0 where is the excess carrier lifetime. We see that p0 n0 in the intrinsic material. ■ Comment The excess carrier lifetime increases as we change from an extrinsic to an intrinsic semiconductor. ■ EXERCISE PROBLEM Ex 6.8 Consider silicon at T 300 K doped at concentrations of Nd 1015 cm3 and Na 0. Assume that n p ni in the excess carrier recombination rate equation and assume parameter values of n0 p0 5 107 s. Calculate the recombination rate of excess carriers if n p 1014 cm3. (Ans. 1.83 10 20 cm3 s1) Intuitively, we can see that the number of majority carriers that are available for recombining with excess minority carriers decreases as the extrinsic semiconductor becomes intrinsic. Since there are fewer carriers available for recombining in the intrinsic material, the mean lifetime of an excess carrier increases. nea29583_ch06_192-240.indd 226 12/11/10 11:17 AM 6.6 Surface Effects 227 *6.6 | SURFACE EFFECTS In all previous discussions, we have implicitly assumed the semiconductors were infinite in extent; thus, we were not concerned with any boundary conditions at a semiconductor surface. In any real application of semiconductors, the material is not infinitely large and therefore surfaces do exist between the semiconductor and an adjacent medium. 6.6.1 Surface States When a semiconductor is abruptly terminated, the perfect periodic nature of the idealized single-crystal lattice ends abruptly at the surface. The disruption of the periodic-potential function results in allowed electronic energy states within the energy bandgap. In the previous section, we argued that simple defects in the semiconductor would create discrete energy states within the bandgap. The abrupt termination of the periodic potential at the surface results in a distribution of allowed energy states within the bandgap, shown schematically in Figure 6.17 along with the discrete energy states in the bulk semiconductor. The Shockley–Read–Hall recombination theory shows that the excess minority carrier lifetime is inversely proportional to the density of trap states. We may argue that since the density of traps at the surface is larger than in the bulk, the excess minority carrier lifetime at the surface will be smaller than the corresponding lifetime in the bulk material. If we consider an extrinsic n-type semiconductor, for example, the recombination rate of excess carriers in the bulk, given by Equation (6.102), is p _ pB R_ (6.106) p0 p0 where pB is the concentration of excess minority carrier holes in the bulk material. We may write a similar expression for the recombination rate of excess carriers at the surface as ps Rs _ (6.107) p0s where ps is the excess minority carrier hole concentration at the surface and p0s is the excess minority carrier hole lifetime at the surface. Electron energy Ec Et Ev Surface Figure 6.17 | Distribution of surface states within the forbidden bandgap. nea29583_ch06_192-240.indd 227 12/11/10 11:17 AM 228 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors ␦p ␦pB ␦ps Distance x Surface Figure 6.18 | Steady-state excess hole concentration versus distance from a semiconductor surface. Assume that excess carriers are being generated at a constant rate throughout the entire semiconductor material. We showed that, in steady state, the generation rate is equal to the recombination rate for the case of a homogeneous, infinite semiconductor. Using this argument, the recombination rates at the surface and in the bulk material must be equal. Since p0s p0, then the excess minority carrier concentration at the surface is smaller than the excess minority carrier concentration in the bulk region, or ps pB. Figure 6.18 shows an example of the excess carrier concentration plotted as a function of distance from the semiconductor surface. EXAMPLE 6.9 Objective: Determine the steady-state excess carrier concentration as a function of distance from the surface of a semiconductor. Consider Figure 6.18, in which the surface is at x 0. Assume that in the n-type semiconductor pB 1014 cm3 and p0 106 s in the bulk, and p0s 107 s at the surface. Assume zero applied electric field and let Dp 10 cm2/s. ■ Solution From Equations (6.106) and (6.107), we have pB _ ps _ p0 p0s so that p0s 107 14 _ 13 3 ps pB _ p0 (10 ) 106 10 cm From Equation (6.56), we can write d 2(p) p Dp__ g _ p0 0 dx2 (6.108) The generation rate can be determined from the steady-state conditions in the bulk, or pB _ 1014 20 3 1 g _ p0 106 10 cm -s nea29583_ch06_192-240.indd 228 12/11/10 11:17 AM 6.6 Surface Effects 229 The solution to Equation (6.107) is of the form p(x) gp0 Ae xLp Be xLp (6.109) As x → , p(x) pB gp0 1014 cm3, which implies that A 0. At x 0, we have p(0) ps 1014 B 1013 cm3 so that B 9 1013. The entire solution for the minority carrier hole concentration as a function of distance from the surface is p(x) 1014 (1 0.9e xLp) where Lp _____ Dpp0 _________ (10)(106) 31.6 m ■ Comment The excess carrier concentration is smaller at the surface than in the bulk. ■ EXERCISE PROBLEM Ex 6.9 (a) Repeat Example 6.9 for the case when 0s 0. (b) What is the excess hole concentration at x 0? (c) For this particular case, what is the recombination rate of excess carriers at the surface? [Ans. (a) p(x) gp0 (1 e xLp); (b) p(0) 0; (c) R ] 6.6.2 Surface Recombination Velocity A gradient in the excess carrier concentration exists near the surface as shown in Figure 6.18; excess carriers from the bulk region diffuse toward the surface where they recombine. This diffusion toward the surface can be described by d(p) Dp n̂ _ dx | surf sp|surf (6.110) where each side of the equation is evaluated at the surface. The parameter n̂ is the unit outward vector normal to the surface. Using the geometry of Figure 6.18, d(p)/dx is a positive quantity and n̂ is negative, so that the parameter s is a positive quantity. A dimensional analysis of Equation (6.110) shows that the parameter s has units of cm/s, or velocity. The parameter s is called the surface recombination velocity. If the excess concentrations at the surface and in the bulk region were equal, then the gradient term would be zero and the surface recombination velocity would be zero. As the excess concentration at the surface becomes smaller, the gradient term becomes larger, and the surface recombination velocity increases. The surface recombination velocity gives some indication of the surface characteristics as compared with the bulk region. nea29583_ch06_192-240.indd 229 12/11/10 11:17 AM 230 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors Equation (6.110) may be used as a boundary condition to the general solution given by Equation (6.109) in Example 6.8. Using Figure 6.18, we have that n̂ 1, and Equation (6.110) becomes d(p) Dp _ dx | surf sp|surf (6.111) We have argued that the coefficient A is zero in Equation (6.109). Then, from Equation (6.109), we can write that psurf p(0) gp0 B and d(p) _ dx | surf d(p) _ dx | x0 (6.112a) B _ Lp (6.112b) Substituting Equations (6.112a) and (6.112b) into Equation (6.111) and solving for the coefficient B, we obtain sgp0 B __ (DpLp) s (6.113) The excess minority carrier hole concentration can then be written as sLpexL p(x) gp0 1 __ Dp sLp EXAMPLE 6.10 (6.114) Objective: Determine the value of surface recombination velocity corresponding to the parameters given in Example 6.9. From Example 6.9, we have that gp0 1014 cm3, Dp 10 cm2/s, Lp 31.6 m, and p(0) 1013 cm3. ■ Solution Writing Equation (6.114) at the surface, we have s p(0) gp0 1 ___ (Dp /Lp) s Solving for the surface recombination velocity, we find that Dp gp0 s_ _1 Lp p(0) which becomes 1014 1 2.85 104 cm/s 10 _ s __ 31.6 104 1013 nea29583_ch06_192-240.indd 230 12/11/10 11:17 AM Glossary of Important Terms 231 ■ Comment This example shows that a surface recombination velocity of approximately s 3 104 cms could seriously degrade the performance of semiconductor devices, such as solar cells, since these devices tend to be fabricated close to a surface. ■ EXERCISE PROBLEM Ex 6.10 (a) Using Equation (6.114), determine p(x) for (i) s and (ii) s 0. (b) What does (i) an infinite surface recombination velocity (s ) and (ii) a zero surface recombination velocity (s 0) imply? [Ans. (a) (i) p(x) gp0 1 exL , (ii) p(x) gp0; (b) (i) p(0) 0, (ii) p(0) gp0 and p(x) constant] p In the above example, the surface influences the excess carrier concentration to the extent that, even at a distance of Lp 31.6 m from the surface, the excess carrier concentration is only two-thirds of the value in the bulk. We will see in later chapters that device performance is dependent in large part on the properties of excess carriers. 6.7 | SUMMARY ■ ■ ■ ■ ■ ■ ■ ■ The processes of excess electron and hole generation and recombination were discussed. The excess carrier generation rate and recombination rate were defined. Excess electrons and holes do not move independently of each other, but move together. This common movement is called ambipolar transport. The ambipolar transport equation was derived and limits of low injection and extrinsic doping were applied to the coefficients. Under these conditions, the excess electrons and holes diffuse and drift together with the characteristics of the minority carrier, a result that is fundamental to the behavior of semiconductor devices. The concept of excess carrier lifetime was developed. Examples of excess carrier behavior as a function of time, as a function of space, and as a function of both time and space were examined. The quasi-Fermi level for electrons and the quasi-Fermi level for holes were defined. The degree of quasi-Fermi level splitting is a measure of departure from thermal equilibrium. The Shockley–Read–Hall theory of recombination was considered. Expressions for the excess minority carrier lifetime were developed. Generation and recombination of excess carriers increase as a result of traps in a semiconductor. The effect of a semiconductor surface influences the behavior of excess electrons and holes. The surface recombination velocity was defined. GLOSSARY OF IMPORTANT TERMS ambipolar diffusion coefficient The effective diffusion coefficient of excess carriers. ambipolar mobility The effective mobility of excess carriers. ambipolar transport The process whereby excess electrons and holes diffuse, drift, and recombine with the same effective diffusion coefficient, mobility, and lifetime. nea29583_ch06_192-240.indd 231 12/11/10 11:17 AM 232 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors ambipolar transport equation The equation describing the behavior of excess carriers as a function of time and space coordinates. carrier generation The process of elevating electrons from the valence band into the conduction band, creating an electron–hole pair. carrier recombination The process whereby an electron “falls” into an empty state in the valence band (a hole) so that an electron–hole pair is annihilated. excess carriers The term describing both excess electrons and excess holes. excess electrons The concentration of electrons in the conduction band over and above the thermal-equilibrium concentration. excess holes The concentration of holes in the valence band over and above the thermal-equilibrium concentration. excess minority carrier lifetime The average time that an excess minority carrier exists before it recombines. generation rate The rate (#/cm3-s) at which electron–hole pairs are created. low-level injection The condition in which the excess carrier concentration is much smaller than the thermal-equilibrium majority carrier concentration. minority carrier diffusion length The___ average distance a minority carrier diffuses before recombining: a parameter equal to D where D and are the minority carrier diffusion coefficient and lifetime, respectively. quasi-Fermi level The quasi-Fermi level for electrons and the quasi-Fermi level for holes relate the nonequilibrium electron and hole concentrations, respectively, to the intrinsic carrier concentration and the intrinsic Fermi level. recombination rate The rate (#/cm3-s) at which electron–hole pairs recombine. surface recombination velocity A parameter that relates the gradient of the excess carrier concentration at a surface to the surface concentration of excess carriers. surface states The electronic energy states that exist within the bandgap at a semiconductor surface. CHECKPOINT After studying this chapter, the reader should have the ability to: ■ ■ ■ ■ ■ ■ ■ ■ ■ ■ nea29583_ch06_192-240.indd 232 Describe the concept of excess carrier generation and recombination. Describe the concept of an excess carrier lifetime. Describe how the time-dependent diffusion equations for holes and electrons are derived. Describe how the ambipolar transport equation is derived. Understand the consequence of the coefficients in the ambipolar transport equation reducing to the minority carrier values under low injection and extrinsic semiconductors. Apply the ambipolar transport equation to various problems. Understand the concept of the dielectric relaxation time constant and what it means. Calculate the quasi-Fermi levels for electrons and holes. Calculate the excess carrier recombination rate for a given concentration of excess carriers. Understand the effect of a surface on the excess carrier concentrations. 12/11/10 11:17 AM Problems 233 REVIEW QUESTIONS 1. Why are the electron generation rate and recombination rate equal in thermal equilibrium? 2. Define the excess carrier recombination rate in terms of excess carrier concentration and lifetime. 3. Explain how the density of holes, for example, can change as a result of a change in the flux of particles. 4. Why is the general ambipolar transport equation nonlinear? 5. Explain qualitatively why a pulse of excess electrons and holes would move together in the presence of an applied electric field. 6. Explain qualitatively why the excess carrier lifetime reduces to that of the minority carrier under low injection. 7. What is the time dependence of the density of excess carriers when the generation rate becomes zero? 8. In the presence of an external force, why doesn’t the density of excess carriers continue to increase with time? 9. When a concentration of one type of excess carrier is suddenly created in a semiconductor, what is the mechanism by which the net charge density quickly becomes zero? 10. State the definition of the quasi-Fermi level for electrons. Repeat for holes. 11. Explain why the presence of traps in a semiconductor increases the recombination rate of excess carriers. 12. Why, in general, is the concentration of excess carriers less at the surface of a semiconductor than in the bulk? PROBLEMS (Note: Use the semiconductor parameters listed in Appendix B if they are not specifically given in a problem. Assume T 300 K.) Section 6.1 Carrier Generation and Recombination Consider silicon at T 300 K that is doped with donor impurity atoms to a concentration of Nd 5 1015 cm3. The excess carrier lifetime is 2 107s. (a) Determine the thermal equilibrium recombination rate of holes. (b) Excess carriers are generated such that n p 1014 cm3. What is the recombination rate of holes for this condition? 6.2 GaAs, at T 300 K, is uniformly doped with acceptor impurity atoms to a concentration of Na 2 1016 cm3. Assume an excess carrier lifetime of 5 107s. (a) Determine the electron–hole recombination rate if the excess electron concentration is n 5 1014 cm3. (b) Using the results of part (a), what is the lifetime of holes? 6.3 An n-type silicon sample contains a donor concentration of Nd 1016 cm3. The minority carrier hole lifetime is found to be p0 20 s. (a) What is the lifetime of the majority carrier electrons? (b) Determine the thermal-equilibrium generation rate for electrons and holes in this material. (c) Determine the thermal-equilibrium recombination rate for electrons and holes in this material. 6.1 nea29583_ch06_192-240.indd 233 12/11/10 11:17 AM 234 CHAPTER 6 6.4 Nonequilibrium Excess Carriers in Semiconductors (a) A sample of semiconductor has a cross-sectional area of 1 cm2 and a thickness of 0.1 cm. Determine the number of electron–hole pairs that are generated per unit volume per unit time by the uniform absorption of 1 watt of light at a wavelength of 6300 Å. Assume each photon creates one electron–hole pair. (b) If the excess minority carrier lifetime is 10 s, what is the steady-state excess carrier concentration? Section 6.2 Mathematical Analysis of Excess Carriers 6.5 6.6 Derive Equation (6.27) from Equations (6.18) and (6.20). Consider a one-dimensional hole flux as shown in Figure 6.4. If the generation rate of holes in this differential volume is gp 1020 cm3-s1 and the recombination rate is 2 1019 cm3-s1, what must be the gradient in the particle current density to maintain a steady-state hole concentration? 6.7 Repeat Problem 6.6 if the generation rate becomes zero. Section 6.3 Ambipolar Transport 6.8 Starting with the continuity equations given by Equations (6.29) and (6.30), derive the ambipolar transport equation given by Equation (6.39). 6.9 A silicon sample at T 300 K has a uniform acceptor concentration of 7 1015 cm3. The excess carrier lifetime is n0 107 s. (a) Determine the ambipolar mobility. (b) Find the ambipolar diffusion coefficient. (c) What are the electron and hole lifetimes? 6.10 Germanium at T 300 K is uniformly doped with donor impurity atoms to a concentration of 4 1013 cm3. The excess carrier lifetime is found to be p0 2 106 s. (a) Determine the ambipolar (i) diffusion coefficient and (ii) mobility. (b) Find the electron and hole lifetimes. 6.11 Assume that an n-type semiconductor is uniformly illuminated, producing a uniform excess generation rate g. Show that in steady state the change in the semiconductor conductivity is given by e(n p) p 0 g Consider a silicon sample at T 300 K that is uniformly doped with acceptor impurity atoms at a concentration of Na 1016 cm3. At t 0, a light source is turned on generating excess carriers uniformly throughout the sample at a rate of g 8 1020 cm3 s1. Assume the minority carrier lifetime is n0 5 107 s, and assume mobility values of n 900 cm2 /V-s and p 380 cm2 /V-s. (a) Determine the conductivity of the silicon as a function of time for t 0. (b) What is the value of conductivity at (i) t 0 and (ii) t ? 6.13 An n-type GaAs semiconductor at T 300 K is uniformly doped at Nd 5 1015 cm3. The minority carrier lifetime is p0 5 108 s. Assume mobility values of n 7500 cm2 /V-s and p 310 cm2 /V-s. A light source is turned on at t 0 generating excess carriers uniformly at a rate of g 4 1021 cm3 s1 and turns off at t 106 s. (a) Determine the excess carrier concentrations versus time over the range 0 t . (b) Calculate the conductivity of the semiconductor versus time over the same time period as part (a). 6.14 A bar of silicon at T 300 K has a length of L 0.05 cm and a cross-sectional area of A 105 cm2. The semiconductor is uniformly doped with Nd 8 1015 cm3 and Na 2 1015 cm3. A voltage of 10 V is applied across the length of the material. For 6.12 nea29583_ch06_192-240.indd 234 12/11/10 11:17 AM Problems 6.15 6.16 6.17 6.18 6.19 235 t 0, the semiconductor has been uniformly illuminated with light, producing an excess carrier generation rate of g 8 1020 cm3 s1. The minority carrier lifetime is p0 5 107 s. At t 0, the light source is turned off. Determine the current in the semiconductor as a function of time for t 0. Silicon at T 300 K is uniformly doped with impurity atoms at concentrations of Na 2 1016 cm3 and Nd 6 1015 cm3 and is in thermal equilibrium for t 0. A light source turns on at t 0 producing excess carriers with a uniform generation rate of g 2 1021 cm3 s1. The electric field is zero. (a) If the maximum, steadystate excess carrier concentrations are n p 5 1014 cm3, determine the excess minority carrier lifetime. (b) Derive the expressions for the excess carrier concentration and excess carrier recombination rate as a function of time. (c) Determine the times at which the excess carrier concentration is equal to (i) one-fourth, (ii) one-half, (iii) three-fourths, and (iv) 95% of the steady-state value. In a GaAs material at T 300 K, the doping concentrations are Nd 8 1015 cm3 and Na 2 1015 cm3. The thermal equilibrium recombination rate is Ro 4 104 cm3 s1. (a) What is the minority carrier lifetime? (b) A uniform generation rate for excess carriers results in an excess carrier recombination rate of R 2 1021 cm3 s1. What is the steady-state excess carrier concentration? (c) What is the excess carrier lifetime? (a) Consider a silicon sample at T 300 K doped with 1016 cm3 donor atoms. Let p0 5 107 s. A light source turns on at t 0 producing excess carriers with a uniform generation rate of g 5 1020 cm3 s1. At t 5 107 s, the light source turns off. (i) Derive the expression(s) for the excess carrier concentration as a function of time over the range 0 t . (ii) What is the value of the excess concentration when the light source turns off. (b) Repeat part (a) for the case when the light source turns off at t 2 106 s. (c) Sketch the excess minority carrier concentrations versus time for parts (a) and (b). A semiconductor is uniformly doped with 1017 cm3 acceptor atoms and has the following properties: Dn 27 cm2/s, Dp 12 cm2/s, n0 5 107 s, and p0 107 s. An external source has been turned on for t 0 producing a uniform concentration of excess carriers at a generation rate of g 1021 cm3 s1. The source turns off at time t 0 and back on at time t 2 106 s. (a) Derive the expressions for the excess carrier concentration as a function of time for 0 t . (b) Determine the value of excess carrier concentration at (i) t 0, (ii) t 2 106 s, and (iii) t . (c) Plot the excess carrier concentration as a function of time. Consider a bar of p-type silicon that is uniformly doped to a value of Na 2 1016 cm3 at T 300 K. The applied electric field is zero. A light source is incident on the end of the semiconductor as shown in Figure P6.19. The steady-state concentration of excess carriers generated at x 0 is p(0) n(0) 2 1014 cm3. Assume the following p type Light x0 x Figure P6.19 | Figure for Problems 6.19 and 6.21. nea29583_ch06_192-240.indd 235 12/11/10 11:17 AM 236 CHAPTER 6 6.20 6.21 6.22 Nonequilibrium Excess Carriers in Semiconductors parameters: n 1200 cm2 /V-s, p 400 cm2 /V-s, n0 106 s, and p0 5 107 s. Neglecting surface effects, (a) determine the steady-state excess electron and hole concentrations as a function of distance into the semiconductor, and (b) calculate the steady-state electron and hole diffusion current densities as a function of distance into the semiconductor. The x 0 end of an Na 1 1014 cm3 doped semi-infinite (x 0) bar of silicon maintained at T 300 K is attached to a “minority carrier digester” which makes np 0 at x 0 (np is the minority carrier electron concentration in a p-type semiconductor). The electric field is zero. (a) Determine the thermal-equilibrium values of n p 0 and p p 0. (b) What is the excess minority carrier concentration at x 0? (c) Derive the expression for the steady-state excess minority carrier concentration as a function of x. In a p-type silicon semiconductor, excess carriers are being generated at the end of the bar at x 0 as shown in Figure P6.19. The uniform doping concentrations are Na 7 1016 cm3 and Nd 2 1016 cm3. The steady-state excess carrier concentrations at x 0 are p(0) n(0) 5 1014 cm3. (Neglect surface effects.) The electric field is zero. Assume semiconductor parameters of n0 p0 106 s, Dn 25 cm2 /s, and Dp 10 cm2 /s. (a) Calculate n and the electron and hole diffusion current densities at x 0. (b) Repeat part (a) for x 5 103 cm. (c) Repeat part (a) for x 15 103 cm. Consider an n-type silicon sample. Excess carriers are generated at x 0 such as shown in Figure 6.6. A constant electric field E0 is applied in the x direction. Show that the steady-state excess carrier concentration is given by p(x) A exp (s_x) where and x 0 and 1 s _ Lp p(x) A exp (sx) _____ 1 2 x 0 p Lp E 0 __ 2Dn Plot the excess carrier concentration p(x) versus x from Problem 6.22 for (a) E0 0 and (b) E0 10 V/cm. *6.24 Consider the semiconductor described in Problem 6.19. Assume a constant electric field E0 is applied in the x direction. (a) Derive the expression for the steady-state excess electron concentration. (Assume the solution is of the form eax.) (b) Plot n versus x for (i) E0 0 and (ii) E0 12 V/cm. (c) Explain the general characteristics of the two curves plotted in part (b). 6.25 Assume that a p-type semiconductor is in thermal equilibrium for t 0 and has an infinite minority carrier lifetime. Also assume that the semiconductor is uniformly illuminated, resulting in a uniform generation rate, g(t), which is given by 6.23 g(t) G0 for 0 t g(t) 0 for t 0 and t T T where G0 is a constant. Find the excess minority carrier concentration as a function of time. *6.26 Consider the n-type semiconductor shown in Figure P6.26. Illumination produces a constant excess carrier generation rate, G0, in the region L x L. Assume that the *Asterisks next to problems indicate problems that are more difficult. nea29583_ch06_192-240.indd 236 12/11/10 11:17 AM Problems 237 Illumination 3L L 0 L 3L x Figure P6.26 | Figure for Problem 6.26. minority carrier lifetime is infinite and assume that the excess minority carrier hole concentration is zero at x 3L and at x 3L. Find the steady-state excess minority carrier concentration versus x, for the case of low injection and for zero applied electric field. 6.27 An n-type semiconductor at T 300 K is used in the Haynes–Shockley experiment. The length of the sample is 0.4 cm and the applied voltage is V1 8V. The contacts A and B are separated by 0.25 cm. The peak of the pulse arrives at contact B 32 s after carrier injection at contact A. The width of the pulse is t 9.35 s. Determine the hole mobility and diffusion coefficient. Compare the results with the Einstein relation. 6.28 Consider the function f(x, t) (4Dt)1 2 exp (x2/4Dt). (a) Show that this function is a solution to the differential equation D( 2f / x2) f t. (b) Show that the integral of the function f(x, t) over x from to is unity for all values of time. (c) Show that this function approaches a function as t approaches zero. 6.29 The basic equation in the Haynes–Shockley experiment is given by Equation (6.70). (a) Plot p(x, t) versus x for various values of t and for E0 0 as well as for E0 ⬆ 0. (b) Plot p(x, t) versus t for various values of x and for E0 0 as well as for E0 ⬆ 0. Section 6.4 Quasi-Fermi Energy Levels An n-type silicon semiconductor, doped at Nd 4 1016 cm3, is steadily illuminated such that g 2 1021 cm3 s1. Assume n0 106 s and p0 5 107 s. (a) Determine the thermal-equilibrium value of EF EFi. (b) Calculate the quasiFermi levels for electrons and holes with respect to EFi. (c) What is the difference (in eV) between EFn and EF ? 6.31 Consider a p-type silicon semiconductor at T 300 K doped at Na 5 1015 cm3. (a) Determine the position of the Fermi level with respect to the intrinsic Fermi level. (b) Excess carriers are generated such that the excess carrier concentration is 10 percent of the thermal-equilibrium majority carrier concentration. Determine the quasiFermi levels with respect to the intrinsic Fermi level. (c) Plot the Fermi level and quasi-Fermi levels with respect to the intrinsic level. 6.32 Consider n-type silicon doped at Nd 5 1015 cm3. It is found that EFn EF 1.02 103 eV. (a) What is the excess carrier concentration? (b) Determine EFn EFi. (c) Calculate EFi EFp. 6.33 A p-type silicon sample is doped at Na 6 1015 cm3. It is determined that EFn EFi 0.270 eV. (a) Determine the excess carrier concentration. (b) Find EFi EFp. (c) (i) Derive the expression for EF EFp. (ii) Find EF EFp. 6.30 nea29583_ch06_192-240.indd 237 12/11/10 11:17 AM 238 CHAPTER 6 6.34 6.35 6.36 6.37 6.38 Nonequilibrium Excess Carriers in Semiconductors Consider n-type GaAs doped at Nd 1016 cm3. (a) For an excess concentration of p (0.02)Nd, determine (i) EFn EFi and (ii) EFi EFp. (b) Repeat part (a) if p (0.1)Nd. A p-type gallium arsenide semiconductor at T 300 K is doped at Na 1016 cm3. The excess carrier concentration varies linearly from 1014 cm3 to zero over a distance of 50 m. Plot the position of the quasi-Fermi levels with respect to the intrinsic Fermi level versus distance. Consider p-type silicon at T 300 K doped to Na 5 1014 cm3. Assume excess carriers are present and assume that EF EFp (0.01)kT. (a) Does this condition correspond to low injection? Why or why not? (b) Determine EFn EFi. An n-type silicon sample is doped with donors at a concentration of Nd 1016 cm3. Excess carriers are generated such that the excess hole concentration is given by p(x) 1014 exp (x104 )cm3. Plot the function EFiEFp versus x over the range 0 x 4 104. An n-type silicon semiconductor is doped at Nd 2 1016 cm3. (a) Plot EFi EFp as a function of p over the range 1011 p 1015 cm3. (Use a log scale for p.) (b) Repeat part (a) for EFn EFi. Section 6.5 Excess Carrier Lifetime Consider Equation (6.99) and the definitions of p0 and n0 by Equations (6.103) and (6.104). Let n p ni. Assume that in a particular region of a semiconductor, n p 0. (a) Determine the recombination rate R. (b) Explain what this result means physically. 6.40 Again consider Equation (6.99) and the definitions of p0 and n0 given by Equations (6.103) and (6.104). Let p0 107 s and n0 5 107 s. Also let n p ni 1010 cm3. Assume very low injection so that n ni. Calculate R/n for a semiconductor which is (a) n-type (n0 p0), (b) intrinsic (n0 p0 ni), and (c) p-type (p0 n0). 6.39 Section 6.6 Surface Effects *6.41 Consider an n-type semiconductor as shown in Figure P6.41, doped at Nd 1016 cm3 and with a uniform excess carrier generation rate equal to g 1021 cm3-s1. Assume that Dp 10 cm 2/s and p0 107 s. The electric field is zero. (a) Determine the steady-state excess minority carrier concentration versus x if the surface recombination velocity at x 0 is (i) s 0, (ii) s 2000 cm/s, and (iii) s . (b) Calculate the excess minority carrier concentration at x 0 for (i) s 0, (ii) s 2000 cm/s, and (iii) s . n type s x0 x Figure P6.41 | Figure for Problem 6.41. nea29583_ch06_192-240.indd 238 12/11/10 11:17 AM Problems 239 s0 s0 p type n type s⬁ x0 x W 30 10–4 cm x Figure P6.42 | Figure for Problem 6.42. s(W ) x W 20 10–4 cm x0 x Figure P6.43 | Figure for Problem 6.43. Illumination s0 x W x0 x W s⬁ Figure P6.44 | Figure for Problem 6.44. *6.42 (a) Consider the p-type semiconductor shown in Figure P6.42 with the following parameters: Na 5 1016 cm3, Dn 25 cm2/s, and n0 5 107 s. The surface recombination velocities at the two surfaces are shown. The electric field is zero. The semiconductor is illuminated at x 0 with an excess carrier generation rate equal to g 2 1021 cm3-s 1. Determine the excess minority carrier electron concentration versus x in steady state. (b) Repeat part (a) for n0 . *6.43 Consider the n-type semiconductor shown in Figure P6.43. Assume that Dp 10 cm2/s and p0 . The electric field is zero. Assume that a flux of excess electrons and holes is incident at x 0. Let the flux of each carrier type be 1019 carriers/cm2-s. Determine the minority carrier hole current versus x if the surface recombination velocity is (a) s(W ) and (b) s(W ) 2000 cm/s. *6.44 A p-type semiconductor is shown in Figure P6.44. The surface recombination velocities are shown. The semiconductor is uniformly illuminated for W x 0 producing a constant excess carrier generation rate G0. Determine the steady-state excess carrier concentration versus x if the minority carrier lifetime is infinite and if the electric field is zero. 6.45 Plot p(x) versus x for various values of s using Equation (6.113). Choose reasonable parameter values. Summary and Review *6.46 Consider an n-type semiconductor as shown in Figure P6.41. The material is doped at Nd 3 1016 cm3 and Na 0. Assume that Dp 12 cm2/s and p0 2 107 s. The electric field is zero. “Design” the surface recombination velocity so that the minority carrier diffusion current density at the surface is no greater than Jp 0.18 A/cm2 with a uniform excess carrier generation rate equal to g 3 10 21 cm3-s1. 6.47 Consider a semiconductor with excess carriers present. From the definition of carrier lifetimes and recombination rates, determine the average time that an electron nea29583_ch06_192-240.indd 239 12/11/10 11:17 AM 240 CHAPTER 6 Nonequilibrium Excess Carriers in Semiconductors stays in the conduction band and the average time that a hole stays in the valence band. Discuss these relations for (a) an intrinsic semiconductor and (b) an n-type semiconductor. *6.48 (a) Design a GaAs photoconductor that is 4 m thick. Assume that the material is doped at Nd 1016 cm3 and has lifetime values of n 0 107 s and p 0 5 108 s. With an excitation of g 1021 cm3 s1, a photocurrent of at least 2 A is required with an applied voltage of 2 V. (b) Repeat the design for a silicon photoconductor that has the same parameters as given in part (a). READING LIST 1. *2. 3. 4. 5. *6. 7. 8. 9. 10. 11. 12. 13. 14. *15. 16. Bube, R. H. Photoelectronic Properties of Semiconductors, New York: Cambridge University Press, 1992. deCogan, D. Solid State Devices: A Quantum Physics Approach. New York: SpringerVerlag, 1987. Dimitrijev, S. Principles of Semiconductor Devices. New York: Oxford University Press, 2006. Hall, R. H. “Electron–Hole Recombination.” Physical Review 87, no. 2 (July 15, 1952), p. 387. Haynes, J. R., and W. Shockley. “The Mobility and Life of Injected Holes and Electrons in Germanium.” Physical Review 81, no. 5 (March 1, 1951), pp. 835–843. Hess, K. Advanced Theory of Semiconductor Devices. Englewood Cliffs, NJ: Prentice Hall, 1988. Kano, K. Semiconductor Devices. Upper Saddle River, NJ: Prentice Hall, 1998. Kingston, R. H. Semiconductor Surface Physics. Philadelphia, PA: University of Pennsylvania Press, 1957. McKelvey, J. P. Solid State Physics for Engineering and Materials Science. Malabar, FL: Krieger Publishing, 1993. Pierret, R. F. Semiconductor Device Fundamentals. Reading, MA: Addison-Wesley, 1996. Shockley, W., and W. T. Read, Jr. “Statistics of the Recombinations of Holes and Electrons.” Physical Review 87, no. 5 (September 1, 1952), pp. 835–842. Singh, J. Semiconductor Devices: An Introduction. New York: McGraw-Hill, 1994. Singh, J. Semiconductor Devices: Basic Principles. New York: John Wiley and Sons, 2001. Streetman, B. G., and S. K. Banerjee. Solid State Electronic Devices, 6th ed. Upper Saddle River, NJ: Pearson Prentice Hall, 2006. Wang, S. Fundamentals of Semiconductor Theory and Device Physics. Englewood Cliffs, NJ: Prentice Hall, 1989. Wolfe, C. M., N. Holonyak, Jr., and G. E. Stillman. Physical Properties of Semiconductors. Englewood Cliffs, NJ: Prentice Hall, 1989. *Indicates references that are at an advanced level compared to this text. nea29583_ch06_192-240.indd 240 12/11/10 11:17 AM C 7 H A P T E R The pn Junction U p to this point in the text, we have been considering the properties of the semiconductor material. We calculated electron and hole concentrations in thermal equilibrium and determined the position of the Fermi level. We then considered the nonequilibrium condition in which excess electrons and holes are present in the semiconductor. We now wish to consider the situation in which a p-type and an n-type semiconductor are brought into contact with one another to form a pn junction. Most semiconductor devices contain at least one junction between p-type and n-type semiconductor regions. Semiconductor device characteristics and operation are intimately connected to these pn junctions, so considerable attention is devoted initially to this basic device. The electrostatics of the zero-biased and reverse-biased pn junction is considered in this chapter. The current–voltage characteristics of the pn junction diode are developed in the next chapter. ■ 7.0 | PREVIEW In this chapter, we will: ■ Consider a uniformly doped pn junction, in which one region of the semiconductor is uniformly doped with acceptor atoms and the adjacent region is uniformly doped with donor atoms. ■ Determine the energy-band diagram of a pn junction in thermal equilibrium. ■ Discuss the creation of a space charge region between the p and n regions. ■ Apply Poisson’s equation to determine the electric field in the space charge region and calculate the built-in potential barrier. ■ Analyze the changes that occur in the pn junction when a reverse-biased voltage is applied. Derive expressions for space charge width and depletion capacitance. ■ Analyze the voltage breakdown characteristics of a pn junction. ■ Consider the properties of a nonuniformly doped pn junction. Specific doping profiles can lead to desirable properties of the pn junction. 241 nea29583_ch07_241-275.indd 241 12/11/10 11:32 AM 242 CHAPTER 7 The pn Junction 7.1 | BASIC STRUCTURE OF THE pn JUNCTION Figure 7.1a schematically shows the pn junction. It is important to realize that the entire semiconductor is a single-crystal material in which one region is doped with acceptor impurity atoms to form the p region and the adjacent region is doped with donor atoms to form the n region. The interface separating the n and p regions is referred to as the metallurgical junction. The impurity doping concentrations in the p and n regions are shown in Figure 7.1b. For simplicity, we will consider a step junction in which the doping concentration is uniform in each region and there is an abrupt change in doping at the junction. Initially, at the metallurgical junction, there is a very large density gradient in both electron and hole concentrations. Majority carrier electrons in the n region will begin diffusing into the p region, and majority carrier holes in the p region will begin diffusing into the n region. If we assume there are no external connections to the semiconductor, then this diffusion process cannot continue indefinitely. As electrons diffuse from the n region, positively charged donor atoms are left behind. Similarly, as holes diffuse from the p region, they uncover negatively charged acceptor atoms. The net positive and negative charges in the n and p regions induce an electric field in the region near the metallurgical junction, in the direction from the positive to the negative charge, or from the n to the p region. The net positively and negatively charged regions are shown in Figure 7.2. These two regions are referred to as the space charge region. Essentially all electrons and holes are swept out of the space charge region by the electric field. Since the space charge region is depleted of any mobile charge, this region is also referred to as the p Na negative charge n Metallurgical junction p (a) ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ Nd positive charge ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ n Space charge region Na E-field Nd Hole diffusion Electron diffusion x0 (b) Figure 7.1 | (a) Simplified geometry of a pn junction; (b) doping profile of an ideal uniformly doped pn junction. nea29583_ch07_241-275.indd 242 “Diffusion force” on holes “Diffusion force” on electrons E-field force on holes E-field force on electrons Figure 7.2 | The space charge region, the electric field, and the forces acting on the charged carriers. 12/11/10 11:32 AM 7.2 Zero Applied Bias 243 depletion region; these two terms will be used interchangeably. Density gradients still exist in the majority carrier concentrations at each edge of the space charge region. We can think of a density gradient as producing a “diffusion force” that acts on the majority carriers. These diffusion forces, acting on the electrons and holes at the edges of the space charge region, are shown in the figure. The electric field in the space charge region produces another force on the electrons and holes, which is in the opposite direction to the diffusion force for each type of particle. In thermal equilibrium, the diffusion force and the E-field force exactly balance each other. 7.2 | ZERO APPLIED BIAS We have considered the basic pn junction structure and discussed briefly how the space charge region is formed. In this section we will examine the properties of the step junction in thermal equilibrium, where no currents exist and no external excitation is applied. We will determine the space charge region width, electric field, and potential through the depletion region. The analysis in this chapter is based on two assumptions that we have considered in previous chapters. The first assumption is that the Boltzmann approximation is valid, which means that each semiconductor region is nondegenerately doped. The second assumption is that complete ionization exists, which means that the temperature of the pn junction is not “too low.” 7.2.1 Built-in Potential Barrier If we assume that no voltage is applied across the pn junction, then the junction is in thermal equilibrium—the Fermi energy level is constant throughout the entire system. Figure 7.3 shows the energy-band diagram for the pn junction in thermal equilibrium. The conduction and valance band energies must bend as we go through the space charge region, since the relative position of the conduction and valence bands with respect to the Fermi energy changes between p and n regions. p n Ec eVbi EFi eFp EF Ev EF eFn EFi Figure 7.3 | Energy-band diagram of a pn junction in thermal equilibrium. nea29583_ch07_241-275.indd 243 12/11/10 11:32 AM 244 CHAPTER 7 The pn Junction Electrons in the conduction band of the n region see a potential barrier in trying to move into the conduction band of the p region. This potential barrier is referred to as the built-in potential barrier and is denoted by Vbi. The built-in potential barrier maintains equilibrium between majority carrier electrons in the n region and minority carrier electrons in the p region, and also between majority carrier holes in the p region and minority carrier holes in the n region. This potential difference across the junction cannot be measured with a voltmeter because new potential barriers will be formed between the probes and the semiconductor that will cancel Vbi. The potential Vbi maintains equilibrium, so no current is produced by this voltage. The intrinsic Fermi level is equidistant from the conduction band edge through the junction; thus, the built-in potential barrier can be determined as the difference between the intrinsic Fermi levels in the p and n regions. We can define the potentials Fn and Fp as shown in Figure 7.3, so we have Vbi Fn Fp (7.1) In the n region, the electron concentration in the conduction band is given by (Ec EF) n0 Nc exp __ kT (7.2) which can also be written in the form EF EFi n0 ni exp __ kT (7.3) where ni and EFi are the intrinsic carrier concentration and the intrinsic Fermi energy, respectively. We may define the potential Fn in the n region as eFn EFi EF (7.4) Equation (7.3) may then be written as (eFn) n0 ni exp __ kT (7.5) Taking the natural log of both sides of Equation (7.5), setting n0 Nd, and solving for the potential, we obtain Nd kT ln _ Fn _ e ni (7.6) Similarly, in the p region, the hole concentration is given by EFi EF p0 Na ni exp __ kT (7.7) where Na is the acceptor concentration. We can define the potential Fp in the p region as eFp EFi EF (7.8) nea29583_ch07_241-275.indd 244 12/11/10 11:32 AM 7.2 Zero Applied Bias 245 Combining Equations (7.7) and (7.8), we find that Na kT ln _ Fp _ e ni (7.9) Finally, the built-in potential barrier for the step junction is found by substituting Equations (7.6) and (7.9) into Equation (7.1), which yields NaNd NaNd kT ln _ Vbi _ Vt ln _ e n2i n2i (7.10) where Vt kT/e and is defined as the thermal voltage. At this time, we should note a subtle but important point concerning notation. Previously in the discussion of a semiconductor material, Nd and Na denoted donor and acceptor impurity concentrations in the same region, thereby forming a compensated semiconductor. From this point on in the text, Nd and Na will denote the net donor and acceptor concentrations in the individual n and p regions, respectively. If the p region, for example, is a compensated material, then Na will represent the difference between the actual acceptor and donor impurity concentrations. The parameter Nd is defined in a similar manner for the n region. Objective: Calculate the built-in potential barrier in a pn junction. EXAMPLE 7.1 Consider a silicon pn junction at T 300 K with doping concentrations of Na 2 1017 cm3 and Nd 1015 cm3. ■ Solution The built-in potential barrier is determined from Equation (7.10) as (2 1017)(1015) Na Nd (0.0259) ln ___ 0.713 V Vbi Vt ln _ 2 (1.5 1010)2 ni If we change the doping concentration in the p region of the pn junction such that the doping concentrations become Na 1016 cm3 and Nd 1015 cm3, then the built-in potential barrier becomes Vbi 0.635 V. ■ Comment The built-in potential barrier changes only slightly as the doping concentrations change by orders of magnitude because of the logarithmic dependence. ■ EXERCISE PROBLEM Ex 7.1 (a) Calculate the built-in potential barrier in a silicon pn junction at T 300 K for (i) Na 5 1015 cm3, Nd 1017 cm3 and (ii) Na 2 1016 cm3, Nd 2 1015 cm3. (b) Repeat part (a) for a GaAs pn junction. [Ans. (a) (i) 0.736 V, (ii) 0.671 V; (b) (i) 1.20 V, (ii) 1.14 V] nea29583_ch07_241-275.indd 245 12/11/10 11:32 AM 246 CHAPTER 7 The pn Junction (C/cm3) p n ⴙeNd ⴙ ⴚxp ⴙxn ⴚ ⴚeNa Figure 7.4 | The space charge density in a uniformly doped pn junction assuming the abrupt junction approximation. 7.2.2 Electric Field An electric field is created in the depletion region by the separation of positive and negative space charge densities. Figure 7.4 shows the volume charge density distribution in the pn junction assuming uniform doping and assuming an abrupt junction approximation. We will assume that the space charge region abruptly ends in the n region at x xn and abruptly ends in the p region at x xp (xp is a positive quantity). The electric field is determined from Poisson’s equation, which, for a onedimensional analysis, is (x) d (x) __ d E(x) __ _ 2 dx2 s dx (7.11) where (x) is the electric potential, E(x) is the electric field, (x) is the volume charge density, and s is the permittivity of the semiconductor. From Figure 7.4, the charge densities are (x) eNa xp x 0 (7.12a) 0 x xn (7.12b) and (x) eNd The electric field in the p region is found by integrating Equation (7.11). We have (x) eNa eNa _ _ E _ dx (7.13) s s dx s x C1 where C1 is a constant of integration. The electric field is assumed to be zero in the neutral p region for x xp since the currents are zero in thermal equilibrium. Since there are no surface charge densities within the pn junction structure, the electric nea29583_ch07_241-275.indd 246 12/11/10 11:32 AM 7.2 Zero Applied Bias 247 field is a continuous function. The constant of integration is determined by setting E 0 at x xp. The electric field in the p region is then given by eNa E_ s (x xp) xp x 0 In the n region, the electric field is determined from (eNd) eNd _ E _ s dx s x C2 (7.14) (7.15) where C2 is again a constant of integration and is determined by setting E 0 at x xn, since the E-field is assumed to be zero in the n region and is a continuous function. Then eNd E_ 0 x xn (7.16) s (xn x) The electric field is also continuous at the metallurgical junction, or at x 0. Setting Equations (7.14) and (7.16) equal to each other at x 0 gives Na xp Nd xn (7.17) Equation (7.17) states that the number of negative charges per unit area in the p region is equal to the number of positive charges per unit area in the n region. Figure 7.5 is a plot of the electric field in the depletion region. The electric field direction is from the n to the p region, or in the negative x direction for this geometry. For the uniformly doped pn junction, the E-field is a linear function of distance through the junction, and the maximum (magnitude) electric field occurs at the metallurgical junction. An electric field exists in the depletion region even when no voltage is applied between the p and n regions. The potential in the junction is found by integrating the electric field. In the p region then, we have eNa (x) E(x)dx _ (7.18) s (x xp) dx p ⴚxp E xⴝ0 n ⴙxn Figure 7.5 | Electric field in the space charge region of a uniformly doped pn junction. nea29583_ch07_241-275.indd 247 12/11/10 11:32 AM 248 CHAPTER 7 The pn Junction or eNa _ x2 (x) _ s 2 xp · x C1 (7.19) where C1 is again a constant of integration. The potential difference through the pn junction is the important parameter, rather than the absolute potential, so we may arbitrarily set the potential equal to zero at x xp . The constant of integration is then found as eN C1 _a x 2p 2s (7.20) so that the potential in the p region can now be written as eN (x) _a (x xp)2 (xp x 0) (7.21) 2s The potential in the n region is determined by integrating the electric field in the n region, or eNd (x) _ (7.22) s (xn x)dx Then eNd x2 _ (x) _ s xn · x 2 C2 (7.23) where C2 is another constant of integration. The potential is a continuous function, so setting Equation (7.21) equal to Equation (7.23) at the metallurgical junction, or at x 0, gives eN C2 _a x2p 2s (7.24) The potential in the n region can thus be written as eNd eNa 2 x2 _ _ (x) _ s xn · x 2 2s xp (0 x xn) (7.25) Figure 7.6 is a plot of the potential through the junction and shows the quadratic dependence on distance. The magnitude of the potential at x xn is equal to the builtin potential barrier. Then from Equation (7.25), we have e N x 2 N x2 Vbi (x xn) _ a p 2s d n (7.26) The potential energy of an electron is given by E e, which means that the electron potential energy also varies as a quadratic function of distance through the space charge region. The quadratic dependence on distance was shown in the energyband diagram of Figure 7.3, although we did not explicitly know the shape of the curve at that time. nea29583_ch07_241-275.indd 248 12/11/10 11:32 AM 7.2 Zero Applied Bias 249 p n Vbi xp xn x0 Figure 7.6 | Electric potential through the space charge region of a uniformly doped pn junction. 7.2.3 Space Charge Width We can determine the distance that the space charge region extends into the p and n regions from the metallurgical junction. This distance is known as the space charge width. From Equation (7.17), we may write, for example, Nd xn xp _ Na (7.27) Then, substituting Equation (7.27) into Equation (7.26) and solving for xn, we obtain Na __ 1 2sVbi _ xn _ Nd Na Nd e 1 2 (7.28) Equation (7.28) gives the space charge width, or the width of the depletion region, xn extending into the n-type region for the case of zero applied voltage. Similarly, if we solve for xn from Equation (7.17) and substitute into Equation (7.26), we find Nd __ 1 2sVbi _ xp _ Na Na Nd e 1 2 (7.29) where xp is the width of the depletion region extending into the p region for the case of zero applied voltage. The total depletion or space charge width W is the sum of the two components, or W xn xp (7.30) Using Equations (7.28) and (7.29), we obtain 2sVbi __ Na Nd W _ e NaNd nea29583_ch07_241-275.indd 249 1 2 (7.31) 12/11/10 11:32 AM 250 CHAPTER 7 The pn Junction The built-in potential barrier can be determined from Equation (7.10), and then the total space charge region width is obtained using Equation (7.31). EXAMPLE 7.2 Objective: Calculate the space charge width and electric field in a pn junction for zero bias. Consider a silicon pn junction at T 300 K with doping concentrations of Na 1016 cm3 and Nd 1015 cm3. ■ Solution In Example 7.1, we determined the built-in potential barrier as Vbi 0.635 V. From Equation (7.31), the space charge width is 2sVbi __ Na Nd W _ e Na Nd 1 2 2(11.7)(8.85 1014)(0.635) __ 1016 1015 _____ 1.6 1019 (1016)(1015) 1 2 0.951 104 cm 0.951 m Using Equations (7.28) and (7.29), we can find xn 0.8644 m, and xp 0.0864 m. The peak electric field at the metallurgical junction, using Equation (7.16) for example, is (1.6 1019)(1015)(0.8644 104) eNd xn ______ Emax _ 1.34 104 V/cm s (11.7)(8.85 1014) ■ Comment The peak electric field in the space charge region of a pn junction is quite large. We must keep in mind, however, that there is no mobile charge in this region; hence there will be no drift current. We may also note, from this example, that the width of each space charge region is a reciprocal function of the doping concentration: The depletion region will extend further into the lower-doped region. ■ EXERCISE PROBLEM Ex 7.2 A silicon pn junction at T 300 K with zero applied bias has doping concentrations of Nd 5 1016 cm3 and Na 5 1015 cm3. Determine xn, xp, W, and Emax. (Ans. xn 4.11 106 cm, xp 4.11 105 cm, W 4.52 105 cm, Emax 3.18 104 V/cm) TEST YOUR UNDERSTANDING TYU 7.2 nea29583_ch07_241-275.indd 250 Calculate Vbi, xn, xp, W, and Emax for a silicon pn junction at zero bias and T 300 K for doping concentrations of (a) Na 2 1017 cm3, Nd 1016 cm3 and (b) Na 4 1015 cm3, Nd 3 1016 cm3. (Ans. Vbi 1.186 V, xn 0.05590 m, xp 0.5590 m, W 0.6149 m, Emax 3.86 104 V/cm) [Ans. (a) Vbi 0.772 V, xn 0.3085 m, xp 0.0154 m, W 0.3240 m, Emax 4.77 104 V/cm; (b) Vbi 0.699 V, xn 0.0596 m, xp 0.4469 m, W 0.5064 m, Emax 2.76 104 V/cm] TYU 7.1 Repeat Exercise Problem Ex 7.2 for a GaAs pn junction. 12/11/10 11:32 AM 7.3 Reverse Applied Bias 251 7.3 | REVERSE APPLIED BIAS If we apply a potential between the p and n regions, we will no longer be in an equilibrium condition—the Fermi energy level will no longer be constant through the system. Figure 7.7 shows the energy-band diagram of the pn junction for the case when a positive voltage is applied to the n region with respect to the p region. As the positive potential is downward, the Fermi level on the n side is below the Fermi level on the p side. The difference between the two is equal to the applied voltage in units of energy. The total potential barrier, indicated by Vtotal, has increased. The applied potential is the reverse-biased condition. The total potential barrier is now given by Vtotal Fn Fp VR (7.32) where VR is the magnitude of the applied reverse-biased voltage. Equation (7.32) can be rewritten as Vtotal Vbi VR (7.33) where Vbi is the same built-in potential barrier we had defined in thermal equilibrium. 7.3.1 Space Charge Width and Electric Field Figure 7.8 shows a pn junction with an applied reverse-biased voltage VR. Also indicated in the figure are the electric field in the space charge region and the electric field Eapp , induced by the applied voltage. The electric fields in the neutral p and n regions are essentially zero, or at least very small, which means that the magnitude of the electric field in the space charge region must increase above the thermal-equilibrium value due to the applied voltage. The electric field originates on positive charge and terminates on negative charge; this means that the number of positive and negative p n Ec EFi eVtotal eFp EFp Ev eVR Ec eFn EFn EFi Ev Figure 7.7 | Energy-band diagram of a pn junction under reverse bias. nea29583_ch07_241-275.indd 251 12/11/10 11:32 AM 252 CHAPTER 7 The pn Junction Eapp ⴚE ⴚ ⴚ ⴚ ⴚ p ⴚ ⴚ ⴚ ⴚ ⴚ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ n W VR Figure 7.8 | A pn junction, with an applied reverse-biased voltage, showing the directions of the electric field induced by VR and the space charge electric field. charges must increase if the electric field increases. For given impurity doping concentrations, the number of positive and negative charges in the depletion region can be increased only if the space charge width W increases. The space charge width W increases, therefore, with an increasing reverse-biased voltage VR. We are assuming that the electric field in the bulk n and p regions is zero. This assumption will become clearer in the next chapter when we discuss the current–voltage characteristics. In all of the previous equations, the built-in potential barrier can be replaced by the total potential barrier. The total space charge width can be written from Equation (7.31) as Na Nd 2s(Vbi VR) __ W ___ Na Nd e 1 2 (7.34) showing that the total space charge width increases as we apply a reverse-biased voltage. By substituting the total potential barrier Vtotal into Equations (7.28) and (7.29), the space charge widths in the n and p regions, respectively, can be found as a function of applied reverse-biased voltage. EXAMPLE 7.3 Objective: Calculate the width of the space charge region in a pn junction when a reversebiased voltage is applied. Again consider a silicon pn junction at T 300 K with doping concentrations of Na 1016 cm3 and Nd 1015 cm3. Assume that ni 1.5 1010 cm3 and VR 5 V. ■ Solution The built-in potential barrier was calculated in Example 7.1 for this case and is Vbi 0.635 V. The space charge width is determined from Equation (7.34). We have 1016 1015 2(11.7)(8.85 1014)(0.635 5) __ W ______ 19 (1016)(1015) 1.6 10 1 2 so that W 2.83 104 cm 2.83 m nea29583_ch07_241-275.indd 252 12/11/10 11:32 AM 7.3 Reverse Applied Bias 253 ■ Comment The space charge width has increased from 0.951 m at zero bias to 2.83 m at a reverse bias of 5 V. ■ EXERCISE PROBLEM Ex 7.3 (a) A silicon pn junction at T 300 K has doping concentrations of Na 5 1015 cm3 and Nd 5 1016 cm3. A reverse-biased voltage of VR 4 V is applied. Determine Vbi, xn, xp, and W. (b) Repeat part (a) for VR 8 V. [Ans. (a) Vbi 0.718 V, xn 0.1054 m, xp 1.054 m, W 1.159 m; (b) Vbi 0.718, xn 0.1432 m, xp 1.432 m, W 1.576 m] The magnitude of the electric field in the depletion region increases with an applied reverse-biased voltage. The electric field is still given by Equations (7.14) and (7.16) and is still a linear function of distance through the space charge region. Since xn and xp increase with reverse-biased voltage, the magnitude of the electric field also increases. The maximum electric field still occurs at the metallurgical junction. The maximum electric field at the metallurgical junction, from Equations (7.14) and (7.16), is eNaxp eNd xn __ Emax __ s s (7.35) If we use either Equation (7.28) or (7.29) in conjunction with the total potential barrier, Vbi VR, then 2e(Vbi VR) __ Na Nd Emax ___ s Na Nd 1 2 (7.36) We can show that the maximum electric field in the pn junction can also be written as 2(Vbi VR) Emax ___ W (7.37) where W is the total space charge width. Objective: Design a pn junction to meet maximum electric field and voltage specifications. Consider a silicon pn junction at T 300 K with a p-type doping concentration of Na 2 1017 cm3. Determine the n-type doping concentration such that the maximum electric field is Emax 2.5 105 V/cm at a reverse-biased voltage of VR 25 V. DESIGN EXAMPLE 7.4 ■ Solution The maximum electric field is given by Equation (7.36). Neglecting Vbi compared to VR, we can write Emax nea29583_ch07_241-275.indd 253 2eV NNNN a d R __ _ s a 1 2 d 12/11/10 11:32 AM 254 CHAPTER 7 The pn Junction or 2(1.6 1019 )(25) ___ (2 1017 )Nd 2.5 105 ____ 14 (11.7)(8.85 10 ) 2 1017 Nd 1 2 which yields Nd 8.43 1015 cm3 ■ Conclusion A smaller value of Nd results in a smaller value of Emax for a given reverse-biased voltage. The value of Nd determined in this example, then, is the maximum value that will meet the specifications. ■ EXERCISE PROBLEM Ex 7.4 The maximum electric field in a reverse-biased GaAs pn junction at T 300 K is to be limited to Emax 7.2 104 V/cm. The doping concentrations are Nd 5 1015 cm3 and Na 3 1016 cm3. Determine the maximum reverse-biased voltage that can be applied. 7.3.2 Junction Capacitance (Ans. VR 3.21 V) Since we have a separation of positive and negative charges in the depletion region, a capacitance is associated with the pn junction. Figure 7.9 shows the charge densities in the depletion region for applied reverse-biased voltages of VR and VR dVR. An increase p n dQ ⴙeNd ⴙ dxp ⴚxp ⴙxn ⴚdQ dxn ⴚ ⴚeNa With applied VR With applied VR dVR Figure 7.9 | Differential change in the space charge width with a differential change in reverse-biased voltage for a uniformly doped pn junction. nea29583_ch07_241-275.indd 254 12/11/10 11:32 AM 7.3 Reverse Applied Bias 255 in the reverse-biased voltage dVR will uncover additional positive charges in the n region and additional negative charges in the p region. The junction capacitance is defined as dQ (7.38) C _ dVR where dQ eNd dxn eNa dxp (7.39) The differential charge dQ is in units of C/cm2 so that the capacitance C is in units of farads per square centimeter F/cm2), or capacitance per unit area. For the total potential barrier, Equation (7.28) may be written as 2s(Vbi VR) _ Na __ 1 xn ___ e Nd Na Nd 1 2 (7.40) The junction capacitance can be written as dQ dx C _ eNd _n dVR dVR (7.41) so that esNaNd C ____ 2(Vbi VR)(Na Nd) 1 2 (7.42) Exactly the same capacitance expression is obtained by considering the space charge region extending into the p region xp. The junction capacitance is also referred to as the depletion layer capacitance. Objective: Calculate the junction capacitance of a pn junction. EXAMPLE 7.5 Consider the same pn junction as that in Example 7.3. Again assume that VR 5 V. ■ Solution The junction capacitance is found from Equation (7.42) as (1.6 1019)(11.7)(8.85 1014)(1016)(1015) C ________ 2(0.635 5)(1016 1015) 1 2 or C 3.66 109 F/cm2 If the cross-sectional area of the pn junction is, for example, A 104 cm2, then the total junction capacitance is C C ⴢ A 0.366 1012 F 0.366 pF ■ Comment The value of junction capacitance is usually in the pF, or smaller, range. nea29583_ch07_241-275.indd 255 12/11/10 11:32 AM 256 CHAPTER 7 The pn Junction ■ EXERCISE PROBLEM Ex 7.5 Consider a GaAs pn junction at T 300 K doped to Na 5 1015 cm3 and Nd 2 1016 cm3. (a) Calculate Vbi. (b) Determine the junction capacitance C for VR 4 V. (c) Repeat part (b) for VR 8 V. [Ans. (a) Vbi 1.16 V; (b) C 8.48 109 F/cm2; (c) C 6.36 109 F/cm2 ] If we compare Equation (7.34) for the total depletion width W of the space charge region under reverse bias and Equation (7.42) for the junction capacitance C , we find that we can write (7.43) C _s W Equation (7.43) is the same as the capacitance per unit area of a parallel plate capacitor. Considering Figure 7.9, we may have come to this same conclusion earlier. Keep in mind that the space charge width is a function of the reverse-biased voltage so that the junction capacitance is also a function of the reverse-biased voltage applied to the pn junction. 7.3.3 One-Sided Junctions Consider a special pn junction called the one-sided junction. If, for example, Na Nd, this junction is referred to as a pn junction. The total space charge width, from Equation (7.34), reduces to W 2 (VeN V ) s bi R ___ 1 2 (7.44) d Considering the expressions for xn and xp, we have for the pn junction xp xn (7.45) W (7.46) and xn Almost the entire space charge layer extends into the low-doped region of the junction. This effect can be seen in Figure 7.10. The junction capacitance of the pn junction reduces to C 2(Ve N V ) s d __ bi 1 2 (7.47) R The depletion layer capacitance of a one-sided junction is a function of the doping concentration in the low-doped region. Equation (7.47) may be manipulated to give 2(V V ) 1 __ _ e N C 2 bi R s (7.48) d which shows that the inverse capacitance squared is a linear function of applied reverse-biased voltage. nea29583_ch07_241-275.indd 256 12/11/10 11:32 AM 7.3 Reverse Applied Bias 257 p n ⴙeNd ⴙ ⴚxp 1 2 C ⴙxn ⴚ Slope ⴚeNa Vbi 0 2 es Nd VR Figure 7.11 | (1/C )2 versus VR of a uniformly doped pn junction. Figure 7.10 | Space charge density of a one-sided pn junction. Figure 7.11 shows a plot of Equation (7.48). The built-in potential of the junction can be determined by extrapolating the curve to the point where (1/C )2 0. The slope of the curve is inversely proportional to the doping concentration of the low-doped region in the junction; thus, this doping concentration can be experimentally determined. The assumptions used in the derivation of this capacitance include uniform doping in both semiconductor regions, the abrupt junction approximation, and a planar junction. Determine the impurity doping concentrations in a pn junction given the parameters from Figure 7.11. Assume that the intercept and the slope of the curve in Figure 7.11 are Vbi 0.725 V and 6.15 1015 (F/cm2 )2 (V)1, respectively, for a silicon pn junction at T 300 K. Objective: EXAMPLE 7.6 ■ Solution The slope of the curve in Figure 7.11 is given by 2/e s Nd, so we may write 1 2 _ 2 ________ Nd _ e s ⴢ slope (1.6 1019)(11.7)(8.85 1014)(6.15 1015) or Nd 1.96 1015 cm3 From the expression for Vbi, which is Na Nd Vbi Vt ln _ n 2i we can solve for Na as n2 1.5 1010 2 Vbi 0.725 Na _i exp _ ___ exp __ Nd Vt 0.0259 1.963 1015 nea29583_ch07_241-275.indd 257 12/11/10 11:32 AM 258 CHAPTER 7 The pn Junction which yields Na 1.64 1017 cm3 ■ Comment The results of this example show that Na Nd; therefore the assumption of a one-sided junction was valid. ■ EXERCISE PROBLEM Ex 7.6 The experimentally measured junction capacitance of a one-sided silicon np junction biased at VR 3 V and at T 300 K is C 0.105 pF. The built-in potential barrier is found to be Vbi 0.765 V. The cross-sectional area is A 105 cm2. Find the doping concentrations. (Ans. Na 5.01 1015 cm3, Nd 3.02 1017 cm3) A one-sided pn junction is useful for experimentally determining the doping concentrations and built-in potential. TEST YOUR UNDERSTANDING TYU 7.3 (a) A silicon pn junction at T 300 K is reverse biased at VR 8 V. The doping concentrations are Na 5 1016 cm3 and Nd 5 1015 cm3. Determine xn, xp, W, and Emax. (b) Repeat part (a) for a reverse-biased voltage of VR 12 V. TYU 7.4 A silicon pn junction at T 300 K has doping concentrations of Nd 3 1016 cm3 and Na 8 1015 cm3, and has a cross-sectional area of A 5 105 cm2. Determine the junction capacitance at (a) VR 2 V and (b) VR 5 V. [Ans. (a) xn 1.43 104 cm, xp 1.43 105 cm, W 1.57 104 cm, Emax 1.11 105 V/cm; (b) xn 1.73 104 cm, xp 1.73 105 cm, W 1.90 104 cm, Emax 1.34 105 V/cm] [Ans. (a) 0.694 pF; (b) 0.478 pF] 7.4 | JUNCTION BREAKDOWN In the last section, we determined the effects of applying a reverse-biased voltage across the pn junction. However, the reverse-biased voltage may not increase without limit; at some particular voltage, the reverse-biased current will increase rapidly. The applied voltage at this point is called the breakdown voltage. Two physical mechanisms give rise to the reverse-biased breakdown in a pn junction: the Zener effect and the avalanche effect. Zener breakdown occurs in highly doped pn junctions through a tunneling mechanism. In a highly doped junction, the conduction and valence bands on opposite sides of the junction are sufficiently close during reverse bias that electrons may tunnel directly from the valence band on the p side into the conduction band on the n side. This tunneling process is schematically shown in Figure 7.12a. The avalanche breakdown process occurs when electrons and/or holes, moving across the space charge region, acquire sufficient energy from the electric field to create electron–hole pairs by colliding with atomic electrons within the depletion region. The avalanche process is schematically shown in Figure 7.12b. The newly nea29583_ch07_241-275.indd 258 12/11/10 11:32 AM 7.4 p region Junction Breakdown 259 n region Ec p Space charge region n EF Ev h E-field e () () Ec EF Ev () () () np Diffusion of electrons () () pn Diffusion of holes (b) (a) Figure 7.12 | (a) Zener breakdown mechanism in a reverse-biased pn junction; (b) avalanche breakdown process in a reverse-biased pn junction. p Space charge region n Ip0 I Ip(x) In(W ) In0 x0 In(x) xW Figure 7.13 | Electron and hole current components through the space charge region during avalanche multiplication. created electrons and holes move in opposite directions due to the electric field and thereby create a reverse-biased current. In addition, the newly generated electrons and/or holes may acquire sufficient energy to ionize other atoms, leading to the avalanche process. For most pn junctions, the predominant breakdown mechanism will be the avalanche effect. If we assume that a reverse-biased electron current In0 enters the depletion region at x 0 as shown in Figure 7.13, the electron current In will increase with distance through the depletion region due to the avalanche process. At x W, the electron current may be written as In (W ) Mn In0 (7.49) nea29583_ch07_241-275.indd 259 12/11/10 11:32 AM 260 CHAPTER 7 The pn Junction where Mn is a multiplication factor. The hole current is increasing through the depletion region from the n to p region and reaches a maximum value at x 0. The total current is constant through the pn junction in steady state. We can write an expression for the incremental electron current at some point x as dIn(x) In(x)n dx Ip(x)p dx (7.50) where n and p are the electron and hole ionization rates, respectively. The ionization rates are the number of electron–hole pairs generated per unit length by an electron (n) or by a hole (p). Equation (7.50) may be written as dIn(x) _ In(x)n Ip(x)p (7.51) dx The total current I is given by I In(x) Ip(x) (7.52) which is a constant. Solving for Ip(x) from Equation (7.52) and substituting into Equation (7.51), we obtain dIn(x) _ (p n)In(x) pI (7.53) dx If we make the assumption that the electron and hole ionization rates are equal so that n p (7.54) then Equation (7.53) may be simplified and integrated through the space charge region. We will obtain W In(W) In(0) I dx (7.55) 0 Using Equation (7.49), Equation (7.55) may be written as Mn In0 In(0) W ___ dx I (7.56) 0 Since Mn In0 I and since In(0) In0, Equation (7.56) becomes 1 W dx 1_ Mn (7.57) 0 The avalanche breakdown voltage is defined to be the voltage at which Mn approaches infinity. The avalanche breakdown condition is then given by W dx 1 (7.58) 0 The ionization rates are strong functions of electric field and, since the electric field is not constant through the space charge region, Equation (7.58) is not easy to evaluate. If we consider, for example, a one-sided pn junction, the maximum electric field is given by eNd xn Emax __ (7.59) s nea29583_ch07_241-275.indd 260 12/11/10 11:32 AM Critical field at breakdown (105 V/cm) 7.4 20 18 16 14 12 10 8 6 4 2 0 1014 Junction Breakdown 261 One-sided abrupt junction at 300 K GaAs Tunneling Avalanche Si 1015 1016 NB 1017 1018 51018 (cm3) Figure 7.14 | Critical electric field at breakdown in a onesided junction as a function of impurity doping concentrations. (From Sze and Ng [14].) The depletion width xn is given approximately as xn 2eV N s R 1 _ ⴢ_ 1 2 (7.60) d where VR is the magnitude of the applied reverse-biased voltage. We have neglected the built-in potential Vbi. If we now define VR to be the breakdown voltage VB, the maximum electric field, Emax, will be defined as a critical electric field, Ecrit, at breakdown. Combining Equations (7.59) and (7.60), we may write s E2crit VB _ 2eNB (7.61) where NB is the semiconductor doping in the low-doped region of the one-sided junction. The critical electric field, plotted in Figure 7.14, is a slight function of doping. We have been considering a uniformly doped planar junction. The breakdown voltage will decrease for a linearly graded junction. (See Section 7.5.) Figure 7.15 shows a plot of the breakdown voltage for a one-sided abrupt junction and a linearly graded junction. If we take into account the curvature of a diffused junction as well, the breakdown voltage will be further degraded. Objective: Design an ideal one-sided np junction diode to meet a breakdown voltage specification. Consider a silicon pn junction diode at T 300 K. Assume that Nd 3 1018 cm3. Design the diode such that the breakdown voltage is VB 100 V. DESIGN EXAMPLE 7.7 ■ Solution From Figure 7.15, we find that the doping concentration in the low-doped side of a one-sided abrupt junction should be approximately 4 1015 cm3 for a breakdown voltage of 100 V. nea29583_ch07_241-275.indd 261 12/11/10 11:32 AM 262 CHAPTER 7 The pn Junction Impurity concentration NB (cm3) 1014 1015 1016 Breakdown voltage VB (V) 1000 GaAs 100 1017 1018 1000 T 300 K One-sided abrupt junction 100 Si Linearly graded junction 10 1 1020 1021 1022 10 1023 1 1024 Impurity gradient a (cm4) Figure 7.15 | Breakdown voltage versus impurity concentration in uniformly doped and linearly graded junctions. (From Sze [14].) For a doping concentration of 4 1015 cm3, the critical electric field, from Figure 7.14, is approximately 3.7 105 V/cm. Then, using Equation (7.61), we find the breakdown voltage as s E2crit ______ (11.7)(8.85 1014)(3.7 105)2 VB _ 110 V 2eNB 2(1.6 1019)(4 1015) which correlates very well with the results from Figure 7.15. ■ Conclusion As Figure 7.15 shows, the breakdown voltage increases as the doping concentration decreases in the low-doped region. ■ EXERCISE PROBLEM A one-sided, planar, uniformly doped silicon pn junction diode is required to have a reverse-biased breakdown voltage of VB 60 V. What is the maximum doping concentration in the low-doped region such that this specification is met? (Ans. NB Ex 7.7 8 1015 cm3) *7.5 | NONUNIFORMLY DOPED JUNCTIONS In the pn junctions considered so far, we have assumed that each semiconductor region has been uniformly doped. In actual pn junction structures, this is rarely true. In some electronic applications, specific nonuniform doping profiles are used to obtain special pn junction capacitance characteristics. nea29583_ch07_241-275.indd 262 12/11/10 11:32 AM 7.5 7.5.1 Nonuniformly Doped Junctions 263 Linearly Graded Junctions If we start with a uniformly doped n-type semiconductor, for example, and diffuse acceptor atoms through the surface, the impurity concentrations will tend to be like those shown in Figure 7.16. The point x x on the figure corresponds to the metallurgical junction. The depletion region extends into the p and n regions from the metallurgical junction as we have discussed previously. The net p-type doping concentration near the metallurgical junction may be approximated as a linear function of distance from the metallurgical junction. Likewise, as a first approximation, the net n-type doping concentration is also a linear function of distance extending into the n region from the metallurgical junction. This effective doping profile is referred to as a linearly graded junction. Figure 7.17 shows the space charge density in the depletion region of the linearly graded junction. For convenience, the metallurgical junction is placed at x 0. The space charge density can be written as (x) eax (7.62) where a is the gradient of the net impurity concentration. The electric field and potential in the space charge region can be determined from Poisson’s equation. We can write (x) _ dE _ eax _ (7.63) s s dx so that the electric field can be found by integration as ea x2 x2 eax dx _ E _ (7.64) 0 s 2s The electric field in the linearly graded junction is a quadratic function of distance rather than the linear function found in the uniformly doped junction. The maximum electric field again occurs at the metallurgical junction. We may note that the electric field is zero at both x x0 and at x x0. The electric field in a nonuniformly Impurity concentration (C/cm3) p region p region n region Na Surface ⴙ x0 Nd ⴚ x0 x0 xx Figure 7.16 | Impurity concentrations of a pn junction with a nonuniformly doped p region. nea29583_ch07_241-275.indd 263 n region Figure 7.17 | Space charge density in a linearly graded pn junction. 12/11/10 11:32 AM 264 CHAPTER 7 The pn Junction doped semiconductor is not exactly zero, but the magnitude of this field is small, so setting E 0 in the bulk regions is still a good approximation. The potential is again found by integrating the electric field as (x) E dx (7.65) If we arbitrarily set 0 at x x0, then the potential through the junction is ea _ x3 x2x _ ea x3 (x) _ 0 2s 3 3s 0 (7.66) The magnitude of the potential at x x0 will equal the built-in potential barrier for this function. We then have that eax30 2·_ Vbi (x0) _ (7.67) 3 s Another expression for the built-in potential barrier for a linearly graded junction can be approximated from the expression used for a uniformly doped junction. We can write Nd (x0)Na(x0) Vbi Vt ln ___ n2i (7.68) where Nd(x0) and Na(x0) are the doping concentrations at the edges of the space charge region. We can relate these doping concentrations to the gradient, so that Nd (x0) ax0 (7.69a) Na(x0) ax0 (7.69b) and Then the built-in potential barrier for the linearly graded junction becomes ax0 Vbi Vt ln _ ni 2 (7.70) There may be situations in which the doping gradient is not the same on either side of the junction, but we will not consider that condition here. If a reverse-biased voltage is applied to the junction, the potential barrier increases. The built-in potential barrier Vbi in the above equations is then replaced by the total potential barrier Vbi VR. Solving for x0 from Equation (7.67) and using the total potential barrier, we obtain s 3·_ x0 _ (V VR) 2 ea bi 1 3 (7.71) The junction capacitance per unit area can be determined by the same method that we used for the uniformly doped junction. Figure 7.18 shows the differential charge nea29583_ch07_241-275.indd 264 12/11/10 11:32 AM 7.5 (C/cm3) Nonuniformly Doped Junctions 265 dQ (x0) dx0 eax0 dx0 dx0 ⴙ x0 x0 x0 ⴚ dx0 dQ Figure 7.18 | Differential change in space charge width with a differential change in reverse-biased voltage for a linearly graded pn junction. dQ , which is uncovered as a differential voltage dVR is applied. The junction capacitance is then dQ dx C _ (eax0) _0 dVR dVR (7.72) Using Equation (7.71), we obtain1 ea2s C ___ 12(Vbi VR) 1 3 (7.73) We may note that C is proportional to (Vbi VR)1 3 for the linearly graded junction as compared to C (Vbi VR)1 2 for the uniformly doped junction. In the linearly graded junction, the capacitance is less dependent on reverse-biased voltage than in the uniformly doped junction. 7.5.2 Hyperabrupt Junctions The uniformly doped junction and linearly graded junction are not the only possible doping profiles. Figure 7.19 shows a generalized one-sided pn junction where the generalized n-type doping concentration for x 0 is given by N Bxm (7.74) The case of m 0 corresponds to the uniformly doped junction, and m 1 corresponds to the linearly graded junction just discussed. The cases of m 2 and m 3 shown would approximate a fairly low-doped epitaxial n-type layer grown 1 In a more exact analysis, Vbi in Equation (7.73) is replaced by a gradient voltage. However, this analysis is beyond the scope of this text. nea29583_ch07_241-275.indd 265 12/11/10 11:32 AM 266 CHAPTER 7 The pn Junction p n x0 m 2 m 3 m 5 3 m 1 3 m 2 n-type doping profiles m0 Bx 0m m 1 x0 x0 Figure 7.19 | Generalized doping profiles of a one-sided pn junction. (From Sze [14].) on a much more heavily doped n substrate layer. When the value of m is negative, we have what is referred to as a hyperabrupt junction. In this case, the n-type doping is larger near the metallurgical junction than in the bulk semiconductor. Equation (7.74) is used to approximate the n-type doping over a small region near x x0 and does not hold at x 0 when m is negative. The junction capacitance can be derived using the same analysis method as before and is given by 1 (m2) eB(m1) s C ___ (7.75) (m 2)(Vbi VR) When m is negative, the capacitance becomes a very strong function of reverse-biased voltage, a desired characteristic in varactor diodes. The term varactor comes from the words variable reactor and means a device whose reactance can be varied in a controlled manner with bias voltage. If a varactor diode and an inductance are in parallel, the resonant frequency of the LC circuit is 1 ___ fr __ 2 LC (7.76) The capacitance of the diode, from Equation (7.75), can be written in the form C C0(Vbi VR)1 (m2) nea29583_ch07_241-275.indd 266 (7.77) 12/11/10 11:32 AM 7.6 Summary 267 In a circuit application, we would, in general, like to have the resonant frequency be a linear function of reverse-biased voltage VR, so we need C V 2 (7.78) From Equation (7.77), the parameter m required is found from 1 2 __ (7.79a) 3 m _ 2 (7.79b) m2 or A specific doping profile will yield the desired capacitance characteristic. 7.6 | SUMMARY ■ ■ ■ ■ ■ ■ ■ ■ ■ A uniformly doped pn junction is initially considered, in which one region of a semiconductor is uniformly doped with acceptor impurities and the adjacent region is uniformly doped with donor impurities. A space charge region, or depletion region, is formed on either side of the metallurgical junction separating the n and p regions. This region is essentially depleted of any mobile electrons or holes. A net positive charge density, due to the positively charged donor impurity ions, exists in the n region and a net negative charge density, due to the negatively charged acceptor impurity ions, exists in the p region. An electric field exists in the depletion region due to the net space charge density. The direction of the electric field is from the n region to the p region. A potential difference exists across the space charge region. Under zero applied bias, this potential difference, known as the built-in potential barrier, maintains thermal equilibrium and holds back majority carrier electrons in the n region and majority carrier holes in the p region. An applied reverse-biased voltage (n region positive with respect to the p region) increases the potential barrier, the space charge width, and the magnitude of the electric field. As the reverse-biased voltage changes, the amount of charge in the depletion region changes. This change in charge with voltage defines the junction capacitance. Avalanche breakdown occurs when a sufficiently large reverse-biased voltage is applied to the pn junction. A large reverse-biased current may then be induced in the pn junction. The breakdown voltage, as a function of the doping concentrations in the pn junction, is derived. In a one-sided pn junction, the breakdown voltage is a function of the doping concentration in the low-doped region. The linearly graded junction represents a nonuniformly doped pn junction. Expressions for the electric field, built-in potential barrier, and junction capacitance are derived. The functional relationships differ from those of the uniformly doped junction. Specific doping profiles can be used to obtain specific capacitance characteristics. A hyperabrupt junction is one in which the doping decreases away from the metallurgical junction. This type of junction is advantageous in varactor diodes that are used in resonant circuits. nea29583_ch07_241-275.indd 267 12/11/10 11:32 AM 268 CHAPTER 7 The pn Junction GLOSSARY OF IMPORTANT TERMS abrupt junction approximation The assumption that there is an abrupt discontinuity in space charge density between the space charge region and the neutral semiconductor region. avalanche breakdown The process whereby a large reverse-biased pn junction current is created due to the generation of electron–hole pairs by the collision of electrons and/or holes with atomic electrons within the space charge region. built-in potential barrier The electrostatic potential difference between the p and n regions of a pn junction in thermal equilibrium. critical electric field The peak electric field in the space charge region at breakdown. depletion layer capacitance Another term for junction capacitance. depletion region Another term for space charge region. hyperabrupt junction A pn junction in which the doping concentration on one side decreases away from the metallurgical junction to achieve a specific capacitance–voltage characteristic. junction capacitance The capacitance of the pn junction under reverse bias. linearly graded junction A pn junction in which the doping concentrations on either side of the metallurgical junction are approximated by a linear distribution. metallurgical junction The interface between the p- and n-doped regions of a pn junction. one-sided junction A pn junction in which one side of the junction is much more heavily doped than the adjacent side. reverse bias The condition in which a positive voltage is applied to the n region with respect to the p region of a pn junction so that the potential barrier between the two regions increases above the thermal-equilibrium built-in potential barrier. space charge region The region on either side of the metallurgical junction in which there is a net charge density due to ionized donors in the n region and ionized acceptors in the p region. space charge width The width of the space charge region, a function of doping concentrations and applied voltage. varactor diode A diode whose reactance can be varied in a controlled manner with bias voltage. CHECKPOINT After studying this chapter, the reader should have the ability to: ■ ■ ■ ■ ■ ■ ■ ■ ■ ■ nea29583_ch07_241-275.indd 268 Describe why and how the space charge region is formed. Draw the energy-band diagram of a zero-biased and reverse-biased pn junction. Define and derive the expression of the built-in potential barrier voltage. Derive the expression for the electric field in space charge region of the pn junction. Describe what happens to the parameters of the space charge region when a reversebiased voltage is applied. Define and explain the junction capacitance. Describe the characteristics and properties of a one-sided pn junction. Describe the avalanche breakdown mechanism in a reverse-biased pn junction. Describe how a linearly graded junction is formed. Define a hyperabrupt junction. 12/11/10 11:32 AM Problems 269 REVIEW QUESTIONS 1. Define the built-in potential voltage and describe how it maintains thermal equilibrium. 2. Why is an electric field formed in the space charge region? Why is the electric field a linear function of distance in a uniformly doped pn junction? 3. Where does the maximum electric field occur in the space charge region? 4. Why is the space charge width larger in the lower doped side of a pn junction? 5. What is the functional dependence of the space charge width on reverse-biased voltage? 6. Why does the space charge width increase with reverse-biased voltage? 7. Why does a capacitance exist in a reverse-biased pn junction? Why does the capacitance decrease with increasing reverse-biased voltage? 8. What is a one-sided pn junction? What parameters can be determined in a one-sided pn junction? 9. Why does the breakdown voltage of a pn junction decrease as the doping concentration increases? 10. What is a linearly graded junction? 11. What is a hyperabrupt junction and what is one advantage or characteristic of such a junction? PROBLEMS Section 7.2 Zero Applied Bias (a) Calculate Vbi in a silicon pn junction at T 300 K for (a) Na 2 1015 cm3 and Nd (i) 2 1015, (ii) 2 1016, and (iii) 2 1017 cm3. (b) Repeat part (a) for Na 2 1017 cm3. 7.2 Calculate the built-in potential barrier, Vbi, for Si, Ge, and GaAs pn junctions if they each have the following dopant concentrations at T 300 K: 7.1 (a) Nd 1014 cm3 Na 1017 cm3 (b) Nd 5 1016 Na 5 1016 (c) Nd 1017 Na 1017 (a) Plot the built-in potential barrier for a symmetrical (Na Nd) silicon pn junction at T 300 K over the range 1014 Na Nd 1017 cm3. (b) Repeat part (a) for a GaAs pn junction. (c) Repeat parts (a) and (b) for T 400 K. 7.4 An abrupt silicon pn junction at zero bias has dopant concentrations of Na 1017 cm3 and Nd 5 1015 cm3. T 300 K. (a) Calculate the Fermi level on each side of the junction with respect to the intrinsic Fermi level. (b) Sketch the equilibrium energyband diagram for the junction and determine Vbi from the diagram and the results of part (a). (c) Calculate Vbi using Equation (7.10), and compare the results to part (b). (d ) Determine xn, xp, and the peak electric field for this junction. 7.5 Repeat problem 7.4 for the case when the doping concentrations are Na Nd 2 1016 cm3. 7.6 A silicon pn junction in thermal equilibrium at T 300 K is doped such that EF EFi 0.365 eV in the n region and EFi EF 0.330 eV in the p region. 7.3 nea29583_ch07_241-275.indd 269 12/11/10 11:32 AM 270 CHAPTER 7 7.7 7.8 7.9 7.10 7.11 7.12 7.13 7.14 The pn Junction (a) Sketch the energy-band diagram for the pn junction. (b) Find the impurity doping concentration in each region. (c) Determine Vbi. Consider a uniformly doped GaAs pn junction with doping concentrations of Na 2 1015 cm3 and Nd 4 1016 cm3. Plot the built-in potential barrier Vbi versus temperature over the range 200 T 400 K. (a) Consider a uniformly doped silicon pn junction at T 300 K. At zero bias, 25 percent of the total space charge region is in the n-region. The built-in potential barrier is Vbi 0.710 V. Determine (i) Na, (ii) Nd, (iii) xn, (iv) xp, and (v) Emax. (b) Repeat part (a) for a GaAs pn junction with Vbi 1.180 V. Consider the impurity doping profile shown in Figure P7.9 in a silicon pn junction. For zero applied voltage, (a) determine Vbi, (b) calculate xn and xp, (c) sketch the thermal equilibrium energy-band diagram, and (d) plot the electric field versus distance through the junction. Consider a uniformly doped silicon pn junction with doping concentrations Na 2 1017 cm3 and Nd 4 1016 cm3. (a) Determine Vbi at T 300 K. (b) Determine the temperature at which Vbi increases by 2 percent. (Trial and error may have to be used.) The doping concentrations in a uniformly doped silicon pn junction are Na 4 1016 cm3 and Nd 2 1015 cm3. The measured built-in potential barrier is Vbi 0.550 V. Determine the temperature at which this result occurs. An “isotype” step junction is one in which the same impurity type doping changes from one concentration value to another value. An n-n isotype doping profile is shown in Figure P7.12. (a) Sketch the thermal equilibrium energy-band diagram of the isotype junction. (b) Using the energy-band diagram, determine the built-in potential barrier. (c) Discuss the charge distribution through the junction. A particular type of junction is an n region adjacent to an intrinsic region. This junction can be modeled as an n-type region to a lightly doped p-type region. Assume the doping concentrations in silicon at T 300 K are Nd 1016 cm3 and Na 1012 cm3. For zero applied bias, determine (a) Vbi, (b) xn, (c) xp, and (d) Emax. Sketch the electric field versus distance through the junction. We are assuming an abrupt depletion approximation for the space charge region. That is, no free carriers exist within the depletion region and the semiconductor abruptly changes to a neutral region outside the space charge region. This approximation is (Na Nd) (cm3) 1016 Nd (cm3) p type 1015 0 2 m n type 4 1015 Figure P7.9 | Figure for Problem 7.9. nea29583_ch07_241-275.indd 270 1016 1015 0 Figure P7.12 | Figure for Problem 7.12. 12/11/10 11:32 AM Problems 271 adequate for most applications, but the abrupt transition does not exist. The space charge region changes over a distance of a few Debye lengths, where the Debye length in the n region is given by skT 1 2 LD _ e2Nd 7.15 Calculate LD and find the ratio of LD /xn for the following conditions. The p-type doping concentration is Na 8 1017 cm3 and the n-type doping concentration is (a) Nd 8 1014 cm3, (b) Nd 2.2 1016 cm3, and (c) Nd 8 1017 cm3. Examine the electric field versus distance through a uniformly doped silicon pn junction at T 300 K as a function of doping concentrations. Assume zero applied bias. Sketch the electric field versus distance through the space charge region and calculate Emax for: (a) Na 1017 cm3 and 1014 Nd 1017 cm3 and (b) Na 1014 cm3 and 1014 Nd 1017 cm3. (c) What can be said about the results for Nd 100 Na or Na 100 Nd? Section 7.3 7.16 7.17 7.18 7.19 7.20 7.21 7.22 Reverse Applied Bias An abrupt silicon pn junction at T 300 K has impurity doping concentrations of Na 5 1016 cm3 and Nd 1015 cm3. Calculate (a) Vbi, (b) W at (i) VR 0 and (ii) VR 5 V, and (c) Emax at (i) VR 0 and (ii) VR 5. Consider the pn junction described in Problem 7.10 for T 300 K. The crosssectional area of the junction is 2 104 cm2 and the applied reverse-biased voltage is VR 2.5 V. Calculate (a) Vbi, (b) xn, xp, W, (c) Emax , and (d) the junction capacitance. An ideal one-sided silicon pn junction at T 300 K is uniformly doped on both sides of the metallurgical junction. It is found that the doping relation is Na 80 Nd and the built-in potential barrier is Vbi 0.740 V. A reverse-biased voltage of VR 10 V is applied. Determine (a) Na, Nd; (b) xp, xn; (c) Emax ; and (d) C j . A silicon np junction is biased at VR 5 V. (a) Determine the change in built-in potential barrier if the doping concentration in the p region increases by a factor of 3. (b) Determine the ratio of junction capacitance when the acceptor doping is 3Na compared to that when the acceptor doping is Na. (c) Why does the junction capacitance increase when the doping concentration increases? (a) The peak electric field in a reverse-biased silicon pn junction is Emax 3 105 V/cm. The doping concentrations are Nd 4 1015 cm3 and Na 4 1017 cm3. Find the magnitude of the reverse-biased voltage. (b) Repeat part (a) for Nd 4 1016 cm3 and Na 4 1017 cm3. (c) Repeat part (a) for Nd Na 4 1017 cm3. Consider two pn silicon junctions at T 300 K reverse biased at VR 5 V. The impurity doping concentrations in junction A are Na 1018 cm3 and Nd 1015 cm3, and those in junction B are Na 1018 cm3 and Nd 1016 cm3. Calculate the ratio of the following parameters for junction A to junction B: (a) W, (b) Emax , and (c) C j . Consider a uniformly doped GaAs pn junction at T 300 K. The junction capacitance at zero bias is Cj(0) and the junction capacitance with a 10-V reverse-biased voltage is Cj (10). The ratio of the capacitances is Cj (0) __ 3.13 Cj (10) Also under reverse bias, the space charge width into the p region is 0.2 of the total space charge width. Determine (a) Vbi and (b) Na, Nd. nea29583_ch07_241-275.indd 271 12/11/10 11:32 AM 272 CHAPTER 7 7.23 7.24 7.25 7.26 7.27 7.28 7.29 The pn Junction A GaAs pn junction at T 300 K has impurity doping concentrations of Na 2 1016 cm3 and Nd 5 1015 cm3. It is determined that the ratio of junction capacitance at two reverse-biased voltages is Cj (VR1) Cj(VR2) 1.5, where VR1 0.5 V. Determine VR2. (a) The impurity doping concentrations in a silicon pn junction at T 300 K are Na 2 1015 cm3 and Nd 4 1016 cm3. The cross-sectional area of the pn junction is 5 104 cm2. Determine the junction capacitance at (i) VR 0 and (ii) VR 5 V. (b) Repeat part (a) for a GaAs pn junction. An abrupt silicon pn junction at T 300 K is uniformly doped with Na 2 1017 cm3 and Nd 5 1015 cm3. The cross-sectional area of the pn junction is 8 104 cm2. An inductance is placed in parallel with the pn junction. (a) With a reversebiased voltage of VR 10 V applied to the pn junction, the resonant frequency of the circuit is f 1.25 MHz. What is the value of the inductance? (b) Using the results of part (a), what is the resonant frequency if the reverse-biased voltage is (i) VR 1 V and (ii) VR 5 V? (a) A uniformly doped silicon pn junction at T 300 K is to be designed such that, at a reverse-biased of VR 10 V, the maximum electric field is limited to Emax 2.5 105 V/cm. Determine the maximum doping concentration in the n region. (Use an approximate value for Vbi.) (b) Repeat part (a) if the maximum electric field is limited to Emax 105 V/cm. (a) A GaAs pn junction at T 300 K, with a cross-sectional area of 104 cm2, is to be designed that meets the following specifications. At a reverse-biased voltage of VR 2 V, 20 percent of the total space charge width is to be in the p region and the total junction capacitance is to be 0.6 pF. Determine Na, Nd, and W. (b) Repeat part (a) if VR 5 V. A silicon pn junction at T 300 K has the doping profile shown in Figure P7.28. Calculate (a) Vbi, (b) xn and xp at zero bias, and (c) the applied bias required so that xn 30 m. Consider a silicon pn junction with the doping profile shown in Figure P7.29. T 300 K. (a) Calculate the applied reverse-biased voltage required so that the space charge region extends entirely through the p region. (b) Determine the space charge width into the n region with the reverse-biased voltage calculated in part (a). (c) Calculate the peak electric field for this applied voltage. n p p (Na Nd ) (cm3) (Na Nd) (cm3) 5 1015 1016 1014 x0 1014 Figure P7.28 | Figure for Problem 7.28. nea29583_ch07_241-275.indd 272 0 50 x (m) 1016 Figure P7.29 | Figure for Problem 7.29. 12/11/10 11:32 AM Problems Na Nd (Nd Na ) (cm3) Na0 5 1015 1 x0 273 Nd0 x 2 1 2 x (m) 5 1015 2 Nd0 i region Figure P7.33 | Figure for Problem 7.33. 7.30 7.31 7.32 *7.33 *7.34 Figure P7.34 | Figure for Problem 7.34. A silicon pn junction has doping concentrations of Na 2 1017 cm3 and Nd 2 1015 cm3. The cross-sectional area is 105 cm2. Calculate (a) Vbi and (b) the junction capacitance at (i) VR 1 V, (ii) VR 3 V, and (iii) VR 5 V. (c) Plot 1 C 2 versus VR and show that the slope can be used to find Nd and the intercept at the voltage axis yields Vbi. The total junction capacitance of a GaAs pn junction at T 300 K is found to be 1.10 pF at VR 1 V. The doping concentration in one region is measured and found to be 8 1016 cm3, and the built-in potential is found to be Vbi 1.20 V. Determine (a) the doping in the other region of the pn junction and (b) the cross-sectional area. (c) The reverse-biased voltage is changed and the capacitance is found to be 0.80 pF. What is the value of VR? Examine how the capacitance C and the function (1/C )2 vary with reverse-biased voltage VR as the doping concentrations change. In particular, consider these plots versus Na for Na 100 Nd and versus Nd for Nd 100 Na. A pn junction has the doping profile shown in Figure P7.33. Assume that xn x0 for all reverse-biased voltages. (a) What is the built-in potential across the junction? (b) For the abrupt junction approximation, sketch the charge density through the junction. (c) Derive the expression for the electric field through the space charge region. A silicon PIN junction has the doping profile shown in Figure P7.34. The “I” corresponds to an ideal intrinsic region in which there is no impurity doping concentration. A reverse-biased voltage is applied to the PIN junction so that the total depletion width extends from 2 m to 2 m. (a) Using Poisson’s equation, calculate the magnitude of the electric field at x 0. (b) Sketch the electric field through the PIN junction. (c) Calculate the reverse-biased voltage that must be applied. Section 7.4 Junction Breakdown Consider a silicon np junction diode. The critical electric field for breakdown in silicon is approximately Ecrit 4 10 5 V/cm. Determine the maximum p-type doping concentration such that the breakdown voltage is (a) 40 V and (b) 20 V. 7.36 Design an abrupt silicon np junction diode that has a reverse breakdown voltage of 80 V. 7.37 (a) The n-type doping concentration in an abrupt pn GaAs junction diode is Nd 1016 cm3. Determine the breakdown voltage. (b) Repeat part (a) for Nd 1015 cm3. 7.35 *Asterisks next to problems indicate problems that are more difficult. nea29583_ch07_241-275.indd 273 12/11/10 11:32 AM 274 CHAPTER 7 The pn Junction 7.38 (a) A symmetrically doped silicon pn junction diode has doping concentrations of Na Nd 2 1016 cm3. Assuming the critical electric field is Ecrit 4 105 V/cm, determine the breakdown voltage. (b) Repeat part (a) if the doping concentrations are Na Nd 5 1015 cm3. 7.39 An abrupt silicon pn junction has an n-region doping concentration of Nd 5 1015 cm3. What must be the minimum n-region width such that avalanche breakdown occurs before the depletion region reaches an ohmic contact (punchthrough)? 7.40 A silicon pn junction diode is doped with Na Nd 1018 cm3. Zener breakdown occurs when the peak electric field reaches 106 V/cm. Determine the reverse-biased breakdown voltage. 7.41 A diode will very often have the doping profile shown in Figure P7.29, which is known as an npp diode. Under reverse bias, the depletion region must remain within the p region to avoid premature breakdown. Assume the p-region doping is 1015 cm3. Determine the reverse-biased voltage such that the depletion region remains within the p region and does not reach breakdown if the p-region width is (a) 75 m and (b) 150 m. For each case, state whether the maximum depletion width or the breakdown voltage is reached first. 7.42 Consider a silicon pn junction at T 300 K whose doping profile varies linearly from Na 1018 cm3 to Nd 1018 cm3 over a distance of 2 m. Estimate the breakdown voltage. Section 7.5 7.43 7.44 Nonuniformly Doped Junctions Consider a linearly graded junction. (a) Starting with Equation (7.62), derive the expression for the electric field given in Equation (7.64). (b) Derive the expression for the potential through the space charge region given by Equation (7.66). The built-in potential barrier of a linearly graded silicon pn junction at T 300 K is Vbi 0.70 V. The junction capacitance measured at VR 3.5 V is C 7.2 109 F/cm2. Find the gradient, a, of the net impurity concentration. Summary and Review (a) A one-sided silicon np junction at T 300 K is doped at Nd 3 1017 cm3. Design the junction such that Cj 0.45 pF at VR 5 V. (b) Calculate the junction capacitance at (i) VR 2.5 V and (ii) VR 0 V. 7.46 A one-sided pn junction with a cross-sectional area of 105 cm2 has a measured builtin potential of Vbi 0.8 V at T 300 K. A plot of (1/Cj)2 versus VR is linear for VR 1 V and is essentially constant for VR 1 V. The capacitance is Cj 0.082 pF at VR 1 V. Determine the doping concentrations on either side of the metallurgical junction that will produce this capacitance characteristic. *7.47 Silicon, at T 300 K, is doped at Nd1 1015 cm3 for x 0 and Nd2 5 1016 cm3 for x 0 to form an n n step junction. (a) Sketch the energy-band diagram. (b) Derive an expression for Vbi. (c) Sketch the charge density, electric field, and potential through the junction. (d) Explain where the charge density came from and is located. *7.48 A diffused silicon pn junction has a linearly graded junction on the p side with a 2 1019 cm4, and a uniform doping of 1015 cm3 on the n side. (a) If the depletion width on the p side is 0.7 m at zero bias, find the total depletion width, built-in potential, and maximum electric field at zero bias. (b) Plot the potential function through the junction. 7.45 nea29583_ch07_241-275.indd 274 12/11/10 11:32 AM Reading List 275 READING LIST 1. 2. *3. 4. 5. 6. *7. 8. *9. 10. *11. 12. 13. 14. 15. *16. 17. Dimitrijev, S. Principles of Semiconductor Devices. New York: Oxford University Press, 2006. Kano, K. Semiconductor Devices. Upper Saddle River, NJ: Prentice Hall, 1998. Li, S. S. Semiconductor Physical Electronics. New York: Plenum Press, 1993. Muller, R. S., and T. I. Kamins. Device Electronics for Integrated Circuits, 2nd ed. New York: John Wiley and Sons, 1986. Navon, D. H. Semiconductor Microdevices and Materials. New York: Holt, Rinehart & Winston, 1986. Neudeck, G. W. The PN Junction Diode. Vol. 2 of the Modular Series on Solid State Devices, 2nd ed. Reading, MA: Addison-Wesley, 1989. Ng, K. K. Complete Guide to Semiconductor Devices. New York: McGraw-Hill, 1995. Pierret, R. F. Semiconductor Device Fundamentals. Reading, MA: Addison-Wesley, 1996. Roulston, D. J. An Introduction to the Physics of Semiconductor Devices. New York: Oxford University Press, 1999. Shur, M. Introduction to Electronic Devices. New York: John Wiley and Sons, 1996. Shur, M. Physics of Semiconductor Devices. Englewood Cliffs, NJ: Prentice Hall, 1990. Singh, J. Semiconductor Devices: Basic Principles. New York: John Wiley and Sons, 2001. Streetman, B. G., and S. K. Banerjee. Solid State Electronic Devices, 6th ed. Upper Saddle River, NJ: Pearson Prentice Hall, 2006. Sze, S. M., and K. K. Ng. Physics of Semiconductor Devices, 3rd ed. Hoboken, NJ: John Wiley and Sons, 2007. Sze, S. M. Semiconductor Devices: Physics and Technology, 2nd ed. New York: John Wiley and Sons, 2001. Wang, S. Fundamentals of Semiconductor Theory and Device Physics. Englewood Cliffs, NJ: Prentice Hall, 1989. Yang, E. S. Microelectronic Devices. New York: McGraw-Hill, 1988. *Indicates references that are at an advanced level compared to this text. nea29583_ch07_241-275.indd 275 12/11/10 11:32 AM C 8 H A P T E R The pn Junction Diode I n the last chapter, we discussed the electrostatics of the pn junction in thermal equilibrium and under reverse bias. We determined the built-in potential barrier at thermal equilibrium and calculated the electric field in the space charge region. We also considered the junction capacitance. In this chapter, we consider the pn junction with a forward-bias voltage applied and determine the current–voltage characteristics. The potential barrier of the pn junction is lowered when a forward-bias voltage is applied, allowing electrons and holes to flow across the space charge region. When holes flow from the p region across the space charge region into the n region, they become excess minority carrier holes and are subject to the excess minority carrier diffusion, drift, and recombination processes discussed in Chapter 6. Likewise, when electrons from the n region flow across the space charge region into the p region, they become excess minority carrier electrons and are subject to these same processes. ■ 8.0 | PREVIEW In this chapter, we will: ■ Consider the process by which the potential barrier of a pn junction is lowered when a forward-bias voltage is applied, so holes and electrons can flow across the junction generating a diode current. ■ Derive the boundary conditions for excess holes in the n region and excesselectrons in the p region, and analyze the behavior of these excess carriers under a forward bias. ■ Derive the ideal current–voltage relation of the forward-biased pn junction diode. ■ Describe and analyze nonideal effects in the pn junction diode such as highlevel injection, and generation and recombination currents. ■ Develop a small-signal equivalent circuit of the pn junction diode. This equivalent circuit is used to relate small time-varying currents and voltages in the pn junction. 276 nea29583_ch08_276-330.indd 276 12/11/10 12:37 PM 8.1 ■ ■ pn Junction Current 277 Discuss large signal diode switching characteristics. Describe a specialized pn junction called a tunnel diode. 8.1 | pn JUNCTION CURRENT When a forward-bias voltage is applied to a pn junction, a current will be induced in the device. We initially consider a qualitative discussion of how charges flow in the pn junction and then consider the mathematical derivation of the current–voltage relationship. 8.1.1 Qualitative Description of Charge Flow in a pn Junction We can qualitatively understand the mechanism of the current in a pn junction by again considering the energy-band diagrams. Figure 8.1a shows the energy-band diagram of a pn junction in thermal equilibrium that was developed in the last chapter. We argued that the potential barrier seen by the electrons, for example, holds back the large concentration of electrons in the n region and keeps them from flowing into the p region. Similarly, the potential barrier seen by the holes holds back the large concentration of holes in the p region and keeps them from flowing into the n region. The potential barrier, then, maintains thermal equilibrium. Figure 8.1b shows the energy-band diagram of a reverse-biased pn junction. The potential of the n region is positive with respect to the p region so the Fermi energy VR W p Va W W n p E n n p E E Electron flow Ec e(Vbi Va) eVbi EFp Ev EFn EFn e(Vbi VR) EFp EFp EFn (a) (b) Hole flow (c) Figure 8.1 A pn junction and its associated energy-band diagram for (a) zero bias, (b) reverse bias, and (c) forward bias. nea29583_ch08_276-330.indd 277 12/11/10 12:37 PM 278 CHAPTER 8 The pn Junction Diode in the n region is lower than that in the p region. The total potential barrier is now larger than that for the zero-bias case. We argued in the last chapter that the increased potential barrier continues to hold back the electrons and holes so that there is still essentially no charge flow and hence essentially no current. Figure 8.1c shows the energy-band diagram for the case when a positive voltage is applied to the p region with respect to the n region. The Fermi level in the p region is now lower than that in the n region. The total potential barrier is now reduced. The smaller potential barrier means that the electric field in the depletion region is also reduced. The smaller electric field means that the electrons and holes are no longer held back in the n and p regions, respectively. There will be a diffusion of holes from the p region across the space charge region where they will flow into the n region. Similarly, there will be a diffusion of electrons from the n region across the space charge region where they will flow into the p region. The flow of charge generates a current through the pn junction. The injection of holes into the n region means that these holes are minority carriers. Likewise, the injection of electrons into the p region means that these electrons are minority carriers. The behavior of these minority carriers is described by the ambipolar transport equations that were discussed in Chapter 6. There will be diffusion as well as recombination of excess carriers in these regions. The diffusion of carriers implies that there will be diffusion currents. The mathematical derivation of the pn junction current–voltage relationship is considered in the next section. 8.1.2 Ideal Current–Voltage Relationship The ideal current–voltage relationship of a pn junction is derived on the basis of four assumptions. (The last assumption has three parts, but each part deals with current.) They are: 1. The abrupt depletion layer approximation applies. The space charge regions have abrupt boundaries, and the semiconductor is neutral outside of the depletion region. 2. The Maxwell–Boltzmann approximation applies to carrier statistics. 3. The concepts of low injection and complete ionization apply. 4a. The total current is a constant throughout the entire pn structure. 4b. The individual electron and hole currents are continuous functions through the pn structure. 4c. The individual electron and hole currents are constant throughout the depletion region. Notation can sometimes appear to be overwhelming in the equations in this chapter. Table 8.1 lists some of the various electron and hole concentration terms that appear. Many terms have already been used in previous chapters but are repeated here for convenience. nea29583_ch08_276-330.indd 278 12/11/10 12:37 PM 8.1 pn Junction Current 279 Table 8.1 | Commonly used terms and notation for this chapter Term Meaning Na Nd nn0 Nd pp0 Na np0 n2i /Na pn0 n2i /Nd np pn np(xp) pn(xn) np np np0 pn pn pn0 8.1.3 Acceptor concentration in the p region of the pn junction Donor concentration in the n region of the pn junction Thermal-equilibrium majority carrier electron concentration in the n region Thermal-equilibrium majority carrier hole concentration in the p region Thermal-equilibrium minority carrier electron concentration in the p region Thermal-equilibrium minority carrier hole concentration in the n region Total minority carrier electron concentration in the p region Total minority carrier hole concentration in the n region Minority carrier electron concentration in the p region at the space charge edge Minority carrier hole concentration in the n region at the space charge edge Excess minority carrier electron concentration in the p region Excess minority carrier hole concentration in the n region Boundary Conditions Figure 8.2 shows the conduction-band energy through the pn junction in thermal equilibrium. The n region contains many more electrons in the conduction band than the p region; the built-in potential barrier prevents this large density of electrons from flowing into the p region. The built-in potential barrier maintains equilibrium between the carrier distributions on either side of the junction. An expression for the built-in potential barrier was derived in the last chapter and was given by Equation (7.10) as Na Nd Vbi Vt ln _ n2i p Electron energy n Ec eVbi ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ Figure 8.2 | Conduction-band energy through a pn junction. nea29583_ch08_276-330.indd 279 12/11/10 12:37 PM 280 CHAPTER 8 The pn Junction Diode If we divide the equation by Vt kT e, take the exponential of both sides, and then take the reciprocal, we obtain ni eVbi _ exp _ 2 Na Nd kT (8.1) If we assume complete ionization, we can write nn0 Nd (8.2) where nn0 is the thermal-equilibrium concentration of majority carrier electrons in the n region. In the p region, we can write n2 np0 _i Na (8.3) where np0 is the thermal-equilibrium concentration of minority carrier electrons. Substituting Equations (8.2) and (8.3) into Equation (8.1), we obtain eVbi np0 nn0 exp _ kT (8.4) This equation relates the minority carrier electron concentration on the p side of the junction to the majority carrier electron concentration on the n side of the junction in thermal equilibrium. If a positive voltage is applied to the p region with respect to the n region, the potential barrier is reduced. Figure 8.3a shows a pn junction with an applied voltage Va. The electric field in the bulk p and n regions is normally very small. Essentially all of the applied voltage is across the junction region. The electric field Eapp induced by the applied voltage is in the opposite direction to the thermal-equilibrium space charge electric field, so the net electric field in the space charge region is reduced below the equilibrium value. The delicate balance between diffusion and the E-field Eapp Wp p p Wn ⴚ ⴚ ⴚ ⴙ ⴙ ⴙ E ⴚ ⴚ ⴚ ⴙ ⴙ ⴙ ⴚ ⴚ ⴚ ⴙ ⴙ ⴙ n Ec e(Vbi Va) n EFi eVa EFp ⴙ Va (a) ⴚ EFn Ev (b) Figure 8.3 | (a) A pn junction with an applied forward-bias voltage showing the directions of the electric field induced by Va and the space charge electric field. (b) Energy-band diagram of the forward-biased pn junction. nea29583_ch08_276-330.indd 280 12/11/10 12:37 PM 8.1 pn Junction Current 281 force achieved at thermal equilibrium is upset. The electric field force that prevented majority carriers from crossing the space charge region is reduced; majority carrier electrons from the n side are now injected across the depletion region into the p material, and majority carrier holes from the p side are injected across the depletion region into the n material. As long as the bias Va is applied, the injection of carriers across the space charge region continues and a current is created in the pn junction. This bias condition is known as forward bias; the energy-band diagram of the forwardbiased pn junction is shown in Figure 8.3b. The potential barrier Vbi in Equation (8.4) can be replaced by (Vbi Va) when the junction is forward biased. Equation (8.4) becomes e (Vbi Va) eVbi eV np nn0 exp ___ nn0 exp _ exp _a kT kT kT (8.5) If we assume low injection, the majority carrier electron concentration nn0, for example, does not change significantly. However, the minority carrier concentration, np, can deviate from its thermal-equilibrium value np0 by orders of magnitude. Using Equation (8.4), we can write Equation (8.5) as eV np np0 exp _a kT (8.6) When a forward-bias voltage is applied to the pn junction, the junction is no longer in thermal equilibrium. The left side of Equation (8.6) is the total minority carrier electron concentration in the p region, which is now greater than the thermal equilibrium value. The forward-bias voltage lowers the potential barrier so that majority carrier electrons from the n region are injected across the junction into the p region, thereby increasing the minority carrier electron concentration. We have produced excess minority carrier electrons in the p region. When the electrons are injected into the p region, these excess carriers are subject to the diffusion and recombination processes we discussed in Chapter 6. Equation (8.6), then, is the expression for the minority carrier electron concentration at the edge of the space charge region in the p region. Exactly the same process occurs for majority carrier holes in the p region, which are injected across the space charge region into the n region under a forward-bias voltage. We can write that eV pn pn0 exp _a kT (8.7) where pn is the concentration of minority carrier holes at the edge of the space charge region in the n region. Figure 8.4 shows these results. By applying a forward-bias voltage, we create excess minority carriers in each region of the pn junction. nea29583_ch08_276-330.indd 281 12/11/10 12:37 PM 282 CHAPTER 8 The pn Junction Diode p n eVa pn(xn) pn0 exp kT [ [ Hole injection Electron injection [ [ eVa np(xp) np0 exp kT pn0 np0 xp x 0 xn Figure 8.4 | Excess minority carrier concentrations at the space charge edges generated by the forward-bias voltage. EXAMPLE 8.1 Objective: Calculate the minority carrier concentrations at the edge of the space charge regions in a forward-biased pn junction. Consider a silicon pn junction at T 300 K. Assume the doping concentration in the n region is Nd 1016 cm3 and the doping concentration in the p region is Na 6 1015 cm3, and assume that a forward bias of 0.60 V is applied to the pn junction. ■ Solution From Equations (8.6) and (8.7) and from Figure 8.4, we have eV np (xp) npo exp _a kT eV pn(xn) pno exp _a kT and The thermal-equilibrium minority carrier concentrations are n2 (1.5 1010)2 npo _i ___ 3.75 10 4 cm3 Na 6 1015 and n2 (1.5 1010)2 pno _i ___ 2.25 10 4 cm3 Nd 1016 We then have 0.60 4.31 1014 cm3 np (xp) 3.75 10 4 exp __ 0.0259 and 0.60 2.59 1014 cm3 pn(xn) 2.25 10 4 exp __ 0.0259 ■ Comment The minority carrier concentrations can increase by many orders of magnitude when a relatively small forward-bias voltage is applied. Low injection still applies, however, since the excess minority carrier concentrations at the space-charge edges are much less than the thermal-equilibrium majority carrier concentrations. nea29583_ch08_276-330.indd 282 12/11/10 12:37 PM 8.1 pn Junction Current 283 ■ EXERCISE PROBLEM Ex 8.1 A silicon pn junction at T 300 K is doped with impurity concentrations of Nd 2 1016 cm3 and Na 5 1016 cm3. The junction is forward biased at Va 0.650 V. Determine the minority carrier concentrations at the space charge edges. Does low injection still apply? [Ans. np(xp) 3.57 1014 cm3, pn(xn) 8.92 1014 cm3, yes] The minority carrier concentrations at the space charge edges, given by Equations (8.6) and (8.7), were derived assuming that a forward-bias voltage (Va 0) was applied across the pn junction. However, nothing in the derivation prevents Va from being negative (reverse bias). If a reverse-biased voltage greater than a few tenths of a volt is applied to the pn junction, then we see from Equations (8.6) and (8.7) that the minority carrier concentrations at the space charge edge are essentially zero. The minority carrier concentrations for the reverse-biased condition drop below the thermal-equilibrium values. 8.1.4 Minority Carrier Distribution We developed, in Chapter 6, the ambipolar transport equation for excess minority carrier holes in an n region. This equation, in one dimension, is 2 (pn) (pn) pn __ (pn) Dp __ pE __ g _ p0 t x x2 (8.8) where pn pn pn0 is the excess minority carrier hole concentration and is the difference between the total and thermal equilibrium minority carrier concentrations. The ambipolar transport equation describes the behavior of excess carriers as a function of time and spatial coordinates. In Chapter 5, we calculated drift current densities in a semiconductor. We determined that relatively large currents could be created with fairly small electric fields. As a first approximation, we assume that the electric field is zero in both the neutral p and n regions. In the n region for x xn, we have that E 0 and g 0. If we also assume steady state so (pn) /t 0, then Equation (8.8) reduces to d (pn) _ p __ n 0 2 dx2 L2p (x xn) (8.9) where L2p Dp p0. For the same set of conditions, the excess minority carrier electron concentration in the p region is determined from d (np) _ np __ 0 2 dx2 L2n (x xp) (8.10) where L2n Dnn0. nea29583_ch08_276-330.indd 283 12/11/10 12:37 PM 284 CHAPTER 8 The pn Junction Diode The boundary conditions for the total minority carrier concentrations are eV pn(xn) pn0 exp _a kT eV np(xp) np0 exp _a kT pn(x → ) pn0 (8.11a) (8.11b) (8.11c) np(x → ) np0 (8.11d) As minority carriers diffuse from the space charge edge into the neutral semiconductor regions, they recombine with majority carriers. We assume that the lengths Wn and Wp shown in Figure 8.3a are very long, meaning in particular that Wn Lp and Wp Ln. The excess minority carrier concentrations must approach zero at distances far from the space charge region. The structure is referred to as a long pn junction. The general solution to Equation (8.9) is pn (x) pn (x) pn0 AexLp BexLp (x xn) (8.12) xp) (8.13) and the general solution to Equation (8.10) is np(x) np(x) np0 CexLn DexLn (x Applying the boundary conditions from Equations (8.11c) and (8.11d), the coefficients A and D must be zero. The coefficients B and C may be determined from the boundary conditions given by Equations (8.11a) and (8.11b). The excess carrier concentrations are then found to be, for (x xn), (8.14) (8.15) eV xn x pn(x) pn(x) pn0 pn0 exp _a 1 exp __ Lp kT and, for (x xp), xp x eV np(x) np(x) np0 np0 exp _a 1 exp __ Ln kT The minority carrier concentrations decay exponentially with distance away from the junction to their thermal-equilibrium values. Figure 8.5 shows these results. Again, we have assumed that both the n-region and the p-region lengths are long compared to the minority carrier diffusion lengths. In Chapter 6, we discussed the concept of quasi-Fermi levels, which apply to excess carriers in a nonequilibium condition. Since excess electrons exist in the neutral p region and excess holes exist in the neutral n region, we can apply quasi-Fermi levels to these regions. We had defined quasi-Fermi levels in terms of carrier concentrations as EFi EFp p po p ni exp __ (8.16) kT nea29583_ch08_276-330.indd 284 12/11/10 12:37 PM 8.1 p pn Junction Current 285 n np(x) pn(x) pn0 np0 xp x 0 xn Figure 8.5 | Steady-state minority carrier concentrations in a pn junction under forward bias. p n Ec Ec EFn EFi EFi EFp Ev Ev xp xn 0 Figure 8.6 | Quasi-Fermi levels through a forward-biased pn junction. and EFn EFi n no n ni exp __ (8.17) kT Figure 8.6 shows the quasi-Fermi levels through the pn junction. From Equations (8.14) and (8.15), the carrier concentrations are exponential functions of distance, and from Equations (8.16) and (8.17), the carrier concentrations are exponential functions of the quasi-Fermi levels. The quasi-Fermi levels are then linear functions of distance in the neutral p and n regions as shown in Figure 8.6. We may note that close to the space charge edge in the p region, EFn EFi 0 which means that n ni. Further from the space charge edge, EFn EFi 0 which means that n ni and the excess electron concentration is approaching zero. The same discussion applies to the excess hole concentration in the n region. At the space charge edge at x xn, we can write, for low injection V V no pn (xn) no pno exp _a n2i exp _a Vt Vt nea29583_ch08_276-330.indd 285 (8.18) 12/11/10 12:37 PM 286 CHAPTER 8 The pn Junction Diode Combining Equations (8.16) and (8.17), we can write EFn EFp np n2i exp __ kT (8.19) Comparing Equations (8.18) and (8.19), the difference in quasi-Fermi levels is related to the applied bias Va and represents the deviation from thermal equilibrium. The difference between EFn and EFp is nearly constant through the depletion region. To review, a forward-bias voltage lowers the built-in potential barrier of a pn junction so that electrons from the n region are injected across the space charge region, creating excess minority carriers in the p region. These excess electrons begin diffusing into the bulk p region where they can recombine with majority carrier holes. The excess minority carrier electron concentration then decreases with distance from the junction. The same discussion applies to holes injected across the space charge region into the n region. 8.1.5 Ideal pn Junction Current The approach we use to determine the current in a pn junction is based on the three parts of the fourth assumption stated earlier in this section. The total current in the junction is the sum of the individual electron and hole currents that are constant through the depletion region. Since the electron and hole currents are continuous functions through the pn junction, the total pn junction current will be the minority carrier hole diffusion current at x xn plus the minority carrier electron diffusion current at x xp. The gradients in the minority carrier concentrations, as shown in Figure 8.5, produce diffusion currents, and since we are assuming the electric field to be zero at the space charge edges, we can neglect any minority carrier drift current component. This approach in determining the pn junction current is shown in Figure 8.7. Current density p n JTotal Jp(xn) Jn(xp) Jp(xn) Jn(xp) xp x0 xn Figure 8.7 | Electron and hole current densities through the space charge region of a pn junction. nea29583_ch08_276-330.indd 286 12/11/10 12:37 PM 8.1 pn Junction Current 287 We can calculate the minority carrier hole diffusion current density at x xn from the relation dpn(x) Jp (xn) eDp __ dx xxn (8.20) Since we are assuming uniformly doped regions, the thermal-equilibrium carrier concentration is constant, so the hole diffusion current density may be written as d(pn(x)) Jp (xn) eDp __ dx xxn (8.21) Taking the derivative of Equation (8.14) and substituting into Equation (8.21), we obtain eDp pn0 eV Jp(xn) __ exp _a 1 Lp kT (8.22) The hole current density for this forward-bias condition is in the x direction, which is from the p to the n region. Similarly, we may calculate the electron diffusion current density at x xp. This may be written as Jn(xp) eDn d(np(x)) __ dx xxp (8.23) Using Equation (8.15), we obtain eDn np0 eV Jn (xp) __ exp _a 1 Ln kT (8.24) The electron current density is also in the x direction. An assumption we made at the beginning was that the individual electron and hole currents were continuous functions and constant through the space charge region. The total current is the sum of the electron and hole currents and is constant through the entire junction. Figure 8.7 again shows a plot of the magnitudes of these currents. The total current density in the pn junction is then eDp pn0 eDn np0 eV J Jp(xn) Jn(xp) __ __ exp _a 1 Lp Ln kT (8.25) Equation (8.25) is the ideal current–voltage relationship of a pn junction. We may define a parameter Js as eDp pn0 eDn np0 Js __ __ Lp Ln nea29583_ch08_276-330.indd 287 (8.26) 12/11/10 12:37 PM 288 CHAPTER 8 The pn Junction Diode J p ⴙ n ⴚ Va J J ⴙ ⴚ Va Js Va Figure 8.8 | Ideal I–V characteristic of a pn junction diode. so that Equation (8.25) may be written as eV J Js exp _a 1 kT (8.27) Equation (8.27), known as the ideal-diode equation, gives a good description of the current–voltage characteristics of the pn junction over a wide range of currents and voltages. Although Equation (8.27) was derived assuming a forward-bias voltage (Va 0), there is nothing to prevent Va from being negative (reverse bias). Equation (8.27) is plotted in Figure 8.8 as a function of forward-bias voltage Va. If the voltage Va becomes negative (reverse bias) by a few kTeV, then the reverse-biased current density becomes independent of the reverse-biased voltage. The parameter Js is then referred to as the reverse-saturation current density. The current–voltage characteristics of the pn junction diode are obviously not bilateral. EXAMPLE 8.2 Objective: Determine the ideal reverse-saturation current density in a silicon pn junction at T 300 K. Consider the following parameters in a silicon pn junction: Na Nd 1016 cm3 Dn 25 cm2 /s Dp 10 cm /s 2 ni 1.5 1010 cm3 p0 n0 5 107 s r 11.7 ■ Solution The ideal reverse-saturation current density is given by eDn np0 eDp pn0 Js __ __ Ln Lp nea29583_ch08_276-330.indd 288 12/11/10 12:37 PM 8.1 pn Junction Current 289 which may be rewritten as Dn _ 1 _ n0 Then 1 Js (1.6 1019)(1.5 1010)2 _ 1016 or ___ ___ 1 Js en2i _ Na Nd Dp _ p0 ________ ________ 25 1 __ _ 7 16 5 10 10 10 __ 5 107 Js 4.16 1011 A/cm2 ■ Comment The ideal reverse-biased saturation current density is very small. If the pn junction crosssectional area were A 104 cm2, for example, then the ideal reverse-biased diode current would be Is 4.15 1015 A. ■ EXERCISE PROBLEM Ex 8.2 Consider a GaAs pn junction diode at T 300 K. The parameters of the device are Nd 2 1016 cm3, Na 8 1015 cm3, Dn 210 cm2/s, Dp 8 cm2/s, no 107 s, and po 5 108 s. Determine the ideal reverse-saturation current density. (Ans. Js 3.30 1018 A/cm2) ln (J ) If the forward-bias voltage in Equation (8.27) is positive by more than a few kT eV, then the (1) term in Equation (8.27) becomes negligible. Figure 8.9 shows the forward-bias current–voltage characteristic when the current is plotted on a log scale. Ideally, this plot yields a straight line when Va is greater than a few kT eV. The forward-bias current is an exponential function of the forward-bias voltage. Js Va Figure 8.9 | Ideal I–V characteristic of a pn junction diode with the current plotted on a log scale. nea29583_ch08_276-330.indd 289 12/11/10 12:37 PM 290 CHAPTER 8 The pn Junction Diode EXAMPLE 8.3 Objective: Design a pn junction diode to produce particular electron and hole current densities at a given forward-bias voltage. Consider a silicon pn junction diode at T 300 K. Design the diode such that Jn 20 A /cm2 and Jp 5 A /cm2 at Va 0.65 V. Assume the remaining semiconductor parameters are as given in Example 8.2. ■ Solution The electron diffusion current density is given by Equation (8.24) as kT eDn np0 eV Jn __ exp _a 1 e Ln ___ 2 kT ni eV Dn _ _ exp _a 1 n0 Na Substituting the numbers, we have _________ 0.0259 (1.5 10 ) 25 0.65 1 __ ___ exp __ 7 ⴢ 20 (1.6 1019) 5 10 10 2 Na which yields Na 1.01 1015 cm3 The hole diffusion current density is given by Equation (8.22) as ___ eDp pn0 Dp _ n2i eVa eV __ _ Jp exp 1 e _ exp _a 1 p0 Nd kT Lp kT Substituting the numbers, we have ________ 5 (1.6 10 19 ) 0.0259 (1.5 10 ) 10 0.65 1 __ ___ exp __ 7 ⴢ 5 10 10 2 Nd which yields Nd 2.55 1015 cm3 ■ Comment The relative magnitude of the electron and hole current densities through a diode can be varied by changing the doping concentrations in the device. ■ EXERCISE PROBLEM Ex 8.3 Using the parameters given in Ex 8.2 for the GaAs diode, determine the electron and hole current densities at the space charge edges, and determine the total current density in the diode for a forward-bias voltage of Va 1.05 V. 8.1.6 Summary of Physics [Ans. Jn (xp) 1.20 A/cm2, Jp (xn) 0.1325 A/cm2, JT 1.33 A/cm2] We have been considering the case of a forward-bias voltage being applied to a pn junction. The forward-bias voltage lowers the potential barrier so that electrons and holes are injected across the space charge region. The injected carriers become minority carriers which then diffuse from the junction and recombine with majority carriers. We calculated the minority carrier diffusion current densities at the edge of the space charge region. We can reconsider Equations (8.14) and (8.15) and determine nea29583_ch08_276-330.indd 290 12/11/10 12:37 PM 8.1 pn Junction Current 291 Current density p n JTotal Majority carrier hole current Majority carrier electron current Jn(xp) Jp(xn) Electron diffusion current Hole diffusion current xp x0 xn Figure 8.10 | Ideal electron and hole current components through a pn junction under forward bias. the minority carrier diffusion current densities as a function of distance through the p and n regions. These results are eDp pn0 eV xn x Jp(x) __ exp _a 1 exp __ Lp Lp kT (x xn) (8.28) xp) (8.29) and eDn np0 xp x eV Jn(x) __ exp _a 1 exp __ Ln Ln kT (x The minority carrier diffusion current densities decay exponentially in each region. However, the total current through the pn junction is constant. The difference between total current and minority carrier diffusion current is a majority carrier current. Figure 8.10 shows the various current components through the pn structure. The drift of majority carrier holes in the p region far from the junction, for example, is to supply holes that are being injected across the space charge region into the n region and also to supply holes that are lost by recombination with excess minority carrier electrons. The same discussion applies to the drift of electrons in the n region. We have seen that excess carriers are created in a forward-biased pn junction. From the results of the ambipolar transport theory derived in Chapter 6, the behavior of the excess carriers is determined by the minority carrier parameters for low injection. In determining the current–voltage relationship of the pn junction, we consider the flow of minority carriers since we know the behavior and characteristics of these particles. It may seem strange, at times, that we concern ourselves so much with minority carriers rather than with the vast number of majority carriers, but the reason for this can be found in the results derived from the ambipolar transport theory. nea29583_ch08_276-330.indd 291 12/11/10 12:37 PM 292 CHAPTER 8 The pn Junction Diode The fact that we now have drift current densities in the p and n regions implies that the electric field in these regions is not zero as we had originally assumed. We can calculate the electric field in the neutral regions and determine the validity of our zero-field approximation. EXAMPLE 8.4 Objective: Calculate the electric field in a neutral region of a silicon diode to produce a given majority carrier drift current density. Consider a silicon pn junction at T 300 K with the parameters given in Example 8.2 and with an applied forward-bias voltage Va 0.65 V. ■ Solution The total forward-bias current density is given by eV 1 J Js exp _ kT We determined the reverse-saturation current density in Example 8.2, so we can write 0.65 1 3.295 A /cm2 J (4.155 10 11) exp __ 0.0259 The total current far from the junction in the n region will be majority carrier electron drift current, so we can write J Jn en Nd E The doping concentration is Nd 1016 cm3, and, if we assume n 1350 cm2 /V-s, then the electric field must be Jn 3.295 E __ _____ 1.525 V /cm en Nd (1.6 1019)(1350)(1016) ■ Comment We assumed, in the derivation of the current–voltage equation, that the electric field in the neutral p and n regions was zero. Although the electric field is not zero, this example shows that the magnitude is very small—thus the approximation of zero electric field is very good. ■ EXERCISE PROBLEM Ex 8.4 Determine the electric field in the neutral n region and neutral p region for the GaAs pn junction diode described in Ex 8.3. 8.1.7 Temperature Effects (Ans. En 0.0694 V/cm, Ep 3.25 V /cm) The ideal reverse-saturation current density Js, given by Equation (8.26), is a function of the thermal-equilibrium minority carrier concentrations np0 and pn0. These minority carrier concentrations are proportional to ni2, which is a very strong function of temperature. For a silicon pn junction, the ideal reverse-saturation current density will increase by approximately a factor of 4 for every 10C increase in temperature. nea29583_ch08_276-330.indd 292 12/11/10 12:37 PM 8.1 pn Junction Current 293 The forward-bias current–voltage relation is given by Equation (8.27). This relation includes Js as well as the exp (eVa /kT) factor, making the forward-bias current–voltage relation a function of temperature also. As temperature increases, less forward-bias voltage is required to obtain the same diode current. If the voltage is held constant, the diode current will increase as temperature increases. The change in forward-bias current with temperature is less sensitive than the reverse-saturation current. Objective: Determine the change in the forward-bias voltage on a pn junction with a change EXAMPLE 8.5 in temperature to maintain a constant diode current. Consider a silicon pn junction initially biased at 0.60 V at T 300 K. Assume the temperature increases to T 310 K. Calculate the change in the forward-bias voltage required to maintain a constant current through the junction. ■ Solution The forward-bias current can be written as follows: Eg eV J exp _ exp _a kT kT If the temperature changes, we may take the ratio of the diode currents at the two temperatures. This ratio is exp (Eg kT2) exp (eVa2 kT2) J2 _____ _ exp (Eg kT1) exp (eVa1 kT1) J1 If current is to be held constant, then J1 J2, and we must have Eg eVa2 __ Eg eVa1 __ kT2 kT1 For T1 300 K, T2 310 K, Eg 1.12 eV, and Va1 0.60 V. We then find 1.12 Va2 __ __ 1.12 0.60 310 300 which yields Va2 0.5827 V ■ Comment The change in the forward-bias voltage is 17.3 mV for a 10°C temperature change. ■ EXERCISE PROBLEM Ex 8.5 Repeat Example 8.5 for a GaAs pn junction diode biased at Va 1.050 V for T 300 K. (Ans. 12.3 mV) 8.1.8 The “Short” Diode We assumed in the previous analysis that both p and n regions were long compared with the minority carrier diffusion lengths. In many pn junction structures, one region may, in fact, be short compared with the minority carrier diffusion length. Figure 8.11 shows one such example: the length Wn is assumed to be much smaller than the minority carrier hole diffusion length, Lp. nea29583_ch08_276-330.indd 293 12/11/10 12:37 PM 294 CHAPTER 8 The pn Junction Diode p n Wn xp 0 xn Figure 8.11 | Geometry of a “short” diode. The steady-state excess minority carrier hole concentration in the n region is determined from Equation (8.9), which is given as d 2 (pn) _ p __ 2n 0 dx2 Lp The original boundary condition at x xn still applies, given by Equation (8.11a) as eV pn(xn) pn0 exp _a kT A second boundary condition needs to be determined. In many cases we assume that an ohmic contact exists at x (x n W n), implying an infinite surface-recombination velocity and therefore an excess minority carrier concentration of zero. The second boundary condition is then written as pn(x xn Wn) pn0 (8.30) The general solution to Equation (8.9) is again given by Equation (8.12), which was pn (x) pn(x) pn0 Aex L BexL p (x p xn) In this case, because of the finite length of the n region, both terms of the general solution must be retained. Applying the boundary conditions of Equations (8.11b) and (8.30), the excess minority carrier concentration is given by sinh [(xn Wn x) Lp] eV pn(x) pn0 exp _a 1 ____ kT sinh[Wn Lp] (8.31) Equation (8.31) is the general solution for the excess minority carrier hole concentration in the n region of a forward-biased pn junction. If Wn Lp, the assumption for the long diode, Equation (8.31) reduces to the previous result given by Equation (8.14). If Wn Lp, we can approximate the hyperbolic sine terms by xn Wn x xn Wn x sinh ___ ___ Lp Lp (8.32a) and W W sinh _n _n Lp Lp (8.32b) Then Equation (8.31) becomes x W x ___ W eV pn(x) pn0 exp _a 1 kT nea29583_ch08_276-330.indd 294 n n (8.33) n 12/11/10 12:37 PM 8.2 Generation–Recombination Currents and High-Injection Levels 295 The minority carrier concentration becomes a linear function of distance. The minority carrier hole diffusion current density is given by d[pn(x)] Jp eDp __ dx so that in the short n region, we have eDppn0 eV Jp(x) __ exp _a 1 Wn kT (8.34) The minority carrier hole diffusion current density now contains the length Wn in the denominator, rather than the diffusion length Lp. The diffusion current density is larger for a short diode than for a long diode since Wn Lp. In addition, since the minority carrier concentration is approximately a linear function of distance through the n region, the minority carrier diffusion current density is a constant. This constant current implies that there is no recombination of minority carriers in the short region. TEST YOUR UNDERSTANDING TYU 8.1 The doping concentrations in a GaAs pn junction diode at T 300 K are Nd 5 1015 cm3 and Na 5 1016 cm3. The minority carrier concentration at either space charge edge is to be no larger than 10 percent of the respective majority carrier concentration. Calculate the maximum forward-bias voltage that can be applied to this junction and still meet the required specifications. TYU 8.2 A silicon pn junction at T 300 K has the following parameters: Na 5 1016 cm3, Nd 1 1016 cm3, Dn 25 cm2 /s, Dp 10 cm2 /s, n0 5 107 s, and p0 1 107 s. The cross-sectional area is A 103 cm2 and the forwardbias voltage is Va 0.625 V. Calculate the (a) minority electron diffusion current at the space charge edge, (b) minority hole diffusion current at the space charge edge, and (c) total current in the pn junction diode. TYU 8.3 Consider the silicon pn junction diode described in TYU 8.2. The p region is long and the n region is short with Wn 2 m. (a) Calculate the electron and hole currents in the depletion region. (b) Why has the hole current increased compared to that found in TYU 8.2? [Ans. Va(max) 1.067 V] [Ans. (a) 0.154 mA; (b) 1.09 mA; (c) 1.24 mA] [Ans. (a) In 0.154 mA. IP 5.44 mA; (b) The hole density gradient has increased.] 8.2 | GENERATION–RECOMBINATION CURRENTS AND HIGH-INJECTION LEVELS In the derivation of the ideal current–voltage relationship, we assumed low injection and neglected any effects occurring within the space charge region. High-level injection and other current components generated within the space charge region cause nea29583_ch08_276-330.indd 295 12/11/10 12:37 PM 296 CHAPTER 8 The pn Junction Diode the I–V relationship to deviate from the ideal expression. The additional currents are generated from the recombination processes discussed in Chapter 6. 8.2.1 Generation–Recombination Currents The recombination rate of excess electrons and holes, given by the Shockley–Read– Hall recombination theory, was written as Cn Cp Nt (np n2i ) R _____ (8.35) Cn(n n ) Cp (p p ) The parameters n and p are, as usual, the concentrations of electrons and holes, respectively. Reverse-Biased Generation Current For a pn junction under reverse bias, we have argued that the mobile electrons and holes have essentially been swept out of the space charge region. Accordingly, within the space charge region, n p 0. The recombination rate from Equation (8.35) becomes CnCp Ntn2i R ___ Cn n Cp p (8.36) The negative sign implies a negative recombination rate; hence, we are really generating electron–hole pairs within the reverse-biased space charge region. The recombination of excess electrons and holes is the process whereby we are trying to reestablish thermal equilibrium. Since the concentration of electrons and holes is essentially zero within the reverse-biased space charge region, electrons and holes are being generated via the trap level to also try to reestablish thermal equilibrium. This generation process is schematically shown in Figure 8.12. As the electrons and holes p n E-field Ec ⴚ EFi ⴚ EFp ⴚ Ev ⴚ ⴚ Jgen ⴙ ⴚ Ec EFn ⴙ EFi ⴙ Ev Figure 8.12 | Generation process in a reverse-biased pn junction. nea29583_ch08_276-330.indd 296 12/11/10 12:37 PM 8.2 Generation–Recombination Currents and High-Injection Levels 297 are generated, they are swept out of the space charge region by the electric field. The flow of charge is in the direction of a reverse-biased current. This reverse-biased generation current, caused by the generation of electrons and holes in the space charge region, is in addition to the ideal reverse-biased saturation current. We may calculate the density of the reverse-biased generation current by considering Equation (8.36). If we make a simplifying assumption and let the trap level be at the intrinsic Fermi level, then from Equations (6.92) and (6.97), we have that n ni and p ni. Equation (8.36) now becomes ni R ___ 1 _ 1 _ NtCp NtCn (8.37) Using the definitions of lifetimes from Equations (6.103) and (6.104), we may write Equation (8.37) as ni R __ p0 n0 (8.38) If we define a new lifetime as the average of p0 and n0, or p0 n0 0 __ 2 (8.39) then the recombination rate can be written as n R _i 20 G (8.40) The negative recombination rate implies a generation rate, so G is the generation rate of electrons and holes in the space charge region. The generation current density may be determined from Jgen W e Gdx (8.41) 0 where the integral is over the space charge region. If we assume that the generation rate is constant throughout the space charge region, then we obtain eniW Jgen _ 20 (8.42) The total reverse-biased current density is the sum of the ideal reverse saturation current density and the generation current density, or JR Js Jgen (8.43) The ideal reverse-saturation current density Js is independent of the reverse-biased voltage. However, Jgen is a function of the depletion width W, which in turn is a function of the reverse-biased voltage. The actual reverse-biased current density, then, is no longer independent of the reverse-biased voltage. nea29583_ch08_276-330.indd 297 12/11/10 12:37 PM 298 CHAPTER 8 The pn Junction Diode EXAMPLE 8.6 Objective: Determine the relative magnitudes of the ideal reverse-saturation current density and the generation current density in a reverse-biased pn junction. Consider a silicon pn junction at T 300 K with parameters Dn 25 cm2 /s, Dp 10 cm2 /s, Na Nd 1016 cm3, and 0 n0 p0 5 107 s. Assume the diode is reverse biased at VR 5 V. ■ Solution The ideal reverse-saturation current density was calculated in Example 8.2 and was found to be Js 4.155 1011 A /cm2. The built-in potential is found as (1016)(1016) Na Nd Vbi Vt ln _ (0.0259) ln ___ 0.695 V n2i (1.5 1010)2 The depletion width is found to be 2 ∈s (Vbi VR) __ Na Nd W ___ e Na Nd 1 2 2(11.7)(8.85 1014)(0.695 5) __ 1016 1016 ______ 1.6 1019 (1016)(1016) 1 2 1.214 104 cm The generation current density is then found to be (1.6 1019)(1.5 1010)(1.214 104) eniW _______ Jgen _ 20 2(5 107) or Jgen 2.914 107 A /cm2 The ratio of the two currents is Jgen ___ _ 2.914 1011 7 Js 4.155 10 7 103 ■ Comment Comparing the solutions for the two current densities, it is obvious that, for the silicon pn junction diode at room temperature, the generation current density is approximately four orders of magnitude larger than the ideal saturation current density. The generation current is the dominant reverse-biased current in a silicon pn junction diode. ■ EXERCISE PROBLEM Ex 8.6 Consider a GaAs pn junction diode at T 300 K with parameters Nd 8 1016 cm3, Na 2 1015 cm3, Dn 207 cm2/s, Dp 9.80 cm2/s, and 0 p0 n0 5 108 s. (a) Calculate the ideal reverse-biased saturation current density. (b) Find the reverse-biased generation current density if the diode is reverse biased at VR 5 V. (c) Determine the ratio of Jgen to Js. [Ans. (a) 1.677 1017 A /cm2; (b) 6.166 1010 A /cm2; (c) 3.68 107] nea29583_ch08_276-330.indd 298 12/11/10 12:37 PM 8.2 Generation–Recombination Currents and High-Injection Levels 299 Forward-Bias Recombination Current For the reverse-biased pn junction, electrons and holes are essentially completely swept out of the space charge region so that n p 0. Under forward bias, however, electrons and holes are injected across the space charge region, so we do, in fact, have some excess carriers in the space charge region. The possibility exists that some of these electrons and holes will recombine within the space charge region and not become part of the minority carrier distribution. The recombination rate of electrons and holes is again given from Equation (8.35) as CnCp Nt np n2i R _____ Cn(n n ) Cp( p p ) Dividing both numerator and denominator by CnCp Nt and using the definitions of n0 and p0, we may write the recombination rate as np n2i R _____ p0 (n n ) n0 (p p ) (8.44) Figure 8.13 shows the energy-band diagram of the forward-biased pn junction. Shown in the figure are the intrinsic Fermi level and the quasi-Fermi levels for electrons and holes. From the results of Chapter 6, we may write the electron concentration as EFn EFi n ni exp __ kT (8.45) (8.46) and the hole concentration as EFi EFp p ni exp __ kT where EFn and EFp are the quasi-Fermi levels for electrons and holes, respectively. p n Ec EFn Ec EFn EFi EFi EFi EFp Ev EFp Ev x0 Figure 8.13 | Energy-band diagram of a forward-biased pn junction including quasi-Fermi levels. nea29583_ch08_276-330.indd 299 12/11/10 12:37 PM 300 CHAPTER 8 The pn Junction Diode Relative recombination rate 6 5 4 3 2 1 0 1 2 3 4 5 6 Relative distance through space charge region Figure 8.14 | Relative magnitude of the recombination rate through the space charge region of a forward-biased pn junction. From Figure 8.13, we may note that (EFn EFi) (EFi EFp) eVa (8.47) where Va is the applied forward-bias voltage. Again, if we assume that the trap level is at the intrinsic Fermi level, then n p ni. Figure 8.14 shows a plot of the relative magnitude of the recombination rate as a function of distance through the space charge region. This plot was generated using Equations (8.44), (8.45), (8.46), and (8.47). A very sharp peak occurs at the metallurgical junction (x 0). At the center of the space charge region, we have eV EFn EFi EFi EFp _a 2 (8.48) Equations (8.45) and (8.46) then become (8.49) (8.50) eV n ni exp _a 2kT and eV p ni exp _a 2kT If we assume that n p ni and that n0 p0 0, then Equation (8.44) becomes [exp (eVa kT) 1] ni ____ Rmax _ (8.51) 20 [exp (eVa 2kT) 1] which is the maximum recombination rate for electrons and holes that occurs at the center of the forward-biased pn junction. If we assume that V a kT /e, we may nea29583_ch08_276-330.indd 300 12/11/10 12:37 PM 8.2 Generation–Recombination Currents and High-Injection Levels 301 neglect the (1) term in the numerator and the (1) term in the denominator. Equation (8.51) then becomes ni eV Rmax _ exp _a 20 2kT (8.52) The recombination current density may be calculated from W Jrec eR dx (8.53) 0 where again the integral is over the entire space charge region. In this case, however, the recombination rate is not a constant through the space charge region. We have calculated the maximum recombination rate at the center of the space charge region, so we may write ni eV Jrec ex _ exp _a (8.54) 20 2kT where x is a length over which the maximum recombination rate is effective. However, since 0 may not be a well-defined or known parameter, it is customary to write eW n eV eV Jrec _i exp _a Jr 0 exp _a 20 2kT 2kT (8.55) where W is the space charge width. Total Forward-Bias Current The total forward-bias current density in the pn junction is the sum of the recombination and the ideal diffusion current densities. Figure 8.15 shows a plot of the minority carrier hole concentration in the neutral p n Recombination p pn(0) pn0 exp ( ) ( ) eVa kT pn(x)␣ exp x Lp pn(0) pn0 x0 Figure 8.15 | Because of recombination, additional holes from the p region must be injected into the space charge region to establish the minority carrier hole concentration in the n region. nea29583_ch08_276-330.indd 301 12/11/10 12:37 PM 302 CHAPTER 8 The pn Junction Diode n region. This distribution yields the ideal hole diffusion current density and is a function of the minority carrier hole diffusion length and the applied junction voltage. The distribution is established as a result of holes being injected across the space charge region. If, now, some of the injected holes in the space charge region are lost due to recombination, then additional holes must be injected from the p region to make up for this loss. The flow of these additional injected carriers, per unit time, results in the recombination current. This added component is schematically shown in the figure. The total forward-bias current density is the sum of the recombination and the ideal diffusion current densities, so we can write J Jrec JD (8.56) where Jrec is given by Equation (8.55) and JD is given by eV JD Js exp _a kT (8.57) The (1) term in Equation (8.27) has been neglected. The parameter Js is the ideal reverse-saturation current density, and from previous discussion, the value of Jr0 from the recombination current is larger than the value of Js. If we take the natural log of Equations (8.55) and (8.57), we obtain eV Va ln Jrec ln Jr0 _a ln Jr0 _ 2Vt 2kT (8.58a) eV V ln JD ln Js _a ln Js _a Vt kT (8.58b) and Figure 8.16 shows the recombination and diffusion current components plotted on a log current scale as a function of Va /Vt. The slopes of the two curves are not the same. Also shown in the figure is the total current density—the sum of the two current components. We may notice that, at a low current density, the recombination current dominates, and at a higher current density, the ideal diffusion current dominates. In general, the diode current–voltage relationship may be written as eV I Is exp _a 1 nkT (8.59) where the parameter n is called the ideality factor. For a large forward-bias voltage, n 1 when diffusion dominates, and for low forward-bias voltage, n 2 when recombination dominates. There is a transition region where 1 n 2. 8.2.2 High-Level Injection In the derivation of the ideal diode I–V relationship, we assumed that low injection was valid. Low injection implies that the excess minority carrier concentrations are always much less than the majority carrier concentration. nea29583_ch08_276-330.indd 302 12/11/10 12:37 PM ln (J) 8.2 Generation–Recombination Currents and High-Injection Levels 303 Total current Ideal diffusion current, JD (slope 1) Recombination current, Jrec 1 (slope 2 ) ln (JR0) ln (Js) eVa kT Figure 8.16 | Ideal diffusion, recombination, and total current in a forward-biased pn junction. However, as the forward-bias voltage increases, the excess carrier concentrations increase and may become comparable or even greater than the majority carrier concentration. From Equation (8.18), we can write Va np ni2 exp _ Vt We have that n no n and p po p, so that V (no n)(po p) ni2 exp _a Vt (8.60) Under high-level injection, we may have n no and p po so that Equation (8.60) becomes approximately (861) (8.62) (n)(p) Va ni2 exp _ Vt n p Va ni exp _ 2Vt Since n p, then The diode current is proportional to the excess carrier concentration so that, under high-level injection, we have Va I exp _ 2Vt nea29583_ch08_276-330.indd 303 (8.63) 12/11/10 12:37 PM CHAPTER 8 The pn Junction Diode I (leg Scale) 304 a Recombination c High-level injection b Ideal Va Figure 8.17 | Forward-bias current versus voltage from low forward bias to high forward bias. In the high-level injection region, it takes a larger increase in diode voltage to produce a given increase in diode current. The diode forward-bias current, from low-bias levels to high-bias levels, is plotted in Figure 8.17. This plot shows the effect of recombination at low-bias voltages and high-level injection at high-bias voltages. TEST YOUR UNDERSTANDING TYU 8.4 Consider a silicon pn junction diode at T 300 K with parameters Na 2 1015 cm3, Nd 8 1016 cm3, Dp 10 cm2 /s, Dn 25 cm2 /s, and 0 p0 n0 107 s. The diode is forward biased at Va 0.35 V. (a) Calculate the ideal diode current density. (b) Find the forward-biased recombination current density. (c) Determine the ratio of recombination current to the ideal diffusion current. [Ans. (a) 2.137 104 A /cm2; (b) 5.020 104 A /cm2; (c) 2.35] 8.3 | SMALL-SIGNAL MODEL OF THE pn JUNCTION We have been considering the dc characteristics of the pn junction diode. When semiconductor devices with pn junctions are used in linear amplifier circuits, for example, sinusoidal signals are superimposed on the dc currents and voltages, so that the small-signal characteristics of the pn junction become important. nea29583_ch08_276-330.indd 304 12/11/10 12:37 PM 8.3 8.3.1 Small-Signal Model of the pn Junction 305 Diffusion Resistance The ideal current–voltage relationship of the pn junction diode was given by Equation (8.27), where J and Js are current densities. If we multiply both sides of the equation by the junction cross-sectional area, we have eV ID Is exp _a 1 kT (8.64) where ID is the diode current and Is is the diode reverse-saturation current. Assume that the diode is forward-biased with a dc voltage V0 producing a dc diode current IDQ. If we now superimpose a small, low-frequency sinusoidal voltage as shown in Figure 8.18, then a small sinusoidal current will be produced, superimposed on the dc current. The ratio of sinusoidal current to sinusoidal voltage is called the incremental conductance. In the limit of a very small sinusoidal current and voltage, the small-signal incremental conductance is just the slope of the dc current–voltage curve, or dID gd _ dVa (8.65) VaV0 The reciprocal of the incremental conductance is the incremental resistance, defined as dV rd _a dID (8.66) IDIDQ where IDQ is the dc quiescent diode current. I 1 Slope r d I IQ Is V0 Va V Figure 8.18 | Curve showing the concept of the small-signal diffusion resistance. nea29583_ch08_276-330.indd 305 12/11/10 12:37 PM 306 CHAPTER 8 The pn Junction Diode If we assume that the diode is biased sufficiently far in the forward-bias region, then the (1) term can be neglected and the incremental conductance becomes IDQ eV0 dID e I exp _ gd _ _ _ Vt dVa V V kT s kT a 0 (8.67) The small-signal incremental resistance is then the reciprocal function, or V rd _t IDQ (8.68) The incremental resistance decreases as the bias current increases, and is inversely proportional to the slope of the I–V characteristic as shown in Figure 8.18. The incremental resistance is also known as the diffusion resistance. 8.3.2 Small-Signal Admittance In the last chapter, we considered the pn junction capacitance as a function of the reverse-biased voltage. When the pn junction diode is forward-biased, another capacitance becomes a factor in the diode admittance. The small-signal admittance, or impedance, of the pn junction under forward bias is derived using the minority carrier diffusion current relations we have already considered. Qualitative Analysis Before we delve into the mathematical analysis, we can qualitatively understand the physical processes that lead to a diffusion capacitance, which is one component of the junction admittance. Figure 8.19a schematically shows a pn junction forward biased with a dc voltage. A small ac voltage is also Va p p n pn0 exp n Holes (a) Vdc t2 t0 t1 p Vdc v^ Vt ) Vdc v^ Vt ) Time pn0 exp vac v^ sin t ( ( x0 (b) n t t1 t t0 t t2 pn0 (c) x0 Figure 8.19 | (a) A pn junction with an ac voltage superimposed on a forward-biased dc value; (b) the hole concentration versus time at the space charge edge; (c) the hole concentration versus distance in the n region at three different times. nea29583_ch08_276-330.indd 306 12/11/10 12:37 PM 8.3 Small-Signal Model of the pn Junction 307 superimposed on the dc voltage so that the total forward-biased voltage can be written as Va Vdc ˆ sin t. As the voltage across the junction changes, the number of holes injected across the space charge region into the n region also changes. Figure 8.19b shows the hole concentration at the space charge edge as a function of time. At t t0, the ac voltage is zero so that the concentration of holes at x 0 is just given by pn(0) pn0 exp (Vdc Vt), which is what we have seen previously. Now, as the ac voltage increases during its positive half cycle, the concentration of holes at x 0 will increase and reach a peak value at t t1, which corresponds to the peak value of the ac voltage. When the ac voltage is on its negative half cycle, the total voltage across the junction decreases so that the concentration of holes at x 0 decreases. The concentration reaches a minimum value at t t2, which corresponds to the time that the ac voltage reaches its maximum negative value. The minority carrier hole concentration at x 0, then, has an ac component superimposed on the dc value as indicated in Figure 8.19b. As previously discussed, the holes at the space charge edge (x 0) diffuse into the n region where they recombine with the majority carrier electrons. We assume that the period of the ac voltage is large compared to the time it takes carriers to diffuse into the n region. The hole concentration as a function of distance into the n region can then be treated as a steady-state distribution. Figure 8.19c shows the steady-state hole concentrations at three different times. At t t0, the ac voltage is zero, so the t t0 curve corresponds to the hole distribution established by the dc voltage. The t t1 curve corresponds to the distribution established when the ac voltage has reached its peak positive value, and the t t2 curve corresponds to the distribution established when the ac voltage has reached its maximum negative value. The shaded areas represents the charge Q that is alternately charged and discharged during the ac voltage cycle. Exactly the same process is occurring in the p region with the electron concentration. The mechanism of charging and discharging of holes in the n region and electrons in the p region leads to a capacitance. This capacitance is called diffusion capacitance. The physical mechanism of this diffusion capacitance is different from that of the junction capacitance discussed in the last chapter. We show that the magnitude of the diffusion capacitance in a forward-biased pn junction is usually substantially larger than the junction capacitance. Mathematical Analysis The minority carrier distribution in the pn junction will be derived for the case when a small sinusoidal voltage is superimposed on the dc junction voltage. We can then determine small signal, or ac, diffusion currents from these minority carrier functions. Figure 8.20 shows the minority carrier distribution in a pn junction when a forward-biased dc voltage is applied. The origin, x 0, is set at the edge of the space charge region on the n side for convenience. The minority carrier hole concentration at x 0 is given by Equation (8.7) as pn(0) pn0 exp (eVa kT), where Va is the applied voltage across the junction. Now let Va V0 v1(t) nea29583_ch08_276-330.indd 307 (8.69) 12/11/10 12:37 PM 308 CHAPTER 8 The pn Junction Diode p n pn(0) pn0 exp np(x) [ ] eVa kT pn(x) np0 pn0 x0 Figure 8.20 | The dc characteristics of a forward-biased pn junction used in the small-signal admittance calculations. where V0 is the dc quiescent bias voltage and v1(t) is the ac signal voltage that is superimposed on this dc level. We may now write e[V0 v1(t)] pn(x 0) pn0 exp ___ pn(0, t) kT (8.70) Equation (8.70) may be written as ev1(t) pn(0, t) pdc exp _ kT (8.71) where eV pdc pn0 exp _0 kT (8.72) If we assume that v1(t) (kT e) Vt, then the exponential term in Equation (8.71) may be expanded into a Taylor series retaining only the linear terms, and the minority carrier hole concentration at x 0 can be written as v1(t) pn(0, t) pdc 1 _ Vt (8.73) If we assume that the time-varying voltage v1(t) is a sinusoidal signal, we can write Equation (8.73) as V̂ pn(0, t) pdc 1 _1 e jt Vt (8.74) whereV̂1 is the phasor of the applied sinusoidal voltage. Equation (8.74) will be used as the boundary condition in the solution of the time-dependent diffusion equation for the minority carrier holes in the n region. In the neutral n region (x 0), the electric field is assumed to be zero; thus, the behavior of the excess minority carrier holes is determined from the equation 2(pn) _ pn (pn) Dp __ p0 __ t x2 nea29583_ch08_276-330.indd 308 (8.75) 12/11/10 12:37 PM 8.3 Small-Signal Model of the pn Junction 309 where pn is the excess hole concentration in the n region. We are assuming that the ac signal voltage v1 (t) is sinusoidal. We then expect the steady-state solution for pn to be of the form of a sinusoidal solution superimposed on the dc solution, or pn(x, t) p0(x) p1(x)ejt (8.76) where p0(x) is the dc excess carrier concentration and p1(x) is the magnitude of the ac component of the excess carrier concentration. The expression for p0(x) is the same as that given in Equation (8.14). Substituting Equation (8.76) into the differential Equation (8.75), we obtain 2 p0(x) __ 2p1(x) jt p0(x) p1(x)ejt Dp __ e ___ (8.77) jp1(x)ejt 2 2 p0 x x We may rewrite this equation, combining the time-dependent and time-independent terms, as Dp p0(x) __ p0(x) p1(x) _ p1(x) ___ p0 Dp __ p0 jp1(x) ejt 0 2 2 2 x 2 x (8.78) If the ac component, p1(x), is zero, then the first bracketed term is just the differential Equation (8.10), which is identically zero. Then we have, from the second bracketed term, d 2p1(x) _ p1(x) Dp __ (8.79) p0 jp1(x) 0 dx2 Noting that L2p Dpp0, Equation (8.79) may be rewritten in the form (1 jp0) d p1(x) __ __ p1(x) 0 2 2 2 dx Lp (8.80) or 2 d p1(x) __ dx2 Cp p1(x) 0 2 (8.81) where (1 jp0) C2p __ L2p (8.82) The general solution to Equation (8.81) is p1(x) K1eC x K2eC x p p (8.83) One boundary condition is that p1(x → ) 0, which implies that the coefficient K2 0. Then p1(x) K1eC x p (8.84) Applying the boundary condition at x 0 from Equation (8.74), we obtain V̂ p1(0) K1 pdc _1 Vt nea29583_ch08_276-330.indd 309 (8.85) 12/11/10 12:37 PM 310 CHAPTER 8 The pn Junction Diode The hole diffusion current density can be calculated at x 0. This is given by pn Jp eDp _ x (8.86) x0 If we consider a homogeneous semiconductor, the derivative of the hole concentration will be just the derivative of the excess hole concentration. Then [p0(x)] (pn) p1(x) eDp __ eDp __ e jt Jp eDp __ x0 x x x 0 x x 0 (8.87) We can write this equation in the form Jp Jp0 jp(t) (8.88) where [p0(x)] Jp0 eDp __ x x0 eDp pn0 eV __ exp _0 1 Lp kT (8.89) Equation (8.89) is the dc component of the hole diffusion current density and is exactly the same as in the ideal I–V relation derived previously. The sinusoidal component of the diffusion current density is then found from p1(x) jt jp(t) Jˆpejt eDp __ (8.90) x e x 0 where Jˆp is the current density phasor. Combining Equations (8.90), (8.84), and (8.85), we have V̂ Jˆp eDp(Cp) pdc _1 ec x Vt x0 p We can write the total ac hole current phasor as (8.91) V̂ Iˆp A Jˆp eADpCppdc _1 (8.92) Vt where A is the cross-sectional area of the pn junction. Substituting the expression for Cp, we obtain eADp pdc ________ V̂ Iˆp __ 1 jp0 _1 (8.93) Lp Vt If we define eADp pdc eADp pn0 eV Ip0 __ __ exp _0 Lp Lp kT (8.94) then Equation (8.93) becomes Iˆp Ip0 ________ V̂ 1 jp 0 _1 Vt (8.95) Going through the same type of analysis for the minority carrier electrons in the p region, we obtain ________ V̂ Iˆn In0 1 jn0 _1 (8.96) Vt nea29583_ch08_276-330.indd 310 12/11/10 12:37 PM 8.3 Small-Signal Model of the pn Junction 311 where eADn np0 eV In0 __ exp _0 (8.97) Ln kT The total ac current phasor is the sum of Iˆp and Iˆn. The pn junction admittance is the total ac current phasor divided by the ac voltage phasor, or ˆp Iˆn ________ ________ Iˆ I_ 1 I Y_ _ 1 jp0 In0 1 jn0 (8.98) p0 Vt V̂1 V̂1 There is not a linear, lumped, finite, passive, bilateral network that can be synthesized to give this admittance function. However, we may make the following approximations. Assume that p0 1 (8.99a) and n0 1 (8.99b) These two assumptions imply that the frequency of the ac signal is not too large. Then we may write ________ jp0 1 jp0 1 _ (8.100a) 2 and ________ jn0 1 jn0 1 _ 2 (8.100b) Substituting Equations (8.100a) and (8.100b) into the admittance Equation (8.98), we obtain jp0 jn0 1 I 1_ Y _ In0 1 _ (8.101) p0 Vt 2 2 If we combine the real and imaginary portions, we get 1 (I I ) j Y _ n0 Vt p0 1 (I _ 2V p0 p0 t In0n0) (8.102) Equation (8.102) may be written in the form Y gd jCd (8.103) The parameter gd is called the diffusion conductance and is given by IDQ 1 (I I ) _ gd _ n0 Vt p0 Vt (8.104) where IDQ is the dc bias current. Equation (8.104) is exactly the same conductance as we obtained previously in Equation (8.67). The parameter Cd is called the diffusion capacitance and is given by 1 (I I ) Cd _ n0 n0 2Vt p0 p0 nea29583_ch08_276-330.indd 311 (8.105) 12/11/10 12:37 PM 312 CHAPTER 8 The pn Junction Diode p region pn(0) pn0 exp [ e (V ^ ) kT 0 n region ] pn(0) pn0 exp [ pn(0) pn0 exp Q e (V ^ ) kT 0 ] [ ] eV0 kT Q pn0 np0 x0 Figure 8.21 | Minority carrier concentration changes with changing forward-bias voltage. The physics of the diffusion capacitance may be seen in Figure 8.21. The dc values of the minority carrier concentrations are shown along with the changes due to the ac component of voltage. The Q charge is alternately being charged and discharged through the junction as the voltage across the junction changes. The change in the stored minority carrier charge as a function of the change in voltage is the diffusion capacitance. One consequence of the approximations p0 1 and n0 1 is that there are no “wiggles” in the minority carrier curves. The sinusoidal frequency is low enough so that the exponential curves are maintained at all times. EXAMPLE 8.7 Objective: Calculate the small-signal admittance parameters of a pn junction diode. This example is intended to give an indication of the magnitude of the diffusion capacitance as compared with the junction capacitance considered in the last chapter. The diffusion resistance will also be calculated. Assume that Na Nd so that pn0 np0. This assumption implies that Ip0 In0. Let T 300 K, p0 107 s, and Ip0 IDQ 1 mA. ■ Solution The diffusion capacitance, with these assumptions, is given by 1 (I ) __ 1 Cd _ (103)(107) 1.93 109 F 2Vt p0 p0 (2)(0.0259) The diffusion resistance is V 0.0259 V 25.9 rd _t __ IDQ 1 mA ■ Comment The value of 1.93 nF for the diffusion capacitance of a forward-biased pn junction is three to four orders of magnitude larger than the junction capacitance of the reverse-biased pn junction, which we calculated in Example 7.5. nea29583_ch08_276-330.indd 312 12/11/10 12:37 PM 8.3 Small-Signal Model of the pn Junction 313 ■ EXERCISE PROBLEM Ex 8.7 A silicon pn junction diode at T 300 K has the following parameters: Nd 8 1016 cm3, Na 2 1015 cm3, Dn 25 cm2 /s, Dp 10 cm2/s, n0 5 107 s, and p0 107 s. The cross-sectional area is A 103 cm2. Determine the diffusion resistance and diffusion capacitance if the diode is forward biased at (a) Va 0.550 V and (b) Va 0.610 V. [Ans. (a) rd 118 , Cd 2.07 nF; (b) rd 11.6 , Cd 20.9 nF] The diffusion capacitance tends to dominate the capacitance terms in a forwardbiased pn junction. The small-signal diffusion resistance can be fairly small if the diode current is a fairly large value. As the diode current decreases, the diffusion resistance increases. We will consider the impedance of forward-biased pn junctions again when we discuss bipolar transistors. 8.3.3 Equivalent Circuit The small-signal equivalent circuit of the forward-biased pn junction is derived from Equation (8.103). This circuit is shown in Figure 8.22a. We need to add the junction capacitance, which will be in parallel with the diffusion resistance and diffusion capacitance. The last element we add, to complete the equivalent circuit, is a series resistance. The neutral n and p regions have finite resistances so the actual pn junction will include a series resistance. The complete equivalent circuit is given in Figure 8.22b. The voltage across the actual junction is V a and the total voltage applied to the pn diode is given by V app. The junction voltage V a is the voltage in the ideal current–voltage expression. We can write the expression Vapp Va Irs (8.106) Figure 8.23 is a plot of the current–voltage characteristic from Equation (8.106) showing the effect of the series resistance. A larger applied voltage is required to rd rs ID Cd Cj rd Va Vapp Cd (a) (b) Figure 8.22 | (a) Small-signal equivalent circuit of ideal forwardbiased pn junction diode; (b) complete small-signal equivalent circuit of pn junction. nea29583_ch08_276-330.indd 313 12/11/10 12:37 PM CHAPTER 8 The pn Junction Diode Effect of rs ln (I ) 314 Ideal Vapp Figure 8.23 | Forward-biased I–V characteristics of a pn junction diode showing the effect of series resistance. achieve the same current value when a series resistance is included. In most diodes, the series resistance will be negligible. In some semiconductor devices with pn junctions, however, the series resistance will be in a feedback loop; in these cases, the resistance is multiplied by a gain factor and becomes non-negligible. TEST YOUR UNDERSTANDING TYU 8.5 A GaAs pn junction diode at T 300 K has the same parameters given in Ex 8.7 except that Dn 207 cm2/s and Dp 9.80 cm2/s. Determine the diffusion resistance and diffusion capacitance if the diode is forward biased at (a) Va 0.970 V and (b) Va 1.045 V. [Ans. (a) rd 263 , Cd 0.940 nF; (b) rd 14.6 , Cd 17.0 nF] TYU 8.6 A silicon pn junction diode at T 300 K has the same parameters as those described in Ex 8.7. The neutral n-region and neutral p-region lengths are 0.01 cm. Estimate the series resistance of the diode (neglect ohmic contacts). (Ans. R 66 ) *8.4 | CHARGE STORAGE AND DIODE TRANSIENTS The pn junction is typically used as an electrical switch. In forward bias, referred to as the on state, a relatively large current can be produced by a small applied voltage; in reverse bias, referred to as the off state, only a very small current will exist. Of primary interest in circuit applications is the speed of the pn junction diode in switching states. We qualitatively discuss the transients that occur and the charge storage effects. We simply state the equations that describe the switching times without any mathematical derivations. nea29583_ch08_276-330.indd 314 12/11/10 12:37 PM 8.4 Va Charge Storage and Diode Transients 315 I p n t0 IF RF RR IR ⴙ ⴚ ⴚ ⴙ VF VR Figure 8.24 | Simple circuit for switching a diode from forward to reverse bias. 8.4.1 The Turn-off Transient Suppose we want to switch a diode from the forward bias on state to the reversebiased off state. Figure 8.24 shows a simple circuit that will switch the applied bias at t 0. For t 0, the forward-bias current is VF Va I IF __ (8.107) RF The minority carrier concentrations in the device, for the applied forward voltage VF, are shown in Figure 8.25a. There is excess minority carrier charge stored in both the p and n regions of the diode. The excess minority carrier concentrations at the space charge edges are supported by the forward-bias junction voltage Va. When the voltage is switched from the forward- to the reverse-biased state, the excess minority carrier concentrations at the space charge edges can no longer be supported and they start to decrease, as shown in Figure 8.25b. The collapse of the minority carrier concentrations at the edges of the space charge region leads to large concentration gradients and diffusion currents in the reverse-biased direction. If we assume, for the moment, that the voltage across the diode junction is small compared with VR, then the reverse-biased current is limited to approximately V I IR _R RR (8.108) The junction capacitances do not allow the junction voltage to change instantaneously. If the current IR were larger than this value, there would be a forward-bias voltage across the junction, which would violate our assumption of a reverse-biased current. nea29583_ch08_276-330.indd 315 12/11/10 12:37 PM 316 CHAPTER 8 n p np(x 0) np0 exp The pn Junction Diode ( ) eVa kT pn(x 0) pn0 exp Forward bias diffusion of electrons ( ) eVa kT Forward bias diffusion of holes pn(x) np(x ) np0 pn0 x 0 x0 x x (a) t 0 t 0 t t1 t t1 t2 t2 ts t4 t t3 t3 Reverse bias diffusion of electrons Reverse bias diffusion of holes t4 ts IF Time t (b) Figure 8.25 | (a) Steady-state forward-bias minority carrier concentrations; (b) minority carrier concentrations at various times during switching. t2 IR ts 0.1IR Figure 8.26 | Current characteristic versus time during diode switching. If the current IR were smaller than this value, there would be a reverse-biased voltage across the junction, which means that the junction voltage would have changed instantaneously. Since the reverse current is limited to the value given by Equation (8.108), the reverse-biased density gradient is constant; thus, the minority carrier concentrations at the space charge edge decrease with time as shown in Figure 8.25b. This reverse current IR will be approximately constant for 0 t ts, where ts is called the storage time. The storage time is the length of time required for the minority carrier concentrations at the space charge edge to reach the thermal-equilibrium values. After this time, the voltage across the junction will begin to change. The current characteristic is shown in Figure 8.26. The reverse current is the flow of the stored minority carrier charge, which is the difference between the minority carrier concentrations at t 0 and t , as shown in Figure 8.25b. nea29583_ch08_276-330.indd 316 12/11/10 12:37 PM 8.4 Charge Storage and Diode Transients 317 The storage time ts can be determined by solving the time-dependent continuity equation. If we consider a one-sided pn junction, the storage time is determined from the equation ___ erf ts IF _ __ (8.109) IF IR p0 where erf (x) is known as the error function. An approximate solution for the storage time can be obtained as I (8.110) ts p 0 ln 1 _F IR The recovery phase for t ts is the time required for the junction to reach its steady-state reverse-biased condition. The remainder of the excess charge is being removed and the space charge width is increasing to the reverse-biased value. The decay time t2 is determined from ___ erf I exp (t2 p 0) t2 IR _ ___ ______ 1 0.1 _ p0 t2 p 0 (8.111) F The total turn-off time is the sum of ts and t2. To switch the diode quickly, we need to be able to produce a large reverse current as well as have a small minority carrier lifetime. In the design of diode circuits, then, the designer must provide a path for the transient reverse-biased current pulse in order to be able to switch the diode quickly. These same effects will be considered when we discuss the switching of bipolar transistors. 8.4.2 The Turn-on Transient The turn-on transient occurs when the diode is switched from its “off” state into the forward-bias “on” state. The turn-on can be accomplished by applying a forwardbias current pulse. The first stage of turn-on occurs very quickly and is the length of time required to narrow the space charge width from the reverse-biased value to its thermal-equilibrium value when Va 0. During this time, ionized donors and acceptors are neutralized as the space charge width narrows. The second stage of the turn-on process is the time required to establish the minority carrier distributions. During this time the voltage across the junction is increasing toward its steady-state value. A small turn-on time is achieved if the minority carrier lifetime is small and if the forward-bias current is small. TEST YOUR UNDERSTANDING TYU 8.7 A one-sided pn silicon diode, which has a forward-bias current of IF 1.75 mA, is switched to reverse bias with an effective reverse-biased voltage of VR 2 V and an effective series resistance of RR 4 k. The minority carrier hole lifetime is 107 s. (a) Determine the storage time ts. (b) Calculate the decay time t2. (c) What is the turn-off time of the diode? [Ans. (a) 0.746 107 s; (b) 1.25 107 s; (c) 2 107 s] nea29583_ch08_276-330.indd 317 12/11/10 12:37 PM 318 CHAPTER 8 The pn Junction Diode *8.5 | THE TUNNEL DIODE The tunnel diode is a pn junction in which both the n and p regions are degenerately doped. As we discuss the operation of this device, we will find a region that exhibits a negative differential resistance. The tunnel diode was used in oscillator circuits in the past, but other types of solid-state devices are now used as high-frequency oscillators; thus, the tunnel diode is really only of academic interest. Nevertheless, this device does demonstrate the phenomenon of tunneling we discussed in Chapter 2. Recall the degenerately doped semiconductors we discussed in Chapter 4: the Fermi level is in the conduction band of a degenerately doped n-type material and in the valence band of a degenerately doped p-type material. Then, even at T 0 K, electrons will exist in the conduction band of the n-type material, and holes (empty states) will exist in the p-type material. Figure 8.27 shows the energy-band diagram of a pn junction in thermal equilibrium for the case when both the n and p regions are degenerately doped. The depletion region width decreases as the doping increases and may be on the order of approximately 100 Å for the case shown in Figure 8.27. The potential barrier at the junction can be approximated by a triangular potential barrier, as shown in Figure 8.28. This potential barrier is similar to the potential barrier used in Chapter 2 to illustrate the tunneling phenomenon. The barrier width is small and the electric field in the space charge region is quite large; thus, a finite probability exists that an electron may tunnel through the forbidden band from one side of the junction to the other. We may qualitatively determine the current–voltage characteristics of the tunnel diode by considering the simplified energy-band diagrams in Figure 8.29. n region Potential energy V(x) p region Ec Ev EF EF Ec x Ev Space charge region Figure 8.27 | Energy-band diagram of a pn junction in thermal equilibrium in which both the n and p regions are degenerately doped. nea29583_ch08_276-330.indd 318 Space charge region Figure 8.28 | Triangular potential barrier approximation of the potential barrier in the tunnel diode. 12/11/10 12:37 PM 8.5 The Tunnel Diode 319 I V (a) I e V (b) I e V e (c) Figure 8.29 | Simplified energy-band diagrams and I–V characteristics of the tunnel diode at (a) zero bias; (b) a slight forward bias; (c) a forward bias producing maximum tunneling current. (continued) nea29583_ch08_276-330.indd 319 12/11/10 12:37 PM 320 CHAPTER 8 The pn Junction Diode I e V (d) I e V (e) Figure 8.29 | (concluded) (d) A higher forward bias showing less tunneling current; (e) a forward bias for which the diffusion current dominates. Figure 8.29a shows the energy-band diagram at zero bias, which produces zero current on the I–V diagram. If we assume, for simplicity, that we are near 0 K, then all energy states are filled below E F on both sides of the junction. Figure 8.29b shows the situation when a small forward-bias voltage is applied to the junction. Electrons in the conduction band of the n region are directly opposite to empty states in the valence band of the p region. There is a finite probability that some of these electrons will tunnel directly into the empty states, producing a forward-bias tunneling current as shown. With a slightly larger forward-bias voltage, as in Figure 8.29c, the maximum number of electrons in the n region will be opposite the maximum number of empty states in the p region; this will produce a maximum tunneling current. As the forward-bias voltage continues to increase, the number of electrons on the n side directly opposite empty states on the p side decreases, as in Figure 8.29d, and the tunneling current will decrease. In Figure 8.29e, there are no electrons on the n side directly opposite to available empty states on the p side. For this forward-bias voltage, the tunneling current will be zero and the normal ideal diffusion current will exist in the device as shown in the I–V characteristics. nea29583_ch08_276-330.indd 320 12/11/10 12:37 PM 8.6 Summary 321 I e V (a) (b) Figure 8.30 | (a) Simplified energy-band diagram of a tunnel diode with a reversebiased voltage; (b) I–V characteristic of a tunnel diode with a reverse-biased voltage. The portion of the curve showing a decrease in current with an increase in voltage is the region of differential negative resistance. The range of voltage and current for this region is quite small; thus, any power generated from an oscillator using this negative resistance property would also be fairly small. A simplified energy-band diagram of the tunnel diode with an applied reversebiased voltage is shown in Figure 8.30a. Electrons in the valence band on the p side are directly opposite empty states in the conduction band on the n side, so electrons can now tunnel directly from the p region into the n region, resulting in a large reverse-biased tunneling current. This tunneling current will exist for any reversebiased voltage. The reverse-biased current will increase monotonically and rapidly with reverse-biased voltage as shown in Figure 8.30b. 8.6 | SUMMARY ■ ■ ■ ■ When a forward-bias voltage is applied across a pn junction (p region positive with respect to the n region), the potential barrier is lowered so that holes from the p region and electrons from the n region can flow across the junction. The boundary conditions relating the minority carrier hole concentration in the n region at the space charge edge and the minority carrier electron concentration in the p region at the space charge edge were derived. The holes that are injected into the n region and the electrons that are injected into the p region now become excess minority carriers. The behavior of the excess minority carrier is described by the ambipolar transport equation developed and described in Chapter 6. Solving the ambipolar transport equation and using the boundary conditions, the steady-state minority carrier hole and electron concentrations in the n region and p region, respectively, were derived. Gradients exist in the minority carrier hole and electron concentrations so that minority carrier diffusion currents exist in the pn junction. These diffusion currents yield the ideal current–voltage relationship of the pn junction diode. nea29583_ch08_276-330.indd 321 12/11/10 12:37 PM 322 CHAPTER 8 ■ ■ ■ ■ The pn Junction Diode Excess carriers are generated in the space charge region of a reverse-biased pn junction. These carriers are swept out by the electric field and create the reverse-biased generation current that is another component of the reverse-biased diode current. Excess carriers recombine in the space charge region of a forward-biased pn junction. This recombination process creates the forward-bias recombination current that is another component of the forward-bias diode current. The small-signal equivalent circuit of the pn junction diode was developed. The two parameters of interest are the diffusion resistance and the diffusion capacitance. When a pn junction is switched from forward bias to reverse bias, the stored excess minority carrier charge must be removed from the junction. The time required to remove this charge is called the storage time and is a limiting factor in the switching speed of a diode. The I–V characteristics of a tunnel diode were developed showing a region of negative differential resistance. GLOSSARY OF IMPORTANT TERMS carrier injection The flow of carriers across the space charge region of a pn junction when a voltage is applied. diffusion capacitance The capacitance of a forward-biased pn junction due to minority carrier storage effects. diffusion conductance The ratio of a low-frequency, small-signal sinusoidal current to voltage in a forward-biased pn junction. diffusion resistance The inverse of diffusion conductance. forward bias The condition in which a positive voltage is applied to the p region with respect to the n region of a pn junction so that the potential barrier between the two regions is lowered below the thermal-equilibrium value. generation current The reverse-biased pn junction current produced by the thermal generation of electron–hole pairs within the space charge region. high-level injection The condition in which the excess carrier concentration becomes comparable to or greater than the majority carrier concentration. “long” diode A pn junction diode in which both the neutral p and n regions are long compared with the respective minority carrier diffusion lengths. recombination current The forward-bias pn junction current produced as a result of the flow of electrons and holes that recombine within the space charge region. reverse saturation current The ideal reverse-biased current in a pn junction. “short” diode A pn junction diode in which at least one of the neutral p or n regions is short compared to the respective minority carrier diffusion length. storage time The time required for the excess minority carrier concentrations at the space charge edge to go from their steady-state values to zero when the diode is switched from forward to reverse bias. CHECKPOINT After studying this chapter, the reader should have the ability to: ■ nea29583_ch08_276-330.indd 322 Describe the mechanism of charge flow across the space charge region of a pn junction when a forward-bias voltage is applied. 12/11/10 12:37 PM Problems ■ ■ ■ ■ ■ ■ ■ ■ 323 State the boundary conditions for the minority carrier concentrations at the edge of the space charge region. Derive the expressions for the steady-state minority carrier concentrations in the pn junction. Derive the ideal current–voltage relationship for a pn junction diode. Describe the characteristics of a “short” diode. Describe generation and recombination currents in a pn junction. Define high-level injection and describe its effect on the diode I–V characteristics. Describe what is meant by diffusion resistance and diffusion capacitance. Describe the turn-off transient response in a pn junction. REVIEW QUESTIONS 1. Sketch the energy bands in a zero-biased, reverse-biased, and forward-biased pn junction. 2. Write the boundary conditions for the excess minority carriers in a pn junction (a) under forward bias and (b) under reverse bias. 3. Sketch the steady-state minority carrier concentrations in a forward-biased pn junction. 4. Explain the procedure that is used in deriving the ideal current–voltage relationship in a pn junction diode. 5. Sketch the electron and hole currents through a forward-biased pn junction diode. Are currents near the junction primarily due to drift or diffusion? What about currents far from the junction? 6. What is the temperature dependence of the ideal reverse-saturation current? 7. What is meant by a “short” diode? 8. Explain the physical mechanism of the (a) generation current and (b) recombination current. 9. Sketch the forward-bias I–V characteristics of a pn junction diode showing the effects of recombination and high-level injection. 10. (a) Explain the physical mechanism of diffusion capacitance. (b) What is diffusion resistance? 11. If a forward-biased pn junction is switched off, explain what happens to the stored minority carriers. In which direction is the current immediately after the diode is switched off? PROBLEMS [Note: In the following problems, assume T 300 K and the following parameters unless otherwise stated. For silicon pn junctions: Dn 25 cm2/s, Dp 10 cm2/s, n0 5 107 s, p0 107 s. For GaAs pn junctions: Dn 205 cm2/s, Dp 9.8 cm2/s, n0 5 108 s, p0 108 s.] Section 8.1 8.1 pn Junction Current (a) Consider an ideal pn junction diode at T 300 K operating in the forward-bias region. Calculate the change in diode voltage that will cause a factor of 10 increase in current. (b) Repeat part (a) for a factor of 100 increase in current. nea29583_ch08_276-330.indd 323 12/11/10 12:37 PM 324 CHAPTER 8 The pn Junction Diode A silicon pn junction has impurity doping concentrations of Nd 2 1015 cm3 and Na 8 1015 cm3. Determine the minority carrier concentrations at the edges of the space charge region for (a) Va 0.45 V, (b) Va 0.55 V, and (c) Va 0.55 V. 8.3 The doping concentrations in a GaAs pn junction are Nd 1016 cm3 and Na 4 1016 cm3. Find the minority carrier concentrations at the edges of the space charge region for (a) Va 0.90 V, (b) Va 1.10 V, and (c) Va 0.95 V. 8.4 (a) The doping concentrations in a silicon pn junction are Nd 5 1015 cm3 and Na 5 1016 cm3. The minority carrier concentration at either space charge edge is to be no larger than 10 percent of the respective majority carrier concentration. (i) Determine the maximum forward-bias voltage that can be applied to the junction and still meet the required specifications. (ii) Is the n-region or p-region concentration the factor that limits the forward-bias voltage? (b) Repeat part (a) if the doping concentrations are Nd 3 1016 cm3 and Na 7 1015 cm3. 8.5 Consider a GaAs pn junction with doping concentrations Na 5 1016 cm3 and Nd 1016 cm3. The junction cross-sectional area is A 103 cm2 and the applied forward-bias voltage is Va 1.10 V. Calculate the (a) minority electron diffusion current at the edge of the space charge region, (b) minority hole diffusion current at the edge of the space charge region, and (c) total current in the pn junction diode. 8.6 An np silicon diode at T 300 K has the following parameters: Nd 1018 cm3, Na 1016 cm3, Dn 25 cm2 /s, Dp 10 cm2 /s, n0 p0 1 s, and A 104 cm2. Determine the diode current for (a) a forward-bias voltage of 0.5 V and (b) a reversebiased voltage of 0.5 V. 8.7 An ideal germanium pn junction diode has the following parameters: Na 4 1015 cm3, Nd 2 1017 cm3, Dp 48 cm2/s, Dn 90 cm2/s, p0 n0 2 106 s, and A 104 cm2. Determine the diode current for (a) a forward-bias voltage of 0.25 V and (b) a reverse-biased voltage of 0.25 V. 8.8 A one-sided p n silicon diode has doping concentrations of Na 5 1017 cm3 and Nd 8 1015 cm3. The minority carrier lifetimes are n0 107 s and p0 8 108 s. The cross-sectional area is A 2 104 cm2. Calculate the (a) reverse-biased saturation current, and (b) the forward-bias current at (i) Va 0.45 V, (ii) Va 0.55 V, and (iii) Va 0.65 V. 8.9 Calculate the applied reverse-biased voltage at which the ideal reverse current in a pn junction diode at T 300 K reaches 90 percent of its reverse-saturation current value. 8.10 Fill in the missing data in the following table. Case Va (V) I (mA) Is (mA) Js (mA/cm2) A (cm2) 1 0.65 0.50 2 104 2 0.70 2 1012 1 103 7 3 0.80 1 10 1 104 8 4 0.72 1.20 2 10 8.11 Consider an ideal silicon pn junction diode. (a) What must be the ratio of Nd /Na so that 90 percent of the current in the depletion region is due to the flow of electrons? (b) Repeat part (a) if 80 percent of the current in the depletion region is due to the flow of holes. 8.12 A silicon pn junction diode is to be designed to operate at T 300 K such that the diode current is I 10 mA at a diode voltage of VD 0.65 V. The ratio of electron current to total current is to be 0.10 and the maximum current density is to be no more than 20 A /cm2. Use the semiconductor parameters given in Example 8.2. 8.2 nea29583_ch08_276-330.indd 324 12/11/10 12:37 PM Problems 325 An ideal silicon pn junction at T 300 K is under forward bias. The minority carrier lifetimes are n0 106 s and p0 107 s. The doping concentration in the n region is Nd 1016 cm3. Plot the ratio of hole current to the total current crossing the space charge region as the p-region doping concentration varies over the range 1015 Na 1018 cm3. (Use a log scale for the doping concentrations.) 8.14 For a silicon pn junction at T 300 K, assume p0 0.1n0 and n 2.4 p. The ratio of electron current crossing the depletion region to the total current is defined as the electron injection efficiency. Determine the expression for the electron injection efficiency as a function of (a) NdNa and (b) the ratio of n-type conductivity to p-type conductivity. 8.15 A silicon pn junction with a cross-sectional area of 104 cm2 has the following properties at T 300 K: 8.13 n region p region Nd 10 cm p0 107 s n 850 cm2 /V-s p 320 cm2 /V-s 17 3 Na 5 1015 cm3 n0 106 s n 1250 cm2 /V-s p 420 cm2 /V-s (a) Sketch the thermal equilibrium energy-band diagram of the pn junction, including the values of the Fermi level with respect to the intrinsic level on each side of the junction. (b) Calculate the reverse-saturation current Is and determine the forward-bias current I at a forward-bias voltage of 0.5 V. (c) Determine the ratio of hole current to total current at the space charge edge xn. 8.16 Consider an ideal silicon pn junction diode with the geometry shown in Figure P8.16. The doping concentrations are Na 5 1016 cm3 and Nd 1.5 1016 cm3, and the minority carrier lifetimes are n0 2 107 s and p0 8 108 s. The crosssectional area is A 5 104 cm2. Calculate (a) the ideal reverse-saturation current due to holes, (b) the ideal reverse-saturation current due to electrons, (c) the hole concentration at x xn for Va 0.8Vbi, (d) the electron current at x xn for Va 0.8 Vbi, and (e) the electron current at x xn (12) Lp for Va 0.8 Vbi. 8.17 Consider the ideal long silicon pn junction shown in Figure P8.17. T 300 K. The n region is doped with 1016 donor atoms per cm3 and the p region is doped with 5 1016 acceptor atoms per cm3. The minority carrier lifetimes are n0 0.05 s and p0 0.01 s. The minority carrier diffusion coefficients are Dn 23 cm2 /s and Dp 8 cm2 /s. The forward-bias voltage is Va 0.610 V. Calculate (a) the excess hole concentration as a function of x for x 0, (b) the hole diffusion current density at x 3 104 cm, and (c) the electron current density at x 3 104 cm. 8.18 The limit of low injection is normally defined to be when the minority carrier concentration at the edge of the space charge region in the low-doped region becomes equal W Va Va p p n n x0 x xp x 0 xn x Figure P8.16 | Figure for Problem 8.16. nea29583_ch08_276-330.indd 325 Figure P8.17 | Figure for Problem 8.17. 12/11/10 12:37 PM 326 CHAPTER 8 8.19 8.20 8.21 8.22 8.23 8.24 *8.25 The pn Junction Diode to one-tenth the majority carrier concentration in this region. Determine the value of the forward-bias voltage at which the limit of low injection is reached for the diode described in (a) Problem 8.7 and (b) Problem 8.8. The cross-sectional area of a silicon pn junction is 103 cm2. The temperature of the diode is T 300 K, and the doping concentrations are Nd 1016 cm3 and Na 8 1015 cm3. Assume minority carrier lifetimes of n0 106 s and p0 107 s. Calculate the total number of excess electrons in the p region and the total number of excess holes in the n region for (a) Va 0.3 V, (b) Va 0.4 V, and (c) Va 0.5 V. Consider two ideal pn junctions at T 300 K, having exactly the same electrical and physical parameters except for the bandgap energy of the semiconductor materials. The first pn junction has a bandgap energy of 0.525 eV and a forward-bias current of 10 mA with Va 0.255 V. For the second pn junction, “design” the bandgap energy so that a forward-bias voltage of Va 0.32 V will produce a current of 10 A. The reverse-biased saturation current is a function of temperature. (a) Assuming that Is varies with temperature only from the intrinsic carrier concentration, show that we can write Is CT 3 exp (Eg kT) where C is a constant and a function only of the diode parameters. (b) Determine the increase in Is as the temperature increases from T 300 K to T 400 K for a (i) germanium diode and (ii) silicon diode. Assume that the mobilities, diffusion coefficients, and minority carrier lifetime parameters are independent of temperature (use the T 300 K values). Assume that n0 106 s, p0 107 s, Nd 5 1015 cm3, and Na 5 1016 cm3. Plot the ideal reverse saturation current density from T 200 K to T 500 K for (a) silicon, (b) germanium, and (c) gallium arsenide ideal pn junctions. (Use a log scale for the current density.) An ideal silicon pn junction diode has a cross-sectional area of A 5 104 cm2. The doping concentrations are Na 4 1015 cm3 and Nd 2 1017 cm3. Assume that Eg 1.12 eV as well as the diffusion coefficients and lifetimes are independent of temperature. The ratio of the magnitude of forward- to reverse-biased currents is to be no less than 2 104 with forward- and reverse-biased voltages of 0.50 V, and the maximum reverse-biased current is to be limited to 1.2 A. Determine the maximum temperature at which the diode will meet these specifications and determine which specification is the limiting factor. (a) A silicon pn junction diode has the geometry shown in Figure 8.11 in which the n region is “short” with a length Wn 0.7 m. The doping concentrations are Na 2 1017 cm3 and Nd 2 1015 cm3. The cross-sectional area is A 103 cm2. Determine (i) the maximum forward-bias voltage such that low injection is still valid, and (ii) the resulting current at this forward-bias voltage. (b) Repeat part (a) if the doping concentrations are reversed such that Na 2 1015 cm3 and Nd 2 1017 cm3. A pn silicon diode is fabricated with a narrow n region as shown in Figure 8.11, in which Wn Lp. Assume the boundary condition of pn pn0 at x xn Wn. (a) Derive the expression for the excess hole concentration pn(x) as given by Equation (8.31). (b) Using the results of part (a), show that the current density in the diode is given by eDp pn0 W eV 1 J __ coth _n exp _ Lp Lp kT *Asterisks next to problems indicate problems that are more difficult. nea29583_ch08_276-330.indd 326 12/11/10 12:37 PM Problems 327 8.26 A silicon diode can be used to measure temperature by operating the diode at a fixed forward-bias current. The forward-bias voltage is then a function of temperature. At T 300 K, the diode voltage is found to be 0.60 V. Determine the diode voltage at (a) T 310 K and (b) T 320 K. 8.27 A forward-biased silicon diode is to be used as a temperature sensor. The diode is forward biased with a constant current source and Va is measured as a function of temperature. (a) Derive an expression for Va (T) assuming that D /L for electrons and holes, and Eg are independent of temperature. (b) If the diode is biased at ID 0.1 mA and if Is 1015 A at T 300 K, plot Va versus T for 20°C T 200°C. (c) Repeat part (b) if ID 1 mA. (d) Determine any changes in the results of parts (a) through (c) if the change in bandgap energy with temperature is taken into account. Section 8.2 8.28 8.29 8.30 8.31 8.32 8.33 *8.34 Generation–Recombination Currents Consider a silicon pn junction diode with an applied reverse-biased voltage of VR 5V. The doping concentrations are Na Nd 4 1016 cm3 and the cross-sectional area is A 104 cm2. Assume minority carrier lifetimes of 0 n0 p0 107 s. Calculate the (a) ideal reverse-saturation current, (b) reverse-biased generation current, and (c) the ratio of the generation current to ideal saturation current. Consider the diode described in Problem 8.28. Assume that all parameters except ni are independent of temperature. (a) Determine the temperature at which Is and Igen will be equal. What are the values of Is and Igen at this temperature? (b) Calculate the forward-bias voltage at which the ideal diffusion current is equal to the recombination current at T 300 K. Consider a GaAs pn junction diode with a cross-sectional area of A 2 104 cm2 and doping concentrations of Na Nd 7 1016 cm3. The electron and hole mobility values are n 5500 cm2/V-s and p 220 cm2/V-s, respectively, and the lifetime values are 0 n0 p0 2 108 s. (a) Calculate the ideal diode current at a (i) reverse-biased voltage of VR 3 V, (ii) forward-bias voltage of Va 0.6 V, (iii) forward-bias voltage of Va 0.8 V, and (iv) forward-bias voltage of Va 1.0 V. (b) (i) Calculate the generation current at VR 3 V. Assuming the recombination current extrapolated to Va 0 is Iro 6 1014 A, determine the generation current at (ii) Va 0.6 V, (iii) Va 0.8 V, and (iv) Va 1.0 V. Consider the pn junction diode described in Problem 8.30. Plot the diode recombination current and the ideal diode current (on a log scale) versus forward-bias voltage over the range 0.1 Va 1.0 V. A silicon pn junction diode at T 300 K has the following parameters: Na Nd 1016 cm3, p0 n0 0 5 107 s, Dp 10 cm2 /s, Dn 25 cm2 /s, and a crosssectional area of 104 cm2. Plot the diode recombination current and the ideal diode current (on a log scale) versus forward-bias voltage over the range 0.1 Va 0.6 V. Consider a GaAs pn diode at T 300 K with Na Nd 1017 cm3 and with a crosssectional area of 5 103 cm2. The minority carrier mobilities are n 3500 cm2 /V-s and p 220 cm2 /V-s. The electron–hole lifetimes are n0 p0 0 108 s. Plot the diode forward-bias current including recombination current between diode voltages of 0.1 VD 1.0 V. Compare this plot to that for an ideal diode. Starting with Equation (8.44) and using the suitable approximations, show that the maximum recombination rate in a forward-biased pn junction is given by Equation (8.52). nea29583_ch08_276-330.indd 327 12/11/10 12:37 PM 328 CHAPTER 8 The pn Junction Diode Illumination p n W VR Figure P8.35 | Figure for Problem 8.35 and 8.36. 8.35 Consider, as shown in Figure P8.35, a uniformly doped silicon pn junction at T 300 K with impurity doping concentrations of Na Nd 5 1015 cm3 and minority carrier lifetimes of n0 p0 0 107 s. A reverse-biased voltage of VR 10 V is applied. A light source is incident only on the space charge region, producing an excess carrier generation rate of g 4 1019 cm3 s1. Calculate the generation current density. 8.36 A long silicon pn junction diode has the following parameters: Nd 1018 cm3, Na 3 1016 cm3, n0 p0 0 107 s, Dn 18 cm2 /s, and Dp 6 cm2 /s. A light source is incident on the space charge region such as shown in Figure P8.35, producing a generation current density of JG 25 mA /cm2. The diode is open circuited. The generation current density forward biases the junction, inducing a forward-bias current in the opposite direction to the generation current. A steady-state condition is reached when the generation current density and forward-bias current density are equal in magnitude. What is the induced forward-bias voltage at this steady-state condition? Section 8.3 Small-Signal Model of the pn Junction 8.37 8.38 8.39 8.40 8.41 nea29583_ch08_276-330.indd 328 (a) Calculate the small-signal diffusion capacitance and diffusion resistance of a silicon pn junction diode biased at IDQ 1.2 mA. Assume the minority carrier lifetimes are 0.5 s in both the n and p regions. (b) Repeat part (a) for the case when the diode is biased at IDQ 0.12 mA. Consider the diode described in Problem 8.37. A sinusoidal signal voltage with a peak value of 50 mV is superimposed on the dc forward-bias voltage. Determine the magnitude of charge that is being alternately charged and discharged in the n region. Consider a pn silicon diode at T 300 K. The diode is forward biased at a current of 1 mA. The hole lifetime in the n region is 107 s. Neglecting the depletion capacitance, calculate the diode impedance at frequencies of 10 kHz, 100 kHz, 1 MHz, and 10 MHz. Consider a silicon pn junction with parameters as described in Problem 8.8. (a) Calculate and plot the depletion capacitance and diffusion capacitance over the voltage range 10 Va 0.75 V. (b) Determine the voltage at which the two capacitances are equal. Consider a p n silicon diode at T 300 K. The slope of the diffusion capacitance versus forward-bias current is 2.5 106 F /A. Determine the hole lifetime and the diffusion capacitance at a forward-bias current of 1 mA. 12/11/10 12:37 PM Problems 8.42 8.43 8.44 8.45 8.46 329 A one-sided p n silicon diode has doping concentrations of Na 4 1017 cm3 and Nd 8 1015 cm3. The diode cross-sectional area is A 5 104 cm2. (a) The maximum diffusion capacitance is to be limited to 1 nF. Determine (i) the maximum current through the diode, (ii) the maximum forward-bias voltage, and (iii) the diffusion resistance. (b) Repeat part (a) if the maximum diffusion capacitance is limited to 0.25 nF. A silicon pn junction diode at T 300 K has a cross-sectional area of 102 cm2. The length of the p region is 0.2 cm and the length of the n region is 0.1 cm. The doping concentrations are Nd 1015 cm3 and Na 1016 cm3. Determine (a) approximately the series resistance of the diode and (b) the current through the diode that will produce a 0.1 V drop across this series resistance. We want to consider the effect of a series resistance on the forward-bias voltage required to achieve a particular diode current. (a) Assume the reverse-saturation current in a diode is Is 1010 A at T 300 K. The resistivity of the n region is 0.2 -cm and the resistivity of the p region is 0.1 -cm. Assume the length of each neutral region is 102 cm and the cross-sectional area is 2 105 cm2. Determine the required applied voltage to achieve a current of (i) 1 mA and (ii) 10 mA. (b) Repeat part (a) neglecting the series resistance. (a) The reverse-saturation current in a diode is Is 5 1012 A. The maximum small-signal diffusion resistance is to be rd 32 . Determine the minimum forwardbias voltage that can be applied to meet this specification. (b) Repeat part (a) if the maximum small-signal diffusion resistance is to be rd 60 . (a) An ideal silicon pn junction diode at T 300 K is forward biased at Va 20 mV. The reverse-saturation current is Is 1013 A. Calculate the smallsignal diffusion resistance. (b) Repeat part (a) for an applied reverse-biased voltage of Va 20 mV. Section 8.4 Charge Storage and Diode Transients 8.47 (a) In switching a pn junction from forward to reverse bias, assume that the ratio of reverse current, IR, to forward current, IF, is 0.2. Determine the ratio of storage time to minority carrier lifetime, ts /p0. (b) Repeat part (a) if the ratio of IR to IF is 1.0. 8.48 A pn junction is switched from forward to reverse bias. The storage time is specified to be s 0.3 p0. (a) Determine the required ratio of IR to IF to meet this specification. (b) Determine t2p0. 8.49 Consider a diode with a junction capacitance of 18 pF at zero bias and 4.2 pF at a reverse-biased voltage of VR 10 V. The minority carrier lifetimes are 107 s. The diode is switched from a forward bias with a current of 2 mA to a reverse-biased voltage of 10 V applied through a 10 k resistor. Estimate the turn-off time. Section 8.5 The Tunnel Diode Consider a silicon pn junction at T 300 K with doping concentration of Nd Na 5 1019 cm3. Assuming the abrupt junction approximation is valid, determine the space charge width at a forward-bias voltage of Va 0.40 V. 8.51 Sketch the energy-band diagram of an abrupt pn junction under zero bias in which the p region is degenerately doped and EC EF in the n region. Sketch the forward- and reverse-biased current–voltage characteristics. This diode is sometimes called a backward diode. Why? 8.50 nea29583_ch08_276-330.indd 329 12/11/10 12:37 PM 330 CHAPTER 8 The pn Junction Diode Summary and Review 8.52 (a) Explain physically why the diffusion capacitance is not important in a reversebiased pn junction. (b) Consider a silicon, a germanium, and gallium arsenide pn junction. If the total current density is the same in each diode under forward bias, discuss the expected relative values of electron and hole current densities. *8.53 A silicon p n junction diode is to be designed to have a breakdown voltage of at least 60 V and to have a forward-bias current of ID 50 mA while still operating under low injection. The minority carrier lifetimes are 0 n0 p0 2 107 s. Determine the doping concentrations and the minimum cross-sectional area. *8.54 The donor and acceptor concentrations on either side of a silicon step junction are equal. (a) Derive an expression for the breakdown voltage in terms of the critical electric field and doping concentration. (b) If the breakdown voltage is to be VB 50 V, specify the range of allowed doping concentrations. READING LIST 1. 2. 3. 4. *5. 6. 7. 8. *9. 10. 11. 12. *13. 14. Dimitrijev, S. Principles of Semiconductor Devices. New York: Oxford University Press, 2006. Kano, K. Semiconductor Devices. Upper Saddle River, NJ: Prentice Hall, 1998. Muller, R. S., and T. I. Kamins. Device Electronics for Integrated Circuits, 2nd ed. New York: John Wiley and Sons, 1986. Neudeck, G. W. The PN Junction Diode. Vol. 2 of the Modular Series on Solid State Devices. 2nd ed. Reading, MA: Addison-Wesley, 1989. Ng, K. K. Complete Guide to Semiconductor Devices. New York: McGraw-Hill, 1995. Pierret, R. F. Semiconductor Device Fundamentals. Reading, MA: Addison-Wesley Publishing Co., 1996. Roulston, D. J. An Introduction to the Physics of Semiconductor Devices. New York: Oxford University Press, 1999. Shur, M. Introduction to Electronic Devices. New York: John Wiley and Sons, 1996. Shur, M. Physics of Semiconductor Devices. Englewood Cliffs, NJ: Prentice Hall, 1990. Streetman, B. G., and S. K. Banerjee. Solid State Electronic Devices, 6th ed. Upper Saddle River, NJ: Pearson Prentice Hall, 2006. Sze, S. M. and K. K. Ng. Physics of Semiconductor Devices, 3rd ed. Hoboken, NJ: John Wiley and Sons, 2007. Sze, S. M. Semiconductor Devices: Physics and Technology, 2nd ed. New York: John Wiley and Sons, 2001. Wang, S. Fundamentals of Semiconductor Theory and Device Physics. Englewood Cliffs, NJ: Prentice Hall, 1989. Yang, E. S. Microelectronic Devices. New York: McGraw-Hill, 1988. *Indicates references that are at an advanced level compared to this text. nea29583_ch08_276-330.indd 330 12/11/10 12:37 PM C 9 H A P T E R Metal–Semiconductor and Semiconductor Heterojunctions I n the preceding two chapters, we have considered the pn junction and assumed that the semiconductor material was the same throughout the structure. This type of junction is referred to as a homojunction. We developed the electrostatics of the junction and derived the current–voltage relationship. In this chapter, we consider the metal–semiconductor junction and the semiconductor heterojunction, in which the material on each side of the junction is not the same. These junctions can also produce diodes. Semiconductor devices, or integrated circuits, must make contact with the outside world. This contact is made through nonrectifying metal–semiconductor junctions, or ohmic contacts. An ohmic contact is a low-resistance junction providing current conduction in both directions. We examine in this chapter the conditions that yield metal–semiconductor ohmic contacts. ■ 9.0 | PREVIEW In this chapter, we will: ■ Determine the energy-band diagram of a metal–semiconductor junction. ■ Investigate the electrostatics of the rectifying metal–semiconductor junction, which is known as the Schottky barrier diode. ■ Derive the ideal current–voltage relation of the Schottky barrier diode. ■ Discuss differences in the current transport mechanism between the Schottky barrier diode and pn junction diode, and discuss differences in turn-on voltage and switching times. ■ Discuss ohmic contacts, which are low-resistance, nonrectifying metal– semiconductor junctions. ■ Investigate the characteristics of a semiconductor heterojunction. 331 nea29583_ch09_331-370.indd 331 12/11/10 12:39 PM 332 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions 9.1 | THE SCHOTTKY BARRIER DIODE One of the first practical semiconductor devices used in the early 1900s was the metal–semiconductor diode. This diode, also called a point contact diode, was made by touching a metallic whisker to an exposed semiconductor surface. These metal– semiconductor diodes were not easily reproduced or mechanically reliable and were replaced by the pn junction in the 1950s. However, semiconductor and vacuum technology is now used to fabricate reproducible and reliable metal–semiconductor contacts. In this section, we consider the metal–semiconductor rectifying contact, or Schottky barrier diode. In most cases, the rectifying contacts are made on n-type semiconductors; for this reason, we concentrate on this type of diode. 9.1.1 Qualitative Characteristics The ideal energy-band diagram for a particular metal and n-type semiconductor before making contact is shown in Figure 9.1a. The vacuum level is used as a reference level. The parameter m is the metal work function (measured in volts), s is Vacuum level e em es Ec EF EFi EF Ev (a) eVbi eB0 Ec EF EF en Ev Depletion region xn W (b) Figure 9.1 | (a) Energy-band diagram of a metal and semiconductor before contact; (b) ideal energy-band diagram of a metal–n-semiconductor junction for m s. nea29583_ch09_331-370.indd 332 12/11/10 12:39 PM 9.1 The Schottky Barrier Diode 333 Table 9.1 | Work functions of some elements Element Ag, silver Al, aluminum Au, gold Cr, chromium Mo, molybdenum Ni, nickel Pd, palladium Pt, platinum Ti, titanium W, tungsten Work function, m 4.26 4.28 5.1 4.5 4.6 5.15 5.12 5.65 4.33 4.55 Table 9.2 | Electron affinity of some semiconductors Element Electron affinity, Ge, germanium Si, silicon GaAs, gallium arsenide AlAs, aluminum arsenide 4.13 4.01 4.07 3.5 the semiconductor work function, and is known as the electron affinity. The work functions of various metals are given in Table 9.1 and the electron affinities of several semiconductors are given in Table 9.2. In Figure 9.1a, we have assumed that m > s . The ideal thermal-equilibrium metal–semiconductor energy-band diagram, for this situation, is shown in Figure 9.1b. Before contact, the Fermi level in the semiconductor was above that in the metal. In order for the Fermi level to become a constant through the system in thermal equilibrium, electrons from the semiconductor flow into the lower energy states in the metal. Positively charged donor atoms remain in the semiconductor, creating a space charge region. The parameter B0 is the ideal barrier height of the semiconductor contact, the potential barrier seen by electrons in the metal trying to move into the semiconductor. This barrier is known as the Schottky barrier and is given, ideally, by B0 (m ) (9.1) On the semiconductor side, Vbi is the built-in potential barrier. This barrier, similar to the case of the pn junction, is the barrier seen by electrons in the conduction band trying to move into the metal. The built-in potential barrier is given by Vbi B0 n (9.2) which makes Vbi a slight function of the semiconductor doping, as is the case in a pn junction. If we apply a positive voltage to the semiconductor with respect to the metal, the semiconductor-to-metal barrier height increases, while B0 remains constant in this idealized case. This bias condition is the reverse bias. If a positive voltage is applied to the metal with respect to the semiconductor, the semiconductor-to-metal barrier Vbi is reduced while B0 again remains essentially constant. In this situation, electrons can more easily flow from the semiconductor into the metal since the barrier has been reduced. This bias condition is the forward bias. The energy-band diagrams for the reverse and forward bias are shown in Figures 9.2a,b where VR is the magnitude of the reverse-biased voltage and Va is the magnitude of the forward-bias voltage. nea29583_ch09_331-370.indd 333 12/11/10 12:39 PM 334 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions eB0 e(Vbi VR) e(Vbi Va) Ec x0 Ec EF eB0 EF Ev Ev x0 x xn (a) x xn (b) Figure 9.2 | Ideal energy-band diagram of a metal–semiconductor junction (a) under reverse bias and (b) under forward bias. The energy-band diagrams versus voltage for the metal–semiconductor junction shown in Figure 9.2 are very similar to those of the pn junction given in the previous chapter. Because of this similarity, we expect the current–voltage characteristics of the Schottky barrier junction to be similar to the exponential behavior of the pn junction diode. The current mechanism here, however, is due to the flow of majority carrier electrons. In forward bias, the barrier seen by the electrons in the semiconductor is reduced, so majority carrier electrons flow more easily from the semiconductor into the metal. The forward-bias current is in the direction from metal to semiconductor: It is an exponential function of the forward-bias voltage Va . 9.1.2 Ideal Junction Properties We can determine the electrostatic properties of the junction in the same way as we do for the pn junction. The electric field in the space charge region is determined from Poisson’s equation. We have that (x) dE _ _ (9.3) s dx where (x) is the space charge volume density and s is the permittivity of the semiconductor. If we assume that the semiconductor doping is uniform, then by integrating Equation (9.3), we obtain eNd eNdx _ E _ (9.4) s dx s C1 where C1 is a constant of integration. The electric field is zero at the space charge edge in the semiconductor, so the constant of integration can be found as eNd xn C1 _ s nea29583_ch09_331-370.indd 334 (9.5) 12/11/10 12:39 PM 9.1 The Schottky Barrier Diode 335 The electric field can then be written as eNd E _ s (xn x) (9.6) which is a linear function of distance, for the uniformly doped semiconductor, and reaches a peak value at the metal–semiconductor interface. Since the E-field is zero inside the metal, a negative surface charge must exist in the metal at the metal– semiconductor junction. The space charge region width, W, may be calculated as we do for the pn junction. The result is identical to that of a one-sided pn junction. For the uniformly doped semiconductor, we have 2s(Vbi VR) W xn ___ eNd 12 (9.7) where VR is the magnitude of the applied reverse-biased voltage. We are again assuming an abrupt junction approximation. Objective: Determine the theoretical barrier height, built-in potential barrier, and maximum electric field in a metal–semiconductor diode for zero applied bias. Consider a contact between tungsten and n-type silicon doped to Nd 1016 cm3 at T 300 K. EXAMPLE 9.1 ■ Solution The metal work function for tungsten (W) from Table 9.1 is m 4.55 V and the electron affinity for silicon from Table 9.2 is 4.01 V. The barrier height is then B0 m 4.55 4.01 0.54 V where B0 is the ideal Schottky barrier height. We can calculate n as Nc 2.8 1019 0.206 V kT ln _ n _ 0.0259 ln __ e Nd 1016 Then Vbi B0 n 0.54 0.206 0.334 V The space charge width at zero bias is 2s Vbi xn _ eNd 12 or 2(11.7)(8.85 1014)(0.334) _____ (1.6 1019)(1016) 12 xn 0.208 104 cm Then the maximum electric field is (1.6 1019)(1016)(0.208 104) eNd xn ______ Emax _ s (11.7)(8.85 1014) or finally Emax 3.21 104 V/cm nea29583_ch09_331-370.indd 335 12/11/10 12:39 PM 336 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions ■ Comment The values of space charge width and electric field are very similar to those obtained for a pn junction. ■ EXERCISE PROBLEM Ex 9.1 Consider an ideal tungsten-to-n-type GaAs junction. Assume the GaAs is doped to a concentration of Nd = 5 1015 cm3 . Determine the theoretical barrier height, the built-in potential barrier, and maximum electric field for the case of zero applied bias. (Ans. B0 0.48 V, Vbi 0.3623 V, Emax 2.24 104 V/cm) A junction capacitance can also be determined in the same way as we do for the pn junction. We have that es Nd dx C eNd _n __ 2 (Vbi VR) dVR 12 (9.8) where C is the capacitance per unit area. If we square the reciprocal of Equation (9.8), we obtain 2(Vbi VR) 1 2 __ _ (9.9) esNd C We can use Equation (9.9) to obtain, to a first approximation, the built-in potential barrier Vbi , and the slope of the curve from Equation (9.9) to yield the semiconductor doping Nd . We can calculate the potential n and then determine the Schottky barrier B0 from Equation (9.2). EXAMPLE 9.2 Objective: To calculate the semiconductor doping concentration and Schottky barrier height from the silicon diode experimental capacitance data shown in Figure 9.3. Assume T 300 K. ■ Solution The intercept of the tungsten–silicon curve is approximately at Vbi 0.40 V. From Equation (9.9), we can write d(1C) (1C) 2 __ __ _ 2 2 VR dVR es Nd Then, from the figure, we have (1C) __ 4.4 1013 2 VR so that 2 Nd ________ 2.7 1017 cm3 (1.6 1019)(11.7)(8.85 1014)(4.4 1013) We can calculate Nc 2.8 1019 0.12 V kT ln _ n _ (0.0259) ln __ e Nd 2.7 1017 so that Bn Vbi n 0.40 0.12 0.52 V where Bn is the actual Schottky barrier height. nea29583_ch09_331-370.indd 336 12/11/10 12:39 PM 9.1 The Schottky Barrier Diode 337 14 W–Si 10 8 (cm2/pF)2 1012 (W–GaAs) 1/C 2 (cm2/pF)2 1013 (W–Si) 12 W– GaAs 6 4 Intercept 2 0 1 0 1 2 3 4 VR (V) Figure 9.3 | 1C 2 versus VR for W–Si and W–GaAs Schottky barrier diodes. (From Sze and Ng [15].) ■ Comment The experimental value of 0.52 V can be compared with the ideal barrier height of B0 0.54 V found in Example 9.1. These results agree fairly well. For other metals, the discrepancy between experiment and theory is larger. ■ EXERCISE PROBLEM Repeat Example 9.2 for the GaAs diode capacitance data shown in Figure 9.3. (Ans. Vbi Ex 9.2 0.64 V, Nd 4.62 1018 cm3) We can see that the built-in potential barrier of the gallium arsenide Schottky diode is larger than that of the silicon diode. This experimental result is normally observed for all types of metal contacts. TEST YOUR UNDERSTANDING TYU 9.1 Consider an ideal chromium-to-n-type silicon Schottky diode at T 300 K. Assume the semiconductor is doped at a concentration of Nd 3 1015 cm3. Determine the (a) ideal Schottky barrier height, (b) built-in potential barrier, (c) peak electric field with an applied reverse-biased voltage of VR 5 V, and (d) junction capacitance per unit area for VR 5 V. [Ans. (a) B0 0.49 V; (b) Vbi 0.253 V; (c) Emax 6.98 104 V/cm; (d) C 6.88 109 F/cm2] nea29583_ch09_331-370.indd 337 12/11/10 12:39 PM CHAPTER 9 TYU 9.2 9.1.3 Metal–Semiconductor and Semiconductor Heterojunctions Repeat TYU 9.1 for an ideal palladium-to-n-type GaAs Schottky diode with the same impurity concentration. [Ans. (a) B0 1.05 V; (b) Vbi 0.919 V; (c) Emax 7 104 V/cm; (d) C 6.86 109 F/cm2] 338 Nonideal Effects on the Barrier Height Schottky Barrier Lowering Several effects alter the actual Schottky barrier height from the theoretical value given by Equation (9.1). The first such effect that we consider is the Schottky effect, or image-force-induced lowering of the potential barrier. An electron in a dielectric material at a distance x from the metal will create an electric field. The electric field can be determined by adding an image charge, e, inside the metal located at the same distance, x, from the interface. This image effect is shown in Figure 9.4a. Note that the E–field lines are perpendicular to the metal surface as we expect. The force on the electron, due to the coulomb attraction with the image force, is e2 eE F __ (9.10) 4s(2x)2 Metal Dielectric E(x) x EF x x0 (b) (a) E(x) xm x eE eB0 eBn EF x0 (c) Figure 9.4 | (a) Image charge and electric field lines at a metal–dielectric interface. (b) Distortion of the potential barrier due to image forces with zero electric field and (c) with a constant electric field. nea29583_ch09_331-370.indd 338 12/11/10 12:39 PM 9.1 The Schottky Barrier Diode The potential can then be found as e e (x) E dx __ dx __ 2 16s x 4 s ⴢ 4(x) x x 339 (9.11) where x is the integration variable and where we have assumed that the potential is zero at x . The potential energy of the electron is e(x): Figure 9.4b is a plot of the potential energy assuming that no other electric fields exist. With an electric field present in the dielectric, the potential is modified and can be written as e Ex (x) __ 16s x (9.12) The potential energy of the electron, including the effect of a constant electric field, is plotted in Figure 9.4c. The peak potential barrier is now lowered. This lowering of the potential barrier is the Schottky effect, or image force–induced lowering. We can find the Schottky barrier lowering, , and the position of the maximum barrier, xm , from the condition that d[e(x)] __ 0 (9.13) dx We find that xm and _______ e __ (9.14) 16s E _____ eE _ (9.15) 4 s Objective: Calculate the Schottky barrier lowering and the position of the maximum barrier EXAMPLE 9.3 height. Consider a gallium arsenide metal–semiconductor contact in which the electric field in the semiconductor is assumed to be E 6.8 104 V/cm. ■ Solution The Schottky barrier lowering is given by Equation (9.15), which in this case yields _____________________ _____ eE _ 4s (1.6 10 )(6.8 10 ) ____ 0.0273 V 14 19 4 4 (13. 1)(8.85 10 ) The position of the maximum barrier height is xm _______ ______________________________ e __ 16sE (1.6 10 ) ______ 19 16(13.1)(8.85 1014)(6.8 104) or xm 2 107 cm 20 Å nea29583_ch09_331-370.indd 339 12/11/10 12:39 PM 340 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions ■ Comment Although the Schottky barrier lowering may seem like a small value, the barrier height and the barrier lowering will appear in exponential terms in the current–voltage relationship. A small change in the barrier height can thus have a significant effect on the current in a Schottky barrier diode. ■ EXERCISE PROBLEM Ex 9.3 Consider the Schottky diode described in Example 9.1. Calculate the Schottky barrier lowering for a reverse-biased voltage of (a) VR 1 V and (b) VR 5 V. [Ans. (a) 0.0281 V; (b) 0.0397 V] Interface States Figure 9.5 shows the measured barrier heights in gallium arsenide and silicon Schottky diodes as a function of metal work functions. There is a monotonic relation between the measured barrier height and the metal work function, but the curves do not fit the simple relation given in Equation (9.1). The barrier height of the metal–semiconductor junction is determined by both the metal work function and the semiconductor surface or interface states. A more detailed energy-band diagram of a metal to n-type semiconductor contact in thermal equilibrium is shown in Figure 9.6. We assume that a narrow interfacial layer of insulator exists between the metal and semiconductor. The interfacial layer can support a potential difference, but will be transparent to the flow of electrons between the metal and semiconductor. The semiconductor also shows a distribution of surface states at the metal–semiconductor interface. We assume that all states below Barrier height, eBn (eV) 1.0 0.8 GaAs 0.6 0.4 Si 0.2 Mg 3.0 Al Ag W Au Pd Pt 5.0 4.0 Metal work function, em (eV) 6.0 Figure 9.5 | Experimental barrier heights as a function of metal work functions for GaAs and Si. (From Crowley and Sze [2].) nea29583_ch09_331-370.indd 340 12/11/10 12:39 PM 9.1 The Schottky Barrier Diode 341 eVox e em eVbi eBn EF en Qss e0 Eg ␦ Figure 9.6 | Energy-band diagram of a metal–semiconductor junction with an interfacial layer and interface states. the surface potential 0 are donor states, which will be neutral if the state contains an electron and positively charged if the state does not contain an electron. We also assume that all states above 0 are acceptor states, which will be neutral if the state does not contain an electron and negatively charged if the state contains an electron. The diagram in Figure 9.6 shows some acceptor states above 0 and below EF. These states tend to contain electrons and are negatively charged. We may assume that the surface state density is constant and equal to Dit states/cm2-eV. The relation between the surface potential, surface state density, and other semiconductor parameters is found to be ______________ i 1 (Eg e0 eBn) _ 2esNd(Bn n) _ [ ( Bn)] eDit eDit m (9.16) We consider two limiting cases. Case 1 Let Dit → . In this case, the right side of Equation (9.16) goes to zero. We then have 1 (E e ) Bn _ (9.17) 0 e g The barrier height is now fixed by the bandgap energy and the potential 0. The barrier height is totally independent of the metal work function and the semiconductor electron affinity. The Fermi level becomes “pinned” at the surface, at the surface potential 0. Case 2 Let Dit → 0. Equation (9.16) reduces to Bn (m ) which is the original ideal expression. The Schottky barrier height is a function of the electric field in the semiconductor through the barrier lowering effect. The barrier height is also a function of the surface states in the semiconductor. The barrier height, then, is modified from the ideal theoretical value. Since the surface state density is not predictable with any degree of certainty, the barrier height must be an experimentally determined parameter. nea29583_ch09_331-370.indd 341 12/11/10 12:39 PM 342 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions TEST YOUR UNDERSTANDING TYU 9.3 Determine the Schottky barrier lowering and the position of the maximum barrier height for the junction described in TYU 9.1. Use the value of the electric field found in TYU 9.1. (Ans. 0.0293 eV, xm 21 Å) 9.1.4 Current–Voltage Relationship The current transport in a metal–semiconductor junction is due mainly to majority carriers as opposed to minority carriers in a pn junction. The basic process in the rectifying contact with an n-type semiconductor is by transport of electrons over the potential barrier, which can be described by the thermionic emission theory. The thermionic emission characteristics are derived by assuming that the barrier height is much larger than kT, so that the Maxwell–Boltzmann approximation applies and that thermal equilibrium is not affected by this process. Figure 9.7 shows the one-dimensional barrier with an applied forward-bias voltage Va and two electron current density components. The current Js → m is the electron current density due to the flow of electrons from the semiconductor into the metal, and the current Jm → s is the electron current density due to the flow of electrons from the metal into the semiconductor. The subscripts of the currents indicate the direction of electron flow. The conventional current direction is opposite to electron flow. Jm Js s m ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ e e(Vbi Va) en eBn eVa Ec Ec EF EF Ev x I Va n I Va Figure 9.7 | Energy-band diagram of a forward-biased metal– semiconductor junction including the image lowering effect. nea29583_ch09_331-370.indd 342 12/11/10 12:39 PM 9.1 The Schottky Barrier Diode 343 The current density Js → m is a function of the concentration of electrons which have x-directed velocities sufficient to overcome the barrier. We may write Js → m e (9.18) vx dn E c where Ec is the minimum energy required for thermionic emission into the metal, vx is the carrier velocity in the direction of transport, and e is the magnitude of the electronic charge. The incremental electron concentration is given by dn gc (E ) fF (E ) dE (9.19) where gc (E) is the density of states in the conduction band and fF (E) is the Fermi– Dirac probability function. Assuming that the Maxwell–Boltzmann approximation applies, we may write (E EF) E Ec exp __ dE kT ______ 4 (2m*n )32 dn __ h3 (9.20) If all of the electron energy above Ec is assumed to be kinetic energy, then we have 1 m* v2 E E _ 2 (9.21) c n The net current density in the metal-to-semiconductor junction can be written as J Js → m J m → s (9.22) which is defined to be positive in the direction from the metal to the semiconductor. We find that eBn J A* T 2 exp __ kT eV 1 exp _ kT a (9.23) where 2 A* 4em*n k __ (9.24) 3 h The parameter A* is called the effective Richardson constant for thermionic emission. Equation (9.23) can be written in the usual diode form as eV J JsT exp _a 1 kT (9.25) where JsT is the reverse-saturation current density and is given by eBn JsT A*T 2 exp __ kT (9.26) We may recall that the Schottky barrier height Bn changes because of the image-force lowering. We have that Bn B0 . Then we can write Equation (9.26) as nea29583_ch09_331-370.indd 343 12/11/10 12:39 PM 344 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions 105 106 Experimental result IR (A) 107 108 109 Theoretical result 1010 1011 103 102 101 100 VR (V) 101 102 Figure 9.8 | Experimental and theoretical reverse-biased currents in a PtSi–Si diode. (From Sze and Ng [15].) eB0 e JsT A*T 2 exp __ exp _ kT kT (9.27) The change in barrier height, , will increase with an increase in the electric field, or with an increase in the applied reverse-biased voltage. Figure 9.8 shows a typical reverse-biased current–voltage characteristic of a Schottky barrier diode. The reversebiased current increases with reverse-biased voltage because of the barrier lowering effect. This figure also shows the Schottky barrier diode going into breakdown. EXAMPLE 9.4 Objective: Determine the effective Richardson constant from the current–voltage characteristics. Consider the tungsten–silicon diode curve in Figure 9.9 and assume a barrier height of Bn 0.67 V. From the figure, JsT 6 105 A/cm2. ■ Solution We have that eBn JsT A* T 2 exp __ kT so that eBn JsT A* _ exp __ kT T2 Then 6 105 exp __ 0.67 114 A/K2-cm2 A* __ 0.0259 (300)2 ■ Comment The experimentally determined value of A* is a very strong function of Bn , since Bn is in the exponential term. A small change in Bn will change the value of the Richardson constant substantially. nea29583_ch09_331-370.indd 344 12/11/10 12:39 PM 9.1 The Schottky Barrier Diode 345 10 0 101 W–Si JF (A/cm2) 102 103 W–GaAs 104 Js 105 106 Js 107 0 0.1 0.2 0.3 Va (V) Figure 9.9 | Forward-bias current density JF versus Va for Wi–Si and W–GaAs diodes. (From Sze and Ng [15].) ■ EXERCISE PROBLEM Ex 9.4 Calculate the ideal Richardson constant for a free electron. (Ans. A* 120 AK2-cm2) We may note that the reverse-saturation current densities of the tungsten–silicon and tungsten–gallium arsenide diodes in Figure 9.9 differ by approximately two orders of magnitude. This two order of magnitude difference will be reflected in the effective Richardson constant, assuming the barrier heights in the two diodes are essentially the same. The definition of the effective Richardson constant, given by Equation (9.24), contains the electron effective mass, which differs substantially between silicon and gallium arsenide. The fact that the effective mass is in the expression for the Richardson constant is a direct result of using the effective density of states function in the thermionic emission theory. The net result is that A* and JsT will vary widely between silicon and gallium arsenide. 9.1.5 Comparison of the Schottky Barrier Diode and the pn Junction Diode Although the ideal current–voltage relationship of the Schottky barrier diode given by Equation (9.25) is of the same form as that of the pn junction diode, there are two important differences between a Schottky diode and a pn junction diode: The first is in the magnitudes of the reverse-saturation current densities and the second is in the switching characteristics. nea29583_ch09_331-370.indd 345 12/11/10 12:39 PM 346 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions The reverse-saturation current density of the Schottky barrier diode was given by Equation (9.26) and is eBn JsT A* T 2 exp __ kT The ideal reverse-saturation current density of the pn junction diode can be written as eDn npo eDp pno Js __ __ (9.28) Ln Lp The form of the two equations is vastly different, and the current mechanism in the two devices is different. The current in a pn junction is determined by the diffusion of minority carriers while the current in a Schottky barrier diode is determined by thermionic emission of majority carriers over a potential barrier. EXAMPLE 9.5 Objective: Calculate the ideal reverse-saturation current densities of a Schottky barrier diode and a pn junction diode. Consider a tungsten barrier on silicon with a measured barrier height of eBn 0.67 eV. The effective Richardson constant is A* 114 A /K 2-cm2. Let T 300 K. ■ Solution If we neglect the barrier lowering effect, we have for the Schottky barrier diode eBn 0.67 5.98 105 A/cm2 JsT A* T 2 exp __ (114)(300)2 exp __ kT 0.0259 Consider a silicon pn junction with the following parameters at T 300 K. Na 1018 cm3 Dp 10 cm2/s 7 s po 10 Nd 1016 cm3 Dn 25 cm2/s 7 s no 10 We can then calculate the following parameters: Lp 1.0 103 cm pno 2.25 104 cm3 Ln 1.58 103 cm npo 2.25 102 cm3 The ideal reverse-saturation current density of the pn junction diode can be determined from Equation (9.28) as (1.6 1019)(25)(2.25 102) _____ (1.6 1019)(10)(2.25 104) Js _____ (1.58 103) (1.0 103) 5.7 1013 3.6 1011 3.66 1011 A/cm2 ■ Comment The ideal reverse-saturation current density of the Schottky barrier junction is orders of magnitude larger than that of the ideal pn junction diode. ■ EXERCISE PROBLEM Ex 9.5 Using the results of Example 9.5, determine the forward-bias voltages required to produce a current of 10 A in each diode. Assume each cross-sectional area is 104 cm2. (Ans. pn junction, Va 0.5628 V; Schottky junction, Va 0.1922 V) nea29583_ch09_331-370.indd 346 12/11/10 12:39 PM 9.1 The Schottky Barrier Diode 347 8 ID (mA) pn junction diode Schottky diode 6 4 2 0 0.2 0.4 VD (V) 0.6 Figure 9.10 | Comparison of forwardbias I–V characteristics between a Schottky diode and a pn junction diode. Recall that the reverse-biased current in a silicon pn junction diode is dominated by the generation current. A typical generation current density is approximately 107 A/cm2, which is still two to three orders of magnitude less than the reversesaturation current density of the Schottky barrier diode. A generation current also exists in the reverse-biased Schottky barrier diode; however, the generation current is negligible compared with the JsT value. Since JsT Js , the forward-bias characteristics of the two types of diodes will also be different. Figure 9.10 shows typical I–V characteristics of a Schottky barrier diode and a pn junction diode. The effective turn-on voltage of the Schottky diode is less than that of the pn junction diode. Objective: Calculate the forward-bias voltage required to induce a forward-bias current EXAMPLE 9.6 density of 10 A/cm2 in a Schottky barrier diode and a pn junction diode. Consider diodes with the parameters given in Example 9.5. We can assume that the pn junction diode will be sufficiently forward biased so that the ideal diffusion current will dominate. Let T 300 K. ■ Solution For the Schottky barrier diode, we have eV J JsT exp _a 1 kT Neglecting the (1) term, we can solve for the forward-bias voltage. We find J V ln _ J (0.0259) ln ___ 10 kT ln _ Va _ 0.312 V t e JsT JsT 5.98 105 For the pn junction diode, we have J (0.0259) ln ___ 10 Va Vt ln _ 0.682 V Js 3.66 1011 nea29583_ch09_331-370.indd 347 12/11/10 12:39 PM 348 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions ■ Comment A comparison of the two forward-bias voltages shows that the Schottky barrier diode has a turn-on voltage that, in this case, is approximately 0.37 V smaller than the turn-on voltage of the pn junction diode. ■ EXERCISE PROBLEM Ex 9.6 A pn junction diode and a Schottky diode have equal cross-sectional areas and have forward-bias currents of 0.5 mA. The reverse-saturation current of the Schottky diode is 5 107 A. The difference in forward-bias voltage between the two diodes is 0.30 V. Determine the reverse-saturation current of the pn junction diode. (Ans. 4.66 1012 A) The actual difference between the turn-on voltages will be a function of the barrier height of the metal–semiconductor contact and the doping concentrations in the pn junction, but the relatively large difference will always be realized. We will consider one application that utilizes the difference in turn-on voltage in Chapter 12, in what is referred to as a Schottky clamped transistor. The second major difference between a Schottky barrier diode and a pn junction diode is in the frequency response, or switching characteristics. In our discussion, we have considered the current in a Schottky diode as being due to the injection of majority carriers over a potential barrier. The energy-band diagram of Figure 9.1, for example, shows that there can be electrons in the metal directly adjacent to empty states in the semiconductor. If an electron from the valence band of the semiconductor were to flow into the metal, this effect would be equivalent to holes being injected into the semiconductor. This injection of holes would create excess minority carrier holes in the n region. However, calculations as well as measurements have shown that the ratio of the minority carrier hole current to the total current is extremely low in most cases. The Schottky barrier diode, then, is a majority carrier device. This fact means that there is no diffusion capacitance associated with a forward-biased Schottky diode. The elimination of the diffusion capacitance makes the Schottky diode a higherfrequency device than the pn junction diode. Also, when switching a Schottky diode from forward to reverse bias, there is no minority carrier stored charge to remove, as is the case in the pn junction diode. Since there is no minority carrier storage time, the Schottky diodes can be used in fast-switching applications. A typical switching time for a Schottky diode is in the picosecond range, while for a pn junction it is normally in the nanosecond range. TEST YOUR UNDERSTANDING TYU 9.4 (a) The reverse-saturation currents of a pn junction and a Schottky diode are 1014 A and 109 A, respectively. Determine the required forward-bias voltages in the pn junction diode and Schottky diode to produce a current of 100 A in each diode. (b) Repeat part (a) for forward bias currents of 1 mA. [Ans. (a) 0.596 V, 0.298 V; (b) 0.656 V, 0.358 V] nea29583_ch09_331-370.indd 348 12/11/10 12:39 PM 9.2 Metal–Semiconductor Ohmic Contacts 349 9.2 | METAL–SEMICONDUCTOR OHMIC CONTACTS Contacts must be made between any semiconductor device, or integrated circuit, and the outside world. These contacts are made via ohmic contacts. Ohmic contacts are metal-to-semiconductor contacts, but in this case they are not rectifying contacts. An ohmic contact is a low-resistance junction providing conduction in both directions between the metal and the semiconductor. Ideally, the current through the ohmic contact is a linear function of applied voltage, and the applied voltage should be very small. Two general types of ohmic contacts are possible: The first type is the ideal nonrectifying barrier, and the second is the tunneling barrier. We define in this section a specific contact resistance that is used to characterize ohmic contacts. 9.2.1 Ideal Nonrectifying Barrier We have considered an ideal metal-n-type semiconductor contact in Figure 9.1 for the case when m > s. Figure 9.11 shows the same ideal contact for the opposite case of m < s. In Figure 9.11a we see the energy levels before contact, and in Figure 9.11b, the barrier after contact for thermal equilibrium. To achieve thermal equilibrium in this junction, electrons flow from the metal into the lower energy states in the semiconductor, which makes the surface of the semiconductor more n type. The excess electron charge in the n-type semiconductor exists essentially as a surface charge density. If a positive voltage is applied to the metal, there is no barrier to electrons flowing from the semiconductor into the metal. If a positive voltage is applied to the semiconductor, the effective barrier height for electrons flowing from the metal into the semiconductor will be approximately Bn n, which is fairly small for a moderately to heavily doped semiconductor. For this bias condition, electrons can easily flow from the metal into the semiconductor. Figure 9.12a shows the energy-band diagram when a positive voltage is applied to the metal with respect to the semiconductor. Electrons can easily flow “downhill” eBn em e EF en es Ec EF EFi Ec EF EFi EF Ev Ev (a) (b) Figure 9.11 | Ideal energy-band diagram (a) before contact and (b) after contact for a metal-n-type semiconductor junction for m s. nea29583_ch09_331-370.indd 349 12/11/10 12:39 PM 350 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions Ec EF EF Ev Ec Ev (a) (b) Figure 9.12 | Ideal energy-band diagram of a metal-n-type semiconductor ohmic contact (a) with a positive voltage applied to the metal and (b) with a positive voltage applied to the semiconductor. e es em Ec EFi EF Ev EF Ec eBp EFi EF Ev EF ep (a) (b) Figure 9.13 | Ideal energy-band diagram (a) before contact and (b) after contact for a metal–p-type semiconductor junction for m s. from the semiconductor into the metal. Figure 9.12b shows the case when a positive voltage is applied to the semiconductor with respect to the metal. Electrons can easily flow over the barrier from the metal into the semiconductor. This junction, then, is an ohmic contact. Figure 9.13 shows an ideal nonrectifying contact between a metal and a p-type semiconductor. Figure 9.13a shows the energy levels before contact for the case when m > s. When contact is made, electrons from the semiconductor flow into the metal to achieve thermal equilibrium, leaving behind more empty states, or holes. The excess concentration of holes at the surface makes the surface of the semiconductor more p type. Electrons from the metal can readily move into the empty states in the semiconductor. This charge movement corresponds to holes flowing from the semiconductor into the metal. We can also visualize holes in the metal flowing into the semiconductor. This junction is also an ohmic contact. The ideal energy bands shown in Figures 9.11 and 9.13 do not take into account the effect of surface states. If we assume that acceptor surface states exist in nea29583_ch09_331-370.indd 350 12/11/10 12:39 PM 9.2 Metal–Semiconductor Ohmic Contacts 351 eBn e e EF Ec EF Ev Figure 9.14 | Energy-band diagram of a heavily doped n-semiconductor-tometal junction. the upper half of the semiconductor bandgap, then, since all the acceptor states are below EF for the case shown in Figure 9.11b, these surface states will be negatively charged and will alter the energy-band diagram. Similarly, if we assume that donor surface states exist in the lower half of the bandgap, then all of the donor states will be positively charged for the case shown in Figure 9.13b; the positively charged surface states will also alter this energy-band diagram. Therefore, if m < s for the metal-n-type semiconductor contact, and if m > s for the metal–p-type semiconductor contact, we may not necessarily form a good ohmic contact. 9.2.2 Tunneling Barrier The space charge width in a rectifying metal–semiconductor contact is inversely proportional to the square root of the semiconductor doping. The width of the depletion region decreases as the doping concentration in the semiconductor increases; thus, as the doping concentration increases, the probability of tunneling through the barrier increases. Figure 9.14 shows a junction in which the metal is in contact with a heavily doped n-type epitaxial layer. Objective: Calculate the space charge width for a Schottky barrier on a heavily doped semiconductor. Consider silicon at T 300 K doped at Nd 7 1018 cm3. Assume a Shottky barrier with Bn 0.67 V. For this case, we can assume that Vbi B0. Neglect the barrier lowering effect. EXAMPLE 9.7 ■ Solution From Equation (9.7), we have for zero applied bias 2sVbi xn _ eNd 12 2(11.7)(8.85 1014)(0.67) _____ (1.6 1019)(7 1018) 12 or xn 1. 1 106 cm 110 Å nea29583_ch09_331-370.indd 351 12/11/10 12:39 PM 352 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions ■ Comment In a heavily doped semiconductor, the depletion width is on the order of angstroms, so that tunneling is now a distinct possibility. For these types of barrier widths, tunneling may become the dominant current mechanism. ■ EXERCISE PROBLEM Ex 9.7 Calculate the space charge width of a rectifying metal–GaAs–semiconductor junction. Assume the n-type doping concentration is Nd 7 1018 cm3 and the built-in potential barrier is Vbi 0.80 V. (Ans. xn 128.7 Å) The tunneling current has the form eBn exp __ Eoo Jt where (9.29) ____ Nd _ e Eoo _ (9.30) sm*n 2 The tunneling current increases exponentially with doping concentration. 9.2.3 Specific Contact Resistance A figure of merit of ohmic contacts is the specific contact resistance, Rc. This parameter is defined as the reciprocal of the derivative of current density with respect to voltage evaluated at zero bias. We may write J Rc _ V 1 -cm2 V0 (9.31) We want Rc to be as small as possible for an ohmic contact. For a rectifying contact with a low to moderate semiconductor doping concentration, the current–voltage relation is given by Equation (9.23) as eBn eV 1 Jn A*T 2 exp __ exp _ kT kT The thermionic emission current is dominant in this junction. The specific contact resistance for this case is then eBn kT exp __ _ e kT ____ Rc (9.32) A*T 2 The specific contact resistance decreases rapidly as the barrier height decreases. For a metal–semiconductor junction with a high impurity doping concentration, the tunneling process will dominate. From Equations (9.29) and (9.30), the specific contact resistance is found to be Rc nea29583_ch09_331-370.indd 352 ____ 2 s mn _ Bn ⴢ ___ exp __ * Nd (9.33) 12/11/10 12:39 PM 9.2 Metal–Semiconductor Ohmic Contacts 353 ND (cm3) 1020 1019 107 1018 1017 300 K Theory PtSi–Si Al–Si B 0.85 V ⵑ ⵑ Rc (-cm2) 103 ⵑ ⵑ 105 101 1 101 0.60 ⵑ ⵑ 103 0.40 105 0 5 10 1 (1010 cm3/2) ND ⵑ ⵑ 107 30 Figure 9.15 | Theoretical and experimental specific contact resistance as a function of doping. (From Sze and Ng [15].) which shows that the specific contact resistance is a very strong function of semiconductor doping. Figure 9.15 shows a plot of the theoretical values of Rc as a function of semiconductor doping. For doping concentrations greater than approximately 1019 cm3, the tunneling process dominates and Rc shows the exponential dependence on Nd. For lower doping concentrations, the Rc values are dependent on the barrier heights and become almost independent of the doping. Also shown in the figure are experimental data for platinum silicide–silicon and aluminum–silicon junctions. Equation (9.33) is the specific contact resistance of the tunneling junction, which corresponds to the metal–n contact shown in Figure 9.14. However, the nn junction also has a specific contact resistance, since there is a barrier associated with this junction. For a fairly low doped n region, this contact resistance may actually dominate the total resistance of the junction. The theory of forming ohmic contacts is straightforward. To form a good ohmic contact, we need to create a low barrier and use a highly doped semiconductor at the surface. However, the actual technology of fabricating good, reliable ohmic contacts is not as easy in practice as in theory. It is also more difficult to fabricate good ohmic contacts on wide-bandgap materials. In general, low barriers are not possible on these materials, so a heavily doped semiconductor at the surface must be used to form a tunneling contact. The formation of a tunneling junction requires diffusion, ion implantation, or perhaps epitaxial growth. The surface doping concentration in nea29583_ch09_331-370.indd 353 12/11/10 12:39 PM 354 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions the semiconductor may be limited to the impurity solubility, which is approximately 5 1019 cm3 for n-type GaAs. Nonuniformities in the surface doping concentration may also prevent the theoretical limit of the specific contact resistance from being reached. In practice, a good deal of empirical processing is usually required before a good ohmic contact is obtained. 9.3 | HETEROJUNCTIONS In the discussion of pn junctions in the previous chapters, we assumed that the semiconductor material is homogeneous throughout the structure. This type of junction is called a homojunction. When two different semiconductor materials are used to form a junction, the junction is called a semiconductor heterojunction. As with many topics in this text, our goal is to provide the basic concepts concerning the heterojunction. The complete analysis of heterojunction structures involves quantum mechanics and detailed calculations that are beyond the scope of this text. The discussion of heterojunctions will, then, be limited to the introduction of some basic concepts. 9.3.1 Heterojunction Materials Since the two materials used to form a heterojunction will have different energy bandgaps, the energy band will have a discontinuity at the junction interface. We may have an abrupt junction in which the semiconductor changes abruptly from a narrow-bandgap material to a wide-bandgap material. On the other hand, if we have a GaAs–AlxGa1xAs system, for example, the value of x may continuously vary over a distance of several nanometers to form a graded heterojunction. Changing the value of x in the AlxGa1xAs system allows us to engineer, or design, the bandgap energy. In order to have a useful heterojunction, the lattice constants of the two materials must be well matched. The lattice match is important because any lattice mismatch can introduce dislocations resulting in interface states. For example, germanium and gallium arsenide have lattice constants matched to within approximately 0.13 percent. Germanium–gallium arsenide heterojunctions have been studied quite extensively. More recently, gallium arsenide–aluminum gallium arsenide (GaAs–AlGaAs) junctions have been investigated quite thoroughly, since the lattice constants of GaAs and the AlGaAs system vary by no more than 0.14 percent. 9.3.2 Energy-Band Diagrams In the formation of a heterojunction with a narrow-bandgap material and a widebandgap material, the alignment of the bandgap energies is important in determining the characteristics of the junction. Figure 9.16 shows three possible situations. In Figure 9.16a, we see the case when the forbidden bandgap of the wide-gap material completely overlaps the bandgap of the narrow-gap material. This case, called straddling, applies to most heterojunctions. We consider only this case here. The other possibilities are called staggered and broken gap and are shown in Figure 9.16b,c. nea29583_ch09_331-370.indd 354 12/11/10 12:39 PM 9.3 Heterojunctions 355 Ec1 Ec1 Ec2 Ec1 Ec2 Ev1 Ec2 Ev1 Ev1 Ev2 Ev 2 Ev2 (b) (a) (c) Figure 9.16 | Relation between narrow-bandgap and wide-bandgap energies: (a) straddling, (b) staggered, and (c) broken gap. There are four basic types of heterojunction. Those in which the dopant type changes at the junction are called anisotype. We can form nP or Np junctions, where the capital letter indicates the larger-bandgap material. Heterojunctions with the same dopant type on either side of the junction are called isotype. We can form nN and pP isotype heterojunctions. Figure 9.17 shows the energy-band diagrams of isolated n-type and P-type materials, with the vacuum level used as a reference. The electron affinity of the wide-bandgap material is less than that of the narrow-bandgap material. The difference between the two conduction band energies is denoted by Ec , and the difference between the two valence band energies is denoted by Ev . From Figure 9.17, we can see that Ec e(n P) (9.34a) Ec Ev EgP Egn Eg (9.34b) and In the ideal abrupt heterojunction using nondegenerately doped semiconductors, the vacuum level is parallel to both conduction bands and valence bands. If the vacuum level is continuous, then the same Ec and Ev discontinuities will exist at the Vacuum level eP en esn Ecn EFn EcP Ec esP Egn EgP Ge GaAs Evn Ev EFP EvP Figure 9.17 | Energy-band diagrams of a narrow-bandgap and a wide-bandgap material before contact. nea29583_ch09_331-370.indd 355 12/11/10 12:39 PM 356 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions eVbiP eVbi eVbin EcP eVbiP Ec EgP eVbin Ecn EFn EFP Egn EvP Ev Evn xn x xn xP x0 x xP Figure 9.18 | Ideal energy-band diagram of an nP heterojunction in thermal equilibrium. heterojunction interface. This ideal situation is known as the electron affinity rule. There is still some uncertainty about the applicability of this rule, but it provides a good starting point for the discussion of heterojunctions. Figure 9.18 shows a general ideal nP heterojunction in thermal equilibrium. In order for the Fermi levels in the two materials to become aligned, electrons from the narrow-gap n region and holes from the wide-gap P region must flow across the junction. As in the case of a homojunction, this flow of charge creates a space charge region in the vicinity of the metallurgical junction. The space charge width into the n-type region is denoted by xn and the space charge width into the P-type region is denoted by xP. The discontinuities in the conduction and valence bands and the change in the vacuum level are shown in the figure. 9.3.3 Two-Dimensional Electron Gas Before we consider the electrostatics of the heterojunction, we will discuss a unique characteristic of an isotype junction. Figure 9.19 shows the energy-band diagram of an nN GaAs–AlGaAs heterojunction in thermal equilibrium. The AlGaAs can be moderately to heavily doped n type, while the GaAs can be more lightly doped or even intrinsic. As mentioned previously, to achieve thermal equilibrium, electrons from the wide-bandgap AlGaAs flow into the GaAs, forming an accumulation layer of electrons in the potential well adjacent to the interface. One basic quantummechanical result that we have found previously is that the energy of an electron contained in a potential well is quantized. The phrase two-dimensional electron gas nea29583_ch09_331-370.indd 356 12/11/10 12:39 PM 9.3 eVbiN Ecn EFn Ec Egn Heterojunctions 357 EcN EFN eVbin EgN Evn Ev EvN Figure 9.19 | Ideal energy-band diagram of an nN heterojunction in thermal equilibrium. refers to the condition in which the electrons have quantized energy levels in one spatial direction (perpendicular to the interface), but are free to move in the other two spatial directions. The potential function near the interface can be approximated by a triangular potential well. Figure 9.20a shows the conduction band edges near the abrupt junction interface and Figure 9.20b shows the approximation of the triangular potential well. We can write V(x) eEz z0 (9.35a) V(z) z (9.35b) 0 Schrodinger’s wave equation can be solved using this potential function. The quantized energy levels are shown in Figure 9.20b. Higher energy levels are usually not considered. V(z) Ec2 EF Ec1 E1 EF E0 GaAs AlGaAs Ev2 z 0 Ev1 (a) (b) Figure 9.20 | (a) Conduction-band edge at N-AlGaAs, n-GaAs heterojunction; (b) triangular well approximation with discrete electron energies. nea29583_ch09_331-370.indd 357 12/11/10 12:39 PM 358 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions n(z) Doped Undoped Ec2 Ec1 EF AlGaAs z Figure 9.21 | Electron density in triangular potential well. GaAs Figure 9.22 | Conduction-band edge at a graded heterojunction. The qualitative distribution of electrons in the potential well is shown in Figure 9.21. A current parallel to the interface will be a function of this electron concentration and of the electron mobility. Since the GaAs can be lightly doped or intrinsic, the two-dimensional electron gas is in a region of low impurity doping so that impurity scattering effects are minimized. The electron mobility will be much larger than if the electrons were in the same region as the ionized donors. The movement of the electrons parallel to the interface will still be influenced by the coulomb attraction of the ionized impurities in the AlGaAs. The effect of these forces can be further reduced by using a graded AlGaAs–GaAs heterojunction. The graded layer is AlxGa1xAs in which the mole fraction x varies with distance. In this case, an intrinsic layer of graded AlGaAs can be sandwiched between the N-type AlGaAs and the intrinsic GaAs. Figure 9.22 shows the conduction-band edges across a graded AlGaAs–GaAs heterojunction in thermal equilibrium. The electrons in the potential well are further separated from the ionized impurities so that the electron mobility is increased above that in an abrupt heterojunction. *9.3.4 Equilibrium Electrostatics We now consider the electrostatics of the nP heterojunction that is shown in Figure 9.18. As in the case of the homojunction, potential differences exist across the space charge regions in both the n region and the P region. These potential differences correspond to the built-in potential barriers on either side of the junction. The built-in potential barrier for this ideal case is defined as shown in Figure 9.18 to be the potential difference across the vacuum level. The built-in potential barrier is the sum of the potential differences across each of the space charge regions. The heterojunction built-in potential barrier, however, is not equal to the difference between the conduction bands across the junction or the difference between the valence bands across the junction, as we defined for the homojunction. Ideally, the total built-in potential barrier Vbi can be found as the difference between the work functions, or Vbi sP sn nea29583_ch09_331-370.indd 358 (9.36) 12/11/10 12:39 PM 9.3 Heterojunctions 359 Equation (9.36), from Figure 9.17, can be written as eVbi [eP EgP (EFP EvP)] [en Egn (EFn Evn)] (9.37a) eVbi e(P n) (EgP Egn) (EFn Evn) (EFP EvP) (9.37b) or which can be expressed as Nvn NvP _ eVbi Ec Eg kT ln _ pno kT ln ppo (9.38) Finally, we can write Equation (9.38) as ppo _ Nvn eVbi Ev kT ln _ pno ⴢ NvP (9.39) where ppo and pno are the hole concentrations in the P and n materials, respectively, and Nvn and NvP are the effective density of states functions in the n and P materials, respectively. We can also obtain an expression for the built-in potential barrier in terms of the conduction band shift as nno _ NcP eVbi Ec kT ln _ (9.40) npo ⴢ Ncn Objective: Determine Ec , Ev , and Vbi for an n–Ge to P–GaAs heterojunction using the EXAMPLE 9.8 electron affinity rule. Consider n-type Ge doped with Nd 1016 cm3 and P-type GaAs doped with Na 1016 cm3. Let T 300 K so that ni 2.4 1013 cm3 for Ge. ■ Solution From Equation (9.34a), we have Ec e(n P) e(4.13 4.07) 0.06 eV and from Equation (9.34b), we have Ev Eg Ec (1.43 0.67) 0.06 0.70 eV To determine Vbi using Equation (9.39), we need to determine pno in Ge, or n2i (2.4 1013)2 pno _ 5.76 1010 cm3 ___ Nd 1016 Then (1016)(6 1018) eVbi 0.70 (0.0259) ln ____ (5.76 1010)(7 1018) or, finally, Vbi 1.0 V ■ Comment There is a nonsymmetry in the Ec and Ev values that will tend to make the potential barriers seen by electrons and holes different. This nonsymmetry does not occur in homojunctions. nea29583_ch09_331-370.indd 359 12/11/10 12:39 PM 360 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions ■ EXERCISE PROBLEM Ex 9.8 Repeat Example 9.8 for an n-Ge-to-P-GaAs heterojunction. The Ge is doped with Nd 1015 cm3 donors and the GaAs doped with Na 1015 cm3 acceptors. Let T 300 K. (Ans. Vbi 0.889 V) We can determine the electric field and potential in the junction from Poisson’s equation in exactly the same way as we do for the homojunction. For homogeneous doping on each side of the junction, we have in the n region eNdn En _ n (xn x) (xn x 0) (9.41a) x xP) (9.41b) and in the P region eNaP EP _ P (xP x) (0 where n and P are the permittivities of the n and P materials, respectively. We may note that En 0 at x xn and EP 0 at x xP. The electric flux density D is continuous across the junction, so n En(x 0) P EP(x 0) (9.42a) Ndn xn NaPxP (9.42b) which gives Equation (9.42b) simply states that the net negative charge in the P region is equal to the net positive charge in the n region—the same condition we had in a pn homojunction. We are neglecting any interface states that may exist at the heterojunction. The electric potential can be found by integrating the electric field through the space charge region so that the potential difference across each region can be determined. We find that eNdn x2 (9.43a) Vbin __n 2n and eNaP x2 VbiP __P 2P (9.43b) Equation (9.42b) can be rewritten as N xn _ _ aP xP (9.44) Ndn The ratio of the built-in potential barriers can then be determined as x PNaP Vbin _ Ndn _ _ P ⴢ_ ⴢ n _ 2 VbiP n NaP 2 P x n Ndn (9.45) Assuming that n and P are of the same order of magnitude, the larger potential difference is across the lower-doped region. nea29583_ch09_331-370.indd 360 12/11/10 12:39 PM 9.3 Heterojunctions 361 The total built-in potential barrier is eNdnx2 eNaPx2 Vbi Vbin VbiP __n __P (9.46) 2n 2P If we solve for xP, for example, from Equation (9.42b) and substitute into Equation (9.46), we can solve for xn as 2n P NaP Vbi xn ____ eNdn(nNdn P NaP) 12 (9.47a) We can also find 2n P NdnVbi xP ____ eNaP (n Ndn P NaP) 12 (9.47b) The total depletion width is found to be 2n P (Ndn NaP)2 Vbi W xn xP ____ eNdnNaP(nNdn P NaP) 12 (9.48) If a reverse-biased voltage is applied across the heterojunction, the same equations apply if Vbi is replaced by Vbi VR . Similarly, if a forward bias is applied, the same equations also apply if Vbi is replaced by Vbi Va. As explained earlier, VR is the magnitude of the reverse-biased voltage and Va is the magnitude of the forward-bias voltage. As in the case of a homojunction, a change in depletion width with a change in junction voltage yields a junction capacitance. We can find for the nP junction eNdnNaPnP Cj _____ 2(nNdn PNaP)(Vbi VR) 12 (F/cm2) (9.49) A plot of (1Cj)2 versus VR again yields a straight line. The extrapolation of this plot of (1Cj )2 0 is used to find the built-in potential barrier, Vbi. Figure 9.18 shows the ideal energy-band diagram for the nP abrupt heterojunction. The experimentally determined values of Ec and Ev may differ from the ideal values determined using the electron affinity rule. One possible explanation for this difference is that most heterojunctions have interface states. If we assume that the electrostatic potential is continuous through the junction, then the electric flux density will be discontinuous at the heterojunction due to the surface charge trapped in the interface states. The interface states will then change the energy-band diagram of the semiconductor heterojunction just as they changed the energy-band diagram of the metal–semiconductor junction. Another possible explanation for the deviation from the ideal is that as the two materials are brought together to form the heterojunction, the electron orbitals of each material begin to interact with each other, resulting in a transition region of a few angstroms at the interface. The energy bandgap is then continuous through this transition region and not a characteristic of either material. However, we still have the relation Ec Ev Eg (9.50) for the straddling type of heterojunction, although the Ec and Ev values may differ from those determined from the electron affinity rule. nea29583_ch09_331-370.indd 361 12/11/10 12:39 PM 362 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions Ecp Ec EcN EFN Egp EFp Evp Ev EgN EvN Figure 9.23 | Ideal energy-band diagram of an Np heterojunction in thermal equilibrium. We may consider the general characteristics of the energy-band diagrams of the other types of heterojunction. Figure 9.23 shows the energy-band diagram of an Np heterojunction. The same Ec and Ev discontinuities exist, although the general shape of the conduction band, for example, is different in the nP and the Np junctions. This difference in energy bands will influence the I–V characteristics of the two junctions. The other two types of heterojunctions are the nN and the pP isotype junctions. The energy-band diagram of the nN junction is shown in Figure 9.19. To achieve thermal equilibrium, electrons from the wide-bandgap material will flow into the narrowbandgap material. A positive space charge region exists in the wide-bandgap material and an accumulation layer of electrons now exists at the interface in the narrow-bandgap material. Since there are a large number of allowed energy states in the conduction band, we expect the space charge width xn and the built-in potential barrier Vbin to be small in the narrow-gap material. The energy-band diagram of the pP heterojunction in thermal equilibrium is shown in Figure 9.24. To achieve thermal equilibrium, holes from the wide-bandgap material will flow into the narrow-bandgap material, creating an accumulation layer of holes in the narrow-bandgap material at the interface. These types of isotype heterojunctions are obviously not possible in a homojunction. EcP Ec Ecp EgP Egp EFp Evp Ev EFP EvP Figure 9.24 | Ideal energy-band diagram of a pP heterojunction in thermal equilibrium. nea29583_ch09_331-370.indd 362 12/11/10 12:39 PM 9.4 *9.3.5 Summary 363 Current–Voltage Characteristics The ideal current–voltage characteristics of a pn homojunction have been developed in Chapter 8. Since the energy-band diagram of a heterojunction is more complicated than that of a homojunction, we would expect the I–V characteristics of the two junctions to differ. One immediate difference between a homojunction and a heterojunction is in the barrier heights seen by the electrons and holes. Since the built-in potential barrier for electrons and holes in a homojunction is the same, the relative magnitude of the electron and hole currents is determined by the relative doping levels. In a heterojunction, the barrier heights seen by electrons and holes are not the same. The energy-band diagrams in Figures 9.18 and 9.23 demonstrate that the barrier heights for electrons and holes in a heterojunction can be significantly different. The barrier height for electrons in Figure 9.18 is larger than that for holes, so we would expect the current due to electrons to be insignificant compared to the hole current. If the barrier height for electrons is 0.2 eV larger than that for holes, the electron current will be approximately a factor of 104 smaller than the hole current, assuming all other parameters are equal. The opposite situation exists for the band diagram shown in Figure 9.23. The conduction-band edge in Figure 9.23 and the valence-band edge in Figure 9.18 are somewhat similar to that of a rectifying metal–semiconductor contact. We derive the current–voltage characteristics of a heterojunction, in general, on the basis of thermionic emission of carriers over the barrier, as we do in the case of metal–semiconductor junction. We can then write E J A* T 2 exp _w kT (9.51) where Ew is an effective barrier height. The barrier height can be increased or reduced by an applied potential across the junction as in the case of a pn homojunction or a Schottky barrier junction. The heterojunction I–V characteristics, however, may need to be modified to include diffusion effects and tunneling effects. Another complicating factor is that the effective mass of a carrier changes from one side of the junction to the other. Although the actual derivation of the I–V relationship of the heterojunction is complex, the general form of the I–V equation is still similar to that of a Schottky barrier diode and is generally dominated by one type of carrier. 9.4 | SUMMARY ■ ■ A metal on a lightly doped semiconductor can produce a rectifying contact that is known as a Schottky barrier diode. The ideal barrier height between the metal and semiconductor is the difference between the metal work function and the semiconductor electron affinity. When a positive voltage is applied to an n-type semiconductor with respect to the metal (reverse bias), the barrier between the semiconductor and metal increases so that there is essentially no flow of charged carriers. When a positive voltage is applied to the metal with respect to an n-type semiconductor (forward bias), the barrier between the semiconductor and metal is lowered so that electrons can easily flow from the semiconductor into the metal by a process called thermionic emission. nea29583_ch09_331-370.indd 363 12/11/10 12:39 PM 364 CHAPTER 9 ■ ■ ■ Metal–Semiconductor and Semiconductor Heterojunctions The ideal current–voltage relationship of the Schottky barrier diode is the same as that of the pn junction diode. However, since the current mechanism is different from that of the pn junction diode, the switching speed of the Schottky diode is faster. In addition, the reverse saturation current of the Schottky diode is larger than that of the pn junction diode, so a Schottky diode requires less forward bias voltage to achieve a given current compared to a pn junction diode. Metal–semiconductor junctions can also form ohmic contacts, which are low-resistance junctions providing conduction in both directions with very little voltage drop across the junction. Semiconductor heterojunctions are formed between two semiconductor materials with different bandgap energies. One useful property of a heterojunction is the creation of a potential well at the interface. Electrons are confined to the potential well in the direction perpendicular to the interface, but are free to move in the other two directions. GLOSSARY OF IMPORTANT TERMS anisotype junction A heterojunction in which the type of dopant changes at the metallurgical junction. electron affinity rule The rule stating that, in an ideal heterojunction, the discontinuity at the conduction band is the difference between the electron affinities in the two semiconductors. heterojunction The junction formed by the contact between two different semiconductor materials. image force–induced lowering The lowering of the peak potential barrier at the metal– semiconductor junction due to an electric field. isotype junction A heterojunction in which the type of dopant is the same on both sides of the junction. ohmic contact A low-resistance metal–semiconductor contact providing conduction in both directions between the metal and semiconductor. Richardson constant The parameter A* in the current–voltage relation of a Schottky diode. Schottky barrier height The potential barrier Bn from the metal to semiconductor in a metal–semiconductor junction. Schottky effect Another term for image force–induced lowering. specific contact resistance The inverse of the slope of the J versus V curve of a metal– semiconductor contact evaluated at V 0. thermionic emission The process by which charge flows over a potential barrier as a result of carriers with sufficient thermal energy. tunneling barrier A thin potential barrier in which the current is dominated by the tunneling of carriers through the barrier. two-dimensional electron gas (2-DEG) The accumulation layer of electrons contained in a potential well at a heterojunction interface. The electrons are free to move in the “other” two spatial directions. CHECKPOINT After studying this chapter, the reader should have the ability to: ■ ■ nea29583_ch09_331-370.indd 364 Sketch the energy-band diagram of zero-biased, reverse-biased, and forward-biased Schottky barrier diodes. Describe the charge flow in a forward-biased Schottky barrier diode. 12/11/10 12:39 PM Problems ■ ■ ■ ■ ■ ■ 365 Explain the Schottky barrier lowering and its effect on the reverse saturation current in a Schottky barrier diode. Explain the effect of interface states on the characteristics of a Schottky barrier diode. Describe one effect of a larger reverse saturation current in a Schottky barrier diode compared to that of a pn junction diode. Describe what is meant by an ohmic contact. Draw the energy-band diagram of an nN heterojunction. Explain what is meant by a two-dimensional electron gas. REVIEW QUESTIONS 1. 2. 3. 4. 5. 6. 7. 8. 9. What is the ideal Schottky barrier height? Indicate the Schottky barrier height on an energy-band diagram. Using an energy-band diagram, indicate the effect of the Schottky barrier lowering. What is the mechanism of charge flow in a forward-biased Schottky barrier diode? Compare the forward-biased current–voltage characteristic of a Schottky barrier diode to that of pn junction diode. Explain the difference in switching characteristics between a Schottky diode and a pn junction diode. Discuss charge storage effects. Sketch the ideal energy-band diagram of a metal–semiconductor junction in which m s. Explain why this is an ohmic contact. Sketch the energy-band diagram of a tunneling junction. Why is this an ohmic contact? What is a heterojunction? What is a 2-D electron gas? PROBLEMS (In the following problems, assume A* 120 A/K2-cm2 for silicon and A* 1.12 A/K2-cm2 for gallium arsenide Schottky diodes unless otherwise stated.) Section 9. 1 The Schottky Barrier Diode 9.1 9.2 9.3 9.4 Consider a contact between Al and n Si doped at Nd 1016 cm3. T 300 K. (a) Draw the energy-band diagrams of the two materials before the junction is formed. (b) Draw the ideal energy band at zero bias after the junction is formed. (c) Calculate B0, xd, and Emax for part (b). (d) Repeat parts (b) and (c) using the data in Figure 9.5. (a) A Schottky barrier diode formed on n-type silicon has a doping concentration of Nd 5 1015 cm3 and a barrier height of B0 0.65 V. Determine the builtin potential barrier Vbi. (b) If the doping concentration changes to Nd 1016 cm3, determine the values of B0 and Vbi. Do these values increase, decrease, or remain the same? (c) Repeat part (b) if the doping concentration is Nd 1015 cm3. Gold is deposited on n-type silicon forming an ideal rectifying junction. The doping concentration is Nd 1016 cm3. Assume T 300 K. Determine the theoretical values of (a) B0, (b) Vbi, and (c) xn and Emax at (i) VR 1 V and (ii) VR 5 V. A Schottky diode is formed by depositing gold on n-type GaAs that is doped at a concentration of Nd 5 1015 cm3. For T 300 K, determine the theoretical values of (a) B0, (b) n, (c) Vbi, and (d) xn and Emax at (i) VR 1 V and (ii) VR 5 V. nea29583_ch09_331-370.indd 365 12/11/10 12:39 PM CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions 15 366 1 2 1 C ( ) 10 3 2 1 0 1 VR (V) 2 Figure P9.7 | Figure for Problem 9.7. 9.5 Repeat Problem 9.4, parts (b) through (d), if the experimentally determined barrier height is found to be Bn 0.88 V. 9.6 (a) A Pt–n-type silicon junction with Nd 1015 cm3 has a cross-sectional area of A 104 cm2. Let T 300 K. Using the data shown in Figure 9.5, determine the junction capacitance at (i) VR 1 V and (ii) VR 5 V. (b) Repeat part (a) for a doping concentration of Nd 1016 cm3. 9.7 A Schottky diode with n-type GaAs at T 300 K yields the 1C2 versus VR plot shown in Figure P9.7, where C is the capacitance per cm2. Determine (a) Vbi, (b) Nd, (c) n, and (d) B0. 9.8 Consider a W–n-type silicon Schottky barrier at T 300 K with Nd 5 1015 cm3. Use the data in Figure 9.5 to determine the barrier height. (a) Determine Vbi, xn, and Emax for (i) VR 1 V and (ii) VR 5 V. (b) Using the values of Emax from part (a), determine the Schottky barrier lowering parameters and xm. 9.9 Starting with Equation (9.12), derive Equations (9.14) and (9.15). 9.10 A Au-n-GaAs Schottky diode at T 300 K is doped at a concentration of Nd 1016 cm3. Use the data in Figure 9.5 to determine the barrier height. Then determine (a) Vbi, xn, and Emax for zero bias. (b) Determine the reverse-biased voltage at which the Schottky barrier lowering, , will be 5 percent of the barrier height. 9.11 Consider n-type silicon doped at Nd 1016 cm3 with a gold contact to form a Schottky diode. Investigate the effect of Schottky barrier lowering. (a) Plot the Schottky barrier lowering versus reverse-biased voltage over the range 0 VR 50 V. (b) Plot the ratio JsT(VR)JsT(VR 0) over the same range of reversebiased voltage. *9.12 The energy-band diagram of a Schottky diode is shown in Figure 9.6. Assume the following parameters: m 5.2 V Eg 1.43 eV s (13.1)0 n 0.10 V 25 Å 4.07 V 0 0.60 V i 0 Nd 1016 cm3 Dit 1013 eV1 cm2 (a) Determine the theoretical barrier height B0 without interface states. (b) Determine the barrier height with interface states. (c) Repeat parts (a) and (b) if m 4.5 V. *Asterisks next to problems indicate problems that are more difficult. nea29583_ch09_331-370.indd 366 12/11/10 12:39 PM Problems 367 *9.13 A Schottky barrier diode contains interface states and an interfacial layer. Assume the following parameters: m 4.75 V Eg 1. 12 eV s (11.7)0 9.14 9.15 9.16 9.17 9.18 *9.19 9.20 9.21 9.22 n 0.164 V 20 Å 4.01 V 0 0.230 V i 0 Nd 5 1016 cm3 B0 0.60 V Determine the interface state density, Dit, in units of eV1 cm2. A Schottky diode at T 300 K is formed with Pt on n-type silicon with a doping concentration of Nd 5 1015 cm3. The barrier height is found to be Bn 0.89 V. Determine (a) n, (b) Vbi, (c) JsT, and (d) Va such that Jn 5 A/cm2. (Neglect the barrier lowering effect.) (a) Consider a Schottky diode at T 300 K that is formed with tungsten on n-type silicon. Use Figure 9.5 to determine the barrier height. Assume a doping concentration of Nd 1016 cm3 and assume a cross-sectional area A 104 cm2. Determine the forward-bias voltage required to induce a current of (i) 10 A, (ii) 100 A, and (iii) 1 mA. (b) Repeat part (a) for a temperature of T 350 K. (Neglect the barrier lowering effect.) An Au-n-GaAs Schottky diode at T 300 K has a doping concentration of Nd 1016 cm3. (a) Using Figure 9.5, determine the barrier height. (b) Calculate the reverse-biased saturation current JsT. (c) Determine the forward-bias voltage required to induce a current density of Jn 10 A/cm2. (d) What is the change in forwardbias voltage necessary to double the current density? (Neglect the Schottky barrier lowering.) (a) Consider an Au–n-type GaAs Schottky diode with a cross-sectional area of 104 cm2. Plot the forward-bias current–voltage characteristics over a voltage range of 0 VD 0.5 V. Plot the current on a log scale. (b) Repeat part (a) for an Au–n-type silicon Schottky diode. (c) What conclusions can be drawn from these results? A Schottky diode at T 300 K is formed between tungsten and n-type silicon doped at Nd 1016 cm3. The cross-sectional area is A 104 cm2. Determine the reverse-biased saturation current at (a) VR 2 V and (b) VR 4 V. (Take into account the Schottky barrier lowering.) Starting with the basic current equation given by Equation (9.18), derive the relation given by Equation (9.23). The reverse-saturation current densities in a pn junction diode and a Schottky diode are 1011 A/cm2 and 6 108 A/cm2, respectively, at T 300 K. The cross-sectional area of the Schottky diode is A 104 cm2. The current in each diode is 0.80 mA. The difference in forward-bias voltages between the two diodes is 0.285 V. Determine (a) the voltage applied to each diode and (b) the cross-sectional area of the pn junction diode. A pn junction diode and a Schottky diode each have cross-sectional areas of A 8 104 cm2. The reverse saturation current densities at T 300 K for the pn junction diode and Schottky diode are 8 1013 A/cm2 and 6 109 A/cm2, respectively. Determine the required forward-bias voltage in each diode to yields currents of (a)150 A, (b) 700 A, and (c) 1.2 mA. (a) The two diodes described in Problem 9.21 are connected in series and are driven by a constant current source of 0.80 mA. Determine (i) the current in each diode and nea29583_ch09_331-370.indd 367 12/11/10 12:39 PM 368 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions (ii) the voltage across each diode. (b) Repeat part (a) for the case when the diodes are connected in parallel. 9.23 A Schottky diode and a pn junction diode have cross-sectional areas of A 7 104 cm2. The reverse-saturation current densities at T 300 K of the Schottky diode and pn junction are 4 108 A/cm2 and 3 1012 A/cm2, respectively. A forward-bias current of 0.8 mA is required in each diode. (a) Determine the forward-bias voltage required across each diode. (b) If the voltage from part (a) is maintained across each diode, determine the current in each diode if the temperature is increased to 400 K. (Take into account the temperature dependence of the reversesaturation currents. Assume Eg 1.12 eV for the pn junction diode and B0 0.82 V for the Schottky diode.) 9.24 Compare the current–voltage characteristics of a Schottky barrier diode and a pn junction diode. Use the results of Example 9.5 and assume diode areas of 5 104 cm2. Plot the current–voltage characteristics on a linear scale over a current range of 0 ID 10 mA. Section 9.2 9.25 9.26 9.27 9.28 9.29 9.30 9.31 nea29583_ch09_331-370.indd 368 Metal–Semiconductor Ohmic Contacts The contact resistance of an ohmic contact is Rc 104 -cm2. Determine the junction resistance if the cross-sectional area is (a) 103 cm2, (b) 104 cm2, and (c) 105 cm2. (a) The contact resistance of an ohmic contact is Rc 5 105 -cm2. The crosssectional area of the junction is 105 cm2. Determine the voltage across the junction if the current is (i) I 1 mA and (ii) I 100 A. (b) Repeat part (a) if the crosssectional area is 106 cm2. An ohmic contact between a metal and silicon may be formed that has a very low barrier height. (a) Determine the value of Bn that will produce a contact resistance of Rc 5 105 -cm2 at T 300 K. (b) Repeat part (a) for a contact resistance of Rc 5 106 -cm2. A metal, with a work function m 4.2 V, is deposited on an n-type silicon semiconductor with s 4.0 V and Eg 1.12 eV. Assume no interface states exist at the junction. Let T 300 K. (a) Sketch the energy-band diagram for zero bias for the case when no space charge region exists at the junction. (b) Determine Nd so that the condition in part (a) is satisfied. (c) What is the potential barrier height seen by electrons in the metal moving into the semiconductor? Consider the energy-band diagram of a silicon Schottky junction under zero bias shown in Figure P9.29. Let B0 0.7 V and T 300 K. Determine the doping required so that xd 50 Å at the point where the potential is B02 below the peak value. (Neglect the barrier lowering effect.) A metal–semiconductor junction is formed between a metal with a work function of 4.3 eV and p-type silicon with an electron affinity of 4.0 eV. The acceptor doping concentration in the silicon is Na 5 1016 cm3. Assume T 300 K. (a) Sketch the thermal equilibrium energy-band diagram. (b) Determine the height of the Schottky barrier. (c) Sketch the energy-band diagram with an applied reverse-biased voltage of VR 3 V. (d) Sketch the energy-band diagram with an applied forward-bias voltage of Va 0.25 V. (a) Consider a metal–semiconductor junction formed between a metal with a work function of 4.65 eV and Ge with an electron affinity of 4.13 eV. The doping 12/11/10 12:39 PM Problems 369 B0 2 xd Ec EF Ev Figure P9.29 | Figure for Problem 9.29. concentration in the Ge material is Nd 6 1013 cm3 and Na 3 1013 cm3. Assume T 300 K. Sketch the zero bias energy-band diagram and determine the Schottky barrier height. (b) Repeat part (a) if the metal work function is 4.35 eV. Section 9.3 Heterojunctions 9.32 Sketch the energy-band diagrams of an abrupt Al0.3Ga0.7As–GaAs heterojunction for: (a) N–AlGaAs, intrinsic GaAs, (b) N–AlGaAs, p–GaAs, and (c) P–AlGaAs, n– GaAs. Assume Eg 1.85 eV for Al0.3Ga0.7As and assume Ec _23 Eg. 9.33 Repeat Problem 9.32 assuming the ideal electron affinity rule. Determine Ec and Ev. *9.34 Starting with Poisson’s equation, derive Equation (9.48) for an abrupt heterojunction. Summary and Review *9.35 (a) Derive an expression for dVadT as a function of current density in a Schottky diode. Assume the minority carrier current is negligible. (b) Compare dVadT for a GaAs Schottky diode to that for a Si Schottky diode. (c) Compare dVadT for a Si Schottky diode to that for a Si pn junction diode. 9.36 The (1Cj)2 versus VR data are measured for two Schottky diodes with equal areas. One diode is fabricated with 1 -cm silicon and the other diode with 5 -cm silicon. The plots intersect the voltage axis as VR 0.5 V for diode A and at VR 1.0 V for diode B. The slope of the plot for diode A is 1.5 1018 (F2-V)1 and that for diode B is 1.5 1017 (F2-V)1. Determine which diode has the higher metal work function and which diode has the lower resistivity silicon. *9.37 Both Schottky barrier diodes and ohmic contacts are to be fabricated by depositing a particular metal on a silicon integrated circuit. The work function of the metal is 4.5 V. Considering the ideal metal–semiconductor contact, determine the allowable range of doping concentrations for each type of contact. Consider both p- and n-type silicon regions. 9.38 Consider an n-GaAs–p-AlGaAs heterojunction in which the bandgap offsets are Ec 0.3 eV and Ev 0. 15 eV. Discuss the difference in the expected electron and hole currents when the junction is forward biased. nea29583_ch09_331-370.indd 369 12/11/10 12:39 PM 370 CHAPTER 9 Metal–Semiconductor and Semiconductor Heterojunctions READING LIST 1. 2. 3. 4. 5. 6. 7. 8. *9. 10. *11. *12. 13. 14. 15. *16. *17. 18. *19. Anderson, R. L. “Experiments on Ge–GaAs Heterojunctions.” Solid-State Electronics 5, no. 5 (September–October 1962), pp. 341–351. Crowley, A. M., and S. M. Sze. “Surface States and Barrier Height of Metal– Semiconductor Systems.” Journal of Applied Physics 36 (1965), p. 3212. Hu, C. C. Modern Semiconductor Devices for Integrated Circuits. Upper Saddle River, NJ: Pearson Prentice Hall, 2010. MacMillan, H. F., H. C. Hamaker, G. F. Virshup, and J. G. Werthen. “Multijunction III-V Solar Cells: Recent and Projected Results.” Twentieth IEEE Photovoltaic Specialists Conference (1988), pp. 48–54. Michaelson, H. B. “Relation between an Atomic Electronegativity Scale and the Work Function.” IBM Journal of Research and Development 22, no. 1 (January 1978), pp. 72–80. Pierret, R. F. Semiconductor Device Fundamentals. Reading, MA: Addison-Wesley, 1996. Rideout, V. L. “A Review of the Theory, Technology and Applications of Metal–Semiconductor Rectifiers.” Thin Solid Films 48, no. 3 (February 1, 1978), pp. 261–291. Roulston, D. J. Bipolar Semiconductor Devices. New York: McGraw-Hill, 1990. Shur, M. GaAs Devices and Circuits. New York: Plenum Press, 1987. ———. Introduction to Electronic Devices. New York: John Wiley and Sons, 1996. ———. Physics of Semiconductor Devices. Englewood Cliffs, NJ: Prentice Hall, 1990. Singh, J. Physics of Semiconductors and Their Heterostructures. New York: McGraw-Hill, 1993. ———. Semiconductor Devices: Basic Principles. New York: John Wiley and Sons, 2001. Streetman, B. G., and S. K. Banerjee. Solid State Electronic Devices. 6th ed. Upper Saddle River, NJ: Pearson Prentice Hall, 2006. Sze, S. M., and K. K. Ng. Physics of Semiconductor Devices, 3rd ed. Hoboken, NJ: John Wiley and Sons, 2007. Wang, S. Fundamentals of Semiconductor Theory and Device Physics. Englewood Cliffs, NJ: Prentice Hall, 1989. Wolfe, C. M., N. Holonyak, Jr., and G. E. Stillman. Physical Properties of Semiconductors. Englewood Cliffs, NJ: Prentice Hall, 1989. Yang, E. S. Microelectronic Devices. New York: McGraw-Hill, 1988. Yuan, J. S. SiGe, GaAs, and InP Heterojunction Bipolar Transistors. New York: John Wiley and Sons, 1999. *Indicates references that are at an advanced level compared to this text. nea29583_ch09_331-370.indd 370 12/11/10 12:39 PM 10 C H A P T E R Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor T he single-junction semiconductor devices that we have considered, including the pn homojunction diode, can be used to produce rectifying current–voltage characteristics and to form electronic switching circuits. The transistor is a multijunction semiconductor device that, in conjunction with other circuit elements, is capable of current gain, voltage gain, and signal power gain. The basic transistor action is the control of current at one terminal by the voltage applied across the other two terminals of the device. The Metal–Oxide–Semiconductor Field-Effect Transistor (MOSFET) is one of two major types of transistors. The fundamental physics of the MOSFET is developed in this chapter. The MOSFET is used extensively in digital circuit applications where, because of its small size, millions of devices can be fabricated in a single integrated circuit. Two complementary configurations of MOS transistors, the n-channel MOSFET and the p-channel MOSFET, can be fabricated. Electronic circuit design becomes very versatile when the two types of devices are used in the same circuit. These circuits are referred to as complementary MOS (CMOS) circuits. ■ 10.0 | PREVIEW In this chapter, we will: ■ Study the characteristics of energy bands as a function of applied voltage in the metal–oxide–semiconductor structure known as the MOS capacitor. The MOS capacitor is the heart of the MOSFET. ■ Discuss the concept of surface inversion in the semiconductor of the MOS capacitor. 371 nea29583_ch10_371-442.indd 371 12/11/10 12:40 PM 372 CHAPTER 10 ■ ■ ■ ■ ■ Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Define and derive the expression for the threshold voltage, which is a basic parameter of the MOSFET. Discuss various physical structures of MOSFETs, including enhancement and depletion mode devices. Derive the ideal current–voltage relationship of the MOSFET. Develop the small-signal equivalent circuit of the MOSFET. This circuit is used to relate small-signal currents and voltages in analog circuits. Derive the frequency limiting factors of the MOSFET. 10.1 | THE TWO-TERMINAL MOS STRUCTURE The heart of the MOSFET is the MOS capacitor shown in Figure 10.1. The metal may be aluminum or some other type of metal, although in many cases, it is actually a high-conductivity polycrystalline silicon that has been deposited on the oxide; however, the term metal is usually still used. The parameter tox in the figure is the thickness of the oxide and ox is the permittivity of the oxide. 10.1.1 Energy-Band Diagrams The physics of the MOS structure can be more easily explained with the aid of the simple parallel-plate capacitor. Figure 10.2a shows a parallel-plate capacitor with the top plate at a negative voltage with respect to the bottom plate. An insulator material separates the two plates. With this bias, a negative charge exists on the top plate, a positive charge exists on the bottom plate, and an electric field is induced between the two plates as shown. The capacitance per unit area for this geometry is C _ d (10.1) where is the permittivity of the insulator and d is the distance between the two plates. The magnitude of the charge per unit area on either plate is Q CV tox ox (10.2) Metal Insulator (oxide) Semiconductor substrate Figure 10.1 | The basic MOS capacitor structure. nea29583_ch10_371-442.indd 372 12/11/10 12:40 PM 10.1 The Two-Terminal MOS Structure 373 ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⑀ d ⴙ ⴚ ⴙ ⴙ ⴚ ⴚ ⴚ E-field ⴙ ⴙ ⴚ E-field p type V h ⴙ V ⴙ ⴙ (a) (b) ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ E-field ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴚ V p type ⴙ Accumulation layer of holes (c) Figure 10.2 | (a) A parallel-plate capacitor showing the electric field and conductor charges. (b) A corresponding MOS capacitor with a negative gate bias showing the electric field and charge flow. (c) The MOS capacitor with an accumulation layer of holes. where the prime indicates charge or capacitance per unit area. The magnitude of the electric field is V E_ d (10.3) Figure 10.2b shows a MOS capacitor with a p-type semiconductor substrate. The top metal gate is at a negative voltage with respect to the semiconductor substrate. From the example of the parallel-plate capacitor, we can see that a negative charge will exist on the top metal plate and an electric field will be induced with the direction shown in the figure. If the electric field were to penetrate into the semiconductor, the majority carrier holes would experience a force toward the oxide–semiconductor interface. Figure 10.2c shows the equilibrium distribution of charge in the MOS capacitor with this particular applied voltage. An accumulation layer of holes at the oxide–semiconductor junction corresponds to the positive charge on the bottom “plate” of the MOS capacitor. Figure 10.3a shows the same MOS capacitor in which the polarity of the applied voltage is reversed. A positive charge now exists on the top metal plate and the induced electric field is in the opposite direction as shown. If the electric field penetrates the semiconductor in this case, majority carrier holes will experience a force away from the oxide–semiconductor interface. As the holes are pushed away from nea29583_ch10_371-442.indd 373 12/11/10 12:40 PM 374 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor the interface, a negative space charge region is created because of the fixed ionized acceptor atoms. The negative charge in the induced depletion region corresponds to the negative charge on the bottom “plate” of the MOS capacitor. Figure 10.3b shows the equilibrium distribution of charge in the MOS capacitor with this applied voltage. The energy-band diagrams of the MOS capacitor with a p-type substrate for various gate biases are shown in Figure 10.4. Figure 10.4a shows the ideal case when zero bias is applied across the MOS device. The energy bands in the semiconductor are flat indicating no net charge exists in the semiconductor. This condition is known as flat band and is discussed in more detail later in the chapter. ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ E-field p type ⴙ xd V h V ⴚ ⴚ p type Induced space charge region (a) (b) Figure 10.3 | The MOS capacitor with a moderate positive gate bias, showing (a) the electric field and charge flow and (b) the induced space charge region. Ec Gate Zero voltage applied EFi EF Ev Oxide p type (a) Ec EFi EF Ev Gate Negative voltage applied Oxide ⴙⴙ ⴙ p type Accumulation layer of holes (b) Ec Gate Positive voltage applied EFi EF Ev Oxide p type xd Induced space charge region (c) Figure 10.4 | The energy-band diagram of a MOS capacitor with a p-type substrate for (a) a zero applied gate bias showing the ideal case, (b) a negative gate bias, and (c) a moderate positive gate bias. nea29583_ch10_371-442.indd 374 12/11/10 12:40 PM 10.1 The Two-Terminal MOS Structure 375 Figure 10.4b shows the energy-band diagram for the case when a negative bias is applied to the gate. (Remember that positive electron energy is plotted “upward” and positive voltage is plotted “downward.”) The valence-band edge is closer to the Fermi level at the oxide–semiconductor interface than in the bulk material, which implies that there is an accumulation of holes. The semiconductor surface appears to be more p-type than the bulk material. The Fermi level is a constant in the semiconductor since the MOS system is in thermal equilibrium and there is no current through the oxide. Figure 10.4c shows the energy-band diagram of the MOS system when a positive voltage is applied to the gate. The conduction- and valence-band edges bend as shown in the figure, indicating a space charge region similar to that in a pn junction. The conduction band and intrinsic Fermi levels move closer to the Fermi level. The induced space charge width is xd. Now consider the case when a still larger positive voltage is applied to the top metal gate of the MOS capacitor. We expect the induced electric field to increase in magnitude and the corresponding positive and negative charges on the MOS capacitor to increase. A larger negative charge in the MOS capacitor implies a larger induced space charge region and more band bending. Figure 10.5 shows such a condition. The intrinsic Fermi level at the surface is now below the Fermi level. The conduction band at the surface is now close to the Fermi level, whereas the valence band is close to the Fermi level in the bulk semiconductor. This result implies that the surface in the semiconductor adjacent to the oxide–semiconductor interface is n type. By applying a sufficiently large positive gate voltage, we have inverted the surface of the semiconductor from a p-type to an n-type semiconductor. We have created an inversion layer of electrons at the oxide–semiconductor interface. In the MOS capacitor structure that we have just considered, we assumed a p-type semiconductor substrate. The same type of energy-band diagrams can be constructed for a MOS capacitor with an n-type semiconductor substrate. Figure 10.6a shows the MOS capacitor structure with a positive voltage applied to the top gate terminal. A positive charge exists on the top gate and an electric field is induced with the direction shown in the figure. An accumulation layer of electrons will be induced in the n-type substrate. The case when a negative voltage is applied to the top gate Inversion layer of electrons Ec Gate “Large” positive voltage EFi EF Ev Oxide p type xd T Figure 10.5 | The energy-band diagram of the MOS capacitor with a p-type substrate for a “large” positive gate bias. nea29583_ch10_371-442.indd 375 12/11/10 12:40 PM 376 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor ⴙ ⴙ ⴙ ⴙ ⴙ ⴙ E-field ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ ⴚ E-field ⴙ ⴚ V n type V ⴚ n type ⴙ Induced positive space charge region Accumulation layer of electrons (a) (b) Figure 10.6 | The MOS capacitor with an n-type substrate for (a) a positive gate bias and (b) a moderate negative gate bias. is shown in Figure 10.6b. A positive space charge region is induced in the n-type semiconductor in this situation. The energy-band diagrams for this MOS capacitor with the n-type substrate are shown in Figure 10.7. Figure 10.7a shows the case when a positive voltage is applied to the gate and an accumulation layer of electrons is formed. Figure 10.7b shows the energy bands when a negative voltage is applied to the gate. The conduction and valence bands now bend upward indicating that a space charge region has been induced in the n-type substrate. Figure 10.7c shows the energy bands when a larger negative voltage is applied to the gate. The conduction and valence bands are bent even more and the intrinsic Fermi level has moved above the Fermi level. The valence band at the surface is now close to the Fermi level, whereas the conduction band is close to the Fermi level in the bulk semiconductor. This result implies that the semiconductor surface adjacent to the oxide–semiconductor interface is p type. By applying a sufficiently large negative voltage to the gate of the MOS capacitor, the semiconductor surface has been inverted from n type to p type. An inversion layer of holes has been induced at the oxide–semiconductor interface. 10.1.2 Depletion Layer Thickness We may calculate the width of the induced space charge region adjacent to the oxide–semiconductor interface. Figure 10.8 shows the space charge region in a ptype semiconductor substrate. The potential fp is the difference (in V) between EFi and EF and is given by Na fp Vt ln _ ni (10.4) where Na is the acceptor doping concentration and ni is the intrinsic carrier concentration. The potential s is called the surface potential; it is the difference (in V) between EFi measured in the bulk semiconductor and EFi measured at the surface. The surface nea29583_ch10_371-442.indd 376 12/11/10 12:40 PM 10.1 The Two-Terminal MOS Structure 377 Accumulation of electrons n type Ec EF EFi Gate Positive voltage applied Oxide Ev (a) Induced positive space charge region n type Ec EF EFi Gate Negative voltage applied Oxide Ev xd (b) n type Ec EF EFi Gate “Large” negative voltage Oxide ⴙⴙ ⴙ Ev Inversion layer of holes (c) Figure 10.7 | The energy-band diagram of the MOS capacitor with an n-type substrate for (a) a positive gate bias, (b) a moderate negative bias, and (c) a “large” negative gate bias. potential is the potential difference across the space charge layer. The space charge width can now be written in a form similar to that of a one-sided pn junction. We can write that 2ss xd _ eNa 12 (10.5) where s is the permittivity of the semiconductor. Equation (10.5) assumes that the abrupt depletion approximation is valid. nea29583_ch10_371-442.indd 377 12/11/10 12:40 PM 378 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Ec es efp EFi EF Ev xd Figure 10.8 | The energy-band diagram in the p-type semiconductor, indicating surface potential. Figure 10.9 shows the energy bands for the case in which s 2fp. The Fermi level at the surface is as far above the intrinsic level as the Fermi level is below the intrinsic level in the bulk semiconductor. The electron concentration at the surface is the same as the hole concentration in the bulk material. This condition is known as the threshold inversion point. The applied gate voltage creating this condition is known as the threshold voltage. If the gate voltage increases above this threshold value, the conduction band will bend slightly closer to the Fermi level, but the change in the conduction band at the surface is now only a slight function of gate voltage. The electron concentration at the surface, however, is an exponential function of the surface potential. The surface potential may increase by a few (kTe) volts, which will change the electron concentration by orders of magnitude, but the space charge width changes only slightly. In this case, then, the space charge region has essentially reached a maximum width. Ec efp es 2efp EFi EF Ev xd xdT Figure 10.9 | The energy-band diagram in the p-type semiconductor at the threshold inversion point. nea29583_ch10_371-442.indd 378 12/11/10 12:40 PM 10.1 The Two-Terminal MOS Structure 379 The maximum space charge width, xdT, at this inversion transition point can be calculated from Equation (10.5) by setting s 2fp. Then 4sfp xdT _ eNa 12 (10.6) Objective: Calculate the maximum space charge width for a given semiconductor doping EXAMPLE 10.1 concentration. Consider silicon at T 300 K doped to Na 1016 cm3. The intrinsic carrier concentration is ni 1.5 1010 cm3. ■ Solution From Equation (10.4), we have Na 1016 __ fp Vt ln _ ni (0.0259) ln 1.5 1010 0.3473 V Then the maximum space charge width is 4s fp xdT __ eNa 10 )(0.3473) 4(11.7)(8.85 (1.6 10 )(10 ) 12 14 _____ 19 12 16 or xdT 0.30 104 cm 0.30 m ■ Comment The maximum induced space charge width is on the same order of magnitude as pn junction space charge widths. ■ EXERCISE PROBLEM Ex 10.1 Consider an oxide-to-p-type silicon junction at T 300 K. The impurity doping concentration in the silicon is Na 2 1015 cm3. Calculate the maximum space charge width. Does the space charge width increase or decrease as the p-type doping concentration decreases? (Ans. xdT 0.629 m, increase) We have been considering a p-type semiconductor substrate. The same maximum induced space charge region width occurs in an n-type substrate. Figure 10.10 is the energy-band diagram at the threshold voltage with an n-type substrate. We can write Nd fn Vt ln _ ni (10.7) and 4s fn xdT __ eNd 12 (10.8) Note that we are always assuming the parameters fp and fn to be positive quantities. Figure 10.11 is a plot of xdT at T 300 K as a function of doping concentration in silicon. The semiconductor doping can be either n type or p type. nea29583_ch10_371-442.indd 379 12/11/10 12:40 PM 380 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor es 2efn Ec EF efn EFi Ev xd T Figure 10.10 | The energy-band diagram in the n-type semiconductor at the threshold inversion point. Maximum depletion width, xdT (m) 10 T 300 K 1.0 Si 0.1 0.01 1014 1015 1016 1017 N, semiconductor doping 1018 (cm3) Figure 10.11 | Maximum induced space charge region width versus semiconductor doping. 10.1.3 Surface Charge Density From the results of Chapter 4, the electron concentration in the conduction band can be written in the form EF EFi n ni exp __ kT (10.9) For a p-type semiconductor substrate, the electron inversion charge density can then be written as (see Figure 10.9) e(fp s) fp s ns ni exp ___ ni exp __ Vt kT nea29583_ch10_371-442.indd 380 (10.10a) 12/11/10 12:40 PM 10.1 The Two-Terminal MOS Structure 381 or fp ns ni exp _ · exp _s Vt Vt (10.10b) where s, is the surface potential greater than 2fp. We may note that fp nst ni exp _ Vt (10.11) where nst is the surface charge density at the threshold inversion point. The electron inversion charge density can then be written as ns nst exp _s Vt (10.12) Figure 10.12 shows the electron inversion charge density as a function of surface potential for the case when the threshold inversion charge density is nst 1016 cm3. We may note that the inversion charge density increases by a factor of 10 with a 60-mV increase in surface potential. As discussed previously, the electron inversion charge density increases rapidly with small increases in surface potential, which means that the space charge width essentially reaches a maximum value. ns (cm3) 1018 1017 1016 2fp (2fp 0.06) (2fp 0.12) s (volts) Figure 10.12 | Electron inversion charge density as a function of surface potential. nea29583_ch10_371-442.indd 381 12/11/10 12:40 PM 382 CHAPTER 10 10.1.4 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Work Function Differences We have been concerned, so far, with the energy-band diagrams of the semiconductor material. Figure 10.13a shows the energy levels in the metal, silicon dioxide (SiO2), and silicon relative to the vacuum level. The metal work function is m and the electron affinity is . The parameter i is the oxide electron affinity and, for SiO2, i 0.9 V. Figure 10.13b shows the energy-band diagram of the entire MOS structure with zero gate voltage applied. The Fermi level is a constant through the entire system at thermal equilibrium. We may define m as a modified metal work function—the potential required to inject an electron from the metal into the conduction band of the oxide. Similarly, is defined as a modified electron affinity. The voltage Vox0 is the potential drop across the oxide for zero applied gate voltage and is not necessarily zero because of the difference between m and . The potential s0 is the surface potential for this case. If we sum the energies from the Fermi level on the metal side to the Fermi level on the semiconductor side, we have Eg em eVox0 e _ es0 eJfp (10.13) 2 Equation (10.13) can be rewritten as Eg Vox0 s0 m _ fp 2e (10.14) Vacuum level Metal Vacuum level ei p-type semiconductor Oxide Oxide conduction band eVox0 Ec e ei em e e Ec EFm EFi (a) p-type silicon M Eg efp es0 EFs Ev Ev Silicon dioxide em Eg 9 eV Metal Ec em 2 EFi EF Ev O S (b) Figure 10.13 | (a) Energy levels in a MOS system prior to contact and (b) energy-band diagram through the MOS structure in thermal equilibrium after contact. nea29583_ch10_371-442.indd 382 12/11/10 12:40 PM 10.1 The Two-Terminal MOS Structure 383 We can define a potential ms as ms E2e _g m (10.15) fp which is known as the metal–semiconductor work function difference. Objective: Determine the metal–semiconductor work function difference, ms, for a given EXAMPLE 10.2 MOS system and semiconductor doping. For an aluminum–silicon dioxide junction, m 3.20 V and, for a silicon–silicon dioxide junction, 3.25 V. We may assume that Eg 1.12 V. Let the p-type doping be Na 1015 cm3. ■ Solution For silicon at T 300 K, we may calculate fp as Na 1015 __ fp Vt ln _ nj (0.0259)ln 1.5 1010 0.288 V Then the metal–semiconductor work function difference is Eg ms m _ fp 3.20 (3.25 0.560 0.288) 2e or ms 0.898 V ■ Comment The value of ms will become more negative as the doping of the p-type substrate increases. ■ EXERCISE PROBLEM Ex 10.2 Repeat Example 10.2 for a semiconductor doping of Na 1016 cm3. (Ans. ms 0.957 V) Degenerately doped polysilicon deposited on the oxide is also often used as the metal gate. Figure 10.14a shows the energy-band diagram of a MOS capacitor with an n polysilicon gate and a p-type substrate. Figure 10.14b shows the energy-band e eVox Eg e 2 efp EF Ec n poly Ec EFi EF Ev e p poly e Eg Eg 2 efp EF Ev Ev M O S (a) M O Ec EFi EF Ev S (b) Figure 10.14 | Energy-band diagram through the MOS structure with a p-type substrate at zero gate bias for (a) an n polysilicon gate and (b) a p polysilicon gate. nea29583_ch10_371-442.indd 383 12/11/10 12:40 PM 384 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor diagram for the case of a p polysilicon gate and the p-type silicon substrate. In the degenerately doped polysilicon, we will initially assume that EF Ec for the n case and EF Ev for the p case. For the n polysilicon gate, the metal–semiconductor work function difference can be written as Eg ms _ fp 2e _2eE g (10.16) fp and for the p polysilicon gate, we have ms Ee E2e E2e _g _g _g fp fp (10.17) However, for degenerately doped n polysilicon and p polysilicon, the Fermi level can be above Ec and below Ev, respectively, by 0.1 to 0.2 V. The experimental ms values will then be slightly different from the values calculated by using Equations (10.16) and (10.17). We have been considering a p-type semiconductor substrate. We may also have an n-type semiconductor substrate in a MOS capacitor. Figure 10.15 shows the energy-band diagram of the MOS capacitor with a metal gate and the n-type semiconductor substrate, for the case when a negative voltage is applied to the gate. The metal–semiconductor work function difference for this case is defined as Eg ms m _ fn 2e (10.18) eVox e⬘m e es efn Ec EF EFi Ev M O S Figure 10.15 | Energy-band diagram through the MOS structure with an n-type substrate for a negative applied gate bias. nea29583_ch10_371-442.indd 384 12/11/10 12:40 PM 10.1 1.0 The Two-Terminal MOS Structure 385 p poly (n Si) 0.8 Au (n Si) 0.6 p poly (p Si) 0.4 ms (V) 0.2 Au (p Si) 0 0.2 0.4 n poly (n Si) Al (n Si) 0.6 Al (p Si) n poly (p Si) 0.8 1.0 1014 1015 1016 1017 NB (cm3) 1018 Figure 10.16 | Metal–semiconductor work function difference versus doping for aluminum, gold, and n and p polysilicon gates. (From Sze [17] and Werner [20].) where fn is assumed to be a positive value. We will have similar expressions for n and p polysilicon gates. Figure 10.16 shows the work function differences as a function of semiconductor doping for the various types of gates. We may note that the magnitudes of ms for the polysilicon gates are somewhat larger than Equations (10.16) and (10.17) predict. This difference again is because the Fermi level is not equal to the conduction-band energy for the n gate and is not equal to the valence-band energy for the p gate. The metal–semiconductor work function difference becomes important in the flatband and threshold voltage parameters discussed next. 10.1.5 Flat-Band Voltage The flat-band voltage is defined as the applied gate voltage such that there is no band bending in the semiconductor and, as a result, zero net space charge in this region. Figure 10.17 shows this flat-band condition. Because of the work function difference and possible trapped charge in the oxide, the voltage across the oxide for this case is not necessarily zero. We have implicitly been assuming that there is zero net charge density in the oxide material. This assumption may not be valid—a net fixed charge density, nea29583_ch10_371-442.indd 385 12/11/10 12:40 PM 386 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Ec EF EFi EF Ev VFB M O S Figure 10.17 | Energy-band diagram of a MOS capacitor at flat band. usually positive, may exist in the insulator. The positive charge has been identified with broken or dangling covalent bonds near the oxide–semiconductor interface. During the thermal formation of SiO2, oxygen diffuses through the oxide and reacts near the Si–SiO2 interface to form the SiO2. Silicon atoms may also break away from the silicon material just prior to reacting to form SiO2. When the oxidation process is terminated, excess silicon may exist in the oxide near the interface, resulting in the dangling bonds. The magnitude of this oxide charge seems, in general, to be a strong function of the oxidizing conditions such as oxidizing ambient and temperature. The charge density can be altered to some degree by annealing the oxide in an argon or nitrogen atmosphere. However, the charge is rarely zero. The net fixed charge in the oxide appears to be located fairly close to the oxide– semiconductor interface. We will assume in the analysis of the MOS structure that an equivalent trapped charge per unit area, Q ss , is located in the oxide directly adjacent to the oxide–semiconductor interface. For the moment, we will ignore any other oxide-type charges that may exist in the device. The parameter Q ss is usually given in terms of number of electronic charges per unit area. Equation (10.14), for zero applied gate voltage, can be written as Vox0 s0 ms (10.19) If a gate voltage is applied, the potential drop across the oxide and the surface potential will change. We can then write VG Vox s (Vox Vox0) (s s0) (10.20) Using Equation (10.19), we have VG Vox s ms (10.21) Figure 10.18 shows the charge distribution in the MOS structure for the flatband condition. There is zero net charge in the semiconductor, and we can assume that an equivalent fixed surface charge density exists in the oxide. The charge density on the metal is Qm, and from charge neutrality we have Qm Qss 0 We can relate Qm to the voltage across the oxide by Qm Vox _ Cox nea29583_ch10_371-442.indd 386 (10.22) (10.23) 12/11/10 12:40 PM 10.1 Metal Qm Oxide The Two-Terminal MOS Structure 387 p-type semiconductor Qss Figure 10.18 | Charge distribution in a MOS capacitor at flat band. where Cox is the oxide capacitance per unit area.1 Substituting Equation (10.22) into Equation (10.23), we have Qss Vox _ (10.24) Cox In the flat-band condition, the surface potential is zero, or s 0. Then from Equation (10.21), we have Qss _ VG VFB ms Cox (10.25) Equation (10.25) is the flat-band voltage for this MOS device. Objective: Calculate the flat-band voltage for a MOS capacitor with a p-type semiconductor EXAMPLE 10.3 substrate. Consider a MOS capacitor with a p-type silicon substrate doped to Na 1016 cm3, a silicon dioxide insulator with a thickness of tox 20 nm 200 Å, and an n polysilicon gate. Assume that Q ss 5 1010 electronic charges per cm2. ■ Solution The work function difference, from Figure 10.16, is ms 1.1V. The oxide capacitance is found to be (3.9)(8.85 1014) ox ____ Cox _ 1.726 107 F/cm2 tox 200 108 The equivalent oxide charge density is Q ss (5 1010)(1.6 1019) 8 109 C/cm2 The flat-band voltage is then determined to be Q ss 8 109 1.15 V VFB ms _ 1.1 ___ Cox 1.726 107 1 Although we will, in general, use the primed notation for capacitance per unit area or charge per unit area, we will omit, for convenience, the prime on the oxide capacitance per unit area parameter. nea29583_ch10_371-442.indd 387 12/11/10 12:40 PM 388 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor ■ Comment The applied gate voltage required to achieve the flat-band condition for this p-type substrate is negative. If the amount of fixed oxide charge increases, the flat-band voltage becomes even more negative. ■ EXERCISE PROBLEM Repeat Example 10.3 for a doping concentration of Na 2 1015 cm3, an oxide thickness of tox 4 nm 40 Å, and Q ss 2 1010 electronic charges per cm2. What is the value of the metal–semiconductor work function difference? 1.03 V, VFB 1.034 V) 10.1.6 (Ans. ms Ex 10.3 Threshold Voltage The threshold voltage is defined as the applied gate voltage required to achieve the threshold inversion point. The threshold inversion point, in turn, is defined as the condition when the surface potential is s 2fp for the p-type semiconductor and s 2fn for the n-type semiconductor. These conditions are shown in Figures 10.9 and 10.10. The threshold voltage will be derived in terms of the electrical and geometrical properties of the MOS capacitor. Figure 10.19 shows the charge distribution through the MOS device at the threshold inversion point for a p-type semiconductor substrate. The space charge width has reached its maximum value. We will assume that there is an equivalent . The oxide charge Qss and the positive charge on the metal gate at threshold is Q mT prime on the charge terms indicates charge per unit area. Even though we are assuming that the surface has been inverted, we will neglect the inversion layer charge at this threshold inversion point. From conservation of charge, we can write Q mT Qss Q SD(max) (10.26) (max) eNa xdT Q SD (10.27) where Metal QmT Oxide p-type semiconductor Qss xdT QSD(max) eNa xdT Figure 10.19 | Charge distribution in a MOS capacitor with a p-type substrate at the threshold inversion point. nea29583_ch10_371-442.indd 388 12/11/10 12:40 PM 10.1 The Two-Terminal MOS Structure 389 Vox Ec EFi EF Ev s VG M O S Figure 10.20 | Energy-band diagram through the MOS structure with a positive applied gate bias. and is the magnitude of the maximum space charge density per unit area of the depletion region. The energy-band diagram of the MOS system with an applied positive gate voltage is shown in Figure 10.20. As we mentioned, an applied gate voltage will change the voltage across the oxide and will change the surface potential. We had from Equation (10.20) that VG Vox s Vox s ms At threshold, we can define VG VTN, where VTN is the threshold voltage that creates the electron inversion layer charge. The surface potential is s 2fp at threshold, so Equation (10.20) can be written as VTN VoxT 2fp ms (10.28) where VoxT is the voltage across the oxide at this threshold inversion point. The voltage VoxT can be related to the charge on the metal and to the oxide capacitance by Q mT VoxT _ (10.29) Cox where again Cox is the oxide capacitance per unit area. Using Equation (10.26), we can write Q mT _ (max) Qss VoxT _ 1 Q SD (10.30) Cox Cox Finally, the threshold voltage can be written as (max) Q SD Qss ms 2fp VTN __ _ Cox Cox or nea29583_ch10_371-442.indd 389 tox VTN Q SD(max) Qss _ ox ms 2fp (10.31a) (10.31b) 12/11/10 12:40 PM 390 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Using the definition of flat-band voltage from Equation (10.25), we can also express the threshold voltage as ( max) Q SD VTN __ VFB 2fp (10.31c) Cox For a given semiconductor material, oxide material, and gate metal, the threshold voltage is a function of semiconductor doping, oxide charge Qss , and oxide thickness. EXAMPLE 10.4 Objective: Calculate the threshold voltage of a MOS system using an aluminum gate. Consider a p-type silicon substrate at T 300 K doped to Na 1015 cm3. Let Q ss 1010 cm2, tox 12 nm 120 Å, and assume the oxide is silicon dioxide. ■ Solution From Figure 10.16, we find ms 0.88 V. The other parameters are Na 1015 __ fp Vt ln _ ni (0.0259) ln 1.5 1010 0.2877 V and 4s fp xdT __ eNa 12 4(11.7)(8.85 1014)(0.2877) _____ (1.6 1019)(1015) 12 8.63 105 cm Then Q SD (max) eNa xdT (1.6 1019)(1015)(8.63 105) 1.381 108 C/cm2 The threshold voltage is now found to be tox VTN Q SD (max) Q ss _ ox ms 2fp 120 108 (1.381 108) (1010)(1.6 1019) ⴢ ____ (3.9)(8.85 1014) 0.88 2 0.2877 or VTN 0.262 V ■ Comment In this example, the semiconductor is fairly lightly doped, which, in conjunction with the positive charge in the oxide and the work function difference, is sufficient to induce an electron inversion layer charge even with zero applied gate voltage. This condition makes the threshold voltage negative. ■ EXERCISE PROBLEM Determine the metal–semiconductor work function difference and the threshold voltage for a silicon MOS device at T 300 K for the following parameters: p polysilicon gate, Na 2 1016 cm3, tox 8 nm 80 Å, and Qss 2 1010 cm2. (Ans. ms Ex 10.4 0.28 V, VTN 1.16 V) A negative threshold voltage for a p-type substrate implies a depletion mode device. A negative voltage must be applied to the gate in order to make the inversion nea29583_ch10_371-442.indd 390 12/11/10 12:40 PM 10.1 The Two-Terminal MOS Structure 391 3 2 VTN (V) 1 0 1 2 Qss 0 Qss 1011 cm2 Qss 5 1011 cm2 Qss 1012 cm2 3 1013 1014 1015 Na 1016 1017 1018 (cm3 ) Figure 10.21 | Threshold voltage of an n-channel MOSFET versus the p-type substrate doping concentration for various values of oxide trapped charge (tox 500 Å, aluminum gate). layer charge equal to zero, whereas a positive gate voltage will induce a larger inversion layer charge. Figure 10.21 is a plot of the threshold voltage VTN as a function of the acceptor doping concentration for various positive oxide charge values. We may note that the p-type semiconductor must be somewhat heavily doped in order to obtain an enhancement mode device. The previous derivation of the threshold voltage assumed a p-type semiconductor substrate. The same type of derivation can be done with an n-type semiconductor substrate, where a negative gate voltage can induce an inversion layer of holes at the oxide–semiconductor interface. Figure 10.15 shows the energy-band diagram of the MOS structure with an ntype substrate and with an applied negative gate voltage. The threshold voltage for this case can be derived and is given by tox VTP Q SD (max) Q ss _ ox ms 2fn where Eg ms m _ fn 2e Q SD (max) eNd xdT 4sfn 12 xdT _ eNd nea29583_ch10_371-442.indd 391 (10.32) (10.33a) (10.33b) (10.33c) 12/11/10 12:40 PM 392 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Nd (cm3) 1013 0 1014 1015 1016 1017 1018 Qss 0 VTP (V) 1 Qss 1011 cm2 2 Qss 5 1011 cm2 3 Qss 1012 cm2 4 Figure 10.22 | Threshold voltage of a p-channel MOSFET versus the n-type substrate doping concentration for various values of oxide trapped charge (tox 500 Å, aluminum gate). and Nd fn Vt ln _ (10.33d) ni We may note that xdT and fn are defined as positive quantities. We may also note that the notation of VTP is the threshold voltage that will induce an inversion layer of holes. We will later drop the N and P subscript notation on the threshold voltage, but, for the moment, the notation may be useful for clarity. Figure 10.22 is a plot of VTP versus doping concentration for several values of Qss. We may note that, for all values of positive oxide charge, this MOS capacitor is always an enhancement mode device. As the Qss charge increases, the threshold voltage becomes more negative, which means that it takes a larger applied gate voltage to create the inversion layer of holes at the oxide–semiconductor interface. DESIGN EXAMPLE 10.5 Objective: Determine the gate material and design the semiconductor doping concentration to yield a specified threshold voltage. Consider a MOS device with silicon dioxide and an n-type silicon substrate. The oxide thickness is tox 12 nm 120 Å and the oxide charge is Q ss 2 1010 cm2 . The threshold voltage is to be approximately VTP 0.3 V. ■ Solution The solution to this design problem is not straight forward, since the doping concentration parameter appears in the terms fn, xdT, Q sD (max), and ms. The threshold voltage, then, is a nonlinear function of Nd. We resort to trial and error to obtain a solution. Figure 10.22 shows the threshold voltage for an aluminum gate system. Since the required threshold voltage in this problem is less negative than the values shown in Figure 10.22, nea29583_ch10_371-442.indd 392 12/11/10 12:40 PM 10.1 The Two-Terminal MOS Structure 393 we require a metal–semiconductor work function difference value that is more positive than for the aluminum gate. We therefore choose a p polysilicon gate. Consider a doping concentration of Nd 1017 cm3. From Figure 10.16, the metal– semiconductor work function difference is ms 1.1 V. The remaining parameters are found to be Nd 1017 __ fn Vt ln _ ni (0.0259) ln 1.5 1010 0.407 V 4s fn xdT __ eNd 12 4(11.7)(8.85 1014)(0.407) _____ (1.6 1019)(1017) 12 1.026 105 cm QSD (max) eNd xdT (1.6 1019)(1017)(1.026 105) 1.642 107 C/cm2 The threshold voltage is determined to be tox VTP [ QSD (max) Qss ] ⴢ _ ox ms 2fn or [(1.642 107) (2 1010)(1.6 1019)] ⴢ (120 108) VTP __________ (3.9)(8.85 1014) 1.1 2(0.407) which yields VTP 0.296 V 0.3 V ■ Comment The negative threshold voltage, with the n-type substrate, implies that this MOS capacitor is an enhancement mode device. The inversion layer charge is zero with zero applied gate voltage, and a negative gate voltage must be applied to induce the hole inversion charge. ■ EXERCISE PROBLEM Ex 10.5 Consider a MOS capacitor with silicon dioxide and an n-type silicon substrate at T 300 K with the following parameters: p polysilicon gate, Nd 2 1016 cm3, tox 20 nm 200 Å, and Qss 5 1010 cm2. Determine the threshold voltage. Is the capacitor an enhancement mode or depletion mode device? (Ans. VTP 0.12 V, enhancement mode) TEST YOUR UNDERSTANDING TYU 10.1 (a) Consider an oxide-to-n-type silicon junction at T 300 K. The impurity doping concentration in the silicon is Nd 8 1015 cm3. Calculate the maximum space charge width in the silicon. (b) Repeat part (a) for a doping concentration of Nd 4 1016 cm3. [Ans. (a) 0.332 m; (b) 0.158 m] nea29583_ch10_371-442.indd 393 12/11/10 12:40 PM 394 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor TYU 10.2 Consider an n polysilicon gate in a MOS structure with a p-type silicon substrate. The doping concentration of the silicon is Na 3 1016 cm3. Using Equation (10.16), find the value of ms. TYU 10.3 Repeat TYU 10.2 for a p polysilicon gate using Equation (10.17). TYU 10.4 Consider the MOS capacitor described in Exercise TYU 10.3. The oxide thickness is tox 16 nm 160 Å and the oxide charge density is Qss 8 1010 cm2. Determine the flat-band voltage. TYU 10.5 Consider an n polysilicon gate on silicon dioxide with a p-type silicon substrate doped to Na 3 1016 cm3. Assume Qss 5 1010 cm2. Determine the required oxide thickness such that the threshold voltage is VTN 0.65 V. (Ans. ms 0.936 V) (Ans. ms 0.184 V) (Ans. 0.125 V) (Ans. tox 45.2 nm 452 Å) 10.2 | CAPACITANCE–VOLTAGE CHARACTERISTICS As mentioned previously, the MOS capacitor structure is the heart of the MOSFET. A great deal of information about the MOS device and the oxide–semiconductor interface can be obtained from the capacitance versus voltage or C–V characteristics of the device. The capacitance of a device is defined as dQ C_ (10.34) dV where dQ is the magnitude of the differential change in charge on one plate as a function of the differential change in voltage dV across the capacitor. The capacitance is a small-signal or ac parameter and is measured by superimposing a small ac voltage on an applied dc gate voltage. The capacitance, then, is measured as a function of the applied dc gate voltage. 10.2.1 Ideal C–V Characteristics First we will consider the ideal C–V characteristics of the MOS capacitor and then discuss some of the deviations that occur from these idealized results. We will initially assume that there is zero charge trapped in the oxide and also that there is no charge trapped at the oxide–semiconductor interface. There are three operating conditions of interest in the MOS capacitor: accumulation, depletion, and inversion. Figure 10.23a shows the energy-band diagram of a MOS capacitor with a p-type substrate for the case when a negative voltage is applied to the gate, inducing an accumulation layer of holes in the semiconductor at the oxide–semiconductor interface. A small differential change in voltage across the MOS structure will cause a differential change in charge on the metal gate and also in the hole accumulation charge, as shown in Figure 10.23b. The differential changes in charge density occur at the edges of the oxide, as in a parallel-plate capacitor. The nea29583_ch10_371-442.indd 394 12/11/10 12:40 PM 10.2 Metal Oxide Capacitance–Voltage Characteristics 395 p-type semiconductor dQ Q Ec EFi EF Ev Q dQ (a) (b) Figure 10.23 | (a) Energy-band diagram through a MOS capacitor for the accumulation mode. (b) Differential charge distribution at accumulation for a differential change in gate voltage. Metal Oxide p-type semiconductor dQ Ec Q xd EFi EF Ev dx Q xd (a) dQ (b) Figure 10.24 | (a) Energy-band diagram through a MOS capacitor for the depletion mode. (b) Differential charge distribution at depletion for a differential change in gate voltage. capacitance C per unit area of the MOS capacitor for this accumulation mode is just the oxide capacitance, or ox C(acc) Cox _ t ox (10.35) Figure 10.24a shows the energy-band diagram of the MOS device when a small positive voltage is applied to the gate, inducing a space charge region in the semiconductor; Figure 10.24b shows the charge distribution through the device for this condition. The oxide capacitance and the capacitance of the depletion region are in series. A small differential change in voltage across the capacitor will cause a differential change in the space charge width. The corresponding differential changes nea29583_ch10_371-442.indd 395 12/11/10 12:40 PM 396 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor in charge densities are shown in the figure. The total capacitance of the series combination is 1 1 _ 1 __ _ (10.36a) CoxCSD C(depl) __ Cox CSD (10.36b) C(depl) Cox CSD or sxd, Equation (10.36b) can be written as Since Cox oxtox and CSD Cox ox C(depl) __ ___ ox C _ ox 1 _ tox s xd CSD (10.37) As the space charge width increases, the total capacitance C(depl) decreases. We had defined the threshold inversion point to be the condition when the maximum depletion width is reached, but there is essentially zero inversion charge den , which is given by sity. This condition will yield a minimum capacitance C min ox C min ___ (10.38) ox tox _ x dT s Figure 10.25a shows the energy-band diagram of this MOS device for the inversion condition. In the ideal case, a small incremental change in the voltage across the MOS capacitor will cause a differential change in the inversion layer charge density. The space charge width does not change. If the inversion charge can respond to the change in capacitor voltage as indicated in Figure 10.25b, then the capacitance is again just the oxide capacitance, or ox C(inv) Cox _ (10.39) tox Metal Oxide p-type semiconductor dQ Ec Q xdT EFi EF Ev Q EF xdT M O dQ S (a) (b) Figure 10.25 | (a) Energy-band diagram through a MOS capacitor for the inversion mode. (b) Differential charge distribution at inversion for a low-frequency differential change in gate voltage. nea29583_ch10_371-442.indd 396 12/11/10 12:40 PM 10.2 Capacitance–Voltage Characteristics C Cox Accumulation Cox CSD CFB 397 Strong inversion Moderate inversion Cmin Depletion VFB 0 VT VG Figure 10.26 | Ideal low-frequency capacitance versus gate voltage of a MOS capacitor with a p-type substrate. Individual capacitance components are also shown. Figure 10.26 shows the ideal capacitance versus gate voltage, or C–V, characteristics of the MOS capacitor with a p-type substrate. The three dashed segments cor , and C min . The solid curve is the ideal net respond to the three components Cox, CSD capacitance of the MOS capacitor. Moderate inversion, which is indicated in the figure, is the transition region between the point when only the space charge density changes with gate voltage and when only the inversion charge density changes with gate voltage. The point on the curve that corresponds to the flat-band condition is of interest. The flat-band condition occurs between the accumulation and depletion conditions. The capacitance at flat band is given by ox__________ _____ CFB (10.40) s ox kT _ _ tox _ e s eNa We may note that the flat-band capacitance is a function of oxide thickness as well as semiconductor doping. The general location of this point on the C–V plot is shown in Figure 10.26. Objective: Calculate Cox, C min, and C FB for a MOS capacitor. EXAMPLE 10.6 Consider a p-type silicon substrate at T 300 K doped to Na 1016 cm3. The oxide is silicon dioxide with a thickness of tox 18 nm 180 Å, and the gate is aluminum. ■ Solution The oxide capacitance is ox ____ (3.9)(8.85 1014) 1.9175 107 F/cm2 Cox _ tox 180 108 To find the minimum capacitance, we need to calculate Na 1016 __ fp Vt ln _ ni (0.0259) ln 1.5 1010 0.3473 V nea29583_ch10_371-442.indd 397 12/11/10 12:40 PM 398 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor and 4s fp xdT __ eNa 12 4(11.7)(8.85 1014)(0.3473) _____ (1.6 1019)(1016) 12 0.30 104 cm Then (3.9)(8.85 1014) 3.9 (0.30 104) 180 108 _ 11.7 ox ______ C min ___ ox tox _ s xdT 2.925 108 F /cm2 We may note that C min ___ _ 2.925 10 0.1525 8 Cox 1.9175 107 The flat-band capacitance is ox ____ ___ C FB V _ eN ox tox _ s t s a (3.9)(8.85 1014) ________________________ _________ (0.0259)(11.7)(8.85 1014) 3.9 _____ 180 108 _ 11.7 (1.6 1019)(1016) 1.091 107 F /cm2 We also note that C FB ___ _ 1.091 10 0.569 7 Cox 1.9175 107 ■ Comment The ratios of C min Cox and C FB Cox are typical values obtained in C–V plots. ■ EXERCISE PROBLEM Ex 10.6 Consider a MOS capacitor with the following parameters: n polysilicon gate, Na 3 1016 cm3, tox 8 nm 80 Å, and Q ss 2 1010 cm2. Determine the ratios C minCox and C FBCox. (Ans. C min Cox 0.118, C FB Cox 0.504) If we assume the oxide capacitance per unit area is Cox 1.9175 107 F/cm2 and the channel length and width are L 2 m and W 20 m, respectively, then the total gate oxide capacitance is CoxT Cox LW (1.9175 107)(2 104)(20 104) 7.67 1014 F 0.0767 pF 76.7 fF The total oxide capacitance in a typical MOS device is quite small. nea29583_ch10_371-442.indd 398 12/11/10 12:40 PM 10.2 Capacitance–Voltage Characteristics 399 C Strong inversion Accumulation Depletion Moderate inversion 0 VG Figure 10.27 | Ideal low-frequency capacitance versus gate voltage of a MOS capacitor with an n-type substrate. The same type of ideal C–V characteristics is obtained for a MOS capacitor with an n-type substrate by changing the sign of the voltage axis. The accumulation condition is obtained for a positive gate bias and the inversion condition is obtained for a negative gate bias. This ideal curve is shown in Figure 10.27. 10.2.2 Frequency Effects Figure 10.25a shows the MOS capacitor with a p-type substrate and biased in the inversion condition. We have argued that a differential change in the capacitor voltage in the ideal case causes a differential change in the inversion layer charge density. However, we must consider the source of electrons that produces a change in the inversion charge density. There are two sources of electrons that can change the charge density of the inversion layer. The first source is by diffusion of minority carrier electrons from the p-type substrate across the space charge region. This diffusion process is the same as that in a reverse-biased pn junction that generates the ideal reverse saturation current. The second source of electrons is by thermal generation of electron–hole pairs within the space charge region. This process is again the same as that in a reverse-biased pn junction generating the reverse-biased generation current. Both of these processes generate electrons at a particular rate. The electron concentration in the inversion layer, then, cannot change instantaneously. If the ac voltage across the MOS capacitor changes rapidly, the change in the inversion layer charge will not be able to respond. The C–V characteristics will then be a function of the frequency of the ac signal used to measure the capacitance. In the limit of a very high frequency, the inversion layer charge will not respond to a differential change in capacitor voltage. Figure 10.28 shows the charge distribution in the MOS capacitor with a p-type substrate. At a high-signal frequency, the differential change in charge occurs at the metal and in the space charge width in the semiconduc , which we discussed earlier. tor. The capacitance of the MOS capacitor is then C min The high-frequency and low-frequency limits of the C–V characteristics are shown in Figure 10.29. In general, high frequency corresponds to a value on the order of 1 MHz and low frequency corresponds to values in the range of 5 to 100 Hz. Typically, the high-frequency characteristics of the MOS capacitor are measured. nea29583_ch10_371-442.indd 399 12/11/10 12:40 PM 400 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Metal Oxide p-type semiconductor |dQ| Q xd T Q dx |dQ| Figure 10.28 | Differential charge distribution at inversion for a high-frequency differential change in gate voltage. Low frequency C Accumulation High frequency Inversion 0 VG Figure 10.29 | Low-frequency and high-frequency capacitance versus gate voltage of a MOS capacitor with a p-type substrate. 10.2.3 Fixed Oxide and Interface Charge Effects In all of the discussion concerning C–V characteristics so far, we have assumed an ideal oxide in which there are no fixed oxide or oxide–semiconductor interface charges. These two types of charges will change the C–V characteristics. We previously discussed how the fixed oxide charge affects the threshold voltage. This charge will also affect the flat-band voltage. The flat-band voltage from Equation (10.25) is given by Q ss VFB ms _ Cox where Qss is the equivalent fixed oxide charge and ms is the metal–semiconductor work function difference. The flat-band voltage shifts to more negative voltages for a positive fixed oxide charge. Since the oxide charge is not a function of gate voltage, the curves nea29583_ch10_371-442.indd 400 12/11/10 12:40 PM 10.2 Qss3 Qss2 Qss2 Qss1 Qss1 0 Capacitance–Voltage Characteristics 401 C Qss 0 (ideal) Cox Ec Cmin VFB3 VFB2 VFB1 VFB0 0 Allowed electronic energy states EFi Donor states Ev VG Figure 10.30 | High-frequency capacitance versus gate voltage of a MOS capacitor with a p-type substrate for several values of effective trapped oxide charge. Acceptor states Figure 10.31 | Schematic diagram showing interface states at the oxide– semiconductor interface. show a parallel shift with oxide charge, and the shape of the C–V curves remains the same as the ideal characteristics. Figure 10.30 shows the high-frequency characteristics of a MOS capacitor with a p-type substrate for several values of fixed positive oxide charge. The C–V characteristics can be used to determine the equivalent fixed oxide charge. For a given MOS structure, ms and Cox are known, so the ideal flat-band voltage and flat-band capacitance can be calculated. The experimental value of flat-band voltage can be measured from the C–V curve, and the value of fixed oxide charge can then be determined. The C–V measurements are a valuable diagnostic tool to characterize a MOS device. This characterization is especially useful in the study of radiation effects on MOS devices, for example. We first encountered oxide–semiconductor interface states in Chapter 9 in the discussion of Schottky barrier diodes. Figure 10.31 shows the energy-band diagram of a semiconductor at the oxide–semiconductor interface. The periodic nature of the semiconductor is abruptly terminated at the interface so that allowed electronic energy levels will exist within the forbidden bandgap. These allowed energy states are referred to as interface states. Charge can flow between the semiconductor and interface states, in contrast to the fixed oxide charge. The net charge in these interface states is a function of the position of the Fermi level in the bandgap. In general, acceptor states exist in the upper half of the bandgap and donor states exist in the lower half of the bandgap. An acceptor state is neutral if the Fermi level is below the state and becomes negatively charged if the Fermi level is above the state. A donor state is neutral if the Fermi level is above the state and becomes positively charged if the Fermi level is below the state. The charge of the interface states is then a function of the gate voltage applied across the MOS capacitor. Figure 10.32a shows the energy-band diagram in a p-type semiconductor of a MOS capacitor biased in the accumulation condition. In this case, there is a net positive charge trapped in the donor states. Now let the gate voltage change to produce the energy-band diagram shown in Figure 10.32b. The Fermi level corresponds to nea29583_ch10_371-442.indd 401 12/11/10 12:40 PM 402 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Neutral acceptors Ec Positive donors EFi Neutral donors EF Ev (a) Ec EFi Neutral acceptors EF Ev Neutral donors (b) Ec Neutral acceptors EFi EF Negative acceptors Ev Neutral donors (c) Figure 10.32 | Energy-band diagram in a p-type semiconductor showing the charge trapped in the interface states when the MOS capacitor is biased (a) in accumulation, (b) at midgap, and (c) at inversion. the intrinsic Fermi level at the surface; thus, all interface states are neutral. This particular bias condition is known as midgap. Figure 10.32c shows the condition at inversion in which there is now a net negative charge in the acceptor states. The net charge in the interface states changes from positive to negative as the gate voltage sweeps from the accumulation, depletion, to the inversion condition. We noted that the C–V curves shifted in the negative gate voltage direction due to positive fixed oxide charge. When interface states are present, the amount and direction of the shift change as we sweep through the gate voltage, since the amount and sign of the interface trapped charge change. The C–V curves now become “smeared out” as shown in Figure 10.33. Again, the C–V measurements can be used as a diagnostic tool in semiconductor device process control. For a given MOS device, the ideal C–V curve can be determined. nea29583_ch10_371-442.indd 402 12/11/10 12:40 PM 10.3 The Basic MOSFET Operation 403 Ideal C CFB (flat-band) With interface states Midgap Threshold 0 VG Figure 10.33 | High-frequency C–V characteristics of a MOS capacitor showing effects of interface states. Any “smearing out” in the experimental curve indicates the presence of interface states and any parallel shift indicates the presence of fixed oxide charge. The amount of smearing out can be used to determine the density of interface states. These types of measurement are extremely useful in the study of radiation effects on MOS devices. 10.3 | THE BASIC MOSFET OPERATION The current in a MOSFET is due to the flow of charge in the inversion layer or channel region adjacent to the oxide–semiconductor interface. We have discussed the creation of the inversion layer charge in enhancement-type MOS capacitors. We may also have depletion-type devices in which a channel already exists at zero gate voltage. 10.3.1 MOSFET Structures There are four basic MOSFET device types. Figure 10.34 shows an n-channel enhancement mode MOSFET. Implicit in the enhancement mode notation is the idea that the semiconductor substrate is not inverted directly under the oxide with zero gate voltage. A positive gate voltage induces the electron inversion layer, which then “connects” the n-type source and the n-type drain regions. The source terminal is the source of carriers that flow through the channel to the drain terminal. For this n-channel device, electrons flow from the source to the drain so the conventional current will enter the drain and leave the source. The conventional circuit symbol for this n-channel enhancement mode device is also shown in the figure. Figure 10.35 shows an n-channel depletion mode MOSFET. An n-channel region exists under the oxide with 0 V applied to the gate. However, we have shown that the threshold voltage of a MOS device with a p-type substrate may be negative; this means that an electron inversion layer already exists with zero gate voltage applied. Such a device is also considered to be a depletion mode device. The n-channel shown in the figure can be an electron inversion layer or an intentionally doped n region. The conventional circuit symbol for the n-channel depletion mode MOSFET is also shown in the figure. Figures 10.36a, b show a p-channel enhancement mode MOSFET and a p-channel depletion mode MOSFET. In the p-channel enhancement mode device, a negative nea29583_ch10_371-442.indd 403 12/11/10 12:40 PM 404 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Source (S) Gate (G) Drain (D) D n n p B G S Substrate or body (B) Figure 10.34 | Cross section and circuit symbol for an n-channel enhancement mode MOSFET. Source (S) Gate (G) Drain (D) D n n p n channel B G S Body (B) Figure 10.35 | Cross section and circuit symbol for an n-channel depletion mode MOSFET. gate voltage must be applied to create an inversion layer of holes that will “connect” the p-type source and drain regions. Holes flow from the source to the drain, so the conventional current will enter the source and leave the drain. A p-channel region exists in the depletion mode device even with zero gate voltage. The conventional circuit symbols are shown in the figure. 10.3.2 Current–Voltage Relationship—Concepts Figure 10.37a shows an n-channel enhancement mode MOSFET with a gate-tosource voltage that is less than the threshold voltage and with only a very small drain-to-source voltage. The source and substrate, or body, terminals are held at ground potential. With this bias configuration, there is no electron inversion layer, the drain-to-substrate pn junction is reverse biased, and the drain current is zero (disregarding pn junction leakage currents). nea29583_ch10_371-442.indd 404 12/11/10 12:40 PM 10.3 Source (S) Gate (G) The Basic MOSFET Operation 405 Drain (D) D p p B n G S Body (B) (a) Source (S) Gate (G) Drain (D) D p p B n p channel G S Body (B) (b) Figure 10.36 | Cross section and circuit symbol for (a) a p-channel enhancement mode MOSFET and (b) a p-channel depletion mode MOSFET. Figure 10.37b shows the same MOSFET with an applied gate voltage such that VGS VT. An electron inversion layer has been created so that when a small drain voltage is applied, the electrons in the inversion layer will flow from the source to the positive drain terminal. The conventional current enters the drain terminal and leaves the source terminal. In this ideal case, there is no current through the oxide to the gate terminal. For small VDS values, the channel region has the characteristics of a resistor, so we can write ID gd VDS (10.41) where gd is defined as the channel conductance in the limit as VDS → 0. The channel conductance is given by W ⴢ Q gd _ (10.42) n n L nea29583_ch10_371-442.indd 405 12/11/10 12:40 PM 406 CHAPTER 10 VGS S Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor VT G VDS D VGS S VT G VDS D ID ID n n n p n Induced electron inversion layer Space charge regions p (a) Space charge regions (b) Figure 10.37 | The n-channel enhancement mode MOSFET (a) with an applied gate voltage VGS applied gate voltage VGS VT. VGS2 ID VT and (b) with an VGS1 VGS1 VGS VT VT VDS Figure 10.38 | ID versus VDS characteristics for small values of VDS at three VGS voltages. where n is the mobility of the electrons in the inversion layer and Qn is the magnitude of the inversion layer charge per unit area. The inversion layer charge is a function of the gate voltage; thus, the basic MOS transistor action is the modulation of the channel conductance by the gate voltage. The channel conductance, in turn, determines the drain current. We will initially assume that the mobility is a constant; we will discuss mobility effects and variations in the next chapter. The ID versus VDS characteristics, for small values of VDS, are shown in Figure 10.38. When VGS VT, the drain current is zero. As VGS becomes larger than VT, channel inversion charge density increases, which increases the channel conductance. A larger value of gd produces a larger initial slope of the ID versus VDS characteristic as shown in the figure. Figure 10.39a shows the basic MOS structure for the case when VGS VT and the applied VDS voltage is small. The thickness of the inversion channel layer in the nea29583_ch10_371-442.indd 406 12/11/10 12:40 PM VGS1 VT Oxide S Channel inversion charge ID ID VDS Depletion region p type VDS L (a) VGS1 Oxide ID ID S VDS Channel inversion charge p type VDS (b) VGS1 Oxide ID ID S VDS (sat) Channel inversion charge p type VDS (sat) VDS (c) VGS1 S Oxide VDS (sat) E-field p type ID ID VDS VDS(sat) Channel inversion charge Saturation region VDS (sat) VDS (d) Figure 10.39 | Cross section and ID versus VDS curve when VGS VT for (a) a small VDS value, (b) a larger VDS value, (c) a value of VDS VDS(sat), and (d) a value of VDS VDS(sat). 407 nea29583_ch10_371-442.indd 407 12/11/10 12:40 PM 408 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor figure qualitatively indicates the relative charge density, which is essentially constant along the entire channel length for this case. The corresponding ID versus VDS curve is shown in the figure. Figure 10.39b shows the situation when the VDS value increases. As the drain voltage increases, the voltage drop across the oxide near the drain terminal decreases, which means that the induced inversion charge density near the drain also decreases. The incremental conductance of the channel at the drain decreases, which then means that the slope of the ID versus VDS curve will decrease. This effect is shown in the ID versus VDS curve in the figure. When VDS increases to the point where the potential drop across the oxide at the drain terminal is equal to VT, the induced inversion charge density is zero at the drain terminal. This effect is schematically shown in Figure 10.39c. At this point, the incremental conductance at the drain is zero, which means that the slope of the ID versus VDS curve is zero. We can write VGS VDS (sat) VT (10.43a) VDS (sat) VGS VT (10.43b) or where VDS (sat) is the drain-to-source voltage producing zero inversion charge density at the drain terminal. When VDS becomes larger than the VDS (sat) value, the point in the channel at which the inversion charge is just zero moves toward the source terminal. In this case, electrons enter the channel at the source, travel through the channel toward the drain, and then, at the point where the charge goes to zero, the electrons are injected into the space charge region where they are swept by the E-field to the drain contact. If we assume that the change in channel length L is small compared to the original length L, then the drain current will be a constant for VDS VDS (sat). The region of the ID versus VDS characteristic is referred to as the saturation region. Figure 10.39d shows this region of operation. When VGS changes, the ID versus VDS curve will change. We saw that, if VGS increases, the initial slope of ID versus VDS increases. We can also note from Equation (10.43b) that the value of VDS (sat) is a function of VGS. We can generate the family of curves for this n-channel enhancement mode MOSFET as shown in Figure 10.40. Figure 10.41 shows an n-channel depletion mode MOSFET. If the n-channel region is actually an induced electron inversion layer created by the metal– semiconductor work function difference and fixed charge in the oxide, the current–voltage characteristics are exactly the same as we have discussed, except that VT is a negative quantity. We may also consider the case when the n-channel region is actually an n-type semiconductor region. In this type of device, a negative gate voltage will induce a space charge region under the oxide, reducing the thickness of the n-channel region. The reduced thickness decreases the channel conductance, which reduces the drain current. A positive gate voltage will create an electron accumulation layer, which increases the drain current. One basic requirement for this device is that the channel nea29583_ch10_371-442.indd 408 12/11/10 12:40 PM 10.3 VDS (sat) VGS VT S VGS5 VGS4 VGS4 VGS3 VGS3 VGS2 VGS2 VGS1 ID VGS1 The Basic MOSFET Operation VT G n 409 D n n channel tc p type 0 VDS B Figure 10.40 | Family of ID versus VDS curves for an n-channel enhancement mode MOSFET. Figure 10.41 | Cross section of an n-channel depletion mode MOSFET. thickness tc must be less than the maximum induced space charge width in order to be able to turn the device off. The general ID versus VDS family of curves for an n-channel depletion mode MOSFET is shown in Figure 10.42. In the next section, we derive the ideal current–voltage relation for the n-channel MOSFET. In the nonsaturation region, we obtain Wn Cox ID __ 2(VGS VT)VDS V 2DS 2L (10.44a) which can be written as k W ID _n ⴢ _ ⴢ 2(VGS VT)VDS V 2DS 2 L (10.44b) ID Kn 2(VGS VT)VDS V 2DS (10.44c) or VDS(sat) VGS VT VGS2 VGS1 ID VGS1 0 VGS 0 VGS3 VT VGS4 0 VGS3 VDS Figure 10.42 | Family of ID versus VDS curves for an n-channel depletion mode MOSFET. nea29583_ch10_371-442.indd 409 12/11/10 12:40 PM 410 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor The parameter kn nCox is called the process conduction parameter for the n-channel MOSFET and has units of A /V 2. The parameter Kn (Wn Cox)2L (kn2) ⴢ (WL) is called the conduction parameter for the n-channel MOSFET and also has units of A /V2. When the transistor is biased in the saturation region, the ideal currernt–voltage relation is given by Wn Cox ID __ (VGS VT)2 2L (10.45a) k W ID _n ⴢ _ ⴢ (VGS VT)2 2 L (10.45b) ID Kn (VGS VT)2 (10.45c) which can be written as or In general, for a given technology, the process conduction parameter, kn, is a constant. From Equations (10.44b) and (10.45b), then, we see that the design of a MOSFET, in terms of current capability, is determined by the width-to-length parameter. The operation of a p-channel device is the same as that of the n-channel device, except the charge carrier is the hole and the conventional current direction and voltage polarities are reversed. *10.3.3 Current–Voltage Relationship—Mathematical Derivation In the previous section, we qualitatively discussed the current–voltage characteristics. In this section, we derive the mathematical relation between the drain current, the gate-to-source voltage, and the drain-to-source voltage. Figure 10.43 shows the geometry of the device that we use in this derivation. In this analysis, we make the following assumptions: 1. 2. 3. 4. 5. The current in the channel is due to drift rather than diffusion. There is no current through the gate oxide. A gradual channel approximation is used in which Ey y Ex x. This approximation means that Ex is essentially a constant. Any fixed oxide charge is an equivalent charge density at the oxide– semiconductor interface. The carrier mobility in the channel is constant. We start the analysis with Ohm’s law, which can be written as Jx Ex (10.46) where is the channel conductivity and Ex is the electric field along the channel created by the drain-to-source voltage. The channel conductivity is given by en n(y), where n is the electron mobility and n(y) is the electron concentration in the inversion layer. nea29583_ch10_371-442.indd 410 12/11/10 12:40 PM 10.3 S Channel inversion layer (electrons) W y The Basic MOSFET Operation 411 Induced D depletion region Oxide x n n L z p substrate Figure 10.43 | Geometry of a MOSFET for ID versus VDS derivation. The total channel current is found by integrating Jx over the cross-sectional area in the y and z directions. Then Ix Jx dy dz (10.47) We may write that y z Qn en(y) dy (10.48) where Qn is the inversion layer charge per unit area and is a negative quantity for this case. Equation (10.47) then becomes Ix W n Qn Ex (10.49) where W is the channel width, the result of integrating over z. Two concepts we use in the currernt–voltage derivation are charge neutrality and Gauss’s law. Figure 10.44 shows the charge densities through the device for VGS VT. The charges are all given in terms of charge per unit area. Using the concept of charge neutrality, we can write Qm Qss Qn Q SD(max) 0 (10.50) The inversion layer charge and induced space charge are negative for this n-channel device. Gauss’s law can be written as En dS QT (10.51) s nea29583_ch10_371-442.indd 411 12/11/10 12:40 PM 412 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Gate Fixed oxide charge, Qss Metal Oxide p-type semiconductor Oxide Qm dx 4 Qss y Eox 2 Surface S 1 xd T x Depletion layer charge, QSD(max) QSD(max) eNa xdT Qn p type Figure 10.44 | Charge distribution in the n-channel enhancement mode MOSFET for VGS VT. 3 Inversion layer charge Qn Figure 10.45 | Geometry for applying Gauss’s law. where the integral is over a closed surface. QT is the total charge enclosed by the surface, and En is the outward directed normal component of the electric field crossing the surface S. Gauss’s law is applied to the surface defined in Figure 10.45. Since the surface must be enclosed, we must take into account the two end surfaces in the x-y plane. However, there is no z-component of the electric field so these two end surfaces do not contribute to the integral of Equation (10.51). Now consider the surfaces labeled 1 and 2 in Figure 10.45. From the gradual channel approximation, we assume that Ex is essentially a constant along the channel length. This assumption means that Ex into surface 2 is the same as Ex out of surface 1. Since the integral in Equation (10.51) involves the outward component of the E-field, the contributions of surfaces 1 and 2 cancel each other. Surface 3 is in the neutral p region, so the electric field is zero at this surface. Surface 4 is the only surface that contributes to Equation (10.51). Taking into account the direction of the electric field in the oxide, Equation (10.51) becomes En dS oxEoxW dx QT (10.52) s where ox is the permittivity of the oxide. The total charge enclosed is (max)]W dx QT [Q ss Q n Q SD (10.53) Combining Equations (10.52) and (10.53), we have (max) oxEox Q ss Q n Q SD (10.54) We now need an expression for Eox. Figure 10.46a shows the oxide and channel. We assume that the source is at ground potential. The voltage Vx is the potential in the channel at a point x along the channel length. The potential difference across the oxide at x is a function of VGS, Vx, and the metal–semiconductor work function difference. nea29583_ch10_371-442.indd 412 12/11/10 12:40 PM 10.3 The Basic MOSFET Operation 413 eVox e Eg 2 VGS em efp es Vox S EFi EFp Ev e(VGS Vx ) EFm M Vx Ec O S x (a) (b) Figure 10.46 | (a) Potentials at a point x along the channel. (b) Energy-band diagram through the MOS structure at the point x. The energy-band diagram through the MOS structure at point x is shown in Figure 10.46b. The Fermi level in the p-type semiconductor is EFp and the Fermi level in the metal is EFm. We have EFp EFm e(VGS Vx) Considering the potential barriers, we can write Eg VGS Vx (m Vox) _ s fp 2e which can also be written as VGS Vx Vox 2fp ms (10.55) (10.56) (10.57) where ms is the metal–semiconductor work function difference, and s 2fp for the inversion condition. The electric field in the oxide is Vox Eox _ (10.58) tox Combining Equations (10.54), (10.57), and (10.58), we find that ox ox Eox _ tox [(VGS Vx) (ms 2fp)] Q ss Q n Q SD(max) (10.59) The inversion charge density, Q n, from Equation (10.59) can be substituted into Equation (10.49) and we obtain dV Ix Wn Cox _x [(VGS Vx) VT] (10.60) dx where Ex dVxdx and VT is the threshold voltage defined by Equation (10.31b). We can now integrate Equation (10.60 ) over the length of the channel. We have L Vx(L) : Ix dx Wn Cox : [(VGS VT) Vx] dVx (10.61) 0 nea29583_ch10_371-442.indd 413 Vx(0) 12/11/10 12:40 PM 414 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor We are assuming a constant mobility n. For the n-channel device, the drain current enters the drain terminal and is a constant along the entire channel length. Letting ID Ix, Equation (10.61) becomes Wn Cox 2 ID __ [2(VGS VT)VDS VDS ] 2L (10.62) Equation (10.62) is valid for VGS VT and for 0 VDS VDS (sat). Equation (10.62) can also be written as k W ID _n ⴢ _ ⴢ 2(VGS VT)VDS V2DS Kn 2(VGS VT) VDS V2DS 2 L (10.63) where kn is the process conduction parameter and Kn is the conduction parameter. These parameters are described and defined in Equations (10.44b) and (10.44c). Figure 10.47 shows plots of Equation (10.62) as a function of VDS for several values of VGS. We can find the value of VDS at the peak current value from ID VDS 0. Then, using Equation (10.62), the peak current occurs when VDS VGS VT (10.64) This value of VDS is just VDS (sat), the point at which saturation occurs. For VDS VDS (sat), the ideal drain current is a constant and is equal to Wn Cox 2 ID (sat) __ [2(VGS VT)VDS (sat) VDS (sat)] 2L (10.65) Using Equation (10.64) for VDS (sat), Equation (10.65) becomes Wn Cox ID (sat) __ (VGS VT)2 2L Equation (10.66) can also be written as k W ID _n ⴢ _ ⴢ (VGS VT)2 Kn (VGS VT)2 2 L (10.66) (10.67) VGS3 ID VGS2 VGS1 VDS Figure 10.47 | Plots of ID versus VDS from Equation (10.62). nea29583_ch10_371-442.indd 414 12/11/10 12:40 PM 10.3 The Basic MOSFET Operation 415 Equation (10.62) is the ideal current–voltage relationship of the n-channel MOSFET in the nonsaturation region for 0 VDS VDS (sat), and Equation (10.66) is the ideal current–voltage relationship of the n-channel MOSFET in the saturation region for VDS VDS (sat). These I–V expressions were explicitly derived for an n-channel enhancement mode device. However, these same equations apply to an n-channel depletion mode MOSFET in which the threshold voltage VT is a negative quantity. Objective: Design the width of a MOSFET such that a specified current is induced for a given applied bias. Consider an ideal n-channel MOSFET with parameters L 1.25 m, n 650 cm2 /V-s, Cox 6.9 108 F /cm2, and VT 0.65 V. Design the channel width W such that ID (sat) 4 mA for VGS 5 V. EXAMPLE 10.7 ■ Solution For the transition biased in the saturation region, we have, from Equation (10.66), Wn Cox ID (sat) __ (VGS VT)2 2L or W(650)(6.9 108) 4 103 ____ ⴢ (5 0.65)2 3.39 W 2(1.25 104) Then W 11.8 m ■ Comment The current capability of a MOSFET is directly proportional to the channel width W. The current handling capability can be increased by increasing W. ■ EXERCISE PROBLEM Ex 10.7 The parameters of an n-channel silicon MOSFET are n 650 cm2 /V-s, tox 8 nm 80 Å, WL 12, and VT 0.40 V. If the transistor is biased in the saturation region, find the drain current for (a) VGS 0.8 V, (b) VGS 1.2 V, and (c) VGS 1.6 V. [Ans. (a) 0.269 mA; (b) 1.077 mA; (c) 2.423 mA] We can use the I–V relations to experimentally determine the mobility and threshold voltage parameters. From Equation (10.62), we can write, for very small values of VDS, Wn Cox ID __ (VGS VT)VDS L (10.68) Figure 10.48a shows a plot of Equation (10.68) as a function of VGS for constant VDS. A straight line is fitted through the points. The deviation from the straight line at low values of VGS is due to subthreshold conduction and the deviation at higher values of VGS nea29583_ch10_371-442.indd 415 12/11/10 12:40 PM 416 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Very small VDS ID ID B A Slope CoxW 2L Slope CoxWVDS L VT VTB VGS VTA VGS (b) (a) Figure 10.48 __| (a) ID versus VGS (for small VDS) for enhancement mode MOSFET. (b) Ideal ID versus VGS in saturation region for enhancement mode (curve A) and depletion mode (curve B) n-channel MOSFETs. is due to mobility being a function of gate voltage. Both of these effects will be considered in the next chapter. The extrapolation of the straight line to zero current gives the threshold voltage, and the slope is proportional to the inversion carrier mobility. Now consider the case when the transistor is biased in the saturation region. If we take the square root of Equation (10.66), we obtain ______ _______ ID(sat) Wn Cox __ (V 2L GS VT) (10.69) Figure 10.48b is a plot of Equation (10.69). In the ideal case, we can obtain the same information from both curves. However, as we will see in the next chapter, the threshold voltage may be a function of VDS in short-channel devices. Since Equation (10.69) applies to devices biased in the saturation region, the VT parameter in this equation may differ from the extrapolated value determined in Figure 10.48a. In general, the nonsaturation current–voltage characteristics will produce the more reliable data. EXAMPLE 10.8 Objective: Determine the inversion carrier mobility from experimental results. Consider an n-channel MOSFET with W 15 m, L 2 m, and Cox 6.9 108 F /cm2. Assume that the drain current in the nonsaturation region for VDS 0.10 V is ID 35 A at VGS 1.5 V and ID 75 A at VGS 2.5 V. ■ Solution From Equation (10.68), we can write Wn Cox ID2 ID1 __ (VGS2 VGS1)VDS L so that 15 (6.9 108)(2.5 1.5)(0.10) 75 106 35 106 _ n 2 nea29583_ch10_371-442.indd 416 12/11/10 12:40 PM 10.3 The Basic MOSFET Operation 417 which yields n 773 cm2 /V-s We can then determine VT 0.625 V ■ Comment The mobility of carriers in the inversion layer is less than that in the bulk semiconductor due to the surface scattering effect. We will discuss this effect in the next chapter. ■ EXERCISE PROBLEM Ex 10.8 An n-channel silicon MOSFET has the following parameters: W 6 m, L 1.5 m, and tox 8 nm 80 Å. When the transistor is biased in the saturation region, the drain current is ID(sat) 0.132 mA at VGS 1.0 V and ID(sat) 0.295 mA at VGS 1.25 V. Determine the electron mobility and the threshold voltage. (Ans. n 600 cm2 /V-s, VT 0.495 V) The current–voltage relationship of a p-channel device can be obtained by the same type of analysis. Figure 10.49 shows a p-channel enhancement mode MOSFET. The voltage polarities and current direction are the reverse of those in the n-channel device. We may note the change in the subscript notation for this device. For the current direction shown in the figure, the I–V relation for the p-channel MOSFET biased in the nonsaturation region is Wp Cox ID __ 2(VSG VT)VSD V2SD 2L (10.70) Equation (10.70) is valid for 0 VSD VSD(sat). VSD VSG S ID G D p p n substrate B Figure 10.49 | Cross section and bias configuration for a p-channel enhancement mode MOSFET. nea29583_ch10_371-442.indd 417 12/11/10 12:40 PM 418 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Equation (10.70) can also be written as kp W ID _ ⴢ _ ⴢ 2(VSG VT)VSD V2SD Kp 2(VSG VT)VSD V2SD 2 L (10.71) where kp pCox is the process conduction parameter for the p-channel MOSFET and Kp (Wp Cox)(2L) (kp 2) ⴢ (WL) is the conduction parameter. When the transistor is biased in the saturation region, the I–V relation is given by Wp Cox ID(sat) __ (VSG VT)2 2L (10.72) Equation (10.72) is valid for VSD VSD (sat). Equation (10.72) can also be written as kp W ID _ ⴢ _ ⴢ (VSG VT)2 Kp(VSG VT)2 2 L (10.73) The source-to-drain saturation voltage is given by VSD(sat) VSG VT (10.74) Note the change in the sign in front of VT and note that the mobility is now the mobility of the holes in the hole inversion layer charge. Keep in mind that VT is negative for a p-channel enhancement mode MOSFET and positive for a depletion mode p-channel device. One assumption we made in the derivation of the currernt–voltage relationship was that the charge neutrality condition given by Equation (10.50) was valid over (max) was constant the entire length of the channel. We implicitly assumed that Q SD along the length of the channel. The space charge width, however, varies between source and drain due to the drain-to-source voltage; it is widest at the drain when VDS 0. A change in the space charge density along the channel length must be balanced by a corresponding change in the inversion layer charge. An increase in the space charge width means that the inversion layer charge is reduced, implying that the drain current and drain-to-source saturation voltage are less than the ideal values. The actual saturation drain current may be as much as 20 percent less than the predicted value due to this bulk charge effect. 10.3.4 Transconductance The MOSFET transconductance is defined as the change in drain current with respect to the corresponding change in gate voltage, or ID gm _ VGS (10.75) The transconductance is sometimes referred to as the transistor gain. nea29583_ch10_371-442.indd 418 12/11/10 12:40 PM 10.3 The Basic MOSFET Operation 419 If we consider an n-channel MOSFET operating in the nonsaturation region, then using Equation (10.62), we have Wn Cox ID gmL _ __ ⴢ VDS VGS L (10.76) The transconductance increases linearly with VDS but is independent of VGS in the nonsaturation region. The I–V characteristics of an n-channel MOSFET in the saturation region are given by Equation (10.66). The transconductance in this region of operation is given by Wn Cox ID(sat) __ gms __ (VGS VT) VGS L (10.77) In the saturation region, the transconductance is a linear function of VGS and is independent of VDS. The transconductance is a function of the geometry of the device as well as of carrier mobility and threshold voltage. The transconductance increases as the width of the device increases, and it also increases as the channel length and oxide thickness decrease. In the design of MOSFET circuits, the size of the transistor, in particular the channel width W, is an important engineering design parameter. 10.3.5 Substrate Bias Effects In all of our analyses so far, the substrate, or body, has been connected to the source and held at ground potential. In MOSFET circuits, the source and body may not be at the same potential. Figure 10.50a shows an n-channel MOSFET and the associated double-subscripted voltage variables. The source-to-substrate pn junction must always be zero or reverse biased, so VSB must always be greater than or equal to zero. S VGS VDS es = e(2fp VSB) G D n n EFi Ec EF Ev es = 2efp EFi Ec EF Ev p substrate EFn Body (B) VSB (a) (b) (c) Figure 10.50 | (a) Applied voltages on an n-channel MOSFET. (b) Energy-band diagram at inversion point when VSB 0. (c) Energy-band diagram at inversion point when VSB 0 is applied. nea29583_ch10_371-442.indd 419 12/11/10 12:40 PM 420 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor If VSB 0, threshold is defined as the condition when s 2fp as we discussed previously and as shown in Figure 10.50b. When VSB 0 the surface will still try to invert when s 2fp. However, these electrons are at a higher potential energy than are the electrons in the source. The newly created electrons will move laterally and flow out of the source terminal. When s 2fp VSB, the surface reaches an equilibrium inversion condition. The energy-band diagram for this condition is shown in Figure 10.50c. The curve represented as EFn is the Fermi level from the p substrate through the reverse-biased source–substrate junction to the source contact. The space charge region width under the oxide increases from the original xdT value when a reverse-biased source–substrate junction voltage is applied. With an applied VSB 0, there is more charge associated with this region. Considering the charge neutrality condition through the MOS structure, the positive charge on the top metal gate must increase to compensate for the increased negative space charge in order to reach the threshold inversion point. So when VSB 0, the threshold voltage of the n-channel MOSFET increases. When VSB 0, we had ___________ Q SD (max) eNaxdT 2es Na(2fp) When VSB (10.78) 0, the space charge width increases and we now have ________________ Q SD eNaxd 2es Na(2fp VSB) (10.79) The change in the space charge density is then _________ ______ ____ Q SD 2es Na 2fp VSB 2fp (10.80) To reach the threshold condition, the applied gate voltage must be increased. The change in threshold voltage can be written as ______ Q SD __ 2e N VT _ s a 2fp VSB 2fp Cox _________ ____ Cox (10.81) 0) VT (VSB 0). We may note that VSB must always be where VT VT (VSB positive so that, for the n-channel device, VT is always positive. The threshold voltage of the n-channel MOSFET will increase as a function of the source–substrate junction voltage. From Equation (10.81), we may define ______ 2es Na __ (10.82) Cox where is defined as the body-effect coefficient. Equation (10.81) may then be written as _________ ____ VT 2fp VSB 2fp nea29583_ch10_371-442.indd 420 (10.83) 12/11/10 12:40 PM 10.3 The Basic MOSFET Operation 421 Objective: Calculate the body-effect coefficient and the change in the threshold voltage due EXAMPLE 10.9 to an applied source-to-body voltage. Consider an n-channel silicon MOSFET at T 300 K. Assume the substrate is doped to Na 3 1016 cm3 and assume the oxide is silicon dioxide with a thickness of tox 20 nm 200 Å. Let VSB 1 V. ■ Solution We can calculate that Na 3 1016 __ fp Vt ln _ ni (0.0259) ln 1.5 1010 0.3758 V and (3.9)(8.85 1014) ox ____ Cox _ 1.726 107 F /cm2 tox 200 108 From Equation (10.82), we find the body-effect coefficient to be ______ [2(1.6 1019)(11.7)(8.85 1014)(3 1016)]12 2es Na ________ __ 1.726 107 Cox or 0.5776 V12 The change in threshold voltage for VSB 1 V is found to be _________ ____ VT 2fp VSB 2fp ____________ _________ (0.5776) 2(0.3758) 1 2(0.3758) (0.5776)[1.3235 0.8669] 0.264 V ■ Comment ______ Figure 10.51 shows plots of ID(sat) versus VGS for various applied values of VSB. The original threshold voltage is assumed to be VTO 0.64 V. VSB 0 1 V 2 V 4 V ID 0 0.64 0.904 1.10 1.40 VGS (V) 2.0 __ Figure 10.51 | Plots of ID versus VGS at several values of VSB for an n-channel MOSFET. nea29583_ch10_371-442.indd 421 12/11/10 12:40 PM 422 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor ■ EXERCISE PROBLEM Ex 10.9 A silicon MOSFET has the following parameters: Na 1016 cm3 and tox 12 nm 120 Å. Calculate (a) the body-effect coefficient and (b) the change in threshold voltage for (i) VSB 1 and (ii) VSB 2 V. [Ans. (a) 0.200 V12; (b) (i) VT 0.0937 V, (ii) VT 0.162 V] If a body or substrate bias is applied to a p-channel device, the threshold voltage is shifted to more negative values. Because the threshold voltage of a p-channel enhancement mode MOSFET is negative, a body voltage will increase the applied negative gate voltage required to create inversion. The same general observation was made for the n-channel MOSFET. TEST YOUR UNDERSTANDING TYU 10.6 The silicon n-channel MOSFET described in Exercise Problem Ex 10.7 is to be redesigned by changing the WL ratio such that ID 100 A when the transistor is biased in the saturation regin with VGS 1.0 V. TYU 10.7 The parameters of a p-channel MOSFET are p 310 cm2 /V-s, tox 220 Å, WL 60, and VT 0.40 V. If the transistor is biased in the saturation region, find the drain current for VSG 1, 1.5, and 2 V. TYU 10.8 The p-channel MOSFET in TYU 10.7 is to be redesigned by changing the (WL) ratio such that ID 200 A when the transistor is biased in the saturation region with VSG 1.25 V. TYU 10.9 Repeat Exercise Problem Ex 10.9 for a substrate impurity doping concentration of Na 1015 cm3. (Ans. WL 1.98) (Ans. ID 0.526, 1.77 and 3.74 mA) (Ans. WL 11.4) [Ans. (a) 0.0633 V12; (b) (i) VT 0.0314 V, (ii) VT 0.0536 V] 10.4 | FREQUENCY LIMITATIONS In many applications, the MOSFET is used in a linear amplifier circuit. A small-signal equivalent circuit for the MOSFET is needed in order to mathematically analyze the electronic circuit. The equivalent circuit contains capacitances and resistances that introduce frequency effects. We initially develop a small-signal equivalent circuit and then discuss the physical factors that limit the frequency response of the MOSFET. A transistor cutoff frequency, which is a figure of merit, is then defined and an expression derived for this factor. 10.4.1 Small-Signal Equivalent Circuit The small-signal equivalent circuit of the MOSFET is constructed from the basic MOSFET geometry. A model based on the inherent capacitances and resistances nea29583_ch10_371-442.indd 422 12/11/10 12:40 PM 10.4 Frequency Limitations 423 G D S Cgsp n Cgd Cgs Cgdp gmVgs rs rd n Cds p Figure 10.52 | Inherent resistances and capacitances in the n-channel MOSFET structure. within the transistor structure, along with elements that represent the basic device equations, is shown in Figure 10.52. One simplifying assumption we will make in the equivalent circuit is that the source and substrate are both tied to ground potential. Two of the capacitances connected to the gate are inherent in the device. These capacitances are Cgs and Cgd, which represent the interaction between the gate and the channel charge near the source and drain terminals, respectively. The remaining two gate capacitances, Cgsp and Cgdp, are parasitic or overlap capacitances. In real devices, the gate oxide will overlap the source and drain contacts because of tolerance or fabrication factors. As we will see, the drain overlap capacitance—Cgdp, in particular—will lower the frequency response of the device. The parameter Cds is the drain-to-substrate pn junction capacitance, and rs and rd are the series resistances associated with the source and drain terminals. The small-signal channel current is controlled by the internal gate-to-source voltage through the transconductance. The small-signal equivalent circuit for the n-channel common-source MOSFET is shown in Figure 10.53. The voltage V gs is the internal gate-to-source voltage that CgdT G D Vgs Vgs rd rds CgsT Cds gmVgs rs S Figure 10.53 | Small-signal equivalent circuit of a commonsource n-channel MOSFET. nea29583_ch10_371-442.indd 423 12/11/10 12:40 PM 424 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor controls the channel current. The parameters CgsT and CgdT are the total gate-to-source and total gate-to-drain capacitances. One parameter, rds, shown in Figure 10.53, is not shown in Figure 10.52. This resistance is associated with the slope ID versus VDS. In the ideal MOSFET biased in the saturation region, ID is independent of VDS so that rds would be infinite. In short-channel-length devices, in particular, rds is finite because of channel length modulation, which we will consider in the next chapter. A simplified small-signal equivalent circuit valid at low frequency is shown in Figure 10.54. The series resistances, rs and rd, have been neglected, so the drain current is essentially only a function of the gate-to-source voltage through the transconductance. The input gate impedance is infinite in this simplified model. The source resistance rs can have a significant effect on the transistor characteristics. Figure 10.55 shows a simplified, low-frequency equivalent circuit including rs but neglecting rds. The drain current is given by Id gmV gs (10.84) and the relation between Vgs and V gs can be found from Vgs Vgs (gmV gs)rs (1 gmrs)V gs G (10.85) D Vgs gmVgs rds S Figure 10.54 | Simplified, low-frequency small-signal equivalent circuit of a common-source n-channel MOSFET. Id G D gmVgs Vgs Vgs rs S Figure 10.55 | Simplified, lowfrequency small-signal equivalent circuit of common-source n-channel MOSFET including source resistance rs. nea29583_ch10_371-442.indd 424 12/11/10 12:40 PM 10.4 Frequency Limitations 425 The drain current from Equation (10.84) can now be written as gm Id __ V gm Vgs 1 gmrs gs (10.86) The source resistance reduces the effective transconductance or transistor gain. The equivalent circuit of the p-channel MOSFET is exactly the same as that of the n-channel except that all voltage polarities and current directions are reversed. The same capacitances and resistances that are in the n-channel model apply to the p-channel model. 10.4.2 Frequency Limitation Factors and Cutoff Frequency There are two basic frequency limitation factors in the MOSFET. The first factor is the channel transit time. If we assume that carriers are traveling at their saturation drift velocity vsat, then the transit time is t L/vsat where L is the channel length. If vsat 107 cm /s and L 1 m, then t 10 ps, which translates into a maximum frequency of 100 GHz. This frequency is much larger than the typical maximum frequency response of a MOSFET. The transit time of carriers through the channel is usually not the limiting factor in the frequency responses of MOSFETs. The second limiting factor is the gate or capacitance charging time. If we neglect rs, rd, rds, and Cds, the resulting equivalent small-signal circuit is shown in Figure 10.56 where RL is a load resistance. The input gate impedance in this equivalent circuit is no longer infinite. Summing currents at the input gate node, we have Ii j CgsTVgs j CgdT (Vgs Vd) (10.87) where Ii is the input current. Likewise, summing currents at the output drain node, we have Vd _ gmVgs j CgdT (Vd Vgs) 0 RL CgdT G Id D I i Vgs (10.88) CgsT gmVgs RL Vd S Figure 10.56 | High-frequency smallsignal equivalent circuit of commonsource n-channel MOSFET. nea29583_ch10_371-442.indd 425 12/11/10 12:40 PM 426 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Id G Ii D CgsT Vgs CM RL gmVgs S Figure 10.57 | Small-signal equivalent circuit including Miller capacitance. Combining Equations (10.87) and (10.88) to eliminate the voltage variable Vd, we can determine the input current as Ii j C gsT 1 gmRL CgdT ___ Vgs 1 j RLCgdT (10.89) Normally, RLCgdT is much less than unity; therefore, we may neglect the (j RLCgdT) term in the denominator. Equation (10.89) then simplifies to Ii j [CgsT CgdT (1 gmRL)]Vgs (10.90) Figure 10.57 shows the equivalent circuit with the equivalent input impedance described by Equation (10.90). The parameter CM is the Miller capacitance and is given by CM CgdT (1 gm RL) (10.91) The serious effect of the drain overlap capacitance now becomes apparent. When the transistor is operating in the saturation region, Cgd essentially becomes zero, but Cgdp is a constant. This parasitic capacitance is multiplied by the gain of the transistor and can become a significant factor in the input impedance. The cutoff frequency fT is defined to be the frequency at which the magnitude of the current gain of the device is unity, or when the magnitude of the input current Ii is equal to the ideal load current Id. From Figure 10.57, we can see that Ii j (CgsT CM)Vgs (10.92) Id gm Vgs (10.93) and the ideal load current is The magnitude of the current gain is then gm Id _ ___ Ii 2 f (CgsT CM) (10.94) Setting the magnitude of the current gain equal to unity at the cutoff frequency, we find gm gm fT ___ __ 2 (CgsT CM) 2 CG (10.95) where CG is the equivalent input gate capacitance. nea29583_ch10_371-442.indd 426 12/11/10 12:40 PM 10.5 The CMOS Technology 427 In the ideal MOSFET, the overlap or parasitic capacitances, Cgsp and Cgdp, are zero. Also, when the transistor is biased in the saturation region, Cgd approaches zero and Cgs is approximately CoxWL. The transconductance of the ideal MOSFET biased in the saturation region and assuming a constant mobility is given by Equation (10.77) as WnCox gms __ (VGS VT) L Then, for this ideal case, the cutoff frequency is Wn Cox __ (VGS VT) n(VGS VT) gm L _ ____ fT ___ 2 2 CG 2 (CoxWL) 2 L (10.96) Objective: Calculate the cutoff frequency of an ideal MOSFET with a constant mobility. EXAMPLE 10.10 Assume that the electron mobility in an n-channel device is n 400 cm2 /V-s and that the channel length is L 4 m. Also assume that VT 1 V and VGS 3 V. ■ Solution From Equation (10.96), the cutoff frequency is n(VGS VT) ___ 400(31) fT ___ 796 MHz 2 L2 2 (4 104)2 ■ Comment In an actual MOSFET, the effect of the parasitic capacitance will substantially reduce the cutoff frequency from that calculated in this example. ■ EXERCISE PROBLEM Ex 10.10 An n-channel silicon MOSFET has the following parameters: n 420 cm2 /V-s, tox 18 nm 180 Å, L 1.2 m, W 24 m, and VT 0.4 V. The transistor is biased in the saturation region at VGS 1.5 V. Determine the cutoff frequency. (Ans. fT 5.11 GHz) TEST YOUR UNDERSTANDING TYU 10.10 Consider the n-channel MOSFET described in Exercise Problem Ex 10.10. The transistor is connected to an effective load resistance of RL 100 k. Calculate the ratio of Miller capacitance CM to gate-to-drain capacitance CgdT. (Ans. 178) *10.5 | THE CMOS TECHNOLOGY The primary objective of this book is to present the basic physics of semiconductor materials and devices without considering in detail the various fabrication processes; this important subject is left to other books. However, there is one MOS technology nea29583_ch10_371-442.indd 427 12/11/10 12:40 PM 428 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor that is used extensively, for which the basic fabrication techniques must be considered in order to understand essential characteristics of these devices and circuits. The MOS technology we consider briefly is the complementary MOS, or CMOS, process. We have considered the physics of both n-channel and p-channel enhancement mode MOSFETs. Both devices are used in a CMOS inverter, which is the basis of CMOS digital logic circuits. The dc power dissipation in a digital circuit can be reduced to very low levels by using a complementary p-channel and n-channel pair. It is necessary to form electrically isolated p- and n-substrate regions in an integrated circuit to accommodate the n- and p-channel transistors. The p-well process has been a commonly used technique for CMOS circuits. The process starts with a fairly low doped n-type silicon substrate in which the p-channel MOSFET will be fabricated. A diffused p region, called a p well, is formed in which the n-channel MOSFET will be fabricated. In most cases, the p-type substrate doping level must be larger than the n-type substrate doping level to obtain the desired threshold voltages. The larger p doping can easily compensate the initial n doping to form the p well. A simplified cross section of the p-well CMOS structure is shown in Figure 10.58a. The notation FOX stands for field oxide, which is a relatively thick oxide separating the devices. The FOX prevents either the n or p substrate from becoming inverted and helps maintain isolation between the two devices. In practice, additional processing steps must be included; for example, providing connections so that the p well and n substrate can be electrically connected to the appropriate voltages. The n substrate Poly-Si gate FOX n n Poly-Si gate FOX p FOX p FOX n FOX n p well p p FOX n well n substrate p substrate (a) (b) Poly-Si gate FOX n n FOX p well p p FOX n well p or n substrate (c) Figure 10.58 | CMOS structures: (a) p well, (b) n well, and (c) twin well. (From Yang [22].) nea29583_ch10_371-442.indd 428 12/11/10 12:40 PM 10.5 The CMOS Technology 429 must always be at a higher potential than the p well; therefore, this pn junction will always be reverse biased. With ion implantation now being extensively used for threshold voltage control, both the n-well CMOS process and twin-well CMOS process can be used. The n-well CMOS process, shown in Figure 10.58b, starts with an optimized p-type substrate that is used to form the n-channel MOSFETs. (The n-channel MOSFETs, in general, have superior characteristics, so this starting point should yield excellent n-channel devices.) The n well is then added, in which the p-channel devices are fabricated. The n-well doping can be controlled by ion implantation. The twin-well CMOS process, shown in Figure 10.58c, allows both the p-well and n-well regions to be optimally doped to control the threshold voltage and transconductance of each transistor. The twin-well process allows a higher packing density because of self-aligned channel stops. One major problem in CMOS circuits has been latch-up. Latch-up refers to a high-current, low-voltage condition that may occur in a four-layer pnpn structure. Figure 10.59a shows the circuit of a CMOS inverter and Figure 10.59b shows a simplified integrated circuit layout of the inverter circuit. In the CMOS layout, p source to n substrate to p well to n source forms such a four-layer structure. The equivalent circuit of this four-layer structure is shown in Figure 10.60. The silicon-controlled rectifier action involves the interaction of the parasitic pnp and npn bipolar transistors. Bipolar transistors are discussed in Chapter 12. The npn transistor corresponds to the vertical n-source to p-well to n-substrate structure and the pnp transistor corresponds to the lateral p-well to n-substrate to p-source structure. Under normal CMOS operation, both parasitic bipolar transistors are cut off. However, under certain conditions, avalanche breakdown may occur in the p-well to nsubstrate junction, driving both bipolar transistors into saturation. This high-current, low-voltage condition—latch-up—can sustain itself by positive feedback. The condition can prevent the CMOS circuit from operating and can also cause permanent damage and burnout of the circuit. Latch-up can be prevented if the product n p is less than unity at all times, where n and p are the common-emitter current gains of the npn and pnp parasitic VDD S p channel Input D Input Output Output D n channel S VDD S n D D p n S p p well n substrate (a) (b) Figure 10.59 | (a) CMOS inverter circuit. (b) Simplified integrated circuit cross section of CMOS inverter. nea29583_ch10_371-442.indd 429 12/11/10 12:40 PM 430 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor VA IA VA IA p p IB1 IC2 n n n p p p n IC1 IB2 n IK IK (a) (b) Figure 10.60 | (a) The splitting of the basic pnpn structure. (b) The two-transistor equivalent circuit of the four-layered pnpn device. bipolar transistors, respectively. One method of preventing latch-up is to “kill” the minority carrier lifetime. Minority carrier lifetime degradation can be accomplished by gold doping or neutron irradiation, either of which introduces deep traps within the semiconductor. The deep traps increase the excess minority carrier recombination rate and reduce current gain. A second method of preventing latch-up is by using proper circuit layout techniques. If the two bipolar transistors can be effectively decoupled, then latch-up can be minimized or prevented. The two parasitic bipolar transistors can also be decoupled by using a different fabrication technology. The silicon-on-insulator technology, for example, allows the n-channel and the p-channel MOSFETs to be isolated from each other by an insulator. This isolation decouples the parasitic bipolar transistors. 10.6 | SUMMARY ■ ■ ■ ■ nea29583_ch10_371-442.indd 430 The fundamental physics and characteristics of the metal-oxide–semiconductor fieldeffect transistor (MOSFET) have been considered in this chapter. The heart of the MOSFET is the MOS capacitor. The energy bands in the semiconductor adjacent to the oxide–semiconductor interface bend, depending upon the voltage applied to the gate. An inversion layer of electrons can be created at the oxide–semiconductor surface in a p-type semiconductor by applying a sufficiently positive gate voltage, and an inversion layer of holes can be created at the oxide–semiconductor surface in an n-type semiconductor by applying a sufficiently negative gate voltage. The threshold voltage is the applied gate voltage required to reach the threshold inversion point. The flat-band voltage was defined and discussed. 12/11/10 12:40 PM Glossary of Important Terms ■ ■ ■ ■ ■ ■ ■ 431 The n-channel MOSFET, both enhancement mode and depletion mode, and the p-channel MOSFET, both enhancement mode and depletion mode, were described. The basic transistor action is the modulation of the current at the drain terminal by the gate-to-source voltage. The ideal MOSFET current–voltage relations were derived. The body-effect coefficient was defined and discussed. The expression for the shift in threshold voltage due to the body effect was derived. A small-signal equivalent circuit of the MOSFET was developed. Various physical factors in the MOSFET that affect the frequency limitations were discussed. An expression for the cutoff frequency was developed. The CMOS technology was briefly considered. GLOSSARY OF IMPORTANT TERMS accumulation layer charge The induced charge directly under an oxide that is in excess of the thermal-equilibrium majority carrier concentration. channel conductance The ratio of drain current to drain-to-source voltage in the limit as VDS → 0. channel conductance modulation The process whereby the channel conductance varies with gate-to-source voltage. CMOS Complementary MOS; the technology that uses both p- and n-channel devices in an electronic circuit fabricated in a single semiconductor chip. conduction parameter The multiplying coefficient of the voltage terms to obtain the MOSFET drain current. cutoff frequency The signal frequency at which the input ac gate current is equal to the output ac drain current. depletion mode MOSFET The type of MOSFET in which a gate voltage must be applied to turn the device off. enhancement mode MOSFET The type of MOSFET in which a gate voltage must be applied to turn the device on. equivalent fixed oxide charge The effective fixed charge in the oxide, Qss, directly adjacent to the oxide–semiconductor interface. field-effect The phenomenon by which an electric field perpendicular to the surface of a semiconductor can modulate the conductance. flat-band voltage The gate voltage that must be applied to create the flat-band condition in which there is no space charge region in the semiconductor under the oxide. interface states The allowed electronic energy states within the bandgap energy at the oxide–semiconductor interface. inversion layer charge The induced charge directly under the oxide, which is the opposite type compared with the semiconductor doping. inversion layer mobility The mobility of carriers in the inversion layer. metal–semiconductor work function difference The parameter ms, a function of the difference between the metal work function and semiconductor electron affinity. oxide capacitance The ratio of oxide permittivity to oxide thickness, which is the capacitance per unit area, Cox. nea29583_ch10_371-442.indd 431 12/11/10 12:40 PM 432 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor process conduction parameter The product of carrier mobility and oxide capacitance. saturation The condition in which the inversion charge density is zero at the drain and the drain current is no longer a function of the drain-to-source voltage. strong inversion The condition in which the inversion charge density is larger than the magnitude of the semiconductor doping concentration. threshold inversion point The condition in which the inversion charge density is equal in magnitude to the semiconductor doping concentration. threshold voltage The gate voltage that must be applied to achieve the threshold inversion point. transconductance The ratio of an incremental change in drain current to the corresponding incremental change in gate voltage. weak inversion The condition in which the inversion charge density is less than the magnitude of the semiconductor doping concentration. CHECKPOINT After studying this chapter, the reader should have the ability to: ■ ■ ■ ■ ■ ■ ■ ■ ■ ■ ■ ■ ■ ■ ■ ■ Sketch the energy-band diagrams in the semiconductor of the MOS capacitor under various bias conditions. Describe the process by which an inversion layer of charge is created in a MOS capacitor. Discuss the reason the space charge width reaches a maximum value once the inversion layer is formed. Discuss what is meant by the metal–semiconductor work function difference and why this value is different between aluminum, n polysilicon, and p polysilicon gates. Describe what is meant by flat-band voltage. Define threshold voltage. Sketch the C–V characteristics of a MOS capacitor with p-type and n-type semiconductor substrates under high-frequency and low-frequency conditions. Discuss the effects of fixed trapped oxide charge and interface states on the C–V characteristics. Sketch the cross sections of n-channel and p-channel MOSFET structures. Explain the basic operation of the MOSFET. Discuss the I–V characteristics of the MOSFET when biased in the nonsaturation and saturation regions. Describe the substrate bias effects on the threshold voltage. Sketch the small-signal equivalent circuit, including capacitances, of the MOSFET, and explain the physical origin of each capacitance. Discuss the condition that defines the cutoff frequency of a MOSFET. Sketch the cross section of a CMOS structure. Discuss what is meant by latch-up in a CMOS structure. REVIEW QUESTIONS 1. Sketch the energy-band diagrams in a MOS capacitor with an n-type substrate in accumulation, depletion, and inversion modes. 2. Describe what is meant by an inversion layer of charge. Describe how an inversion layer of charge can be formed in a MOS capacitor with a p-type substrate. nea29583_ch10_371-442.indd 432 12/11/10 12:40 PM Problems 433 3. Why does the space charge region in the semiconductor of a MOS capacitor reach a maximum width once the inversion layer is formed? 4. Define surface potential. Does the surface potential change significantly with gate voltage once threshold is reached? 5. Sketch the energy-band diagram through a MOS structure with a p-type substrate and an n polysilicon gate under zero bias. 6. Define the flat-band voltage. Sketch the energy-band diagram in a MOS capacitor at flat band. 7. Define the threshold voltage. What is the surface potential at the threshold voltage? 8. Sketch the C–V characteristics of a MOS capacitor with an n-type substrate under the low-frequency condition. How do the characteristics change for the high-frequency condition? 9. Indicate the approximate capacitance at flat band on the C–V characteristic of a MOS capacitor with a p-type substrate under the high-frequency condition. 10. What is the effect on the C–V characteristics of a MOS capacitor with a p-type substrate if the amount of positive trapped oxide charge increases? 11. Qualitatively sketch the inversion charge density in the channel region when the transistor is biased in the nonsaturation region. Repeat for the case when the transistor is biased in the saturation region. 12. Define VDS(sat). 13. Define enhancement mode and depletion mode for both n-channel and p-channel devices. 14. Sketch the charge distribution through a MOS capacitor with a p-type substrate when biased in the inversion mode. Write the charge neutrality equation. 15. Discuss why the threshold voltage changes when a reverse-biased source-to-substrate voltage is applied to a MOSFET. PROBLEMS (Note: In the following problems, assume the semiconductor and oxide in the MOS system are silicon and silicon dioxide, respectively, and assume the temperature is T 300 K unless otherwise stated. Use Figure 10.16 to determine the metal–semiconductor work function difference.) Section 10.1 The Two-Terminal MOS Structure 10.1 10.2 10.3 The dc charge distributions of four ideal MOS capacitors are shown in Figure P10.1. For each case: (a) Is the semiconductor n or p type? (b) Is the device biased in the accumulation, depletion, or inversion mode? (c) Draw the energyband diagram in the semiconductor region. (a) Calculate the maximum space charge width xdT and the maximum space charge density Q SD (max) in a MOS capacitor with a p-type silicon substrate at T 300 K for doping concentrations of (i) Na 7 1015 cm3 and (ii) Na 3 1016 cm3. (b) Repeat part (a) for T 350 K. (a) Consider a MOS capacitor at T 300 K with an n-type silicon substrate. Determine the silicon doping concentration such that Q SD (max) 1.25 108 C/cm2. (b) What is the surface potential that results in the maximum space charge width? nea29583_ch10_371-442.indd 433 12/11/10 12:40 PM 434 CHAPTER 10 M Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor O S M O (a) M O S (b) S (c) M O S (d) Figure P10.1 | Figure for Problem 10.1. 10.4 10.5 10.6 10.7 10.8 nea29583_ch10_371-442.indd 434 Determine the metal–semiconductor work function difference ms in a MOS structure with p-type silicon for the case when the gate is (a) aluminum, (b) n polysilicon, and (c) p polysilicon. Let Na 6 1015 cm3. The silicon impurity doping concentration in an aluminum–silicon dioxide-silicon MOS device is Na 4 1016 cm3. Using the parameters in Example 10.2, determine the metal–semiconductor work function difference ms. Consider a MOS capacitor with an n-type silicon substrate. A metal–semiconductor work function difference of ms 0.30 V is required. Determine the silicon doping concentration required to meet this specification when the gate is (a) n polysilicon, (b) p polysilicon, and (c) aluminum. If a particular gate cannot meet this specification, explain why. (a) Consider the MOS capacitor described in Problem 10.5. For an oxide thickness of tox 20 nm 200 Å and an oxide charge of Q ss 5 1010 cm2, calculate the flat-band voltage. (b) Repeat part (a) for an oxide thickness of tox 8 nm 80 Å. (a) Consider an n polysilicon–silicon dioxide–n-type silicon MOS structure. Let Nd 4 1015 cm3. Calculate the ideal flat-band voltage for tox 20 nm 200 Å. (b) Considering the results of part (a), determine the shift in flat-band voltage for (i) Q ss 4 1010 cm2 and (ii) Q ss 1011 cm2. (c) Repeat parts (a) and (b) for an oxide thickness of tox 12 nm 120 Å. 12/11/10 12:40 PM Problems 10.9 10.10 10.11 10.12 10.13 10.14 10.15 10.16 10.17 10.18 *10.19 *10.20 435 Consider an aluminum gate–silicon dioxide–p-type silicon MOS structure with tox 450 Å. The silicon doping is Na 2 1016 cm3 and the flat-band voltage is VFB 1.0 V. Determine the fixed oxide charge Q ss . Consider a MOS device with a p-type silicon substrate with Na 2 1016 cm3. The oxide thickness is tox 15 nm 150 Å and the equivalent oxide charge is Q ss 7 1010 cm2. Calculate the threshold voltage for (a) an n polysilicon gate, (b) a p polysilicon gate, and (c) an aluminum gate. Repeat Problem 10.10 for an n-type silicon substrate with a doping of Nd 3 1015 cm3. A 400-Å oxide is grown on p-type silicon with Na 5 1015 cm3. The flat-band voltage is 0.9 V. Calculate the surface potential at the threshold inversion point as well as the threshold voltage assuming negligible oxide charge. Also find the maximum space charge width for this device. A MOS device with an aluminum gate is fabricated on a p-type silicon substrate. The oxide thickness is tox 22 nm 220 Å and the trapped oxide charge is Q ss 4 1010 cm2. The measured threshold voltage is VT 0.45 V. Determine the p-type doping concentration. Consider a MOS device with the following parameters: p polysilicon gate, n-type silicon substrate, tox 18 nm 180 Å, and Q ss 4 1010 cm2. Determine the silicon doping concentration such that the threshold voltage is in the range 0.35 VTP 0.25 V. Repeat Problem 10.13 for an n-type silicon substrate if the measured threshold voltage is VT 0.975 V. Determine the n-type doping concentration. An n polysilicon gate–silicon dioxide–silicon MOS capacitor has an oxide thickness of tox 18 nm 180 Å and a doping of Na 1015 cm3. The oxide charge density is Qss 6 1010 cm2. Calculate the (a) flat-band voltage and (b) threshold voltage. An n-channel depletion mode MOSFET with an n polysilicon gate is shown in Figure 10.41. The n-channel doping is Nd 1015 cm3 and the oxide thickness is tox 500 Å. The equivalent fixed oxide charge is Q ss 1010 cm2. The n-channel thickness tc is equal to the maximum induced space charge width. (Disregard the space charge region at the n-channel–p-substrate junction.) (a) Determine the channel thickness tc and (b) calculate the threshold voltage. Consider a MOS capacitor with an n polysilicon gate and n-type silicon substrate. Assume Na 1016 cm3 and let EF Ec 0.2 eV in the n polysilicon. Assume the oxide has a thickness of tox 300 Å. Also assume that (polysilicon) (singlecrystal silicon). (a) Sketch the energy-band diagrams (i) for VG 0 and (ii) at flat band. (b) Calculate the metal–semiconductor work function difference. (c) Calculate the threshold voltage for the ideal case of zero fixed oxide charge and zero interface states. The threshold voltage of an n-channel MOSFET is given by Equation (10.31a). Plot VT versus temperature over the range 200 T 450 K. Consider both an aluminum gate and an n polysilicon gate. Assume the work functions are independent of temperature and use device parameters similar to those in Example 10.4. Plot the threshold voltage of an n-channel MOSFET versus p-type substrate doping concentration similar to Figure 10.21. Consider both n and p polysilicon gates. Use reasonable device parameters. *Asterisks next to problems indicate problems that are more difficult. nea29583_ch10_371-442.indd 435 12/11/10 12:40 PM 436 CHAPTER 10 *10.21 10.22 Plot the threshold voltage of a p-channel MOSFET versus n-type substrate doping concentration similar to Figure 10.22. Consider both n and p polysilicon gates. Use reasonable device parameters. Consider an NMOS device with the parameters given in Problem 10.12. Plot VT versus tox over the range 20 tox 500 Å. Section 10.2 10.23 10.24 *10.25 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Capacitance–Voltage Characteristics An ideal MOS capacitor with an n polysilicon gate has a silicon dioxide thickness of tox 12 nm 120 Å on a p-type silicon substrate doped at Na 1016 cm3. Determine the capacitance Cox, CFB, Cmin, and C(inv) at (a) f 1 Hz and (b) f 1 MHz. (c) Determine VFB and VT. (d) Sketch CCox versus VG for parts (a) and (b). Repeat Problem 10.23 for an ideal MOS capacitor with a p polysilicon gate and an n-type silicon substrate doped at Nd 5 1014 cm3. Using superposition, show that the shift in the flat-band voltage due to a fixed charge distribution (x) in the oxide is given by t x (x) 1 _ VFB _ dx Cox 0 tox ox 10.26 10.27 10.28 10.29 Using the results of Problem 10.25, calculate the shift in flat-band voltage for tox 20 nm 200 Å for the following oxide charge distributions: (a) Q ss 8 1010 cm2 is entirely located at the oxide–semiconductor interface, (b) Q ss 8 1010 cm2 is uniformly distributed throughout the oxide, and (c) Q ss 8 1010 cm2 forms a triangular distribution with the peak at the oxide– semiconductor interface and is zero at the metal–oxide interface. An ideal MOS capacitor is fabricated by using intrinsic silicon and an n polysilicon gate. (a) Sketch the energy-band diagram through the MOS structure under flat-band conditions. (b) Sketch the low-frequency C–V characteristics from negative to positive gate voltage. Consider a MOS capacitor with a p-type substrate. Assume that donor-type interface traps exist only at midgap (i.e., at EFi). Sketch the high-frequency C–V curve from accumulation to inversion. Compare this sketch to the ideal C–V plot. Consider an SOS capacitor as shown in Figure P10.29. Assume the SiO2 is ideal (no trapped charge) and has a thickness of tox 500 Å. The doping concentrations are Nd 1016 cm3 and Na 1016 cm3. (a) Sketch the energy-band diagram through the device for (i) flat band, (ii) VG 3 V, and (iii) VG 3 V. (b) Calculate the flat-band voltage. (c) Estimate the voltage across the oxide for (i) VG 3 V and (ii) VG 3 V. (d) Sketch the high-frequency C–V characteristic curve. tox VG n type SiO2 p type Figure P10.29 | Figure for Problem 10.29. nea29583_ch10_371-442.indd 436 12/11/10 12:40 PM Problems 437 C (pF) 200 CFB 20 VFB 0 0.8 V VG Figure P10.30 | Figure for Problem 10.30. C 5 4 3 1 2 0 VG Figure P10.31 | Figure for Problem 10.31. 10.30 10.31 The high-frequency C–V characteristic curve of a MOS capacitor is shown in Figure P10.30. The area of the device is 2 103 cm2. The metal–semiconductor work function difference is ms 0.50 V, the oxide is SiO2, the semiconductor is silicon, and the semiconductor doping concentration is 2 1016 cm3. (a) Is the semiconductor n or p type? (b) What is the oxide thickness? (c) What is the equivalent trapped oxide charge density? (d) Determine the flat-band capacitance. Consider the high-frequency C–V plot shown in Figure P10.31. (a) Indicate which points correspond to flat-band, inversion, accumulation, threshold, and depletion modes. (b) Sketch the energy-band diagram in the semiconductor for each condition. Section 10.3 The Basic MOSFET Operation 10.32 An expression that includes the inversion charge density is given by Equation (10.59). Consider the definition of threshold voltage and show that the inversion charge density goes to zero at the drain terminal at saturation. (Hint: Let Vx VDS VDS(sat).) nea29583_ch10_371-442.indd 437 12/11/10 12:40 PM 438 CHAPTER 10 10.33 10.34 10.35 10.36 10.37 10.38 10.39 10.40 10.41 10.42 10.43 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Consider an n-channel MOSFET with the following parameters: k n 0.18 mA/V2, WL 8, and VT 0.4 V. Determine the drain current ID for (a) VGS 0.8 V, VDS 0.2 V; (b) VGS 0.8 V, VDS 1.2 V; (c) VGS 0.8 V, VDS 2.5 V; and (d) VGS 1.2 V, VDS 2.5 V. A p-channel MOSFET has the following parameters: kp 0.10 mA/V2, WL 15, and VT 0.4 V. Calculate the drain current ID for (a) VSG 0.8 V, VSD 0.25 V; (b) VSG 0.8 V, VSD 1.0 V; (c) VSG 1.2 V, VSD 1.0 V; and (d) VSG 1.2 V, VSD 2.0 V. The parameters of an n-channel MOSFET are kn 0.6 mA/V2 and VT 0.8 V. The drain current is 1 mA with applied voltages of VGS 1.4 V, VSB 0, and VDS 4 V. (a) What is the WL value? (b) What is the value of ID for VGS 1.85 V, VSB 0, and VDS 6 V? (c) Determine the value of ID for VGS 1.2 V, VSB 0, and VDS 0.15 V. Consider a p-channel MOSFET with the following parameters: kp 0.12 mA/V2 and WL 20. The drain current is 100 A with applied voltages of VSG 0, VBS 0, and VSD 1.0 V. (a) Determine the VT value. (b) Determine the drain current ID for VSG 0.4 V, VSB 0, and VSD 1.5 V. (c) What is the value of ID for VSG 0.6 V, VSB 0, and VSD 0.15 V? An ideal n-channel MOSFET has the following parameters: VT 0.45 V, n 425 cm2/V-s, tox 11 nm 110 Å, W 20 m, and L 1.2 m. (a) Plot ID versus VDS for 0 VDS 3 V and for VGS______ 0, 0.6, 1.2, 1.8, and 2.4 V. Indicate on each curve the VDS (sat) point. (b) Plot ID (sat) versus VGS for 0 VGS 2.4 V. (c) Plot ID versus VGS for 0 VGS 2.4 V and for VDS 0.1 V. Consider an ideal p-channel MOSFET with the following parameters: VT 0.35 V, p 210 cm2/V-s, tox 11 nm 110 Å, W 35 m, and L 1.2 m. (a) Plot ID versus VSD for 0 VSD 3 V and for VSG______ 0, 0.6, 1.2, 1.8, and 2.4 V. Indicate on each curve the VSD (sat) point. (b) Plot ID (sat) versus VSG for 0 VSG 2.4 V. (c) Plot ID versus VSG for 0 VSG 2.4 V and for VSD 0.1 V. Consider an n-channel MOSFET with the same parameters as described in Problem 10.37 except that VT 0.8 V. (a) Plot______ ID versus VDS for 0 VDS 3 V and for VGS 0.8, 0, 0.8, and 1.6 V. (b) Plot ID (sat) versus VGS for 0.8 VGS 1.6 V. Consider an n-channel enhancement mode MOSFET biased as shown in Figure P10.40. Sketch the current–voltage characteristics, ID versus VDS, for (a) VGD 0, (b) VGD VT2, and (c) VGD 2VT. Figure P10.41 shows the cross section of an NMOS device that includes source and drain resistances. These resistances take into account the bulk n semiconductor resistance and the ohmic contact resistance. The current–voltage relations can be generated by replacing VGS by VGIDRS and VDS by VDID(RS RD) in the ideal equations. Assume transistor parameters of VT 1 V and Kn 1 mA/V2. (a) Plot the following curves on the same graph: ID versus VD for VG 2 V and VG 3 V over the range 0 VD 5 V for (i ) RS RD 0 and __ (ii) RS RD 1 k. (b) Plot the following curves on the same graph: ID versus VG for VD 0.1 V and VD 5 V over the range 0 ID 1 mA for (i) RS RD 0 and (ii) RS RD 1 k. An n-channel MOSFET has the same parameters as given in Problem 10.37. The gate terminal is connected to the drain terminal. Plot ID versus VDS for 0 VDS 5 V. Determine the range of VDS over which the transistor is biased in the nonsaturation and saturation regions. The channel conductance for a p-channel MOSFET is defined as ID gd _ VSD nea29583_ch10_371-442.indd 438 VSD→0 12/11/10 12:40 PM Problems VD VG S 439 VGD G S D VDS G ID Channel D n RD RS n p type p type Figure P10.40 | Figure for Problem 10.40. 10.44 10.45 10.46 Figure P10.41 | Figure for Problem 10.41. Plot the channel conductance for the p-channel MOSFET described in Problem 10.38 for 0 VSG 2.4. The transconductance of an n-channel MOSFET is found to be gm ID VGS 1.25 mA/V when measured at VDS 50 mV. The threshold voltage is VT 0.3 V. (a) Determine the conductance parameter Kn. (b) What is the current at VGS 0.8 V and VDS 50 mV? (c) Determine the current at VGS 0.8 V and VDS 1.5 V. The experimental characteristics of an ideal n-channel MOSFET biased in the saturation region are shown in Figure P10.45. If WL 10 and tox 425 Å, determine VT and n. One curve of an n-channel MOSFET is characterized by the following parameters: ID (sat) 2 104 A, VDS (sat) 4 V, and VT 0.8 V. (a) What is the gate voltage? (b) What is the value of the conduction parameter? (c) If VG 2 V and VDS 2 V, determine ID. (d) If VG 3 V and VDS 1 V, determine ID. (e) For each of the conditions given in (c) and (d), sketch the inversion charge density and depletion region through the channel. 0.05 ID (A12) 0.04 0.03 0.02 0.01 0 1 VGS (V) 2 3 Figure P10.45 | Figure for Problem 10.45. nea29583_ch10_371-442.indd 439 12/11/10 12:40 PM 440 CHAPTER 10 10.47 10.48 10.49 10.50 10.51 10.52 10.53 10.54 (a) An ideal n-channel MOSFET has parameters tox 18 nm 180 Å, n 450 cm2/V-s, and VT 0.4 V. The measured current in the saturation region is ID (sat) 0.8 mA when biased at VGS 2.0 V. Determine the (i) process conduction parameter and (ii) width-to-length ratio. (b) An ideal p-channel MOSFET has the same oxide thickness as given in part (a), a mobility of p 210 cm2/V-s, and a threshold voltage of VT 0.4 V. The measured current in the saturation region is also ID (sat) 0.8 mA when biased at VSG 2.0 V. Determine the (i) process conduction parameter and (ii) width-to-length ratio. Consider the n-channel MOSFET described in Problem 10.37. (a) Calculate gmL for VDS 0.10 V. (b) Find gms for VGS 1.5 V. Consider the p-channel MOSFET described in Problem 10.38. (a) Calculate gmL for VSD 0.10 V. (b) Find gms for VSG 1.5 V. An n-channel MOSFET has the following parameters: Na 5 1016 cm3, tox 15 nm 150 Å, n 450 cm2/V-s, VFB 0.5 V, L 1.2 m, and W 8 m. ______ (a) Determine the body-effect coefficient. (b) Plot ID (sat) versus VGS over the range 0 ID 0.5 mA for source-to-body voltages of (i) VSB 0, (ii) VSB 1 V, (iii) VSB 2 V, and (iv) VSB 4 V. (c) What are the threshold voltages for the conditions given in part (b)? The substrate doping and body-effect coefficient of an n-channel MOSFET are Na 1016 cm3 and 0.12 V12, respectively. The threshold voltage is found to be VT 0.5 V when biased at VSB 2.5 V. What is the threshold voltage at VSB 0? A p-channel MOSFET has an oxide thickness of tox 20 nm 200 Å and a substrate doping of Nd 5 1015 cm3. (a) Find the body-effect coefficient. (b) Determine the body-to-source voltage, VBS, such that the shift in threshold voltage, VT, from the VBS 0 curve is VT 0.22 V. An NMOS device has the following parameters: n poly gate, tox 400 Å, Na 1015 cm3, and Qss 5 1010 cm2. (a) Determine VT. (b) Is it possible to apply a VSB voltage such that VT 0? If so, what is the value of VSB? Investigate the threshold voltage shift due to substrate bias. The threshold shift is given by Equation (10.81). Plot VT versus VSB over the range 0 VSB 5 V for several values of Na and tox. Determine the conditions for which VT is limited to a maximum value of 0.7 V over the range of VSB. Section 10.4 10.55 10.56 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor Frequency Limitations Consider an ideal n-channel MOSFET with a width-to-length ratio of (WL) 10, an electron mobility of n 400 cm2 /V-s, an oxide thickness of tox 475 Å, and a threshold voltage of VT 0.65 V. (a) Determine the maximum value of source resistance so that the saturation transconductance gms is reduced by no more than 20 percent from its ideal value when VGS 5 V. (b) Using the value of rs calculated in part (a), how much is gms reduced from its ideal value when VGS 3 V? An n-channel MOSFET has the following parameters: n 400 cm2 /V-s L 2 m VT 0.75 V nea29583_ch10_371-442.indd 440 tox 500 Å W 20 m 12/11/10 12:40 PM Reading List 10.57 441 Assume the transistor is biased in the saturation region at VGS 4 V. (a) Calculate the ideal cutoff frequency. (b) Assume that the gate oxide overlaps both the source and drain contacts by 0.75 m. If a load resistance of RL 10 k is connected to the output, calculate the cutoff frequency. Repeat Problem 10.56 for the case when the electrons are traveling at a saturation velocity of vsat 4 106 cm /s. Summary and Review *10.58 *10.59 *10.60 *10.61 Design an ideal silicon n-channel MOSFET with a polysilicon gate to have a threshold voltage of VT 0.65 V. Assume an oxide thickness of tox 300 Å, a channel length of L 1.25 m, and a nominal value of Q ss 1.5 1011 cm2. It is desired to have a drain current of ID 50 A at VGS 2.5 V and VDS 0.1 V. Determine the substrate doping concentration, channel width, and type of gate required. Design an ideal silicon n-channel depletion mode MOSFET with a polysilicon gate to have a threshold voltage of VT 0.65 V. Assume an oxide thickness of tox 300 Å, a channel length of L 1.25 m, and a nominal value of Q ss 1.5 1011 cm2. It is desired to have a drain current of ID (sat) 50 A at VGS 0. Determine the type of gate, substrate doping concentration, and channel width required. Consider the CMOS inverter circuit shown in Figure 10.59a. Ideal n- and p-channel devices are to be designed with channel lengths of L 2.5 m and oxide thicknesses of tox 450 Å. Assume the inversion channel mobilities are one-half the bulk values. The threshold voltages of the n- and p-channel transistors are to be 0.5 V and 0.5 V, respectively. The drain current is to be ID 0.256 mA when the input voltage to the inverter is 1.5 V and 3.5 V with VDD 5 V. The gate material is to be the same in each device. Determine the type of gate, substrate doping concentrations, and channel widths. A complementary pair of ideal n-channel and p-channel MOSFETs is to be designed to produce the same I–V characteristics when they are equivalently biased. The devices are to have the same oxide thickness of 250 Å and the same channel length of L 2 m. Assume the SiO2 layer is ideal. The n-channel device is to have a channel width of W 20 m. Assume constant inversion layer mobilities of n 600 cm2 /V-s and p 220 cm2 /V-s. (a) Determine p-type and n-type substrate doping concentrations. (b) What are the threshold voltages? (c) What is the width of the p-channel device? READING LIST Dimitrijev, S. Principles of Semiconductor Devices. New York: Oxford University, 2006. 2. Hu, C. C. Modern Semiconductor Devices for Integrated Cicuits. Upper Saddle River, NJ: Pearson Prentice Hall, 2010. 3. Kano, K. Semiconductor Devices. Upper Saddle River, NJ: Prentice Hall, 1998. 4. Muller, R. S., and T. I. Kamins. Device Electronics for Integrated Circuits. 2nd ed. New York: Wiley, 1986. 1. nea29583_ch10_371-442.indd 441 12/11/10 12:40 PM 442 CHAPTER 10 Fundamentals of the Metal–Oxide–Semiconductor Field-Effect Transistor 5. Ng, K. K. Complete Guide to Semiconductor Devices. New York: McGraw-Hill, 1995. 6. Nicollian, E. H., and J. R. Brews. MOS Physics and Technology. New York: Wiley, 1982. 7. Ong, D. G. Modern MOS Technology: Processes, Devices, and Design. New York: McGraw-Hill, 1984. 8. Pierret, R. F. Semiconductor Device Fundamentals. Reading, MA: Addison-Wesley, 1996. 9. Roulston, D. J. An Introduction to the Physics of Semiconductor Devices. New York: Oxford University Press, 1999. 10. Schroder, D. K. Advanced MOS Devices, Modular Series on Solid State Devices. Reading, MA: Addison-Wesley, 1987. 11. Shur, M. Introduction to Electronic Devices. New York: John Wiley & Sons, Inc., 1996. *12. _______ Physics of Semiconductor Devices. Englewood Cliffs, NJ: Prentice Hall, 1990. 13. Singh, J. Semiconductor Devices: An Introduction. New York: McGraw-Hill, 1994. 14. _______ Semiconductor Devices: Basic Principles. New York: Wiley, 2001. 15. Streetman, B. G., and S. K. Banerjee. Solid State Electronic Devices. 6th ed. Upper Saddle River, NJ: Pearson Prentice Hall, 2006. 16. Sze, S. M. High-Speed Semiconductor Devices. New York: Wiley, 1990. 17. Sze, S. M. and K. K. Ng. Physics of Semiconductor Devices, 3rd ed. Hoboken, NJ: John Wiley & Sons, Inc., 2007. 18. Taur, Y. and T. H. Ning. Fundamentals of Modern VLSI Devices, 2nd ed. Cambridge University Press, 2009. *19. Tsividis, Y. Operation and Modeling of the MOS Transistor. 2nd ed. Burr Ridge, IL: McGraw-Hill, 1999. 20. Werner, W. M. “The Work Function Difference of the MOS System with Aluminum Field Plates and Polycrystalline Silicon Field Plates.” Solid State Electronics 17, (1974), pp. 769–775. 21. Yamaguchi, T., S. Morimoto, G. H. Kawamoto, and J. C. DeLacy. “Process and Device Performance of 1 m-Channel n-Well CMOS Technology.” IEEE Transactions on Electron Devices ED-31 (February 1984), pp. 205–214. 22. Yang, E. S. Microelectronic Devices. New York: McGraw-Hill, 1988. *Indicates references that are at an advanced level compared to this text. nea29583_ch10_371-442.indd 442 12/11/10 12:40 PM 11 C H A P T E R Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts I n this chapter we present additional concepts that are commonly encountered in metal–oxide–semiconductor field-effect transistors (MOSFETs). These concepts include nonideal effects, small device geometry, breakdown, threshold voltage adjustment by ion implantation, and radiation effects. Although there are a multitude of details that become important when fabricating MOSFETs in ICs, we are able to consider only a few here. Many additional details can be found in more advanced texts. ■ 11.0 | PREVIEW In this chapter, we will: ■ Describe and analyze subthreshold conduction, which is the phenomenon whereby current is induced in the channel before the defined threshold voltage is reached. ■ Analyze channel length modulation, which is a characteristic of short-channel lengths and leads to a finite output resistance. ■ Consider the effects of a decrease in carrier mobility due to increasing gate voltage. ■ Analyze the effects of carrier saturation velocity. Carriers can easily reach their saturation velocity in short-channel devices. ■ Discuss MOSFET scaling, which describes how various parameters must be changed as device size is decreased. ■ Consider the deviations in threshold voltage due to small geometry devices, including short channel length devices and small channel width devices. 443 nea29583_ch11_443-490.indd 443 12/11/10 12:42 PM 444 CHAPTER 11 ■ ■ ■ Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts Describe and analyze various voltage breakdown mechanisms in MOSFETs. Describe and analyze the technique of threshold voltage adjustment by ion implantation. Consider the introduction of trapped oxide charges by ionizing radiation and hot electron effects. 11.1 | NONIDEAL EFFECTS As with any semiconductor device, the experimental characteristics of MOSFETs deviate to some degree from the ideal relations that have been theoretically derived using the various assumptions and approximations. In this section, we consider five effects that cause deviations from the assumptions used in the ideal derivations. These effects are subthreshold conduction, channel length modulation, mobility variations, velocity saturation, and ballistic transport. 11.1.1 Subthreshold Conduction The ideal current–voltage relationship predicts zero drain current when the gate-tosource voltage is less than or equal to the threshold voltage. Experimentally, ID is not zero when VGS VT. Figure 11.1 shows a comparison between the ideal characteristic that was derived, and the experimental results. The drain current, which exists for VGS VT, is known as the subthreshold current. Figure 11.2 shows the energy-band diagram of an MOS structure with a p-type substrate biased so that s 2fp. At the same time, the Fermi level is closer to the conduction band than the valence band, so the semiconductor surface develops the ID Ec Experimental es Ideal VT VGS Figure 11.1 | Comparison of__ ideal and experimental plots of ID versus VGS. nea29583_ch11_443-490.indd 444 efpEFi EF Ev Figure 11.2 | Energy-band diagram when fp s 2fp. 12/11/10 12:42 PM 11.1 Gate VDS S D n n p Nonideal Effects 0 p 2p Vbi e (a) (b) 0 0 p 2p Vbi 445 p e 2p Vbi (c) e (d) Figure 11.3 | (a) Cross section along channel length of n-channel MOSFET. Energy-band diagrams along channel length at (b) accumulation, (c) weak inversion, and (d) inversion. characteristics of a lightly doped n-type material. We would expect, then, to observe some conduction between the n source and drain contacts through this weakly inverted channel. The condition for fp s 2fp is known as weak inversion. Figure 11.3 shows the surface potential along the length of the channel at accumulation, weak inversion, and threshold for the case when a small drain voltage is applied. The bulk p-substrate is assumed to be at zero potential. Figure 11.3b, c shows the accumulation and weak inversion cases. There is a potential barrier between the n source and channel region which the electrons must overcome in order to generate a channel current. A comparison of these barriers with those in pn junctions would suggest that the channel current is an exponential function of VGS. In the inversion mode, shown in Figure 11.3d, the barrier is so small that we lose the exponential dependence, since the junction is more like an ohmic contact. The actual derivation of the subthreshold current is beyond the scope of this chapter. We can write that eVGS ID (sub) exp _ kT eV · 1 exp __ kT DS (11.1) If VDS is larger than a few (kTe) volts, then the subthreshold current is independent of VDS. Figure 11.4 shows the exponential behavior of the subthreshold current for several body-to-source voltages. Also shown on the curves are the threshold voltage values. Ideally, a change in gate voltage on approximately 60 mV produces an order of magnitude change in the subthreshold current. A detailed analysis of the subthreshold condition shows that the slope of the ID versus VDS curve is a function of the semiconductor doping and is also a function of the interface state density. The nea29583_ch11_443-490.indd 445 12/11/10 12:42 PM 446 CHAPTER 11 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts 105 VT 1.04 V 106 1.71 V 2.61 V 3.29 V 1010 1011 0 1 3 V 1 V 109 2 VGS ( V ) 5 V 108 VBS 0 V ID (A) 107 3 4 Figure 11.4 | Subthreshold current– voltage characteristics for several values of substrate voltage (the threshold voltage is indicated on each curve). (From Schroder [17].) measurement of the slope of these curves has been used to experimentally determine the oxide–semiconductor interface state density. If a MOSFET is biased at or even slightly below the threshold voltage, the drain current is not zero. The subthreshold current may add significantly to power dissipation in a large-scale integrated circuit in which hundreds or thousands of MOSFETs are used. The circuit design must include the subthreshold current or ensure that the MOSFET is biased sufficiently below the threshold voltage in the “off ” state. 11.1.2 Channel Length Modulation We assumed in the derivation of the ideal current–voltage relationship that the channel length L was a constant. However, when the MOSFET is biased in the saturation region, the depletion region at the drain terminal extends laterally into the channel, reducing the effective channel length. Since the depletion region width is bias dependent, the effective channel length is also bias dependent and is modulated by the drain-to-source voltage. This channel length modulation effect is shown in Figure 11.5 for an n-channel MOSFET. The depletion width extending into the p-region of a pn junction under zero bias can be written as ______ xp nea29583_ch11_443-490.indd 446 2s f p __ eN (11.2) a 12/11/10 12:42 PM 11.1 VGS Nonideal Effects 447 Inversion charge S VDS n n L L p type VDS (sat) VGS VT VDS VDS VDS (sat) Figure 11.5 | Cross-section of an n-channel MOSFET showing the channel length modulation effect. For a one-sided np junction, essentially all of the applied reverse-biased voltage is across the low-doped p region. The space charge width of the drain–substrate junction is approximately _____________ xp eN ( 2s _ fp a VDS) (11.3) However, the space charge region defined by L, as shown in Figure 11.5, does not begin to form until VDS VDS (sat). As a first approximation, we can write that L is the total space charge width minus the space charge width that exists when VDS VDS (sat), or ____ L eN 2s _ a ___________________ ____________ f p VDS (sat) VDS f p VDS (sat) (11.4) where VDS VDS VDS (sat) (11.5) The applied drain-to-source voltage is VDS and we are assuming that VDS VDS (sat). As a second approximation at determining L, we can consider Figure 11.6 and revisit the one-dimensional Poisson’s equation. The electric field Esat is the lateral electric field at the point where the inversion layer charge is pinched off. Neglecting any charges that exist due to current, we can write (x) dE _ _ dx s (11.6) where (x) eNa and is a constant for a uniformly doped substrate. Integrating Equation (11.6) and applying the boundary conditions give the electric field in the space charge region defined by L: eNa x E _ s Esat nea29583_ch11_443-490.indd 447 (11.7) 12/11/10 12:42 PM 448 CHAPTER 11 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts Gate VGS VT Drain VDS VDS (sat) Esat n E Inversion charge x0 x L p type Figure 11.6 | Expanded view of cross section near the drain terminal of an n-channel MOSFET showing the channel length modulation effect. The potential in this region is (x) eNa x2 Edx _ Esat x C1 2s (11.8) where C1 is a constant of integration. The boundary conditions are (x 0) VDS (sat) and (x L) VDS. Substituting these boundary conditions into Equation (11.8), we obtain eNa( L)2 VDS __ Esat ( L) VDS (sat) 2s (11.9) Solving for L, we can write ____ L eN 2s _ a ___________________ ___ sat [VDS VDS(sat)] sat (11.10) where 2 Esat sat _s · _ eNa 2 2 In general, the value of Esat is in the range 104 Esat 2 105 V /cm. Other models used to determine L include the negative charges due to the drain current and also include two-dimensional effects. These models are not considered here. Since the drain current is inversely proportional to the channel length, we may write L ID __ I L L D (11.11) where ID is the actual drain current and ID is the ideal drain current. Since L is a function of VDS, ID is now also a function of VDS even though the transistor is biased in the saturation region. nea29583_ch11_443-490.indd 448 12/11/10 12:42 PM ID (mA) 11.1 8 7 6 5 4 3 2 1 0 L 0.73 m Z 30 m NA 7 1016 cm3 d 258 Å VBS 0 Exp Theory Nonideal Effects 449 VG 4 V 3V 2V 1V 1 2 3 VD (V ) 4 5 Figure 11.7 | Current–voltage characteristics of a MOSFET showing short-channel effects. (From Sze [22].) Since ID is now a function of VDS, the output resistance is no longer infinite. The drain current in the saturation region can be written as k W ID _n · _ · (VGS VT)2 (1 VDS) 2 L (11.12) where is the channel length modulation parameter. The output resistance is given by k2 · WL · (V ID ro _ VDS 1 _n _ GS VT)2 · 1 (11.13a) Since is normally small, Equation (11.13a) can be written as ro 1 _ (11.13b) ID Figure 11.7 shows some typical ID versus VDS curves with positive slopes in the saturation region due to channel length modulation. As the MOSFET dimensions become smaller, the change in the channel length L becomes a larger fraction of the original length L, and the channel length modulation becomes more severe. Objective: Determine the increase in drain current due to short channel modulation. EXAMPLE 11.1 Consider an n-channel MOSFET with a substrate doping concentration of Na 2 1016 cm3, a threshold voltage of VT 0.4 V, and a channel length of L 1 m. The device is biased at VGS 1 V and VDS 2.5 V. Determine the ratio of actual drain current compared to the ideal value. ■ Solution We find Na 2 1016 __ f p Vt ln _ ni (0.0259) ln 1.5 1010 0.3653 V VDS (sat) VGS VT 1.0 0.4 0.6 V nea29583_ch11_443-490.indd 449 12/11/10 12:42 PM 450 CHAPTER 11 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts and VDS VDS VDS (sat) 2.5 0.6 1.9 V Using Equation (11.4), we determine ____ L eN 2s _ a ___________________ ____________________ (1.6 ____________ f p VDS (sat) VDS f p VDS (sat) 14 _________________ ___________ 2(11.7)(8.85 10 ) ____ 0.3653 0.6 1.9 0.3653 0.6 19 16 1.807 10 5 10 )(2 10 ) cm or L 0.1807 m Then ID __ 1 L _ 1.22 __ ID L L 1 0.1807 ■ Comment The actual drain current increases as the effective channel length decreases when the transistor is biased in the saturation region. ■ EXERCISE PROBLEM Ex 11.1 An n-channel MOSFET has the same properties as described in Example 11.1 except for the channel length. The transistor is biased at VGS 0.8 V and VDS 2.5 V. Find the minimum channel length such that the ratio of actual drain current to the ideal drain current due to channel length modulation is no larger than 1.35. 11.1.3 Mobility Variation (Ans. L 0.698 m) In the derivation of the ideal I–V relationship, we explicitly assumed that the mobility was a constant. However, this assumption must be modified for two reasons. The first effect to be considered is the variation in mobility with gate voltage. The second reason for a mobility variation is that the effective carrier mobility decreases as the carrier approaches the velocity saturation limit. This effect is discussed in the next section. The inversion layer charge is induced by a vertical electric field, which is shown in Figure 11.8 for an n-channel device. A positive gate voltage produces a force on the electrons in the inversion layer toward the surface. As the electrons travel through the channel toward the drain, they are attracted to the surface, but then are repelled by localized coulombic forces. This effect, schematically shown in Figure 11.9, is called surface scattering. The surface scattering effect reduces mobility. If there is a positive fixed oxide charge near the oxide-semiconductor interface, the mobility will be further reduced due to the additional coulomb interaction. nea29583_ch11_443-490.indd 450 12/11/10 12:42 PM 11.1 Nonideal Effects 451 VGS Inversion charge VDS S E-field D n n Oxide S D p Space charge region Induced space charge region Inversion layer Figure 11.8 | Vertical electric field in an n-channel MOSFET. Figure 11.9 | Schematic of carrier surface scattering effects. The relationship between the inversion charge mobility and the transverse electric field is usually measured experimentally. An effective transverse electric field can be defined as 1 1 _ Eeff _ (11.14) s QSD (max) 2 Qn The effective inversion charge mobility can be determined from the channel conductance as a function of gate voltage. Figure 11.10 shows the effective electron mobility at T 300 K for different doping levels and different oxide thicknesses. The effective mobility is only a function of the electric field at the inversion layer and is independent of oxide thickness. The effective mobility may be represented by Eeff eff 0 _ E0 1 /3 (11.15) where 0 and E0 are constants determined from experimental results. Electron mobility (cm2/V· s) 2000 Slope 1/3 1000 400 200 104 105 106 Effective field in inversion layer, Eeff (V/cm) Figure 11.10 | Measured inversion layer electron mobility versus electric field at the inversion layer. (From Yang [25].) nea29583_ch11_443-490.indd 451 12/11/10 12:42 PM 452 CHAPTER 11 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts The effective inversion charge mobility is a strong function of temperature because of lattice scattering. As the temperature is reduced, the mobility increases. EXAMPLE 11.2 Objective: Calculate the effective electric field at threshold for a given semiconductor doping concentration. Consider a p-type silicon substrate at T 300 K doped to Na 3 1016 cm3. ■ Solution From the results of Chapter 10, we can calculate Na 3 1016 __ f p Vt ln _ ni (0.0259) ln 1.5 1010 0.376 V and 4s f p xdT __ eNa which is xdT 0.18 m. Then 1 /2 4(11.7)(8.85 1014)(0.376) _____ (1.6 1019)(3 1016) QSD (max) eNa xdT 8.64 1 /2 108 C /cm2 At the threshold inversion point, we may assume that Qn 0, so the effective electric field from Equation (11.14) is found as 8.64 108 1 ____ Eeff _ s QSD (max) (11.7)(8.85 1014) 8.34 104 V /cm ■ Comment We can see, from Figure 11.10, that this value of effective transverse electric field at the surface is sufficient for the effective inversion charge mobility to be significantly less than the bulk semiconductor value. ■ EXERCISE PROBLEM Determine (using Figure 11.10) the effective inversion layer electron mobility for a surface electric field of Eeff 2 105 V /cm. (Ans. n Ex 11.2 550 cm2 /V-s) The effective mobility is a function of gate voltage through the inversion charge density in Equation (11.14). As the gate voltage increases, the carrier mobility decreases even further. 11.1.4 Velocity Saturation In the analysis of the long-channel MOSFET, we assume the mobility to be constant, which means that the drift velocity increases without limit as the electric field increases. In this ideal case, the carrier velocity increases until the ideal current is attained. However, we have seen that the carrier velocity saturates with increasing electric field. Velocity saturation will become more prominent in shorter-channel devices since the corresponding horizontal electric field is generally larger. nea29583_ch11_443-490.indd 452 12/11/10 12:42 PM 11.1 Nonideal Effects 453 In the ideal I–V relationship, current saturation occurs when the inversion charge density becomes zero at the drain terminal, or when VDS VDS (sat) VGS VT (11.16) for the n-channel MOSFET. However, velocity saturation can change this saturation condition. Velocity saturation will occur when the horizontal electric field is approximately 104 V /cm. If VDS 5 V in a device with a channel length of L 1 m, the average electric field is 5 104 V /cm. Velocity saturation, then, is very likely to occur in short-channel devices. The modified ID(sat) characteristics are described approximately by ID (sat) W Cox (VGS VT)vsat (11.17) where vsat is the saturation velocity (approximately 10 cm /s for electrons in bulk silicon) and Cox is the gate oxide capacitance per cm2. The saturation velocity will decrease somewhat with applied gate voltage because of the vertical electric field and surface scattering. Velocity saturation will yield an ID(sat) value smaller than that predicted by the ideal relation, and it will yield a smaller VDS (sat) value than predicted. The ID(sat) current is also approximately linear with VGS, instead of having the ideal square law dependence predicted previously. There are several models of mobility versus electric field. One particular relation that is commonly used is eff ___ (11.18) eff E 2 1/2 _ 1 vsat 7 Figure 11.11 shows a comparison of drain current versus drain-to-source voltage characteristics for constant mobility and for field-dependent mobility. The smaller values of ID(sat) and the approximate linear dependence on VGS may be noted for the field-dependent mobility curves. The transconductance is found from ID(sat) WCox vsat gms __ VGS (11.19) which is now independent of VGS and VDS when velocity saturation occurs. The drain current is saturated by the velocity saturation effect, which leads to a constant transconductance. When velocity saturation occurs, the cutoff frequency is given by gm υsat WCox vsat _ fT __ __ 2 CG 2 (Cox WL) 2L (11.20) where the parasitic capacitances are assumed to be negligible. 11.1.5 Ballistic Transport Scattering events in a semiconductor limit the velocity of carriers to an average drift velocity as discussed in Chapter 5. The average drift velocity is a function of the nea29583_ch11_443-490.indd 453 12/11/10 12:42 PM 454 CHAPTER 11 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts 3.0 VG 5 V Constant mobility Velocity saturation 2.0 ID (mA) 4V VG 5 V 3V 4V 1.0 3V 2V 0 1V 0 5 VD (V ) 10 Figure 11.11 | Comparison of ID versus VD characteristics for constant mobility (dashed curves) and for field-dependent mobility and velocity saturation effects (solid curves). (From Sze and Ng [22].) mean time between collisions or the mean distance between scattering events. In the long-channel device, the channel length L is much longer than the mean distance between collisions l, so that an average carrier drift velocity exists. As the MOSFET channel length is reduced, the mean distance between collisions l may become comparable to L so that the previous analysis may not be valid. If the channel length is further reduced so that L l, then a large fraction of carriers could travel from the source to the drain without experiencing a scattering event. This motion of carriers is called ballistic transport. Ballistic transport means that carriers travel faster than the average drift velocity or the saturation velocity, and this effect can lead to very fast devices. Ballistic transport occurs in submicron (L 1 m) devices. As the MOSFET technology continues to shrink the channel length toward the 0.1 m value, the ballistic transport phenomenon will become more important. TEST YOUR UNDERSTANDING TYU 11.1 Consider a MOSFET biased in the subthreshold region with VD kT /e. For the ideal relationship given, what change in gate-to-source voltage produces a factor of 10 change in drain current? (Ans. VGS 59.64 mV) nea29583_ch11_443-490.indd 454 12/11/10 12:42 PM 11.2 TYU 11.2 MOSFET Scaling 455 Consider an NMOS transistor with the following parameters: n 1000 cm2/V-s, Cox 108 F /cm2, W 10 m, L 1 m, VT 0.4 V, and vsat 5 106 cm /s. Plot on the same graph ID (sat) versus VGS over the range 0 VGS 4 V for the case (a) of an ideal transistor (Equation (10.45a) and (b) when velocity saturation occurs (Equation (11.17). [Ans. (a) ID (sat) 50(VGS 0.4)2 A; (b) ID (sat) 50(VGS 0.4) A] 11.2 | MOSFET SCALING As we noted in the previous chapter, the frequency response of MOSFETs increases as the channel length decreases. The driving force in CMOS technology evolution in the last couple of decades has been reduced channel lengths. Channel lengths of 0.13 m or less are now the norm. One question that must be considered is what other device parameters must be scaled as the channel length is scaled down. 11.2.1 Constant-Field Scaling The principle of constant-field scaling is that device dimensions and device voltages be scaled such that electric fields (both horizontal and vertical) remain essentially constant. To ensure that the reliability of the scaled device is not compromised, the electric fields in the scaled device must not increase. Figure 11.12a shows the cross section and parameters of an original NMOS device and Figure 11.12b shows the scaled device, where the scaling parameter is k. Typically, k 0.7 per generation of a given technology. As seen in the figure, the channel length is scaled from L to kL. To maintain a constant horizontal electric field, the drain voltage must also be scaled from VD to kVD. The maximum gate voltage will also be scaled from VG to kVG so that the gate and drain voltages remain compatible. To maintain a constant vertical electric field, the oxide thickness then must also be scaled from tox to ktox. The maximum depletion width at the drain terminal, for a one-sided pn junction, is ___________ xD 2(Vbi VD) ___ (11.21) eNa VG kVG VD kV0 tox ktox rj rj krj krj kL L Na doping Na doping k (a) (b) Figure 11.12 | Cross section of (a) original NMOS transistor and (b) scaled NMOS transistor. nea29583_ch11_443-490.indd 455 12/11/10 12:42 PM 456 CHAPTER 11 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts Table 11.1 | Summary of constant-field device scaling Device and circuit parameters Scaling factor (k 1) Device dimensions (L, tox, W, xj) Doping concentration (Na, Nd) Voltages Electric field Carrier velocity Depletion widths Capacitance (C At) Drift current Device density Power density Power dissipation per device (P IV ) Circuit delay time ( CV1) Powerdelay product (P ) Scaled parameters Effect on device parameters Effect on circuit parameters k 1k k 1 1 k k k 1k2 1 k2 k k3 Source: Taur and Ning [23]. Since the channel length is being reduced, the depletion widths also need to be reduced. If the substrate doping concentration is increased by the factor (1/k), then the depletion width is reduced by approximately the factor k since VD is reduced by k. The drain current per channel width, for the transistor biased in the saturation region, can be written as nox nox ID _ _ (VG VT)2 → __ (kVG VT)2 W 2toxL 2(ktox)(kL) constant (11.22) The drift current per channel width remains essentially a constant, so if the channel width is reduced by k, then the drain current is also reduced by k. The area of the device, A WL, is then reduced by k2 and the power, P IV, is also reduced by k2. The power density in the chip remains unchanged. Table 11.1 summarizes the device scaling and the effect on circuit parameters. Keep in mind that the width and length of interconnect lines are also assumed to be reduced by the same scaling factor. 11.2.2 Threshold Voltage—First Approximation In constant-field scaling, the device voltages are reduced by the scaling factor k. It would seem appropriate that the threshold voltage should also be scaled by the same factor. The threshold voltage, for a uniformly doped substrate, can be written as __________ 2eNa(2f p) VT VFB 2f p ___ Cox (11.23) The first two terms in Equation (11.23) are functions of material parameters that do not scale and are only very slight __ functions of doping concentration. The last term is approximately proportional to k , so the threshold voltage does not scale directly with the scaling factor k. nea29583_ch11_443-490.indd 456 12/11/10 12:42 PM 11.3 Threshold Voltage Modifications 457 The effect of short channels on the threshold voltage is discussed further in section 11.3 of this chapter. 11.2.3 Generalized Scaling In constant-field scaling, the applied voltages are scaled with the same scaling factor k as the device dimensions. However, in actual technology evolution, voltages have not been reduced with the same scaling factor. There has been reluctance, for example, to change standardized power supply levels that have been used in circuits earlier. In addition, other factors that do not scale, such as threshold voltage and subthreshold currents, have made the reduction in applied voltages less desirable. As a consequence, electric fields in MOS devices have tended to increase as device dimensions shrinked. Consequences of increased electric fields are reduced reliability and increased power density. As the power density increases, the device temperature may increase. Increased temperature may affect the device reliability. As the oxide thickness is reduced and the electric field is increased, gate oxides are closer to breakdown and oxide integrity may be more difficult to maintain. In addition, direct tunneling of carriers through the oxide may be more likely to occur. Increased electric fields may also increase the chances of hot-electron effects, which are discussed later in this chapter. Reducing device dimensions, then, can introduce challenging problems that must be solved. TEST YOUR UNDERSTANDING An NMOS transistor has the following parameters: L 1 m, W 10 m, tox 250 Å, Na 5 1015 cm3, and applied voltages of 3 V. If the device is to be scaled using constant-field scaling, determine the new device parameters for a scaling factor of k 0.7. (Ans. L 0.7 m, W 7 m, tox 175 Å, Na 7.14 and applied voltages of 2.1 V) TYU 11.3 1015 cm3, 11.3 | THRESHOLD VOLTAGE MODIFICATIONS We have derived the ideal MOSFET relations in the previous chapter, including expressions for threshold voltage and for the current–voltage characteristics. We now consider some of the nonideal effects including channel length modulation. Additional effects on threshold voltage occur as the devices shrink in size. A reduction in channel length increases the transconductance and frequency response of the MOSFET, and a reduction in channel width increases the packing density in an integrated circuit. A reduction in either or both the channel length and channel width can affect the threshold voltage. 11.3.1 Short-Channel Effects For the ideal MOSFET, we have derived the threshold voltage using the concept of charge neutrality in which the sum of charges in the metal oxide inversion layer and nea29583_ch11_443-490.indd 457 12/11/10 12:42 PM 458 CHAPTER 11 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts Gate Gate Oxide Oxide n n n Qn n p p Q SD(max) (a) (b) Figure 11.13 | Cross section of a long n-channel MOSFET (a) at flat band and (b) at inversion. semiconductor space charge region is zero. We assumed that the gate area was the same as the active area in the semiconductor. Using this assumption, we have considered only equivalent surface charge densities and neglected any effects on threshold voltage that may occur due to source and drain space charge regions that extend into the active channel region. Figure 11.13a shows the cross section of a long n-channel MOSFET at flat band, with zero source and drain voltage applied. The space charge regions at the source and drain extend into the channel region but occupy only a small fraction of the entire channel region. The gate voltage, then, will control essentially all of the space charge induced in the channel region at inversion as shown in Figure 11.13b. As the channel length decreases, the fraction of charge in the channel region controlled by the gate decreases. This effect can be seen in Figure 11.14 for the flat-band condition. As the drain voltage increases, the reverse-biased space charge region at the drain extends further into the channel area and the gate controls even less bulk charge. The amount of charge in the channel region, QSD (max), controlled by the gate, affects the threshold voltage and can be seen from Equation (11.24) tox VTN QSD(max) Qss _ ox ms 2f p (11.24) We can quantitatively determine the short-channel effects on the threshold voltage by considering the parameters shown in Figure 11.15. The source and drain junctions are characterized by a diffused junction depth rj. We will assume that the lateral diffusion distance under the gate is the same as the vertical diffusion distance. This assumption is a reasonably good approximation for diffused junctions but becomes less accurate for ion implanted junctions. We will initially consider the case when the source, drain, and body contacts are all at ground potential. The basic assumption in this analysis is that the bulk charge in the trapezoidal region under the gate is controlled by the gate. The potential difference across the bulk space charge region is 2f p at the threshold inversion point, and the built-in potential barrier height of the source and drain junctions is also approximately 2 f p, implying that the three space charge widths are essentially equal. We can then write xs nea29583_ch11_443-490.indd 458 xd xdT xdT (11.25) 12/11/10 12:42 PM 11.3 Threshold Voltage Modifications 459 VG n rj n xdT L L xs Gate p Oxide n xd n p Figure 11.15 | Charge sharing in the short-channel threshold voltage model. Figure 11.14 | Cross section of a short n-channel MOSFET at flat band. (From Yau [26].) Using the geometrical approximation, the average bulk charge per unit area QB in the trapezoid is LL QB · L eNa xdT __ (11.26) 2 From the geometry, we can show that ________ rj 2xdT LL 1_ __ 1_ (11.27) rj 1 L 2L Then QB eNa xdT rj 1_ L ________ 1 2xr dT _ 1 j (11.28) Equation (11.28) is now used in place of QSD(max) in the expression for the threshold voltage. Since QSD(max) eNa xdT, we can find VT as Cox ________ L 1 2xr rj eNa xdT _ VT __ dT _ 1 j (11.29) where VT VT (short channel) VT (long channel) (11.30) As the channel length decreases, the threshold voltage shifts in the negative direction so that an n-channel MOSFET shifts toward depletion mode. Objective: Calculate the threshold voltage shift due to short-channel effects. Consider an n-channel MOSFET with Na 3 tox 20 nm 200 Å. nea29583_ch11_443-490.indd 459 EXAMPLE 11.3 1016 cm3, L 1.0 m, rj 0.3 m, and 12/11/10 12:42 PM 460 CHAPTER 11 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts ■ Solution We can find (3.9)(8.85 1014) ox ____ Cox _ 1.726 107 F /cm2 tox 200 108 Na 3 1016 __ fp Vt ln _ ni (0.0259) ln 1.5 1010 0.3758 V and 4s fp xdT __ eNa 4(11.7)(8.85 (1.6 10 0.18 104 cm 0.18 m 12 14 10 )(0.3758) _____ 19 )(3 16 10 ) 12 The shift in threshold voltage is now found as ________ 1 2xr rj eNa xdT _ VT __ Cox L dT _ 1 j 19 16 4 1.726 107 or __________ 1 1.0 1 2(0.18) 0.3 (1.6 10 )(3 10 )(0.18 10 ) 0.3 _______ _ __ VT 0.0726 V ■ Comment If the design value of the threshold voltage of an n-channel MOSFET is to be VT 0.35 V, for example, a shift of VT 0.0726 V due to short-channel effects is significant and needs to be taken into account. ■ EXERCISE PROBLEM Ex 11.3 Repeat Example 11.3 if the device parameters are Na 1016 cm3, L 0.75 m, rj 0.25 m, and tox 12 nm 120 Å. (Ans. VT 0.0469 V) The effect of short channels becomes more pronounced as the channel length is reduced further. The shift in threshold voltage with channel length for an n-channel MOSFET is shown in Figure 11.16. As the substrate doping increases, the initial threshold voltage increases, as we have seen in the previous chapter, and the short-channel threshold shift also becomes larger. The short-channel effects on threshold voltage do not become significant until the channel length becomes less than approximately 2 m. The threshold voltage shift also becomes smaller as the diffusion depth rj becomes smaller so that very shallow junctions reduce the threshold voltage dependence on channel length. Equation (11.29) is derived assuming that the source, channel, and drain space charge widths are all equal. If we now apply a drain voltage, the space charge width at the drain terminal widens, which makes L smaller, and the amount of bulk charge controlled by the gate voltage decreases. This effect makes the threshold voltage a function of drain voltage. As the drain voltage increases, the threshold voltage of an n-channel MOSFET decreases. The threshold voltage versus channel length is nea29583_ch11_443-490.indd 460 12/11/10 12:42 PM 11.3 Threshold Voltage Modifications 461 7 1017 6 tox 50 nm rj 0.5 m VGB 5 V 0.6 5 1016 Threshold voltage (V) VT VFB (V) 5 4 3 1016 2 Na 1 0 1015 1 2 3 L, m 4 5 6 VBS 1.25 V 0.4 VBS 0 V 0.2 VDS 4 V 0 0 VDS 0.125 1 2 3 4 5 6 Channel length (m ) 7 Figure 11.16 | Threshold voltage versus channel length for various substrate dopings. Figure 11.17 | Threshold voltage versus channel length for two values of drain-tosource and body-to-source voltage. (From Yau [26].) (From Yang [25].) plotted in Figure 11.17 for two values of drain-to-source voltage and two values of body-to-source voltage. 11.3.2 Narrow-Channel Effects Figure 11.18 shows the cross section along the channel width of an n-channel MOSFET biased at inversion. The current is perpendicular to the channel width through the inversion charge. We may note in the figure that there is an additional space charge region at each end of the channel width. This additional charge is controlled by the gate voltage but is not included in the derivation of the ideal threshold voltage relation. The threshold voltage expression must be modified to include this additional charge. L xdT W p type Figure 11.18 | Cross section of an n-channel MOSFET showing the depletion region along the width of the device. nea29583_ch11_443-490.indd 461 12/11/10 12:42 PM 462 CHAPTER 11 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts If we neglect short-channel effects, the gate-controlled bulk charge can be written as QB QB0 QB (11.31) where QB is the total bulk charge, QB0 is the ideal bulk charge, and QB is the additional bulk charge at the ends of the channel width. For a uniformly doped p-type semiconductor biased at the threshold inversion point, we may write QB0 eNa WLxdT (11.32) QB eNa LxdT ( xdT) (11.33) and where is a fitting parameter that accounts for the lateral space charge width. The lateral space charge width may not be the same as the vertical width xdT due to the thicker field oxide at the ends, and /or due to the nonuniform semiconductor doping created by an ion implantation. If the ends were a semicircle, then /2. We may now write QB QB0 QB eNa WL xdT eNa LxdT ( xdT) xdT eNa WL xdT 1 _ W (11.34) The effect of the end space charge regions becomes significant as the width W decreases and the factor ( xdT) becomes a significant fraction of the width W. The change in threshold voltage due to the additional space charge is xdT eNa xdT _ VT __ W Cox (11.35) The shift in threshold voltage due to a narrow channel is in the positive direction for the n-channel MOSFET. As the width W becomes smaller, the shift in threshold voltage becomes larger. EXAMPLE 11.4 Objective: Design the channel width that will limit the threshold voltage shift because of narrow channel effects to a specified value. Consider a silicon n-channel MOSFET with Na 3 1016 cm3 and tox 20 nm 200 Å. Let /2. Assume that the threshold voltage shift is to be limited to VT 0.2 V. ■ Solution We find Cox 1.726 107 F /cm2 and xdT 0.18 m From Equation (11.35), we can express the channel width as (0.18 104)2 (1.6 1019)(3 1016) _ eNa x2dT _______ 2 W __ (1.726 107)(0.2) Cox (VT) 7.08 nea29583_ch11_443-490.indd 462 105 cm 12/11/10 12:42 PM 11.3 Threshold Voltage Modifications 463 or W 0.708 m ■ Comment We may note that the threshold voltage shift of VT 0.2 V occurs at a channel width of W 0.708 m, which is approximately four times larger than the induced space charge width xdT. ■ EXERCISE PROBLEM Ex 11.4 Repeat Example 11.4 for Na 1016 cm3 and tox 8 nm 80 Å. Determine the channel width such that the threshold voltage shift is limited to VT 0.1 V. (Ans. W 0.524 m) Figure 11.19 shows the threshold voltage as a function of channel width. We can again note that the threshold voltage shift begins to become apparent for channel widths that are large compared to the induced space charge width. Figure 11.20a, b shows qualitatively the threshold voltage shifts due to shortchannel and narrow-channel effects, respectively, in n-channel MOSFETs. The narrow-channel device produces a larger threshold voltage; the short-channel device produces a smaller threshold voltage. For devices exhibiting both short-channel and narrow-channel effects, the two models need to be combined into a three-dimensional volume approximation of the space charge region controlled by the gate. 0.75 0.70 Threshold voltage (volts) 0.65 0.60 0.55 Na 1.71 1016 cm3 0.45 Na 1.55 1016 cm3 0.40 Na 1.25 1016 cm3 0.50 0.35 0.30 2 4 6 8 10 12 14 16 18 20 Width W (m) Figure 11.19 | Threshold voltage versus channel width (solid curves, theoretical; points, experimental). (From Akers and Sanchez [1].) nea29583_ch11_443-490.indd 463 12/11/10 12:42 PM 464 CHAPTER 11 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts VT VT L W (a) (b) Figure 11.20 | Qualitative variation of threshold voltage (a) with channel length and (b) with channel width. 11.4 | ADDITIONAL ELECTRICAL CHARACTERISTICS There is a tremendous volume of information on MOSFETs that cannot be included in an introductory text on semiconductor physics and devices. However, two additional topics should be included here: breakdown voltage and threshold adjustment by ion implantation. 11.4.1 Breakdown Voltage Several voltage breakdown mechanisms in the MOSFET must be considered, including voltage breakdown across the oxide as well as the various voltage breakdown mechanisms in the semiconductor junctions. Oxide Breakdown We have assumed that the oxide is a perfect insulator. However, if the electric field in the oxide becomes large enough, breakdown can occur, which can lead to a catastrophic failure. In silicon dioxide, the electric field at breakdown is on the order of 6 106 V /cm. This breakdown field is larger than that in silicon, but the gate oxides are also quite thin. A gate voltage of approximately 30 V would produce breakdown in an oxide with a thickness of 500 Å. However, a safety margin of a factor of 3 is common, so that the maximum safe gate voltage with tox 500 Å would be 10 V. A safety margin is necessary since there may be defects in the oxide that lower the breakdown field. Oxide breakdown is normally not a serious problem except in power devices and ultrathin oxide devices. Other oxide degradation problems are discussed later in this chapter. Avalanche Breakdown Avalanche breakdown may occur by impact ionization in the space charge region near the drain terminal. We have considered avalanche breakdown in pn junctions in Chapter 7. In an ideal planar one-sided pn junction, breakdown is a function primarily of the doping concentration in the low-doped region of the junction. For the MOSFET, the low-doped region corresponds to the semiconductor substrate. If a p-type substrate doping is Na 3 1016 cm3, for example, the pn junction breakdown voltage would be approximately 25 V for a planar junction. However, the n drain contact may be a fairly shallow diffused region with nea29583_ch11_443-490.indd 464 12/11/10 12:42 PM 11.4 Additional Electrical Characteristics G 465 D n p E-field B Figure 11.21 | Curvature effect on the electric field in the drain junction. ID VD Figure 11.22 | Current–voltage characteristic showing the snapback breakdown effect. a large curvature. The electric field in the depletion region tends to be concentrated at the curvature, which lowers the breakdown voltage. This curvature effect is shown in Figure 11.21. Near Avalanche and Snapback Breakdown1 Another breakdown mechanism results in the S-shaped breakdown curve shown in Figure 11.22. This breakdown process is due to second order effects and can be explained with the aid of Figure 11.23. The n-channel enhancement-mode MOSFET geometry in Figure 11.23a shows the 1 This section may be postponed until after the bipolar transistor is considered in Chapter 12. nea29583_ch11_443-490.indd 465 12/11/10 12:42 PM 466 CHAPTER 11 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts G G VDS n n S p D (a) (b) Figure 11.23 | (a) Cross section of the n-channel MOSFET. (b) Equivalent circuit including the parasitic bipolar transistor. n-type source and drain contacts along with the p-type substrate. The source and body are at ground potential. The n(source)-p(substrate)-n(drain) structure also forms a parasitic bipolar transistor. The equivalent circuit is shown in Figure 11.23b. Figure 11.24a shows the device when avalanche breakdown is just beginning in the space charge region near the drain. We tend to think of the avalanche breakdown suddenly occurring at a particular voltage. However, avalanche breakdown is a gradual process that starts at low current levels and for electric fields somewhat below the breakdown field. The electrons generated by the avalanche process flow into the drain and contribute to the drain current. The avalanche-generated holes generally flow through the substrate to the body terminal. Since the substrate has a nonzero resistance, a voltage drop is produced as shown. This potential difference drives the source-to-substrate pn junction into forward bias near the source terminal. The source is heavily doped n-type; thus, a large number of electrons can be injected from the source contact into the substrate under forward bias. This process becomes G D S n p n E-field E ICBO IE ␣IE C B (a) (b) Figure 11.24 | (a) Substrate current–induced voltage drop caused by avalanche multiplication at the drain. (b) Currents in the parasitic bipolar transistor. nea29583_ch11_443-490.indd 466 12/11/10 12:42 PM 11.4 Additional Electrical Characteristics 467 severe as the voltage drop in the substrate approaches 0.6 to 0.7 V. A fraction of the injected electrons diffuses across the parasitic base region into the reverse-biased drain space charge region where they also add to the drain current. The avalanche breakdown process is a function of not only the electric field but the number of carriers involved. The rate of avalanche breakdown increases as the number of carriers in the drain space charge region increases. We now have a regenerative or positive feedback mechanism. Avalanche breakdown near the drain terminal produces the substrate current, which produces the forward-biased source-substrate pn junction voltage. The forward-biased junction injects carriers that can diffuse back to the drain and increase the avalanche process. The positive feedback produces an unstable system. The snapback or negative resistance portion of the curve shown in Figure 11.22 can now be explained by using the parasitic bipolar transistor. The potential of the base of the bipolar transistor near the emitter (source) is almost floating, since this voltage is determined primarily by the avalanche-generated substrate current rather than an externally applied voltage. For the open-base bipolar transistor shown in Figure 11.24, we can write IC IE ICB0 (11.36) where is the common base current gain and ICB0 is the base-collector leakage current. For an open base, IC IE, so Equation (11.36) becomes IC IC ICB0 (11.37) At breakdown, the current in the B–C junction is multiplied by the multiplication factor M, so we have IC M( IC ICB0) (11.38) Solving for IC we obtain MICB0 IC __ 1 M (11.39) Breakdown is defined as the condition that produces IC → . For a single reversebiased pn junction, M → at breakdown. However, from Equation (11.39), breakdown is now defined to be the condition when M → 1 or, for the open-base condition, breakdown occurs when M → 1 / , which is a much lower multiplication factor than for the simple pn junction. An empirical relation for the multiplication factor is usually written as 1 M ___ 1 (VCE /VBD)m (11.40) where m is an empirical constant in the range of 3 to 6 and VBD is the junction breakdown voltage. The common base current gain factor is a strong function of collector current for small values of collector current. This effect will be discussed in Chapter 12 on bipolar transistors. At low currents, the recombination current in the B-E junction is a significant fraction of the total current so that the common base current gain is small. nea29583_ch11_443-490.indd 467 12/11/10 12:42 PM 468 CHAPTER 11 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts As the collector current increases, the value of increases. As avalanche breakdown begins and IC is small, particular values of M and VCE are required to produce the condition of M 1. As the collector current increases, increases; therefore, smaller values of M and VCE are required to produce the avalanche breakdown condition. The snapback, or negative resistance, breakdown characteristic is then produced. Only a fraction of the injected electrons from the forward-biased source-substrate junction are collected by the drain terminal. A more exact calculation of the snapback characteristic would necessarily involve taking into account this fraction; thus, the simple model would need to be modified. However, the above discussion qualitatively describes the snapback effect. The snapback effect can be minimized by using a heavily doped substrate that will prevent any significant voltage drop from being developed. A thin epitaxial p-type layer with the proper doping concentration to produce the required threshold voltage can be grown on a heavily doped substrate. Near Punch-Through Effects Punch-through is the condition at which the drainto-substrate space charge region extends completely across the channel region to the source-to-substrate space charge region. In this situation, the barrier between the source and drain is completely eliminated and a very large drain current would exist. However, the drain current will begin to increase rapidly before the actual punch-through condition is reached. This characteristic is referred to as the near punch-through condition, also known as Drain-Induced Barrier Lowering (DIBL). Figure 11.25a shows the ideal energy-band diagram from source to drain for a long n-channel MOSFET for the case when VGS VT and when the drain-to-source voltage is relatively small. The large potential barriers prevent significant current between the drain and source. Figure 11.25b shows the energy-band diagram when a relatively large drain voltage VDS2 is applied. The space charge region near the drain terminal is beginning to interact with the source space charge region and the potential barrier is being lowered. Since the current is an exponential function of barrier height, the current will increase very rapidly with drain voltage once this near punch-through Source Channel Ec EF Drain eVDS1 Ev eVDS eVDS2 EFs Ec EFd Ev (a) (b) Figure 11.25 | (a) Equipotential plot along the surface of a long-channel MOSFET. (b) Equipotential plot along the surface of a short-channel MOSFET before and after punch-through. nea29583_ch11_443-490.indd 468 12/11/10 12:42 PM 11.4 Additional Electrical Characteristics 469 ID 0 VDS Figure 11.26 | Typical I–V characteristics of a MOSFET exhibiting punchthrough effects. condition has been reached. Figure 11.26 shows some typical characteristics of a short-channel device with a near punch-through condition. Objective: Calculate the theoretical punch-through voltage assuming the abrupt junction approximation. Consider an n-channel MOSFET with source and drain doping concentrations of Nd 1019 cm3 and a channel region doping of Na 1016 cm3. Assume a channel length of L 1.2 m, and assume the source and body are at ground potential. EXAMPLE 11.5 ■ Solution The pn junction built-in potential barrier is given by (1016)(1019) Na Nd Vbi Vt ln _ (0.0259) ln ___ 0.874 V (1.5 1010)2 n2i The zero-biased source–substrate pn junction width is 2sVbi xd0 _ eNa 12 2(11.7)(8.85 1014)(0.874) _____ (1.6 1019)(1016) 12 0.336 m The reverse-biased drain-substrate pn junction width is given by 2s(Vbi VDS) xd ___ eNa 12 At punch-through, we will have xd0 xd L or 0.336 xd 1.2 which gives xd 0.864 m at the punch-through condition. We can then find x2d eNa ______ (0.864 104)2(1.6 1019)(1016) Vbi VDS __ 2s 2(11.7)(8.85 1014) 5.77 V nea29583_ch11_443-490.indd 469 12/11/10 12:42 PM 470 CHAPTER 11 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts The punch-through voltage is then found as VDS 5.77 0.874 4.9 V ■ Comment As the two space charge regions approach punch-through, the abrupt junction approximation is no longer a good assumption. The drain current will begin to increase rapidly before the theoretical punch-through voltage is reached. ■ EXERCISE PROBLEM Ex 11.5 Repeat Example 11.5 for a substrate doping concentration of Na 3 and a channel length of L 0.8 m. 1016 cm3 (Ans. VDS 7.52 V) For a doping of 1016 cm3, the two space charge regions will begin to interact when the abrupt depletion layers are approximately 0.25 m apart. The drain voltage at which this near punch-through condition, also known as drain-induced barrier lowering, occurs is significantly less than the ideal punch-through voltage such as calculated in Example 11.5 (see Problem 11.33). *11.4.2 The Lightly Doped Drain Transistor The junction breakdown voltage is a function of the maximum electric field. As the channel length becomes smaller, the bias voltages may not be scaled down accordingly, so the junction electric fields become larger. As the electric field increases, near avalanche breakdown and near punch-through effects become more serious. In addition, as device geometries are scaled down, the parasitic bipolar device becomes more dominant and breakdown effects are enhanced. One approach that reduces these breakdown effects is to alter the doping profile of the drain contact. The Lightly Doped Drain (LDD) design and doping profiles are shown in Figure 11.27a, the conventional MOSFET and doping profiles are shown in Figure 11.27b for comparison. By introducing the lightly doped region, the peak electric field in the space charge region is reduced and the breakdown effects are minimized. The peak electric field at the drain junction is a function of the semiconductor doping as well as the curvature of the n drain region. Figure 11.28 shows the physical geometries of a conventional n drain contact and an LDD structure superimposed on the same plot. The magnitude of the electric field at the oxide–semiconductor interface in the LDD structure is less than in the conventional structure. The electric field in the conventional device peaks approximately at the metallurgical junction and drops quickly to zero in the drain because no field can exist in the highly conductive n region. On the other hand, the electric field in the LDD device extends across the n-region before dropping to zero at the drain. This effect minimizes breakdown and the hot electron effects, which we discuss in Section 11.5.3. Two disadvantages of the LDD device are an increase in both fabrication complexity and drain resistance. The added processing steps, however, produce a device with significant improvements in performance. The cross section of the LDD device nea29583_ch11_443-490.indd 470 12/11/10 12:42 PM 11.4 A Poly-Si A n n Additional Electrical Characteristics n n B B Poly-Si n p 471 n 0.3 m 20 20 19 19 18 log Nd, Na log Nd , Na Section A-A n 17 n 16 Section B-B 18 n 17 16 p p 15 0.1 0.2 0.3 0.4 0.5 0.6 Distance (m) 0.7 0.8 15 0.9 0.1 0.2 0.3 (a) 0.4 0.5 0.6 Distance (m) 0.7 0.8 0.9 (b) Figure 11.27 | (a) The lightly doped drain (LDD) structure. (b) Conventional structure. (From Ogura et al. [12].) LDD Conventional Gate 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 x component of E (104 Vcm) n Conventional 5 4 3 2 1 n n LDD 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 Position along surface (m) Figure 11.28 | Magnitude of the electric field at the Si–SiO2 interface as a function of distance; VDS 10 V. VSB 2 V, VGS VT. (From Ogura et al. [12].) shown in Figure 11.27 indicates a lightly doped n region at the source terminal also. The inclusion of this region does not improve device performance, but does reduce the fabrication complexity as much as possible. The added series resistances increase power dissipation in the device; this must be taken into account in high-power devices. nea29583_ch11_443-490.indd 471 12/11/10 12:42 PM 472 CHAPTER 11 11.4.3 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts Threshold Adjustment by Ion Implantation Several factors, such as fixed oxide charge, metal–semiconductor work function difference, oxide thickness, and semiconductor doping, influence the threshold voltage. Although all of these parameters may be fixed in a particular design and fabrication process, the resulting threshold voltage may not be acceptable for all applications. Ion implantation can be used to change and adjust the substrate doping near the oxide–semiconductor surface to provide the desired threshold voltage. In addition, ion implantation is used for more than doping the channel. It is used extensively as a standard part of device fabrication; for example, it is used to form the source and drain regions of the transistor. To change the doping and thereby change the threshold voltage, a precise, controlled number of either donor or acceptor ions are implanted into the semiconductor near the oxide surface. When an MOS device is biased in either depletion or inversion and when the implanted dopant atoms are within the induced space charge region, then the ionized dopant charge adds to (or subtracts from) the maximum space charge density, which controls the threshold voltage. An implant of acceptor ions into either a p- or n-type substrate will shift the threshold voltage to more positive values, while an implant of donor ions will shift the threshold voltage to more negative values. Ion implantation can be carried out to change a depletion-mode device to enhancement-mode or an enhancement-mode device to depletion-mode, which is an important application of this technology. As a first approximation, assume that DI acceptor atoms per cm2 are implanted into a p-type substrate directly adjacent to the oxide–semiconductor interface as shown in Figure 11.29a. The shift in threshold voltage due to the implant is eD VT _I Cox (11.41) If donor atoms were implanted into the p-type substrate, the space charge density would be reduced; thus, the threshold voltage would shift in the negative voltage direction. Metal Metal p-type semiconductor Oxide DI (cm2) NS Na x0 (a) p-type semiconductor Oxide x xdT Na x0 x xI x xdT (b) Figure 11.29 | (a) Ion-implanted profile approximated by a delta function. (b) Ionimplanted profile approximated by a step function in which the depth xi is less than the space charge width xdT. nea29583_ch11_443-490.indd 472 12/11/10 12:42 PM 11.4 Additional Electrical Characteristics 473 A second type of implant approximation is the step junction, shown in Figure 11.29b. If the induced space charge width at the threshold inversion point is less than xI, then the threshold voltage is determined on the basis of a semiconductor with a uniform doping concentration of Ns atoms per cm3. On the other hand, if the induced space charge width is greater than xI at the threshold inversion point, then a new expression for xdT must be derived. We can apply Poisson’s equation and show that the maximum induced space charge width after the step implant is ____ xdT eN 2 ex 2s _ 2f p _I (Ns Na) 2s a 12 (11.42) The threshold voltage after a step implant for the case when xdT ten as xI can be writ- eD VT VT0 _I Cox (11.43) where VT0 is the preimplant threshold voltage. The parameter DI is given by DI (Ns Na)xI (11.44) 2 which is the number per cm of implanted ions. The preimplant threshold voltage is eNaxdT0 VT0 VFB0 2f p0 __ (11.45) Cox where the subscript 0 indicates the preimplant values. Objective: Design the ion implant dose required to adjust the threshold voltage to a specified value. Consider an n-channel silicon MOSFET with a doping of Na 5 1015 cm3, an oxide thickness of tox 18 nm 180 Å, and an initial flat-band voltage of VFBO 1.25 V. Determine the ion implantation dose such that a threshold voltage of VT 0.4 V is obtained. EXAMPLE 11.6 ■ Solution We find that Na 5 1015 __ fpO Vt ln _ ni (0.0259) ln 1.5 1010 0.3294 V 4s fpO xdTO __ eNa 0.4130 4(11.7)(8.85 (1.6 10 12 14 10 )(0.3294) _____ 19 )(5 15 10 ) 12 104 cm and (3.9)(8.85 1014) ox ____ 1.9175 107 F /cm2 Cox _ tox 180 108 The initial pre-implant threshold voltage is eNa xdTO VTO VFBO 2fpO __ Cox (1.6 1019)(5 1015)(0.4130 104) 1.25 2(0.3294) _______ 1.9175 107 0.419 V nea29583_ch11_443-490.indd 473 12/11/10 12:42 PM 474 CHAPTER 11 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts The threshold voltage after implant, from Equation (11.43), is eD VT VTO _I Cox so that (1.6 1019)DI 0.40 0.419 ___ 1.9175 107 which gives DI 9.815 1011 cm2 If the uniform step implant extends to a depth of xI 0.15 m, for example, then the equivalent acceptor concentration at the surface is DI Ns Na _ xI or Ns 5 11 9.815 10 1015 ___ 0.15 104 so that Ns 7.04 1016 cm3 ■ Comment It is assumed in the above calculation that the induced space charge width in the channel region is greater than the ion implant dept xI. The calculation satisfies our assumptions. ■ EXERCISE PROBLEM A silicon MOSFET has the following parameters: Na 1015 cm3, p polysilicon gate with an initial flat-band voltage of VFBO 0.95 V, and an oxide thickness of tox 12 nm 120 Å. A final threshold voltage of VT 0.40 V is required. Assume the idealized delta function for the ion implant profile shown in Figure 11.29a. (a) What type of ion (acceptor or donor) should be implanted? (b) Determine the required ion dose DI. [Ans. (a) donor ions; (b) DI 2.11 Ex 11.6 1012 cm2] The actual implant dose versus distance is neither a delta function nor a step function; it tends to be a Gaussian-type distribution. The threshold shift due to a nonuniform ion implant density may be defined as the shift in curves of Ninv versus VG, where Ninv is the inversion carrier density per cm2. This shift corresponds to an experimental shift of drain current versus VG when the transistor is biased in the linear mode. The criteria of the threshold inversion point as s 2f p in the implanted devices have an uncertain meaning because of the nonuniform doping in the substrate. The determination of the threshold voltage becomes more complicated and will not be made here. TEST YOUR UNDERSTANDING Repeat Exercise Problem Ex 11.6 for a final threshold voltage of (a) VT 0.25 V and (b) VT 0.25 V. 1011 cm2; (b) DI 2.03 1011 cm2 ] nea29583_ch11_443-490.indd 474 [Ans. (a) DI 8.02 TYU 11.4 12/11/10 12:42 PM 11.5 Radiation and Hot-Electron Effects 475 *11.5 | RADIATION AND HOT-ELECTRON EFFECTS We have considered the effects of fixed trapped oxide charge and interface state charge on the capacitance–voltage characteristics of MOS capacitors and on the MOSFET characteristics. These charges can exist because the oxide is essentially a perfect dielectric and a net charge density can exist in a dielectric material. Two processes that generate these charges are ionizing radiation and impact ionization in the drain region of a MOSFET operating near avalanche breakdown. MOS devices are exposed to ionizing radiation, for example, in communication satellites orbiting through the Van Allen radiation belts. The ionizing radiation can produce additional fixed oxide charge and also additional interface states. In this short discussion of radiation effects in MOSFETs, we are concerned only with the permanent effects that occur in the device characteristics. Another source can generate oxide charge and interface states: the hot electron effect. Electrons near the drain terminal of a MOSFET operating near avalanche breakdown can have energies that are much larger than the thermal-equilibrium value. These hot electrons have energies sufficient to penetrate the oxide–semiconductor barrier. 11.5.1 Radiation-Induced Oxide Charge Gamma-rays or x-rays incident on semiconductor or oxide materials can interact with valence band electrons. The incident radiation photons can impart enough energy to a valence electron to elevate the electron into the conduction band; an empty state or hole is also produced in the valence band. This process generates electron– hole pairs. These newly generated electrons and holes can move through a material under the influence of an electric field. Figure 11.30 shows the energy-band diagram of an MOS device with a p-type substrate and a positive gate voltage. The bandgap energy of silicon dioxide is SiO2 Gate (4) Radiation-induced interface traps within Si bandgap Si EC 1.1 eV EF EV (3) Deep hole trapping near Si/SiO2 interface (2) Hopping transport of holes through localized states in SiO2 bulk (1) Electron–hole pairs generated by ionizing radiation Figure 11.30 | Schematic of ionizing radiation–induced processes in an MOS capacitor with a positive gate bias. (From Ma and Dressendorfer [7].) nea29583_ch11_443-490.indd 475 12/11/10 12:42 PM 476 CHAPTER 11 Metal–Oxide–Semiconductor Field-Effect Transistor: Additional Concepts approximately 9 eV. The figure schematically shows the creation of an electron–hole pair in the oxide by ionizing radiation. The force on the radiation-induced electron is toward the gate and the force on the radiation-induced hole is toward the semiconductor. It has been found that generated electrons in the oxide are fairly mobile, with a mobility